This page intentionally left blank
Crystals, Defects and Microstructures Materials science has emerged as one of the ...

Author:
Phillips R.

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

This page intentionally left blank

Crystals, Defects and Microstructures Materials science has emerged as one of the central pillars of the modern physical sciences and engineering, and is now even beginning to claim a role in the biological sciences. A central tenet in the analysis of materials is the structure–property paradigm, which proposes a direct connection between the geometric structures within a material and its properties. The increasing power of high-speed computation has had a major impact on theoretical materials science and has permitted the systematic examination of this connection between structure and properties. In this textbook, Rob Phillips examines the various methods that have been used in the study of crystals, defects and microstructures and that have made such computations possible. The author presents many of the key general principles used in the modeling of materials, and punctuates the text with real case studies drawn from recent research. A second key theme is the presentation of recent efforts that have been developed to treat problems involving either multiple spatial or temporal scales simultaneously. This text is intended for graduate students and researchers in science and engineering with an interest in the theoretical constructs that have been devised to undertake the study of materials.

Crystals, Defects and Microstructures Modeling Across Scales ROB PHILLIPS Brown University, Providence RI

The Pitt Building, Trumpington Street, Cambridge, United Kingdom The Edinburgh Building, Cambridge CB2 2RU, UK 40 West 20th Street, New York, NY 10011-4211, USA 477 Williamstown Road, Port Melbourne, VIC 3207, Australia Ruiz de Alarcón 13, 28014 Madrid, Spain Dock House, The Waterfront, Cape Town 8001, South Africa http://www.cambridge.org © Robert B. Phillips 2004 First published in printed format 2001 ISBN 0-511-04108-X eBook (netLibrary) ISBN 0-521-79005-0 hardback ISBN 0-521-79357-2 paperback

Dedicated to Sonic’s accomplices

Contents

Preface Acknowledgements Notes on Units, Scales and Conventions

page xv xxi xxiv

Part one: Thinking About the Material World 1 1.1

1.2

1.3 2 2.1 2.2

2.3

2.4

1

Idealizing Material Response A Material World 1.1.1 Materials: A Databook Perspective 1.1.2 The Structure–Properties Paradigm 1.1.3 Controlling Structure: The World of Heat and Beat Modeling of Materials 1.2.1 The Case for Modeling 1.2.2 Modeling Deﬁned: Contrasting Perspectives 1.2.3 Case Studies in Modeling 1.2.4 Modeling and the Computer: Numerical Analysis vs Simulation Further Reading

3 3 3 8 12 14 14 15 18 25 26

Continuum Mechanics Revisited Continuum Mechanics as an Effective Theory Kinematics: The Geometry of Deformation 2.2.1 Deformation Mappings and Strain 2.2.2 Geometry of Rigid Deformation 2.2.3 Geometry of Slip and Twinning 2.2.4 Geometry of Structural Transformations Forces and Balance Laws 2.3.1 Forces Within Continua: Stress Tensors 2.3.2 Equations of Continuum Dynamics 2.3.3 Conﬁgurational Forces and the Dynamics of Defects Continuum Descriptions of Deformation and Failure 2.4.1 Constitutive Modeling

29 29 31 32 35 36 37 39 39 41 44 51 51

vii

viii

2.5

2.6 2.7 2.8 3 3.1 3.2

3.3

3.4 3.5

Contents

2.4.2 Linear Elastic Response of Materials 2.4.3 Plastic Response of Crystals and Polycrystals 2.4.4 Continuum Picture of Fracture Boundary Value Problems and Modeling 2.5.1 Principle of Minimum Potential Energy and Reciprocal Theorem 2.5.2 Elastic Green Function 2.5.3 Method of Eigenstrains 2.5.4 Numerical Solutions: Finite Element Method Difﬁculties with the Continuum Approach Further Reading Problems

51 54 60 64 64 66 69 72 75 76 78

Quantum and Statistical Mechanics Revisited Background Quantum Mechanics 3.2.1 Background and Formalism 3.2.2 Catalog of Important Solutions 3.2.3 Finite Elements and Schr¨odinger 3.2.4 Quantum Corrals: A Finite Element Analysis 3.2.5 Metals and the Electron Gas 3.2.6 Quantum Mechanics of Bonding Statistical Mechanics 3.3.1 Background 3.3.2 Entropy of Mixing 3.3.3 The Canonical Distribution 3.3.4 Information Theoretic Approach to Statistical Mechanics 3.3.5 Statistical Mechanics Models for Materials 3.3.6 Bounds and Inequalities: The Bogoliubov Inequality 3.3.7 Correlation Functions: The Kinematics of Order 3.3.8 Computational Statistical Mechanics Further Reading Problems

81 81 82 82 87 94 101 103 109 115 115 119 122 126 129 135 137 139 142 144

Part two: Energetics of Crystalline Solids

147

4 4.1 4.2

149 149 152 152

Energetic Description of Cohesion in Solids The Role of the Total Energy in Modeling Materials Conceptual Backdrop for Characterizing the Total Energy 4.2.1 Atomistic and Continuum Descriptions Contrasted

Contents

4.2.2

4.3

4.4

4.5

4.6

4.7 4.8 4.9 5 5.1 5.2

The Many-Particle Hamiltonian and Degree of Freedom Reduction Pair Potentials 4.3.1 Generic Pair Potentials 4.3.2 Free Electron Pair Potentials Potentials with Environmental and Angular Dependence 4.4.1 Diagnostics for Evaluating Potentials 4.4.2 Pair Functionals 4.4.3 Angular Forces: A First Look Tight-Binding Calculations of the Total Energy 4.5.1 The Tight-Binding Method 4.5.2 An Aside on Periodic Solids: k-space Methods 4.5.3 Real Space Tight-Binding Methods First-Principles Calculations of the Total Energy 4.6.1 Managing the Many-Particle Hamiltonian 4.6.2 Total Energies in the Local Density Approximation Choosing a Description of the Total Energy: Challenges and Conundrums Further Reading Problems

ix

154 156 156 158 164 164 165 172 176 176 184 189 197 198 200 203 204 206

5.5 5.6

Thermal and Elastic Properties of Crystals Thermal and Elastic Material Response Mechanics of the Harmonic Solid 5.2.1 Total Energy of the Thermally Fluctuating Solid 5.2.2 Atomic Motion and Normal Modes 5.2.3 Phonons 5.2.4 Buckminsterfullerene and Nanotubes: A Case Study in Vibration Thermodynamics of Solids 5.3.1 Harmonic Approximation 5.3.2 Beyond the Harmonic Approximation Modeling the Elastic Properties of Materials 5.4.1 Linear Elastic Moduli 5.4.2 Nonlinear Elastic Material Response: Cauchy–Born Elasticity Further Reading Problems

229 231 231 239 244 244 248 250 251

6 6.1 6.2

Structural Energies and Phase Diagrams Structures in Solids Atomic-Level Geometry in Materials

253 253 254

5.3

5.4

210 210 213 214 216 228

x

6.3

6.4

6.5

6.6 6.7 6.8

Contents

Structural energies of solids 6.3.1 Pair Potentials and Structural Stability 6.3.2 Structural Stability in Transition Metals 6.3.3 Structural Stability Reconsidered: The Case of Elemental Si Elemental Phase Diagrams 6.4.1 Free Energy of the Crystalline Solid 6.4.2 Free Energy of the Liquid 6.4.3 Putting It All Together 6.4.4 An Einstein Model for Structural Change 6.4.5 A Case Study in Elemental Mg Alloy Phase Diagrams 6.5.1 Constructing the Effective Energy: Cluster Expansions 6.5.2 Statistical Mechanics for the Effective Hamiltonian 6.5.3 The Effective Hamiltonian Revisited: Relaxations and Vibrations 6.5.4 The Alloy Free Energy 6.5.5 Case Study: Oxygen Ordering in High TC Superconductors Summary Further Reading Problems

Part three: Geometric Structures in Solids: Defects and Microstructures 7 7.1 7.2 7.3

7.4

7.5

Point Defects in Solids Point Defects and Material Response 7.1.1 Material Properties Related to Point Disorder Diffusion 7.2.1 Effective Theories of Diffusion Geometries and Energies of Point Defects 7.3.1 Crystallographic Preliminaries 7.3.2 A Continuum Perspective on Point Defects 7.3.3 Microscopic Theories of Point Defects 7.3.4 Point Defects in Si: A Case Study Point Defect Motions 7.4.1 Material Parameters for Mass Transport 7.4.2 Diffusion via Transition State Theory 7.4.3 Diffusion via Molecular Dynamics 7.4.4 A Case Study in Diffusion: Interstitials in Si Defect Clustering

260 261 264 265 268 268 275 277 278 280 282 283 291 297 299 300 304 304 305

309 311 311 312 318 318 326 327 328 332 341 344 345 346 351 353 356

Contents

xi

7.6 7.7

Further Reading Problems

356 359

8 8.1

Line Defects in Solids Permanent Deformation of Materials 8.1.1 Yield and Hardening 8.1.2 Structural Consequences of Plastic Deformation 8.1.3 Single Crystal Slip and the Schmid Law The Ideal Strength Concept and the Need for Dislocations Geometry of Slip 8.3.1 Topological Signature of Dislocations 8.3.2 Crystallography of Slip Elastic Models of Single Dislocations 8.4.1 The Screw Dislocation 8.4.2 The Volterra Formula 8.4.3 The Edge Dislocation 8.4.4 Mixed Dislocations Interaction Energies and Forces 8.5.1 The Peach–Koehler Formula 8.5.2 Interactions and Images: Peach–Koehler Applied 8.5.3 The Line Tension Approximation Modeling the Dislocation Core: Beyond Linearity 8.6.1 Dislocation Dissociation 8.6.2 The Peierls–Nabarro Model 8.6.3 Structural Details of the Dislocation Core Three-Dimensional Dislocation Conﬁgurations 8.7.1 Dislocation Bow-Out 8.7.2 Kinks and Jogs 8.7.3 Cross Slip 8.7.4 Dislocation Sources 8.7.5 Dislocation Junctions Further Reading Problems

362 362 363 365 367 369 371 372 375 382 382 388 391 392 393 395 398 402 404 404 406 412 415 416 418 423 426 430 435 437

Wall Defects in Solids Interfaces in Materials 9.1.1 Interfacial Conﬁnement Free Surfaces 9.2.1 Crystallography and Energetics of Ideal Surfaces 9.2.2 Reconstruction at Surfaces 9.2.3 Steps on Surfaces

441 441 442 446 447 452 474

8.2 8.3

8.4

8.5

8.6

8.7

8.8 8.9 9 9.1 9.2

xii

9.3

9.4

9.5 9.6 9.7 9.8

Contents

Stacking Faults and Twins 9.3.1 Structure and Energetics of Stacking Faults 9.3.2 Planar Faults and Phase Diagrams Grain Boundaries 9.4.1 Bicrystal Geometry 9.4.2 Grain Boundaries in Polycrystals 9.4.3 Energetic Description of Grain Boundaries 9.4.4 Triple Junctions of Grain Boundaries Diffuse Interfaces Modeling Interfaces: A Retrospective Further Reading Problems

476 477 484 487 489 492 494 500 501 502 503 505

10 Microstructure and its Evolution 10.1 Microstructures in Materials 10.1.1 Microstructural Taxonomy 10.1.2 Microstructural Change 10.1.3 Models of Microstructure and its Evolution 10.2 Inclusions as Microstructure 10.2.1 Eshelby and the Elastic Inclusion 10.2.2 The Question of Equilibrium Shapes 10.2.3 Precipitate Morphologies and Interfacial Energy 10.2.4 Equilibrium Shapes: Elastic and Interfacial Energy 10.2.5 A Case Study in Inclusions: Precipitate Nucleation 10.2.6 Temporal Evolution of Two-Phase Microstructures 10.3 Microstructure in Martensites 10.3.1 The Experimental Situation 10.3.2 Geometrical and Energetic Preliminaries 10.3.3 Twinning and Compatibility 10.3.4 Fine-Phase Microstructures and Attainment 10.3.5 The Austenite–Martensite Free Energy Reconsidered 10.4 Microstructural Evolution in Polycrystals 10.4.1 Phenomenology of Grain Growth 10.4.2 Modeling Grain Growth 10.5 Microstructure and Materials 10.6 Further Reading 10.7 Problems

507 508 508 516 519 520 520 527 528 529 537 540 546 547 551 554 560 565 566 567 568 580 580 582

Part four: Facing the Multiscale Challenge of Real Material Behavior

585

Contents

11 Points, Lines and Walls: Defect Interactions and Material Response 11.1 Defect Interactions and the Complexity of Real Material Behavior 11.2 Diffusion at Extended Defects 11.2.1 Background on Short-Circuit Diffusion 11.2.2 Diffusion at Surfaces 11.3 Mass Transport Assisted Deformation 11.3.1 Phenomenology of Creep 11.3.2 Nabarro–Herring and Coble Creep 11.4 Dislocations and Interfaces 11.4.1 Dislocation Models of Grain Boundaries 11.4.2 Dislocation Pile-Ups and Slip Transmission 11.5 Cracks and Dislocations 11.5.1 Variation on a Theme of Irwin 11.5.2 Dislocation Screening at a Crack Tip 11.5.3 Dislocation Nucleation at a Crack Tip 11.6 Dislocations and Obstacles: Strengthening 11.6.1 Conceptual Overview of the Motion of Dislocations Through a Field of Obstacles 11.6.2 The Force Between Dislocations and Glide Obstacles 11.6.3 The Question of Statistical Superposition 11.6.4 Solution Hardening 11.6.5 Precipitate Hardening 11.6.6 Dislocation–Dislocation Interactions and Work Hardening 11.7 Further Reading 11.8 Problems 12 Bridging Scales: Effective Theory Construction 12.1 Problems Involving Multiple Length and Time Scales 12.1.1 Problems with Multiple Temporal Scales: The Example of Diffusion 12.1.2 Problems with Multiple Spatial Scales: The Example of Plasticity 12.1.3 Generalities on Modeling Problems Involving Multiple Scales 12.2 Historic Examples of Multiscale Modeling 12.3 Effective Theory Construction 12.3.1 Degree of Freedom Selection: State Variables, Order Parameters and Conﬁgurational Coordinates 12.3.2 Dynamical Evolution of Relevant Variables: Gradient Flow Dynamics and Variational Principles 12.3.3 Inhomogeneous Systems and the Role of Locality

xiii

587 587 588 588 589 592 593 595 599 600 604 609 610 611 615 620 622 625 628 633 636 642 644 647 649 651 652 653 655 658 668 669 674 685

xiv

12.4

12.5

12.6

12.7 12.8

Contents

12.3.4 Models with Internal Structure 12.3.5 Effective Hamiltonians Bridging Scales in Microstructural Evolution 12.4.1 Hierarchical Treatment of Diffusive Processes 12.4.2 From Surface Diffusion to Film Growth 12.4.3 Solidiﬁcation Microstructures 12.4.4 Two-Phase Microstructures Revisited 12.4.5 A Retrospective on Modeling Microstructural Evolution Bridging Scales in Plasticity 12.5.1 Mesoscopic Dislocation Dynamics 12.5.2 A Case Study in Dislocations and Plasticity: Nanoindentation 12.5.3 A Retrospective on Modeling Plasticity Using Dislocation Dynamics Bridging Scales in Fracture 12.6.1 Atomic-Level Bond Breaking 12.6.2 Cohesive Surface Models 12.6.3 Cohesive Surface Description of Crack Tip Dislocation Nucleation Further Reading Problems

688 697 701 701 709 711 715 718 719 720 728 731 732 732 734 735 736 738

13 Universality and Speciﬁcity in Materials 13.1 Materials Observed 13.1.1 What is a Material: Another Look 13.1.2 Structural Observations 13.1.3 Concluding Observations on the Observations 13.2 How Far Have We Come? 13.2.1 Universality in Materials 13.2.2 Speciﬁcity in Materials 13.2.3 The Program Criticized 13.3 Intriguing Open Questions 13.4 In Which the Author Takes His Leave

742 743 743 744 746 748 749 750 751 752 754

References Index

757 771

Preface

Materials science as a formal discipline has quietly emerged as one of the central pillars of the physical sciences. Whether one interests oneself in the creation of lighter, more durable surfboards, or in the invention of new technologies to free up the trafﬁc jam on the world wide web, in the end, these questions will always imply demands which must be met by new classes of materials. Though the study of materials is largely rooted in the enlightened empiricism of traditional metallurgy, the advent of high-speed computers and the emergence of robust quantum simulations suggests new engineering strategies in which mechanism-based understanding might be hoped to lead to new materials. As a result of the maturation of theoretical materials science, it has become increasingly possible to identify a corpus of central results which serve as the basis for the analysis of materials. In addition, increasingly complex materials with structures at many different scales have led to the emergence of methods built around the explicit consideration of multiple scales simultaneously. As a result of these advances, this book attempts to take stock of the present capacity for modeling materials, with the word modeling used in the broadest sense. The book is divided into four basic parts. It opens with an overview of some of the key issues concerning materials that one might hope to succeed in modeling. Special reference is made to the notion of material parameters as characterized by the broad variety of data about materials that may be found in any databook. Though my comments on material response will be rather generic, my efforts to model such response will be restricted almost exclusively to crystalline solids. Though I am ashamed to have ignored so many classes of important and interesting materials, in the end, even restricting myself to crystalline materials left me with a project that exceeds my competence. After the introduction to material response, I present something like a modelers toolkit with a review of the key ideas from continuum mechanics, quantum mechanics and statistical mechanics that one might want to bring to the evaluation of a particular problem in the mechanics of materials. My argument here is that these three broad ﬁelds of study serve as the cornerstone for the rest of what we will do. The second main section of the xv

xvi

Preface

book is entitled ‘Energetics of Crystalline Solids’ and aims to describe the various tools that may be brought to bear on the problem of understanding the properties of perfect crystals. The argument made here is that the understanding we will require later concerning the role of defects in materials will have more impact when measured against the backdrop of the perfect solid. Particular emphasis in chaps. 4–6 is placed on computing the total energies of a given solid and using these energies to deduce the thermal and elastic properties of solids and the structural stability of different materials as revealed by phase diagrams. It should be noted that though I have restricted my attention to crystalline solids, much of what we will say in these chapters can be borrowed without alteration in the context of noncrystalline solids (and even liquids). Part 3, ‘Geometric Structures in Solids: Defects and Microstructures’ is organized according to the dimensionality of the various defects that populate materials and considers point defects (chap. 7), line defects (chap. 8) and interfacial defects (chap. 9). The organization of the material along dimensional lines is in the end somewhat artiﬁcial, but provides an organizational thread which has been useful to me if not the reader. Once an understanding of these various defects is in hand, I make an attempt at describing the assembly of these defects into a material’s microstructure (chap. 10). The ﬁnal part of the book, ‘Facing the Multiscale Challenge of Real Material Behavior’, should be seen as the culmination of the efforts set forth in the preceding chapters with the aim being to see just how far the modeler can go in the attempt to concretely consider material behavior. In addition, I have had a go at trying to seek the generic features of those models in which a deliberate attempt has been made to eliminate degrees of freedom. Indeed, my contention is that the enormous current interest in ‘multiscale modeling’ is born in large part of a self-conscious attempt to construct theories in a way that will lend them computational efﬁciency. Though there has been an incontrovertible increase in computational power, it has carried with it an attendant perception that almost always our appetite will outstrip our abilities. As a result, modelers throughout the physical sciences have had to seek to reformulate existing theories and to create new ones in a way that is ever mindful of the need to reduce computational burden. My reasons for writing this book are primarily selﬁsh. I have found that the only way I can really learn something is by self-study, and in particular, by seeking understanding at the level of the details – factors of 2 and π included. I consider myself one of the lucky few, namely, those who are able to earn a living as a college professor. Indeed, my privileges are greater yet. Almost daily I count my good fortune for having landed in the Solid Mechanics group at Brown University. One of the challenges in entering such a group has been to grope my way to some modicum of understanding in the area of the mechanics of materials. This book represents one part of that groping and reﬂects my own sense of some of the key

Preface

xvii

strategies that may be brought to bear on modeling material behavior. As part of the process of bringing myself up to speed for attempting to write this book, I have also undertaken the writing of a number of review articles with which the perceptive reader will undoubtedly see some overlap. This process was intentional in the hope that by working with various coauthors a useful vision of much of the material included here could be built up. Similarly, many of the ideas set forth here have been tested out in courses given at Brown, Caltech, the National University of Singapore and the Institut National Polytechnique de Grenoble. My intention in writing this book has not been to produce an encyclopedic compendium of all that is known concerning the modeling of materials and their properties. Rather, I have attempted to consider a sufﬁciently diverse set of problems to reveal the habit of mind that can be brought to the study of materials. Indeed, the book is largely anecdotal, with what I perceive to be fundamental ideas punctuated by more speculative ‘case studies’ that may not stand the test of time. As a result, the book has mixed character, alternating back and forth between text and monograph mode. In his outstanding book The Gift of Fire, Richard Mitchell notes the distinction between knowing and knowing about. The aims of the present work move back and forth between these objectives, with my hope being that after reading those sections having to do with general principles (and working the corresponding problems), the reader will ‘know’ these ideas. By way of contrast, the case studies are put forth more in the spirit of ‘knowing about’ with the hope that such studies will familiarize the reader with the implementation of the general ideas as well as the attendant literature, and will embolden him or her to set out to carry through a detailed case study themselves. I should also note that although many a preface emboldens the reader with the claim that various chapters can be read independently, I have written the present work very much as narrative, with the same idea presented in a different light several (or even many) different times, each contrasted with the other. For example, the discussion on Bridging Scales in Microstructural Evolution in chap. 12 presupposes a knowledge of what has gone before in chap. 10. Though it is true that one can read one without the other, it is certain that the message I wish to convey about microstructure and its evolution can only be gleaned by reading them both. For me, the book was written as a single entity and its logic is intertwined accordingly. In keeping with this general philosophy, the book is populated by a minimum of numerical tables in which speciﬁc data are presented. Rather, I have opted for pictorial and graphical representation of numerical results with the aim being the presentation of trends rather than detailed quantitative insights. On the other hand, there are a number of instances in which I present tables of data, but in the more sympathetic form of pictures. The calculations of the group of Skriver come to mind in this regard since they have done the service of providing the energies of

xviii

Preface

a number of defects (vacancies – ﬁg. 7.15, surfaces – ﬁg. 9.5 and step energies – ﬁg. 9.29) for a whole host of different materials, using the same theoretical analysis in each instance raising the possibility of a meaningful assessment of the trends. In addition, at times I have resorted to presenting collages of experimental data since I often feel it is beyond my competence to bring expert judgement to one experiment vs another and thus leave it to the reader to explore several sources and thereby decide for his or herself. My selection of material is also based in part upon a sinking feeling I sometimes get both while attending meetings and while cranking out the next calculation at my desk: it seems that so much of ‘research’ (mine included) is slated for obsolescence from the moment of its inception. It has always seemed to me that pedagogy is an ideal litmus test of signiﬁcance. Is a particular piece of work something that I would want to tell my students? The difﬁculty in answering this question is further exacerbated by the pedagogical uncertainties that attend the increasing reliance on numerical solutions and computer simulation. How exactly are we to communicate what is being learned from computational approaches? I have tried to follow a basic formula in many of the later chapters in the book. An attempt is ﬁrst made to illustrate the fundamental principles involved in contemplating a given class of material properties. These generic ideas, which are assumed to be largely uncontroversial, are then illustrated in an iterative fashion with a given case study examined from as many different angles as possible. For example, in discussing structural stability of Si, I make a point of showing how these questions can be addressed both from the perspective of empirical potentials and using ﬁrst-principles quantum mechanical treatments. Similarly, in my treatment of grain growth, I show how the Potts model, phase ﬁeld models and sharp interface models may all be used to examine the same basic process. My logic in these instances is to encourage a breadth of perspective ﬁltered by a critical eye that sees the shortcomings of all of these approaches. In the end, this book reﬂects my quest to unearth some of the exciting developments in the modeling of thermomechanical properties which have the power to either instruct or predict or entertain. In addition to commenting on what is in this book, it is with a trace of sadness that I also note what is not. With the narrowing of time between a given day of writing and the date of my self-imposed deadline, as well as with the increasingly swollen zip disks and hard copies of my book, it became increasingly clear that I must abandon many of my original intentions and resort to wholesale slashing. It is with particular regret that I eliminated my discussions of thermal conductivity, electromigration, the use of path integral methods to study diffusion and the electronic structure of quantum dots. In the end, I came to the view that I must stop and return to more active daily participation in family, sleep and my own research. I should also note that despite its length, in the end experts will recognize that my

Preface

xix

book has provided only a caricature of their ﬁelds. My aim was to highlight what seemed to me to be either the most general ideas or the most intriguing from each broad area. A word of explanation concerning references and further reading is in order. Ultimately, I decided to reference the works of others in only two ways. First, the Further Reading sections at the end of each chapter make reference only to those books or articles that form a part of my working and thinking vocabulary. Each time reference is made to one of these works, I attempt to provide some editorial comment as to why it has appeared on my list. My taste is idiosyncratic: if given the choice, I will always seek out that author who tells me something other than the party line, who has forged his or her own vision. I hold to this same mean in graduate teaching with the conviction that students are not interested in a watered down regurgitation of what they can read in the textbook – a unique perspective is what interests me. In addition to the suggestions for further reading, I have also compiled a single bibliography at the end of the book. This list serves an entirely different purpose and there is only a single way to get on it. These books and articles are those from which I have borrowed ﬁgures, followed derivations or turned the analysis into a ‘case study’. One of my abiding aims has been to try to ﬁgure out which part of the work on modeling has earned some level of permanence. Certain models (for example the quantum corral discussed in chap. 2) are pedagogically satisfying and at the same time permit immediate comparison with experiment. This is the ideal situation and, wherever possible, I have attempted to include them. In addition, I have also sought those steps forward that illustrate a certain approach that, in my opinion, should be imitated. As is evident from the preceding paragraphs, my bibliographic acumen is severely limited. The reference list is not encyclopedic and reﬂects my taste for browsing the index in a few favorite journals such as Physical Review B and Physical Review Letters, Journal of Mechanics and Physics of Solids, Metallurgical Transactions A, Philosophical Magazine and Acta Metallurgica. I am a particular fan of the ‘Overview’ sections in Acta Metallurgica and the articles written by award recipients in Metallurgical Transactions. Further, my choice of references is biased in favor of friends and acquaintances, due largely to the fact that in these instances I have had the beneﬁt of private discussions in order to learn what really happened. This is especially true in those cases where I sought a picture to illustrate a concept such as, for example, a polycrystalline microstructure. In these cases, it was most convenient to tap acquaintances, resulting in an over representation of work carried out at Brown. Hence, while my choice of references should be seen as something of an endorsement for those that are here, it should not be seen as a rejection of those that are not.

xx

Preface

Another feature of the book deserving of comment is the problem sets that are to be found at the end of each chapter. Many of these problems have already had a tour of duty in the various courses that I have taught at Brown and Caltech. On the other hand, there is a reasonable fraction of these problems that have not seen the light of day before now and thus risk having bugs of various types. The problems come in all types ranging from the ﬂeshing out of material covered in the chapters themselves to the construction of full-ﬂedged computational solutions to problems that are otherwise not tractable. A few stylistic comments are also in order. For the most part, I have written the book in the ﬁrst person plural, making constant reference to ‘we’ this and ‘we’ that. My reason for selecting this language is an honest reﬂection of my presumed relation with the reader – I imagine us both, you the reader and me, side by side and examining each question as it arises, almost always in a questioning tone: can we do better? I have reserved the more personal and subjective ‘I’ for those places where it is really my opinion that is being espoused as, for example, in the sections on Further Reading. In addition, the book is written in an informal (and at times light) style with various asides and observations. I fear that I will probably be charged with both ﬂippancy and arrogance, but wish to note at the outset that my hope was to produce a book that was to some extent fun to read. But even more importantly, I have tried to have fun in its writing. Three hours a morning for four years is a lot of hours to sit by oneself and I confess that on many occasions I could not resist certain turns of phrase or observations that amused me. Rob Phillips Barrington RI 2000

Acknowledgements

As a voracious reader myself, I am a veteran of many a preface and its attendant list of acknowledgements. What I realize now that it is my turn to make such a list is that for one such as me, who owes so much to so many, acknowledgements are deeply felt and yet are probably irrelevant to the anonymous reader. As said above, I wrote this book largely for myself in the hope that I would learn something in the act of so doing. This learning can be divided along two main lines, one emanating from the isolated groping I did at my desk, and the other from the pleasant meaningful interactions I have had with the people it is the business of this section to acknowledge. These paragraphs are for me and my family, my friends and my teachers. To all of you who have taught, tolerated, scolded, encouraged, discouraged, challenged and befriended me, let me state it simply: thank you for enriching my life. I now see the dangers inherent in making a list of names, but have decided to risk it on the grounds that I wish to express my indebtedness to some people publicly. I am grateful to William Martin and Andrew Galambos who literally opened up a new world of scientiﬁc thinking to my teenage mind, and life has never been the same. I am also grateful to Solomon Deressa, Chuck Campbell and Anders Carlsson, all of whom gave me a chance when I probably didn’t deserve one, and from whom, I have learned much. It is a pleasure to acknowledge my various friends at Brown from whom I have taken the vast majority of the courses offered in our Solid Mechanics curriculum (B. Freund – Stress Waves, Thin Films; R. Clifton – Advanced Continuum Mechanics; K.-S. Kim – Foundations of Continuum Mechanics; A. Bower – Plasticity; F. Shih – Finite Element Method; C. Briant – Mechanical Properties of Materials; and Mig Ortiz who taught Dislocations in Solids and much else through private consultation). Indeed, the inimitable Professor Ortiz has been the kind of friend and collaborator that one is lucky to ﬁnd even once. My good fortune at Brown has also been built around the chance to learn from a series of outstanding graduate students and postdocs. Ellad Tadmor, Ron Miller, Vijay Shenoy, David Rodney and Harley Johnson all were a key part of my ﬁrst ﬁve years at Brown and I can only hope they learned a fraction as much xxi

xxii

Acknowledgements

from me as I did from them. More recently, I have beneﬁted enormously from my interactions with Nitin Bhate, Dan Pawaskar, Kedar Hardikar and David Olmsted. As I said above, much of the fun in writing this book came from the interactions I had with others. I must single out Kaushik Bhattacharya, Rick James, Art Voter, Mig Ortiz, Chris Wolverton, Vivek Shenoy and Mark Asta, all of whom need special acknowledgement for running a veritable intellectual babysitting operation. I have also beneﬁted from expert advice on a number of different chapters from Janet Blume, Jane Kondev, Craig Black, Saryn Goldberg, Deepa Bhate, Anders Carlsson, K.-J. Cho, John Jameson, Tim Kaxiras, Stephen Foiles, Fabrizio Cleri, Mark Asta, Chris Wolverton, Art Voter, Luciano Colombo, Ladislas Kubin, Lyle Roelofs, Lloyd Whitman, Clyde Briant, Ben Freund, Dan Pawaskar, Karsten Jacobsen, Perry Leo, Kaushik Bhattacharya, Rick James, Simon Gill, Kevin Hane, T. Abinandanan, Peter Gumbsch, Long-Qing Chen, Georges Saada, Peter Voorhees, Alan Ardell, Emily Carter, Alan Needleman, Sam Andrews, Didier de Fontaine, Jakob Schiotz, Craig Carter, Jim Warren, Humphrey Maris, Zhigang Suo, Alan Cocks, Gilles Canova, Fred Kocks, Jim Sethna, Walt Drugan, Mike Marder, Bob Kohn, and Bill Nix and Mike Ashby indirectly as a result of a series of bootlegged course notes from excellent courses they have given. My book has also been read cover to cover by a number of hearty souls (Ron Miller, David Rodney, David Olmsted, Rob Rudd, Nitin Bhate, Walt Drugan and Bill Curtin) who made immensely useful suggestions that took my manuscript from an infantile performance to something that might be considered presentable. Of course, any errors that remain are strictly my own responsibility and indeed, at several junctures throughout the text, my arguments are suspect. It is also my great pleasure to thank Maryam Saleh who literally sketched, traced, drew and redrew over 300 ﬁgures, and Lorayn Palumbo who took care of everything from making sure I didn’t forget to teach my class to taking care of all manner of miscellaneous tasks. I am happy to extend my warmest thanks also to Amy Phillips who submitted literally hundreds of requests for permission to reprint ﬁgures. I would also like to thank Florence Padgett from Cambridge University Press who has supported me through the various stages of frustration that attended the writing of this book and, similarly, Simon Capelin. I would also like to acknowledge the outstanding editorial efforts of Maureen Storey who suggested all manner of improvements. The opportunity to write this book was supported generously through my wonderful NSF Career Award. As will be evident to any reader of my book, I have tried to present as many of my conclusions as possible in pictorial form. The task of amassing the various ﬁgures that form the backbone of this work was lightened enormously by the generous help of many friends, namely, Sharvan Kumar, Mike Mills, Peter Voorhees, Dan Fridline, Allan Bower, Alan Schwartzman, Harley Johnson,

Acknowledgements

xxiii

Karsten Jacobsen, Jakob Schiøtz, Rolf Heid, Rajiv Kalia, Sanjay Kodiyalam, Rick James, Kedar Hardikar, Dan Pawaskar, Charles McMahon, Vasily Bulatov, David Vanderbilt, Ralf Mueller, Lindsey Munro, Luciano Colombo, Tomas de la Rubia, George Gilmer, Christophe Coupeau, Marc Legros, Kevin Hemker, Sean Ling, Ian Robertson, Torben Rasmussen, Nasr Ghoniem, Klaus Schwarz, Marc Fivel, Bill Gerberich, David Rodney, Vivek Shenoy, Hans Skriver, Lloyd Whitman, Furio Ercolessi, Martin Bazant, Dieter Wolf, David Seidman, Craig Carter, Eric Chason, Stuart Wright, Brent Adams, Bob Hyland, Subra Suresh, Clyde Briant, Alan Ardell, Mitch Luskin, Liz Holm, Simon Gill, T. Abinandanan, Long Chen, Michael Ortiz (da Mig), Eberhard Bodenschatz, Art Voter, Chris Roland, Chris Wolverton, Charles-Andre Gandin, Michel Rappaz, Nik Provatas, John Hamilton, Farid Abraham, Harry Bhadesia and David Clarke. Thank you all again. My parents and sisters provided me a rich and interesting family life for which I count my blessings more each day and for which I thank them. Though the writing of this book took much time and effort spent in solitude to the sounds of Santana, Yehudi Menuhin, Bobby Caldwell, Eric Clapton, Sarah Brightman and others, in the end, it is but a small thing when measured against the things that really count such as a family. Many authors close their acknowledgements with accolades for their families who tolerated their absence and fatigue, etc. My temptations are different and can be stated succinctly by noting that it is my greatest pleasure to round out this list of acknowledgements by thanking Amy, Casey and Molly, who make coming home even more fun than going to work.

Notes on Units, Scales and Conventions

In the chapters to follow, one of our aims is to try to recast many of our results in numerical form, giving an impression of the many interesting scales (length, time, energy, stress, etc.) that arise in discussing solids. A prerequisite to such discussions is to make sure that a correspondence has been constructed between the units favored here and those encountered in the everyday experience of the reader. Geometric and Structural Notions. One of the most signiﬁcant single ideas that will appear in what follows is the important role played by geometric structures at a number of different scales within materials. Indeed, the coupling between structure and properties is an element of central orthodoxy in materials science. In characterizing the structures within materials, it is clearly overly pedantic to hold to any single set of units for characterizing such structures, and we will comfortably interchange between a few different units of measure. The smallest scales that we will touch upon are those tied to the existence of atoms and their arrangements to form crystalline solids. Two fundamental units of length are ˚ = 10−10 m) and the most popular in this setting, namely, the a˚ ngstrom (1 A −10 Bohr radius (a0 ≈ 0.529 177 × 10 m). The a˚ ngstrom should be seen as a member in the series of scales which are all simple factors of 10 away from the meter itself. On the other hand, the Bohr radius arises as a natural unit of length in assessing atomic-scale processes since it is built up as a combination of the fundamental constants characterizing these processes, namely, a0 = h¯ 2 /m e e2 , where h¯ is Planck’s constant, m e is the mass of the electron and e is the charge on an electron. We will also occasionally resort to the use of nanometers (1 nm = 10−9 m) as an alternative unit of length when characterizing atomic-scale processes. When characterizing structures at the microstructural level, we will try to hold to a single unit of length, the micron (1 µm = 10−6 m). Note that a human hair has dimensions on the order of 50 µm. The use of both nanometers and microns will be seen as characteristic of the dimensions of many structural features such as precipitates xxiv

Notes on Units, Scales and Conventions

xxv

and inclusions as well as the grains making up polycrystals. In our ambition of providing meaningful geometric classiﬁcations of solids, it will also be necessary to make reference to units of area and volume, both of which will be reported either ˚ 2 or m2 for areas using a˚ ngstroms or meters as the base unit, resulting in either A ˚ 3 or m3 for volumes. and A Time Scales and Temporal Processes. One of our recurring themes in the pages to follow will be the role of disparate scales in characterizing processes and structures within materials. In addition to the diversity of spatial scales, there are a host of processes in solids which are themselves characterized by widely different time scales. As a result, we will be forced to adopt a series of different measures of the passage of time. One of the elemental processes in solids that will occupy much of our attention is that of the vibrations of solids. As will become evident in later chapters, atomic vibrations are characterized by frequencies on the order of 1013 –1014 Hz, which corresponds to a time scale on the order of one-tenth of a picosecond. As a result, we will make use of both 1.0 fs = 10−15 s and 1.0 ps = 10−12 s in describing atomic motions. Force and Energy. Just as with the characterization of the various geometric structures that populate solids we will stick to a few standard units of measure: we will adopt a strategy of characterizing the various measures of force, stress and energy in terms of a few basic units. The two units of force that will occupy centerstage in the pages that follow are the standard MKS unit, the newton, ˚ (eV is a unit of energy) which is much and the less familiar choice of eV/A more representative of the types of forces that arise in characterizing atomic-scale motions. When translated into units of stress, we will ﬁnd it advantageous again to adopt two distinct sets of units, namely, the MKS unit of stress, the pascal ˚ 3 . In addition, we will ﬁnd (1 Pa = 1 N/m2 ) and the atomic-scale analog, eV/A it convenient to interchange between units of energy reported in both joules and electron volts (eV). In particular, we recall that the conversion between these two sets of units is given by 1.0 eV ≈ 1.602 × 10−19 J. On the other hand, from time to time we will also invoke the rydberg as a unit of energy. This unit of energy arises naturally in characterizing the energy levels of atoms and can be expressed in terms of fundamental constants as Ry = me4 /2h¯ 2 . Note that the conversion between Ry and eV is, 1 Ry = 13.6058 eV. In our analysis of activated processes, we will repeatedly ﬁnd it advantageous to reckon our energies in dimensionless form, where the energy scale is determined by k B T , here k B ≈ 1.38 × 10−23 J/K is Boltzmann’s constant. We note that a useful rule of thumb is that for room temperature, k B T ≈ 1/40 eV. For the remainder of the book, we will suppress the subscript on k B .

xxvi

Notes on Units, Scales and Conventions

Material Parameters. The key means whereby material speciﬁcity enters continuum theories is via phenomenological material parameters. For example, in describing the elastic properties of solids, linear elastic models of material response posit a linear relation between stress and strain. The coefﬁcient of proportionality is the elastic modulus tensor. Similarly, in the context of dissipative processes such as mass and thermal transport, there are coefﬁcients that relate ﬂuxes to their associated driving forces. From the standpoint of the sets of units to be used to describe the various material parameters that characterize solids, our aim is to make use of one of two sets of units, either the traditional MKS units or those in which the eV is the unit of energy and the a˚ ngstrom is the unit of length. Conventions. During the course of this work we will resort to several key conventions repeatedly. One important example is that of the summation convention which instructs us to sum on all repeated indices. For example, the dot product of two vectors may be written a · b = a1 b1 + a2 b2 + a3 b3 = ai bi .

(1)

A second key notational convention that will be invoked repeatedly is the deﬁnition of the dyadic product given by (a ⊗ b)v = a(b · v). Another key convention that will be used repeatedly is the notation that {ai } refers to the set a1 , a2 , . . . , a N . When carrying out integrations, volumes will typically be denoted by while the boundary of such a volume will be denoted as ∂.

Part one Thinking About the Material World

ONE

Idealizing Material Response

1.1 A Material World Steel glows while being processed, aluminum does not. Red lasers are commonplace, while at the time of this writing, the drive to attain bright blue light is being hotly contested with the advent of a new generation of nitride materials. Whether we consider the metal and concrete structures that ﬁll our cities or the optical ﬁbers that link them, materials form the very backdrop against which our technological world unfolds. What is more, ingenious materials have been a central part of our increasing technological and scientiﬁc sophistication from the moment man took up tools in hand, playing a role in historic periods spanning from the Bronze Age to the Information Age. From the heterostructures that make possible the use of exotic electronic states in optoelectronic devices to the application of shape memory alloys as ﬁlters for blood clots, the inception of novel materials is a central part of modern invention. While in the nineteenth century, invention was acknowledged through the celebrity of inventors like Nikola Tesla, it has become such a constant part of everyday life that inventors have been thrust into anonymity and we are faced daily with the temptation to forget to what incredible levels of advancement man’s use of materials has been taken. Part of the challenge that attends these novel and sophisticated uses of materials is that of constructing reliable insights into the origins of the properties that make them attractive. The aim of the present chapter is to examine the intellectual constructs that have been put forth to characterize material response, and to take a ﬁrst look at the types of models that have been advanced to explain this response. 1.1.1 Materials: A Databook Perspective What is a material? The answer to this seemingly nonsensical question strikes right to the heart of some of the key issues it is the aim of this book to examine. 3

4

1 Idealizing Material Response

From the most naive of perspectives, questions surrounding the deﬁning qualities of a particular material are easily answered in terms of our everyday perceptions: weight, luster, color, hardness, susceptibility to heating. However, these simple notions are a reﬂection of a deeper underlying identity, an identity that is revealed quantitatively the moment one poses the question of precisely how a given material replies when affected by some external probe. If we subject a material to a force, it changes shape. If we apply a potential difference, electrical current might ﬂow. And if the temperatures of the two ends of a sample are different, a ﬂow of heat results. In each of these cases, these experiments reveal something further about the identity of the material in question. One of the overarching conceptual themes that has emerged from such simple experiments and that rests behind the quantitative description of materials is the idea of a material parameter. For example, Hooke’s original efforts, which were aimed at uncovering the relation between a body’s extension and the applied force that engendered it, led to the recognition that there exist a series of numbers, namely the elastic moduli, that characterize the elastic response of that material under different loading conditions. Similarly, there is a well established tradition of subjecting materials to applied ﬁelds which result in the emergence of various ﬂuxes such as the electrical and thermal currents mentioned above. Allied with these ﬂuxes are material parameters that link the response (i.e. the ﬂux) to the applied ﬁeld. In these cases and many more, the central idea is that a particular material can be identiﬁed in terms of the speciﬁc values adopted by its material parameters. In fact, for some purposes, a particular material may be idealized completely in terms of a set of such parameters. For the elastician, single crystal Al is characterized by a density and three elastic constants, namely, C11 = 106.78 GPa, C12 = 60.74 GPa and C44 = 28.21 GPa (data for Al at 300 K taken from Simmons and Wang (1971)). By way of contrast, to the engineer concerned with the application of Al in thermal environments, Al is speciﬁed in terms of a density and a thermal conductivity κ = 2.37 W/(cm K) (data for Al at 300 K taken from Shackelford et al. (1995)). This type of idealization of a material in which its entire identity is represented by but a few numbers is one of far-reaching subtlety. In the context of the elastic constants, all of the relevant atomic bond stretching and bending has been subsumed into the three material parameters introduced above. Similarly, the full complexity of the scattering of phonons giving rise to the thermal properties of a material has also been subsumed into just one or a few numbers. One of our primary missions in the coming chapters will be to explore how such effective theories of material behavior may be built strictly on the basis of such material parameters and to examine what gives rise to the difference in these parameters from one material to the next.

1.1 A Material World

5

From the standpoint of the idea given above, a particular material is characterized by a set of numbers that can be unearthed in a databook. For example, important parameters include the density ρ, the yield stress σ y , the fracture toughness K I C and the diffusion constant D. We note that in each case there is a number that can be looked up that characterizes the weight of a material in some normalized terms (i.e. the density), the resistance of the material to permanent deformation and fracture (yield strength and toughness), the ease with which mass can be transported within the material at elevated temperatures (diffusion constant) and any of a number of other possibilities. Our main point is to illustrate the way in which a given number (or set of numbers) can be used to introduce material speciﬁcity into continuum treatments of material response. For example, in considering the continuum treatment of mass transport, it is held that the ﬂux of mass is proportional to the gradient in concentration, with the constant of proportionality being the diffusion constant. This same basic strategy is exploited repeatedly and always hinges on the fact that the complexity of the atomic-level processes characterizing a given phenomenon can be replaced with a surrogate in the form of material parameters. The signiﬁcance of the notion of a material parameter is further clariﬁed by putting the properties of different materials into juxtaposition with one another. In ﬁgs. 1.1 and 1.2, we follow Ashby (1989) with some representative examples of the range of values taken on by a few prominent material properties, namely the Young’s modulus, the yield strength, the fracture toughness and the thermal conductivity. The basic idea adopted in Ashby’s approach is to allow the contrasts between the properties of different materials to speak for themselves. One of our aims in the chapters that follow will be to develop plausible explanations for the range of data indicated schematically in ﬁg. 1.1, with special attention reserved for thermomechanical properties. Despite the power of the idea of a material parameter, it must be greeted with caution. For many features of materials, certain ‘properties’ are not intrinsic. For example, both the yield strength and fracture toughness of a material depend upon its internal constitution. That is, the measured material response can depend upon microstructural features such as the grain size, the porosity, etc. Depending upon the extent to which the material has been subjected to prior working and annealing, these properties can vary considerably. Even a seemingly elementary property such as the density can depend signiﬁcantly upon that material’s life history. For a material such as tungsten which is often processed using the techniques of powder metallurgy, the density depends strongly upon the processing history. The signiﬁcance of the types of observations given above is the realization that many material properties depend upon more than just the identity of the particular atomic constituents that make up that material. Indeed, one of our central themes will

6

1 Idealizing Material Response

Fig. 1.1. Elastic and plastic properties of a wide class of materials (adapted from Ashby (1989)).

1.1 A Material World

7

Fig. 1.2. Fracture and thermal properties of a wide class of materials (adapted from Ashby (1989)).

8

1 Idealizing Material Response

be the argument that microstructural features such as point defects, dislocations and grain boundaries can each alter the measured macroscopic ‘properties’ of a material. One of our primary concerns in the pages that follow is to understand the emergence of material properties on the basis of the geometric structures that populate materials. This critical link between structure and properties has been canonized through the structure–properties paradigm which elevates the analysis of structure as a prerequisite to understanding properties. We have tried, in this section, to present something of the backdrop against which we will develop models of material behavior, especially with reference to thermomechanical properties. As an introduction to such models we ﬁrst examine the role played by geometric structure in dictating material properties, followed by an overview of the ways in which materials may be tailored to yield particular values of these material parameters.

1.1.2 The Structure–Properties Paradigm In the previous section we noted that, in the abstract, Al (or any other material) may be characterized by a series of numbers, its material parameters, to be found in a databook. However, as we already hinted at, because of the history dependence of material properties, the description of such properties is entirely more subtle. There is no one aluminum, nor one steel, nor one zirconia. Depending upon the thermomechanical history of a material, properties ranging from the yield strength to the thermal and electrical conductivity can be completely altered. The simplest explanation for this variability is the fact that different thermomechanical histories result in different internal structures. A fundamental tenet of materials science hinted at in the discussion above is the structure–properties paradigm. The claim is that by virtue of a material’s structure many of its associated properties are determined. Structure is an intrinsically geometric notion and one of the abiding themes in this book will be the constant reminder that it is structure on a variety of different length scales that gives rise to many of the well-known properties of materials. From the atomic-scale perspective we will constantly return to the implications of the fact that a material has a given crystal structure, whether it be for its role in dictating the properties of interfacial defects such as antiphase boundaries or the elastic anisotropy that must enter elasticity theory if the crystal symmetries are to be properly accounted for. Next, we will devote repeated attention to the lattice defects that disturb the uninterrupted monotony of the perfect crystal. Vacancies, interstitials, dislocations, stacking faults, grain boundaries and cracks will each claim centerstage in turn. At yet lower resolution, it is geometry at the microstructural scale that comes into relief and will occupy much of our attention. At each of these scales we will return to

1.1 A Material World

9

Fig. 1.3. Yield strength data for steel as a function of grain size d (adapted from Leslie (1981)). Plot shows dependence of yield stress on inverse power of grain size. The legends at the top of the ﬁgure show the actual grain size as measured in both µm and using the ASTM units for grain size.

the question of the structure–properties paradigm, always with a critical eye, to see just how far it may take us in our desire to unearth the behavior of real materials. A celebrated example of the coupling of structure and properties is exhibited in ﬁg. 1.3 in which the relation between the yield strength and the grain size is depicted. In particular, the Hall–Petch relation √ posits a relation between the yield stress and the grain size of the form σ y ∝ 1/ d, where d is the grain size of the material. The Hall–Petch relation leads us to two of the most important notions to be found in contemplating materials: the existence of microstructure and its implications for material properties, and the development of scaling laws for characterizing material response. An immediate consequence of the results depicted here is the insight that not only are structures at the atomic scale important, but so too are the geometric structures found at the microstructural scale. We have noted that the attempt to understand materials demands that we confront a hierarchy of geometric structures, starting with the atomic-level geometries presented by the crystal lattice and increasing in scale to the level of the isolated defects that exist within materials to their assembly into the material’s microstructure itself. The quest to understand the structure of a given material inevitably commences with the phase diagram. Phase diagrams are one of the primary road maps of the materials scientist. Such diagrams represent a summary of a series of tedious analyses aimed at determining the equilibrium atomic-scale structure of a given element or mixture of elements for a series of temperatures (and possibly

10

1 Idealizing Material Response

Fig. 1.4. Phase diagram of elemental sulfur (adapted from Young (1991)).

pressures). In ﬁgs. 1.4 and 1.5, we show the equilibrium phase diagrams of elemental sulfur and the iron–carbon system. The particular choices of materials shown here are meant to give a feel for the existence of the rich atomic-level complexity that is found in both elemental systems and their alloy counterparts. Note that in the case of elemental sulfur, there are not less than ten different equilibrium structures corresponding to different values of the temperature and pressure. These structures are built around molecular S8 and range from orthorhombic to monoclinic lattices. The iron–carbon phase diagram illustrates a similar structural diversity, with each phase boundary separating distinct structural outcomes. Phase diagrams like those discussed above have as their primary mission a succinct description of the atomic-level geometries that are adopted by a given system. However, as we have already mentioned, there is structure to be found on many different length scales, and one of the surprises of deeper reﬂection is the realization that despite the fact that phase diagrams reﬂect the equilibrium state of a given material, they can even instruct us concerning the metastable microstructures that occur at larger scales. The simplest example of such thinking is that associated with precipitation reactions in which an overabundance of substitutional impurities is frozen into a system by quenching from high temperatures. If the material is subsequently annealed, the phase diagram leads us to expect a two-phase

1.1 A Material World

11

Fig. 1.5. Phase diagram for the iron–carbon system (adapted from Ashby and Jones (1986)).

microstructure in which the overabundance of substitutional impurities is now taken up in the relevant equilibrium phase. What this suggests is that strategies can be concocted for preparing particular metastable states with desirable properties. It is this insight that has led to many of the heat and beat strategies that have attracted pejorative attention to the materials engineer. A broad description of the signiﬁcance of phase diagrams to materials science may be found in Massalski (1989). As noted above, the phase diagram instructs our intuitions concerning the atomic-level geometries of materials. At the next level of geometric complexity in the hierarchy of structures that exist within a material, we must confront the defects that populate materials. Indeed, one of the key realizations that we will revisit from a number of different perspectives is that of the role of defects in the determination of material response. What this means is that the structure–properties paradigm makes an ambiguous use of the word ‘structure’ since in different situations, the structures being referenced can range all the way from atomic-scale structure to that of the nature of the grains making up a polycrystal. At the level of the defect

12

1 Idealizing Material Response

geometries found within materials, our present argument is that if we trace yield in crystals to the mechanisms which engender it for example, it is the motion of dislocations which will be implicated. Similarly, if we pursue the stress–strain curve to its limits, the material will fail either through crack propagation or void coalescence or some other defect mechanism. The implication of this insight is that much of the work of modeling the thermomechanical behavior of materials can be reduced to that of carrying out the structure–properties linkage at the level of defect structures within materials. In later chapters, we will adopt a hierarchical approach to constructing models of material response. First, we will examine the way in which atomistic models can be used to uncover the structural rearrangements in defect ‘cores’ which are a signature of the nonlinear interatomic interactions that are difﬁcult to capture within continuum theory. Once these tools are in hand, we will turn to an analysis of the dominant defect types themselves, with a classiﬁcation scheme centered on the dimensionality of these defects. Having successfully captured the structure and energetics of single defects, our next mission will be to understand the role of defects as conspiratorial partners in the emergence of observed macroscopic behavior. The uncovering of this conspiracy will in the end always lead us to questions of averaging. The challenge here is in forging the connection between the behavior of single defects, on one hand, and the macroscopic material response, on the other, which often emerges as a synthetic response of many defects in concert.

1.1.3 Controlling Structure: The World of Heat and Beat In the previous section we considered the critical role played by structures at a number of different scales in determining material properties. From the standpoint of the materials engineer this insight may be recast as a challenge: how may the various structures within a material be tailored so as to yield desired properties? Metallurgy has a longstanding reputation as an empirical subject founded upon the twin pillars of heating and beating a material to some desired form. Whether one resorts to cold working a material or subjecting it to a high-temperature anneal, the outcome of these processes is a change in the internal constitution of that material at one or more scales. Because of these structural changes, there is a concomitant change in the properties of the material. Indeed, these strategies for altering the structure of materials should be seen as the answer to the challenge posed above. By carefully selecting the thermal and mechanical history of a material, it is possible to tailor a number of different features of that material. Low-temperature anneals can induce precipitate reactions that increase the yield stress. Cold working changes the dislocation density, and this too alters the yield stress. If the material

1.1 A Material World

13

Fig. 1.6. Schematic of the different microstructures for the Ni–Al system that are obtained using different thermomechanical processing schedules (adapted from Kumar et al. (1992)). The ﬁgure illustrates precipitation at grain boundaries and within grains.

is exposed to a particular chemical atmosphere it can result in a thin surface layer that can increase the material’s hardness, a strategy that is adopted in the production of carburized steels. In each of these examples, through annealing (heat) or deformation (beat) or both, the internal structures within the material are changed and as a result, so too are the macroscopic properties. As an explicit example of how a material changes when subjected to the type of processing program introduced above, ﬁg. 1.6 shows a schematic of the microstructures that arise from slightly different chemical compositions and for different thermal histories for Ni-rich Ni–Al alloys. The ﬁgure illustrates the signiﬁcant variety in microstructure as a function both of slight ( 0, E˙ surf is the increase in surface energy and may be written down directly as E˙ surf = 4γ a, ˙ where γ is the surface energy and (a, ˙ a) is the dissipative potential and is of the form (a, ˙ a) = a˙ 2 /2M. The factor of 4 in the expression for E˙ surf results from the fact that for a crack of length 2a such as that under consideration here, there is both a top and bottom face contributing to the overall surface energy. To proceed with the calculation, we must still determine the rate of change of E elastic . For a crack of length 2a under plane strain conditions and subject to a remote load σ0 , the elastic energy is given by (a result which we apologize for quoting without proof, see Lawn (1993)) E elastic (a) = −

πa 2 σ02 (1 − ν 2 ) , E

(2.71)

˙ a) is given by implying that E˙ elastic (a, 2πaσ02 (1 − ν 2 ) E˙ elastic (a, a. ˙ ˙ a) = − E

(2.72)

Note that E is the Young modulus and ν is the Poisson ratio for the material of interest. We are now ready to turn to the concrete implementation of the variational statement of eqn (2.70). Evaluation of ∂/∂ a˙ results in the equation of motion 2πaσ02 (1 − ν 2 ) a˙ = − 4γ . M E

(2.73)

Grifﬁth sought the criticality condition at which a˙ = 0. That is, his argument (which was carried out completely differently than we have done here) was to determine the precise condition under which the elastic energy release rate would just compensate for the energy that must be donated to create new free surface. Regardless of the route taken to get the result, this condition results in a critical

2.4 Continuum Descriptions of Deformation and Failure

63

stress for crack initiation of the form σ0crit

=

2Eγ . πa(1 − ν 2 )

(2.74)

Much of the discussion given above can be recast in the language of section 2.3.3. In particular, we see that the question posed above was how does the total potential energy of the system change during incremental crack extension? This may be recast in mathematical form as G=−

∂ E elastic , ∂a

(2.75)

where G is the mechanical energy release rate. The key point to be made presently is the observation that the quantity −∂ E elastic /∂a is exactly the type of conﬁgurational force introduced earlier and, as a result, we may invoke the ideas presented there. In particular, in the fracture context, eqn (2.45) is of such importance it is digniﬁed with a special name, namely, the J -integral and given by ∂u l Ji = W n i − σlm n m ds. (2.76) ∂ xi The integral is framed in the context of a two-dimensional geometry with the contour parameterized by s. The key point is that by evaluating this integral it is possible to reproduce exactly the type of result given in eqn (2.71). For the purposes of the present discussion, there were three main ideas that we wished to put forth concerning fracture. First, we noted that if fracture is imagined to be a homogeneous process in which bonds in the perfect crystal are stretched until they break, this leads to a critical stress for fracture (the ideal tensile strength) known to be completely out of line with experimental values. As a remedy to this paradox, it was realized that ﬂaws such as cracks could have the effect of locally magnifying the remotely applied stress to levels consonant with that needed to break atomic-level bonds. The linear elastic theory of fracture mechanics teaches us how to assess the elastic consequences of these defects, a subject we will return to in chap. 11. Finally, we wished to illustrate how using energetic arguments like those of Grifﬁth, which we have reformulated in the language of conﬁgurational forces and the associated variational principle presented in section 2.3.3, the critical stress for crack initiation may be determined on the basis of microscopic parameters such as the surface energy. It bears emphasizing again that it is particularly interesting how far a linear elastic analysis can take us in evaluating what is an intrinsically nonlinear process.

64

2 Continuum Mechanics Revisited

2.5 Boundary Value Problems and Modeling From the standpoint of the continuum simulation of processes in the mechanics of materials, modeling ultimately boils down to the solution of boundary value problems. What this means in particular is the search for solutions of the equations of continuum dynamics in conjunction with some constitutive model and boundary conditions of relevance to the problem at hand. In this section after setting down some of the key theoretical tools used in continuum modeling, we set ourselves the task of striking a balance between the analytic and numerical tools that have been set forth for solving boundary value problems. In particular, we will examine Green function techniques in the setting of linear elasticity as well as the use of the ﬁnite element method as the basis for numerical solutions.

2.5.1 Principle of Minimum Potential Energy and Reciprocal Theorem In many of the cases in which we resort to the theoretical analysis of a particular problem from a continuum perspective, it will be from the point of view of the linear theory of elasticity. Though we have already introduced the fundamental governing equations of continuum mechanics as well as their linear elastic incarnation, in many instances it will be useful to assign these ideas a variational character. In the context of linear elastic solids, the global principle presiding over equilibrium states (which we assert without proof, for details see Gurtin (1981), for example) is the fact that they are privileged states characterized by the property that they minimize the total potential energy. In particular, in the context of linear elastic boundary value problems, the equilibrium displacement ﬁelds are minimizers of the potential energy functional W ({u i, j })d V − t · ud A − f · ud V, (2.77) [u(x)] =

∂

where the ﬁrst term on the right hand side yields the elastic energy stored in the body, the second term is associated with the potential energy of external loads that are communicated to the body at its surface and the third term provides a measure of the work associated with body forces. The formal statement of the principle is that of all the kinematically admissible ﬁelds (i.e. those ﬁelds that are sufﬁciently smooth and satisfy the displacement boundary conditions), the equilibrium ﬁelds will minimize the functional of eqn (2.77). The importance of this theorem will be especially felt in two separate contexts. First, in a number of instances, it will be most natural to construct models of a given problem which are couched in the language of energetics. In many such instances, the total energy will be parameterized in terms of one or several conﬁgurational coordinates, and the resulting minimization will seek their optimal conﬁguration. The principle

2.5 Boundary Value Problems and Modeling

65

of minimum potential energy will also see action as the basis of many of the approximation strategies that are adopted to solve linear elastic boundary value problems, and in particular, the ﬁnite element method. To illustrate the equivalence of the energy minimization principle advanced above and the linear elastic equilibrium equations of section 2.4.2, we resort to evaluating the functional derivative of eqn (2.77) and setting it equal to zero, or in mathematical terms δ/δu i = 0. Equivalently, working in indicial notation, we ﬁnd 1 1 Ci jkl δi j kl d V + Ci jkl i j δkl d V − f i δu i d V − ti δu i d A. δ = 2 2 ∂ (2.78) Exploiting the symmetries of the elastic modulus tensor and the strain tensor, the ﬁrst two terms may be joined to form σi j δi j d V . Rewriting the integrand σi j δi j as ∂ ∂ δu i = (σi j δu i ) − σi j, j δu i , (2.79) σi j ∂ xj ∂ xj and plugging this result back into the expression given above followed by an application of the divergence theorem leaves us with (σi j n j − ti )δu i d A = 0. (2.80) δ = (σi j, j + f i )δu i d V +

∂

The signiﬁcance of this result emerges once it is recalled that δu i itself is arbitrary except for the fact that δu i = 0 on that part of the boundary for which u is prescribed, and hence that the integrands themselves must vanish. But in the case of the integral over , this results in Ci jkl u k,l j + f i = 0 which is nothing more than the original linear elastic equilibrium equations for a homogeneous material. Further, applying the same reasoning to the surface integrals compels us to accept that σi j n j = ti on that part of the boundary characterized by traction boundary conditions. Again, what all of this means is that there is an equivalence between the original equilibrium equations for linear elasticity and insisting that the potential energy [u(x)] be minimized. As remarked above, in most instances in fact, we will favor the energetic interpretation of equilibrium. In addition to the theoretical advantages offered by the principle of minimum potential energy, our elastic analyses will also be aided by the reciprocal theorem. This theorem is a special example of a more general class of reciprocal theorems and considers two elastic states (u(1) , (1) , σ (1) ) and (u(2) , (2) , σ (2) ), where each state satisﬁes the equilibrium equations and boundary conditions associated with body force ﬁelds f1 and f2 , respectively. The theorem asserts that the work done by the external forces of system 1 on the displacements of system 2 is equal to the work done by the external forces of system 2 on the displacements of system 1.

66

2 Continuum Mechanics Revisited

Mathematically, this is written as t(1) · u(2) d A + f (1) · u(2) d V = ∂

∂

t(2) · u(1) d A +

f (2) · u(1) d V. (2.81)

The signiﬁcance of this result will be appreciated later (for example in section 8.4.2) when we see that it can be used for the construction of fundamental solutions for the elastic displacement ﬁelds of defects such as dislocations. The proof of the reciprocal theorem is based upon two fundamental realizations. First, we note the relation (1) (2) (1) (2) t ·u dA + f · u dV = (1) : C (2) d V. (2.82) ∂

The veracity of this expression can be shown by running the divergence theorem in reverse, basically turning the argument given above to prove the principle of minimum potential energy around. This result in conjunction with the application of symmetries of the tensor of elastic moduli allows us to note (1) : C (2) d V = (2) : C (1) d V. (2.83)

Based on this latter result, the reciprocal theorem is immediate.

2.5.2 Elastic Green Function One of the most powerful means for solving boundary value problems in linear elasticity is that of Green functions. The Green function approach offers the possibility of building up solutions to complex problems on the basis of insights garnered from the solution to the problem of a unit point load. The pivotal assumption exploited in this context is that of linearity which allows us to use the fact that a sum of solutions to a given problem is itself a solution, a result known as the superposition principle. As a result of this principle and a knowledge of the Green function, solutions to generic problems are written as integrals over a kernel provided by the fundamental solution itself. As noted above, the elastic Green function yields the elastic ﬁelds induced by a point load. The ideas here resemble those from the setting of electrodynamics where point sources of charge are the basis of the Green function approach. Recall from earlier that the equilibrium equations that govern the continuum are given by σi j, j + f i = 0,

(2.84)

where σi j is the i j th component of the Cauchy stress and f i are the components of the body force. In the special case of an isotropic linear elastic solid, we have seen that these equations reduce to the Navier equations shown in eqn (2.55).

2.5 Boundary Value Problems and Modeling

67

To construct the elastic Green function for an isotropic linear elastic solid, we make a special choice of the body force ﬁeld, namely, f(r) = f0 δ(r), where f0 is a constant vector. In this case, we will denote the displacement ﬁeld as G ik (r) with the interpretation that this is the i th component of displacement in the case in which there is a unit force in the k th direction, f0 = ek . To be more precise about the problem of interest, we now seek the solution to this problem in an inﬁnite body in which it is presumed that the elastic constants are uniform. In light of these deﬁnitions and comments, the equilibrium equation for the Green function may be written as (λ + µ)

∂2 ∂ ∂ G m j (r) + µ G i j (r) = −δi j δ(r). ∂ xi ∂ xm ∂ xl ∂ xl

(2.85)

Interesting strategies have been adopted for explicitly determining G(r) both in real space as well as Fourier space. Here we follow de Wit (1960) in adopting the Fourier space scheme, leaving the real space solution for the ambitious reader. To ﬁnd the Green function, we exploit our Fourier transform convention: ˜ (2.86) G i j (k) = G i j (r)e−ik·r d 3 r, and G i j (r) =

1 (2π )3

G˜ i j (k)eik·r d 3 k.

(2.87)

Upon Fourier transforming eqn (2.85) as dictated by the deﬁnitions given above, we ﬁnd (2.88) (λ + µ)ki km G˜ m j (k) + µk 2 G˜ i j (k) = δi j , where ki is the i th component of the wavevector k. The k-space Green function can be found by multiplying the previous equation by ki and summing on the repeated index i, which yields the result, km G˜ m j =

kj , (λ + 2µ)k 2

(2.89)

which may be substituted into eqn (2.88). After carrying out the resulting manipulation, the explicit expression for the Green function in Fourier space is

1 (λ + µ) ki k j ˜ δi j − . (2.90) G i j (k) = µk 2 (λ + 2µ) k 2 This result will serve as the cornerstone for many of our developments in the elastic theory of dislocations. We are similarly now in a position to obtain the Green function in real space which, when coupled with the reciprocal theorem, will allow for the determination of the displacement ﬁelds associated with various defects.

68

2 Continuum Mechanics Revisited

Following the procedure used in electrostatics where it is found that the Fourier transform of the Coulomb potential yields a k −2 dependence, we can invert the expression found above rather easily as

δi j xi x j 1 (2.91) (λ + 3µ) + (λ + µ) 3 . G i j (r) = 8π µ(λ + 2µ) r r As a result of these various algebraic machinations, we are now prepared to construct solutions to problems in isotropic elasticity through superposition of the fundamental solution constructed above. The Green function enables us to ﬁnd the displacements at point x given the presence of a point force at point x . However, because of the linearity of the underlying governing equations, the solution for an arbitrary force distribution can be built up as a superposition over a collection of such point forces. That is, we claim that the solution to Ci jkl u k, jl = − f i is u k (x) = G km (x − x ) f m (x )d 3 x . (2.92)

The proof of this claim can be sketched in abstract terms as follows. If we are to write the original governing equation for the displacements as L(x)u(x) = −f(x), where L is the linear operator associated with the various differentiations in the equilibrium equations, then the equation satisﬁed by the Green function may be written as L(x)G(x −x ) = −Iδ(x − x ). Our assertion is that the displacements are given by u(x) = G(x − x )f(x )d 3 x . Application of the operator L to this equation for the displacements results in 3 L(x)u(x) = L(x)G(x − x )f(x )d x = − f(x )δ(x − x )d 3 x = −f(x),

(2.93) demonstrating that when we write the displacements as a convolution inte gral, namely, u(x) = G(x − x )f(x )d 3 x , the original governing equations are satisﬁed. Eqn (2.92) is the culmination of our efforts to compute the displacements due to an arbitrary distribution of body forces. Although this result will be of paramount importance in coming chapters, it is also important to acknowledge its limitations. First, we have assumed that the medium of interest is isotropic. Further reﬁnements are necessary to recast this result in a form that is appropriate for anisotropic elastic solids. A detailed accounting of the anisotropic results is spelled out in Bacon et al. (1979). The second key limitation of our result is the fact that it was founded upon the assumption that the body of interest is inﬁnite in extent. On the other hand, there are a variety of problems in which we will be interested in the presence of defects near surfaces and for which the half-space Green function will be needed. Yet another problem with our analysis is the assumption that the elastic constants

2.5 Boundary Value Problems and Modeling

69

Fig. 2.13. Four schematic examples of eigenstrains: (a) spherical inclusion, (b) eigenstrain due to thermal expansion, (c) dislocation loop and (d) eigenstrain due to wedge of martensite.

are the same throughout the material. On the other hand, when it comes time (see chap. 10) to investigate the elastic consequences of second-phase particles, the moduli of the inclusion can differ from those of the matrix, and again, the particulars (though not the concept) of our Green function analysis will have to be amended.

2.5.3 Method of Eigenstrains A very powerful technique in conjunction with that of elastic Green functions is the method of eigenstrains. The eigenstrain concept allows us to solve elasticity problems for a continuum with internal heterogeneities such as dislocations or inclusions, by replacing these heterogeneities by effective body force ﬁelds. An eigenstrain is deﬁned as a strain without any attendant internal stresses. The deﬁnition is abstract without the clariﬁcation afforded by particular examples. In ﬁg. 2.13, we show four distinct examples of elastic media in the presence of eigenstrains. For example, as shown in ﬁg. 2.13(a), an inclusion may be characterized by a strain i∗j which carries the information about how the inclusion differs structurally from the matrix material. In addition, we should note that in the absence of the constraining effect provided by the matrix, the eigenstrain i∗j has

70

2 Continuum Mechanics Revisited

Fig. 2.14. Energy as a function of shear for a generic crystalline solid. The periodicity of the energy proﬁle reﬂects the existence of certain lattice invariant shears which correspond to the ‘stress-free strains’ considered in the method of eigenstrains (adapted from Tadmor et al. (1996)).

no associated stress. Similarly, as shown in ﬁg. 2.13(b), if a crystal is to undergo thermal expansion, the associated strains can be thought of as eigenstrains since they imply no internal stresses. Dislocations can also be characterized in terms of eigenstrains since the region of the crystal that has slipped (see ﬁg. 2.13(c)) has suffered a lattice invariant shear. In ﬁg. 2.13(d) we imagine the case of a solid, part of which has undergone a phase transformation. Like in the inclusion example introduced above, the phase transformed region is characterized by an eigenstrain. Further insights into the eigenstrain concept can be obtained on the basis of energetic arguments. We imagine an energy landscape which characterizes the energy of the continuum as a function of the relevant kinematic measure such as the strain. In many cases of interest, the energy landscape is nonconvex, with different wells corresponding to different structural alternatives. The eigenstrain concept allows for the emergence of structures in which one part of the continuum corresponds to one well in the energy landscape while some other part of the continuum corresponds to a different well. In computing stresses, we appeal not to the total strain, but rather the departure of the strain from the well of interest. In many problems, different parts of the body are characterized by different eigenstrains. Clearly, in making a transition from one eigenstrain to another, speciﬁc regions will not be associated with a well in the energy landscape, and it is largely these incompatibilities that give rise to internal stresses. A concrete example of these energetic arguments can be made through consideration of simple shear. In generic terms, if a particular crystal is subject to a monotonically increasing shear, the energy as a function of this shear will have qualitative features such as those shown in ﬁg. 2.14. The existence of the periodicity in the energy

2.5 Boundary Value Problems and Modeling

71

proﬁle reﬂects the fact that there exist certain lattice invariant shears that map the Bravais lattice onto itself. The fundamental idea of the method of eigenstrains is the argument that if the system is sheared such that it occupies one of the minimum energy wells, there will be no associated stress. In mathematical terms, the implementation of the eigenstrain concept is carried out by representing the geometrical state of interest by some distribution of ‘stress-free strains’ which can be mapped onto an equivalent set of body forces, the solution for which can be obtained using the relevant Green function. To illustrate the problem with a concrete example, we follow Eshelby in thinking of an elastic inclusion. The key point is that this inclusion is subject to some internal strain i∗j , such as arises from a structural transformation, and for which there is no associated stress. The outcome of the hypothesis advanced above is that the stress is computed as ∗ σi j = Ci jkl (u tot k,l − kl ),

(2.94)

where u tot k,l is the displacement gradient of the total displacement ﬁeld. Note that the physical meaning of this equation corresponds to our statement above that it is only the departure of the strain from the nearest energy well that leads to the generation of stresses, and not the total strain. The imposition of the condition of equilibrium, namely, σi j, j = 0 in this context is then equivalent to ∗ Ci jkl u tot k,l j = C i jkl kl, j .

(2.95)

Since the eigenstrain itself is prescribed, eqn (2.95) can be interpreted as corresponding to a homogeneous elastic body, now in the presence of an effective body eff ∗ force f i = −Ci jkl kl, j . Note that in the context of the effective theory concept which we will return to repeatedly throughout this book, the eigenstrain idea allows us to replace some heterogeneity within a continuum by a series of effective body forces resulting in a tractable (sometimes) elasticity problem. As a result of the deﬁnition of the effective body force ﬁeld, the Green function machinery elucidated above may be exploited. In particular, recall eqn (2.92) which expresses the displacement ﬁelds as an integral over the force distribution. In the present setting, the unknown displacements may be written as a convolution integral of the elastic Green function and the effective body force distribution as ∗ u k (x) = − G km (x − x )Cmrst st,r (x )d 3 x . (2.96)

Of course, there are a number of manipulations (integration by parts, for example) that can be carried out in order to restate this result in a more convenient fashion. On the other hand, our intention at this point is to introduce the conceptual framework, and to reserve the explicit use of the method of eigenstrains until later.

72

2 Continuum Mechanics Revisited

2.5.4 Numerical Solutions: Finite Element Method Despite the existence of powerful analytical tools that allow for explicit solution of certain problems of interest, in general, the modeler cannot count on the existence of analytic solutions to most questions. To remedy this problem, one must resort to numerical approaches, or further simplify the problem so as to reﬁne it to the point that analytic progress is possible. In this section, we discuss one of the key numerical engines used in the continuum analysis of boundary value problems, namely, the ﬁnite element method. The ﬁnite element method replaces the search for unknown ﬁelds (i.e. the solutions to the governing equations) with the search for a discrete representation of those ﬁelds at a set of points known as nodes, with the values of the ﬁeld quantities between the nodes determined via interpolation. From the standpoint of the principle of minimum potential energy introduced earlier, the ﬁnite element method effects the replacement [u(x)] → ({ui }),

(2.97)

where [u(x)] is a functional of the unknown displacement ﬁelds and ({ui }) is a function of a discrete set of nodal displacements indexed by the integer i which runs from 1 to N , where N is the number of nodes. We note that the ﬁnite element method is in no way restricted to elasticity problems, but that such problems will serve as a convenient vehicle for our discussion. The central ideas associated with the ﬁnite element approach may be summarized as follows. First, the original boundary value problem is stated in weak form (i.e. the relevant partial differential equations are restated in integral form). Next, the continuum is parceled up into discrete regions known as elements, with the unknown ﬁeld variables considered at the points of intersection of these elements known as nodes. The net result of this discretization is that we have now replaced a problem in which we are searching for an unknown function u(x) with a search for discrete set of 3N variables {ui } (i.e. the three components of displacement for each of the N nodes). One crucial observation at this juncture is that the elements need not be uniform, thereby allowing for mesh design in which near rapidly varying parts of the solution, one uses high resolution, while in regions of slow variation larger elements can be supported. From the perspective of variational principles, the idea embodied in the ﬁnite element approach is similar to that in other schemes: identify that particular linear combination of basis functions that is ‘best’ in a sense to be deﬁned below. The approximate solution of interest is built up as linear combinations of basis functions, and the crucial question becomes how to formulate the original boundary value problem in terms of the relevant expansion coefﬁcients.

2.5 Boundary Value Problems and Modeling

73

Fig. 2.15. Replacement of a continuous body with a set of ﬁnite elements. In this case, the unknown displacement ﬁeld has been replaced by a discrete set of unknown nodal displacements, un .

Recall that within the continuum mechanics setting set forth in section 2.3.2, the equations of equilibrium may be written as σi j, j + f i = 0.

(2.98)

Our present task is to rewrite these equations in integral (or weak) form which will simplify the formulation in terms of ﬁnite elements. We introduce a series of ‘test functions’ wi (x) that satisfy the relevant displacement boundary conditions which are hence denoted as admissible ﬁelds and now contract these test functions with the equation given above and integrate over the spatial region of interest. This strategy results in wi σi j, j d V + wi f i d V = 0. (2.99)

If we now use integration by parts on the ﬁrst term in this equation, we are left with wi, j σi j d V = ti wi d A + f i wi d V, (2.100)

∂

where we have used ti = σi j n j . As yet, our exercise corresponds to nothing more than a statement of the principle of virtual work. On the other hand, if we now proceed with the concrete consideration of the test functions wi (x), it is possible to construct a numerical framework. As yet, our statements have been general and do not reﬂect our wish to replace the continuous problem with a discrete analog. We now imagine that the body is discretized into a set of elements which meet at vertices denoted as nodes and indicated in ﬁg. 2.15. Within each element, the value of the displacement is

74

2 Continuum Mechanics Revisited

Fig. 2.16. Schematic illustration of the three triangular shape functions tied to the different nodes of a triangular element.

obtained via interpolation according to u(x) = ui Ni (x),

(2.101)

i

where the subscript i refers to nodes and Ni (x) is the ‘shape function’ attached to the i th node and deﬁned through Ni (x j ) = δi j . That is, the i th shape function is 1 at the i th node and vanishes at neighboring nodes. These shape functions are illustrated in ﬁg. 2.16 in the case of linear triangular elements. In essence what we are saying is that the solution is determined at a discrete set of nodal values, and if we interest ourselves in the solution elsewhere, it is to be determined by interpolation in terms of those nodal values via a series of interpolation functions which are commonly referred to as shape functions. If we substitute the interpolated displacements as denoted above into the integral statement of the equilibrium equations, and furthermore, we take as our test functions the Ni s themselves (i.e. wi (x) = Ni (x)), we ﬁnd a series of equations in the unknown coefﬁcients of the form Ku = f,

(2.102)

where K is known as the stiffness matrix (and for nonlinear problems can depend upon u itself) and f is the force matrix. To make the treatment given above more than just an abstraction, we now consider the case of one-dimensional elasticity. We imagine our one-dimensional elastic medium to have length a and to be characterized by an elastic stiffness k. The traction vector, t (x), is directly related to the gradients in displacements by t = kdu/d x. Our weak statement of the equilibrium equations may be written as a a dw du dx = k f wd x + [t (a)w(a) − t (0)w(0)]. (2.103) dx dx 0 0 At this point, we are primarily confronted with a series of algebraic manipulations founded upon the ﬁnite element edicts described above. First, we approximate the solution u(x) in terms of the ﬁnite element shape functions, u(x) = i u i Ni (x). Secondly, we make the correspondence between the test functions w(x) and the

2.6 Difﬁculties with the Continuum Approach

75

shape functions themselves. For example, the equation resulting from the assertion w(x) = N j (x) is a a d N j (x) d Ni (x) dx = ui k f (x)N j (x)d x + [t (a)N j (a) − t (0)N j (0)]. dx dx 0 0 i (2.104) This equation may now be rewritten as K ji u i = f j (2.105) i

if we make the correspondence

K ji =

k 0

a

d N j (x) d Ni (x) d x, dx dx

(2.106)

a

fj =

f (x)N j (x)d x + [t (a)N j (a) − t (0)N j (0)].

(2.107)

0

The result of this analysis is a series of coupled algebraic equations in the unknown nodal displacements. For the linear problem we have considered here, these equations are themselves linear (though they are not in general) and our problem reduces to little more than diagonalization of the relevant stiffness matrix which, as seen above, can be computed as products of material parameters and geometric factors. In this section, we have seen how one may formulate numerical strategies for confronting the types of boundary value problems that arise in the continuum description of materials. The key point is the replacement of the problem involving unknown continuum ﬁelds with a discrete reckoning of the problem in which only a discrete set of unknowns at particular points (i.e. the nodes) are to be determined. In the next chapter we will undertake the consideration of the methods of quantum mechanics, and in this setting will ﬁnd once again that the ﬁnite element method offers numerical ﬂexibility in solving differential equations. 2.6 Difﬁculties with the Continuum Approach One of the key beneﬁts provided by the types of approaches advocated in this chapter is that the mathematics associated with solving for three unknown ﬁelds (for example) is more sympathetic than that of solving coupled ordinary differential equations in a number of variables of Avogradrian dimensions. On the other hand, continuum approaches have their disadvantages as well. We have noted earlier that one of the primary difﬁculties tied to the use of continuum models is their reliance on constitutive assumptions. In some instances, we will see that the constitutive models adopted are often selected as much for their theoretical convenience as

76

2 Continuum Mechanics Revisited

for their phenomenological realism. It is on these grounds that we will appeal to microscopic theories as the proper basis for informing higher-level constitutive strategies. A second difﬁculty that attends the use of continuum models is the fact that such models are indifferent to the presence of a minimum length scale as dictated by the typical separation between atoms. This absence of small scale resolution within the continuum framework can have a souring inﬂuence on the success of such theories in predicting features in the immediate vicinity of defects. One of our main objectives will be to show how, via the device of incorporating nonlinear information into our models, many of these difﬁculties may be sidestepped. As a result of the evident appeal of microscopic insights into the ultimate origins of continuum behavior, in the next chapter we undertake a review of the theoretical foundations of microscopic modeling, the partnership of quantum and statistical mechanics.

2.7 Further Reading Continuum Mechanics Continuum Mechanics by P. Chadwick, Halsted Press, New York: New York, 1976. My personal favorite, Chadwick’s book is direct and to the point, and full of clever insights and interesting examples. An Introduction to Continuum Mechanics by M. Gurtin, Academic Press Inc., San Diego: California, 1981. Gurtin’s book is a classic among solid mechanicians and gives a thorough treatment of much of the material found in the present chapter. ‘Mechanics of Solids’ by J. R. Rice in Encyclopedia Britannica Vol. 23, pg. 734 (1993) is an outstanding overview of the entire realm of solid mechanics, giving coverage not only of the principles of continuum mechanics, but also their applications to deformation and fracture with interesting historical and philosophic commentary. Nonlinear Continuum Mechanics for Finite Element Analysis by J. Bonet and R. D. Wood, Cambridge University Press, Cambridge: England, 1997. This book provides an interesting discussion of many of the concepts discussed in the present chapter and includes commentary on the numerical implementation of these same concepts. Mathematical Theory of Elasticity by I. S. Sokolnikoff, Krieger Publishing Company, Malabar: Florida, 1983. One of the classic texts on elasticity theory. Theory of Elasticity by S. P. Timoshenko and J. N. Goodier, McGraw Hill Book

2.7 Further Reading

77

Company, New York: New York, 1970. My personal taste for this book is founded on the fact that it is full of solutions to elasticity problems of interest. Theory of Elasticity by L. D. Landau and E. M. Lifshitz, Pergamon Press, Oxford: England, 1970. Written in the terse style that the Landau and Lifshitz series is famous for, the book is full of solutions and insights. Micromechanics of Defects in Solids by T. Mura, Kluwer Academic Publishers, Dordrecht: The Netherlands, 1993. Mura’s book is a neglected classic which features an enormous number of examples on the use of Green functions in conjunction with the method of eigenstrains. Plasticity The Mathematical Theory of Plasticity by R. Hill, Clarendon Press, Oxford: England, 1967. The deﬁnitive work on the mathematical theory of plasticity. This book goes well beyond our treatment regarding continuum descriptions of plasticity without entering into the question of how plasticity emerges as the result of defect motion. Continuum Theory of Plasticity by A. S. Khan and S. Huang, John Wiley and Sons, New York: New York, 1995. The subject of plasticity is lacking in texts that are directed at interpreting plastic deformation on the basis of the underlying mechanisms. This book provides an overview of much of the machinery that is invoked in current considerations of plasticity. Fracture ‘Mathematical Analysis in the Mechanics of Fracture’ by James R. Rice, from Vol. II of Fracture edited by G. Sih, Academic Press, New York: New York, 1968. Rice’s account of fracture remains, in my opinion, one of the deﬁnitive statements of many of the key ideas in the subject. Section E on Energy Variations and Associated Methods is especially pertinent to our discussion on conﬁgurational forces and gives an in depth application of these ideas in the fracture context. Dynamic Fracture Mechanics by L. B. Freund, Cambridge University Press, Cambridge: England, 1990. A careful account of many of the fundamental ideas of interest in the analysis of fracture with special reference to dynamics. Fracture of Brittle Solids by Brian Lawn, Cambridge University Press, Cambridge: England, 1993. I have found Lawn’s book quite readable and a useful place to become acquainted not only with much of the phenomenology of fracture, but also with some of the key ideas in that ﬁeld. Elementary Engineering Fracture Mechanics by D. Broek, Martinus Nijhoff

78

2 Continuum Mechanics Revisited

Publishers, The Hague: Holland, 1982. A readable account of many of the central ideas in the analysis of fracture.

The Finite Element Method The Finite Element Method by T. J. R. Hughes, Prentice Hall Inc., Englewood Cliffs: New Jersey, 1987. An exhaustive coverage of the mathematical formalism of ﬁnite elements. Computational Differential Equations by K. Eriksson, D. Estep, P. Hansbo and C. Johnson, Cambridge University Press, Cambridge: England, 1996. A wonderful book with many interesting historical sidelights that describes the numerical tools that arise in the solution of boundary value problems using continuum mechanics. A First Course in the Numerical Analysis of Differential Equations by A. Iserles, Cambridge University Press, Cambridge: England, 1996. This book, especially in the later chapters, treats many of the numerical issues of interest to those practicing ﬁnite elements. An Introduction to the Finite Element Method by J. N. Reddy, McGraw-Hill, New York: New York, 1993. A readable introduction to the conceptual foundations of the ﬁnite element method.

2.8 Problems

1 Deformation Gradient and Volume Change An additional insight into the signiﬁcance of the deformation gradient tensor can be gleaned by evaluating the scalar triple product of three noncoplanar vectors a, b and c both before and after a homogeneous deformation. In the undeformed conﬁguration, the vectors a, b and c span a region whose volume is given by a · (b × c). In the deformed conﬁguration, the transformed region has a volume given by Fa · (Fb × Fc). Show that the reference and deformed volumes are related by Fa · (Fb × Fc) = (det F)a · (b × c).

(2.108)

Interpret this result and demonstrate that for a pure shear there is no volume change.

2.8 Problems

79

2 Finite and Inﬁnitesimal Strains Consider a deformation mapping that is nothing more than a rigid rotation about the z-axis. First, explicitly write down the deformation mapping and then compute both the Green strain and the inﬁnitesimal strain tensors associated with this deformation mapping. In general, the inﬁnitesimal strains are nonzero. Why? 3 Cauchy Tetrahedron and Equilibrium In this problem, use the balance of linear momentum to deduce the Cauchy stress by writing down the equations of continuum dynamics for the tetrahedral volume element shown in ﬁg. 2.7. Assign an area S to the face of the tetrahedron with normal n and further denote the distance from the origin to this plane along the direction n by h. Show that the dynamical equations may be written as Dv V. (2.109) t(n) S + fV − t(e1 ) S1 − t(e2 ) S2 − t(e3 ) S3 − = ρ Dt Rewrite S1 , S2 , S3 and V in terms of S, h and the components of the vector n normal to S and then evaluate the limiting value of the expression given above as h → 0. Now, by adopting the convention that the traction vector on the i th Cartesian plane can be written as t(ei ) = σ ji e j ,

(2.110)

show that t(n) = σ n. 4 Isotropic Elasticity and Navier Equations Use the constitutive equation for an isotropic linear elastic solid given in eqn (2.54) in conjunction with the equilibrium equation of eqn (2.84), derive the Navier equations in both direct and indicial notation. Fourier transform these equations and verify eqn (2.88). 5 Elastic Green Function for an Isotropic Solid The elastic Green function is a useful tool in the analysis of a variety of problems in the elasticity of defects in solids. In this problem, we consider the various steps in the derivation of the elastic Green function for an inﬁnite, isotropic solid. In particular, ﬂesh out the details involved in the derivation of eqn (2.90) and carry out the Fourier inversion to obtain eqn (2.91).

80

2 Continuum Mechanics Revisited

6 Displacements for an Elastic Inclusion using the Method of Eigenstrains Consider a spherical inclusion characterized by an eigenstrain i∗j = δi j . (a) For an isotropic linear elastic solid, write the effective body forces associated with this eigenstrain. (b) Use the effective body force derived in part (a) in conjunction with eqn (2.96) to obtain an integral representation for the displacements due to the spherical inclusion. 7 Airy Stress Function and the Biharmonic Equation The biharmonic equation in many instances has an analogous role in continuum mechanics to that of Laplace’s equation in electrostatics. In the context of two-dimensional continuum mechanics, the biharmonic equation arises after introduction of a scalar potential known as the Airy stress function φ such that ∂ 2φ , ∂ x22 ∂ 2φ σ22 = 2 , ∂ x1 ∂ 2φ . σ12 = − ∂ x1 ∂ x2 σ11 =

(2.111) (2.112) (2.113)

Given this deﬁnition of the Airy stress function, show that the equilibrium equations are satisﬁed. The compatibility condition for inﬁnitesimal strains for planar problems may be written as ∂ 2 yy ∂ 2 x y ∂ 2 x x . (2.114) + = 2 ∂ y2 ∂x2 ∂ x∂ y Compatibility conditions address the fact that the various components of the strain tensor may not be stated independently since they are all related through the fact that they are derived as gradients of the displacement ﬁelds. Using the statement of compatibility given above, the constitutive equations for an isotropic linear elastic solid and the deﬁnition of the Airy stress function show that the compatibility condition given above, when written in terms of the Airy stress function, results in the biharmonic equation ∇ 4 φ = 0.

THREE

Quantum and Statistical Mechanics Revisited

3.1 Background In the previous chapter we examined the central tenets of continuum mechanics with an eye to how these ideas can be tailored to the modeling of the mechanical properties of materials. During our consideration of continuum mechanics, we found that one of the key features of any continuum theory is its reliance on some phenomenological constitutive model which is the vehicle whereby mechanistic and material speciﬁcity enter that theory. As was said before, the equations of continuum dynamics are by themselves a continuous representation of the balance of linear momentum and make no reference to the particulars of the material in question. It is the role of the constitutive model to inform the equations of continuum dynamics whether we are talking about the plastic deformation of metals or the washing of waves across a beach. A key realization rooted in the microscopic perspective is the idea that the constitutive response, used in the continuum settings described in the previous chapter, reﬂects a collective response on the part of the microscopic degrees of freedom. It is the business of quantum and statistical mechanics to calculate the average behavior that leads to this collective response. In addition to our interest in effective macroscopic behavior, one of our primary aims is to produce plausible microscopic insights into the mechanisms responsible for observed macroscopic behavior. For example, is there a microscopic explanation for the difference in the Young’s modulus of lead and silicon? Or, under what conditions might one expect to see creep mediated by grain boundary diffusion as opposed to bulk diffusion? Or, how does the yield strength depend upon the concentration of some alloying element? As noted above, microscopic modeling is founded upon the two complementary ediﬁces of quantum and statistical mechanics. From the present perspective, quantum mechanics allows us to capture the electronic origins of many of the internal energy differences that accompany processes central to the mechanics of 81

82

3 Quantum and Statistical Mechanics Revisited

materials. Similarly, statistical mechanics provides a venue within which it is possible to effect a quantitative treatment of the many degrees of freedom that conspire to yield observed macroscopic response. Our purpose in this chapter is to revisit some of the key ideas associated with these two disciplines, with emphasis on features of these theories that will ﬁnd their way into our later thinking.

3.2 Quantum Mechanics Quantum mechanics is the appropriate fundamental theory for describing phenomena ranging from bonding in fullerenes to superconductivity to the behavior of neutron stars. For our purposes, quantum mechanics should be seen in its role as the theory which describes the electronic origins of bonding in solids. In many cases, it is found that the very existence of solids is the result of a collective response on the part of the electronic degrees of freedom. In particular, the free energy is lower when the atoms conspire to form a solid than when they remain in isolation, and a key contribution to the total free energy arises from the electronic degrees of freedom. In the previous chapter, we noted that the principle of linear momentum balance leads to the central ‘governing equation’ of continuum mechanics. Similarly, within the context of nonrelativistic quantum mechanics, there is another such governing equation, namely that of Schr¨odinger. Though the conceptual origins of the Schr¨odinger equation are tied to a long and fascinating history, here we opt for the axiomatic approach in which the governing equation is asserted without derivation and is instead queried for its implications.

3.2.1 Background and Formalism Quantum mechanics represents one of the cornerstones of modern physics. Though there were a variety of different clues (such as the ultraviolet catastrophe associated with blackbody radiation, the low-temperature speciﬁc heats of solids, the photoelectric effect and the existence of discrete spectral lines) which each pointed towards quantum mechanics in its own way, we will focus on one of these threads, the so-called wave-particle duality, since this duality can at least point us in the direction of the Schr¨odinger equation. Though classical electromagnetic theory as embodied in Maxwell’s equations led to an interpretation of light in terms of waves, the photoelectric effect inspired Einstein to the view that in its interactions with matter, light might be better thought of from a corpuscular perspective. A complementary view of matter which took quantitative form in the hands of de Broglie was the contention that in some cases matter should be thought of in wave-like terms. In most naive

3.2 Quantum Mechanics

83

terms, the idea is that one should attribute a wavelength λ = h/ p to a particle with momentum p, where h is Planck’s constant. Indeed, the discovery that electrons form interference patterns provided further impetus towards the discovery of a mathematical description of these ‘matter waves’. Schr¨odinger was inspired by an analogy between classical mechanics and the ray theory of light, and hoped that a mechanics could be found that would stand in the same relation to wave optics that classical mechanics does to ray optics. The result of this inspiration is the famed Schr¨odinger equation. This equation determines the features of the electronic wave function, ψ(r). In turn, the wave function itself has a kinematic character and serves to characterize the ‘state’ of the system. A convenient analogy is that the wave function characterizes the state of a system within the quantum framework in a fashion that is analogous to the way that the coordinates and momenta characterize the state of a system within classical mechanics. Just as in classical descriptions, once the coordinates {qi , pi } are determined, all observables that depend upon those coordinates can be evaluated, so too in quantum mechanics, once the wave function is determined, there are well-deﬁned prescriptions for determining the expected values of quantities of interest. The interpretation of the wave function (here given in the one-dimensional setting, though the generalization to higher dimensions is clear) is that |ψ(x)|2 d x = ψ ∗ (x)ψ(x)d x is the probability that a particle will be found between x and x + d x. Note that we have introduced the notation ψ ∗ (x) which instructs us to use the complex conjugate of the wave function ψ(x). When written in time-independent form for a single particle interacting with a potential V (r), the Schr¨odinger equation takes the form −

h¯ 2 2 ∇ ψ(r) + V (r)ψ(r) = Eψ(r). 2m

(3.1)

The quantity E is the energy eigenvalue associated with a given wave function, while m is the mass of the particle of interest. In its role as the governing equation of quantum systems, the Schr¨odinger equation for a given problem amounts to the solution of a boundary value problem. Depending upon the nature of the potential V (r) that the particle experiences and the associated boundary conditions, one ﬁnds different solutions ψn (r) with associated stationary energy states, E n . Unlike the governing equations of continuum mechanics, these solutions involve a fundamental physical parameter with dimensions of action, namely, Planck’s constant, which is denoted here by h¯ = h/2π . Later we will see that Planck’s constant sets the energy scale of interest for many problems relating to electrons in solids. As noted above, the Schr¨odinger equation yields not only the electronic wave functions, but also the spectrum of energy eigenvalues E n which are available to the system. These eigenvalues, in turn, are the basis for the determination of the

84

3 Quantum and Statistical Mechanics Revisited

total energy of the system, whether it be an atom, a molecule or a solid. It is upon reckoning the relative distributions of eigenvalues for different conﬁgurations that we can construct a picture of why some conﬁgurations are more favorable than others. For example, if our aim is to determine the ground state geometry of a particular molecule, this question can be unambiguously answered by comparing the total energies of the geometric alternatives. The relation between a given classical Hamiltonian and its quantum counterpart depends upon the transcription between classical dynamical variables and certain operators that act upon the space of wave functions. The basic idea is to take the classical Hamiltonian, replace the relevant dynamical variables by their operator analogs, and then to solve the resulting differential equation, Hˆ ψ = Eψ.

(3.2)

This equation is a restatement of eqn (3.1) and we have introduced the notation that aˆabove a quantity signals that quantity as an operator. Note that we are considering the time-independent setting and for now have made reference only to a single particle. To make the classical–quantum transcription more complete, the recipe is to replace classical dynamical variables by their operator analogs according to p → −i h¯ ∇

(3.3)

r → r.

(3.4)

and

The Schr¨odinger equation corresponding to a given classical Hamiltonian is then obtained by replacing all of the dynamical variables in the original Hamiltonian with their operator analogs. With our realization that dynamical variables are represented as operators, we can also raise the question of how to compute observed quantities within the framework of quantum mechanics. The essential rule is that if we are interested ˆ p) when the system is in in obtaining the expectation value of the operator O(r, the state ψ, then this is evaluated as ˆ ˆ p) = ψ| O|ψ ˆ (3.5) O(r, = d 3 rψ ∗ (r) Oψ(r). Here we have introduced the bra (ψ|) and ket (|ψ) notation of Dirac which for us will serve as a shorthand way of representing certain integrals. This assertion is of special importance in our enterprise in the context of the energy for which the relevant expectation value may be written ˆ E = ψ| H |ψ = d 3 rψ ∗ (r) Hˆ ψ(r). (3.6)

3.2 Quantum Mechanics

85

Indeed, one sense in which this expression will be seen again is in its role as the basis of variational approximations for the wave function. Rather than solving for ψ itself, our idea will be to represent it as a linear combination of some set of basis functions, and to choose the coefﬁcients in the linear combination that minimize E. To explicitly solve a problem using the machinery of quantum mechanics, one speciﬁes the potential experienced by the particle within the Schr¨odinger equation which results in a corresponding boundary value problem. Upon solving this problem one ﬁnds the spectrum of allowed energy eigenvalues. The paradigmatic example of this program is the hydrogen atom, wherein one speciﬁes the Coulombic potential that characterizes the interaction between the nucleus and the electron and ﬁnds that the energy eigenvalues are consonant with the well-known Balmer formula of nineteenth century spectroscopy. In addition to the hydrogen problem, there are a variety of model problems that can also be solved analytically. For less tractable problems one can resort to perturbative treatments wherein more complicated potentials can be treated systematically. In the sections that follow, we undertake the solution of a few of these problems that are of particular interest in our attempt to build plausible models of material behavior. Not only will these models illustrate the fundamental concepts of quantum mechanics, but they will indeed prove useful in our quest to build models of materials. As a quick example to set notation and illustrate a few more points concerning formalism, we consider the problem of a single particle in a one-dimensional box. In this problem, the potential that acts on the particle is of the form 0 if 0 < x < a V (x) = (3.7) ∞ otherwise. If we like, we can think of this potential as the simplest model of the conﬁning effect of a free surface. The meaning of the potential is that the particle is ‘bound’ to the region 0 < x < a. As a result, all that we really need do is solve the equation −

h¯ 2 d 2 ψ = Eψ(x), 2m d x 2

(3.8)

subject to the boundary condition ψ(0) = ψ(a) = 0. These boundary conditions guarantee that the probability of ﬁnding the particle outside of the box is zero. By inspection, the solutions are of the form πnx 2 sin , (3.9) ψn (x) = a a a √ where the constant 2/a is chosen to guarantee that 0 |ψ(x)|2 d x is normalized to unity for reasons that we will see shortly and n is an integer that insures that

86

3 Quantum and Statistical Mechanics Revisited

Fig. 3.1. Ground state and ﬁrst excited state wave functions associated with particle in a box problem. The wave functions are drawn such that their zeroes correspond to the energy of the corresponding state.

the boundary conditions are satisﬁed. In addition to the wave functions, the energy eigenvalue corresponding to the n th wave function is En =

h¯ 2 π 2 n 2 . 2ma 2

(3.10)

The ground state and ﬁrst excited state wave functions for this problem are shown in ﬁg. 3.1. Each wave function has been plotted such that the zeroes of the wave function occur at the value on the vertical energy axis corresponding to that particular state. Thus, in the dimensionless units favored in the ﬁgure, ψ1 (x) has an energy E 1 = 1, while ψ2 (x) is associated with the energy E 2 = 4. As yet, our quick tour of quantum mechanics has featured the key ideas needed to examine the properties of systems involving only a single particle. However, if we are to generalize to the case in which we are asked to examine the quantum mechanics of more than one particle at a time, there is an additional idea that must supplement those introduced above, namely, the Pauli exclusion principle. This principle is at the heart of the regularities present in the periodic table. Though there are a number of different ways of stating the exclusion principle, we state it in words as the edict that no two particles may occupy the same quantum state. This principle applies to the subclass of particles known as fermions and characterized by half-integer spin. In the context of our one-dimensional particle in a box problem presented above, what the Pauli principle tells us is that if we wish to

3.2 Quantum Mechanics

87

put two electrons in the box, then in reckoning the total energy we say that one of the particles occupies the ground state and the second occupies the ﬁrst excited state with a resulting total energy E tot = E 1 + E 2 = 5, where the energy is written in the dimensionless units already introduced in ﬁg. 3.1. We confess to ignoring the extra subtleties associated with an explicit inclusion of spin.

3.2.2 Catalog of Important Solutions The solutions to a few different problems within the quantum mechanical setting will serve as the backdrop for many of the models of materials that will be set forth in later chapters. The quantum mechanical oscillator will serve as our jumping off point for the analysis of the thermodynamics of solids, while the solution to the problem of the hydrogen atom will give us a basis within which to discuss bonding in solids. Consequently, we take up the solution of these problems presently. Harmonic Oscillator. One exercise that proves central to modeling the thermal properties of materials is that of a particle bounded by a quadratic potential well. Our interest in the harmonic oscillator arises from the following observation. The particles that make up an N -atom solid may be thought of as spanning a 3N -dimensional conﬁguration space with the potential energy of interaction given by U (x 1 , x2 , . . . , x3N ). This function gives the potential energy of a given atomic conﬁguration, and regardless of the exact details of the potential energy surface, one may imagine representing this surface in the vicinity of points of equilibrium in terms of a collection of quadratic wells. It is on this basis that the harmonic oscillator serves as a jumping off point for an analysis of the vibrations of solids and reveals itself as of special interest to the modeling of materials. In anticipation of our use of this model in chaps. 5 and 6, we recount the quantum mechanical treatment of a particle in a quadratic potential. For the case of the one-dimensional harmonic oscillator the potential energy is given by V (x) = 12 kx 2 , which is parameterized in terms of a stiffness constant k. After some manipulation, the Schr¨odinger equation associated with this potential may be written as d 2ψ + (α − βx 2 )ψ = 0, dx2

(3.11)

where α = 2m E/h¯ 2 and β = m 2 ω2 /h¯ 2 , and with the constant ω2 = k/m corresponding to the classical frequency of vibration. Equations of this generic form suggest a rescaling of the variables motivated by the attempt to isolate the term quadratic in x. In particular, this equation can be further simpliﬁed if we 1 make the change of variables y = β 4 x which results in a restatement of the original

88

3 Quantum and Statistical Mechanics Revisited

Schr¨odinger equation in terms of natural coordinates as 2E d 2φ 2 − y φ = 0, + h¯ ω dy 2

(3.12)

where we have deﬁned a new function φ(y) which reﬂects the change of variables. 2 Asymptotic analysis suggests a trial solution of the form φ(y) = f (y)e−y /2 . 2 This form is suggested by the fact that e−y /2 satisfactorily describes the large-y behavior of the solution, namely, that the particle is bound within the quadratic well. Substitution of this trial solution into the original differential equation results in an auxiliary equation for the unknown function f (y). In particular, we ﬁnd 2E − 1 f (y) = 0. (3.13) f (y) − 2y f (y) + h¯ ω The details of the solution to this equation are of less immediate interest to us than the nature of the solutions themselves. Sufﬁce it to note that this equation admits of a solution in power series form, and that these solutions guarantee the vanishing of the wave function as y → ∞ only if the series is truncated after a ﬁnite number of terms. This large y boundary condition meets with our intuition that the solutions must ultimately vanish at large distances. That is, we expect the particle to be bound by the oscillator potential. The polynomials that result upon truncating the series are the so-called Hermite polynomials. Our requirement that the series solution be truncated after a ﬁnite number of terms is imposed by insisting that 2E = 2n + 1, (3.14) h¯ ω where n is an integer. Imposition of the boundary condition results in quantization of the allowed energy levels which can be labeled as E n = (n + 12 )h¯ ω. Note that even for the ground state (n = 0), the energy is nonzero (the so-called zero point energy). The wave functions that are associated with these various energies are themselves labeled by the integer n (n is known as a quantum number) and can be written as 1 mω 4 − mωx 2 1 mω 2h¯ H e x , (3.15) ψn (x) = n n 1 h¯ 2 2 (n!) 2 π h¯ where Hn (x) is a Hermite polynomial of order n. The ﬁrst few eigenfunctions and their associated energy levels are indicated schematically in ﬁg. 3.2. One of the key observations concerning our solution is that the probability of ﬁnding a particle in the classically forbidden region is nonzero. For example, if we consider the state labeled by n = 0, the maximum classical amplitude of vibration is given by equating the ﬁxed total energy, namely 12 h¯ ω, and the

3.2 Quantum Mechanics

89

Fig. 3.2. Schematic illustrating the harmonic oscillator potential and the associated wave functions. The wave functions are plotted such that the zeroes of ψi (x) intersect the energy axis at that energy corresponding to the energy of the i th state. 2 classical expression for the energy, which is given by 12 mω2 xmax , where xmax is the maximum displacement. This operation implies a maximum classical amplitude √ of vibration of x max = h¯ /mω. As is evident from the ﬁgure, the wave function bleeds out of the classical region with nonzero amplitude even at values of x in excess of the classical turning point. Many of the features of nonrelativistic quantum mechanics have revealed themselves in this problem. First, we have seen that as a result of imposition of the boundary conditions the allowed energy states are discrete. Secondly, we note a progression of associated wave functions, those tied to higher energies having more nodes, and all of which allow the particle to penetrate into the classically forbidden region. For the harmonic oscillator in particular, we have found a series of equally spaced energy levels that will loom important in our quest to understand the entropy of vibration of crystalline solids. In fact, when we undertake our analysis of the thermal motions of crystals, we will need exactly the spectrum of eigenvalues we have uncovered in examining what may at ﬁrst blush seem an unduly artiﬁcial example.

The Hydrogen Atom. The hydrogen atom is the problem against which many other models are measured. In confronting a new subject, often one seeks the ‘hydrogen atom’ of that ﬁeld, that is, the illustrative example that at once contains sufﬁcient complexity to capture the key ingredients of the problem without at the same time exacting too high an analytic toll. In this section our aim is to highlight the key features of the quantum mechanical investigation of the hydrogen atom. Our reason for doing so is derived in part from the fact that in attempting to build up models of the bonding in solids, we will ﬁnd ourselves appealing repeatedly to the

90

3 Quantum and Statistical Mechanics Revisited

hydrogenic wave functions to build intuition concerning the interactions between neighboring atoms. As with the harmonic oscillator, our starting point is the Schr¨odinger equation itself. In this case, the equation may be written in the form −

h¯ 2 2 ∇ ψ(r) + V (|r|)ψ(r) = Eψ(r), 2m

(3.16)

where for the moment we have speciﬁed the potential only to the extent that we note it is of the central force form. There is virtue in continuing our analysis in generic terms without yet specifying which central potential will be of interest, though we will do well to anticipate our eventual appeal to the special case of the Coulomb potential pertinent to the hydrogen atom. There are a number of ways to proceed at this point, and we will pursue the classic description in terms of the solution to a differential equation. By virtue of the presumed spherical symmetry of this problem, we carry out a separation of variables, with the result that the radial and angular terms are decoupled. This may be seen by starting with the Laplacian operator in spherical coordinates which leads to a Schr¨odinger equation of the form,

1 ∂ ∂ 1 ∂2 h¯ 2 1 ∂ 2 ∂ r + 2 sin θ + ψ(r) − 2m r 2 ∂r ∂r r sin θ ∂θ ∂θ r 2 sin2 θ ∂φ 2 + [V (|r|) − E]ψ(r) = 0. (3.17) We now seek a solution of the form ψ(r, θ, φ) = R(r )Y (θ, φ) which may be inserted into the equation above. Upon so doing and after the requisite reorganization of terms, we ﬁnd that our problem is reduced to

∂Y 1 h¯ 2 1 1 ∂ ∂ 2Y −h¯ 2 1 ∂ 2∂R 2 r +r [V (r )−E] = sin θ + . 2m R ∂r ∂r 2m Y sin θ ∂θ ∂θ Y sin2 θ ∂φ 2 (3.18) The result is an equation in which one side depends upon one set of variables while the other side depends upon a different set of variables and leads us to conclude that both sides are equal to a constant which, with feigned insight, we call l(l + 1). We now further assume that the angular solution may be factored into the form, Y (θ, φ) = P(θ)u(φ). Substituting this solution into the angular equation results once again in a decoupling of the θ and φ dependence and a second separation constant, namely, 1 d 2u dP sin θ d − sin θ + l(l + 1) sin2 θ = m 2 . = (3.19) u dφ 2 P dθ dθ As a result of these manipulations, the problem of solving the Schr¨odinger equation

3.2 Quantum Mechanics

91

for a particle in the presence of a central force potential has been reduced to the solution of three ordinary differential equations which may be written as

and

d 2u = −m 2 u, dφ 2

(3.20)

dP m2 1 d sin θ + l(l + 1)P − 2 P = 0, sin θ dθ dθ sin θ

(3.21)

d R 2mr 2 d2 R + 2 [E − V (r )] − l(l + 1) = 0. + 2r dr 2 dr h¯

(3.22)

and r2

The φ equation is routine and has solutions of the form u(φ) = eimφ . The requirement of periodicity of the wave function, namely that u(φ) = u(φ + 2π), restricts m to integer values. The θ equation is simpliﬁed by making the change of variables z = cos θ, resulting in the associated Legendre equation

2 m2 dF 2 d F (1 − z ) 2 − 2z F = 0, (3.23) + l(l + 1) − dz dz 1 − z2 which can be tackled via series solution. Rather than examining the strategy for solving the equation, we merely quote the solutions and attempt to learn something of their nature and signiﬁcance. The general solution to the associated Legendre equation may be written in the form F(z) = a Plm (z) + bQ lm (z), where the functions Plm (z) and Q lm (z) are known as associated Legendre polynomials. The solution Q lm (z) is rejected on the grounds that it is singular when z = ±1, and hence we keep only the Plm s. The compositions of the solutions to the θ and φ equations, by virtue of their relevance to all problems with spherical symmetry, are so important as to merit a special name, the spherical harmonics. These solutions bear the same relation to spherical problems that the Bessel functions do to those with cylindrical symmetry. The spherical harmonics, Ylm (θ, φ), may be written as Ylm (θ, φ) = Plm (cos θ)eimφ .

(3.24)

In the present context, their importance attaches to their role in describing the angular dependence of the hydrogenic wave functions. When we take up bonding in solids, we will see that the angular character implied by the spherical harmonics makes itself known in macroscopic observables as fundamental as those of the elastic moduli. We now take up the speciﬁc nature of the radial wave function. From eqn (3.18), we see that to make further progress requires the speciﬁcation of a particular form for V (r ). For the case of the hydrogen atom, V (r ) is of

92

3 Quantum and Statistical Mechanics Revisited

the Coulomb form. A choice must be made with regard to units in treating the electrostatic interaction, and we adopt the esu units within which the Coulomb potential is of the form V (r ) = e2 /r and results in a radial equation of the form

2 e2 h¯ 2l(l + 1) d R 2mr 2 2d R R = 0. (3.25) + 2 E+ − + 2r r dr 2 dr r 2mr 2 h¯ The radial equation can be further simpliﬁed into a recognizable form if one makes the substitution f (r ) = r R(r ), leading to

d2 f e2 l(l + 1) 2m f = 0. (3.26) − f + 2 E+ dr 2 r2 r h¯ What we have succeeded in doing is to rework the radial equation into exactly the form of a one-dimensional Schr¨odinger equation in the presence of an effective potential e2 h¯ 2 l(l + 1) . (3.27) + r 2m r 2 As in our analysis of the θ equation, rather than bothering with the niceties of solving this radial equation, we will quote its solutions and consider their signiﬁcance. The strategy that is adopted in solving this equation is in many respects similar to that used in solving the problem of the harmonic oscillator. One assumes on the basis of asymptotics that the solution may be written as a product of a term of the form e−βr and some as yet undetermined function. What results is a new differential equation, analogous to the Hermite differential equation we confronted in solving the harmonic oscillator, and this equation may be solved in terms of special functions known as the associated Laguerre polynomials, which depend upon the quantum numbers n and l and result in a radial wave function of the form r l 2l+1 2r −r/na0 . (3.28) L n−l−1 Rnl (r ) = e na0 na0 Veff (r ) = −

Here we have denoted the associated Laguerre polynomials as L 2l+1 n−l−1 . A few of these radial functions are shown in ﬁg. 3.3. In anticipation of the fact that we will later invoke hydrogen-like orbitals in the context of our discussion of electronic structure in chap. 4, we note that it is conventional to label orbitals using both their principal quantum number, n, and their orbital angular momentum number l. In particular, a hierarchy of states at a given n is built running from l = 0 to l = n − 1. For example, for n = 4 we have 4s, 4p, 4d and 4f states, where l = 0 is labeled s, l = 1 is labeled p, l = 2 is labeled d and l = 3 is labeled f. Like in the case of the harmonic oscillator, our insistence that the wave functions be bounded for large-r forces a truncation of the series in the form of

3.2 Quantum Mechanics

93

Fig. 3.3. Radial probability distributions for various low-lying states of hydrogen (adapted from Condon and Shortley (1935)).

polynomials. Further, this condition that the wave functions vanish at inﬁnity imposes restrictions on the allowed values of the energy which are En = −

me4 , 2h¯ 2 n 2

(3.29)

where n assumes only integral values. We note that the energies depend only upon the principal quantum number n. The implication of this result is that the various states of different angular momenta (labeled by l and m) are degenerate. In

94

3 Quantum and Statistical Mechanics Revisited

numerical form, the series of energy states introduced above is of the form 13.6 eV, (3.30) n2 providing a clear idea of the energy scale associated with problems of this type. We have found that the generic hydrogenic wave function takes the form En ≈ −

ψnlm (r) = Rnl (r )Ylm (θ, φ),

(3.31)

with associated energy eigenvalues of the form given in eqn (3.29). This solution will prove of great utility in our later development of the linear combination of atomic orbitals (or tight-binding) method.

3.2.3 Finite Elements and Schr¨odinger Recall from chap. 2 that often in the solution of differential equations, useful strategies are constructed on the basis of the weak form of the governing equation of interest in which a differential equation is replaced by an integral statement of the same governing principle. In the previous chapter, we described the ﬁnite element method, with special reference to the theory of linear elasticity, and we showed how a weak statement of the equilibrium equations could be constructed. In the present section, we wish to exploit such thinking within the context of the Schr¨odinger equation, with special reference to the problem of the particle in a box considered above and its two-dimensional generalization to the problem of a quantum corral. Our preliminary exercise will state the problem in one dimension, with the generalization to follow shortly. The one-dimensional Schr¨odinger equation may be written h¯ 2 d 2 ψ + V (x)ψ = Eψ. (3.32) − 2m d x 2 In the present case, the weak form is obtained by multiplying eqn (3.32) by some test function and integrating the ﬁrst term by parts. For the purposes of concreteness in the present setting, we imagine a problem for which the domain of interest runs from the origin to point x = a, and for which the wave functions vanish at the boundaries. We note that the Schr¨odinger equation could have been stated alternatively as the Euler–Lagrange equation for the functional a a h¯ 2 a dψ 2 2 dx + V (x)|ψ(x)| d x − E |ψ(x)|2 d x. (3.33) [ψ(x)] = 2m 0 d x 0 0 The ﬁnite element strategy is to replace this functional with a function of the N unknown values ψn (not to be confused with wave functions related to the hydrogen

3.2 Quantum Mechanics

95

atom from the previous section) of the wave function at the nodes of the ﬁnite element mesh. That is, we imagine a discretization of the region [0, a] by N distinct points which are taken to be the nodes of the ﬁnite element mesh. The problem of solving the Schr¨odinger equation then becomes one of determining not the entire function ψ(x), but rather for the values of ψ (i.e. ψn ) at the nodal positions, with the understanding that the value of the wave function at points between the nodes is obtained by ﬁnite element interpolation. Speciﬁcally, as with our earlier treatment of the ﬁnite element method, we imagine shape functions Ni (x) centered at each node, with the subscript i labeling the node of interest. It is then asserted that the wave function is given as ψ(x) =

N

ψn Nn (x),

(3.34)

n=1

and similarly the potential (which is known) is expanded in terms of the shape functions via N V (x) = Vn Nn (x). (3.35) n=1

What this means is that to write down the interpolated potential V (x), we ﬁnd the values of the potential at the nodes, Vn = V (xn ) and interpolate elsewhere using eqn (3.35). By virtue of the ﬁnite element ansatz, we may now effect a mapping between the functional [ψ(x)] and the function ({ψn }). In particular, upon substituting ψ(x) and V (x) from eqs (3.34) and (3.35) into eqn (3.33) and simplifying to the case in which we drop all reference to the fact that the wave function can be complex rather than real, we have h¯ 2 a d Ni (x) d N j (x) [ψ(x)] → ({ψn }) = dx ψi ψ j 2m i j 0 dx dx a Vk ψi ψ j Ni (x)N j (x)Nk (x)d x + i

−E

j

0

k

i

j

a

ψi ψ j Ni (x)N j (x)d x. 0

This result may be simpliﬁed considerably if we invoke the deﬁnitions h¯ 2 a d Ni (x) d N j (x) d x, Ki j = 2m 0 dx dx a Vi j = Vk Ni (x)N j (x)Nk (x)d x, k

0

(3.36)

96

3 Quantum and Statistical Mechanics Revisited

Mi j =

a

Ni (x)N j (x)d x. 0

Note that these matrices are functions only of known quantities, namely, the potential V (x) and the shape functions N (x). It is convenient to further simplify by introducing Hi j = K i j + Vi j , with the result that the function of interest is [Hi j − E Mi j ]ψi ψ j . (3.37) ({ψn }) = ij

At this point, we need to implement our original variational statement by seeking those ψn s that minimize the function ({ψn }). Imposition of this condition via ∂ = 0, ∂ψn results in the reformulation of the original problem as [Hn j − E Mn j ]ψ j = 0.

(3.38)

(3.39)

j

As a speciﬁc realization of these ideas, consider the celebrated problem of the one-dimensional particle in a box already introduced earlier in the chapter. Our ambition is to examine this problem from the perspective of the ﬁnite element machinery introduced above. The problem is posed as follows. A particle is conﬁned to the region between 0 and a with the proviso that within the well the potential V (x) vanishes. In addition, we assert the boundary condition that the wave function vanishes at the boundaries (i.e. ψ(0) = ψ(a) = 0). In this case, the Schr¨odinger equation is d 2 ψ(x) 2m E + 2 ψ(x) = 0. (3.40) dx2 h¯ We are searching for the wave functions and associated energy eigenvalues. From an analytic perspective, this problem is entirely routine with the result that the n th eigenfunction is of the form given in eqn (3.9) and the corresponding eigenvalues as given in eqn (3.10). Our objective is to see to what extent we can recover these results using the ﬁnite element method. Further, the relevant ﬁnite element analysis can be carried out almost entirely by hand. We imagine discretizing the region between 0 and a with N + 1 nodes as illustrated in ﬁg. 3.4. The representation of the wave function is now restricted entirely to the values of the wave function at the nodes, ψi , with the value between nodes determined by interpolation via ψ(x) = i ψi Ni (x). The particular choices of shape functions used in the present analysis are shown in ﬁg. 3.4 as well. Because of the fact that the shape functions are highly localized, the matrices K i j and Mi j introduced above will be nonzero only for the cases in which j = i or

3.2 Quantum Mechanics

97

Fig. 3.4. Schematic illustration of the nodes used to discretize the particle in a box problem and the corresponding ﬁnite element shape functions.

j = i ± 1. For a given level of approximation (as represented by the number of elements used in the analysis), the solution of the Schr¨odinger equation has been reduced to the construction of the matrix Hi j − E Mi j and the determination of the associated energy eigenvalues. In abstract terms, the relevant matrix elements may be evaluated as follows. Consider the case in which there are N + 1 nodes as shown in ﬁg. 3.4. First, we note that since within the region of interest there is no potential V (x), Hi j = K i j . The matrix element K ii is found as xi

xi + a N d Nil (x) 2 d Nir (x) 2 h¯ 2 dx + dx , (3.41) K ii = 2m xi − Na dx dx xi where we have introduced the notation Nir (x) to represent the shape function facing to the right of the i th node and Nil (x) to represent the shape function facing to the left of the i th node. These shape functions are written as N (xi − x) + 1, a N Nil (x) = (x − xi ) + 1, a

Nir (x) =

(3.42) (3.43)

and are characterized by the property that Ni (x j ) = δi j . In light of these deﬁnitions, the integrals in eqn (3.41) may be evaluated with the result K ii =

h¯ 2 N . ma

(3.44)

In a similar way, the matrix element K i,i+1 (which by symmetry is equal to K i,i−1 ) may be written as a l (x) h¯ 2 xi + N d Nir (x) d Ni+1 d x. (3.45) K i,i+1 = 2m xi dx dx The region of integration is determined by the fact that the only nonzero overlap between the i th and (i + 1)th shape functions is in the element sharing the i th and

98

3 Quantum and Statistical Mechanics Revisited

(i + 1)th nodes which is the region between xi and xi + a/N . Again, in light of the deﬁnition of the shape functions, it is easily shown that K i,i±1 = −

h¯ 2 N . 2ma

(3.46)

We also require the various matrix elements of the form Mi j which reﬂect the overlap of adjacent shape functions. The diagonal matrix elements may be written as xi xi + a N l 2 Mii = [Ni (x)] d x + [Nir (x)]2 d x. (3.47) xi − Na

xi

Performing the requisite integrals results in Mii =

2a . 3N

Similarly, the off-diagonal matrix elements may be written xi + a N l Nir (x)Ni+1 (x)d x, Mi,i+1 =

(3.48)

(3.49)

xi

with the result Mi,i±1 =

a . 6N

(3.50)

Once the various matrix elements are in hand, we can now search for the eigenvalues associated with a given ﬁnite element approximation. As a starting point, consider the case N = 2 in which there is only a single unconstrained nodal degree of freedom. In this case, the matrix of eqn (3.39) reduces to (K 11 − E M11 )ψ1 = 0. As a result, we see that our ﬁrst approximation to the ground state energy for the particle in the box is given by E 1(N =2) = K 11 /M11 = 6h¯ 2 /ma 2 . At the next level of approximation, we consider the case in which N = 3. If we adopt the notation that K ii = α and Mi,i±1 = β, then K i,i±1 = −α/2 and Mii = 4β. For the case N = 3, therefore, the resulting condition for the eigenvalues is α α − 4Eβ − − Eβ 2 = 0. (3.51) det α − − Eβ α − 4Eβ 2 The resulting energy eigenvalues are E 1(N =3) = α/10β and E 2(N =3) = α/2β and are represented in terms of h¯ 2 /2ma 2 in table 3.1, as are increasing levels of approximation. The act of taking our analysis to the next level of approximation (i.e. the use of more elements) requires neither further physical nor mathematical

3.2 Quantum Mechanics

99

Table 3.1. Eigenvalues associated with ﬁnite element approximation to solutions for Schr¨odinger equation for a particle in a one-dimensional box. Energies are reported in units of h¯ 2 /2ma 2 . Approximation

E1

E2

E3

E4

N =2 N =3 N =4 N =5 Exact

6.000 5.400 5.098 5.048 4.935

27.000 22.44 21.6 19.739

58.057 54.0 44.415

113.91 108.0 78.896

elaboration. The generic form of the secular equation, the roots of which are the energy eigenvalues, is tridiagonal and takes the form α 0 0 ··· 0 α − 4Eβ − − Eβ 2 α α 0 ··· 0 − − Eβ α − 4Eβ − − Eβ 2 2 α α ··· 0 0 − − Eβ α − 4Eβ − − Eβ 2 2 det .. .. .. .. .. .. . . . . . . . . . . α .. .. .. .. ··· − − Eβ 2 α 0 0 0 ··· − − Eβ α − 4Eβ 2 = 0.

(3.52)

The fact that the matrix is nonzero only in a strip near the main diagonal is an immediate consequence of the locality of the shape functions which implies that the overlap between different shape functions vanishes except in the case of neighboring elements. The result of carrying out calculations with increasing numbers of elements are summarized in table 3.1, and give a feel for the rate of convergence of the results. In addition to questions concerning the distribution of energy eigenvalues for this problem, we can also demand the implications of our ﬁnite element analysis for the wave functions. As a result of our knowledge of the energy eigenvalues, eqn (3.39) can be exploited to determine the wave functions themselves. By substituting the eigenvalues into these coupled equations, we can then solve for the corresponding ψi s. The simplest realization of this program is for the case N = 2 introduced above in which there is only a single free nodal degree of freedom. In this case, the value of ψ1 is determined entirely by the constraint of normalization. That is, we

100

3 Quantum and Statistical Mechanics Revisited

Fig. 3.5. Illustration of the ﬁnite element interpolated approximate wave functions: (a) ground state wave function for the N = 2 approximation; (b) ground state and ﬁrst excited state wave functions for the N = 3 approximation.

require that we have

a 0

ψ 2 (x)d x = 1. In this case, because of ﬁnite element interpolation, a 2 if x ≤ ψ1 x a 2 . ψ1(N =2) (x) = a 2 if x > ψ1 2 − x a 2

(3.53)

Our notation ψm(N =P) (x) indicates the m th eigenstate associated with the ﬁnite element approximation in which N = P. In the case above, the constraint of √ normalization requires that ψ1 = 3/a. The ground state wave function as obtained from our N = 2 approximation is illustrated in ﬁg. 3.5. A more instructive example of the ﬁnite element approximation to the wave function is provided by the case N = 3. In this case, by substituting the values of the energy eigenvalues back into eqn (3.39), we obtain equations for determining the ratio ψ1 /ψ2 . In particular, we ﬁnd that ψ1 K 12 − E M12 =− . ψ2 K 11 − E M11

(3.54)

For the ground state energy, this results in ψ1 /ψ2 = 1 while for the ﬁrst excited state we have ψ1 /ψ2 = −1. Again, in conjunction with the requirement that the

3.2 Quantum Mechanics

101

Fig. 3.6. Successive steps in the construction of a quantum corral using the tip of a scanning tunneling microscope (courtesy of D. Eigler).

wave functions be normalized, ψ1 and ψ2 can be unambiguously determined, with the result being shown in ﬁg. 3.5.

3.2.4 Quantum Corrals: A Finite Element Analysis Quantum mechanics is a subject that is well endowed with a series of enlightening schoolboy exercises. However, one of the fascinating features that has accompanied the attainment of atomic-level experimental probes is the ability to carry out experiments that attempt to mimic these very same problems. In this section we will examine the issues surrounding the solution of the problem of the ‘quantum corral’, in which a series of atoms are brought together on a crystal surface into a closed circular conﬁguration. The presence of these surface atoms has the effect in turn of conﬁning electrons, the states of which can be probed experimentally using scanning tunneling microscopy. In ﬁg. 3.6 a sequence of images is shown that represents the stages in constructing the quantum corral itself. From the standpoint of the Schr¨odinger equation, this is another example of a ‘particle in a box’ problem which in this case is effectively two-dimensional. In particular, the potential within the corral region is assumed to be zero, while the

102

3 Quantum and Statistical Mechanics Revisited

ring of atoms at the boundary is treated in the model as the source of an inﬁnite potential barrier. The inﬁnite barrier is translated into a boundary condition for the wave function at the boundary of the corral (r = a), namely, ψ(a, θ ) = 0. We begin by writing the Schr¨odinger equation in polar coordinates, 1 ∂2 1 ∂ h¯ 2 ∂ 2 (3.55) + 2 2 ψ(r, θ ) = Eψ(r, θ ), + − 2m ∂r 2 r ∂r r ∂θ and immediately attempt a solution in the separated form, ψ(r, θ ) = R(r )u(θ ). The differential equation can then be rearranged into two terms, one of which depends only upon r while the other depends only upon θ . As we noted in the case of the hydrogen atom, the equality of two independent functions to one another implies that both must, in turn, be equal to a constant which we denote m 2 in anticipation of the resulting differential equation. As a result of our separation of variables strategy, the problem of solving the Schr¨odinger equation for the quantum corral is reduced to that of solving two ordinary differential equations. In particular, we have 2m E d2 R 1 d R n2 + + − R = 0, (3.56) dr 2 r dr r2 h¯ 2 and d 2u + m 2 u = 0. (3.57) dθ 2 The r equation can be massaged into the form of a Bessel equation while the θ equation is elementary. As a result of these insights, the solution may be written as Jn ( 2m E/h¯ 2 r )eimθ . It now remains to impose our boundary conditions. We require that the solution be periodic in the angular coordinate, which implies that m is restricted to integer values, and that the wave function vanish when r = a. This second condition means that 2m E nl a = z nl , (3.58) h¯ 2 where z nl is the l th zero of the n th Bessel function. We see that each energy eigenvalue E nl is labeled by two quantum numbers, n and l. A more interesting perspective on the quantum corral problem is garnered from a ﬁnite element analysis. Since we have already carried through a detailed implementation of the ﬁnite element strategy with regard to the one-dimensional particle in a box, here we only note the salient features of the problem. To illustrate the character of two-dimensional ﬁnite elements, the circular region over which the solution is sought is discretized into a series of ﬁnite elements. An example of the type of mesh that is generated is shown in ﬁg. 3.7. We should also note

3.2 Quantum Mechanics

103

Fig. 3.7. Finite element mesh used to compute the eigenstates of the quantum corral (courtesy of Harley Johnson).

that a full two-dimensional treatment of this problem is an overkill since, as was already shown, the original problem can be reduced to the search for solutions of a one-dimensional radial equation. On the other hand, the two-dimensional solution is enlightening from the ﬁnite element perspective. As with the one-dimensional case described earlier, the unknowns are the nodal values of the wave function, ψn . To determine the wave functions between nodes, ﬁnite element interpolation is used, in this case with the relevant shape functions taking the form of triangular sheets such that the value of the shape function is 1 at one of the three nodes making up a given triangle, and 0 at the other two nodes and varying linearly in between. Once again, the Hamiltonian matrix is constructed and the resulting secular equation is solved with the result being a series of eigenvalues. In addition, the nodal values of the wave functions associated with the various states are determined as a result of this analysis, and two of the ﬁnite element wave functions are shown in ﬁg. 3.8. 3.2.5 Metals and the Electron Gas So far, our quantum mechanics examples have been rather far aﬁeld from questions of immediate interest to our study of solids. In particular, we aim to see what light quantum mechanics sheds on the origin of bonding and cohesion in solids. To do so, in this introductory chapter we consider two opposite extremes. Presently, we consider the limit in which each atom is imagined to donate one or more electrons to the solid which are then distributed throughout the solid. The resulting model is the so-called electron gas model and will be returned to repeatedly in coming

104

3 Quantum and Statistical Mechanics Revisited

Fig. 3.8. Two different eigenfunctions for the quantum corral as obtained by using a two-dimensional ﬁnite element calculation (courtesy of Harley Johnson).

chapters. The other limit that will be considered in the next section is that in which it is imagined that the formation of the solid results in a small overlap between the atomic orbitals associated with different atoms. This picture will lead to the so-called tight-binding method (or linear combination of atomic orbitals). With our interest in the bonding of solids, we undertake an analysis of the electron gas, which in simplest terms is nothing more than a three-dimensional version of the particle in a box problem which we have already seen in both its one- and two-dimensional guises. Here the physical idea is that some subset of electrons is donated from some host atoms such as sodium or aluminum, and can be thought of as being distributed within a box, with the only conﬁning potential they experience arising from the presence of the boundaries of the solid themselves. In addition, for the time being we advance the assumption that the positive charge associated with the ions is distributed uniformly so as to guarantee charge neutrality. This approximation is the basis of the free electron theory of metals. However, in considering this idealized model, we are immediately confronted with one of the intriguing paradoxes of the electronic theory of solids, namely, the surprising efﬁcacy of independent particle models. Note that we have said nothing of the interactions between electrons. We will revisit this conundrum in later chapters, while for now maintaining our assumption that the electrons behave as though they are independent. Within the model of a metal proposed above, the Schr¨odinger equation becomes −

h¯ 2 2 ∇ ψ(r ) = Eψ(r ), 2m

(3.59)

3.2 Quantum Mechanics

105

with the additional proviso that the wave functions satisfy boundary conditions to be elaborated below. The solution in this is immediate and is seen to take the √ case ik·r familiar plane wave form, ψ(r) = (1/ )e . Here we have adopted the notation box. This factor appears in the = L 3 , where L is the edge length of the conﬁning wave function as a result of our demand that |ψ(r)|2 d 3 r = 1, a normalization condition. Note that in light of our probabilistic interpretation of the wave function, we see that the electron can be thought of as uniformly spread out throughout the conﬁning box. Associated with a plane wave characterized by a wavevector k, is an energy eigenvalue given by E k = h¯ 2 k 2 /2m. Note that the dependence of the energy on the wavevector k is isotropic. The choice of a ﬁnite-sized box imposes restrictions on the allowed values of the wavevector. In particular, if we impose periodic boundary conditions of the form ψ(x, y, z) = ψ(x + L , y, z), we ﬁnd that the wavevectors can only take the values ki = 2πm i /L, where m i is an integer. Note that we could just as well have chosen boundary conditions in which the wave functions vanish at the boundary, with no change in our conclusions concerning the energetics of the electron gas. If we wish to characterize these eigenvalues geometrically it is convenient to think of a discrete lattice of allowable points in ‘k-space’. Each set of integers (m 1 , m 2 , m 3 ) labels a point in this space and is tied to a particular energy eigenvalue Em1m2m3 =

2π 2 h¯ 2 2 (m 1 + m 22 + m 23 ). m L2

(3.60)

The set of allowed points in k-space is depicted schematically in ﬁg. 3.9. The isotropy of the energy spectrum implies a wide range of degeneracies which are of interest as we ﬁll these states. To probe the implications of our solution, we now need to implement the Pauli principle described earlier. The goal is to assign to the various energy states their relevant occupancies, that is, how many electrons are to be assigned to each state? The Pauli principle demands that only one electron be assigned to each state (or two electrons for each k-vector if we acknowledge the two possible states of spin). This requirement is tied at a deeper level to the existence of certain symmetry requirements for the electronic wave function. For the case of electrons (fermions), one insists that the electron wave function be antisymmetric. In the context of our problem, this demand is equivalent to the assertion that only one electron be allowed to occupy each energy state. The prescription that emerges for computing the total electronic energy of our system, then, is to sum up the energies associated with the lowest eigenvalues, until all of the electrons have been suitably assigned to an associated energy. For the sake of concreteness, we assume that the conﬁning box has cube edges of dimension L. Further, we assume that N atoms occupy this box and that each has

106

3 Quantum and Statistical Mechanics Revisited

Fig. 3.9. Depiction of allowed k-points associated with energy eigenvalues for particle in a threedimensional box. The series of k-points shown in the ﬁgure are those in the positive octant of k-space falling within a spherical shell of such k-points.

donated a single valence electron which results in an electron density ρ = N /L 3 . The total electronic energy in our noninteracting electron model can then be found N by evaluating the discrete sum over the energy eigenvalues (i.e. 2 i=1 E i , where the energies are rank ordered E 1 < E 2 < · · · < E N and the factor of 2 accounts for spin) and terminating this sum once N states have been occupied. However, in the limit that our box is sufﬁciently large, the energy levels are so closely spaced we can just as well evaluate this energy by replacing the discrete sum with an integral over a continuous distribution of eigenvalues. To see this, note that adjacent energy levels have an energy difference of order 2π 2 h¯ 2 /m L 2 . The integration that arises in replacing the discrete summation is most conveniently realized in k-space. To effect this integration, it is ﬁrst necessary to identify the number of states per unit volume of k-space. Recall that the points in k-space are of the form km 1 ,m 2 ,m 3 = (2π/L)(m 1 , m 2 , m 3 ), and hence occupy the vertices of a simple cubic lattice in k-space. As a result, each such point may be assigned a volume (2π/L)3 . This observation comes from the recognition that the lattice parameter in k-space is 3 3 2π/L. Hence we make the identiﬁcation N = (L/2π) d k and it is seen that the total energy is given by 3 L h¯ 2 k 2 3 (3.61) d k, E tot = 2 2π k 2m

3.2 Quantum Mechanics

107

where the factor of 2 accounts for the fact that each k-point can accommodate two electrons, one for each component of spin. Here we have done nothing more than replace the sum over occupied states with the integral given above, where the prefactor serves as a density of states and insures that our volume element d 3 k is properly weighted. Because of the isotropy of the energy spectrum when viewed from the k-space perspective, this integration can be carried out in spherical coordinates, where the radius of the resulting sphere is denoted as the Fermi wavevector, k F . It is clear that the magnitude of the Fermi wavevector is intimately tied to the electronic density, but how? Here, we see that the total number of states contained within this k-space sphere is the same as half the total number of electrons (again the factor of 2 arising because of spin). The volume of the Fermi sphere is k = 4π k 3F /3, while the volume per state is (2π/L)3 . Hence, the ratio of these numbers must yield the total number of electrons and 1 leads to the conclusion that k F = (3π 2 ρ) 3 . Given the radius of the Fermi sphere, we are now in a position to evaluate the total energy of our electron gas. Upon explicitly writing the integral given above in spherical coordinates, we ﬁnd 3 k F 2π π 2 4 L h¯ k sin θk dkdφk dθk , (3.62) E tot = 2 2π 2m 0 0 0 where we include the subscript k as a reminder that our integration is carried out over a sphere in k-space. Performing the relevant integrations leads to the conclusion that h¯ 2 k 5F E tot = , (3.63) V 10π 2 m which can in turn be converted into an average energy per electron of 3 h¯ 2 k 2F 3 E tot = = F . (3.64) N 5 2m 5 Here we have introduced the notion of the Fermi energy which is denoted by F . This energy, like the Fermi wavevector, can be obtained explicitly in terms of the electron density. In fact, since shortly we will use the energy of the electron gas to obtain the optimal density, it is convenient to rewrite eqn (3.64) in terms of the 1 density, recalling that k F = (3π 2 ρ) 3 as E tot =

3 h¯ 2 2 (3π 2 ρ) 3 , 5 2m

(3.65) 2

illustrating that this part of the electron gas energy scales as ρ 3 . If we take a typical ˚ −3 , the associated Fermi energy is roughly 7 eV, some 300 density such as 0.1 A times larger than the thermal energy scale at room temperature, for example.

108

3 Quantum and Statistical Mechanics Revisited

The results for the electron gas obtained above can be pushed much further. In particular, the rudimentary calculation developed thus far can serve as a jumping off point for an evaluation of the lattice parameter and bulk moduli of simple metals. As it stands, the energy we have determined for the electron gas is a monotonically increasing function of the density and thus there is as yet no provision for an optimal density. However, we can now supplement the analysis given above by treating the effect of electron–electron interactions perturbatively. In this case, the details of the calculation will take us too far aﬁeld, so we will have to be satisﬁed with sketching what is involved in making the calculation and in quoting the results. The basic idea is that we wish to evaluate the expectation value of the perturbed Hamiltonian H =

1 e2 , 2 i= j |ri − r j |

(3.66)

which characterizes the electron–electron interaction. Physically what this means is that we are trying to determine the correction to the energy of eqn (3.65) as a result of putting the electron interaction back into the problem. This correction is determined by using the ground state wave function of the unperturbed electron gas (this is the normal rule of ﬁrst-order perturbation theory), which we already know from the previous section is a product of plane waves that have been appropriately antisymmetrized to respect the Pauli principle. In particular, we must evaluate E ee = ψtot |H |ψtot , where ψtot (r1 , . . . , r N ) is of the form 1 ik ·r √ e 1 1 1 ik ·r 1 √ e 2 1 ψtot (r1 , . . . , r N ) = √ .. N! . 1 ik ·r √ e N 1

1 √ eik1 ·r2 1 ik2 ·r2 √ e .. . 1 √ eik N ·r2

(3.67)

··· ··· .. . ···

1 √ eik1 ·r N 1 ik2 ·r N √ e .. . 1 √ eik N ·r N

, (3.68)

a construction known as the Slater determinant that instructs us how to build up a properly antisymmetrized wave function as a product of one-electron wave functions. Note that we have been slightly sloppy by omitting the added dependence on the spin coordinates in the wave function. For full details, see chap. 3 of Pines (1963) or chap. 1 of Fetter and Walecka (1971). As is evident from the form of the integrals that will result from evaluating the expectation value demanded in eqn (3.67), the outcome of this analysis depends upon the Fourier transform

3.2 Quantum Mechanics

109

of the Coulomb potential itself. Careful evaluation of the integrals demanded by eqn (3.67) results in a contribution to the total energy of the electron gas of the form 3 h¯ 2 1 E interact = − (3π 2 ρ) 3 , (3.69) 2π 2ma0 where a0 is the Bohr radius and is given by a0 = h¯ 2 /me2 . Note that the sign of this contribution to the energy is negative, resulting in a competition between the two terms we have found and a consequent emergence of an optimal density. The result of adding together the two contributions to the energy of the electron gas is E egas =

3 h¯ 2 3 h¯ 2 2 1 (3π 2 ρ) 3 − (3π 2 ρ) 3 . 5 2m 2π 2ma0

(3.70)

This energy has a minimum at a certain optimal density which may be found by evaluating ∂ E egas /∂ρ = 0, resulting in ρopt =

125 . 192π 5 a03

(3.71)

This density may be converted in turn to an estimate for the lattice parameter by assuming that the atom at each lattice site of the bcc lattice has donated a single electron. In particular, the lattice parameter implied by these arguments is 1 384π 5 3 ˚ aeg = a0 ≈ 5.2 A. (3.72) 125 This number should be contrasted with the experimental lattice constant of a typical ˚ In free electron metal such as sodium, for which the lattice parameter is 4.23 A. addition to the lattice parameter, this model may also be used to estimate the bulk modulus of free electron metals by resorting to the deﬁnition B = V (∂ 2 E/∂ V 2 ). This is left as an exercise for the reader. In the present context, this example was intended to serve as a reminder of how one formulates a simple model for the quantum mechanics of electrons in metals and, also, how the Pauli principle leads to an explicit algorithm for the ﬁlling up of these energy levels in the case of multielectron systems. In addition, we have seen how this model allows for the explicit determination (in a model sense) of the cohesive energy and bulk modulus of metals.

3.2.6 Quantum Mechanics of Bonding As we hinted at in the section on the hydrogen atom, when we turn our attention to the origins of bonding in molecules and solids, a useful alternative to the

110

3 Quantum and Statistical Mechanics Revisited

Fig. 3.10. Disposition of wave functions of neighboring atoms during the process of bond formation.

electron gas physics described above is to build our picture around the simple ideas suggested by the H2 molecule. As shown in ﬁg. 3.10, the hydrogenic wave functions on the atoms of interest begin to overlap once these atoms are sufﬁciently close. Conceptually, we see that once this happens, the nuclear potential on one of the atoms begins to amend the wave function tied to the other. In this section, our task is to compute this interaction and to demonstrate how it makes possible the reduction in energy more commonly known as bonding. We begin with a discussion of bonding in the abstract, and then turn to an explicit treatment of the H2 molecule itself, and show how what is learned there can be generalized to systems of increasing size. The ideas developed here provide the conceptual foundations for our development of the tight-binding method in chap. 4. The intuition leading to this approach is best coached by an analogy. If we are to consider a system of masses and springs such as is shown in ﬁg. 3.11, our various oscillators will vibrate independently, each at its own natural frequency. If we now imagine connecting the oscillators, as also shown in the ﬁgure, it is immediate that the vibrational frequencies are altered by the interaction. In particular, if we consider the simple case where the masses and spring constants are all equal, we ﬁnd that the frequencies are split in the manner indicated in the ﬁgure. The quantum mechanical analog of the spring problem, also illustrated schematically in ﬁg. 3.11, is the idea that when two atoms are sufﬁciently far apart, their respective atomic energy levels at energy E a are undisturbed, and the atoms should be thought of as independent. On the other hand, when the atoms are in sufﬁciently close proximity, the potential due to one nucleus begins to inﬂuence the electron centered on the other. This interaction has the effect of splitting the original energy levels as indicated in the ﬁgure. For a two-atom molecule in which each atom

3.2 Quantum Mechanics

111

Fig. 3.11. Analogy between problem of coupled oscillators and that of bonding in molecules.

donates one electron, the difference in energy between the original isolated atoms and the molecule is E bond = −2|h|, the bonding energy. From a physical perspective, our strategy in thinking about bonding has certain key similarities to our treatment of the free electron gas. In particular, we assume that the properties of the molecule (or solid) can be obtained by solving a oneelectron Schr¨odinger equation and then ﬁlling up energy levels in accordance with the Pauli principle. This means that we completely ignore the interaction between the electrons themselves. Hence, for the two-atom molecule of interest here, the Schr¨odinger equation may be written h¯ 2 2 ∇ ψ + V1 (r)ψ + V2 (r)ψ = Eψ. (3.73) 2m In this equation, the total potential experienced by the electron is obtained by −

112

3 Quantum and Statistical Mechanics Revisited

summing up the separate nuclear potentials emanating from the two nuclei, V1 and V2 . Rather than trying to ﬁnd those functions which satisfy the Schr¨odinger equation written above, we adopt a simpler variational approach in which the search for unknown functions is replaced by the search for unknown coefﬁcients. The basis for this strategy is a variational argument. We represent the wave function for the molecule as a linear combination of the atomic orbitals centered on the two nuclei, that is, ψ = a1 φ1 + a2 φ2 ,

(3.74)

where φ1 and φ2 are the atomic orbitals on sites 1 and 2, and the ai s are the coefﬁcients we aim to determine. We have adopted a minimalist approach in which rather than using a basis consisting of all of the atomic orbitals associated with each site, we just borrow a single 1s orbital (i.e. |1, 1s and |2, 1s, where the ﬁrst index labels the site and the second labels the orbital type) from each atom and assume that the molecular wave function can, to a ﬁrst approximation, be represented as a linear combination of these functions. A more sophisticated treatment could include more basis functions such as the 2s and 2p states, and so on. The basis of the determination of the unknown coefﬁcients is the recognition that the expectation value of the energy can be written as E = ψ| Hˆ |ψ,

(3.75)

and our task is to ﬁnd those ai s that minimize this expression. In fact, this is exactly the same argument we adopted in our description of the ﬁnite element approach to the Schr¨odinger equation, with the difference being the choice of basis functions. As a result of the arguments given above, we write the function to be minimized as (a1 , a2 ) = a1 φ1 + a2 φ2 | Hˆ |a1 φ1 + a2 φ2 − Ea1 φ1 + a2 φ2 |a1 φ1 + a2 φ2 , (3.76) in perfect analogy with eqn (3.36). If we write this out explicitly term by term, the result is (a1 , a2 ) = a1∗ a1 φ1 | Hˆ |φ1 + a1∗ a2 φ1 | Hˆ |φ2 + a2∗ a1 φ2 | Hˆ |φ1 + a2∗ a2 φ2 | Hˆ |φ2 − E(a1∗ a1 φ1 |φ1 + a1∗ a2 φ1 |φ2 + a2∗ a1 φ2 |φ1 + a2∗ a2 φ2 |φ2 ),

(3.77)

an equation which can be further simpliﬁed if we adopt the notation E 1 = φ1 | Hˆ |φ1 , E 2 = φ2 | Hˆ |φ2 , and h = φ1 | Hˆ |φ2 = φ2 | Hˆ |φ1 . Applying these deﬁnitions to the result given above, and exploiting the assumption of orthonormality (i.e. φi |φ j = δi j ), which is, strictly speaking, not true, we now

3.2 Quantum Mechanics

113

Fig. 3.12. Solutions for H2 molecule using the two-orbital basis.

ﬁnd (a1 , a2 ) = a1∗ a1 E 1 + a1∗ a2 h + a2∗ a1 h + a2∗ a2 E 2 − E(a1∗ a1 + a2∗ a2 ).

(3.78)

For simplicity, we now assume that the two atoms are identical (i.e. E 1 = E 2 ) and further, choose our zero of energy such that E 1 = 0. If we now minimize this function with respect to the ai s, in particular by enforcing ∂/∂ai∗ = 0 for i = 1, 2, we can ﬁnd the optimal choice for these coefﬁcients. Effecting the minimization suggested above results in two coupled algebraic equation that are more conveniently written in matrix form as a1 0 −|h| a1 =E . (3.79) a2 a2 −|h| 0 Note that we have used our knowledge of the sign of h to rewrite it as h = −|h|, a result of the fact that the potential energy of interaction represented by this parameter is negative. The result of solving these √ equations is two solutions, one with energy E = −|h| and wave function ψ1 =√(1/ 2)(φ1 +φ2 ) and the other with energy E = |h| and wave function ψ1 = (1/ 2)(φ1 − φ2 ). These two solutions are shown in ﬁg. 3.12.

114

3 Quantum and Statistical Mechanics Revisited

Fig. 3.13. Series of molecules of increasing size and associated molecular eigenstates. The wave functions are indicated schematically with shaded atoms corresponding to one sign of relevant atomic orbital and unshaded atoms corresponding to opposite sign for relevant orbital (adapted from Hoffmann (1988)). Note that the spacing of energy levels is schematic and there is no relation indicated between the energy scales for different size molecules.

Recall that the question we originally posed was that of the origin of bonding. As a result of the solution worked out above, we are now in a position to address this question. With the zero of energy chosen above, the energy of the two isolated atoms is E atoms = 0. For the molecule, we ﬁll energy levels according to Pauli’s principle, which for the two-electron problem of interest here means one spin-up electron and one spin-down electron are both assigned energy −|h| with the result that the energy difference between the molecule and the free atoms is E bond = −2|h|. The energy is lowered by virtue of the partnership struck up between the two free atoms: a bond has formed. This idea is illustrated graphically in ﬁg. 3.12 where it is seen that there is an enhancement in the probability distribution in the region between the two atoms, a signature of the formation of bond charge. The generalization of this problem to the case of increasingly larger collections of atoms is straightforward and is founded upon the construction of larger matrices of the variety described above. For example, if we consider the problem of three atoms which occupy the vertices of an equilateral triangle, a 3 × 3 matrix emerges with three resulting eigenvalues. The distribution of energy eigenvalues for increasing system sizes is indicated schematically in ﬁg. 3.13. This ﬁgure demonstrates the way in which the energy can be lowered as a result of atoms conspiring to form bonds. In chap. 4, we will undertake a systematic analysis

3.3 Statistical Mechanics

115

of bonding in solids, using what we have learned of quantum mechanics in the preceding pages. In this part of the chapter, we have seen that quantum mechanics provides the microscopic foundations for evaluating the disposition of the electronic degrees of freedom. Just as continuum mechanics provides the setting within which one solves the boundary value problems related to the deformation of solids, quantum mechanics provides a scheme for attacking the boundary value problems associated with electrons in solids. Of course, quantum mechanics has a much wider scope than we have hinted at here, but our aim has been to couch it in terms of the subject at hand, namely, the modeling of materials. In this case, it is the role of quantum mechanics in instructing us as to the nature of bonding in solids that is of most importance, and as will be seen in coming chapters, these ideas will be an indispensable part of our modeling efforts.

3.3 Statistical Mechanics 3.3.1 Background Thermodynamics provides the conceptual cornerstone upon which one builds the analysis of systems in equilibrium. The elemental theoretical statement that can be made about such systems is embodied in Gibbs’ variational principle. This asserts that a certain function of state, namely the entropy, is a maximum in equilibrium so long as the system is subject to the additional constraint of constant total energy. The usual intuitive notions one attaches to the analysis of systems in contact with each other such as equality of temperature, pressure and chemical potential emerge from this principle quite naturally. For example, if we consider the box shown in ﬁg. 3.14 with an internal partition that is rigid and impermeable, the variational principle noted above can be used to determine the privileged terminal state (i.e. the state of equilibrium) that results from removing the constraints offered by the wall. The argument is that for the overall closed system, the total energy is given by E tot = E 1 + E 2 = const., implying that d E 1 = −d E 2 . On the assumption that the entropy S is additive, we note that ∂ S1 ∂ S2 d Stot = d E1 + d E2. (3.80) ∂ E 1 V ,N ∂ E 2 V ,N 1

1

2

2

These derivatives are evaluated at ﬁxed volumes V1 and V2 as well as ﬁxed particle numbers N1 and N2 . If we now replace d E 2 with −d E 1 , we see that the condition of maximum entropy is equivalent to the statement that ∂ S2 ∂ S1 = , (3.81) ∂ E1 ∂ E2

116

3 Quantum and Statistical Mechanics Revisited

Fig. 3.14. Partitioning of the system under consideration into two boxes which may freely exchange energy.

which because of the deﬁnition of temperature as 1/T = (∂ S/∂ E)|V,N , we recognize as the condition of equality of temperature between the two subsystems. If we consider in turn the case in which the wall is permeable (d N1 = −d N2 ) or may move (d V1 = −d V2 ), the conditions of equal chemical potential and pressure result. As it stands, the type of thermodynamic assertions ﬂeshed out above are indifferent to microscopic considerations, though it is certainly of great interest to unearth their microscopic origins. In this part of the chapter our aim is to investigate statistical mechanics. A key insight that emerges from these ideas is the probabilistic nature of equilibrium states. We take the view that statistical mechanics is the microscopic partner of equilibrium thermodynamics. While equilibrium thermodynamics does not concern itself with the mechanistic underpinnings of observed behavior, statistical mechanics teaches how one may deduce macroscopic features of a system as the result of a postulated microscopic model. Such models are widespread, doing service in problems such as the calculation of electric and magnetic susceptibilities, the analysis of the equilibrium concentrations of point defects in solids and the determination of the vibrational entropy of solids and its connection to phase transformations. Our treatment begins on a philosophical note with an attempt to elucidate the business of statistical mechanics. Next, we will turn to an analysis of the formal apparatus of statistical mechanics with a view of the partition function and how

3.3 Statistical Mechanics

117

it may be used in the evaluation of quantities of thermodynamic interest. The harmonic oscillator will loom large in our discussion as a result of the contention that this model may serve as a basis for the analysis of material properties, such as the speciﬁc heat, the vibrational entropy and the microscopic origins of the diffusion constant. This discussion will then be couched in the alternative language of information theory. These arguments will identify the role of inference in statistical mechanics, and will make more evident how we treat systems in the face of incomplete knowledge of that system’s microscopic state. This will be followed by a computational view of statistical mechanics. Here the task will be to see how the use of computing lends itself to a numerical statement of the program of statistical mechanics, with a brief overview of molecular dynamics and the Monte Carlo method. Our starting point is an assessment of the meaning of a macroscopic observable state. Thermodynamic states are parameterized by a small number of relevant macroscopic variables such as the energy, E, the volume, V , the pressure, p, and the various mole numbers, n α . As Callen (1985) has eloquently noted in the introductory sections of his book, it is well nigh miraculous that despite the ostensible need of 1023 degrees of freedom to fully characterize the state of a system, all but a few of them ‘are macroscopically irrelevant.’ Indeed, a key outcome of the statistical mechanical approach is an insight into how macroscopic parameters arise as averages over the microscopic degrees of freedom. Our fundamental contention is that a given macroscopic state is consistent with an enormous number of associated microscopic states. This observation lends itself to a nomenclature which distinguishes between macrostates and microstates. For the moment, we do not distinguish between the classical and quantum versions of these microstates, though we will see later that in some cases, such as that of the speciﬁc heat of solids, there are dramatic differences in the outcome of classical and quantum analyses. Classical physics envisions a continuum of microscopic states parameterized by the conjugate variables qi and pi , where these are the coordinates and momenta of the i th particle, respectively. For a system composed of N particles, each microstate corresponds to a particular point in a 6N -dimensional space referred to as ‘phase space’, with the dynamical variables varying continuously as the system winds about on its trajectory through this space. A given point within the classical phase space corresponds to a particular realization of the coordinates (q1 , p1 , q2 , p2 , . . . , q N , p N ) = ({qi , pi }). On the other hand, within quantum mechanics, these states are discretely reckoned and each microstate is parameterized by distinct quantum numbers. The notion of a microstate is perhaps most easily understood by virtue of an example. We imagine a closed box containing an ideal gas. Our use of the term ‘closed’ is meant to imply that in this case the volume, the number of particles and

118

3 Quantum and Statistical Mechanics Revisited

Fig. 3.15. Comparison of two possible microstates for particles in a box.

the energy of the system are all held constant and assume the values V, N and E, respectively. Within either the classical or quantum settings we may immediately identify the nature of the microstates available to the gas. The speciﬁcation of a particular point in phase space implies knowledge of a geometrical character. In particular, the speciﬁcation of the 3N coordinates qi identiﬁes the locations of all of the particles while the 3N momenta pi characterize their motions. The momenta of the molecules of the gas are imagined to be distributed in some way that is consistent with the assumed total energy, E. In addition, there is a conﬁgurational part of the microstate. One possible geometric conﬁguration which corresponds to an allowable microstate of the gas would have all of the molecules bunched in one corner of the box. Intuitively, such a state seems unlikely. On the other hand, there are many more microstates in which the molecules are distributed evenly throughout the box. These two alternatives are contrasted in ﬁg. 3.15. We can estimate the probability of the state in which the particles are bunched in one corner as (Vc /Vtot ) N , where Vc is the volume of the region where the particles are assumed to be bunched. In keeping with the assumption of noninteracting particles that is the essence of the ideal gas, we have assumed that the probability that a given particle will be in any subregion is given by the ratio of the volume of that subregion to the whole volume. The key feature of interest for the calculation given above is that all such microstates (including the unlikely state in which all the molecules are localized in some small region) are consistent with the overall macrostate characterized by the observables V, N and E. The postulate that rests behind the explicit calculation of macroscopic observables is that such observables are averages that emerge as a result of the system ranging over the allowed microstates. For our purposes, the central assumption upon which the rest of our development is ﬁxed is that all such microstates

3.3 Statistical Mechanics

119

consistent with the overall macrostate are equally likely. This statement is sometimes referred to as the principle of equal a priori probabilities or the principle of insufﬁcient reason. At ﬁrst sight, it may seem odd that this statement has calculable consequences. But as will be shown below, this postulate provides a logical basis for statistical mechanics and is used to derive the analytic machinery which makes the theory so powerful. The quantitative basis for the linkage between macro- and microstates is provided by the prescription for computing the entropy S(E, V, N ) in terms of the number of microstates, namely, S(E, V, N ) = k B ln (E, V, N ),

(3.82)

where (E, V, N ) is the number of microstates available to the system when it has energy, E, occupies a volume, V , and consists of N particles. This equation is a key example of the type of link between the microscopic and macroscopic perspectives that is our aim. In this case, it is the entropy, S, a property of the macrostate that is related to (E, V, N ), the associated microscopic quantity which characterizes the number of ways of realizing the macroscopic state of interest. The constant that links these two quantities is Boltzmann’s constant and will hereafter be referred to simply as k. The immense signiﬁcance of this equation is tied to the fact that it provides a mechanistic interpretation of the notion of entropy, while at the same time rooting the notion of equilibrium in probabilistic ideas. In particular, the assertion that emerges from this equation in conjunction with Gibbs’ variational statement, is that the equilibrium state (the state of maximum entropy) is really the macrostate corresponding to the largest number of microscopic realizations. As a result, we see that the primary business of statistical mechanics has been reduced to that of counting the number of microstates accessible to the system once the energy, volume and particle number have been ﬁxed.

3.3.2 Entropy of Mixing In this section, we take up the view of the statistical origins of entropy and equilibrium that was introduced in the previous section. We advance the view that equilibrium can no longer be viewed as a matter of certainty, but rather only as a matter of enormous likelihood. An example which is at once simple, enlightening and useful is related to the entropy of mixing, where it is imagined that two constituents are randomly distributed among N sites subject to the constraint that N A + N B = N , as depicted in ﬁg. 3.16. The analysis of the entropy of mixing serves as a viable starting point for the consideration of problems such as the conﬁgurational entropy of a two-component alloy, the distribution of vacancies within a single crystal at equilibrium and the arrangements of magnetic spins.

120

3 Quantum and Statistical Mechanics Revisited

Fig. 3.16. Two-dimensional schematic representation of two distinct alloy conﬁgurations where different atom types are represented by different colors: (a) disordered state, (b) ordered state.

We note that if we have a total of N sites to occupy, there are N ! different ways of occupying these sites on the assumption that each conﬁguration is distinct. However, in our case this logic must be amended on the basis of the realization that there are N A equivalent A objects and N B equivalent B objects. This implies that in reality there are N! = (3.83) N A !N B ! distinct conﬁgurations. The denominator in this expression eliminates the redundancy which results from the fact that the A objects are indistinguishable among themselves as are the B objects. Following Boltzmann’s equation linking the entropy and the number of microstates, the entropy that follows from this enumeration is N! . (3.84) S = k ln N A !N B ! As we can see in this instance, the calculation of the entropy of mixing has been reduced to the combinatorial problem of identifying the number of distinct microstates consistent with our overall macrostate which is characterized by a ﬁxed number of A and B objects. Further insights into this conﬁgurational entropy can be gleaned from an attempt to reckon the logarithms in an approximate fashion. We note that our expression for the entropy may be rewritten as S = k(ln N ! − ln N A ! − ln N B !).

(3.85)

Following Reif (1965), these sums may be written explicitly as ln N ! = ln 1 + ln 2 + · · · + ln N .

(3.86)

3.3 Statistical Mechanics

121

Fig. 3.17. Approximations associated with Stirling approximation.

This sum may be represented graphically as shown in ﬁg. 3.17, which suggests the approximate expression N ln x d x = N ln N − N . (3.87) ln N ! ≈ 1

Here it must be noted that we have made an imprecise description of what under more formal terms is known as the Stirling approximation. Within the context of our characterization of the conﬁgurational entropy, the Stirling approximation of ln N ! allows us to rewrite the entropy as S = k[(N A + N B ) ln(N A + N B ) − N A ln N A − N B ln N B ].

(3.88)

If we now deﬁne the variable c = N A /N and rearrange terms it is found that S = −k N [(1 − c) ln(1 − c) + c ln c].

(3.89)

This entropy is shown in ﬁg. 3.18 as a function of the concentration variable. In chap. 7, it will be shown that this result is one piece of the free energy that reﬂects the competition between the energy cost to increase the number of vacancies in a solid and the free energy lowering increase in entropy that attends an increase in the number of such vacancies. The arguments given above were built around the idea of an isolated system. However, there are both mathematical and physical reasons to favor a treatment in which we imagine our system as being in contact with a reservoir at ﬁxed temperature. For example, our later discussion of annealing is a realization of this claim. A particular sample of interest (a chunk of metal, for example), is subjected to external heating with the aim of examining the change in its microstructure. In this case, the model of an isolated system is inappropriate. Rather, we should model

122

3 Quantum and Statistical Mechanics Revisited

Fig. 3.18. Entropy of mixing associated with binary conﬁgurations.

the system as being in contact with a reservoir with which it exchanges energy. This scenario leads to the canonical distribution which will form the substance of the next section. 3.3.3 The Canonical Distribution For many problems, consideration of the isolated system envisioned above is inadequate. In particular, it is often of interest to consider a subsystem in contact with a reservoir. Such reservoirs can either be a source of energy or particles, and one imagines free communication between the subsystem of interest and its associated reservoir. The conceptual trick introduced to allow for rigorous treatment of this problem, without advancing assumptions beyond those made already, is to treat the entire universe of subsystem plus reservoir as a closed system unto itself. Within this setting, we once again carry out the same sort of counting arguments introduced in the previous section for an isolated system. However, unlike the previous case, we will derive expressions for the underlying thermodynamics which can be couched purely in terms of the degrees of freedom of only the subsystem. As a ﬁrst example, we consider the problem in which the subsystem and reservoir are free to exchange only energy, as is indicated schematically in ﬁg. 3.19. In this case, the number of microstates available to the subsystem is s (E s ), where the subscript s refers to the subsystem. Similarly, the number of microstates available to the reservoir is given by r (E − E s ). From the perspective of the composite universe made up of the system and its reservoir, the total energy is

3.3 Statistical Mechanics

123

Fig. 3.19. Composite system composed of a subsystem and a reservoir with which it is free to exchange energy.

constant, and the number of microstates available to that composite system when the subsystem has energy E s is given by composite (E; E s ) = s (E s )r (E − E s ). Here we have noted that the total number of states available to the composite system at a given E s is the product of the number of states available to the reservoir and those available to the subsystem. Note that the total number of microstates available to the composite system is gotten as tot (E) = s composite (E; E s ). Equilibrium between the reservoir and the subsystem is attained when the entropy is maximized, which corresponds to ﬁnding that distribution of energy between the subsystem and reservoir which corresponds to the largest number of total microstates. Within the microcanonical formalism presented in the previous section we asserted that all microstates are equally likely. In the present situation, we center our interest just on the subsystem. The price we pay for restricting our interest to the nonisolated subsystem is that we no longer ﬁnd all states are of equal probability. Though the states of the composite universe are all equally likely, we will ﬁnd that there is a calculable energy dependence to the probability for a given energy state for the subsystem. To make our analysis concrete, we begin by noting that if we consider the circumstance in which the subsystem is in a nondegenerate state of energy, E a (i.e. s (E a ) = 1), then the total number of states available to the composite universe of system plus reservoir is composite (E) = r (E − E a ). What we have done here is to identify the subset of states of the composite system that is consonant with the subsystem having deﬁnite energy E a . We continue with the observation that the probability P(E a ) of ﬁnding the system in this state is proportional to the number of microstates available to the reservoir. That is, P(E a ) ∝ r (E − E a ). The speciﬁc dependence of this probability on the energy E a can be garnered from the

124

3 Quantum and Statistical Mechanics Revisited

following argument. First, we note that as a consequence of the assertion made above we have r (E − E a ) eln[r (E−Ea )] P(E a ) = = ln[ (E−E )] . (3.90) b P(E b ) r (E − E b ) e r This equation notes that the ratio of the probabilities of ﬁnding the subsystem with two particular energies is equal to the ratios of the corresponding number of states available to the reservoir at the two energies of interest. The remainder of our analysis can be built around the presumed smallness of E a with respect to E itself, which affords an opportunity for Taylor expansion of the slowly varying logarithms in the form ∂ ln r (3.91) Ea . ln r (E − E a ) ln r (E) − ∂E Coupled with the thermodynamic identity that relates the temperature to the energy dependence of the entropy, namely, 1 ∂S 1 ∂ ln = = , (3.92) ∂E k ∂E kT we are left to conclude that 1 −(Ea /kT ) e , (3.93) Z where Z is an as-yet undetermined constant. In fact, for the practical purposes of everyday calculation, it is the ‘constant’ Z that depends on parameters such as T and V which is the basis of many calculations. This quantity, known as the partition function, is found by insisting that our probability distribution be suitably normalized, namely, 1 −(En /kT ) P(E n ) = e = 1. (3.94) Z n n P(E a ) =

This expression states that the partition function itself can be determined from knowledge of the energy levels via Z= e−(En /kT ) . (3.95) n

Our notation is meant to argue that the subsystem can have any of a number of different energies, labeled by the set of integers n. We would do well at this point to reﬂect on the preceding argument. Throughout, our derivation has rested on the central assertion upon which the microcanonical distribution is built, namely, that of the equal likelihood of all microstates consistent with the given macrostate. In this case, however, we have seen ﬁt to examine a subsystem in contact with a thermally rigid reservoir which can freely donate and receive energy

3.3 Statistical Mechanics

125

without altering its temperature. By examining, within a microcanonical setting, the properties of the composite universe of subsystem plus reservoir, we have been able to identify the unequal probabilities attached to the subsystem’s energy levels. What has emerged is a scheme in which only the parameters characterizing the subsystem need be considered. Having established the probability distribution that characterizes our subsystem when in contact with a reservoir, we now seek insights into the thermodynamic implications of this solution. As a ﬁrst example, suppose we are interested in determining the average energy of the subsystem. On the basis of the familiar notion of determining averages associated with a given probability distribution, it is immediate that 1 E n P(E n ) = E n e−(En /kT ) . (3.96) E = Z n n This expression may be considerably simpliﬁed on the recognition that we may deﬁne a variable β = 1/kT , and that

E n e−β En = −

n

1 ∂Z . Z ∂β

(3.97)

Hence, we have that E = −

∂ ln Z . ∂β

(3.98)

This result supports our contention that it is the partition function that serves as the analytic engine for calculating quantities of thermodynamic interest. The speciﬁc heat, which is a measure of the stiffness of the system to thermal ﬂuctuations, will emerge later as an additional material parameter which looks to microscopic models for its origins. Within the statistical mechanical formalism we have set up here, the speciﬁc heat may be easily determined on the recognition that C V = ∂E/∂ T |V . Upon exploiting the deﬁnition of β, this may be rewritten as C V = kβ 2

∂ 2 ln Z . ∂β 2

(3.99)

An alternative and more streamlined approach to the types of results described above emerges once we have made contact between the partition function and the Helmholtz free energy. Recall that thermodynamic quantities such as the pressure and entropy may be evaluated simply as derivatives of the Helmholtz free energy as ∂F ∂F , S=− . (3.100) p=− ∂V T ∂T V

126

3 Quantum and Statistical Mechanics Revisited

The connection of the partition function to the Helmholtz free energy is effected via the expression F = −kT ln Z .

(3.101)

This result is yet another example of an equation (like the Boltzmann expression for the entropy) which connects macroscopic and microscopic quantities. The origins of this equation can be obtained on the basis of thermodynamic reasoning and to probe these details the reader is encouraged to examine chap. 16 of Callen (1985) or the ﬁrst sections of Feynman (1972). In the following section we will examine how this machinery may be brought to bear on some model problems.

3.3.4 Information Theoretic Approach to Statistical Mechanics Until now, our treatment of statistical mechanics has been founded upon the assumption that this theory reﬂects the average treatment of the coupled microscopic degrees of freedom that make up a material. However, in this section we follow an alternative view in which it is held that statistical mechanics is not a physical theory at all, but is rather an example of a calculus of uncertainty in which inference in the face of incomplete information is put on a rigorous footing. Indeed, the Boltzmann factor introduced above has been used in problems ranging from image reconstruction to the analysis of time series data lending support to the claim that the fundamental ideas transcend their historical origins in physics. The central idea is that the algorithm of statistical mechanics is but one example of how reasoning should proceed when we are confronted with incomplete knowledge. The ideas associated with the information theoretic approach to statistical mechanics may be sketched as follows. We begin with the observation that our task is to infer the probability of the various microstates that the system is capable of adopting. From the macroscopic perspective, all that we may know about a system might be its mean energy, E. Given so little information about the distribution of microstates it seems brash to assume that anything deﬁnitive may be argued for. However, such problems form the province of probabilistic reasoning, and in conjunction with the ideas of information theory, much progress can be made. We follow Shannon in attaching a measure to the quality of our knowledge of a system’s disposition as revealed by the probability distribution that describes it. For an overview of these ideas, we refer the reader to Jaynes (1983). For example, if we consider the rolling of a die, the best we might do is to enumerate the six possible outcomes and to attribute to each an equal likelihood. This is low-quality information. On the other hand, if the die were loaded and we could say with certainty that only the face with a one would be revealed, our state of knowledge is of the highest quality.

3.3 Statistical Mechanics

127

Associated with a discrete probability distribution with N outcomes Shannon identiﬁes an entropy, H ( p1 , p2 , . . . , p N ), which lends quantitative weight to our intuitive notions about the quality of information associated with that distribution. The derivation of the particular functional form taken by H ({ pi }) is based on a few fundamental desiderata. First, given N possible outcomes, the case in which all such outcomes are equally likely will maximize the function H . This statement corresponds to our intuition that the case of equal likelihood of all outcomes corresponds to maximal ignorance. The probability distribution is featureless and there is nothing about it that inclines us to favor one outcome over any other. Secondly, if we now imagine increasing the number n of equally likely outcomes, the function H ({1/n}) should be a monotonically increasing function of n. This too jibes with our intuition that as the number of outcomes is increased, our knowledge is degraded. The ﬁnal requirement of the function H is based upon its additivity. If we specify the state of the system in two steps (i.e. there are n rooms, each of which contains m boxes), the reckoning of the information entropy must be consistent with the result of specifying all of the information at once (i.e. there are n ×m outcomes). On the basis of these few basic requirements, the claim is that the function H ( p1 , p2 , . . . , p N ) is uniquely determined and that it provides a measure of the information content of the probability distribution it characterizes. The outcome of the reasoning hinted at above is the claim that the function H is given by pi ln pi . (3.102) H ( p1 , p2 , . . . , p N ) = −k i

That is, if we are given a discrete probability distribution { pi }, the function H ({ pi }) provides a unique measure of the information content of that distribution. The beauty of this result is that it provides a foundation upon which to do inferential reasoning. In particular, when faced with the question of determining a probability distribution (such as, for example, in the context of constructing a statistical ensemble which gives the probabilities of various microstates), it gives us a way to determine the best distribution. As yet, we have said nothing of statistical mechanics, and it is just this fact that makes the information theoretic approach to inference of utility to X-ray crystallographers, radio astronomers attempting to decipher noisy data and statistical mechanicians alike. In light of the developments described above, the Gibbsian variational principle may be seen in a different light. The idea is that the maximization of entropy may be alternatively viewed as a statement of unbiased inference: choose that probability distribution that assumes nothing that is not forced on us by the data themselves. To see the workings of the maximum entropy approach, we begin with the trivial example of N outcomes with our only knowledge being the enumeration of the

128

3 Quantum and Statistical Mechanics Revisited

states themselves. In this case, our intuition anticipates the probability distribution in which all outcomes are equally likely. To see how this arises from the principle of maximum entropy, we maximize the augmented function pi ln pi + λ pi − 1 , (3.103) S = − i

i

where λ is a Lagrange multiplier used to enforce the constraint that the distribution be normalized. Also, we have absorbed the constant k into the Lagrange multiplier. Maximizing this function with respect to the pi s results in pi = eλ−1 , independent of i, revealing that all outcomes are equally likely. The determination of the constant is based on the recognition that i pi = 1, and yields pi = eλ−1 = 1/N . Note that we have provided theoretical justiﬁcation for the principle of equal a priori probabilities that was adopted earlier. We see that this is the best guess that can be made on our very limited data. The key point is that rather than asserting equal a priori probabilities as an article of faith we have shown that it is the best distribution that we can possibly assign in the sense that it most faithfully represents our degree of ignorance concerning the various outcomes. A more enlightening example is that in which not only is the constraint of normalization of the probability distribution imposed, but it is assumed that we know the average value of some quantity, for example, E = i E i pi (E i ). In this case, we again consider an augmented function, which involves two Lagrange multipliers, one tied to each constraint, and given by pi ln pi − λ pi − 1 − β pi E i − E . (3.104) S = − i

i

i

Note that once again the ﬁrst constraint imposes normalization of the distribution. Maximizing this augmented function leads to the conclusion that p j = e−1−λ−β E j . Imposition of the normalization requirement, j p j = 1, implies that 1 e−1−λ = e−β E j ,

(3.105)

j

which is consonant with our expectation that we should recover the partition function as the relevant normalization factor for the canonical distribution. A deeper question concerns the Lagrange multiplier β which is formally determined via the nonlinear equation E = −

∂ ln Z . ∂β

(3.106)

3.3 Statistical Mechanics

129

3.3.5 Statistical Mechanics Models for Materials Statistical Mechanics of the Harmonic Oscillator. As has already been argued in this chapter, the harmonic oscillator often serves as the basis for the construction of various phenomena in materials. For example, it will serve as the basis for our analysis of vibrations in solids, and, in turn, of our analysis of the vibrational entropy which will be seen to dictate the onset of certain structural phase transformations in solids. We will also see that the harmonic oscillator provides the foundation for consideration of the jumps between adjacent sites that are the microscopic basis of the process of diffusion. In light of these claims, it is useful to commence our study of the thermodynamic properties of the harmonic oscillator from the statistical mechanical perspective. In particular, our task is to consider a single harmonic oscillator in presumed contact with a heat reservoir and to seek the various properties of this system, such as its mean energy and speciﬁc heat. As we found in the section on quantum mechanics, such an oscillator is characterized by a series of equally spaced energy levels of the form E n = (n + 12 )h¯ ω. From the point of view of the previous section on the formalism tied to the canonical distribution, we see that the consideration of this problem amounts to deriving the partition function. In this case it is given by 1 ] ¯ e−[(n+ 2 )hω/kT . (3.107) Z= n

The contribution of the zero point energy can be factored out of the sum leaving us with ¯ ¯ e−n hω/kT , (3.108) Z = e−hω/2kT n ¯ which upon the substitution x = e−hω/kT is seen to be a simple geometric series and can be immediately summed to yield

Z=

¯ e−hω/2kT . ¯ 1 − e−hω/kT

(3.109)

As a result, we are left with the insight that the free energy of such an oscillator is given by h¯ ω ¯ + kT ln(1 − e−hω/kT ). (3.110) F= 2 This equation will arise in chap. 6 in the context of structural transformations in solids when it comes time to evaluate the contribution made by vibrations to the total free energy of a solid. As shown earlier, the thermodynamic properties of this system can be reckoned as derivatives of the logarithm of the partition function with respect to the inverse

130

3 Quantum and Statistical Mechanics Revisited

temperature. For example, the mean energy is given by E = −

h¯ ω h¯ ω ∂ ln Z = + hω/kT . ∂β 2 e¯ −1

(3.111)

This result should be contrasted with expectations founded on the classical equipartition theorem which asserts that an oscillator should have a mean energy of kT . Here we note two ideas. First, in the low-temperature limit, the mean energy approaches a constant value that is just the zero point energy observed earlier in our quantum analysis of the same problem. Secondly, it is seen that in the high-temperature limit, the mean energy approaches the classical equipartition result E= kT . This can be seen by expanding the exponential in the denominator ¯ −1 of the second term to leading order in the inverse temperature (i.e. ehω/kT h¯ ω/kT ). As a result, the mean energy is thus E (h¯ ω/2) + kT . With the presumed largeness of the temperature as revealed in the inequality h¯ ω/kT 1, this yields the classical equipartition result. These results will all make their appearance later in several different contexts including in our discussion of phase diagrams in chap. 6. Statistical Mechanics of the Ising Model. A tremendously important model within statistical mechanics at large, and for materials in particular, is the Ising model. This model is built around the notion that the various sites on a lattice admit of two distinct states. The disposition of a given site is represented through a spin variable σi which can take the values ±1, with the two values corresponding to the two states. With these ‘kinematic’ preliminaries settled, it is possible to write the energy (i.e. the Hamiltonian) as a function of the occupations of these spin variables as E Ising = Ji j σi σ j . (3.112) i j

In its simplest form, we can take the coupling constants Ji j as being equal so that the energy may be rewritten as E Ising = J i j σi σ j and further we restrict our attention to the near-neighbor variant of this model in which only spins on neighboring sites interact. At this point, we see that the physics of this model is determined in large measure by the sign of J , with J > 0 favoring those states in which adjacent sites are unlike, whereas when J < 0, the energy favors alignment of neighboring spins. The statistical mechanics of this model surrounds the question of the competition between the energy which favors an ordering of the various spins and the entropy term in the free energy which favors a disordering of the arrangement of spins. Before entering into questions concerning the ‘solution’ of this model, we should ﬁrst recount some of the uses to which it has been put and to foreshadow its

3.3 Statistical Mechanics

131

signiﬁcance to our endeavor. The Ising model has enormous signiﬁcance beyond the limited range of applications it has in modeling materials. Nevertheless, even for what we will want to say, the Ising model will often serve as a paradigm for the analysis of a wide range of problems in materials modeling. In chronological terms, the Ising model will see duty as the basis for our analysis of phase diagrams, the various stacking arrangements that arise in the so-called polytypes, some of our discussion of surface reconstructions and will provide a foundation for the use of the Potts model in the analysis of grain growth. Though the Ising model is amenable to full analytic solution in one and two dimensions, we will make use of it in the more general three-dimensional setting and will therefore have to resort to either analytic approximations or full numerics to really probe its implications. On the other hand, examination of this model in the reduced dimensionality setting can be very revealing to illustrate the various tools of statistical mechanics in action. In addition, the reduced dimensionality problems will also help foreshadow the difﬁculties we shall face in confronting the three-dimensional problem that will arise in the consideration of phase diagrams, for example. As has already been noted throughout this chapter, the engine for our analysis of the thermodynamic properties of a given model is the partition function, which for the Ising model may be written as ··· exp(−β Ji j σi σ j ). (3.113) Z= σ1 =±1

σ N =±1

ij

The sums in front of the exponential are an instruction to consider all possible 2 N conﬁgurations of the N -spin system. For the one-dimensional case, there are a variety of possible schemes for evaluating the partition function, and thereby the thermodynamics. One appealing scheme that illustrates one of the themes we will belabor repeatedly is that of degree of freedom thinning in which degrees of freedom are eliminated by integrating over particular subsets of the full set of degrees of freedom. Indeed, in chap. 12, we will attempt to make generic comments on strategies for eliminating degrees of freedom. In the present case, the idea is to evaluate the partition sum explicitly for half the spins. For example, we can elect to integrate over the even-numbered spins, resulting in an effective Hamiltonian in which only the odd-numbered spins appear explicitly, though at the price of introduction of new coupling parameters in the model. An instructive description of this procedure may be found in Maris and Kadanoff (1978), whom we follow below. To see the idea in practice, the partition function of eqn (3.113) is reorganized as ··· e K (σ1 σ2 +σ2 σ3 ) e K (σ3 σ4 +σ4 σ5 ) · · · , (3.114) Z= σ1 =±1

σ N =±1

132

3 Quantum and Statistical Mechanics Revisited

where the constant K = J/kT has been introduced. We may now sum over the spins with even labels, resulting in · · · (e K (σ1 +σ3 ) + e−K (σ1 +σ3 ) )(e K (σ3 +σ5 ) + e−K (σ3 +σ5 ) ) · · · . (3.115) Z= σ1 =±1 σ3 =±1

The goal is to seek a scheme to rewrite this result that takes precisely the same form as the original partition function. In concrete terms, this implies that we seek an f (K ) such that

e K (σi +σi+2 ) + e−K (σi +σi+2 ) = f (K )e K σi σi+2 .

(3.116)

Note that this equation involving the unknown function f (K ) must be true whatever our choices for σi = ±1 and σi+2 = ±1 may be. In particular, for σi = σi+2 = 1, this becomes

e2K + e−2K = f (K )e K ,

(3.117)

while for σi = −σi+2 , eqn (3.116) becomes

2 = f (K )e−K .

(3.118)

Eqns (3.117) and (3.118) may now be solved for f (K ) and K with the result that 1 f (K ) = 2 cosh 2 2K and K = 12 ln cosh 2K . Note that in the more formidable setting in higher dimensions, the degree of freedom thinning procedure leads to equations for the ‘renormalized’ coupling constant (i.e. K ) that may be treated only approximately. The result obtained above leads now to the key insight of the analysis, namely, the relation between the partition functions of the system with N degrees of freedom and that of the thinned down model involving only N /2 degrees of freedom. Using our new found results for the constant K and the function f (K ), we may relate these partition functions as N

Z (N , K ) = [ f (K )] 2 Z (N /2, K ),

(3.119)

where the dependence of the partition function on both the number of degrees of freedom and the the coupling constant has been made explicit. The next step in the argument is the recognition that the free energy (i.e. F = −kT ln Z ) scales with the system size and thus we may write, ln Z = N ζ (K ). Taking the logarithm of eqn (3.119) and using the fact that ln Z (N , K ) = N ζ (K ), results in 1

ζ (K ) = 2ζ (K ) − ln[2 cosh 2 (2K )].

(3.120)

What is the good of this set of results? The key point is the identiﬁcation of a recursive strategy for obtaining the partition function. In particular, in the present setting, we note that in the high-temperature limit, Z = 2 N resulting in the

3.3 Statistical Mechanics

133

observation that ζ (K → 0) = ln 2. On the basis of the knowledge of ζ (K ) at this particular point, we can now iterate to determine the functions of interest at other points in parameter space. Our discussion of the Ising model was primarily intended to introduce the physics of the model itself. However, because of its conceptual relevance to many of the strategies to be adopted later in the book, we have also illustrated the use of real space renormalization group ideas for degree of freedom thinning. We note again that our later uses of the Ising model will be for problems in which exact analytic progress is presently unavailable, and for which either approximate or numerical procedures will be resorted to. Statistical Mechanics of Electrons. Later in the book, we will repeatedly require insights into the generalization of the arguments made earlier in the context of the electron gas for ﬁlling up energy states at ﬁnite temperatures. Recall our discussion of the electron gas given earlier in which all states with wavevectors |k| ≤ k F were unequivocally occupied and those with |k| > k F were unequivocally not occupied. This picture must be amended at ﬁnite temperatures, since in this case, by virtue of thermal excitation, some fraction of electrons will ﬁll states of higher energy. The distribution which governs the ﬁnite temperature distribution of electrons is the so-called Fermi–Dirac distribution, and it is that distribution (both its derivation and signiﬁcance) that occupies our attention presently. The ﬁrst question we pose is of wider generality than is needed to consider the question of electron occupancies. In particular, we ask for the relevant probability distribution for those problems in which not only is the average value of the energy prescribed, but so too is the average number of particles, N . In this case, using the maximum entropy ideas introduced above, the entropy and its associated constraints may be written as pi ln pi − λ pi − 1 − β pi E i − E − α pi Ni − N . S =− i

i

i

i

(3.121) The index i is a superindex that refers to a particular realization of both E and N . If we now follow the same procedure used earlier to derive the canonical distribution by maximizing the entropy, it is found that the resulting probabilities are of the form 1 (3.122) pi = P(E, N ) = e−β(E−µN ) . Z In this case, we have introduced the Gibbs sum deﬁned as e−(E−µN )/kT . Z= states

(3.123)

134

3 Quantum and Statistical Mechanics Revisited

Fig. 3.20. Fermi–Dirac distribution for several different temperatures.

Note that the passage from the formal result based on information theoretic reasoning to the physical setting of interest here involved the recognition of the Lagrange multiplier α being related to the chemical potential through α = µ/kT . The results obtained above are of such general importance when applied to the case of electrons (more generally to fermions) that the resulting distribution has its own nomenclature and is referred to as the Fermi–Dirac distribution. To see how eqn (3.122) is applied to determine the average number of particles in a given quantum state when the particles themselves obey the Pauli principle, we consider a particular electronic state with energy . In this case, the Gibbs sum is of the form Z = 1 + e−β(−µ) .

(3.124)

The reasoning behind this assertion is the statement that there are only two allowed states to consider: the state is unoccupied (E = 0, N = 0) and the state is occupied by a single particle (E = , N = 1). As a result, the mean occupancy of this state is obtained as 1 e−β(−µ) = β(−µ)+1 , (3.125) N () = −β(−µ) 1+e e which is the sought after Fermi–Dirac distribution which presides over questions of the occupancy of electron states at ﬁnite temperatures. In ﬁg. 3.20, we show this distribution for several different temperatures. For ease of plotting, we have rescaled variables so that the Fermi–Dirac distribution is written in the form 1 , (3.126) N ( f, βµ) = βµ( f −1) e +1

3.3 Statistical Mechanics

135

where f has been introduced as a way of characterizing what fraction the energy of interest is of the energy µ. It is evident from the ﬁgure that at low temperatures (i.e. βµ 1) we recover the results of our earlier analysis, namely, that all states with energy lower than F (note that F is the zero temperature µ, i.e. F = µ(0)) are occupied while those above this energy are not. On the other hand, we also see that at higher temperatures there is a reduction in the mean occupancy of states with energy below F and a corresponding enhancement in the occupancy of those states just above F . 3.3.6 Bounds and Inequalities: The Bogoliubov Inequality There are many instances in which an exact analytic solution for the partition function (or the free energy) will be beyond our reach. One notable example that will arise in chap. 6 is that of the free energy of a liquid. In such instances, there are several related strategies that may be adopted. It is possible to adopt perturbative approaches in which the statistical mechanics of the unperturbed state is in hand, and approximations for the problem of interest are arrived at through a series of systematic corrections. A related approach is the attempt to bound the exact free energy through the use of robust inequalities such as the Bogoliubov inequality to be introduced below. With this principle in hand, the bounds can be variationally improved by introducing free parameters in the ‘reference’ Hamiltonian, which are then chosen to yield the best possible bound. The basic idea is as follows: we assume that the free energy of real interest is that associated with a Hamiltonian H , for which the exact calculation of the free energy is intractable. We then imagine an allied Hamiltonian, denoted H0 , for which the partition function and free energy may be evaluated. The inequality that will serve us in the present context asserts that Fexact ≤ F0 + (H − H0 )0 ,

(3.127)

where the average on the right hand side is evaluated with respect to the distribution that derives from the Hamiltonian H0 . What this inequality teaches us is that if we can ﬁnd an approximate Hamiltonian for which we can evaluate the partition function, then we can provide bounds on the free energy of the system described by the full H = H0 + H1 , where we have introduced the notation H1 to describe the perturbation that is added to the original H0 . Presently, we consider a few of the details associated with the derivation of the Bogoliubov inequality. Our treatment mirrors that of Callen (1985) who, once again, we ﬁnd gets to the point in the cleanest and most immediate fashion. As said above, we imagine that the problem of real interest is characterized by a Hamiltonian H which may be written in terms of some reference Hamiltonian H0

136

3 Quantum and Statistical Mechanics Revisited

Fig. 3.21. Schematic of the free energy as a function of the parameter λ discussed in the context of the Bogoliubov inequality.

as H (λ) = H0 + λH1 ,

(3.128)

where λ is a tunable parameter which weights the contribution of the perturbation to the reference Hamiltonian. We introduce the notation Z = tr e−β H , with the symbol tr referring to the trace operation, though it should be read as ‘sum over all conﬁgurations’. Evaluation of the derivatives of the exact free energy Fexact (λ) = −kT ln tr e−β H with respect to λ reveal that d Fexact = H1 , dλ

(3.129)

d 2 Fexact = −β(H1 − H1 )2 . dλ2

(3.130)

The signiﬁcance of the latter equation is that it demonstrates that for all λ, the curvature of the function Fexact (λ) is negative. Why should this observation ﬁll us with enthusiasm? The relevance of this insight is revealed graphically in ﬁg. 3.21, where it is seen that we may construct an approximate free energy (a ﬁrst-order Taylor expansion in powers of λ) of the form d Fexact λ, (3.131) Fapprox (λ) = Fexact (λ = 0) + dλ λ=0 which is guaranteed to satisfy the inequality Fexact (λ = 1) ≤ Fapprox (λ = 1), by virtue of what we have learned about the curvature of the function Fexact (λ).

3.3 Statistical Mechanics

137

What has been done, in essence, is to exploit our certainty about the sign of the curvature of the free energy with respect to λ to carry out a Taylor expansion of that free energy with respect to λ on the hope that the leading order expansion will be sufﬁciently accurate. Note that when the slope of Fexact (λ) is evaluated explicitly, we ﬁnd tr H1 e−β(H0 +λH1 ) d Fexact = , (3.132) dλ tr e−β(H0 +λH1 ) which for the special case of λ = 0 yields d Fexact = H1 0 , dλ

(3.133)

where H1 0 signiﬁes the evaluation of the average value of H1 (or H − H0 ) with respect to the distribution function arising only from the reference Hamiltonian. The implication of these results is that with only a knowledge of the distribution function for the reference state, we are able to put bounds on the exact free energy. To see this mathematically, we plug the result of eqn (3.133) into eqn (3.131) with the result that Fexact ≤ Fexact (λ = 0) + H − H0 0 .

(3.134)

Recall that Fexact (λ = 0) is nothing more than the free energy associated with the Hamiltonian H0 which, by hypothesis, we know how to compute. As a result, we have demonstrated the existence of the sought after bound on the exact free energy. The ﬁnishing touches are usually put on the analysis by allowing the reference Hamiltonian to have some dependence on adjustable parameters that are determined to minimize the right hand side of eqn (3.134). We note that as a result of this scheme, the better the choice of H0 , the higher will be the quality of the resulting variational estimate of the free energy.

3.3.7 Correlation Functions: The Kinematics of Order Conventional kinematic notions are built around the idea that the system of interest can be characterized by a series of simple states without any reference to microscopic ﬂuctuations or disorder. On the other hand, in the analysis of systems at ﬁnite temperature or in the presence of the effects of disorder, it is essential to build up measures that characterize the disposition of the system while at the same time acknowledging the possibility of an incomplete state of order within that system. Just as strain measures served as the primary kinematic engine used in our analysis of continua, the notion of a correlation function will serve to characterize the disposition of those systems that are better thought of statistically. Indeed, we will ﬁnd that in problems ranging from the ‘spins’ introduced earlier in conjunction

138

3 Quantum and Statistical Mechanics Revisited

with the Ising model, to the density (and its ﬂuctuations), and even to the heights on fracture surfaces, correlation functions provide a quantitative language for describing the statistical state of systems with many degrees of freedom. As is already evident from the discussion of this chapter, many-particle systems are often described in terms of averages over microscopic variables. For example, the net magnetization M of a spin system can be thought of as an average of the form M = N µσi , where N is the total number of spins per unit volume, µ is the magnetic moment per spin and σi is the spin variable at site i. The notion of the correlation function is introduced in light of the knowledge that by virtue of the dynamics of the microscopic variables, the macroscopic variables themselves are subject to ﬂuctuations. The extent of these ﬂuctuations is conveniently quantiﬁed using the notion of the correlation function which achieves a greater signiﬁcance because of its relation to the response of a system to external probes, including the scattering of X-rays, electrons or neutrons. The basic idea is to quantify the extent to which the behavior of a particular microscopic quantity such as the spin at site i, σi , is correlated with that of the spin σ j at site j. By deﬁnition, the pair correlation function of σi and σ j is deﬁned by Ci j = σi σ j − σi σ j .

(3.135)

What we note is that if the joint probability distribution P(σi , σ j ) is of the form P(σi , σ j ) = P(σi )P(σ j ), then σi σ j = σi σ j , the spins are uncorrelated, and correspondingly, the correlation function Ci j vanishes. The importance of correlation functions as a way of characterizing systems with many degrees of freedom can be argued for from a number of different angles, but here we simply note that a knowledge of such functions serves as a basis for computing ‘susceptibilities’ of various types in a number of different systems, and can be thought of as providing a kinematics of order. From a structural perspective, these ideas can be couched in slightly different terms by considering the two-particle distribution function deﬁned by ρ (2) (r1 , r2 ) = δ(r1 − ri )δ(r2 − r j ) . (3.136) i= j

The two-particle distribution tells us the probability that particles will be found at r1 and r2 and will thereby serve as the basis for determining the energy of interaction between different pairs of particles when the best statements we can make about the system are statistical. For example, when describing the energetics of liquids our statements about the structure of that liquid will be couched in the language of distribution functions. In preparation for our later work on the free energy of liquids (see chap. 6), we ﬁnd it convenient to introduce an auxilliary

3.3 Statistical Mechanics

139

quantity, the pair correlation function g(r1 , r2 ), which is deﬁned through ρ (2) (r1 , r2 ) = ρ(r1 )ρ(r2 )g(r1 , r2 ).

(3.137)

This deﬁnition simplifes considerably in the case of an isotropic liquid for which the single particle density is a constant (i.e. ρ(r) = N /V ), resulting in the radial distribution function g(r ). As said above, these deﬁnitions will form a part of our later thinking.

3.3.8 Computational Statistical Mechanics As yet, we have described some of the analytic tools that are available to forge a statistical connection between macroscopic observables and the microstates that lead to them. The advent of high-speed numerical computation opened up alternative strategies for effecting this connection which permitted a literal interpretation of the notion of an average. The key idea is to allow the system to visit a sequence of microscopic ‘realizations’ of the macroscopic state of interest. By effecting an average for the quantity of interest over the various members in this set of realizations, the statistical average of interest is performed explicitly. On the one hand, molecular dynamics obtains average quantities by repeatedly evaluating the dynamical variable of interest as it takes on a succession of values as the system winds through phase space. Alternatively, Monte Carlo methods allow for construction of copies of a particular system that one envisions in speaking of the ‘ensemble averages’ of Gibbs. In this case, rather than explicitly tracking the system along some trajectory through phase space, we imagine an ensemble of copies of the system of interest, each corresponding to some different microstate and which are representative members of the set being averaged over. In both the molecular dynamics and Monte Carlo methods, the mentality is to construct explicit microscopic realizations of the system of interest in which once the microscopic degrees of freedom have been identiﬁed and the nature of their interaction understood, one explicitly constructs some subset of the allowable microstates and performs averages over them. In this part of the chapter, our aim is to describe a few of the highlights of both the molecular dynamics and Monte Carlo approaches to computational statistical mechanics. We begin with a review of the notion of microstate, this time with the idea of identifying how one might treat such states from the perspective of the computer. Having identiﬁed the nature of such states, we will take up in turn the alternatives offered by the molecular dynamics and Monte Carlo schemes for effecting the averages over these microstates. As noted in the preface, the availability of computers has in many cases changed the conduct of theoretical analysis. One of the ﬁelds to beneﬁt from the emergence

140

3 Quantum and Statistical Mechanics Revisited

Fig. 3.22. Wandering of a Ag adatom on the Ag(111) surface as revealed using molecular dynamics (adapted from Boisvert and Lewis (1996)).

of powerful computational alternatives to traditional analytic approaches is that of statistical mechanics. If we follow the line of reasoning suggested by molecular dynamics, the argument is made that the averages of interest can be realized by following the system in its trajectory in phase space via the expression 1 T At = A({ p(t), q(t)})dt. (3.138) T 0 In this case, our notation indicates that we are considering the time average ( t ) of the quantity A which itself is a function of the dynamical variables. Those variables are represented here generically by q(t) and p(t),with q a conﬁgurational coordinate and p the associated momentum. The averaging process is tied to the type of trajectory indicated schematically in ﬁg. 3.22, where we have artiﬁcially reduced the problem to a two-dimensional scenario that allows for visualization. Molecular dynamics provides a scheme for explicitly evaluating these averages by computing A at various time intervals while allowing the particles to range over the trajectories resulting from their respective equations of motion. In the simplest classical terms, carrying out a molecular dynamics simulation involves a few key steps. First, it is necessary to identify some force law that governs the interactions between the particles which make up the system. The microscopic origins of the force laws themselves will be taken up in chap. 4, and for the moment we merely presuppose their existence. It is then imagined that these particles evolve under their mutual interactions according to Newton’s second law of motion. If we adopt the most naive picture in which all of the atoms are placed in a closed box at ﬁxed energy, we ﬁnd a set of 3N coupled second-order ordinary

3.3 Statistical Mechanics

141

differential equations of the form d 2 ri = Fi . (3.139) dt 2 A host of clever schemes have been devised for integrating these equations of motion in a manner that is at once efﬁcient and stable. One well-known integration scheme is that of Verlet (though we note that more accurate methods are generally used in practice). One notes that for a sufﬁciently small time step, the position at times t ± δt may be expressed as mi

1 d 2 ri 2 dri δt + δt . dt 2 dt 2 By adding the two resulting expressions and rearranging terms, we ﬁnd ri (t ± δt) ≈ ri (t) ±

(3.140)

d 2 ri 2 δt . (3.141) dt 2 Though there are a variety of sophisticated schemes for carrying out the integrations required here, we choose to emphasize the physical insights gained thus far. The choice of a time step δt strikes to the heart of one of the key difﬁculties in carrying out the types of simulations advocated here. The processes of interest to the mechanics of materials involve a broad range of time scales. At the smallest end of that spectrum, we have the time scale associated with atomic vibrations. Clearly, if we are to simulate the thermal properties of solids, the time step must be a small fraction of the vibrational period. By way of contrast, if our aim is the investigation of deformation processes that are slaved to mass transport, the time scale can be many orders of magnitude larger than the picosecond scale associated with thermal vibrations, resulting in a gross mismatch between the time step required for carrying out temporal integrations, and the time scale associated with the process of interest. This question will be addressed in chap. 12 when we describe the hyperdynamics method. In addition to questions surrounding the treatment of multiple time scales, another intriguing problem is posed by simulating a system in contact with a thermal reservoir. Until now, we have envisaged a system that is maintained at ﬁxed total energy. In many cases, one would rather mimic a system at ﬁxed temperature. One of the more interesting aspects of molecular dynamics is the role of effective theories for mimicking the presence of either thermal or pressure reservoirs. The point is that through the trick of incorporating a single extra set of conjugate variables, the effect of a thermal reservoir may be accounted for rigorously while maintaining the Hamiltonian description of the underlying dynamics. The approach we will follow here was pioneered by Nos´e (1984) and Hoover (1985). ri (t + δt) = −ri (t − δt) + 2ri (t) +

142

3 Quantum and Statistical Mechanics Revisited

Nos´e argues that the presence of the thermal reservoir may be accounted for in the Hamiltonian context by incorporating an additional set of conjugate variables, {s, ps }. The Hamiltonian for the extended system is given by H=

p2 ps2 i + gkT ln s. + V ({q }) + eff i 2ms 2 2Q i

(3.142)

For the present purposes, all that we really wish to note is that in light of this Hamiltonian, it becomes possible to carry out averages that are effectively those associated with a canonical ensemble, or said differently, with a system maintained at a temperature T . These ideas are described very nicely in Frenkel and Smit (1996). As already mentioned, an alternative to the explicit contemplation of microscopic trajectories is the construction of a stochastic approach in which various microscopic realizations of a system are constructed so as to respect the underlying distribution. Much has been made of the necessity of ergodic assumptions in statistical mechanics which allow for a replacement of the type of temporal average described above by the alternative ensemble averages immortalized by Gibbs. Here the idea is that rather than following the system on its excursions through phase space, one generates a series of macroscopically equivalent copies of the system, and averages over the members of this ‘ensemble’. For example, if our interest is in the thermodynamic properties of an alloy with constituents A and B, we can imagine generating alternative occupations of the various crystal lattice sites on the basis of random occupancy. Two snapshots corresponding to different members of the ensemble under consideration here were shown in ﬁg. 3.16. The underlying physical contention is the equivalency of the averaging process when effected either via the ensemble trick introduced above or by following the system as it ranges over its dynamic trajectory. Besides providing the foundation on which Monte Carlo methods are built, we have seen that the ensemble picture serves as the basis for much of the analytic machinery which is used to conduct the investigations of statistical mechanics. if one generates a sequence of states based upon the rule that a given state is ‘accepted’ with probability 1 if the new state lowers the energy and with probability e−βE is the new state increases the energy, then the resulting distribution will be canonical. For further details, I am especially fond of the discussion of Frenkel and Smit (1996). 3.4 Further Reading Quantum Mechanics Principles of Quantum Mechanics by R. Shankar, Plenum Press, New York: New York, 1980. A personal favorite on the subject of quantum mechanics. Shankar

3.4 Further Reading

143

does a ﬁne job of integrating the mathematical formalism and physical principles of quantum mechanics with their roots in many of the historical ideas of classical mechanics. His discussion of path integral methods is enlightening and readable. Quantum Theory by David Bohm, Prentice-Hall, Inc., Englewood Cliffs: New Jersey, 1951. Bohm’s book brings both clarity and completeness to many of the features of quantum mechanics that are of importance for the work carried out in the present book. Quantum States of Atoms, Molecules and Solids by M. A. Morrison, T. L. Estle and N. F. Lane, Prentice-Hall, Inc., Englewood Cliffs: New Jersey, 1976. Not a well-known book, but one I like very much as it has much that is practical to offer concerning the application of quantum mechanics to understanding bonding in solids. Thermodynamics and Statistical Mechanics E. T. Jaynes: Papers on Probability and Statistics edited by R. D. Rosenkranz, D. Reidel Publishing Company, Dordrecht: The Netherlands, 1983. The presence of this work on the list reﬂects my enormous prejudice in favor of the information theoretic approach to statistical mechanics as pioneered by Edwin T. Jaynes. This book is one of my prize possessions and at the time of this writing has no trace of its original hardback cover as a result of the many trips the book has made. Statistical Mechanics by R. P. Feynman, The Benjamin/Cummings Publishing Company, Inc., Reading: Massachusetts, 1972. This book bears the usual stamp of Feynman’s idiosyncratic approach to physics. There are many perspectives to be found here that will not be found elsewhere. States of Matter by D. L. Goodstein, Prentice-Hall, Inc., Englewood Cliffs: New Jersey, 1975. This often humorous book is full of insights into everything from the meaning of the partition function to the origins of Bragg scattering. Principles of Statistical Mechanics by A. Katz, W. H. Freeman and Company, San Francisco: California, 1967. This book remains virtually unknown, but again reﬂects my own taste for the information theoretic perspective. This book offers some hints as to the possible uses of this perspective to build more complete theories of nonequilibrium processes. Thermodynamics and an Introduction to Thermostatics by H. B. Callen, John Wiley and Sons, New York: New York, 1985. The perceptive reader will recognize on short order my own afﬁnity for the book of Callen. His treatment of the central ideas of both thermodynamics and statistical mechanics is clean and enlightening, and I share the author’s view that classical thermodynamics is primarily a theory of thermostatics.

144

3 Quantum and Statistical Mechanics Revisited

Fundamentals of Statistical Mechanics, Manuscript and Notes of Felix Bloch, prepared by John Dirk Walecka, Stanford University Press, Stanford: California, 1989. I have found this book eminently readable and interesting. ‘The Expanding Scope of Thermodynamics in Physical Metallurgy’ by J. W. Cahn, Materials Transactions, JIM, 35, 377 (1994). Cahn’s article is full of interesting ideas concerning both the signiﬁcance of previous thermodynamic achievements and the possible expansion of thermodynamic ideas to novel ways of treating interfaces and lattice effects.

Computational Statistical Mechanics Understanding Molecular Simulation by Daan Frenkel and Berend Smit, Academic Press, San Diego: California, 1996. An extremely serious book written at a high level and full of detailed insights. The Art of Molecular Dynamics Simulation by D. C. Rapaport, Cambridge University Press, Cambridge: England, 1995. This book gives a modern introduction to the subject of computer simulation, with special reference to molecular dynamics. ‘The Virtual Matter Laboratory’, M. J. Gillan, Contemporary Physics, 38, 115 (1997) provides an overview of some of the key ideas associated with the use of the ideas presented in this chapter as the basis of simulations of the properties of matter.

3.5 Problems

1 Particle in a Box by the Finite Element Method Flesh out the details of the discussion of the use of the ﬁnite element method to solve the problem of a particle in a box. In particular, derive eqns (3.44), (3.46), (3.48), (3.50) and table 3.1.

2 Finite Elements and the Schr¨odinger equation In this chapter, we discussed the use of the ﬁnite element method to solve the Schr¨odinger equation. Use the same formalism to solve the Schr¨odinger equation for a quantum corral of elliptical shape.

3.5 Problems

145

Fig. 3.23. Two three-atom conﬁgurations to be considered in problem 4.

3 Two-Dimensional Electron Gas Construct a two-dimensional analog of the electron gas model developed in this chapter. Begin by solving the relevant Schr¨odinger equation and obtaining the set of discrete energy eigenvalues. Assume that in the square box of area A there are N free electrons. Obtain the electronic energy by ﬁlling up the various energy states. How does the resulting energy depend upon the density?

4 Tight-Binding Model of Three-Atom Molecules Using the arguments introduced earlier for considering the H2 molecule, consider two separate three-atom conﬁgurations and their associated binding energies. In particular, consider both a three-atom chain with near-neighbor interactions as well as an equilateral triangle geometry as shown in ﬁg. 3.23. Use the same basis (i.e. one s-orbital per atom) and maintain the notation introduced earlier, namely, that i|H | j = h. Construct the appropriate 3 × 3 Hamiltonian matrices for these two different geometries and ﬁnd their corresponding eigenvalues. Fill up the lowest lying energy states and thereby ﬁnd the electronic contribution to the binding energies of both conﬁgurations in the case in which there is one electron per atom.

5 The Stirling Approximation Revisited To obtain an explicit analytic expression for the entropy of mixing as shown in eqn (3.89), we exploited the Stirling approximation. Plot both the exact and the approximate entropy (as gotten from the Stirling approximation) for systems of size N = 10, 100 and 1000.

6 Statistical Mechanics of a Two-Level System Consider a system characterized by two distinct energy levels, 0 and 0 + . Write down the partition function and compute the average energy and speciﬁc heat for this system.

146

3 Quantum and Statistical Mechanics Revisited

7 Entropy Maximization and the Dishonest Die In this problem we will examine the way in which maximum entropy can be used to confront a problem in incomplete information. The basic idea is that we are told that the mean value that emerges after many rolls of a die is 4.5. On this information, we are urged to make a best guess as to the probability of rolling a 1, 2, 3, 4, 5 and 6. Apply the principle of maximum entropy in order to deduce the probability p(n) by applying the constraint 4.5 = n np(n). 8 Partition Function for the One-Dimensional Ising Model For the one-dimensional Ising model with near-neighbor interactions with a Hamiltonian of the form (i.e. zero ﬁeld) J σi σ j , (3.143) H= i j

compute the partition function, the free energy and the average energy. 9 Statistical Mechanics of the Harmonic Oscillator In the text we sketched the treatment of the statistical mechanics of the harmonic oscillator. Flesh out that discussion by explicitly obtaining the partition function, the free energy, the average energy, the entropy and speciﬁc heat for such an oscillator. Plot these quantities as a function of temperature. 10 Monte Carlo Treatment of the Ising Model Write a computer program that allows for the Monte Carlo simulation of the two-dimensional Ising model. The program should use periodic boundary conditions. Generate representative conﬁgurations at a number of different temperatures and attempt to deduce the nature of the phase transition found as a function of temperature. To monitor the state of the system, evaluate the average spin on each site as a function of temperature. In addition you may wish to monitor the values of spin correlation functions such as were described in section 3.3.7.

Part two Energetics of Crystalline Solids

FOUR

Energetic Description of Cohesion in Solids

4.1 The Role of the Total Energy in Modeling Materials A recurring theme in the study of materials is the connection between structure and properties. Whether our description of structure is made at the level of the crystal lattice or the defect arrangements that populate the material or even at the level of continuum deformation ﬁelds, a crucial prerequisite which precedes the connection of structure and properties is the ability to describe the total energy of the system of interest. In each case, we seek a function (or functional) such that given a description of the system’s geometry, the energy of that system can be obtained on the basis of the kinematic measures that have been used to characterize that geometry. As we have discussed earlier (see chap. 2), the geometry of deformation may be captured in a number of different ways. Microscopic theories are based upon explicitly accounting for each and every atomic coordinate. Alternatively, a continuum description envisions a sort of kinematic slavery in which the motion of a continuum material particle implies the associated evolution of large numbers of microscopic coordinates. From the standpoint of microscopic theories, the computation of the total energy requires a description in terms of the atomic positions. In this instance, we seek a reliable function E tot ({Ri }), where {Ri } refers to the set of all nuclear coordinates and serves to describe the geometry at the microscale. For a more complete analysis, this picture should reﬂect the electronic degrees of freedom as well. By way of contrast, a description in terms of a continuum model often results in a phenomenological treatment of the total energy in which the energy is postulated to vary in accordance with some functional of the relevant strain measures. Here we seek a functional E tot [F] which relates the spatially varying deformation ﬁeld and the attendant energy. Note that in accordance with the distinction made between interesting and uninteresting motions in chap. 2, the energy of deformation should depend only on relative motions of material particles. As will become evident 149

150

4 Energetic Description of Cohesion in Solids

in this and subsequent chapters, there are a variety of means for describing the energetics of deformation, each with its own merits and advantages. It is of special interest to uncover the way in which insights at the microscopic scale can be bootstrapped for use at scales normally reserved for continuum approaches. As mentioned above, the total energy often serves as the point of entry for the analysis of material behavior. To whet our appetite for subsequent developments and to illustrate how the total energy impacts material properties we consider three different examples; the elastic moduli, the diffusion constant and the so-called gamma surface. As was already made clear in chap. 2, the elastic moduli are the phenomenological cornerstone of the linear theory of elasticity. Given these parameters, one is positioned to evaluate the stored energy of an arbitrary state of deformation so long as the displacement gradients are not too large. In chap. 5, we will show how by exploiting an analogy between the microscopic and macroscopic descriptions of the total energy the elastic moduli themselves may be computed strictly on the basis of microscopic considerations such as those that form the backbone of this chapter. The basic idea is founded on the recognition that for small deformations, the stored energy is quadratic in the appropriate strain measure. In addition to their ability to probe the energy cost for small excursions from some reference state, microscopic calculations can also be used to examine the energetics of large homogeneous deformations. This type of behavior is indicated schematically in ﬁg. 4.1. By exploiting a series of total energy calculations at the microscopic scale, each associated with a different overall state of strain, the curvature of the energy about the minimum may be determined and thus the moduli. Just as the elastic moduli characterize the properties of a material in the context of elastic boundary value problems, the diffusion coefﬁcient serves as the phenomenological basis for solving boundary value problems involving mass transport. In chap. 7, we will explicitly evaluate the diffusion constant on the basis of microscopic arguments. To do so, we will require an energetic analysis of certain saddle point conﬁgurations on a multi-dimensional potential energy surface. To compute them one must have solved the problem posed in this chapter: given a certain geometric conﬁguration, what is the total energy? For the problem of diffusion, it is the energy as a function of the diffusing atom’s position, also known as the ‘reaction coordinate’, that determines the diffusion rate. This type of analysis is indicated in ﬁg. 4.2 where the energy of a Pb adatom on a Ge surface is computed for a series of different adatom positions. These calculations were carried out using the types of ﬁrst-principles techniques to be described at the end of this chapter. In section 12.3.4, we will discuss a wide class of constitutive models that are broadly known as cohesive surface models. These models postulate the existence of an elastic potential that can be used to describe sliding and opening of interfaces.

4.1 The Role of the Total Energy in Modeling Materials

151

Fig. 4.1. Energy as a function of shear deformation in Al (adapted from Mehl and Boyer (1991)). The lattice parameter a is ﬁxed during the deformation and hence the energy characterizes a oneparameter family of deformations of the fcc lattice, with the members of the family parameterized by b.

Fig. 4.2. Energy of a diffusing adatom as a function of reaction coordinate (after Kaxiras and Erlebacher (1994)).

In the context of the mechanics of materials, such analyses are of value in describing both plasticity and fracture. What will be required in the determination

152

4 Energetic Description of Cohesion in Solids

of these elastic potentials, like for the problems described above, is the relative energies of a number of different conﬁgurations. Our reason for calling attention to these models at this point is to drive home the signiﬁcance of the total energy, whether that energy is being considered in the context of elasticity, mass transport or fracture. The aim of the present chapter is to give examples of the broad classes of microscopic energy functionals that are available to make such calculations. 4.2 Conceptual Backdrop for Characterizing the Total Energy 4.2.1 Atomistic and Continuum Descriptions Contrasted One of the key questions posed in this chapter is how best to reconcile microscopic descriptions, which are presumed to represent the true mechanistic underpinnings of a given process, and phenomenological descriptions, whose aim is to capture the essential physics of a particular process, and to use this reduced description as a predictive tool. The philosophies of these two types of calculations are strikingly different. The microscopic viewpoint champions a complete description of the ‘relevant’ degrees of freedom, with an explicit reckoning of the interactions and evolution of all of them. The total energy may then be written in the form E tot ({Ri , rn }) which highlights the dependence of the total energy on each and every microscopic degree of freedom. Note that here we have explicitly acknowledged the presence not only of the nuclei {Ri }, but also the electrons which are characterized in a classical description by coordinates {rn }. We note that in some instances, such as in density functional theory, the dependence on the electronic degrees of freedom is effected via a dependence of the total energy on the electron density, ρ(r ), which may be written as E tot [ρ(r); {Ri }]. Continuum descriptions are built around energy functionals which depend upon kinematic measures such as displacement ﬁelds as opposed to atomic coordinates, and the neglected atomic-level degrees of freedom make their appearance only implicitly through the presence of material parameters such as the elastic moduli. Whether the description of the total energy is based upon microscopic or continuum notions, ultimately, all such energy functionals represent a reduction in complexity relative to the full microscopic Hamiltonian. The type of degree of freedom reduction we have in mind can be illustrated on the basis of an analogy borrowed from statistical mechanics. If we begin with a system of spins on a lattice which interact according to a near-neighbor Ising model, the total energy may be written E tot ({σi }) = i J σi σi+1 . If we now use the dodge of constructing block spins by adding up the spins in small groups, the total energy may be rewritten in terms of the new block spin variables mediated by some new effective coupling constant Jeff . That is, the reduced description of the total block . In this case, the missing degrees of energy is E tot ({σiblock }) = i Jeff σiblock σi+1

4.2 Conceptual Backdrop for Characterizing the Total Energy

153

freedom only make their presence known through the effective coupling constant Jeff . The simplest example of this type of degree of freedom as pertains to the energy of solids emerges through consideration of the meaning of the elastic moduli. From the continuum perspective, the elastic moduli are material parameters whose values cannot be determined by the continuum theory itself. Within such a framework, the moduli represent the energy cost associated with special afﬁne deformations of the solid. For example, a pure breathing mode has an energy that scales with the bulk modulus B. Thus, we write the energy change upon altering the volume by an amount V as 1 (V )2 . (4.1) E = B 2 V One then makes a bolder assertion. It is hypothesized that even in the presence of some inhomogeneous deformation, the total energy may be obtained as an integral over the strain energy density which is itself obtained by appealing only to the local state of deformation. This leads to the form described in chap. 2: 1 E tot = Ci jkl i j (x)kl (x)dx. (4.2) 2 On the other hand, the microscopic view of such elastic distortions reﬂects the modiﬁcation of a multitude of atomic bonds. The energy cost associated with a given deformation is nothing more than the outcome of evaluating the energies of the distinct atomic constituents. Remarkably, these two perspectives merge in the form of the elastic moduli. That is, the energetics of the complex arrangements of atomic bonds that result from some complicated inhomogeneous deformation can in the end be represented (at least in the case of small deformations) via the relevant elastic moduli. In subsequent chapters, we will reﬁne this description by demonstrating the nature of the coupling between microscopic and continuum descriptions of elasticity by explicitly computing a microscopic expression for the moduli using a simple model potential. However, bonding in solids is an inherently quantum mechanical process and thereby, at least in principle, requires a consideration of the electronic degrees of freedom. In the remainder of this chapter we will investigate the ways in which the total energy can be evaluated from the microscopic perspective. First, we will examine those methods in which the electronic degrees of freedom are subsumed in some effective description. The result of adopting this strategy is that the total energies we will write can only be considered as approximations. We begin by considering pair potential models of bonding in solids. Such models provide a transparent scheme for evaluating the total energy, though they are often of limited quantitative value. In this case, the idea is that the pair potential is an effective

154

4 Energetic Description of Cohesion in Solids

representation of the underlying electronic degrees of freedom which enter only through a parametric dependence of the potentials on the electron density. A more thorough analysis of the electronic degrees of freedom suggests a class of total energy functionals known as effective medium and angular force schemes in which additional features of the physics of bonding are incorporated. These methods are evaluated in turn, with a summarizing commentary on the limitations inherent in all of these methods. Subsequently, we will highlight the key ideas involved in extending the microscopic analysis to permit incorporation of the electronic degrees of freedom. The crowning achievement here is the Hohenberg–Kohn theorem which shows how the total energy may be evaluated as a functional of the electronic density. Further, this scheme allows for a variational treatment of the total energy which amazingly leads to a set of effective single particle equations that are an exact description of the complex many-body system encountered when thinking about electrons in solids. 4.2.2 The Many-Particle Hamiltonian and Degree of Freedom Reduction From a quantum mechanical perspective, the starting point for any analysis of the total energy is the relevant Hamiltonian for the system of interest. In the present setting, it is cohesion in solids that is our concern and hence it is the Hamiltonian characterizing the motions and interactions of all of the nuclei and electrons in the system that must be considered. On qualitative grounds, our intuition coaches us to expect not only the kinetic energy terms for both the electrons and nuclei, but also their mutual interactions via the Coulomb potential. In particular, the Hamiltonian may be written as p2j Z e2 Z 2 e2 P2 e2 1 i + + − + . 2M 2m 2 i j |ri − r j | |ri − R j | |Ri − R j | i j ij ij

(4.3)

The terms in this Hamiltonian are successively, the kinetic energy associated with the nuclei, the kinetic energy associated with the electrons, the Coulomb interaction between the electrons, the electron–nucleus Coulomb interaction and ﬁnally, the nuclear–nuclear Coulomb interaction. Note that since we have assumed only a single mass M, our attention is momentarily restricted to the case of a one-component system. As an antidote to the nearly hopeless complexity presented by the problem of the coupling of degrees of freedom revealed in eqn (4.3), a number of different strategies have been constructed. Such strategies can be divided along two main lines, although this division is in the end an oversimpliﬁcation. One set of ideas surrounds the attempt to remove the electronic degrees of freedom altogether,

4.2 Conceptual Backdrop for Characterizing the Total Energy

155

electing to bury them in effective interactions between the ions. Note that in these approaches, the exact energy is replaced by an approximate surrogate via E exact ({Ri , rn }) → E approx ({Ri }).

(4.4)

As will be shown in coming sections, wide classes of total energy descriptions fall under this general heading including traditional pair potential descriptions, pair functionals, angular force schemes and cluster functionals. The second general class of schemes, which almost always imply a higher level of faithfulness to the full Hamiltonian, are those in which reference to the electrons is maintained explicitly. In this case, the mapping between the exact and approximate descriptions is of the form, E exact ({Ri , rn }) → E approx ({Ri , rn }),

(4.5)

E exact ({Ri , rn }) → E approx [ρ(r), {Ri }],

(4.6)

or as was said already

where the second expression highlights the use of a function ρ(r) to characterize the disposition of the electronic degrees of freedom. Later in the present chapter, we will discuss both tight-binding models (section 4.5) and the use of density functional theory (section 4.6) as ways to effect this type of approximate mapping between the full Hamiltonian and more tractable approximations. The ideas embodied in eqns (4.5), (4.6) and (4.7) constitute profound exercises in effective theory construction. Though considerable hype surrounds the use of the term ‘multiscale modeling’, efforts to confront the difﬁculties inherent in the many-body problem that is cohesion in solids provide a perfect example of the philosophy behind systematic degree of freedom elimination which is itself at the heart of multiscale modeling. The ﬁrst step taken in the attempt to pare down the problem is to exploit the so-called Born–Oppenheimer approximation. Though this approximation will not enter into our calculations in any material way, it is crucial to our enterprise from a philosophic perspective since it illustrates the way in which degrees of freedom can be unlinked, and thereby, problems can be rendered more tractable. The central physical idea is to separate the nuclear and electronic motions on the basis of the smallness of the ratio m/M, where m is the electron mass and M is that of the relevant nuclei. Indeed, from a multiscale perspective, the Born–Oppenheimer approximation represents the simplest of cases in which there is a natural separation of scales, upon which may be founded the scale-bridging ansatz. The physical argument that is made is that the electronic motions are so fast relative to the nuclear motions that we may imagine the electrons to respond to an essentially static set of nuclear positions. The outcome of adopting this view is

156

4 Energetic Description of Cohesion in Solids

that the ionic coordinates only appear parametrically in the Schr¨odinger equation for the electrons. The key observations may be summarized as follows. The Schr¨odinger equation we are faced with solving in the context of the Hamiltonian of eqn (4.3) is of the form H ψ({Ri , rn }) = Eψ({Ri , rn }),

(4.7)

where our notation highlights the dependence of the wave function on all of the nuclear and electronic coordinates. The strategy at this point is to attempt a solution of the form ψ({Ri , rn }) = ψe ({rn }; {Ri })ψn ({Ri }),

(4.8)

where ψe and ψn refer to the solutions to the electron and nuclear problems, respectively. To be more precise, ψe ({rn }; {Ri }) is a solution to the problem (Te + Vee + Ven )ψe ({rn }; {Ri }) = E e ψe ({rn }; {Ri }),

(4.9)

where we have introduced the notation Te to describe the electron kinetic energy, Vee is the electron–electron interaction and Ven is the interaction between the electrons and the nuclei. In addition, this problem is solved with respect to ﬁxed nuclear coordinates {Ri } on the grounds that the nuclei are effectively frozen on the time scale of electronic motions. The ﬁnal step in the approximation is to solve the Schr¨odinger equation for the nuclei of the form (Tn + Vnn + E e )ψn ({Ri }) = E n ψn ({Ri }),

(4.10)

where it is to be noted that the energy eigenvalue from the electron problem ends up as part of the effective potential for the nuclear problem.

4.3 Pair Potentials 4.3.1 Generic Pair Potentials As said earlier, almost the entire business of the present chapter will be to examine the various ways in which the overwhelming complexity presented by the full Hamiltonian of eqn (4.3) has been tamed. Perhaps the simplest example of simplifying the total energy is via an approximation of the form 1 E exact ({Ri , rn }) → E approx ({Ri }) = V (Ri j ), (4.11) 2 ij where V (Ri j ) is the pair potential, and Ri j is the distance between the i th and j th particles. Examples of the pairwise decomposition of the total energy are as old as Newtonian physics itself. Both the gravitational and Coulomb problems exhibit

4.3 Pair Potentials

157

Fig. 4.3. Lennard–Jones pair potential plotted in dimensionless units.

such additivity. Indeed, the ability to write the gravitational potential of a given mass distribution with density ρ(r) as ρ(r )d 3 r (4.12) φ(r) = G |r − r | may be traced directly to such pairwise additivity. To understand the origins of pair potentials, we begin by reﬂecting on their nature in a generic sense, and then turn to an explicit evaluation of quantum mechanically based pair potentials from the standpoint of perturbation theory. As noted above, the total energy within a pair potential setting may be written as E tot = (1/2) i j Veff (Ri j ), where Ri j is the distance between the i th and j th atoms. The logic in this case is that the total energy may be decomposed into a number of distinct contributions, one from each of the bonds that make up the system. Perhaps the most familiar example of such potentials is that of the Lennard–Jones potentials which are intended to reﬂect the polarization interactions that occur in closed-shell systems in which the charge distribution on a given atom may be rearranged as a result of the presence of the neighboring atoms. Within the context of the Lennard–Jones potentials, the energy of interaction between atoms at sites separated by a distance r is 12 6

σ σ , (4.13) − V (r ) = V0 r r where V0 is a parameter determining the depth of the potential well and σ is a length scale that determines the position of the minimum. An example of a Lennard–Jones potential, plotted in dimensionless units, is shown in ﬁg. 4.3.

158

4 Energetic Description of Cohesion in Solids

Once the pair potential has been speciﬁed, it is a straightforward exercise given the atomic positions to compute the total energy. For simplicity, consider a pair potential Veff (r ) whose form is left unspeciﬁed. Further, consider the simplifying assumption that this potential reﬂects a coupling only between ‘nearest neighbors’. To compute the total energy of a given conﬁguration, all that is required is that we sum up the independent contributions of all distinct bonds. For example, if we consider an fcc crystal with lattice parameter a0 , the total energy within the context of a generic potential in which only near-neighbor atoms are presumed to interact is given by a0 N E tot = (4.14) Veff (rnn ) = 6N Veff √ . 2 neighbors 2 In the previous expression we have exploited the fact that in the fcc crystal, each atom is surrounded by an identical √ environment that is composed of twelve near neighbors at a distance of a0 / 2. Because of the high symmetry of the perfect fcc geometry, it was possible to carry out the total energy computation analytically. The basic idea associated with a pair potential calculation of the total energy is to sum over the entirety of bonds between each atom and its ‘neighbors’. When confronted with a more complex geometry, it is likely that we will be reduced to numerical computation, but the concept remains unchanged.

4.3.2 Free Electron Pair Potentials Though simple analytic expressions such as the Lennard–Jones form adopted above (at least the attractive part) may be constructed on the basis of a sound quantum mechanical plausibility argument, the derivation of pair potentials for free electron systems is even more enlightening and strikes to the heart of bonding in metallic systems. An even more important reason for the current discussion is the explicit way in which the effective description of the total energy referred to in eqn (4.4) is effected. As will be shown below, the electronic degrees of freedom are literally integrated out with the result that 1 ¯ = V (Ri j ; ρ). ¯ (4.15) E exact ({Ri , rn }) → E approx ({Ri }; ρ) 2 ij Note, however, that there is a remnant of the electronic degrees of freedom in the form of a dependence of the potentials on the mean electron density. The starting point for our free electron analysis is the assertion that to a ﬁrst approximation, simple metallic systems may be thought of as consisting of a uniform electron gas with a density determined by how many electrons each atom has donated to the ‘electron sea’. The underlying conceptual model is that

4.3 Pair Potentials

159

described in chap. 3 for electrons in a three-dimensional box. That model is now supplemented by imagining the box to contain not only the free electrons, but also the ions that have donated them. Our task is to compute the total energy of such a system. The presence of the ion cores which have donated the free electrons to the electron gas is then imagined to impose a weak periodic perturbation on the quiescent electron gas. For the present purposes, the key result is that within the conﬁnes of perturbation theory, if the effect of these ion cores is carried to second order in the weak perturbing potential, the total energy of the system may be written in real space in exactly the form of a pair potential. We have now advanced the view that the effect of the ionic cores may be treated as a weak perturbating potential Vp (r) on the free electron states discussed earlier. The presence of the perturbing potentials will have the effect of altering the free electron E k = h¯ 2 k 2 /2m, √ energies, (0) and the free electron wave functions, ψk (r ) = (1/ )eik·r . We begin by recalling that within quantum mechanical perturbation theory, the ﬁrst- and second-order corrections to the energy of the n th eigenstate, E n(1) and E n(2) , may be written as (1) E n = ψn(0)∗ (r)Vp (r)ψn(0) (r)d 3 r (4.16) and E n(2)

=

| ψ (0)∗ (r)Vp (r)ψ (0) (r)d 3 r|2 n k E n(0) − E k(0)

k=n

,

(4.17)

where Vp (r) is the perturbing potential derived from the ionic potentials, ψn(0) (r) is the n th wave function of the unperturbed system and E n(0) is the n th energy eigenvalue in the absence of the perturbation. The results written above should be thought of in the following context. Our preliminary investigation of the electrons in a metal was restricted to the assumption that the presence of the ionic cores is completely irrelevant. We solved this problem in the introductory sections on quantum mechanics in the last chapter. We have now introduced a periodic array of ionic potentials and have included their contribution to the total energy perturbatively. The picture at this point is that the total potential experienced by an electron in the box as a result of the presence of the ionic cores may be written as Vps (|r − Rn |). (4.18) V (r) = n

We have introduced the notation Vps to denote the atomic pseudopotentials. These pseudopotentials are meant to characterize the interaction of the valence (i.e. outer) electrons with the nucleus and its associated tightly bound core electrons. Our aim now is to assess the corrections to the total energy of the electron gas as a result of

160

4 Energetic Description of Cohesion in Solids

the perturbation due to the ionic cores. To begin with, we consider the alteration of the energy in ﬁrst-order perturbation theory. The change in energy of a plane wave state with √ wavevector k is obtained using eqn (4.16) with wave functions ψk(0) (r) = (1/ )eik·r and is given by 1 e−ik·r V (r)eik·r d 3 r. (4.19) E k(1) = We see immediately that this results in an energy shift E = (1/ ) V (r)d 3 r that is independent of the wavevector. As a result, the conclusion is that to ﬁrst order, the presence of the ionic cores does nothing more than impose a uniform shift on the energies of all of the free electron states. It is thus uninteresting as concerns different structural arrangements but contributes to the overall cohesive energy. We now look to second-order pertubation theory for a determination of a nontrivial change in the energy. Our strategy will be to ﬁrst compute the energy change associated with a state of a particular wavevector and, subsequently, to sum the change over all occupied states. The net result is the second-order energy change for the electron gas in the presence of a particular ionic conﬁguration. The second-order shift to a state with wavevector k is obtained using eqn (4.17), again √ (0) ik·r with wave functions ψk (r) = (1/ )e and energies E k(0) = h¯ 2 k 2 /2m and is given by 2 1 −ik·r i(k+q)·r 3 e V (r)e d r . (4.20) E k(2) = h¯ 2 2 q=0 2 (k − |k + q| ) 2m We now use eqn (4.18) to obtain 2 2 1 iq·Rn 1 iq·r 3 e Vps (r)e d r a N n . E k(2) = h¯ 2 2 q=0 2 (k − |k + q| ) 2m

(4.21)

We have used a simple relation between the total volume and the atomic volume a , namely, = N a . Note that the factors in the numerator are both of particularly simple forms, with the term involving Vps clearly revealed as the Fourier transform of the atomic pseudopotential. It is convenient to invoke the notational convention 1 iq·Rn S(q) = e , (4.22) N n

4.3 Pair Potentials

161

which is the structure factor and is only dependent upon the geometry of the ionic positions. If we replace the sum overq with the corresponding integral, using the well-worn identity q → (V /2π )3 d 3 q, our expression for the energy change to second order for the state with wavevector k is |S(q)|2 |Vps (q)|2 V (2) 3 . (4.23) d q Ek = (2π )3 h¯ 2 2 2 (k − |k + q| ) 2m Our claim is that this expression may now be manipulated in such a way that when it is time to sum the energy change over all of the occupied states, the total energy change will be seen as a sum over effective pair potentials. With the Fourier transform of the atomic pseudopotential in hand, it is possible to evaluate the energy change explicitly. However, rather than concerning ourselves with the particulars associated with the speciﬁc choice of pseudopotential, we will work in the abstract, holding a course that will reveal the emergence of the pair potential as an effective theory for the electronic degrees of freedom as quickly as possible. To demonstrate that the energy shift described above may be written as a sum over pair terms, we proceed as follows. Note that what we have done above is to identify the energy change to second order for the free electron state of wavevector k. In order to assess the total energy change of the free electron gas in the presence of the potentials due to the ionic cores, we must now sum over all of the occupied free electron states. This results in a second-order change in the band structure part of the total energy per atom of |S(q)|2 |Vps (q)|2 2 V band 3 d . (4.24) q E tot = N |k|≤k F (2π )3 h¯ 2 2 2 (k − |k + q| ) 2m Note that everything except for S(q) is structure-independent. By expanding the structure factor explicitly in terms of its deﬁnition given in eqn (4.22), it is evident that the energy has decomposed into a series of pair terms as 1 band E tot = φeff (Rm − Rn ), (4.25) 2N m,n with the effective pair interaction given by

iq·(Rm −Rn ) 4V |Vps (q)|2 3 e d q . (4.26) φeff (Rm − Rn ) = (2π )3 |k|≤k F h¯ 2 2 2 (k − |k + q| ) 2m We now note that in addition to the electronic contribution to the structural part of the energy, the term computed above must be supplemented by the repulsion between the ions. We should also note that if our emphasis had been on computing

162

4 Energetic Description of Cohesion in Solids

Fig. 4.4. Pair potentials for Al as computed using perturbation analysis (adapted from Hafner (1987)). The four separate potentials shown here reﬂect different treatments of the electron–electron interaction, where RPA, IU, LDA and VS refer to the names of different approximations used in the construction of potentials.

the potential itself, rather than on demonstrating the way in which the electronic degrees of freedom are subsumed in an effective potential, we could have worked out expressions in which the Fourier transform of the pseudopotential is used explicitly and in which the sums over k and q are performed explicitly leaving in the end a single one-dimensional integral. As a ﬁnal word of caution, it should be noted that we have been lax in our treatment of screening effects which would modify the quantitative details of what we have said, though not the overall argument concerning the integrating out of the electronic degrees of freedom. For further details, the reader is encouraged to consult Harrison (1980) or Hafner (1987). The outcome of a calculation such as that given above is not entirely unambiguous. In particular, the choice of atomic pseudopotential and the treatment of screening effects can lead to potentials with different qualitative features. For the sake of discussion, in ﬁg. 4.4 we show a series of pair potentials for Al developed using different schemes for handling these effects. For our purposes, the key insight to emerge from this analysis is that we have seen how, on the basis of a free electron picture of metals, one may systematically construct effective pair potentials. Though our primary emphasis will center on the calculation of energies, it is also worth remembering that the total energy serves as the basis for the determination of forces as well. In many instances (i.e. static relaxation or molecular dynamics), the

4.3 Pair Potentials

163

calculation of forces is a prerequisite to the performance of structural relaxation. If we are to consider a generic pair potential of the form 1 φ(Rmn ), (4.27) E tot = 2 mn then the force in the α th Cartesian direction on particle i is given by f iα = −

∂ E tot , ∂ Riα

(4.28)

where we have introduced the notation Riα to characterize the α th component of the position vector Ri . Explicit evaluation of the derivative we are instructed to perform results in the force (Riα − Rmα ) φ(Rim ) . (4.29) f iα = − Rim m Despite the virtues inherent in using pair potentials, they also exhibit certain physical features that are troubling. Once the total energy has been written in the pair potential form, we note that the bond strength is explicitly independent of the environment. What this means is that no matter how many neighbors atom i may have, its bond with atom j has energy φeff (Ri j ). In the next section, we will see that ab initio calculations suggest that the environmental independence presumed in pair potential models is a faulty assumption. In addition to this fundamental qualitative shortcoming, there are other quantitative problems as well. When we undertake an analysis of elastic properties in ensuing chapters, the conceptual foundations for the microscopic evaluation of the moduli will be laid in terms of pair potentials. This development will be made not so much out of necessity, but rather because the pair potential description lays bare the central idea behind the evaluation of the moduli. One of the outcomes of such an analysis will be the realization of just how restrictive is a pair potential description of the total energy (especially in those cases in which volume-dependent terms are neglected). We will show, for example, that for cubic crystals, the elastic moduli C12 and C44 are equal, in contradiction with observation. Though there are ways to soften this blow, fundamentally, the pair description is left wanting. A second difﬁculty with the pair potential description is manifest when we attempt to consider defect formation energies. Speciﬁcally, we will also show that the pair potential description implies a formation energy for vacancies that is a vast overestimate relative to the numbers found in experiment. As is true for the elastic moduli, there are modiﬁcations that can be considered, but not without a sense that the crucial physics is being ignored. In response to these difﬁculties, and others, concerted efforts have been made to extend our description of the energetics of

164

4 Energetic Description of Cohesion in Solids

solids without paying the full price of ab initio calculation. We undertake such analyses now.

4.4 Potentials with Environmental and Angular Dependence As we have noted above and will see in more detail later, the pair potential description is littered with difﬁculties. There are a few directions which can be taken that will be seen to cure some of them. We begin with a qualitative discussion of these issues, and turn in what follows to the development of both angular force schemes and effective medium theories that patch some of these troubles, primarily through the device of incorporating more of what we know about the nature of bonding in solids.

4.4.1 Diagnostics for Evaluating Potentials We begin with a few qualitative insights into where the pair potential description might be lacking. One question we might pose that could expose a particularly problematic assumption of a pair potential description would be: how does the strength of a given bond depend upon whether or not the atom is participating in other bonds? Using ﬁrst-principles calculations one can address this question systematically by repeatedly evaluating the strength of bonds for a range of different geometries. By ﬁrst-principles calculations, we mean fully quantum mechanical calculations that are, at least in principle, parameter-free. An example of this strategy is revealed in ﬁg. 4.5 where it is seen that the strength of the bond goes roughly inversely as the square root of the coordination number. That is, as the number of neighbors to a given atom increases, the energy associated with each bond goes down. The ﬁrst-principles calculations were performed by considering a number of different structures, some observed, others hypothetical, which have near-neighbor environments that differ considerably in terms of coordination number. For example, the diamond cubic structure features only four near-neighbor bonds while the fcc structure is characterized by twelve. The energies of each of these structures were computed using the type of ﬁrst-principles techniques to be described later in the chapter, and then the resulting energies were plotted in a normalized form that revealed the energy per bond. In the context of pair potentials, what do these results teach us? Stated simply, the conclusion is that the bond strength has a certain environmental dependence. As will become evident in what follows, this environmental dependence can be mimicked by a class of energy functionals that are known variously as effective medium theories, Finnis–Sinclair potentials, glue models, the embedded atom method and pair functionals.

4.4 Potentials with Environmental and Angular Dependence

165

Fig. 4.5. Energy per atom for a variety of different structures in Al having different coordination 1

numbers (after Payne et al. (1996)). The curve is a ﬁt to the functional form E = E 0 + α Z 2 + β Z , where Z refers to the coordination number of a given atom.

A second perspective on the weakness of pair potentials comes from a consideration of bond angles. For example, if we are to consider a simple pair potential of the Morse or Lennard–Jones form in which there is a minimum associated with the near-neighbor separation, it is difﬁcult to imagine how open structures such as those found in the covalent semiconductors could be stabilized. The argument in this case might go as follows: twelve bonds taking advantage of the near-neighbor separation is better than only four. As a result, we are inclined to the view that there must be something particularly energetically important about the existence of certain bond angles.

4.4.2 Pair Functionals At the next level of sophistication beyond pair potentials, a variety of methods which can broadly be classiﬁed as pair functionals have been developed. In keeping with the various surrogates for the full Hamiltonian introduced in eqns (4.4), (4.5) and (4.30), the total energy in the pair functional setting is given by 1 φ(Ri j ) + F(ρi ), (4.30) E exact ({Ri , rn }) → E approx [ρ(r), {Ri }] = 2 ij i as will be seen below. Pair functionals can be motivated in a number of different ways, a few of which will be taken up here. One route to pair functionals is to

166

4 Energetic Description of Cohesion in Solids

Fig. 4.6. Energy cost to embed ion in electron gas of particular density ( from Jacobsen et al. (1987)).

revisit the electron gas, seen in a different light from that discussed in the context of free electron pair potentials. The physical picture that we will adopt here may be summarized as follows. The question that is posed is what is the energy cost to deposit an ion into a homogeneous electron gas of density ρ? What is found and will be discussed at some level of detail below is that there is an optimum electronic density (i.e. an energy minimizing density), and that optimal density depends upon the identity of the ion being placed in the electron gas. Consideration of ﬁg. 4.6 reveals the outcome of a series of numerical calculations made using density functional theory for a host of elements. What is learned from these calculations is that an ion of a particular type has a taste as to what the optimal local electron density should be. This insight provides the opportunity to construct a new class of energy functional which overcomes some of the limitations of the pair potential description. The philosophy of the pair functional approach is perhaps best illustrated via a concrete example. Consider fcc Ni. In this case, we know on the basis of the results shown above, that the Ni atom prefers to live in a certain equilibrium electron density. As yet, we have not seen how to exploit this insight in the context of particular geometric arrangements of a series of Ni atoms. We may see our way through this difﬁculty as follows. If we center our attention on a particular Ni atom, we may think of it as being deposited in an electron gas, the density of which is dictated by the number and proximity of its neighbors. The hypothesized energy

4.4 Potentials with Environmental and Angular Dependence

167

functional that captures that dependence may be written as E embedding = F(ρ),

(4.31)

where we further suppose that the electron density of the electron gas that the Ni atom ﬁnds itself in is given by f (Ri j ). (4.32) ρi = j=i

This equation tells us how to determine the ‘density’ of the electron gas at the site of interest which we denote ρi in terms of the geometric disposition of the neighboring atoms. In particular, f (R) is a pairwise function that characterizes the decay of electronic density from a given site. Hence, if we wish to ﬁnd the contribution of atom j to the density at site i, the function f (R) evaluated at the distance R = |Ri − R j | tells us exactly how much electronic density bleeds off from site j onto its neighbors. To bring the development of the pair functional approach to its completion, we assume that the total energy may be divided into two parts; one part whose aim is to mimic the type of electron gas embedding terms envisaged above and another whose intent is to reﬂect the Coulombic (possibly screened) interactions between the various nuclei. As yet, we have examined the embedding energy on the basis of the quantum mechanics of the electron gas. We have argued that on the basis of legitimate numerical evidence from quantum calculations one can construct the functional F(ρ). On the other hand, a large body of work has been built around the idea of taking one’s cue from the quantum mechanical foundations laid above, but instead to assume a pragmatist’s position and to ﬁt the various functional forms on the basis of known data. The embedded atom method is predicated on the latter alternative, and posits a total energy of the form, 1 φ(Ri j ) + F(ρi ), (4.33) E tot = 2 ij i where the density on site i is given in turn by an equation of the form of eqn (4.32) above. Our appeal that pair potentials were inadequate for capturing many of the energetic features of real materials was founded in part upon the environmental dependence of the bond strengths, captured in ﬁg. 4.5. It is of interest to revisit this question in light of the simple embedding form adopted above. As with our discussion of the free electron pair potentials, our aim at the moment is not to discuss the optimal choice of embedding functions but rather to identify the extra physics that makes such energy functionals an improvement over pair potentials. For the sake of argument, consider the same near-neighbor model discussed earlier

168

4 Energetic Description of Cohesion in Solids

Fig. 4.7. Model geometries used to illustrate computation of total energy within pair functional formalism: (a) linear chain, (b) square lattice.

in which the density due to a single neighbor at the equilibrium distance Rnn is given by f 0 . Our aim now is to consider the energy/atom for a few distinct structures in order to explicitly exhibit the environmental dependence that was claimed to be of interest above, and to build facility in using this functional form. For the linear chain of atoms (see ﬁg. 4.7), the total energy per atom within the embedded atom context is given by E chain = φ(Rnn ) + F(2 f 0 ).

(4.34)

This result reﬂects the fact that every atom on the chain has an identical environment with two near neighbors at the equilibrium distance. If we continue along the lines set above and consider the total energy of the square lattice depicted in ﬁg. 4.7, it is seen to have a total energy of E square = 2φ(Rnn ) + F(4 f 0 ).

(4.35)

The analysis precedes similarly for other cases of interest, such as, for example, the fcc structure, which has a total energy of E f cc = 6φ(Rnn ) + F(12 f 0 ).

(4.36)

Note that in the absence of the embedding term the total energy per bond is constant √ as expected. However, if we adopt the form F(ρ) = ρ which will be motivated

4.4 Potentials with Environmental and Angular Dependence

169

Fig. 4.8. Universal binding energy relation (adapted from Rose et al. (1984)).

after we have introduced the tight-binding method, the energy per bond is clearly not constant. One of the cleanest routes to determining embedding functions is by invoking the universal binding energy relation (UBER) (Rose et al. 1984). On the basis of a vast collection of experience with ﬁrst-principles calculations of a range of materials, it was found that the total energy as a function of lattice parameter may be ﬁtted to

r −α( r −1) E tot (r ) = −E c 1 + α − 1 e r0 , (4.37) r0 where r is a measure of the interatomic separation and α and r0 are scaling parameters which collapse the speciﬁc material data onto the universal curve. An example of this scaling behavior as a function of the lattice parameter for a range of materials is shown in ﬁg. 4.8. This form for the total energy suggests a strategy for constructing embedding functions via the following argument. We assume the pair potential is of some speciﬁed form. Once this form is adopted, the embedding function may be deduced as the difference between the total energy as given by the universal binding energy relation and the total contribution to the pair potential. To illustrate this procedure, we follow Johnson (1988) by assuming a nearneighbor only interaction. Hence, as was shown in eqn (4.36), the energy of a given atom is E i = F(ρi ) + 6φ(Rnn ). If we now assert that the left hand side

170

4 Energetic Description of Cohesion in Solids

of this equation is determined by the universal binding energy relation, then the embedding function is F[ρ(R)] = E UBER (R) − 6φ(R).

(4.38)

Johnson makes the explicit choice of density function ρ(r ) = f e

−β( rr −1) 0

,

(4.39)

and deﬁnes the pair potential as φ(r ) = φ0 e

−γ ( rr −1) 0

.

(4.40)

Note that we have imitated Johnson’s notation in which the quantity f is a constant factor that appears in the determination of the density ρ, and the parameters r0 , β, γ and φ0 are other parameters that are determined through the ﬁtting procedure. Once the density function and the pair potential have been speciﬁed, the determination of the embedding function is complete in principle. In this case, because of the choice of functions, the relevant equations can be solved analytically with the result that the embedding energy is given by βα γβ α ρ ρ ρ F(ρ) = −E c 1 − ln − 6φ0 . (4.41) β ρ0 ρ0 ρ0 The basic strategy used in deriving this form for the embedding function is the recognition that the density function ρ(r ) may be inverted to yield 1 ρ(r ) r − 1 = − ln , r0 β ρ0

(4.42)

where ρ0 is the density when the interatomic separation is r0 . This form for the embedding energy is contrasted with others in ﬁg. 4.9. The central importance of this particular embedding strategy is that now that the analytic form is in hand, it is possible to examine a range of secondary quantities such as the elastic moduli, surface energies and point defect formation energies analytically. Of course, there exist signiﬁcantly more sophisticated (and accurate) schemes for carrying out pair functional calculations. While such functions may be preferable in the attempt to calculate real material properties, the Johnson potential serves as an ideal pedagogic vehicle for discussing embedding energies. From the standpoint of ‘back of the envelope’ exercises, one may use analytic near-neighbor models such as that proposed by Johnson to estimate quantities ranging from the (111) surface energy to the vacancy formation energy. In addition to the importance of energies, a number of situations demand a knowledge of the forces between atoms. We have already seen in eqn (4.29) how forces are computed within the pair potential setting. The presence of the

4.4 Potentials with Environmental and Angular Dependence

171

Fig. 4.9. Various representations of the embedding energy for Cu (adapted from Johnson (1988)). The solid curve is the embedding function for Cu derived from UBER as described in text, the dashed curve is a ﬁt for the embedding function and the dotted curve corresponds to an embedding function √ of the Finnis–Sinclair form in which F(ρ) ∝ ρ.

embedding term in the pair functional setting leads to additional subtlety in the computation of forces. In particular, the expression for the force on the i th atom due to the embedding term is given by ˆ ji , fi = − (F (ρ j )ρi + F (ρi )ρ j )R (4.43) j=i

ˆ ji is the unit vector pointing from the j th to the i th atom. It is left to the where R reader to derive this result explicitly in the problems at the end of the chapter. A ﬁnal intriguing point about energy functionals like those described in this section is that they may be transformed into an effective pair potential description of the total energy. This claim is an interesting example of the various layers in effective theory construction and reﬂects a transformation of the form 1 E approx [ρ(r), {Ri }] → E approx ({Ri }; ρref ) = Veff (Ri j ; ρref ), (4.44) 2 ij where ρref denotes the dependence of the resulting pair potential on a reference density. Thus, the effective pair potential developed to describe bulk environments will differ considerably from that derived to account for free surfaces. Indeed, these potentials will reﬂect exactly the environment-dependent bond strengthening that is the hallmark of the pair functional approach. The reader is asked to ﬁll in the details of this development in the problem section at the end of the chapter.

172

4 Energetic Description of Cohesion in Solids

4.4.3 Angular Forces: A First Look There are some circumstances in which the inclusion of the ‘many-body’ terms present in pair functionals is insufﬁcient and recourse must be made to angular terms. As yet, our discussion has been dominated by metals. On the other hand, more than ﬁfty different potentials have grown up around the question of how best to model covalent materials, with Si as the dominant example. One of the remarkable features of Si in the solid state is its open structure, characterized by only four neighboring atoms in the ﬁrst neighbor shell in contrast with the twelve neighbors found in close-packed structures. As a result of this structural clue, it seems that the insistence on the coupling between bond lengths and energy must be supplemented by consideration of the energetics of bond angles. As will be seen below, both angular potentials and cluster functionals have been developed to characterize materials such as Si. Our aim here is to give a ﬂavor of these developments by recourse to two of the most celebrated total energy schemes used in semiconductors: the Stillinger–Weber angular potentials and the Tersoff cluster functional. The Stillinger–Weber potentials were developed with the mind of explaining the condensed phases of Si, including the fact that in the liquid state, the coordination number of Si atoms increases. The basic structure of the Stillinger–Weber potential is revealed in the expression for the total energy which is 1 1 V2 (Ri j ) + V3 (Ri , R j , Rk ), (4.45) E tot ({Ri }) = 2 i, j 3! i, j,k with the ﬁrst term corresponding to a pair potential of the type with which we are already familiar, and the second term is an angular term which imposes penalties when the angles in three-atom triangles deviate from particularly stable values. The potentials themselves are represented as Ri j , (4.46) V2 (Ri j ) = f 2 σ and

V3 (Ri , R j , Rk ) = f 3

Ri R j Rk , , . σ σ σ

The functions f 2 (Ri j ) and f 3 (Ri , R j , Rk ) are deﬁned by −1 A(B R − p − R −q )e[(r −a) ] if r < a f 2 (R) = 0 otherwise

(4.47)

(4.48)

and f 3 (Ri , R j , Rk ) = h(Ri j , Rik , θ jik ) + h(R ji , R jk , θi jk ) + h(Rki , Rk j , θik j ). (4.49)

4.4 Potentials with Environmental and Angular Dependence

173

Fig. 4.10. Stillinger–Weber angular term.

The novel feature associated with the Stillinger–Weber potentials is this angular term. To be more speciﬁc, the three-body terms have an angular dependence of the form 1 2 −1 −1 , (4.50) h(Ri j , Rik , θ jik ) = λe[γ (Ri j −a) +γ (Rik −a) ] cos θ jik + 3 where only the angle-dependent part of this function is shown in ﬁg. 4.10. Recall that in our discussion of pair potentials, structural stability was attributed to the fact that particular structures have bond lengths that take advantage of minima in the pair potential. On the other hand, the existence of angular potentials paves the way for a second form of correspondence between structure and energetics. In particular, now not only must bond length constraints be satisﬁed, but bond angle constraints as well. In this case, we see that the angular term is minimized in the case that θ ≈ 109.47◦ , corresponding to the favorability of the tetrahedral angles that characterize the sp3 bonding in many covalent materials. The computation of the total energy in the context of a total energy scheme involving angular forces is quite analogous to that considered in the pair potential setting. Indeed, that part of the energy due to the pair potential terms is identical to those considered earlier. However, the angular terms involve a more careful analysis of the neighbor environment for a given atom. In particular, these terms require that a three-body contribution to the total energy be made for each and every triplet of atoms in which the distances between neighbors are smaller than the range of V3 . To illustrate the reckoning of these three-body contributions

174

4 Energetic Description of Cohesion in Solids

Fig. 4.11. Schematic of the triangular lattice used in computing the total energy using angular forces.

to the total energy, we consider the simple case of the perfect two-dimensional triangular lattice shown in ﬁg. 4.11, and we further assume that the range of V3 is chosen such that only near-neighbor atoms are considered. Given these simplifying assumptions, the total energy per atom may be computed as E tot = 3V2 (Rnn ) + 6h(Rnn , 60◦ ) + 6h(Rnn , 120◦ ) + 3h(Rnn , 180◦ ),

(4.51)

where we have used the notation h(Rnn , θ) = h(Rnn , Rnn , θ ). The contribution of the angular term was arrived at by noting that by translational invariance, each and every atom has an identical local environment. In more complicated geometrical situations, the strategy required is similar. Essentially, it is necessary to ﬁnd all three-atom clusters that are within the required proximity and to sum up their contributions separately. Note that our example is especially artiﬁcial in the context of the Stillinger– Weber potential since for the triangular lattice it is 60◦ angles, and not the tetrahedral angles, that form the central angular motif. However, our reason for including this example is not to argue for the stability of the triangular lattice in the Stillinger–Weber context, but rather to show how calculations are made using this potential. We also note that in the remainder of the book, the Stillinger–Weber potential will often be invoked as the model of choice for discussing empirical treatments of Si in much the same way that the Johnson potential will serve as one of our key paradigms for pair functionals. The Stillinger–Weber scheme lacks the explicit environmental dependence that was argued to be of importance in our discussion of pair functionals. However, environmental dependence has been accounted for in covalent materials as well. Tersoff (1988) was one of the ﬁrst to suggest such a scheme, and his total energy

4.4 Potentials with Environmental and Angular Dependence

175

takes the form E tot =

1 r [V (Ri j ) + bi j V a (Ri j )], 2 ij

(4.52)

where V r (Ri j ) is a repulsive potential of the form Ae−λ1 Ri j and, similarly, V a (Ri j ) is an attractive potential of the form Be−λ2 Ri j . As Tersoff notes, the key novelty is buried in the function bi j . Indeed, it is via this function that both the environmental and angular dependences enter the potential. The form adopted by Tersoff is bi j = (1 + β n ζinj )(−1/2n) ,

(4.53)

where the function ζi j is in turn given by f c (Rik )g(θi jk ). ζi j =

(4.54)

k=i j

The function f c (R) is a cutoff function and passes quickly but smoothly from unity to zero as R → Rc , where Rc is a cutoff distance. The function g(θi jk ) is an angular term of the form g(θ ) = 1 +

c2 c2 − . d 2 d 2 + (h − cos θ )2

(4.55)

While these potentials are notationally complex, they are conceptually simple in terms of the basic physics they incorporate. In particular, potentials of this type invoke both of the new physical ideas presented in this section: environmental dependence and angular forces. In particular, the quantity denoted bi j guarantees that the interaction between two given atoms will depend upon both the number and disposition of neighboring atoms. For our purposes, the key advantage of the Tersoff potential is its attempt to capture effects which are outside of the purview of more traditional potentials. The Stillinger–Weber and Tersoff schemes as introduced above are essentially ad hoc. In forthcoming chapters, we will describe some of the successes and shortcomings of models like these. These examples will show that it is important to build intuition concerning the bonding in solids in order to formulate a clear idea as to when a particular empirical description of the energy is suitable and when it can be expected to fail. One way to service this ambition is to develop a more systematic scheme for deriving such potentials, or if not deriving them, then at least developing plausibility arguments for their functional form. The tack adopted here is to appeal to an understanding of the electronic structure of a material with special reference to the electronic density of states and its moments (which will be deﬁned shortly).

176

4 Energetic Description of Cohesion in Solids

4.5 Tight-Binding Calculations of the Total Energy Thus far, our emphasis has been on methods in which no explicit reference is made to the electronic degrees of freedom. In the present section we make our ﬁrst concession in the direction of incorporating electronic structure information into the total energy in the form of the tight-binding method. From the perspective of the general discussion given at the beginning of the chapter, the tight-binding total energy can be thought of in terms of the replacement E exact ({Ri , rn }) → E approx ({Ri , αi }),

(4.56)

where the coefﬁcients {αi } are expansion coefﬁcients that characterize the electronic wave function. That is, the tight-binding scheme represents an approximate treatment of the electronic structure of the material. The rudiments of the tight-binding method can be spelled out as follows. First, we take our cue from the discussion of the H2 molecule given in chap. 3, where we noted that the total molecular wave function could be written as a linear combination of atomic wave functions centered on the various sites making up the molecule. In the case of a solid, we will adopt the same strategy, this time with the electronic wave function of the entire solid being built up as a linear combination of the atomic wave functions centered on the various sites that make up the solid. The coefﬁcients in the linear combination of these basis functions will then be thought of as variational parameters, chosen so as to obtain the lowest possible energy. Finally, the resulting Hamiltonian matrix is diagonalized with the resulting eigenvalues serving as the basis for the calculation of the electronic contribution to the total energy. The tight-binding method will be exploited in two distinct senses. The ﬁrst main thrust of this section will be to show how the tight-binding method can be used to compute the total energy directly without recourse to some reduced description in terms of pair functionals or angular forces. Secondly, tight-binding arguments will be invoked in order to provide a plausibility argument for the form of both the pair functionals and angular potentials introduced in previous sections. Ultimately, the potentials will be seen to inherit the angular features of the moments of the electronic density of states. Prior to undertaking either of these objectives, we must ﬁrst describe the tight-binding method itself. 4.5.1 The Tight-Binding Method The tight-binding method is based upon the same set of observations that inspired the approach to molecular bonding introduced in chap. 3. We imagine that in the act of assembling the solid, the wave functions that characterize the isolated atoms are viable building blocks for describing even the complex wave function appropriate to the solid. When atoms are brought into one another’s proximity, the

4.5 Tight-Binding Calculations of the Total Energy

177

atomic energy levels associated with the outer valence electrons are disturbed as a result of the overlap of wave functions on adjacent atoms. This simple observation leads to a naive picture of the formation of the chemical bond. In particular, by summing up the occupied one-electron eigenvalues, one determines the electronic part of the total energy. As was shown in ﬁg. 3.13, as the number of atoms participating in the molecule increases, the resulting electronic spectrum becomes increasingly complex. Our discussion of the tight-binding method is intended to set forth in quantitative detail the recipe for computing the one-electron eigenvalues for solids. As noted already, the starting point of the analysis is an approximation to the total electronic wave function for the solid. In particular, we seek a wave function of the form n N aiα φα (r − Ri ), (4.57) ψ(r) = i=1 α=1

which we will write more compactly as |ψ =

N n

aiα |i, α.

(4.58)

i=1 α=1

The sum over i in eqns (4.57) and (4.58) runs over the number of atoms N in the solid, while the sum on α is over the number of orbitals per site. The atomic-like orbital of type α centered on site i is written as |i, α = φα (r − Ri ). Indeed, the nature of these orbitals and the size of the parameter n strikes right to the heart of the minimalist character of the semiempirical tight-binding method. As an example of the characteristics of the type of basis |i, α that might be used in a tight-binding calculation, we consider two distinct cases, that of Si, a covalently bonded semiconductor with an energy gap, and W, a transition metal with an electronic structure that is dominated by its d-electrons. We consider both examples, since each sheds different light on the questions that arise in the tight-binding context. As mentioned above, the basic spirit of tight-binding theory is minimalist in the sense that one searches for the smallest possible basis for expanding the total wave function. For the case of W, this might mean considering only ﬁve d-orbitals per atom. Recall from the discussion of chap. 3 that the solution of the atomic hydrogen problem resulted in a series of energy eigenvalues and their associated wave functions. These solutions could be organized along the lines of their angular momenta, with the possibility of s-orbitals (l = 0), p-orbitals (l = 1), d-orbitals (l = 2) and so on. For the case at hand, it is the 5d orbitals of W that serve as our basis. That is, each W atom has electrons from the 5d shell which contribute to the overall electronic wave function for the solid. We also observe that if we are interested in Si, for example, rather than

178

4 Energetic Description of Cohesion in Solids

W, our expansion will center on the outer 3s and 3p electrons. In this case, the total wave function is built up out of the four such basis functions at each site which for the i th site we label as |i, 3s, |i, 3px , |i, 3p y and |i, 3pz . Note that in keeping with our aim to shed unnecessary degrees of freedom, all reference to core electrons has been omitted; they are assumed to be unchanged by the proximity of neighboring atoms. In addition, the basis itself is incomplete in the mathematical sense, since we have not included higher energy atomic states such as |i, 4s, etc. in the basis. Having identiﬁed the nature of our approximation to the wave function, the next step in the argument concerns the evaluation of the energy. In particular, we aim to determine the series of coefﬁcients aiα which state with what weight the α th orbital on site i (i.e. |i, α) contributes to the total wave function |ψ. The scheme is to construct an energy function that depends upon the set of coefﬁcients aiα and to ﬁnd the values of those coefﬁcients that minimize that energy. Just as was done in our ﬁnite element treatment of the Schr¨odinger equation in chap. 3, we have replaced the problem of ﬁnding unknown functions (i.e. the wave functions) with that of ﬁnding unknown coefﬁcients through the device of writing the energy function ({aiα }) = ψ| Hˆ |ψ − Eψ|ψ,

(4.59)

where it is understood that the wave function ψ depends explicitly on the as-yet undetermined coefﬁcients aiα . Substitution of the total wave function given in eqn (4.58) into eqn (4.59) results in ({aiα }) =

N n

αβ

αβ

∗ (h i j − E Si j )aiα a jβ ,

(4.60)

i, j=1 α,β=1

where we have introduced the notation αβ ˆ φα∗ (r − Ri ) Hˆ φβ (r − R j )d 3 r, h i j = i, α| H | j, β =

(4.61)

and αβ Si j

= i, α| j, β = αβ

φα∗ (r − Ri )φβ (r − R j )d 3 r. αβ

(4.62)

The nature of the matrices h i j and Si j is subtle and as a result has been tackled from a number of different perspectives. Since our aim is to present ideas rather than to give an exhaustive description of each and every alternative approach to a given problem, the present discussion will try to highlight some of αβ the distinguishing features of these quantities. The matrix Si j provides a measure of the overlap of wave functions on adjacent sites, and is often described as the ‘overlap matrix’. For the purposes of the present discussion, we adopt the simplest

4.5 Tight-Binding Calculations of the Total Energy

179

approximation of orthonormality which is characterized mathematically as αβ

Si j = δi j δαβ ,

(4.63)

with the proviso that nonorthogonal tight-binding methods have much to recommend them and hence, the interested reader should pursue this matter further. αβ We make equally strong approximations in the context of the matrix h i j as well by resorting to the so-called two-center approximation. The basic idea of this approximation may be understood in qualitative terms by noting that the total Hamiltonian is constructed as a sum of potentials arising from the different atoms N (i.e. V (r) = i=1 Vatom (r − Ri )). The essence of the two-center approximation αβ is to say that the only terms from V (r) contributing to h i j are those arising from Vatom (r − Ri ) or Vatom (r − R j ). Within this approximation, a given matrix element depends upon both the separation and relative orientation of atoms i and j. The interactions between orbitals on different sites can be parameterized in terms of certain energetic factors Vssσ , Vppσ , etc. and the direction cosines l, m, n of the vector connecting the i th and j th atoms. As yet, however, our discussion has been generic and has not revealed insights into the nature of the tight-binding matrix elements themselves. To best see in qualitative terms where these matrix elements come from, we return to the simpler molecular setting. Recall that the orbitals of different angular momentum character have wave functions characterized by different numbers of lobes. An s-orbital is spherically symmetric, while p-orbitals have single lobes. As a result, the matrix elements which parameterize the interactions between orbitals on different sites depend exclusively on geometric/symmetry characteristics of the participating orbitals and, in particular, on the symmetry of these orbitals about the axis joining the two sites of interest. For example, for s-orbitals, the symmetry about the bond axis is such that we can rotate the orbitals about the bond axis with impunity (i.e. there is axial symmetry). Such bonds are labeled as σ bonds, and lead to the coupling Vssσ . However, axial symmetry bonds can also occur for p-orbitals. For example, if we have two atoms aligned along the z-axis, and consider the interaction between the pz -orbital on the ﬁrst atom and the pz -orbital on the second atom, this too has azimuthal symmetry and is parameterized by the coupling Vppσ . On the other hand, if we consider the coupling of pz -orbitals between two atoms that are neighbors along the x-axis, then the symmetry of their coupling is denoted by π, and leads to couplings of the form Vppπ . The geometry of orbitals associated with these couplings is depicted in ﬁg. 4.12. We take up the question of how precisely parameters such as Vssσ , Vppσ , Vppπ , Vddσ , etc. are determined later in this section. p p For example, for two p y -orbitals, the matrix element h i jy y can be split up into a term involving Vppσ and a second term involving Vppπ . As a result of these

180

4 Energetic Description of Cohesion in Solids

s Vss px

s Vsp -Vsp px states

px Vpp px

py Vpp py

states pz Vpp pz

Fig. 4.12. Schematic indication of the different symmetry types associated with couplings between orbitals on different sites (adapted from Harrison (1980)).

4.5 Tight-Binding Calculations of the Total Energy

181

Fig. 4.13. Radial dependence of the tight-binding coupling parameters for Si (adapted from Kwon et al. (1994)).

arguments, the calculation of the Hamiltonian matrix is reduced to a series of simple geometric operations (i.e. the determination of the direction cosines of the vector joining the two atoms of interest) in conjunction with a table known as the Slater–Koster table which illustrates how two orbitals are coupled. In addition to the dependence of the coupling between two sites on the relative orientation of the vector joining them, there is also a strong dependence of these couplings on the distance between the two sites. An example of the radial dependence of these couplings is shown in ﬁg. 4.13. Once the Hamiltonian matrix is in hand, the next step in the procedure is to seek the energy minimizing coefﬁcients {aiα }. This minimization is effected by ∗ computing ∂/∂aiα = 0 for all i and α, and results in a series of coupled algebraic equations that may be written in matrix form as (Hpp − Eδ pp )a p = 0, (4.64) p

where we have introduced the superindex p that runs from 1 to n N , with each p corresponding to a different one of the n N choices of i and α. This implies that we will have n N equations in the unknowns {aiα }. The result of solving these equations will be n N different energy eigenvalues and their corresponding set of expansion coefﬁcients which in turn determine the wave function itself. What has been learned thus far? We have noted that in the context of our truncated basis, built from the atomic orbitals characterizing the free atoms, the

182

4 Energetic Description of Cohesion in Solids

solution of the Schr¨odinger equation is mapped onto the equivalent problem of ﬁnding that set of expansion coefﬁcients that minimize the total energy. Like in the ﬁnite element context discussed earlier, minimization problems of this type lead to coupled equations such as that found in eqn (4.64). From the point of view of that set of equations, our problem has been reduced to a series of coupled linear algebraic equations and to ﬁnd the undetermined coefﬁcients we must diagonalize the Hamiltonian matrix. The result of this exercise is a series of energy eigenvalues that represent, within the conﬁnes of the present model, the allowed energy states of the solid. The spectrum of energy eigenvalues that emerge from the type of calculation spelled out above can be complex in the sense that there can be a large number of such eigenvalues spread across a wide range of energies. One way to tame this complexity is by virtue of the electronic density of states (DOS). The density of states is essentially a histogram that characterizes the distribution of eigenvalues which arise from solving problems concerning either the vibrational or electronic states of solids. In particular, the electronic density of states is deﬁned as δ(E − E i ), (4.65) ρ(E) = i

where the sum i is over the energy eigenvalues. Our present objective is to develop an understanding of the physical origins of these eigenvalues in the context of the electronic structure of a material. We already saw a schematic example of such a density of states in ﬁg. 3.13 which shows the densities of states for a series of model problems treated in the one-electron framework adopted in chap. 3. The vertical axis in that ﬁgure speciﬁes the energy of a given eigenstate. The more complex tight-binding analysis introduced here results in n N eigenvalues which may be used within the context of eqn (4.65) to obtain the density of states. Once the density of states has been determined, the electronic contribution to the energy may be obtained by summing the energies of all the occupied states. In terms of the density of states itself, this amounts to an evaluation of the integral F ρ(E)Ed E, (4.66) E el = 2 −∞

where the factor of 2 accounts for the fact that each state may be occupied by an electron of two different spins. The equation written above is the continuum limit of the discrete sum over energy eigenvalues (i.e. E el = 2 i i ) that we adopted earlier. In order to compute the total energy, the electronic term introduced above must be supplemented by a phenomenological treatment of those terms left out of the tight-binding description including the interactions between the various nuclei.

4.5 Tight-Binding Calculations of the Total Energy

183

This extra piece of the energy is often represented as a pair potential resulting in a total energy of the form F 1 Veff (Ri j ) + 2 Eρ(E)d E. (4.67) E tot ({Ri }) = 2 ij −∞ The effective pair potential can be determined by insisting that certain properties such as the lattice parameter, the cohesive energy and the bulk modulus are accurately reproduced. Of course, more sophisticated ﬁtting schemes are also possible. From a more concrete perspective, the application of eqn (4.67) is carried out as follows. A computational cell is considered in which the set of nuclear coordinates {Ri } is known. Given these coordinates, it is then possible to determine the various αβ matrix elements h i j which characterize the coupling of the α th orbital on site i to the β th orbital on site j. By assembling all such matrix elements, the full Hamiltonian matrix is thus known, and one can resort to either k-space or real space methods to determine the all-important density of states, ρ(E). Given this density of states, the electronic contribution to the total energy is determined by carrying out the integration indicated in eqn (4.67). The Fermi level itself (i.e. the upper limit of the integral) is determined by insisting that the atoms have the appropriate number of electrons. By tuning the Fermi energy, one tunes between the empty band and full band limits. In addition to the electronic term, we are also required to consider the pair term which demands lattice sums no different than those undertaken in our discussion of pair potentials. This procedure, therefore, gives an unambiguous transcription between a set of atomic positions and a corresponding total energy, thus paving the way for the investigation of questions relating to the coupling of structure and material properties. In chap. 6, we will return to the types of total energy analysis discussed here with special reference to the ability of tight-binding models to capture the relative energetics of competing crystal structures. In addition, in subsequent chapters, we will repeatedly make reference to the application of these methods for examining the energetics of a wide range of processes and mechanisms. The tight-binding method is a convenient entry level way to undertake calculations of the total energy in which reference to the electronic degrees of freedom is made explicitly. In addition, it has the added virtue that the calculations are computationally less demanding than those involving a more faithful treatment of the electronic degrees of freedom. Despite our ability to now write down with some level of conﬁdence the tight-binding description, our treatment has been overly cavalier in that we have as yet not stated how one might go about determining the Hamiltonian matrix αβ elements, h i j . Note that in precise terms these matrix elements describe the

184

4 Energetic Description of Cohesion in Solids

coupling between orbitals of character α and β on sites i and j, respectively. The basic thrust of the type of semiempirical tight-binding theories that it is our aim to discuss here is to assume that the interactions between orbitals on different sites may be empirically parameterized (through the parameters Vssσ , Vspσ , etc.) without ever really entering the debate as to the fundamental interactions between nuclei and electrons. The question of how to go about determining these ﬁtting parameters will be taken up once we have seen how the tight-binding description is carried out in the context of periodic solids. 4.5.2 An Aside on Periodic Solids: k-space Methods The description of tight binding introduced above advanced no assumptions about the symmetries present in the atomic-level geometry. As a result, the Hamiltonian matrix and the symmetries of the eigenfunctions deﬁed any generic classiﬁcation of the states along lines of their symmetries. On the other hand, in crystalline solids, the existence of translational symmetry leads to the expectation that the wave functions will have very special properties that guarantee that the charge density is the same in every unit cell. In particular, the existence of translational symmetries gives rise to so-called k-space methods which are the thrust of the present discussion. We specialize our discussion to periodic solids with the recognition that there are a wide variety of problems for which translational symmetry is lacking and that will therefore demand the more general perspective introduced above. Because of the presence of the regularity associated with a crystal with periodicity, we may invoke Bloch’s theorem which asserts that the wave function in one cell of the crystal differs from that in another by a phase factor. In particular, using the notation from earlier in this section, the total wave function for a periodic solid with one atom per unit cell is 1

|ψk = √ nN

n N

aα eik·Ri |i, α.

(4.68)

i=1 α=1

The ﬁrst sum is over cells, the i th of which is speciﬁed by the Bravais lattice vector Ri , while the second sum is over the set of orbitals α which are assumed to be centered on each site and participating in the formation of the solid. If there were more than one atom per unit cell, we would be required to introduce an additional index in eqn (4.68) and an attendant sum over the atoms within the unit cell. We leave these elaborations to the reader. Because of the translational periodicity, we know much more about the solution than we did in the case represented by eqn (4.58). This knowledge reveals itself when we imitate the procedure described earlier in that instead of having n N algebraic equations in the n N unknown

4.5 Tight-Binding Calculations of the Total Energy

185

coefﬁcients aiα , translational symmetry collapses the problem into a series of n coupled algebraic equations in the n unknowns aα , where n is the number of orbitals on each site. Imitating the treatment given in eqn (4.60), we can once again elucidate our variational strategy, but this time with the added knowledge that the wave function takes the special form given in eqn (4.68). In particular, the function we aim to minimize is (4.69) periodic ({aα }) = ψk | Hˆ |ψk − E k ψk |ψk , which in light of eqn (4.68) may be rewritten as periodic ({aα }) =

N n n j=1 α=1 β=1

αβ

eik·Rj aα∗ aβ h i j − E k

n α=1

aα∗ aα .

(4.70)

The energy eigenstates in the periodic case are labeled by the wave vector k. If we now seek those aα s that minimize eqn (4.70), and introduce the notation Hαβ (k) =

N

αβ

h i j eik·Rj ,

(4.71)

j=1

then the resulting problem may be rewritten as (Hαβ (k) − E k δαβ )aβ = 0.

(4.72)

β

The structure of our result is identical to that obtained in eqn (4.64) in the absence of any consideration of crystal symmetry. On the other hand, it should be remarked that the dimensionality of the matrix in this case is equal to the number of orbitals per atom, n, rather than the product n N (our statements are based on the assumption that there is only one atom per cell). As a result of the derivation given above, in order to compute the eigenvalues for a periodic solid, we must ﬁrst construct the Hamiltonian matrix H(k) and then repeatedly ﬁnd its eigenvalues for each k-point. Thus, rather than carrying out one matrix diagonalization on a matrix of dimension n N × n N , in principle, we carry out N diagonalizations of an n × n matrix. To complete the description, it is also necessary to understand the nature of the k-vectors themselves. For the purposes of the present discussion, we consider a one-dimensional periodic chain along the x-direction of N atoms with a spacing a between the atoms on the chain. One statement of Bloch’s theorem, which we set forth in one-dimensional language, is the assertion that the wave function in the n th cell ψn and that in the (n + 1)th cell, ψn+1 is given by ψn+1 = eika ψn .

(4.73)

186

4 Energetic Description of Cohesion in Solids

The periodicity of this one-dimensional crystal implies that ψ1 = ψ N +1 , or eik N a = 1,

(4.74)

which illustrates that the allowed k-vectors are of the form kn =

2πn , Na

(4.75)

where the integer n can assume the values 0, 1, . . . , N − 1. This collection of vectors deﬁnes a ﬁnite region in k-space known as the ﬁrst Brillouin zone. For the one-dimensional case being discussed here, it is convenient to consider the N vectors that run between −π/a and π/a. The three-dimensional analogs of the concepts introduced here involve no particular subtlety and are left to the reader as an exercise. In addition, further elaboration of these concepts can be found in Ashcroft and Mermin (1976). To illustrate the ideas presented above in concrete form, we now consider two separate one-dimensional examples of increasing sophistication. In the ﬁrst case, we consider a one-dimensional periodic solid and examine a tight-binding basis that consists of one s-orbital per site. As seen from the deﬁnition of the matrix H(k) given in eqn (4.71), this case is elementary since the Hamiltonian matrix itself is one-dimensional and may be written as H (k) = heika + he−ika ,

(4.76)

where we have introduced the parameter h to characterize the coupling between orbitals on neighboring sites. All interactions beyond those at the near-neighbor level are neglected and we have assumed that the ‘on-site’ coupling (i.e. i|H |i) is zero. Hence, the outcome of this calculation is a dispersion relation for the electronic states of the form E(k) = 2h cos ka.

(4.77)

This dispersion relation is plotted in ﬁg. 4.14. A more revealing example is provided by that of a linear chain in which each atom has four-basis functions, namely, s, px , p y and pz . This basis is of the same variety as that which is often used in the analysis of Si. In the present setting, the Hamiltonian matrix H(k) is obtained by recourse to the deﬁnition of eqn (4.71). In particular, we note that in the one-dimensional setting considered here, there p p p p ss are only six nonvanishing matrix elements, namely, h i,i = s , h i,ix x = h i,iy y = p p pz pz p p sp y y x x x ss h i,i = p , h i,i±1 = Vssσ , h i,i±1 = Vppσ , h i,i±1 = Vspσ and h i,i±1 = Vppπ . As a

4.5 Tight-Binding Calculations of the Total Energy

187

Fig. 4.14. Dispersion relation for a one-dimensional s-band tight-binding model.

result, the Hamiltonian matrix can be written down immediately as H(k) = s + 2Vssσ cos ka

2Vspσ cos ka 0 0

2Vspσ cos ka

0

0

p + 2Vppσ cos ka

0

0

0

p + 2Vppπ cos ka

0

0

0

p + 2Vppπ cos ka

.

(4.78) Because the structure of this matrix involves only a 2 × 2 subblock that is nondiagonal, two of the four energy bands are already determined and are degenerate with the form E(k) = p + 2Vppπ cos ka.

(4.79)

To ﬁnd the remaining two energy bands, we diagonalize the remaining 2 × 2 piece with the result that s + p + (Vssσ + Vppσ ) cos ka E ± (k) = 2 1 1 2 ) cos2 ka] 2 , ± [()2 + 4(Vσ )() cos ka + (4(Vσ )2 + 16Vspσ 2 (4.80) where we have introduced the notation = s − p and Vσ = Vssσ − Vppσ .

188

4 Energetic Description of Cohesion in Solids

Given our discussion of the band structures that arise on the basis of tightbinding arguments, we are now prepared to look a little more deeply into the logic behind the ﬁtting of tight-binding parameters. It is not really possible to provide any deﬁnitive statement which encompasses the diversity of ideas that have been brought to bear on the question of how best to determine tight-binding parameters. Evidently, there are any of a number of different schemes, many of which are founded on a sensible rationale. On the one hand, it is possible to imagine constructing parameterizations on the basis of the goodness of the ﬁt to the band structure itself. In these cases, one notes that the values of the energy at certain k-points within the Brillouin zone can be determined simply in terms of the unknown tight-binding parameters, with the result that a ﬁt is possible. However, in another sense, it is often the total energy that is of concern, so one can imagine determining the tight-binding parameters on the basis of energetic criteria. In either case, the central idea is more or less to determine the tight-binding expressions for a series of properties of interest a1 , a2 , . . . , an . In each case, from the tight-binding perspective, these properties are functions of the unknown parameters, and one’s task is to determine these parameters on the basis of these constraints. In mathematical terms, we are noting that f 1 (Vssσ , Vspσ , . . .) = a1 , f 2 (Vssσ , Vspσ , . . .) = a2 , .. . f n (Vssσ , Vspσ , . . .) = an .

(4.81)

Depending upon the strategy that has been adopted, it is possible to have as many equations as there are unknown coefﬁcients, in which case one is reduced to solving n equations in n unknowns. On the other hand, the number of equations could conceivably outnumber the number of unknowns in which case one resorts to solving these equations in the least-squares sense. An example of the type of success that can be attained by exploiting the tight-binding framework in the context of periodic solids is shown in ﬁg. 4.15, where the result of a tight-binding characterization of the band structure of Mo is contrasted with that determined from a full ﬁrst-principles calculation. For the present purposes, the key recognition is that once this type of ﬁtting procedure has been undertaken, it is possible to carry out calculations on both the electronic and structural properties of essentially arbitrary geometric conﬁgurations as long as the number of atoms is not so large as to be beyond the capacity to calculate.

4.5 Tight-Binding Calculations of the Total Energy

189

1

1

Fig. 4.15. Band structure for Mo as obtained from tight-binding calculations and from density functional theory (from Mehl and Papaconstantopoulos (1996)). The notation , N, H, etc. refers to particular k-points within the Brillouin zone.

4.5.3 Real Space Tight-Binding Methods Earlier in this chapter, we introduced pair and cluster functionals as approximate effective theories in which explicit reference to the electronic degrees of freedom had been removed. In each case, we introduced these total energy schemes on

190

4 Energetic Description of Cohesion in Solids

heuristic grounds without giving any strong arguments as to the origins of their particular functional forms. In the present section, we will see how tight-binding theory may be used to motivate both pair and cluster functionals, yielding both of the essential pieces of new physics represented by these schemes: environmental and angular dependence. As a preliminary to our discussion of the emergence of both pair functionals and angular forces from tight-binding theory, we ﬁrst discuss the moments of the density of states which serve as a useful basis for these developments. We begin with the recognition that every distribution has its moments. In particular, the n th moment of the density of states is deﬁned by ∞ µn = E n ρ(E)d E. (4.82) −∞

The moments of the density of states can be seen to be related to the electronic structure itself through the following argument. The shape of the electronic density of states determines the outcome of the one-electron sum embodied in eqn (4.66). The shape of the density of states is in turn determined by its moments. The connection between geometry and the electronic structure in the moments’ setting is revealed when we note that the moments may be written as products of matrix elements over directed paths starting and ending on the same atom. For the purposes of the present discussion we will consider an s-band tight-binding method in which our notation is collapsed in the form |i, s → |i. The elaboration to the more general situation in which there is more than one orbital per site can be carried out relatively painlessly. If we are interested in the second moment associated with a particular site, a more useful but equivalent deﬁnition to that given in eqn (4.82) is µ2 (i) = i|H 2 |i. Making use of the identity I = j | j j|, we see that the second moment may be written in the form µ2 (i) = h(Ri j )h(R ji ), (4.83) j

where h(Ri j ) = i|H | j. What this means is that to ﬁnd the second moment associated with a given site, we sum up all the products called for in eqn (4.83). For example, for an fcc crystal in which the matrix elements are assumed to vanish for distances greater than the near-neighbor distance, the second moment is 12h(Rnn )2 . For the higher-order moments, we have µ3 (i) = h(Ri j )h(R jk )h(Rki ) (4.84) jk

and µ4 (i) =

jkl

h(Ri j )h(R jk )h(Rkl )h(Rli ).

(4.85)

4.5 Tight-Binding Calculations of the Total Energy

191

These are the two lowest-order moments beyond the second moment itself. In this expression, the quantities h(R) characterize the strength of interaction between orbitals that are separated by a distance R. Yet higher-order moments can be obtained by recourse to the same basic ideas. Rectangular Band Model and Pair Functionals. As stated earlier, the ‘derivation’ of the pair functional ansatz may be approached from a variety of different viewpoints. One particularly revealing avenue which is relevant to understanding the emergence of pair functional descriptions of cohesion in transition metals such as Pd or Cu is to adopt the rectangular band model . This model density of states is shown in ﬁg. 4.16(a), and is contrasted with a rigorous density functional calculation of a transition metal density of states in ﬁg. 4.16(b). Despite the presence of a range of detail in the ﬁrst-principles density of states, the rectangular band model is very useful in elucidating qualitative trends in quantities such as the electronic contribution to the cohesive energy that depend upon integrated properties of the density of states. The rectangular band model posits that the density of states is constant over some range of energies and zero otherwise. The constant value associated with the density of states is chosen such that W/2 ρ(E)d E, (4.86) Nfull = 2 −W/2

where Nfull is the total number of electrons that can be accommodated in the band (including spin). This implies that the density of states within our rectangular band ansatz is given by ρ(E) = Nfull /2W . We may use this density of states to evaluate the electronic contribution to the total energy as a function of the ﬁlling of the band (i.e. the number of electrons, Ne ). The electronic contribution to the energy is given by Nfull F E el = Ed E, (4.87) W −W/2 where the Fermi energy, F , is dependent upon the band ﬁlling Ne through Nfull F d E, (4.88) Ne = W −W/2 yielding

Ne 1 F = W . − Nfull 2

(4.89)

In light of these insights, it is seen then that the electronic contribution to the

192

4 Energetic Description of Cohesion in Solids

Fig. 4.16. Comparison of ‘exact’ and rectangular band densities of states for osmium (adapted from Harrison (1980)): (a) density of states for osmium as computed using density functional theory and (b) density of states constructed by superposing a rectangular band model with a free-electron-like density of states. Rising lines in the two curves are a measure of the integrated density of states.

bonding energy is given by Nfull W E el = − 2

Ne Nfull

Ne 1− . Nfull

(4.90)

4.5 Tight-Binding Calculations of the Total Energy

193

Fig. 4.17. Band energy associated with rectangular band density of states. Energy is plotted in dimensionless units, scaled by the width of the band, W . Similarly, the band ﬁlling is plotted as a fraction of the full band.

The parabolic bonding proﬁle revealed above is shown in ﬁg. 4.17 and may be contrasted with the measured cohesive energies shown in ﬁg. 4.18, which in the case of the transition metals reveal just the same trends. The picture that we have advanced here is one of rigid bands in which it is imagined that in passing from one element to the next as we traverse the transition series, all that changes is the ﬁlling of the d-band, with no change in the density of states from one element to the next. It is also important to note that the bonding energy scales with the bandwidth, an observation that will makes its appearance shortly in the context of pair functionals. The rectangular band model developed above may be used as a tool to gain insights into the type of functional form that should be presumed in pair functionals such as those introduced earlier. In particular, if we consider a particular choice of band ﬁlling (i.e. ﬁx our attention on describing the energetics of a particular element), then the electronic contribution to the total energy of eqn (4.90) scales with the second moment of the density of states, since eqn (4.90) can be rewritten √ on the basis of the observation that W ∝ µ2 . To see that the bandwidth and the second moment of the density of states are indeed related, a plausibility argument can be made by appealing to a calculation of the second moment of the rectangular band density of states. In this case, the second moment is µ2 = 5W 2 /12, showing that the bandwidth scales with the square root of the second moment. Thus, if we consider as an example the case of a half-ﬁlled d-band (i.e. Ne /Nfull = 1/2) then √ eqn (4.90) tells us that E el = − 15µ2 /4. On the basis of the reasoning given

194

4 Energetic Description of Cohesion in Solids

Fig. 4.18. Experimental energies of cohesion as a function of the number of d-electrons (n d ) for the three transition metal series (adapted from Young (1991)).

above, the rectangular band model suggests a total energy that is written as the sum of the electronic contribution and a pair potential term that accounts for the interactions between nuclei, resulting in 1 φ(Ri j ) − α µ2 (i), (4.91) E tot = 2 ij i where the constant α is a parameter that depends upon the band ﬁlling and can be deduced on fundamental grounds or used as a ﬁtting parameter. To ﬁnish the argument, we need to know the way in which the second moment itself depends upon the geometric arrangement of atoms. At this point, it sufﬁces to note that if we are interested in the second moment associated with a particular site, it may be determined using eqn (4.83). The fact that the second moment can be written in pairwise form immediately suggests the correspondence between the pair functionals presented earlier and our present argument. Because the second moment is itself of the pairwise additive form, it is now seen that, like in the embedded atom description explored earlier, the energy per bond depends upon the coordination number. Moments and Angular Forces. Our aim in the present setting is to exploit the geometry of the densities of states in order to construct effective potentials for describing the bonding in solids which go beyond the pairwise forms considered thus far. We follow Carlsson (1991) in formulating that description. First, we reiterate that our aim is not the construction of the most up-to-date potentials that

4.5 Tight-Binding Calculations of the Total Energy

195

may be imagined. Rather, we wish to understand the microscopic origins of the angular terms which might appear in a total energy functional. For example, the total energy can take the form 1 eff 1 eff V2 (Ri , R j ) + V (Ri , R j , Rk ) 2 ij 3! i jk 3 1 eff V (Ri , R j , Rk , Rl ) + · · · . + 4! i jkl 4

E tot =

(4.92)

Our aim at this point is an analysis of the quantum mechanical underpinnings for the angular terms introduced above. We begin by assuming the existence of some reference state, the energy of which shall serve as our zero and from which all other energies are measured. In this state, if we assume that only n moments of the density of states are known, the electronic contribution to the total energy is given by ref

ref

E el = E(µ2 , µ3 , . . . , µref n ).

(4.93)

By way of contrast, if we interest ourselves in a particular conﬁguration and aim to determine its energy relative to the reference state, that energy may be written ref

ref

E el = E(µ2 + δµ2 , µ3 + δµ3 , . . . , µref n + δµn ),

(4.94)

where the δµi s reﬂect the difference between the moments of the reference state and the structure of interest. We now adopt the usual dodge of Taylor expanding in the presumed small deviations from the reference environment, resulting in an expression for the total energy change of the form ∂E E el = (µn − µref (4.95) n ). ∂µ n ref n This expression is enlightening in that it reveals that the effective interatomic potentials have inherited the explicit angular dependence of the moments and, further, that the potentials have an environmental dependence that is dictated by the ‘susceptibility’ ∂ E/∂µn . By absorbing the constant terms involving the reference state into our deﬁnition of the potentials, the energy of a given state may now be written as n ∂ E E el = µ(k) (4.96) n . ∂µ n ref k=1 n We have adopted the notation µn(k) to signify the contribution to the n th moment arising from paths connecting k atoms. We now seek a correspondence between eff eqns (4.92) and (4.96). In particular, Vk (R1 , . . . , Rk ) is obtained by adding up all

196

4 Energetic Description of Cohesion in Solids

the terms in eqn (4.96) involving atoms 1, 2, . . . , k. For example, the effective pair potential is given by eff V2 (Ri , R j )

=2

Nm ∂E n=2

∂µn

µ(2) n (Ri , R j ),

(4.97)

ref

th where we have deﬁned µ(2) n (Ri , R j ) as the two-atom contribution to the n moment involving atoms i and j. Note that we are considering two-atom contributions to all moments between the 2nd moment and the Nmth moment. Similar expressions are obtained in the case of the higher-order potentials. As said before, the key observation is that the potentials inherit the angular dependence of the moments. Though the notation used above is admittedly cumbersome, the basic idea associated with the development of these potentials is relatively straightforward. The idea was to expand the energy about a reference environment and to adopt a functional form for the potentials that is a direct inheritance from the moments of the density of states which themselves are deﬁned as directed paths involving the atoms in a given cluster. We must maintain the insight that the energies are measured relative to a reference environment. In particular, the susceptibilities are evaluated for the reference environment. As a result, depending upon the choice of reference environment, the relative strengths of the potentials will vary. To see this explicitly, consider the effective pair potential tied to the rectangular band model √ √ discussed above. Since E el scales as µ2 , we see that ∂ E el /∂µ2 ∝ 1/ µ2 . The implication of this result is that for a reference environment with a small µ2 (i.e. the atoms have fewer neighbors, such as at a surface) the effective potential is stronger. An example of the type of potentials that result upon adopting a strategy like that given above is shown in ﬁg. 4.19. We focus attention on the effective interactions involving clusters of four atoms The four-body terms are based upon a slightly more sophisticated scheme than that used here involving a basis more complex than the simple tight-binding basis considered here, but the basic concepts are identical. In this case, we see that for a metal such as Mo, four-body planar clusters with 90◦ angles are energetically costly and point to a substantial lowering of the energy of the bcc structure (which has no such clusters based on ﬁrst neighbors) and the fcc structure. As we have seen in the preceding sections, the development of empirical potentials is a mixture of plausibility arguments and sound guesswork. Despite their successes in accounting for the features of defects in a range of materials, even the best of potentials at times suffer from fatal weaknesses. Our aim now is to give a ﬂavor of the many attempts that have been put forth to build satisfactory interatomic descriptions for the direct simulation of problems of interest concerning real materials. One perspective has been offered by Heine et al. (1991) who note

4.6 First-Principles Calculations of the Total Energy

197

Fig. 4.19. Four-body potential for Mo (adapted from Moriarty (1990)).

“The success of the ‘glue’ models, which take many-atom forces speciﬁcally into account, has been impressive particularly in accounting for subtle effects such as the reconstructions of the Au surface. By way of contrast, one can point to the sad history of attempts to ﬁnd a satisfactory force model for Si. There has been a whole succession of models, each ﬁtted to experimental data plus the computed energies of a range of unstable structures covering quite a variety of bonding geometries. Yet each model failed when confronted a year or so later by the energy of some new structure.” At the time of this writing it remains an open question whether or not any satisfactory scheme can be developed for treating covalent materials. For the moment, the most reliable scheme is to use the full quantum mechanical description described in the next section. 4.6 First-Principles Calculations of the Total Energy As yet, our discussion has focused on the attempt to construct energy functionals in which there is some level of empiricism that mimics to a greater or lesser extent the presumed exact results of a full quantum mechanics calculation. Our reason for shying away from the full quantum mechanical calculations themselves was founded upon the fact that these methods are computationally intensive, and hence must be undertaken with the foresight to insure that they are used only when really necessary. It is the purpose of the present section to sketch the way in which ﬁrst-principles calculations are constructed.

198

4 Energetic Description of Cohesion in Solids

As our starting point, we begin by reminding ourselves of the basic facts that make the full many-electron problem so difﬁcult. A useful starting point is the Hamiltonian that describes both the electrons and the nuclei from which they are derived. The full many-particle Hamiltonian made its appearance in eqn (4.3), where it was shown that the various particle coordinates are linked in an exceedingly complicated way. If we adopt the purists’s perspective, we demand the full wave function which is a function not only of the electronic degrees of freedom, but of the nuclear degrees of freedom as well. As is clear from the full Hamiltonian, the Schr¨odinger equation corresponding to this many-body description is a coupled problem of enormous proportions. Nevertheless, through a combination of path-breaking theorems and numerical inventiveness, the calculation of electronic structure and associated total energies has still become routine. 4.6.1 Managing the Many-Particle Hamiltonian Density Functional Theory and the Local Density Approximation Even in light of the insights afforded by the Born–Oppenheimer approximation, our problem remains hopelessly complex. The true wave function of the system may be written as ψ(r1 , r2 , r3 , . . . , r N ), where we must bear in mind, N can be a number of Avogadrian proportions. Furthermore, if we attempt the separation of variables ansatz, what is found is that the equation for the i th electron depends in a nonlinear way upon the single particle wave functions of all of the other electrons. Though there is a colorful history of attempts to cope with these difﬁculties, we skip forth to the major conceptual breakthrough that made possible a systematic approach to these problems. In the language of the beginning of the chapter, the basic idea used in the density functional setting is to effect a replacement E exact ({Ri , rn }) → E approx [ρ(r), {Ri }].

(4.98)

In particular, Hohenberg and Kohn advanced the view that the total energy of the many-electron system may be written as a unique functional of the electron density of the form, ρ(r )ρ(r ) 3 3 1 d rd r + Vext (r)ρ(r)d 3 r, E[ρ(r )] = T [ρ(r)] + E xc [ρ(r)] + 2 |r − r | (4.99) and that the ground state energy of the system is attained on minimizing this functional. The various terms in this equation shape up as follows. T [ρ(r)] is the kinetic energy term, while the term E xc [ρ(r)] is the so-called exchange-correlation energy and refers to parts of the many-electron interaction whose origin is quantum mechanical. The remaining terms correspond to the direct electron–electron

4.6 First-Principles Calculations of the Total Energy

199

interaction and the interaction of electrons with an external potential (which can include the ions). In the problem section at the end of the chapter, we take up the question of how a simple model for the kinetic energy functional can be built up using what we have already learned about the electron gas. As it stands, the statement given above is exact. The profundity of the insight buried in the density functional given above is related to the fact that it allows for an exact mapping of our perceived hopeless many-electron problem onto a set of effective single particle equations. The only difﬁculty is that the functional itself is unknown. However, the strategy suggested in eqn (4.98) is to use a local approximation to the exchange-correlation functional which results in a series of approximate, but highly accurate, one-electron equations. We also note that local approximations like those introduced here will reveal themselves of relevance in other continuum settings. As said above, the key assertion is that the ground state energy corresponds to that density that minimizes the functional of eqn (4.99). Of course, until something can be said about the form of T [ρ(r)] and E xc [ρ(r)], we don’t have a practical scheme for obtaining the total energy. The next key step in the analysis was the introduction of an approximation which converted the original problem into a corresponding problem for a ﬁctitious system involving noninteracting electrons in the presence of an effective potential. The key approximation is known as the local density approximation and consists in the statement E xc [ρ(r)] = xc (ρ(r))d 3 r. (4.100) As we said above, in the absence of knowledge of the exchange-correlation functional E xc [ρ(r)] itself, our results were only suggestive. The key additional insight that makes this formulation a viable calculational scheme is the local density approximation in which, once again, appeal is made to the properties of the electron gas. In this instance, the idea is to presume that the exchange-correlation functional may be approximated by the electron gas exchange-correlation functional xc (ρ), which is known. The use of this functional in the solid is based upon the assumption that the local behavior of the electrons in the solid mimic those of the corresponding homogeneous electron gas at the same density. In light of this approximation, we are now prepared to seek the energy minimizing density ρ(r) which is obtained by minimizing this functional, that is by effecting the functional derivative δ E[ρ(r)]/δρ(r) = 0.

(4.101)

This results in a set of single particle equations, known as the Kohn–Sham

200

4 Energetic Description of Cohesion in Solids

equations given by h¯ 2 2 ∇ ψi (r) + Veff (r)ψi (r) = i ψi (r). 2m The effective potential is given in turn as δ E xc ρ(r )dr + . Veff (r) = Vext (r) + |r − r | δρ(r) −

(4.102)

(4.103)

Note that at this point we have turned the original (hopeless) many-body problem into a series of effective single particle Schr¨odinger equations. As will become increasingly evident below, there are a number of different particular realizations of the general ideas being set forth here. For example, in the context of the exchange-correlation energy itself, there are several popular parameterizations of the density dependence of the exchange-correlation energy that are in use. Recall that the exchange-correlation energy is representative of those parts of the electron–electron interaction which are purely quantum in nature. Part of the variety that attends the various computer implementations of density functional theory in the local density approximation surrounds the different parameterizations for this term. The key point is that from an analytic perspective, even after making the simplifying assumption that it is the exchange-correlation energy of the uniform electron gas that is needed, xc (ρ) cannot be described fully. Often, one resorts to parameterizations which satisfy known constraints in the limits that the density of the electron gas is either very high or very low, and then searches for interpolation formulae in the intervening density regime which can be informed on the basis of quantum Monte Carlo calculations of this property. A detailed discussion of many of the popular parameterizations for this term can be found in table 7.1 of Dreizler and Gross (1990) and the attendant prose. 4.6.2 Total Energies in the Local Density Approximation Once the effective single particle equations have been derived, there are almost limitless possibilities in terms of the different schemes that have been invented to solve them. By way of contrast, the assertion is often made that if the calculations in these different realizations of the ﬁrst-principles methodology are made correctly, then the predictions of these different implementations should be the same. Interactions Between Nuclei and Electrons Note that in our treatment of the Kohn–Sham equations, we assume the existence of an external potential Vext (r) which characterizes the interactions of the nuclei and the electrons. Given our interest in modeling the properties of solid materials,

4.6 First-Principles Calculations of the Total Energy

201

Vext will arise as a superposition of the potentials associated with each of the nuclei making up the solid. In the most direct of pictures, one can imagine treating the solid by superposing the ‘bare’ nuclear potentials for each atom, and subsequently solving for the disposition of each and every electron. This approach is the basis of the various ‘all-electron’ methods. As an alternative to the explicit treatment of each and every electron, a variety of methods have grown up around the use of effective potentials in which Vext is meant to mimic the nucleus and its complement of core electrons which are presumed to be indifferent to the changes in environment in going from the free atom to the solid. Indeed, much of the spirit of this book centers on the idea of reduced descriptions in which degrees of freedom are eliminated in the name of both conceptual simplicity and computational tractability and the use of pseudopotentials like those described above is a compelling example of this strategy. It is crucial to realize that in the process of formation of the solid, many of the low-lying atomic states (i.e. those electrons that are tightly bound to the nucleus in inner shells) are disturbed very little by the formation of the solid. As a result, pseudopotential schemes attempt to exploit this observation by creating an effective potential in which the nucleus and the core electrons together serve to inﬂuence the outer electrons. The key idea is a choice of pseudopotential that reproduces known properties such as atomic wave functions or the scattering properties associated with the full potential. An example of a pseudopotential is given in ﬁg. 4.20. For our purposes our interest in this idea is as observers rather than practitioners, with the key insight gleaned from the observation being the formal way in which degrees of freedom are eliminated. Choosing a Basis In our statement of the Kohn–Sham equations, nothing has been said about the way in which ψ(r) itself will be determined. Many methods share the common feature that the wave function is presumed to exist as a linear combination of some set of basis functions which might be written generically as αn bn (r), (4.104) ψ(r) = n

where αn is the weight associated with the n th basis function bn (r). Just as with the earlier statement of tight-binding theory, solving the relevant equations becomes a search for unknown coefﬁcients rather than unknown functions. Part of the variety associated with the many different incarnations of density functional codes is associated with this choice of basis functions. For example, in the spirit of the earlier tight-binding discussion, one can imagine a basis constructed out of functions localized about each atomic site. Alternatively, we can

202

4 Energetic Description of Cohesion in Solids

pseudo

rc

r

v Vpseudo

Z/r

Fig. 4.20. Schematic of pseudopotential and associated pseudowave function (adapted from Payne et al. (1992)).

take our cue from the physics of the electron gas and attempt to expand the total wave function in terms of a free-electron-like basis. If one is to use the so-called plane wave basis set, then the generic wave function for a state characterized by wave vector k is represented as ak+G ei(k+G)·r . (4.105) ψk (r) = G

In this case, the vectors G are members of the set of reciprocal lattice vectors and eqn (4.105) really amounts to a three-dimensional Fourier series. The task of solving the Kohn–Sham equations is then reduced to solving for the unknown coefﬁcients ak+G . The only difﬁculty is that the potential that arises in the equation depends upon the solution. As a result, one resorts to iterative solution strategies. Computing the Electronic Structure and the Total Energy Once the Kohn–Sham equations have been solved, we are in a position to evaluate energies, forces and the electronic structure of a material itself. In particular, with the eigenvalues i and corresponding wave functions ψi (r) we can compute the energy of the system explicitly. As can be seen from the discussion given above, and as has been true with each of the total energy methods introduced in this chapter, in the end we are left with a scheme such that once the nuclear

4.7 Choosing a Description of the Total Energy: Challenges and Conundrums 203

Fig. 4.21. Densities of states for several bcc transition metals as computed using density functional theory (adapted from Eriksson et al. (1992)).

coordinates have been provided, one can compute the corresponding energy. From the perspective of computational materials science, this step is of primary importance since it is the key to ﬁrst examining the structure and energetics of the various defects that populate materials, and ultimately to explicating how those structures conspire to give rise to the properties of materials. Part of the added value of using methods in which the electronic degrees of freedom are treated explicitly is the insights that may be garnered concerning the electronic properties of a material. To provide some feel for the types of results that emerge, an example of the densities of states for several materials is shown in ﬁg. 4.21.

4.7 Choosing a Description of the Total Energy: Challenges and Conundrums This chapter has emphasized the microscopic approach to computing the total energy of solids. We have seen that there are a number of different schemes for computing the total energy, each with its own advantages and difﬁculties. In simplest terms, the largest conundrum faced in the selection of a total energy description concerns the compromise that must usually be made between computational tractability and accuracy. Treatments featuring the electronic degrees of freedom explicitly are often plagued by the inability to treat system sizes capable of

204

4 Energetic Description of Cohesion in Solids

resolving the problem of interest without the contaminating inﬂuences of nearby boundaries. On the other hand, empirical schemes, while able to handle much larger system sizes, suffer a shortcoming of similar magnitude in that the results can often be charged with lacking physical realism. In subsequent chapters, we will show how the types of energy functionals described here may be used as a tool for computing the properties of materials. Part of our approach will be to attempt to tackle particular case studies from the perspective of several different total energy methods. Our intention in adopting this approach is to illustrate the way in which some methods provide a clearer physical picture of the problem at hand, while others are to be noted for their physical accuracy. 4.8 Further Reading ‘Beyond Pair Potentials’ by A. E. Carlsson, in Solid State Physics edited by H. Ehrenreich and D. Turnbull, Academic Press, San Diego: California, Vol. 43, pg. 1, 1990. This article gives a thorough discussion of the conceptual underpinnings associated with efforts to build effective potentials as a way to eliminate explicit reference to electronic degrees of freedom. ‘Many-atom interactions in solids’ by V. Heine, I. J. Robertson and M. C. Payne, Phil. Trans. Roy. Soc. Lond., A334, 393 (1991) gives a thoroughly thoughtful overview of the difﬁculties that must be faced in trying to create effective theories of interatomic interactions in which explicit reference to the electronic degrees of freedom has been renounced. Electronic Structure and the Properties of Solids by W. A. Harrison, W. H. Freeman and Company, San Francisco: California, 1980. Harrison’s book espouses the tight-binding perspective in a way that reveals how this method may be applied to consider materials ranging from Si to Ta. I have learned much from this book. ‘Tight-binding modelling of materials’ by G. M. Goringe, D. R. Bowler and E. Hern´andez, Rep. Prog. Phys., 60, 1447 (1997). This article gives an up-to-date review of the continued uses of the tight-binding formalism. Solids and Surfaces: A Chemist’s View of Bonding in Extended Structures by R. Hoffmann, VCH Publishers, New York: New York, 1988. This book reﬂects the chemist’s intuition as regards bonding in solids. Hoffmann has a special talent for constructing plausible models of the electronic structure of solids on the basis of insights strictly in terms of the crystalline geometry and the character of the underlying atomic orbitals. Another book that espouses the chemical perspective on bonding in solids is

4.8 Further Reading

205

Chemical Bonding in Solids by J. K. Burdett, Oxford University Press, Oxford: England, 1995. One of the key features that I enjoy in looking at the work of both Hoffmann and Burdett is their willingness to confront systems not only with a high level of structural complexity, but chemical complexity as well. Bonding and Structure of Molecules and Solids by D. Pettifor, Clarendon Press, Oxford: England, 1995. A superb contribution aimed at explaining the fundamental physical reasoning associated with constructing models of bonding in solids. Primary emphasis is placed on metals and covalent materials. The Electronic Structure and Chemistry of Solids by P. A. Cox, Oxford University Press, Oxford: England, 1987. Like the book by Hoffmann, this book takes a more chemical perspective of bonding in solids. Though the mathematical sophistication demanded of the reader is fairly low, this does not imply that there is not much to be learned here. A book I have returned to repeatedly. ‘Iterative minimization techniques for ab initio total energy calculations: molecular dynamics and conjugate gradients’, by M. C. Payne, M. P. Teter, D. C. Allan, T. A. Arias and J. D. Joannopoulos, Rev. Mod. Phys., 64, 1045 (1992). Despite the title which makes it appear highly specialized, this article has much to offer on everything from the LDA formalism itself, to issues of convergence and the use of LDA calculations (rather than classical potentials) as the basis of molecular dynamics. ‘Modern Electron Theory’ by M. W. Finnis in Electron Theory in Alloy Design edited by D. G. Pettifor and A. H. Cottrell, Institute of Materials, London: England, 1992. This is my favorite article on ﬁrst-principles calculations. Finnis spells out all of the key points involved in carrying out ﬁrst-principles calculations of the total energy. ‘Understanding quasi-particles: observable many-body effects in metals and 3 He’ by J. W. Wilkins in Fermi Surface edited by M. Springford, Cambridge University Press, New York: New York, 1980. Wilkins’ article describes many of the issues that arise in thinking about the many-body aspects of the total energy in solids. Density Functional Theory by R. M. Dreizler and E. K. U. Gross, Springer-Verlag, Berlin: Germany, 1990. This book concerns itself primarily with the formalism of density functional theory and less with the speciﬁcs of a given computer implementation. It has much to offer on the origins of the Kohn–Sham equations, the treatment of the exchange-correlation energy and on reﬁnements such as gradient corrections.

206

4 Energetic Description of Cohesion in Solids

4.9 Problems

1 Fitting parameters in the Lennard–Jones potential In this chapter, we introduced the Lennard–Jones potential given by 12 6

σ σ . − V (r ) = V0 r r

(4.106)

Determine the constants V0 and σ for fcc Xe by using the fact that the cohesive ˚ Energy energy of Xe is 0.17 eV/atom and the lattice parameter is 6.13 A. ˚ Carry out the units for the potential should be in eV and length units in A. solution to this problem both analytically (by ﬁtting these energies only for a near-neighbor model) and numerically, by using six-neighbor shells. For further details see Kittel (1976).

2 Morse Potential and Cohesion in Cu The Morse potential is given by V (r ) = V0 (e−2a(r −r0 ) − 2e−a(r −r0 ) ), where V0 , a and r0 are parameters to be determined by ﬁtting to experimental data. Using the experimental data for the cohesive energy of fcc Cu (E coh = 336 kJ/mole), ˚ and the bulk modulus the fcc Cu equilibrium lattice parameter (a0 = 3.61 A) ˚ −1 ) and r0 (in (B = 134.3 GPa), determine the parameters V0 (in eV), a (in A ˚ under the assumption that only near-neighbor atoms interact. A)

3 Forces within the Pair Functional Formalism Given the prescription for the total energy as deﬁned within the pair functional formalism, compute the expression for the force on atom i as a result of its interactions with its neighbors. In particular, compute Fi = −∂ E tot /∂ xi , remembering that there is implicit dependence on xi through the density. Use your result to demonstrate that if the cutoff range of the interactions is denoted as Rcut , then the motion of an atom at a distance of 2Rcut from the atom of interest can result in a force on that atom. The result of this calculation is given in eqn (4.43).

4 Effective Pair Interactions from Pair Functionals The pair functional formalism may be recast in the language of pair potentials by computing an effective pair potential which is valid for environments close

4.9 Problems

207

to some reference environment. In this problem, starting with eqn (4.33), consider small deviations about some reference environment characterized by an electron density ρref . By writing the total density at a given site as ρref + δρ and Taylor expanding the embedding term, show that the resulting expression for the total energy takes the form of a pair potential. Using Johnson’s analytic embedded-atom functions introduced in this chapter, obtain and plot the effective pair potentials valid for both the bulk environment and for the (100) surface of an fcc crystal.

5 Stillinger–Weber Energy for Si in Diamond Cubic Structure In eqn (4.51) we derived an expression for the total energy of a twodimensional triangular lattice. That expression was for a geometrically unrealistic structure for a covalently bonded material. Derive an analogous expression for the total energy of Si when in the diamond cubic structure.

6 Forces Associated with Stillinger–Weber Potentials Obtain an expression for the forces between atoms in a system characterized by the Stillinger–Weber potential. An explicit expression may be found in Wilson et al. (1990).

7 Electronically Driven Structural Transformations Consider an s-band tight-binding Hamiltonian with matrix elements i|H | j = h 0 /r , where r is the distance between atoms i and j. The goal of this problem is to examine the electronic driving force for dimerization of a linear chain of atoms by examining the electronic structure and resulting cohesive energy for a chain of atoms with nominal lattice parameter a0 as shown in ﬁg. 4.22. Consider a dimerization reaction in which the new lattice is characterized by alternating spacings a0 − δ and a0 + δ with the result that there are two atoms per unit cell with a lattice parameter of 2a0 . Assume that each atom has one electron (i.e. the case of half-ﬁlling) and obtain the electronic contribution to the energy as a function of the parameter δ. Note that each atom is coupled only to its near neighbors on the left and right, though the strength of that coupling is scaled by 1/r as described above. Plot the electronic energy as a function of δ and comment on the implications of your result.

208

4 Energetic Description of Cohesion in Solids

Fig. 4.22. Chain geometries to be considered in problem 7 corresponding to: (a) the undimerized state and (b) the dimerized state.

8 d-Band Tight-Binding Model for fcc Metal In this problem you are asked to obtain an expression for the dispersion relation along the (100) direction in k-space for fcc Ni. The calculation should be done using a basis of ﬁve d-orbitals per atom, with the parameters Vddσ , Vddπ and Vddδ chosen in the ratio Vddσ : Vddπ : Vddδ = −6 : 4 : −1.

9 Tight-Binding for Crystals with Multiple Atoms per Unit Cell In eqn (4.68), we developed the tight-binding formalism for periodic systems in which there was only one atom per unit cell, with each such atom donating n basis functions to the total electronic wave function. Generalize the discussion presented there to allow for the presence of more than one atom per cell. In concrete terms, this means that the basis functions acquire a new index, |i, J, α, where the index i speciﬁes the unit cell, J is a label for the atoms within a unit cell and α remains the label of the various orbitals on each site.

10 Density of States for Electron Gas In the previous chapter we described the physics of the electron gas. Using the ideas described there, deduce the density of states, ρ(E) for the one-, two- and three-dimensional electron gas. In particular, show how the density of states scales with the energy and plot your results. Recover the expression for the cohesive energy of the electron gas by evaluating integrals of the form F E el = 2 ρ(E)Ed E. (4.107) 0

4.9 Problems

209

11 Simple Model for the Kinetic Energy Functional The density functional introduced in eqn (4.99) featured a kinetic energy term denoted T [ρ(r)]. In this problem, derive an expression for a kinetic energy functional based upon the simple electron gas physics described in chap. 3. In particular, if the total kinetic energy per atom is of the form 3 h¯ 2 E eg 2 = (3π 2 ρ) 3 , (4.108) N 5 2m then what form should the kinetic energy density t(ρ(r)) take in writing a kinetic energy functional of the form T [ρ(r)] = t (ρ(r))d 3 r? Now that this kinetic energy functional is in hand, write an approximate functional for thetotal energy of the form ρ(r )ρ(r ) 3 3 1 3 d rd r + Vext (r)ρ(r)d 3 r, E T F [ρ(r)] = t (ρ(r))d r + 2 |r − r | (4.109) subject to the constraint that ρ(r)d 3 r = N , (4.110) where N is the total number of electrons. Note that we have introduced the notation E T F [ρ(r)] to refer to the fact that we are making the Thomas–Fermi approximation. By computing the functional derivative of the Thomas–Fermi functional subject to the constraint given above, obtain the equation satisﬁed by the ground state density.

FIVE

Thermal and Elastic Properties of Crystals

5.1 Thermal and Elastic Material Response As yet, our discussion of modeling the energetics of crystalline solids has centered on the analysis of atomic conﬁgurations that are undisturbed by deformation, by the thermal vibrations that are inevitably present at ﬁnite temperatures or by defects. Before embarking on an analysis of the full-ﬂedged defected solid, we begin with a consideration of geometric states that may be thought of as relatively gentle perturbations about the perfect crystal. In particular, the aim of the present chapter is to assess the energetics of both thermal vibrations and elastic deformations, with a treatment that is uniﬁed by the fact that in both cases the energy can be expanded about that of the perfect crystal which serves as the reference state. Prior to examining the ways in which the methods of chap. 4 can be used to examine the energetics of both thermal vibrations and elastic deformations, we consider the signiﬁcance of these excitations to the properties of materials at large. The methods of the present chapter feed into our quest to understand the properties of materials in several distinct ways. First, as will be described in the following paragraphs, a variety of important material properties involve the energetics of thermal vibration or elastic deformation directly, including the speciﬁc heat, the thermal conductivity, the thermal expansion and the elastic moduli themselves. However, in addition to the direct signiﬁcance of the ideas to be presented here to the analysis of thermal properties, much of what we will have to say will form the methodological backdrop for our discussion of the thermodynamic ideas invoked to understand phase diagrams, diffusion and microstructural evolution. In chap. 4 we argued that much can be learned by comparing the energetics of different competing states of a crystalline solid. One set of material parameters that can be understood on the basis of total energy methods like those presented in the previous chapter in conjunction with the methods of statistical mechanics are those related to the thermal response of materials. Indeed, one of the workhorses 210

5.1 Thermal and Elastic Material Response

211

Fig. 5.1. Speciﬁc heat for Cu as obtained from Debye model contrasted with experimental results (adaptation of Debye’s original results by Reif (1965)).

of the statistical mechanics curriculum is the evaluation of the speciﬁc heat of crystalline solids as a function of the temperature. A representative example of the experimentally observed speciﬁc heat of solids is shown in ﬁg. 5.1. Our discussion of the theoretical apparatus that is needed to understand these data will provide a variety of lessons in the use of total energy methods in conjunction with statistical mechanics. A second class of material parameters associated with the thermal behavior of solids is more traditionally thought of as those associated with ‘anharmonic effects’ in solids and includes the thermal conductivity and the coefﬁcient of thermal expansion. As already shown in ﬁg. 1.2, the thermal conductivity of different material classes ranges over a number of orders of magnitude and involves a variety of different mechanisms including the scattering of phonons by point defects as will be brieﬂy described in chap. 7. The coefﬁcient of thermal expansion also looms as an important material parameter, with an increasingly important technological role as a result of the reliance on complex heterostructures in which many different materials are joined together. In these cases, it is the mismatch in thermal expansion coefﬁcient which is of particular signiﬁcance since this mismatch results in thermal stresses that can lead to mechanical failure. The use of thermal expansion mismatch as an engineering tool in the form of the bimetallic strip dates at least as far back as the creation of the famed clocks of John Harrison described in Dava Sobel’s Longitude (1995). It is amusing to note that the application of thermal mismatch preceded its understanding on the basis of statistical mechanics by nearly 250 years.

212

5 Thermal and Elastic Properties of Crystals

In addition to the thermal properties mentioned above, the present chapter also has as its charter the investigation of the elastic (both linear and nonlinear) properties of solids. We begin by noting that the linear theory of elasticity is one of several prototypical continuum theories and is at the heart of analyses of problems ranging from the formation of dislocations in Six Ge1−x to the deformation of bridges subjected to loads from wind and earthquakes. As noted earlier, continuum theories such as the linear theory of elasticity are silent on the values of the material parameters used to characterize solids. As a result, it is the business of subscale analysis, such as is offered by the types of microscopic energy functionals described in the previous chapter, to evaluate the elastic response of different materials. An example of the diversity of elastic properties as measured by the Young modulus is shown in ﬁg. 1.1. In the preceding paragraphs, we have given a sketch of some of the material parameters that are explicitly tied to the thermal and elastic response of solids. However, as we already noted, the tools developed to examine these material parameters are of much broader importance to the generic aim of modeling materials and their response. Indeed, the ideas to be presented in the present chapter serve as the backbone for an analysis of thermostatics (i.e. the study of equilibria) and of kinetics in solids. The discussion above was meant to highlight the various material parameters related to the thermal properties of solids. In the following paragraphs we also show the origins of the methodological relevance of the material in the present chapter to our later examination of both equilibria and kinetics in solids. One of the central points of contact between the methods of the present chapter and an analysis of material response will be the application of these methods to the construction of free energies. Whether our aim is the investigation of phase diagrams or the driving forces on interfaces, one of the elemental challenges that will be faced will be that of the construction of the relevant free energy. For example, in the context of phase diagrams, we will see that a central part in the competition between different phases is played by the vibrational entropy of these competing phases. In addition to the consideration of equilibrium problems, the treatment of thermal excitations is also important to the investigation of kinetics. An intriguing insight into kinetics is that in many cases, the tools for treating thermal excitations to be described in this chapter can be used to consider driven processes such as diffusion. As will be noted in chap. 7, models of kinetics are tied to the idea that as a result of the random excursion of atoms from their equilibrium positions, a system may occasionally pass from one well in the multi-dimensional potential energy surface to another. Indeed, this eventuality has already been rendered pictorially in ﬁg. 3.22 where we saw an adatom hopping from one energy well to the next in its

5.2 Mechanics of the Harmonic Solid

213

excursion across a crystal surface. As will be seen below, the treatment of these excursions, at least in the case of small displacements, can be put on a formal basis that allows for the construction of explicit models of thermal activation. A less explicit way in which the methods of the present chapter are of paramount importance is the way in which they can instruct us in our aim of building effective theories based on some reduced set of degrees of freedom. As we have emphasized repeatedly, one of our central tasks is the construction of effective theories in which the degrees of freedom used in the model subsume the full set of microscopic degrees of freedom. For instance, in chap. 8, we will see that despite the complicated atomic-level motions which attend plastic deformation, it is possible to construct models based on defect-level entities, namely, dislocations, without mandating the consideration of atomic positions or motions explicitly. These dislocations represent the collective motion of huge numbers of atoms which have suffered relative displacements across a common slip plane. An interesting side effect of our construction of such effective models is that they require that we institute some notion of dissipation. For example, as the dislocation traverses the crystal some of the energy associated with its center of mass motion is transferred to the microscopic degrees of freedom which are disguised from the effective theory that interests itself only in the overall dislocation motion. The methods of the present chapter begin to teach us how to think of the coupling of the center of mass motions of defects to atomic-level motions, and thereby to construct models of dissipation. The plan of the following sections is as follows. First, we undertake an analysis of the energetics of a solid when the atoms are presumed to make small excursions about their equilibrium positions. This is followed by a classical analysis of the normal modes of vibration that attend such small excursions. We will see in this case that an arbitrary state of motion may be speciﬁed and its subsequent evolution traced. The quantum theory of the same problem is then undertaken with the result that we can consider the problem of the speciﬁc heat of solids. This analysis will lead to an explicit calculation of thermodynamic quantities as weighted integrals over the frequencies of vibration.

5.2 Mechanics of the Harmonic Solid As noted in the introduction to the present chapter, the contemplation of thermal and elastic excitations necessitates that we go beyond the uninterrupted monotony of the perfect crystal. As a ﬁrst concession in this direction, we now spell out the way in which the energy of a weakly excited solid can be thought of as resulting from excursions about the perfect crystal reference state. Once the total energy of such excursions is in hand, we will be in a position to write down equations of

214

5 Thermal and Elastic Properties of Crystals

motion for these excursions, and to probe their implications for the thermal and elastic properties of solids.

5.2.1 Total Energy of the Thermally Fluctuating Solid Our starting point for the analysis of the thermal and elastic properties of crystals is an approximation. We begin with the assertion that the motions of the i th atom, will be captured kinematically through a displacement ﬁeld ui which is a measure of the deviations from the atomic positions of the perfect lattice. It is presumed that this displacement is small in comparison with the lattice parameter, |ui | a0 . Though within the context of the true total energy surface of our crystal (i.e. E tot (R1 , R2 , . . . , R N )) this approximation is unnecessary, we will see that by assuming the smallness of the excursions taken by the atoms of interest, a well-deﬁned and tractable formulation of the thermal properties of the solid may be made. As in chap. 4, we posit the existence of a total energy function of the form E tot (R1 , R2 , . . . , R N ) = E tot ({Ri }), where {Ri } denotes the entire set of ionic coordinates. For simplicity, the total energy is allowed to depend only upon the ionic positions (i.e. we have ignored the explicit dependence of the total energy function on the electronic degrees of freedom thus assuming that the system remains on the Born–Oppenheimer energy surface). Since our interest is in ref excursions about the equilibrium positions Ri , we now advance an expansion of the total energy about the reference conﬁguration in powers of the small displacements ui . In particular, the total energy of the instantaneous ﬂuctuating ref snapshot of the solid characterized by atomic positions {Ri + ui } is written as ref

ref

E tot ({Ri + ui }) = E tot ({Ri }) +

∂ E tot i,α

+

∂ Riα

u iα

1 ∂ 2 E tot u iα u jβ + · · · . 2 iα jβ ∂ Riα R jβ

(5.1)

The α th component of displacement of the i th ion is denoted u iα . The rationale for our strategy is cast in geometric terms in ﬁg. 5.2 which shows the quadratic approximation to a fully nonlinear energy surface in the neighborhood of the minimum for an idealized two-dimensional conﬁguration space. This ﬁgure allows us to contrast the energy in both its exact and approximate guises. It is clear that in the vicinity of the minimum, the total energy is well characterized by what will shortly be revealed as a far-reaching but tractable model. Further progress can be made in trimming down the various terms embodied in the equation above by recognizing that the expansion is built around

5.2 Mechanics of the Harmonic Solid

215

Full Nonlinear Potential

Quadratic Potential

Fig. 5.2. Nonlinear potential energy V (x1 , x2 ) and corresponding quadratic approximation to that potential. The cutaway in the upper left hand corner shows one quadrant of the two potentials to illustrate their correspondence in the limit of small displacements.

the equilibrium conﬁguration and hence the terms linear in u iα can be eliminated since at equilibrium we have ∂ E tot /∂ Riα = 0. Furthermore, since the ﬁrst term is an uninteresting constant it is found convenient to deﬁne our zero of energy as ref E tot ({Ri }) = 0 leaving us with the result that ref

E tot ({Ri + ui }) =

1 αβ K u iα u jβ , 2 iα jβ i j

(5.2)

where the stiffness matrix (more conventionally known as the force constant matrix) is deﬁned by αβ

Ki j =

∂ 2 E tot . ∂ Riα ∂ R jβ

(5.3)

Note that the expressions we have written thus far are entirely generic. All that we have assumed is the existence of a total energy function that is dependent upon the set of ionic positions. Our analysis is thus indifferent to the microscopic energy functional used to compute E tot and hence the results are equally valid for total energy methods ranging from pair potentials to fully quantum mechanical E tot s. On

216

5 Thermal and Elastic Properties of Crystals

the other hand, the ease with which we can expect to determine the stiffness matrix is signiﬁcantly different, with pair potentials allowing for analytic determination of K and density functional calculations demanding a signiﬁcant computational effort. From the standpoint of our consideration of effective theories, it is especially interesting to note that regardless of our choice of microscopic energy functional, the result embodied in eqn (5.2) is nothing but a sophisticated model of atoms coupled with springs.

5.2.2 Atomic Motion and Normal Modes Having identiﬁed our approximation to the total energy associated with small vibrations about equilibrium, we are now in a position to construct the classical equations of motion which dictate the ionic motions. If we make the simplifying assumption that we are concerned with an elemental material (i.e. all the masses are identical, etc.), thus surrendering some of the possible generality of our treatment, the equation of motion for the α th component of displacement associated with the i th ion is given by m

αβ ∂ E tot d 2 u iα = − = − K i j u jβ . dt 2 ∂ Riα jβ

(5.4)

We note, however, that the added complication of including different masses at different sites does not change any of the key physical ideas. For further details the reader is urged to consult Maradudin et al. (1971). What has emerged from our analysis is a series of coupled linear differential equations in which the accelerations at one site are coupled to the displacements at the other sites. Though clearly our ambition at this point is to solve these coupled differential equations, we may recast this objective in different terms. In particular, we are after the appropriate linear combinations of the atomic-level displacements which will render the matrix K diagonal and lead to independent ‘modes’ of vibration. We anticipate the nature of the desired result by insisting that the solution take the form of a normal mode solution (which in the quantum setting we will refer to as phonons) in that each and every atom is imagined to vibrate with the same frequency ω but with different amplitudes. This conjectured behavior calls for the trial solution u iα (t) = u iα eiωt ,

(5.5)

where u iα is the amplitude of the displacement and where the physical motion is obtained by considering the real part of this expression. We hope the reader will forgive our notation in which the letter i serves both as a label of atomic positions as well as the unit imaginary number. Note that as yet we have presumed nothing

5.2 Mechanics of the Harmonic Solid

217

Fig. 5.3. Mass–spring system consisting of two point masses used in normal mode analysis considered in eqn (5.9).

about the possible geometric symmetries of the atomic positions. On the assumed solution given above, we ﬁnd that the equations of motion may be rewritten as αβ K i j u jβ . (5.6) −mω2 u iα = − jβ

This series of coupled linear equations in the unknowns u iα may be seen in a different light if written in direct form as the matrix equation, [K − mω2 I]u = 0,

(5.7)

where I is the identity matrix. Here we use the compact notation in which the displacements u iα are contained in the vector u 11

u 12 u 13 u= u 21 . ..

.

(5.8)

uN3 When our problem is recast in this form it is clear that we are reconsidering it as one of matrix diagonalization. Our task is to ﬁnd that change of variables built around linear combinations of the u iα s that results in a diagonal K. Each such linear combination of atomic displacements (the eigenvector) will be seen to act as an independent harmonic oscillator of a particular frequency, and will be denoted as ‘normal coordinates’. Before undertaking the formal analysis of vibrations in solids, it is worthwhile to see the machinery described above in action. For concreteness and utter simplicity, we elect to begin with a two-degrees-of-freedom system such as that depicted in ﬁg. 5.3. Displacements in all but the x-direction are forbidden, and we assume that both masses m are equal and that all three springs are characterized by a stiffness k. By inspection, the total potential energy in this case may be written as 1 1 1 V (u 1 , u 2 ) = ku 21 + ku 22 + k(u 2 − u 1 )2 , 2 2 2

(5.9)

218

5 Thermal and Elastic Properties of Crystals

where u i refers to the x-component of displacement of mass i. Following the prescription outlined in eqn (5.4), the two equations of motion become m u¨ 1 + 2ku 1 − ku 2 = 0,

(5.10)

m u¨ 2 + 2ku 2 − ku 1 = 0.

(5.11)

and

These equations can be rewritten in the more sympathetic matrix form as u1 u1 2k −k = mω2 . −k 2k u2 u2

(5.12)

This equation may be rewritten as the requirement 2k − mω2 −k det = 0, (5.13) −k 2k − mω2 √ √ which results in the vibrational frequencies ω− = k/m and ω+ = 3k/m. In fact, we could have arrived at the lower of these frequencies without calculation by noting that this mode corresponds to the motion of the two masses in unison without any stretching of the spring that couples them. In effect, they are vibrating as if they are only attached to the springs that are tied to the walls. The eigenvectors that are allied with our two frequencies correspond precisely to the motion in unison described above and the opposite mode in which the two masses are exactly out of phase. The general solution in this instance may then be written as 1 1 u 1 (t) = A1 cos ω− t + B1 sin ω− t 1 1 u 2 (t) 1 1 (5.14) + A2 cos ω+ t + B2 sin ω+ t. −1 −1 The undetermined coefﬁcients Ai and Bi allow for the speciﬁcation of the relevant initial data in the form of the initial positions and velocities of the two masses. In the more general setting in which we imagine 3N degrees of freedom, our analysis goes through in the same way. As mentioned earlier, the strategy remains one of ﬁnding independent normal modes in which every ion is presumed to vibrate at the same frequency. As with our two-masses problem, in principle all that remains is a diagonalization of the stiffness matrix K. If we consider the generalization to a fully three-dimensional situation, then the α th component of displacement of the i th ion may be represented in general terms as (s) u iα (t) = u iα (As cos ωs t + Bs sin ωs t), (5.15) s

where As and Bs are as-yet undetermined constants that insure that our solution has

5.2 Mechanics of the Harmonic Solid

219

(s) the full generality needed to capture an arbitrary state of displacement, u iα is that th part of the eigenvector associated with the s normal mode that is tied to the α th component of displacement of atom i and the sum over s is a sum over the various normal modes. As yet, we have illustrated that the mechanics of harmonic vibrations can be reduced to the consideration of a series of independent normal modes. This normal mode decomposition is an especially powerful insight in that it points the way to the statistical mechanical treatment of the problem of the thermal vibrations of a crystal. The Hamiltonian for the problem of harmonic vibrations can be written as

H=

p2 1 αβ iα + K u iα u jβ , 2m 2 i j αβ i j iα

(5.16)

where piα is the α th component of momentum associated with atom i and the second term is the harmonic part of the potential energy of the system as introduced in eqn (5.2). The key result we will highlight presently is that when this Hamiltonian is rewritten in terms of the normal modes, it reduces to a series of uncoupled harmonic oscillators which from the point of view of both quantum and statistical mechanics may each be treated independently. As it stands, the Hamiltonian as written in eqn (5.16) represents a coupled problem since the equation of motion for the i th atom depends upon the coordinates of the remaining atoms. Again in keeping with our contention that much of the business of effective theory construction is about ﬁnding the right degrees of freedom, we note that in the present context by adopting the correct linear combinations of the original coordinates {u iα }, the original problem can be recast in much simpler terms. To simplify the analysis, we introduce the notation ηr (t) = Ar cos ωr t + Br sin ωr t. In terms of this notational convention, eqn (5.15) may be rewritten as (s) u iα ηs (t), (5.17) u iα (t) = s

and hence the original Hamiltonian may similarly be rewritten as 1 αβ (r ) (s) 1 (r ) (s) u iα u iα η˙r (t)η˙ s (t) + K u u ηr (t)ηs (t). (5.18) H= m 2 iα r s 2 i j αβ r s i j iα iβ This expression may now be cast in its most useful form by recourse to certain (s) . In particular, key orthogonality relations satisﬁed by the eigenvectors u iα (r ) (s) we assert without proof (see Marion (1970)) that iα u iα u iα = δr s and that αβ (r ) (s) 2 i K i j u iα u ibeta = ωr δr s . In light of these orthogonality relations, our Hamiltonian reduces to 1 1 2 2 2 η˙ (t) + ωr ηr (t) . (5.19) H= 2 r 2 r

220

5 Thermal and Elastic Properties of Crystals

What we have learned is that our change to normal coordinates yields a series of independent harmonic oscillators. From the statistical mechanical viewpoint, this signiﬁes that the statistical mechanics of the collective vibrations of the harmonic solid can be evaluated on a mode by mode basis using nothing more than the simple ideas associated with the one-dimensional oscillator that were reviewed in chap. 3. We have already learned a great deal about the atomic-level treatment of vibrations in solids and in the paragraphs that follow intend to consolidate our gains by invoking the known translational periodicity of crystals. Let us examine what more can be said about the vibrational spectrum without actually doing any calculations. First, we note that for a generic conﬁguration of N atoms, there will be 3N vibrational modes, corresponding to the dimensionality of the stiffness matrix itself. We have found that the eigenvectors associated with the stiffness matrix may be constructed to form an orthonormal set, and that we can determine coefﬁcients such that arbitrary initial data may be matched. However, as yet there has been a serious oversight in our reasoning. We have forgotten that in the case of crystalline solids, the repetitive nature of the geometry implies special symmetry relations that lead to vast simpliﬁcations in the analysis of both their electronic and vibrational states. At this point we are poised to replace our problem of diagonalization of a 3N × 3N matrix by N diagonalizations of a 3 × 3 matrix. The crucial insight that makes this further simpliﬁcation of our problem possible is known as either Bloch’s theorem or Floquet analysis. As was already shown in chap. 4 (see eqn (4.68)), the basic idea is the assertion that on account of the translational periodicity, the solution in one unit cell can differ from that in other cells by at most a phase factor. The physical content of the statement above can be translated into mathematical terms by recognizing that this extra piece of information about the solution allows us to go beyond the trial solution of eqn (5.5), to suggest u iα (t) = u α eiq·Ri −iωt .

(5.20)

Note that we have presumed something further about the solution than we did in our earlier case which ignored the translational periodicity. Here we impose the idea that the solutions in different cells differ by a phase factor tied to the Bravais lattice vector Ri . The result is that the eigenvector u α has no dependence upon the site i; we need only ﬁnd the eigenvectors associated with the contents of a single unit cell, and the motions of atoms within all remaining cells are unequivocally determined. Substitution of the expression given above into the equations of motion yields αβ K i j u β (q)eiq·Rj = 0. (5.21) −mωq2 u α (q)eiq·Ri + jβ

By virtue of the crystal’s periodicity we can, without loss of generality, take Ri =

5.2 Mechanics of the Harmonic Solid

0. The equation given above may consequently be rewritten Dαβ (q)u β (q) = 0, −mωq2 u α (q) +

221

(5.22)

β

where we have deﬁned the ‘dynamical matrix’ as αβ K 0 j eiq·Rj . Dαβ (q) =

(5.23)

j

As a result of these deﬁnitions, eqn (5.22) may be rewritten in matrix form as [D(q) − mω2 I]u(q) = 0.

(5.24)

Just as was found in the discussion prior to eqn (4.75), the set of allowed q vectors is restricted because of the condition that the crystal is periodic. Indeed, because of this restriction, the q vectors are of the form qx = 2πm 1 /N a, q y = 2πm 2 /N a and qz = 2π m 3 /N a, where m 1 , m 2 and m 3 take only integer values. We have thus reduced our original problem which demanded the diagonalization of a 3N × 3N matrix to a problem in which we diagonalize a 3 × 3 matrix N times, where q adopts N different values and labels the different vibrational states. Here we have trimmed our analysis down such that we consider only the case in which there is one atom per unit cell. Aside from index gymnastics, the extension to more atoms in each cell is relatively uneventful. Note also that the present discussion parallels, even in the details, that already given in the context of the electronic structure of periodic solids in chap. 4. What we have learned is that our solutions may be labeled in terms of the vector q, which is known as the wavevector of the mode of interest. Each such mode corresponds to a displacement wave with wavelength λ = 2π/|q|. This interpretation makes it clear that there is a maximum |q| above which the oscillations are associated with lengths smaller than the lattice parameter and hence imply no additional information. This insight leads to an alternative interpretation of the signiﬁcance of the ﬁrst Brillouin zone relative to that presented in chap. 4. As an aside, we also note that had we elected to ignore the translational periodicity, we could just as well have solved the problem using the normal mode idea developed earlier. If we had followed this route, we would have determined 3N vibrational frequencies (as we have by invoking the translational periodicity), but our classiﬁcation of the solutions would have been severely hindered. The standard textbook exercise for illuminating the ideas discussed above in their full generality is that of the linear chain of atoms. The simplest variant of this exercise assumes that all the masses are the same as are all of the springs joining them. In this case, the dynamical matrix itself is one-dimensional and hence its

222

5 Thermal and Elastic Properties of Crystals

eigenvalues are immediate. From above, we note that K 011j eiq R j , D11 (q) =

(5.25)

j

where in our case we have K 00 = 2k, and K 01 = K 0,−1 = −k. To see this, recall that the total potential energy of our one-dimensional chain can be written in simplest terms as 1 ki j (u i − u j )2 . (5.26) E tot = 2 ij If we make the simplifying assumption of only nearest-neighbor interactions via springs of stiffness k, then the only terms involving atom 0 are 1 (5.27) E 0 = k (u 0 − u −1 )2 + (u 1 − u 0 )2 . 2 In light of this insight, it follows that the elements of the stiffness matrix are those assigned above. Explicitly evaluating the sums demanded by the dynamical matrix, yields the spectrum 4k qa sin . (5.28) ω(q) = m 2 This spectrum of vibrational frequencies is shown in ﬁg. 5.4. We note again that the signiﬁcance of this result is that it tells us that if we are interested in a particular displacement wave characterized by the wavevector q, the corresponding frequency associated with that wave will be ω(q). One of the key outcomes of this calculation is that it shows that in the limit of long wavelengths (i.e. small qs) the conventional elastic wave solution is recovered (i.e. ω = Cq, where C is the relevant sound velocity), while at the zone edges the waves are clearly dispersive. The use of the word dispersive is intended to convey the idea that the wave speed, dω/dq, depends explicitly on q. An additional way in which the outcome of the normal mode analysis may be analyzed is by recourse to the distribution of vibrational frequencies. This distribution of modes is captured most succinctly via the vibrational density of states deﬁned by ρ(ω) =

N modes

δ(ω − ωn ).

(5.29)

n=1

The idea here is that the Nmodes vibrational frequencies may be bunched up over certain frequencies, and will have some maximum frequency. Just as the electronic density of states introduced in chap. 4 succinctly encompassed much of the key information about the electronic spectrum, the vibrational density of states will

5.2 Mechanics of the Harmonic Solid

223

Fig. 5.4. Dispersion relation, ω vs q, for a linear chain of atoms.

play an analogous role in our analysis of the thermodynamics of solids. In the case of the linear chain, we may arrive at the vibrational density of states analytically. Before venturing our analytic solution for the vibrational density of states, we examine the ideas pictorially. In ﬁg. 5.4 we examine the dispersion relation. Note that each region of q-space of width 2π/N a corresponds to a single mode. (In fact, we need to be slightly cautious on this point since in addition to the mode with wavevector q there is a partner mode with wavevector −q.) However, we have interested ourselves in the distribution of states as a function of frequency ω. The correspondence is made in the ﬁgure where we note that in regions where ∂ω/∂q ≈ 0, there are many q-vectors per unit interval in ω while for those regions where ∂ω/∂q is large, there are but a few. To compute the vibrational density of states explicitly, we make the correspondence ρ(ω)dω = (N a/π )dq. What we have noted is that in a region of q-space of width dq, there are 2dq/(2π/N a) states since the uniform spacing between q-points is 2π/N a and the factor of 2 in the numerator accounts for the q and −q degeneracy. We may reorganize this statement as ρ(ω) =

1 Na . π |dω/dq|

(5.30)

For the dispersion relation given above for the linear chain, we have ω0 a qa dω = cos , dq 2 2

(5.31)

√ where we have deﬁned ω0 = 4K /m. We must now rewrite the right hand side of this equation in terms of ω. We note that qa −1 ω . (5.32) = sin 2 ω0

224

5 Thermal and Elastic Properties of Crystals

Fig. 5.5. Vibrational density of states associated with linear chain.

This is nothing more than an inversion of the dispersion relation. In geometric " 2 2 terms, what we have learned is that cos(qa/2) = ω0 − ω /ω0 and thus ρ(ω) =

1 2N " , π ω2 − ω2 0

(5.33)

which is shown in ﬁg. 5.5. As noted earlier, the vibrational density of states provides an alternative representation of the information content present in the dispersion relation, though there is a loss of information concerning the q vector associated with each frequency. As will be seen in subsequent discussions, a knowledge of the vibrational density of states will allow us to compute key thermodynamic properties such as the entropy associated with thermal vibrations. What has been lost in our treatment of the restricted geometry of the onedimensional chain is the possibility for different wave polarizations to be associated with each wavevector. In particular, for a three-dimensional crystal, we expect to recover modes in which the vibrations are either parallel to the wavevector (longitudinal) or perpendicular to it (transverse). On the other hand, the formalism outlined above already makes the outcome of this analysis abundantly clear. In particular, for a simple three-dimensional problem in which we imagine only one atom per unit cell, we see that there are three distinct solutions that emerge from our matrix diagonalization, each of which corresponds to a different polarization. To make these ideas concrete, we consider the case of a solid characterized by a pair potential and with a total energy of the form E tot =

1 φ(Ri j ). 2 ij

(5.34)

5.2 Mechanics of the Harmonic Solid

225

αβ

Our charter is to ﬁrst compute the matrix K i j introduced earlier and then to evaluate its Fourier transform in preparation for the computation of the spectrum αβ of vibrational frequencies. By deﬁnition, the matrix K i j is obtained as αβ

Ki j =

∂ 2 E tot . ∂ Riα ∂ R jβ

(5.35)

Within the pair potential formalism under consideration presently, this involves a series of exercises in the use of the chain rule since we have to evaluate terms of the form ∂ E tot 1 ∂ Rlm = φ (Rlm ) . (5.36) ∂ Riα 2 lm ∂ Riα Note that there is a slight burden of notational baggage which we will try to dispel by observing that we have deﬁned Rlm = |Rl − Rm |, and at the same time have used Riα to denote the α th Cartesian component of the position vector of atom i. Thus we have adopted a convention in which a pair of Latin indices implies consideration of a pair of atoms, while a mixed pair of a single Latin and a single Greek index refers to a particular component of the position vector of a given atom. Carrying out the differentiations demanded by eqn (5.35), the force constant matrix may be written as αβ

(Riα − Rmα )(Riβ − Rmβ ) δi j 2 Rim m (Riα − R jα )(Riβ − R jβ ) − φ (Ri j ) Ri2j δi j δαβ (Riα − Rmα )(Riβ − Rmβ ) + φ (Rim ) − φ (Rim ) δi j 3 Rim Rim m m

Ki j =

φ (Rim )

+ φ (Ri j )

(Riα − R jα )(Riβ − R jβ ) δαβ − φ (Ri j ) . 3 Ri j Ri j

(5.37)

We show this result primarily to illustrate that what are really required to determine the force constant matrix are the derivatives of the relevant interatomic potential, and then the consideration of a series of lattice sums as embodied in the various m s that appear above. Once the force constant matrix is in hand, the next step in the procedure for obtaining the spectrum of vibrational frequencies is the determination of the dynamical matrix. For the simple case in which there is only one atom per unit cell, this amounts to carrying out the sums illustrated in eqn (5.23). It is worth exploring this question a little further. We note that we require the αβ sum Dαβ (q) = j K 0 j eiq·Rj . Analytic progress can be made by exploiting several

226

5 Thermal and Elastic Properties of Crystals αβ

key symmetries of the force constant matrix K i j . First, we claim that there is a αβ sum rule of the form j K 0 j = 0 which arises from the fact that if every atom is displaced by the same amount, there is no net force on any atom (for further details see the problems at the end of the chapter). This then allows us to note that we can rewrite the self-term in the force constant matrix as αβ αβ K0 j . (5.38) K 00 = − j=0

As a result of the observation implicit in eqn (5.38), we can now write the dynamical matrix as αβ Dαβ (q) = K 0 j (eiq·Rj − 1). (5.39) j=0

This may be further simpliﬁed by noting that for every term R j in the sum we will have a partner term −R j , and also by using the fact that the force constant matrix is the same for these partner terms. As a result, we have 1 αβ iq·Rj Dαβ (q) = K (e + e−iq·Rj − 2), (5.40) 2 j=0 0 j which after simpliﬁcation leaves us with Dαβ (q) = −2

j=0

αβ

K 0 j sin2

q · Rj . 2

(5.41)

The conclusion of this analysis is that we can obtain the dynamical matrix by performing lattice sums involving only those parts of the force constant matrix that αβ do not involve the self-terms (i.e. K 00 ). We note that the analysis we have made until now has been performed in the somewhat sterile setting of a pair potential description of the total energy. On the other hand, the use of more complex energy functionals does not introduce any new conceptual features. As a case study in the calculation of the relation between ω and q (also known as phonon dispersion relations) for three-dimensional crystals, we consider the analysis of normal modes of vibration in fcc Al. As will be evident repeatedly as coming chapters unfold, one of our principal themes will be to examine particular problems from the perspective of several different total energy schemes simultaneously. In the present context, our plan is to consider the dispersion relations in Al as computed using both empirical pair functional calculations as well as ﬁrst-principles calculations. As the analysis given above illustrated for the case of a pair potential, the determination of the dynamical matrix demands the evaluation of lattice sums involving the products of geometric factors and the derivatives of the various

5.2 Mechanics of the Harmonic Solid [q00]

X

[qq0]

227 [qqq]

L

10

Al

T2

(THz)

8

6

4

L L

L

T1

T

T

2

0 0.00 0.25 0.50 0.75 1.00 q

0.75

0.50 q

0.25

0.00

0.25 q

0.50

Fig. 5.6. Phonon dispersion relation for Al as computed using pair functional approach (adapted from Mishin et al. (1999)). The lines correspond to the theoretical results and the points are experimental data obtained from neutron scattering.

energy terms. The basic procedure is unchanged in the case of the pair functional scheme although the presence of the embedding term introduces a whole new set of terms in the force constant matrix and hence in the dynamical matrix as well. A particularly simple description of these additional terms may be found in Finnis and Sinclair (1984). Once the lattice sums required in the computation of the force constant matrix have been carried out, all that remains is the calculation and subsequent diagonalization of the dynamical matrix with results like those shown in ﬁg. 5.6. The results given above can be measured not only against those resulting from experiments, but also against those deduced on the basis of ﬁrst-principles calculations. An example of the outcome of a ﬁrst-principles analysis of phonons in fcc Al is shown in ﬁg. 5.7 (Quong and Klein 1992). These calculations were carried out using pseudopotentials to represent the ion–electron interaction and with a plane wave basis for expanding the wave function. We note in passing that the use of ﬁrst-principles techniques to compute the phonon spectrum involves further subtleties than were hinted at in our discussion above, and we content ourselves only with showing the results of such calculation. We wish to emphasize that our primary ambition in the present setting has not been to debate the vices and virtues of any particular treatment of the lattice vibrations of a particular system. Rather, our aim has been to illustrate what is involved in carrying out such calculations and to reveal the way in which the outcome of these calculations is communicated,

228

5 Thermal and Elastic Properties of Crystals

Fig. 5.7. Phonon dispersion relation for Al as computed using ﬁrst-principles methods (adapted from Quong and Klein (1992)).

namely in terms of the types of phonon dispersion relations shown in ﬁgs. 5.6 and 5.7.

5.2.3 Phonons Until now, our treatment has been built in exactly the same terms that might have been used in work on normal modes of vibration in the latter part of the nineteenth century. However, it is incumbent upon us to revisit these same ideas within the quantum mechanical setting. The starting point of our analysis is the observation embodied in eqn (5.19), namely, that our harmonic Hamiltonian admits of a decomposition into a series of independent one-dimensional harmonic oscillators. We may build upon this observation by treating each and every such oscillator on the basis of the quantum mechanics discussed in chap. 3. In light of this observation, for example, we may write the total energy of the harmonic solid as

1 (5.42) n(q, α) + h¯ ωq,α . E= 2 q,α The interpretation that we adopt in this setting is that the various modes are each characterized by a different occupation number, n(q, α), where q characterizes the wavevector of the mode of interest and α labels the various polarizations. In this context, the occupation of each normal mode is associated with a discrete entity known as a phonon. Each such phonon carries an energy h¯ ω(q, s) and a momentum h¯ q and may be assigned properties traditionally thought of as being tied to particles. For example, phonons may scatter off of one another. However, we also note that in order to develop a full picture of the phonons and their interactions,

5.2 Mechanics of the Harmonic Solid

229

Fig. 5.8. Schematic of the C60 molecule (adapted from Woo et al. (1993)).

it is necessary to extend the harmonic treatment of vibrations entertained above to include the anharmonic effects which give rise to such scattering.

5.2.4 Buckminsterfullerene and Nanotubes: A Case Study in Vibration One of the approaches favored in the present work is the idea of attempting to give a thorough description of robust physical principles followed by more speculative application of those principles to problems of current interest. One class of materials that has garnered particular attention in recent years is the class of fullerenes in which by virtue of either ﬁve- or seven-membered rings, curvature is induced in the normally ﬂat packings of carbon based upon six-membered rings. The most celebrated such example is perhaps the C60 molecule in which a total of 60 carbon atoms form a molecular structure with vertices reminiscent of those on a soccer ball. Beyond the interest that has attached to C60 itself, there has been a surge of interest in carbon nanotubes. The aim of the present subsection is to give a sense of how the physics of phonons introduced above plays out in the context of relatively complex molecules and solids. The C60 molecule is shown in ﬁg. 5.8. The distinctive ﬁve-fold rings are clearly evident in the ﬁgure. In this instance, we have 3N = 180 independent degrees of freedom, although six of them are associated with uninteresting rigid body translations and rotations. Our aim in the present section is to examine the nature of vibrations in several exotic carbon structures, and we begin with the C60 itself. The calculations to be described here were based on ﬁrst-principles techniques in which the electron–ion interaction was handled using pseudopotentials in conjunction with a mixed basis including both plane wave states and localized s- and p-orbitals associated with the carbon atoms (Bohnen et al. 1995). As has already been made clear, to

230

5 Thermal and Elastic Properties of Crystals

Fig. 5.9. Vibrational displacement patterns associated with ﬁve different modes of the C60 molecule (adapted from Heid et al. (1997)). The left and right hand panels correspond to opposite extremes in motion associated with a given mode. Labels associated with each mode characterize the symmetry of the displacement pattern.

obtain the phonon frequencies, it is necessary to construct the dynamical matrix. Diagonalization of this matrix results in a series of vibrational frequencies ωs and associated eigenvectors which give the relative amplitudes of vibration for the different degrees of freedom. The disposition of the vibrational frequencies may be summarized pictorially via the vibrational density of states. Note that in a highly symmetric object like the C60 molecule the occurrence of certain degeneracies in this spectrum is not accidental and can be predicted on the grounds of this symmetry without doing any explicit matrix diagonalizations. In addition to our interest in the spectrum of vibrational frequencies that emerge from the type of analysis being described here, it is also of interest to characterize the nature of the associated eigenvectors. Recall that these eigenvectors yield the nature of the displacement patterns that will be associated with a given mode of vibration. In the case of C60 , some of the different displacement patterns are revealed in ﬁg. 5.9, though the amplitudes of the displacements are exaggerated to more easily reveal the symmetry of the various modes. As noted above, in addition to the interest that has been attached to the C60 molecule and its crystalline incarnations, a torrent of interest has also developed around the existence of carbon nanotubes in which planar graphite-like packings of carbon atoms are folded onto themselves to form cylinders. We note that there is great variety in the structures that can be created since the line along which the original planar sheet is cut prior to wrapping it to form a tube can be chosen in many different ways. In addition, different tube radii can be selected. In ﬁg. 5.10

5.3 Thermodynamics of Solids

231

Fig. 5.10. Dispersion relations for several different carbon nanotube structures (adapted from Yu et al. (1995)).

we show the results of tight-binding calculations of the vibrational spectrum of several different nanotube variants. Part of the value in presenting these results is the reminder that calculations of quantities such as the vibrational spectrum of a material can be carried out in any of a number of different ways. Already in this chapter we have seen such dispersion relations computed using pair functionals (for Al), ﬁrst principles (for fcc Al and C60 ) and tight-binding analysis (the present case). Just as was possible with the analysis revealed of the displacement patterns in C60 , it is possible to examine the nature of the vibrations associated with nanotubes as well. An example of the various eigenvectors associated with a particular nanotube is shown in ﬁg. 5.11.

5.3 Thermodynamics of Solids 5.3.1 Harmonic Approximation As we saw above, what emerges from our detailed analysis of the vibrational spectrum of a solid can be neatly captured in terms of the vibrational density of states, ρ(ω). The point of this exercise will be seen more clearly shortly as we will observe that the thermodynamic functions such as the Helmholtz free energy can be written as integrals over the various allowed frequencies, appropriately weighted by the vibrational density of states. In chap. 3 it was noted that upon consideration of a single oscillator of natural frequency ω, the associated Helmholtz free energy is F=

h¯ ω ) ¯ + kT ln(1 − e−(hω/kT ). 2

(5.43)

232

5 Thermal and Elastic Properties of Crystals

Fig. 5.11. Illustration of a variety of different vibrational modes of one of the broad class of carbon nanotubes (adapted from Yu et al. (1995)).

In light of our observations from above, namely that the vibrational contribution to the energy of the crystal may be written as a sum of independent harmonic oscillators, this result for the Helmholtz free energy may be immediately generalized. In particular, we note that once the vibrational density of states has been determined

5.3 Thermodynamics of Solids

it is immediate that ∞ ∞ h¯ ω ) ¯ ρ(ω)dω + kT ρ(ω) ln(1 − e−(hω/kT )dω. F= 2 0 0

233

(5.44)

Note that all reference to the wavevector has been eliminated as a result of the fact that ρ(ω) is obtained by averaging over all wave vectors within the Brillouin zone, and is hence indifferent to the polarization and propagation vector of a given normal mode. In sections 5.22 and 5.24, we have made schematic evaluations of the nature of the vibrational spectrum (see ﬁg. 5.5). At this point, it is convenient to construct approximate model representations of the vibrational spectrum with the aim of gleaning some insight into how the vibrational free energy affects material properties such as the speciﬁc heat, the thermal expansion coefﬁcient and processes such as structural phase transformations. One useful tool for characterizing a distribution such as the vibrational density of states is through its moments, deﬁned by ∞ µn = ωn ρ(ω)dω. (5.45) 0

The most naive model we can imagine is to insist that whatever model we select for the density of states faithfully reproduces the ﬁrst moment of the exact vibrational density of states. That is, ∞ ∞ ωρexact (ω)dω = ωρmodel (ω)dω. (5.46) 0

0

We can guarantee this by following Einstein and asserting that all of the spectral weight is concentrated in a single vibrational frequency, ω E . That is, we approximate the full density of states with the replacement ρexact (ω) → ρ E (ω) = 3N δ(ω − ω E ). The partition function for the model presented above is given by 3N β hω ¯ E e− 2 Z= . ¯ E 1 − e−β hω

(5.47)

(5.48)

This may be seen by noting that the partition function may be written as a series of sums of the form

∞ ∞ 1 h¯ ωi . ··· exp −β ni + (5.49) Z= 2 n 3N i n =0 1

234

5 Thermal and Elastic Properties of Crystals

However, in the case of the Einstein model ωi = ω E for all ω and hence the sum indicated above may be rewritten as

∞ ∞ 1 1 h¯ ω E · · · h¯ ω E , (5.50) exp −β n 1 + exp −β n 3N + Z= 2 2 n =0 n =0 1

3N

which is equivalent to the product written in eqn (5.48). As noted already in chap. 3, once the partition function is in hand, we are in a position to evaluate properties of thermodynamic interest such as the average energy which is given by eqn (3.98) and in the present context may be written as U = −

3N h¯ ω E 3N h¯ ω E ∂ ln Z = + β hω . ∂β 2 e ¯ E −1

(5.51)

Recalling the deﬁnition of the speciﬁc heat as the temperature derivative of the average energy (see eqn (3.99)), it is found that for the Einstein solid C V = 3N k(β h¯ ω E )2

¯ E eβ hω . β hω (e ¯ E − 1)2

(5.52)

The average energy and the associated speciﬁc heat are plotted in ﬁg. 5.12. These are precisely the same results derived in our treatment of the statistical mechanics of a single oscillator in chap. 3, but now imbued with the extra insights that come from knowing how the vibrational frequencies emerge from microscopic analysis. This model represents one of the ﬁrst (if not the ﬁrst) examples of the use of reasoning based on quantum theory in order to deduce the properties of materials. One of the key features of this result is the fact that at high temperatures it reduces to the known high-temperature limit, C V = 3N k, while vanishing at low temperature (though not with the proper scaling with T as we shall see in our discussion of the Debye model). As yet, we have made a very crude approximation to the exact density of states. In particular, we have replaced the full vibrational density of states by a single delta function according to the prescription ρ(ω) = δ(ω − ωn ) → 3N δ(ω − ω E ). (5.53) n

We now consider a more quantitative model of the vibrational density of states which makes a remarkable linkage between continuum and discrete lattice descriptions. In particular, we undertake the Debye model in which the vibrational density of states is built in terms of an isotropic linear elastic reckoning of the phonon dispersions. Recall from above that in order to effect an accurate calculation of the true phonon dispersion relation, one must consider the dynamical matrix. Our approach here, on the other hand, is to produce a model representation of the phonon dispersions which is valid for long wavelengths and breaks down at

5.3 Thermodynamics of Solids

235

Fig. 5.12. Plots of the dimensionless average energy and speciﬁc heat resulting from the Einstein model. The average energy is scaled by 3N E E , where E E = h¯ ω E , while the speciﬁc heat is reported in units of 3N k. The temperature is also plotted in units of the Einstein temperature given by TE = h¯ ω E /k.

shorter wavelengths. One approach to this analysis is to linearize the dynamical matrix. An alternative route is to compute the linear elastic dispersion relation explicitly. In order to make this calculation it is well to recall the equations of linear elastodynamics, namely, Ci jkl u k,l j = ρ

∂ 2ui . ∂t 2

(5.54)

In the present setting ρ is the mass density while the subscript i identiﬁes a particular Cartesian component of the displacement ﬁeld. In this equation recall that Ci jkl is the elastic modulus tensor which in the case of an isotropic linear elastic solid is given by Ci jkl = λδi j δkl + µ(δik δ jl + δil δ jk ). Following our earlier footsteps from chap. 2 this leads in turn to the Navier equations (see eqn (2.55))

236

5 Thermal and Elastic Properties of Crystals

which it is to be remembered are given by (λ + µ)∇(∇ · u) + µ∇ 2 u = ρ

∂ 2u , ∂t 2

(5.55)

in the dynamical case. These equations admit of wave solutions of the form u i = u i0 ei(q·r−ωt) like those advanced in the treatment of vibrations in terms of the dynamical matrix. Substitution of this trial solution into the Navier equations yields their q-space analog, namely, [(λ + µ)qi q j + µq 2 δi j − ρω2 δi j ]u j0 = 0.

(5.56)

Once again, our problem of determining the wave solutions associated with our medium has been reduced to a problem of matrix diagonalization. The eigenvalues of the acoustic tensor or Christoffel tensor, Ai j = (λ + µ)qi q j + µq 2 δi j , are found to be µ q (5.57) ωT = ρ and

ωL =

λ + 2µ q, ρ

(5.58)

corresponding to transverse (ωT ) and longitudinal (ω L ) waves, in which the displacements are either perpendicular or parallel to the propagation direction, respectively. The solution associated with transverse waves is doubly degenerate in that there are two distinct solutions with this same eigenfrequency. The solution arrived at in our linear elastic model may be contrasted with those determined earlier in the lattice treatment of the same problem. In ﬁg. 5.13 the dispersion relation along an arbitrary direction in q-space is shown for our elastic model of vibrations. Note that as a result of the presumed isotropy of the medium, no q-directions are singled out and the dispersion relation is the same in every direction in q-space. Though our elastic model of the vibrations of solids is of more far reaching signiﬁcance, at present our main interest in it is as the basis for a deeper analysis of the speciﬁc heats of solids. From the standpoint of the contribution of the thermal vibrations to the speciﬁc heat, we now need to determine the density of states associated with this dispersion relation. As was noted earlier in the context of phonons, the density of states in q-space is constant, with one state per unit volume V /(2π )3 of q-space. That is, the set of allowed q-vectors form a lattice in q-space with each and every lattice point corresponding to a different allowed state. Our intention now is to recast this result in frequency space. We know that in a volume d 3 q of q-space there

5.3 Thermodynamics of Solids

237

Fig. 5.13. Dispersion relation obtained if solid is characterized by linear elastic constitutive model.

are V /(2π)3 d 3 q states. We now interest ourselves in the total number of states between two constant ω surfaces at ω and ω + dω. The total number of states in this shell is V dq⊥ d A, N= (5.59) (2π )3 where dq⊥ is the height of the volume element at a given position on the constant frequency surface being integrated over and d A is the area element on the constant frequency surface. The logic behind this equation is that we have asked how many states are in the shell of thickness dq⊥ . Now we note that the increment in frequency over that same height is given by dω = |∇q ω|dq⊥ , suggesting the alternative and more useful expression V dω ρ(ω)dω = , (5.60) d A (2π )3 |∇q ω| for the vibrational density of states. Use of this expression in the context of the dispersion relations obtained above yields 2 V ω2 1 (5.61) + 3 , ρ(ω) = 2π 2 c3L cT where we have introduced the elastic wave speeds, c L = dω L /dq and cT = dωT /dq. We are now in a position to make an evaluation of the speciﬁc heat within this model. Recall from earlier that the average energy of an oscillator of frequency ω

238

5 Thermal and Elastic Properties of Crystals

is given by U =

h¯ ω , ¯ −1 eβ hω

(5.62)

where we have dropped reference to the zero point energy for simplicity. For our collection of oscillators described by the vibrational density of states determined above, we have then ωD h¯ V 1 2 ω3 dω U = , (5.63) + ¯ −1 2π 2 c3L eβ hω cT3 0 where as yet all that remains undetermined is the upper cutoff frequency ω D , known as the Debye frequency. However, we know that the total number of modes of the system is 3N , where N is the number of atoms. As a result, we know that the density of states when integrated up to ω D must yield 3N . That is, ωD ρ(ω)dω = 3N . (5.64) 0

The reasoning invoked here is really no different than that associated with the Fermi level in electronic problems where we insisted that upon integrating the electronic density of states up to this level, the correct number of electrons was obtained (see eqn (4.88), for example). If we deﬁne the mean wave speed via 3 1 2 = 3 + 3, c¯3 cL cT

(5.65)

then the density of states may be rewritten as ρ(ω) = 3V ω2 /2π 2 c¯3 , which when substituted into the equation constraining the number of modes to 3N yields ω D = 1 2 c(6π ¯ N /V ) 3 . If we further deﬁne the Debye temperature θ D via h¯ ω D = kθ D , our expressions for the average energy may be differentiated to yield the speciﬁc heat which may itself be written in the considerably simpliﬁed form 3 θ D 4 u T T u e du . (5.66) Cv = 9k N u − 1)2 θD (e 0 The Debye result for the speciﬁc heat of a solid is of profound signiﬁcance in elucidating the key physical features that attend the thermal properties of solids. One key observation that is immediate is that in the limit when the temperature is low in comparison with the Debye temperature, we have θ D /T → ∞, which implies that the upper limit in the integral given in eqn (5.66) may be taken as inﬁnity. The consequence of this insight is that the low-temperature speciﬁc heat scales with the temperature as T 3 . This result emerges in light of the fact that the integral is a pure number which has no dependence on the temperature. In particular, we note the characteristic T 3 scaling that is compared with experimental

5.3 Thermodynamics of Solids

239

values in ﬁg. 5.1. In the other extreme, namely at very high temperatures, we note that the Debye result may be rearranged to recover the classical result C V = 3N k of Dulong and Petit. Physically, the success of the Debye model may be attributed to the fact that at low temperatures it is only the low-energy (or low-frequency) parts of the phonon spectrum which are excited. This part of the spectrum corresponds in part to the long-wavelength part of the spectrum which is precisely that part of the dispersion relation that is captured correctly by the Debye model. By way of contrast, the high-temperature result recovers the equipartition theorem and is predicated upon a correct assessment of the total number of modes to be shared. The Debye result then smoothly interpolates between these two limits. As a reminder of what we have accomplished and where it ﬁts into our broader program, we summarize the arguments of the chapter up until this point. We begin by noting that in the limit in which it is imagined that the excursions of atoms as they exercise thermal vibrations are sufﬁciently small, the potential energy of all solids reduces to a sophisticated model of coupled springs. This is a fascinating example of the type of effective theory construction that we have harped on repeatedly and note that in this case it is an especially intriguing conclusion since this result is indifferent to the type of bonding in the solid, whether it be metallic, covalent, ionic or something else. Once the energetics of the harmonic solid was in hand, we were then able to demonstrate that there exists a natural set of coordinates (i.e. normal coordinates) for characterizing the vibrations of a solid as a set of independent oscillators. Finally, as a result of our knowledge of the vibrational spectrum of a solid, the tools of statistical mechanics were invoked in order to determine the mean energy and speciﬁc heat, and as will be shown in the next chapter, these same arguments can be exploited to examine the vibrational entropy and to determine its role in the free energy balance separating competing different crystal structures. We now turn to an examination of some of the anharmonic effects in solids such as the thermal expansion and the thermal conductivity.

5.3.2 Beyond the Harmonic Approximation Thus far, our analysis has been entirely predicated upon the harmonic approximation advanced in eqn (5.2). On the other hand, real crystals are characterized by nonlinear force laws and the resulting anharmonic effects are part of the story from the outset. If we conﬁne our interest to the speciﬁc heat, we see that much may be made of the harmonic approximation. However, if we aim to press our modeling efforts further, for example, to consider the thermal expansion or the thermal conductivity, we will see that the harmonic approximation does not sufﬁce. Let us ﬂesh out the logic in the case of the coefﬁcient of thermal expansion. Our ﬁrst ambition will be to demonstrate that the harmonic approximation predicts

240

5 Thermal and Elastic Properties of Crystals

zero thermal expansion. This will be followed by an explicit incorporation of anharmonicity. We have seen that as a consequence of the harmonic Hamiltonian that has been set up thus far, our oscillators decouple and in cases which attempt to capture the transport of energy via heating, there is no mechanism whereby energy may be communicated from one mode to the other. This shortcoming of the model may be amended by including coupling between the modes, which as we will show below, arises naturally if we go beyond the harmonic approximation. The simplest route to visualizing the physics of this problem is to assume that our harmonic model is supplemented by anharmonic terms, such as αβγ i jk u iα u jβ u kγ + · · · . (5.67) H anh = iα

jβ

kγ

This result urges us to consider the nonlinear terms which must supplement the αβγ quadratic model set forth in eqn (5.2). The coefﬁcients i jk are deﬁned in analogy αβ with the K i j deﬁned in eqn (5.3) and are given by αβγ

i jk =

∂ 3 E tot . ∂ Riα ∂ R jβ ∂ Rkγ

(5.68)

There are certain subtleties associated with the order to which the expansion of eqn (5.67) is carried and for a discussion of which we refer the perspicacious reader to chap. 25 of Ashcroft and Mermin (1976). If we maintain the use of normal coordinates, but now including the anharmonic terms which are represented via these coordinates, it is seen that the various modes are no longer independent. For the purposes of the present discussion, we see that these anharmonic terms have the effect of insuring that the equation of motion for the n th mode is altered by coupling to the rest of the mode variables. This result bears formal resemblance to the Navier–Stokes equations which when written in terms of the Fourier variables yield a series of mode coupled equations. We have already noted that the physics of both thermal expansion and thermal conductivity demand the inclusion of these higher-order terms. Recall that the coefﬁcient of thermal expansion is deﬁned as 1 ∂P α= , (5.69) 3B ∂ T V where B is the bulk modulus, itself deﬁned as B = −V (∂ p/∂ V )T . We may evaluate the pressure, needed to compute the thermal expansion coefﬁcient, as p = −(∂ F/∂ V )T . Using the fact that the Helmholtz free energy is obtained as

5.3 Thermodynamics of Solids

a sum over all modes as h¯ ω(q, α) ¯ + kT ln(1 − e−β hω(q,α) ), F= 2 q,α q,α the pressure may be written in turn as h¯ −∂ω(q, α) −∂ω(q, α)

1 + . p= h¯ β hω(q,α) ¯ ∂V ∂V e −1 q,α 2 q,α

241

(5.70)

(5.71)

In both of these sums, we are summing over the wavevector q and the polarization α of the various phonons. What we have found is that all of the putative volume dependence of the free energy is tied to the vibrational frequencies themselves. Once we have determined p, then the thermal expansion coefﬁcient may be computed as

∂ω(q, α) ∂n(ω, T ) 1 , (5.72) −h¯ α= 3B q,α ∂V ∂T where we have deﬁned n(ω, T ) =

1 . )−1 ¯ e(hω/kT

(5.73)

Though we have determined the coefﬁcient of thermal expansion in principle, the entirety of our analysis is focused on how the vibrational frequencies are altered under a uniform dilatational strain. However, in the absence of some form of anharmonicity, this model is as yet plagued with a fatal ﬂaw; the vibrational frequencies within the harmonic approximation have no such volume dependence. At this point, our idea is to revisit the expansion of eqn (5.2) with the ambition of determining how an effective volume dependence to the phonon frequencies can be acquired. In particular, we return to the expansion given in eqn (5.2), but now adjusted to reﬂect the presence of a homogeneous strain. If we imagine that ref the equilibrium positions of the undeformed crystal are given by Ri , then in the presence of a state of deformation characterized by the deformation gradient F, ref these positions are amended to FRi . The thermal vibrations about these positions ref follow by expanding E tot ({FRi + ui }). Terms will now arise that couple the homogeneous strain to the thermal vibrations. In particular, if we keep terms only to second order in the expansion we have, ∂ E tot ref ref u iα E tot ({FRi + ui }) = E tot ({FRi }) + ∂ Ri,α F i,α 2 ∂ E tot 1 + u iα u jβ . (5.74) 2 i,α j,β ∂ Riα ∂ R jβ F

242

5 Thermal and Elastic Properties of Crystals

Note that the stiffness coefﬁcients are now evaluated at the strained reference state (as signiﬁed by the notation (∂ E tot /∂ Riα )F ) rather than for the state of zero strain considered in our earlier treatment of the harmonic approximation. To make further progress, we specialize the discussion to the case of a crystal subject to a homogeneous strain for which the deformation gradient is a multiple of the identity (i.e. strict volume change given by F = λI). We now reconsider the stiffness coefﬁcients, but with the aim of evaluating them about the zero strain reference state. For example, we may rewrite the ﬁrst-order term via Taylor expansion as 2 ∂ E tot ∂ E tot ∂ E tot = + λ. (5.75) ∂ Ri,α F ∂ Ri,α 0 ∂ Ri,α ∂λ 0 Note that when this expansion is reinserted into eqn (5.74), the ﬁrst term will clearly vanish on account of the equilibrium condition, namely, (∂ E tot /∂ Riα )0 = 0. Through use of the chain rule, we rewrite the term that is linear in λ as 2 ∂ 2 E tot ∂ E tot λ= λRkγ . (5.76) ∂ Riα ∂λ 0 ∂ Riα ∂ Rkγ 0 kγ Substituting this result back into the expansion for the total energy, it is noted that for crystals with centrosymmetry, this term will vanish because every term involving λRkγ will have a compensating partner −λRkγ . We now adopt precisely the same strategy, this time with respect to the terms in the total energy that are quadratic in the displacements. In particular, we have 2 2 ∂ E tot ∂ E tot ∂ 3 E tot = + λ. (5.77) ∂ Riα ∂ R jβ F ∂ Riα ∂ R jβ 0 ∂ Riα ∂ R jβ ∂λ 0 αβ

The ﬁrst term on the right hand side is recognized precisely as the matrix K i j introduced earlier. The term that is linear in λ may be evaluated via the chain rule as ∂ 3 E tot ∂ 3 E tot λRkγ . = (5.78) ∂ Riα ∂ R jβ ∂λ ∂ Riα ∂ R jβ ∂ Rkγ kγ As a result of these manipulations, eqn (5.74) may be rewritten as 1 αβ 1 αβγ ref E tot ({FRi + ui }) = K i j u iα u jβ + λRkγ u iα u jβ , 2 i,α j,β 2 iα jβ kγ i jk (5.79) where we have thrown away uninteresting constant terms. This result may be rewritten more provocatively as 1 αβ ref αβ (K + δ K i j )u iα u jβ , (5.80) E tot ({FRi + ui }) = 2 i,α j,β i j

5.3 Thermodynamics of Solids

where we have made the deﬁnition αβ

δ Ki j =

αβγ

i jk λRkγ .

243

(5.81)

kγ

The consequence of this analysis is that the original stiffness matrix has been amended by terms that are linear in the strain λ and that therefore adjust the vibrational frequencies under a volume change. In particular, the ‘renormalized’ frequencies arise as the eigenvalues of the stiffness matrix

K = K + δK.

(5.82)

We are now in a position to reconsider the vibrational frequencies in light of the imposition of a small homogeneous strain. Recall that our strategy was to use the quadratic potential energy to produce equations of motion. Inspection of the potential energy developed above makes it clear that the term that is quadratic in the displacements has acquired additional complexity. In particular, if we derive the equations of motion on the basis of both our earlier quadratic terms and those considered here, then we ﬁnd that they may be written as αβ αβ (K i j + δ K i j )u jβ . (5.83) m u¨ iα = − jβ

Because of the term δK, when we evaluate ∂ω(q, α)/∂ V , as demanded by eqn (5.72) in our deduction of the thermal expansion coefﬁcient, it will no longer vanish as it would if we were only to keep K. The phonon frequencies have acquired a volume dependence by virtue of the quasiharmonic approximation which amounts to a volume-dependent renormalization of the force constant matrix. There are a few lessons learned from this analysis. First, we note that as was claimed above, keeping only the harmonic terms in the expansion of the potential energy results in no volume dependence to the vibrational frequencies, and hence to no thermal expansion. This is seen because the parameter λ, which carries the information about such volume dependence, makes its ﬁrst appearance in αβγ conjunction with the manifestly anharmonic term, i jk . This insight prepares us for the quasiharmonic approximation in which the volume dependence of the vibrational frequencies appears in a way that masquerades as a harmonic term. We are now in a position to revisit the analysis of the thermal expansion presented earlier. In particular, we note that the thermal expansion coefﬁcient may now be evaluated by attributing a particular form to the volume dependence of the phonon frequencies. In order to reveal the application of the developments advanced above, we undertake an analysis of the thermal expansion in the

244

5 Thermal and Elastic Properties of Crystals

relatively sterile setting of a one-dimensional chain of atoms interacting through a near-neighbor pair potential model for the total energy. As usual, the elaborations of the model to either higher dimensions or other total energy methods do not involve any new questions of logic, though they may imply severe notational and computational demands. It is one of my largest regrets to have foregone a discussion of the thermal conductivity. Such a discussion would have been opportune at this point since it involves much of the same logic that we invoked in our discussion of the thermal expansion, though reworked along the lines of examining the way in which mode coupling leads to phonon scattering. The interested reader is referred to several of the books described in the Further Reading section at the end of the present chapter. 5.4 Modeling the Elastic Properties of Materials As was discussed in some detail in chap. 2, the notion of an elastic solid is a powerful idealization in which the action of the entirety of microscopic degrees of freedom are subsumed into but a few material parameters known as the elastic constants. Depending upon the material symmetry, the number of independent elastic constants can vary. For example, as is well known, a cubic crystal has three independent elastic moduli. For crystals with lower symmetry, the number of elastic constants is larger. The aim of the present section is ﬁrst to examine the physical origins of the elastic moduli and how they can be obtained on the basis of microscopic reasoning, and then to consider the nonlinear generalization of the ideas of linear elasticity for the consideration of nonlinear stored energy functions. 5.4.1 Linear Elastic Moduli If a crystal is subjected to small strain elastic deformation it is convenient to imagine the energetics of the strained solid in terms of the linear theory of elasticity. As we noted in chap. 2, the stored strain energy may be captured via the elastic strain energy density which in this context is a strictly local quantity of the form 1 (5.84) W () = Ci jkl i j kl . 2 As usual, we are employing the summation convention which demands that we sum over all repeated indices. This relation is posited to apply pointwise, meaning that even if the state of deformation is spatially varying, the energy stored in the body by virtue of elastic deformation is obtained by adding up the energy of each volume element as though it had suffered homogeneous deformation. Despite our

5.4 Modeling the Elastic Properties of Materials

245

replacement of the entirety of the set of atomistic degrees of freedom with an effective description in terms of elastic strains, we may restore contact with the microscopic degrees of freedom via the elastic moduli in a way that will be made evident below. For our present purposes, we note that the correspondence of interest is given by 1 1 def undef Ci jkl i j kl = [E tot ({Ri }) − E tot ({Ri })]. (5.85) 2 The logic embodied in this expression is built around the recognition that from the continuum perspective the elastic strain energy density is the energy per unit volume above and beyond that of the perfect crystal and is given by the left hand side of eqn (5.85). The microscopic evaluation of this same quantity is def obtained by computing the energy of the deformed state (i.e. E tot ({Ri })) and subtracting off the energy of the perfect crystal which we have referred to as undef E tot ({Ri }), and then appropriately normalizing that energy with a volume factor so as to produce an energy density. To make the connection given in def eqn (5.85) computationally useful, we expand the total energy E tot ({Ri }) about the unstrained reference state, keeping terms only to second order in the strains. In particular, we write def

undef

E tot ({Ri }) ≈ E tot ({Ri

}) +

∂ E tot ∂i j

i j + ref

2 1 ∂ E tot i j kl . 2 ∂i j ∂kl ref

(5.86)

On the recognition that the expansion is about the reference state and hence that the linear term in the expansion vanishes (i.e. (∂ E tot /∂i j )ref = 0), eqn (5.85) reduces to 1 ∂ 2 E tot 1 Ci jkl i j kl = i j kl , 2 2 ∂i j ∂kl

(5.87)

where as usual we sum over all repeated indices, which illustrates that the elastic moduli are obtained as Ci jkl =

1 ∂ 2 E tot . ∂i j ∂kl

(5.88)

It is worth noting that this expression is generic as a means of extracting the elastic moduli from microscopic calculations. We have not, as yet, specialized to any particular choice of microscopic energy functional. The physical interpretation of this result is recalled in ﬁg. 5.2. The basic observations may be summarized as follows. First, we note that the actual energy landscape is nonlinear. One next adopts the view that even in the presence of ﬁnite deformations, there is a

246

5 Thermal and Elastic Properties of Crystals

strain energy density of the form W (F) which is a function of the macroscopic deformation gradient. In the neighborhoods of the minima of this nonconvex energy surface, it is convenient to parameterize the potential as a series of parabolic wells, the curvatures of which may be identiﬁed with the elastic moduli as we have done in eqn (5.88). In light of these gains we are now in a position to explicitly determine the elastic properties. As a ﬁrst step in this direction we exploit a pair potential description of the total energy. As promised in chap. 4, it will emerge shortly that such a description has serious shortcomings as concerns the elastic properties of materials. On the other hand, the pair potential picture has the salutary effect of demonstrating just how the atomic-level interactions manifest themselves in macroscopic observables such as the elastic moduli. Once we have seen just how these ideas emerge, the way will be paved for a more quantitative analysis of elasticity using more sophisticated total energy functionals. Within the pair potential setting where the total energy is given by E tot = 1 mn Veff (r mn ), the elastic moduli are given by 2 Ci jkl =

1 ∂ ∂ Veff (rmn ). 2 ∂i j ∂kl mn

(5.89)

Through judicious use of the chain rule, we end up with the generic expression

1 ∂rmn ∂rmn ∂ 2rmn + V (rmn ) V (rmn ) . (5.90) Ci jkl = 2 mn ∂i j ∂kl ∂i j ∂kl In this case, rmn refers to the distance between the m th and n th atoms in the deformed state in which the crystal is subjected to some homogeneous strain. If we assume that the deformed and reference positions are related by ri = FRi , then ri j may be rewritten as (5.91) ri j = Ri j · Ri j + 2Ri j · E · Ri j , where we have used the fact that the deformation gradient F and the Lagrangian strain tensor E are related by E = 12 (FT F − I) as shown in eqn (2.6), and we have used the deﬁnition Ri j = Ri − R j . In the limit of small displacement gradients we may replace E with in eqn (5.91). As a result of these geometric insights, the geometric derivatives written above may be evaluated with the result that

(Rm ) Rmi Rmj Rmk Rml Veff 1 Veff (Rm ) − . (5.92) Ci jkl = 2at m Rm Rm2 We have added another layer of notation in the form of the quantity at which is the volume per atom associated with the crystal of interest as well as the quantities Rmi , which refer to the i th Cartesian component of the position vector of the m th atom,

5.4 Modeling the Elastic Properties of Materials

247

with the sum over m referring to the various neighbors that the atom at the origin is coupled to via the potential Veff (Rm ). The notation is admittedly unpleasant, but I am too entrenched in the habit of writing Ci jkl rather than the more consistent Cαβγ δ , where Greek indices are associated with Cartesian components. The result obtained in eqn (5.92) is of interest for a number of reasons including what it has to teach us about the energetics associated with pair potentials. For concreteness, we consider the case of an fcc crystal and specialize to the case of a near-neighbor pair potential for which Veff (Rm ) = 0 as a result of the equilibrium condition. We are interested in obtaining the three cubic elastic moduli, C11 , C12 and C44 . Note that all neighbors of a given atom are characterized by position vectors of the form R = (a0 /2)(110). If we are to√assess the sums called for in eqn (5.92), what emerges is that C11 = 2Veff (a0 / 2)/a0 and C12 = C44 = C11 /2, a result which is generally at odds with experimental ﬁndings. In fairness to our pair potential calculations, our results could have been improved by the inclusion of terms in the energy which are explicitly volume-dependent and structure-independent such as the electron gas terms described in chap. 3 (see eqn (3.64)). In addition, our reason for introducing this calculation was not so much to criticize pair potentials as to illustrate the conceptual ideas associated with a real calculation of the elastic moduli. An alternative to the analytic approach adopted above is to take a computational strategy in which the energies of the various deformed states in the neighborhood of the reference state are computed explicitly using whatever total energy method is under consideration. The set of total energies obtained in this way is then ﬁt as a quadratic function of the relevant strain measure, with the elastic modulus of interest (or some linear combination of the moduli) being related to the curvature of this function about the minimum. For example, as shown in ﬁg. 5.14, one can carry out a series of calculations of the energy of a crystal as a function of the volume. As long as the departures from the equilibrium volume are sufﬁciently small, the energy can be written in the form 1 E tot = α(V − V0 )2 , 2

(5.93)

where α is a stiffness parameter related to the bulk modulus and V0 is the equilibrium volume. Similar results are obtained for other types of deformation (for example, shearing deformations) resulting in the possibilty of obtaining a complete set of linear elastic moduli directly on the basis of microscopic calculations. Note also that in describing this strategy we have not made any particular choice about the nature of the underlying microscopic energy functional. Indeed, this strategy is robust and can be carried out with methods ranging all the way from pair potentials to ﬁrst-principles techniques.

248

5 Thermal and Elastic Properties of Crystals

Fig. 5.14. Energy as a function of volumetric strain as computed using atomic-scale analysis in terms of embedded-atom potentials (courtesy of D. Pawaskar). The atomistic result is compared with the quadratic ﬁt like that suggested in eqn (5.93).

5.4.2 Nonlinear Elastic Material Response: Cauchy–Born Elasticity As yet, our reﬂections on the elastic properties of solids have ventured only so far as the small-strain regime. On the other hand, one of the powerful inheritances of our use of microscopic methods for computing the total energy is the ease with which we may compute the energetics of states of arbitrarily large homogeneous deformations. Indeed, this was already hinted at in ﬁg. 4.1. As one of our central missions is to uncover the relation between microscopic and continuum perspectives, it is of interest to further examine the correspondence between kinematic notions such as the deformation gradient and conventional ideas from crystallography. One useful point of contact between these two sets of ideas is provided by the Cauchy–Born rule. The idea here is that the rearrangement of a crystalline material by virtue of some deformation mapping may be interpreted via its effect on the Bravais lattice vectors themselves. In particular, the Cauchy–Born rule asserts that if the Bravais lattice vectors before deformation are denoted by Ei , then the deformed Bravais lattice vectors are determined by ei = FEi . As will become evident below, this rule can be used as the basis for determining the stored energy function W (F) associated with nonlinear deformations F. The Cauchy–Born strategy yields interesting insights in a number of contexts one of which is in the kinematic description of structural transformations. A

5.4 Modeling the Elastic Properties of Materials

249

Fig. 5.15. Schematic of the assumption inherent in the Cauchy–Born rule which assumes that the crystal lattice may be thought of as locally having suffered an afﬁne deformation (courtesy of K. Bhattacharya).

schematic of the fundamental geometric idea associated with the Cauchy–Born rule is shown in ﬁg. 5.15 in which it is seen that even though the overall state of deformation may be spatially varying, it is possible to advance the assumption of a deformation that is locally afﬁne. As seen in the ﬁgure, despite the fact that the overall body has been subjected to an inhomogeneous deformation, locally, the crystal behaves as though it is of inﬁnite extent and has been subjected to homogeneous deformation. From the standpoint of the microscopic total energy methods presented in the previous chapter, the Cauchy–Born rule may be used to compute the stored energy function W (F). Indeed, we have already shown two different examples of this thinking in ﬁgs. 2.14 and 4.1. The key message of both of these ﬁgures is not only the nonlinearity of the energy landscape once the displacements become too large, but even further, its nonconvexity. The idea invoked in carrying out such calculations is that we can evaluate the energy of a given conﬁguration, characterized by Bravais lattice vectors ei = FEi as W ({ei }), via W ({ei }) =

E tot ({ei }) − E tot ({Ei }) .

(5.94)

In a word, the problem is reduced to one of computing the energy of two different homogeneous conﬁgurations, and as usual, the concept is indifferent to choice of underlying microscopic energy functional. A particularly important example of this strategy concerns the energetics of shearing deformations. In particular, as shown in ﬁg. 2.14, the energetics of shearing deformations immediately reveals the presence of lattice invariant shears. Further, the presence of zero-energy wells corresponding to speciﬁc values of the shear is precisely the physics that gives rise to the existence of dislocations. We will later see (see section 10.3) that similar ideas are relevant to the emergence of microstructures in systems having multiple degenerate energy wells. It is also important to note that a strain energy density

250

5 Thermal and Elastic Properties of Crystals

function like that given in eqn (5.94) can be used as the basis of a hyperelastic constitutive model which permits the calculation of stresses via P=

∂ W (F) . ∂F

(5.95)

Further details of this idea can be found in Tadmor et al. (1996).

5.5 Further Reading Introduction to Lattice Dynamics by M. Dove, Cambridge University Press, Cambridge: England, 1993. I really like Dove’s book. Unlike the present work, it has the virtue of being short and to the point. The discussion of anharmonic effects is instructive. ‘Group Theory and Normal Modes’ by A. Nussbaum, Am. J. Phys., 36, 529 (1968) provides an interesting tutorial introduction to the use of symmetry to reduce the computational overhead associated with a given calculation of the normal modes. Theory of Lattice Dynamics in the Harmonic Approximation by A. A. Maradudin, E. W. Montroll, G. H. Weiss and I. P. Ipatova, Academic Press, New York: New York, 1971. A formidable volume with not only a full accounting for the fundamentals of vibrations in solids, but also including issues such as the effects of defects on vibrations in solids. Imaging Phonons: Acoustic Wave Propagation in Solids by James P. Wolfe, Cambridge University Press, Cambridge: England, 1998. Wolfe’s book has a number of different insights into the concepts discussed in the present chapter as well as a wealth of material which goes well beyond the present discussion. Thermodynamics of Crystals by D. C. Wallace, Dover Publications, Inc., Mineola: New York, 1998. Wallace’s chaps. 2–4 give a thorough discussion of the material that has been sketched in the present chapter. Thermal Conduction in Solids by R. Berman, Clarendon Press, Oxford: England, 1976. A useful compendium of insights into the problem of thermal conduction. ‘Thermal Conductivity and Lattice Vibrational Modes’ by P. G. Klemens, in Solid State Physics edited by F. Seitz and D. Turnbull, Academic Press, San Diego: California, Vol. 7, pg. 1, 1958. I ﬁnd the sections on scattering due to defects in this article to be quite useful. ‘Theory of Thermal Conductivity of Solids at Low Temperatures’ by P.Carruthers, Rev. Mod. Phys., 33, 92 (1961). This article is probably severely dated, but I still ﬁnd it to be instructive reading.

5.6 Problems

251

5.6 Problems

1 Normal Modes for Chain with Three Masses Consider a three-mass generalization of the system shown in ﬁg. 5.3. Compute the vibrational frequencies and associated eigenvectors on the assumption that each mass has only one degree of freedom, namely, motions along the line joining the masses. Assume that the masses are all identical as are the spring constants.

2 Properties of the Force Constants and the Dynamical Matrix In this problem, we revisit the formalism associated with the force constants and the dynamical matrix. Recall that the force on the i th atom in the α th direction is given by αβ K i j u jβ , (5.96) Fiα = − jβ

where u jβ denotes the displacement of the j th atom in the β th Cartesian direction. Using this expression for the force, show that if all atoms are displaced by the same constant vector, that this implies the sum rule αβ K i j = 0. (5.97) j

3 Phonons in Morse Potential Cu Obtain an analytic expression for the zone edge phonons in fcc Cu using the Morse potential derived in the previous chapter. To do so, begin by deriving eqn (5.37) and then carry out the appropriate lattice sums explicitly for the Morse potential to obtain the force constant matrix. In addition, obtain a numerical solution for the phonon dispersion relation along the (100) direction. 4 Phonons using the Pair Functional Formalism Generalize the discussion given in this chapter based on pair potentials in order to deduce the force constant matrix for a total energy based on pair functionals. The result of this analysis can be found in Finnis and Sinclair (1984). Having obtained this expression for the force constant matrix, use the Johnson potential presented in the previous chapter and compute the phonon

252

5 Thermal and Elastic Properties of Crystals

dispersion relations in Cu. In addition, compute the phonon density of states for Cu and compare the resulting structure of this function to the parabolic shape expected on the basis of the Debye model. 5 Elaboration of the Debye Model In this problem, deduce the eigenvalues of the Christoffel tensor and also recreate the vibrational density of states for the Debye model given in eqn (5.61). In light of these results, ﬁll in the various steps culminating in eqn (5.66). 6 Elastic Moduli for fcc Cu from Morse Potential Using the Morse pair potential for Cu derived in the problems of the previous chapter, derive C11 , C12 and C44 . Carry out this analysis both analytically and numerically. For the numerical results, you will need to compute the energetics of three independent deformations and then to ﬁt the resulting energy curves to obtain these moduli. 7 Expression for Elastic Moduli of Cubic Crystals from Pair Functionals Using the generic deﬁnition of the total energy as deﬁned within the pair functional formalism, derive an expression for the elastic moduli. Once this result is in hand, use the explicit expressions associated with the Johnson potential to obtain the elastic moduli for Cu. 8 Cauchy–Born Elasticity Using the Cauchy–Born rule in conjunction with the Johnson embedded-atom potential, compute the energy of a shearing deformation on (111) planes in the [110] direction. Show that the energy has the form given in ﬁg. 2.14.

SIX

Structural Energies and Phase Diagrams

6.1 Structures in Solids A central tenet of materials science is the intimate relation between structure and properties, an idea that has been elevated to what one might call the structure–properties paradigm. However, we must proceed with caution, even on this seemingly innocent point, since materials exhibit geometrical structures on many different scales. As a result, when making reference to the connection between structure and properties, we must ask ourselves: structure at what scale? This chapter is the ﬁrst in a long series that will culminate in a discussion of microstructure, in which we will confront the various geometric structures found in solids. The bottom rung in the ladder of structures that make up this hierarchy is that of the atomic-scale geometry of the perfect crystal. It is geometry at this scale that concerns us in the present chapter. In crystalline solids, the atomic-scale geometry is tied to the regular arrangements of atoms and is described in terms of the Bravais lattice. At this scale, the modeling of structure refers to our ability to appropriately decipher the phase diagram of a particular material. What is the equilibrium crystal structure? What happens to the stable phase as a function of an applied stress, changes in temperature or changes in composition? And a more subtle question, what are the favored metastable arrangements that can be reached by the system? At the next level of description, there are a host of issues related still to the atomic-level geometry, but now as concerns the various defects that disturb the perfect crystal. For example, as we raise the temperature, what will be the distribution of vacancies within a crystal, and what governs the dislocation structures that are revealed in electron microscopy images? These defects will occupy much of our attention in coming chapters. At larger scales yet, an investigation of the relation between structure and properties must by necessity also acknowledge structure at the scale of the microstructure itself. Here, it is evident that we are faced again with questions 253

254

6 Structural Energies and Phase Diagrams

related to metastability and that our theory must answer to these demands. Our ﬁrst step towards answering these questions will show how microscopic analysis can yield meaningful insights into the nature of atomic-level geometry.

6.2 Atomic-Level Geometry in Materials As noted above and hinted at in the sections on microscopic approaches to the total energy, the ability to correctly capture the energetics of competing crystal structures and their various defects is a central mission faced in the modeling of materials. Before embarking on an analysis of the structure and energetics of the many defects that populate solids and lend them their fascinating properties, we must ﬁrst ensure our ability to differentiate the various competing crystal structures found in the elements and their compounds that serve as the backbone of materials science. Casual inspection of the periodic table reveals that already at the level of elemental materials, a whole range of atomic-level structures may occur. The room temperature structures of elemental materials are summarized in ﬁg. 6.1. A fascinating resource concerning the structure of the elements is Young’s Phase Diagrams of the Elements (1991), a book that rewards its reader with insights into the startling complexity found in crystalline solids, even without the complicating inﬂuence of the compositional degrees of freedom that are present in compounds. Fig. 6.1 reveals a number of important and intriguing structural trends, all of which serve as a challenge to our analysis. For example, it is seen that a wide assortment of elements adopt the close-packed fcc and hcp structures. In particular, the rare-gas solids (aside from He) all adopt the fcc structure. We also note that the transition metals (i.e. the rows running from Sc to Cu, Y to Ag and La to Au) adopt a nearly regular progression starting with the hcp structure, passing to the bcc structure at the middle of the transition series and ending with the fcc structure at the noble metals (Cu, Ag, Au). These structural trends can be traced in turn to the ﬁlling of the transition metal d-band as the number of d-electrons per atom increases as the transition series is traversed from left to right. The bcc structure also plays a crucial role in the description of elemental materials, with the most regular trend being the occurrence of this structure in the alkali metals such as Li, Na and their partners in the same column of the periodic table. Covalent materials, such as Si and Ge, are also cubic but take on the much more open diamond structure. A more exotic cubic structure is adopted by elemental Mn which is built up of 58 atoms. In this case, it is the complicating effects of magnetism that can be blamed for the structural complexity. In addition to the high-symmetry cubic phases, there are a collection of bad actors which adopt structures of much lower symmetry. For example, the group

6.2 Atomic-Level Geometry in Materials

255

Fig. 6.1. Periodic table with identiﬁcation of the crystal structures adopted by the various elements (adapted from McMahon and Graham (1992)).

V elements (N, P, As, Sb and Bi) adopt several orthorhombic and rhombohedral phases. Additional structural complexity is ushered in as a result of the fact that in certain cases, the basic building blocks are no longer individual atoms, but rather molecules. The most stunning example of this effect is revealed in S which has a room temperature orthorhombic crystal structure built up of 16 S8 molecules in each unit cell. To drive home the complexity revealed at the structural level even in the case of elemental materials, ﬁg. 6.2 shows the temperature–pressure phase diagrams of a few representative elements. There are a few trends to be remarked. First, we note that for several of the close-packed metals that at high temperatures they undergo a transformation to the bcc structure, as seen in the ﬁgure for the representative example of Ti, and as is true in addition for Zr and Hf. A more complex situation featuring a series of cubic structures is that of Mn which undergoes a number of different structural transformations with increasing temperature. Oxygen is also characterized by a phase diagram of remarkable complexity, in this case with the fundamental structural building blocks being O2 molecules. In addition to the role of the temperature as a control parameter which serves to tune the relative stability of competing phases, the application of a hydrostatic stress can also induce structural change. This claim is substantiated in the particular case of Si shown in ﬁg. 6.2 which undergoes a transition from the diamond cubic to the centered

256

6 Structural Energies and Phase Diagrams

Fig. 6.2. Pressure–temperature phase diagrams of a few representative elements (adapted from Young (1991)).

tetragonal β-Sn phase at a pressure of roughly 11.3 GPa, and more generically in ﬁg. 6.3. Indeed, an important open question is how such phase diagrams will generalize when the material is subjected to more general states of stress. In the case of a material like sulfur (see ﬁg. 1.4), we have already seen that the equilibrium structure is a delicate function of the particular region of parameter space under consideration. From the standpoint of equilibrium thermodynamics, despite the unarguable complexity of the phase diagrams described above, we must conclude that these various structures are nothing more than different realizations of the minima in the appropriate free energy. Our present challenge is to see if

6.2 Atomic-Level Geometry in Materials

257

Fig. 6.3. Dependence of the equilibrium structure on the pressure for several representative transition metals (adapted from Young (1991)).

we can learn what competing features give rise to the stability of the different competitors. Beyond the simple elemental structures considered above, we are faced with the more serious task of deducing the structures that arise once we allow for more than a single element and the attendant chemical complexity. Here again, the challenges to the materials modeler are seemingly limitless. To reveal this complexity, we consider a few representative binary systems as shown in ﬁg. 6.4. For intermetallics, the Cu–Au system may be the most celebrated of all examples. In this case, one of the key qualitative features to note is the existence of both low-temperature ordered phases and a high-temperature disordered phase. The low-temperature ordered phases are particularly appealing from a modeling perspective since they can all be thought of as superstructures on the fcc lattice which are built up as different decorations of the fcc lattice on the basis of the various Cu and Au atoms. A second example of an intermetallic phase diagram is that of the TiAl intermetallic system shown in ﬁg. 6.4(b), a material that has been the subject of intense interest in recent years. In addition to the α (hcp) and β (bcc) solid solutions, we note the presence of the ordered Ti3 Al hexagonal phase, the TiAl L10 phase and the ordered fcc TiAl2 phase. Phase diagrams associated with systems other than intermetallics are also of interest. Our third example, shown in ﬁg. 6.4(c), the Si–Ge system, is interesting primarily for what it is not. In particular, we note the marked lack of complexity

258

6 Structural Energies and Phase Diagrams

(Au,Cu)

1800 1700 1600 1500 1400 ( -Ti) 1300 1200 1100 1000 Ti3Al 900 800 ( -Ti) 700 600 500

(a)

20

30

40

50

60 70 80 90100

0

10

2100

(Al) TiAl2

-TiAl3

20

2046.5+ 7.5˚C

30

40 ~60

L1 + L2

2054˚C M.P.

Temperature ˚C

Temperature ˚C

2300

1414˚C

1400

TiAl3

Weight Percent Oxygen

Weight Percent Silicon 10

TiAl

0 10 20 30 40 50 60 70 80 90 100 Al Ti Atomic Percent Aluminum (b)

Atomic Percent Copper 0

L

LPS

Temperature ˚C

Temperature ˚C

Weight Percent Copper

1300

1200

1100

1000

+0.5 59.5_

1900 1700 1500

Al2O3

1300

L1+ Al2O3

1100 900 660.452 C 0, the jump in the displacement ﬁeld be equal to the Burgers vector (i.e. u 3 (x1 , 0+ ) − u 3 (x1 , 0− ) = b). Our notation u 3 (x1 , 0+ ) means that the ﬁeld u 3 is to be evaluated just above the slip plane (i.e. x2 = ). This geometry of this problem inspires a description in terms of cylindrical coordinates, within which a plausible form for the displacements is the assumption that, like a helical ramp in a parking garage, the displacements increase linearly in the winding angle, θ, yielding the solution bθ . (8.10) 2π This displacement ﬁeld may also be represented simply in terms of Cartesian coordinates, resulting in the expression b −1 x 2 , (8.11) tan u 3 (x1 , x2 ) = 2π x1 u 3 (r, θ, z) =

and the associated strains b x2 , 2 4π x1 + x22 x1 b 32 (x1 , x2 ) = . 4π x12 + x22

31 (x1 , x2 ) = −

The stress tensor corresponding to these strains may be written as 0 0 −x2 µb 0 σ = 0 x1 . 2π(x12 + x22 ) −x2 x1 0

(8.12) (8.13)

(8.14)

384

8 Line Defects in Solids

Note that care must be taken with the choice of sign of the Burgers vector to actually use these equations in practice. The signiﬁcance of the results given above may be seen in a number of different contexts. Indeed, the solution for the perfect screw dislocation in an isotropic linear elastic medium provides a window on much of what we will wish to know even in the more generic setting of an arbitrary curved dislocation. Further, this simple result also serves as the basis for our realization that all is not well with the continuum solution. One insight that emerges immediately from our consideration of the screw dislocation is the nature of the energies associated with dislocations. Cursory inspection of the dislocation solution determined above reveals that the strain ﬁelds are singular as the dislocation core region is approached; a feature that highlights the ultimate need for calculations that respect the discrete lattice scale, either through explicit resolution of the atomic degrees of freedom or through use of suitable constitutive and kinematic nonlinearity within a continuum framework. If we are willing to suspend momentarily the question of the behavior in the nearcore region, it is of great interest to determine that part of the total energy of a dislocation that arises by virtue of the elastic energy stored in its deformation ﬁelds. The simplest statement of the energy associated with a dislocation by virtue of its deformation ﬁelds is to integrate the strain energy density over the volume. Recall that for a linear elastic solid, the strain energy density may be written as 1 W () = Ci jkl i j kl . 2

(8.15)

Alternatively, if we assume that there are no body forces, then the divergence theorem in conjunction with the equilibrium equations asserts 1 1 tk u k d A. (8.16) Ci jkl i j kl = 2 ∂ 2 Hence, we ﬁnd that the total elastic energy can be found by performing surface integrations associated with the tractions. It is this device that we will follow here. Though in principle we must evaluate the surface integral not only on the slipped surface, but also on both an outer and an inner circular surface, the only surface that must be considered in ∂ is that of the cut along the slip plane as shown in ﬁg. 8.17. In fact, it can be shown that the contribution on both the outer and inner surfaces vanish. In terms of the coordinate system speciﬁed above, we are left with the necessity of evaluating the traction vector ti = σi2 n 2 , which yields t3 = σ32 . From our assessment of the displacement ﬁelds, we note that the relevant component of the stress tensor is given as σ32 = µu 3,2 =

µb x1 . 2π x12 + x22

(8.17)

8.4 Elastic Models of Single Dislocations

385

Fig. 8.17. Schematic of slip plane as used within a continuum setting.

In light of this result, we are prepared to evaluate the strain energy which is obtained by integrating R µb2 1 L , (8.18) dz dx E =2 2 0 4π x r0 where we have exploited the fact that along the slip plane, x2 = 0. The factor of 2 in front of the integral reﬂects the presence of both symmetry equivalent terms, σ32 and σ23 . The limits of integration for the integral along the line direction make it clear that we are reckoning the energy per unit length of dislocation, while the x-integral reﬂects the existence of a large distance cutoff corresponding to the dimensions of the body and a lower scale cutoff, corresponding loosely with the scale at which elasticity theory breaks down. The result of this analysis is that the energy per unit length along the dislocation line is R µb2 ln E= . (8.19) 4π r0 This result is at once enlightening and troubling. On the one hand, on the basis of relatively little effort we have constructed an evaluation of the elastic energy associated with a screw dislocation, and while our analysis depended upon the simplicity of the screw dislocation solution, we will ﬁnd that the qualitative features of our result are unchanged by the introduction of subtleties such as mixed character to the dislocation’s Burgers vector and elastic anisotropy. On the other hand, to avoid a divergence in the energy we have been forced to introduce a phenomenological parameter r0 known as the core radius, which can only be guessed at within the conﬁnes of our continuum model. Further, we note that our result for the energy is logarithmically divergent not only for the short-range part of the ﬁelds, but for the long-range parts as well. Clearly, there is more to be discovered. An interesting estimate of the signiﬁcance of the core parameter can be constructed by harking back to our discussion of the ideal strength concept. There, we noted that when shear stresses reach a value on the order of µ/2π, the forces

386

8 Line Defects in Solids

Fig. 8.18. Model of stresses in core region of dislocation based upon the ideal shear strength. The elastically diverging stresses are cutoff for r < rc on the assumption that the stresses within the core region have a constant value τideal .

are sufﬁciently high to begin the shearing of adjacent crystal planes. Hence, we take the view here that the core radius may be deﬁned as that region over which the stresses have reached values consonant with the ideal strength. One estimate of the core radius is to take that distance along the x-axis at which the shear stress reaches the ideal strength, which yields r0 = b. As noted above, it is standard to idealize the core as a cylindrical region, although the locus of points of constant shear stress is certainly not circular as such a model would suppose. This simple model of the core radius can be exploited to make an estimate for the energy associated with the core itself. The basic idea is to make the pessimistic assumption that within the region of radius r0 , the stresses are constant at the level of the ideal shear strength. This situation is depicted schematically in ﬁg. 8.18. Our estimate of the core energy amounts to nothing more than computing the strain energy stored in this region on the assumption of a constant state of strain corresponding to that at the ideal strength limit. In particular, we note that the only terms appearing in the assessment of the strain energy density are of the form σ31 31 and σ32 32 . The total strain energy within the core region is given as 1 (8.20) E core = (σ31 31 + σ32 32 )(πr02 )L , 2 where the last two factors are geometric and characterize the cylindrical volume element under consideration. We note that for the special case of the screw dislocation, σ31 31 + σ32 32 = µb2 /8π 2r02 , with the result that E core = µb2 L/8π .

8.4 Elastic Models of Single Dislocations

387

Hence, within this simple model, the energy of the dislocation per unit length may be written as 1 R µb2 E disloc ln + . (8.21) = L 4π r0 2 For concreteness, it is of interest to examine the typical energy scale associated with a straight dislocation line. Consider a hypothetical material for which the ˚ and take as our outer cutoff and shear modulus is 50 GPa, the Burgers vector is 3 A ˚ inner cutoff radii, 1 µm and 3 A respectively. In this case, we see that the energy associated with each segment with a length comparable to the lattice spacing is of order 6 eV. Though our analysis can be reﬁned in a number of ways, there is no escaping the fact that the energy scale here is huge on the scale of that associated with room temperature. As a result, we are momentarily left to wonder whether dislocations can arise purely by virtue of thermal ﬂuctuations. We have still not exhausted the insights that can be gleaned from this simplest of dislocation models. Before taking up the question of the displacement ﬁelds associated with a generic dislocation loop, we ﬁrst examine the question of whether or not it is plausible that entropic effects can compensate for the huge energy associated with the dislocation, thereby raising the possibility of the existence of an equilibrium distribution of such defects. There are a few different entropic mechanisms that can be imagined as a consequence of the presence of dislocations. On the one hand, it is clear that the presence of such dislocations will alter the vibrational spectrum of the material with an attendant change in its vibrational entropy. Another contribution to the entropy is that due to the wandering of the dislocation line itself and corresponds to a conﬁgurational term. A crude estimate of this latter effect is to assume that on passing from one atomic layer to the next, the dislocation can change directions towards any of the neighboring atoms. Hence, the entropy per layer spacing is of the order S = k ln z,

(8.22)

where z represents the number of neighbors along the line direction and we will make the simplifying assumption that ln z ≈ 1. Hence, the contribution of conﬁgurational terms to the free energy of a dislocation is of order T S = kT , which is negligible in comparison with the enormous internal energy cost of the dislocation line itself. Our initial foray into the elastic theory of dislocations has revealed much about both the structure and energetics of dislocations. From the continuum standpoint, the determination of the displacement ﬁelds (in this case u 3 ) is equivalent to solving for the ‘structure’ of the dislocation. We have determined a generic feature of such ﬁelds, namely, the presence of long-range strains that decay as r −1 . Another

388

8 Line Defects in Solids

generic feature of the elastic solution is the fact that in the immediate vicinity of the dislocation core, the elastic theory breaks down. It has also become evident from our analysis that unlike point defects, dislocations have energies well above those for which an equilibrium distribution can be expected.

8.4.2 The Volterra Formula As yet, our treatment of the elastic theory of single dislocations has depended upon the simplicity of the equilibrium equations that emerge for the particular geometry of a straight screw dislocation. While further progress can be made for specialized geometries, it is perhaps more instructive to seek generic insights into the deformation ﬁelds that attend the presence of dislocations of arbitrary geometry. In particular, we will concern ourselves with a closed dislocation loop. One approach for the elastic analysis of dislocations that is especially appealing is built around the use of the elastic Green function. As is customary, we will initially restrict our analysis to isotropic materials, though extension to an anisotropic setting, while not trivial, can be managed, at least formally. The aim of our elastic analysis will be a full characterization of the elastic ﬁelds (i.e. stresses, strains and displacements) associated with the dislocation of interest, as well as a description of its energy. Though the elastic ﬁelds are of interest in their own right, we will see in section 8.5 that it is the coupling of these ﬁelds, either to applied stresses or to internal stresses due to other defects, that makes for the beginnings of a picture of the origins of phenomena such as strain and solution hardening. The reciprocal theorem points the way to an idea that will allow for the calculation of the displacements associated with a dislocation loop of arbitrary shape. As discussed in chap. 2, the reciprocal theorem asserts that two sets of σ (2) , u(2) , f (2) ), associated with the same σ (1) , u(1) , f (1) ) and (σ equilibrium ﬁelds (σ body (i.e. they satisfy the equilibrium equations), are related by the expression t(1) · u(2) d A + f(1) · u(2) d V = t(2) · u(1) d A + f(2) · u(1) d V. (8.23) ∂

∂

Within the context of the elastic Green function, the reciprocal theorem serves as a jumping off point for the construction of fundamental solutions to a number of different problems. For example, we will ﬁrst show how the reciprocal theorem may be used to construct the solution for an arbitrary dislocation loop via consideration of a distribution of point forces. Later, the fundamental dislocation solution will be bootstrapped to construct solutions associated with the problem of a cracked solid. We consider the generic problem of a dislocated solid with a loop such as that shown in ﬁg. 8.10. Here we imagine two different conﬁgurations associated with

8.4 Elastic Models of Single Dislocations

389

the same inﬁnite body that is described appropriately as an isotropic linear elastic solid. In the ﬁrst body, we imagine a dislocation loop as shown with ﬁelds labeled by the superscript (d), while in the second, we consider a point force at position r and the associated ﬁelds which are labeled with a superscript ( p). For the dislocation case there are no body forces and hence f (d) = 0. By the reciprocal theorem we note that (d) ( p) ( p) (d) t ·u dA = t ·u dA + f ( p) · u(d) d V. (8.24) ∂

∂

The basic idea is to exploit the fact that the displacements associated with the point force are already known, and correspond to the elastic Green function. Further, the displacements associated with the dislocation are prescribed on the slip plane. We can rewrite the surface integral that spans the slipped region as t(d) · u( p) d A = t(d) (−) · u( p) (−)d A + t(d) (+) · u( p) (+)d A. (8.25) ∂

∂−

∂+

(d)

In this case t (+) refers to the traction associated with the dislocation just above the slip plane while t(d) (−) refers to the value of the traction just below the slip plane. However, since the displacement ﬁelds (u( p) ) associated with the point force are continuous across the slip plane, u( p) (−) = u( p) (+). Similarly, the tractions across the slip plane must be equal and opposite (i.e. t(d) (+) = −t(d) (−)). As a result, we are left with (d) ( p) (d) ( p) t ·u dA = t (+) · u (+)d A − t(d) (+) · u( p) (+)d A = 0. ∂

∂−

∂+

(8.26) Hence, the only terms remaining from our implementation of the reciprocal theorem yield the rather simpler expression ( p) (d) t · u d A = − f ( p) · u(d) d V (8.27) ∂

Following the same decomposition of the surface integrals suggested above, we may rewrite the term involving the tractions as t( p) · u(d) d A = t( p) (+) · [u(d) (+) − u(d) (−)]d A. (8.28) ∂

∂

If we now recall that the jump in the displacement ﬁeld across the slip plane is nothing more than the Burgers vector and we exploit the fact that the traction vector is related to the stress tensor via t( p) = σ ( p) n, then the left hand side of eqn (8.28) may be rewritten as ( p) t( p) · u(d) d A = − σi j n j bi d A. (8.29) ∂

∂

390

8 Line Defects in Solids

Recalling our linear elastic constitutive assumption, we may further simplify this result to read ( p) (d) p) t ·u dA = − Ci jmn u (m,n n j bi d A. (8.30) ∂

∂

Thus far, we have treated only one side of eqn (8.27). Our next task is to probe the signiﬁcance of the term involving the body force. Through the artiﬁce of choosing the ﬁelds associated with a point force as our complementary ﬁelds, the dislocation solutions can be obtained directly. In particular, we note that if ( p) f j (r ) = f j δ(r − r ), then we have

f ( p) · u(d) d V = u (d) k (r) f k ,

(8.31)

which involves the unknown dislocation displacement ﬁeld. We may tidy up this ( p) result by recalling that u m that appears in eqn (8.30) is the solution for the point ( p) force problem and hence is given by u m = −G mk f k . As a result, our efforts culminate in the expression, u k (r) = − Ci jmn G mk,n (r − r )n j bi d A , (8.32) ∂

a result known as Volterra’s formula. Note that this result is a special case of the formula we wrote earlier in the eigenstrain context as eqn (2.96). The physical content of this result is that we have found a way by integrating only on the slipped surface to determine the displacement ﬁelds (in linear elasticity) throughout space. In practice, this method is unwieldy for consideration of the standard textbook examples concerning straight dislocations of either pure edge or screw character. On the other hand, for determining the ﬁelds resulting from dislocation loops of arbitrary shape, this formula and its variants are considerably more enlightening. Despite the heavy-handedness of the Volterra formula in the context of straight dislocations, it is instructive to see it in action. As an example of this line of thought, we now use the Volterra formula to reconstruct the displacement ﬁelds associated with a screw dislocation. As was shown earlier, the displacement ﬁelds that are carried by a screw dislocation in an isotropic linear elastic medium may be easily arrived at through the insight that the equilibrium equations reduce to Laplace’s equation in the single unknown ﬁeld, u 3 . Here we instead consider these ﬁelds as the result of our Green function analysis. We orient our coordinate system such that the Burgers vector is given by b = (0, 0, b) and the normal to the slip plane is n = (0, 1, 0). Further, we recall eqn (2.54) which gives the elastic modulus tensor in terms of the Lam´e constants. Substitution of these quantities into the

8.4 Elastic Models of Single Dislocations

Volterra formula yields u m (r ) = −µb

391

∂

(G 33,2 + G 23,3 )d A.

(8.33)

The derivatives of the Green function that we are instructed to evaluate can be carried out through reference to eqn (2.91) resulting in 0 ∞ −µby (λ + 3µ) dx dz u 3 (r ) = 3 8πµ(λ + 2µ) −∞ −∞ [(x − x )2 + y 2 + z 2 ] 2 3(λ + µ)z 2 . (8.34) + 5 [(x − x )2 + y 2 + z 2 ] 2 Not surprisingly, the resulting integrals are entirely tractable and lead to the result b −1 y , (8.35) tan u 3 (r ) = − 2π x in exact coincidence with the displacements that emerge in the simpler, more standard treatment as already revealed in eqn (8.11). A similar analysis can be performed in the context of the conventional edge dislocation within the isotropic elasticity context (see Problems).

8.4.3 The Edge Dislocation We have now succeeded in identifying the deformations induced by a screw dislocation, and have also found a generic formula for the ﬁelds due to an arbitrary dislocation. Our present task is to return to the edge dislocation for the purposes of completeness and because this solution will make its way into our future analysis. This is particularly evident in the case of isotropic linear elasticity where we will ﬁnd that even for dislocations of mixed character, their geometries may be thought of as a superposition of pure edge and pure screw dislocations. Recall from our discussion in chap. 2 that the solution of elasticity problems of the two-dimensional variety presented by the edge dislocation is often amenable to a treatment in terms of the Airy stress function. Consultation of Hirth and Lothe (1992), for example, reveals a well-deﬁned prescription for determining the Airy stress function. The outcome of this analysis is the recognition that the stresses in the case of an edge dislocation are given by σx x (x, y) = − σ yy (x, y) =

y(3x 2 + y 2 ) µb , 2π(1 − ν) (x 2 + y 2 )2

y(x 2 − y 2 ) µb , 2π(1 − ν) (x 2 + y 2 )2

(8.36) (8.37)

392

8 Line Defects in Solids

σx y (x, y) =

µb x(x 2 − y 2 ) . 2π(1 − ν) (x 2 + y 2 )2

(8.38)

Earlier we made the promise that the energy stored in the elastic ﬁelds had a generic logarithmic character, regardless of the type of the dislocation. To compute the elastic strain energy associated with the edge dislocation we use eqn (8.16). In the context of the stress ﬁelds given above, R E strain µb b µb2 R dx = = ln . (8.39) L 2 2π(1 − ν) r0 x 4π(1 − ν) r0 The integrand is determined by computing the tractions on the slip plane using the stresses for the edge dislocation described above, and as claimed, the structure of the energy is exactly the same as that found earlier for the screw dislocation. 8.4.4 Mixed Dislocations As noted earlier, generic dislocations have neither pure screw nor pure edge character. If we consider a straight dislocation with line direction ξ = (0, 1, 0), then the dislocation has a Burgers vector of the form b = b(sin θ, cos θ, 0), where θ is the angle between the line direction and the Burgers vector. We see that using this notation, a screw dislocation is characterized by θ = 0 and an edge dislocation similarly by θ = 90◦ . For the special case in which we consider an isotropic linear elastic material, the total stress ﬁeld due to a mixed dislocation is a superposition of the ﬁelds due to its edge and screw components treated separately. What this means in particular is that the stress tensor can be written as e e s σ11 σ12 σ13 e e s σ = σ12 (8.40) σ22 σ23 . s s e σ13 σ23 σ33 The superscripts e and s refer to edge and screw and serve as an instruction to use the isotropic linear elastic stress ﬁelds for the edge and screw dislocation, respectively, but with the Burgers vector adjusted to account for relevant trigonometric weighting factors. Elastic isotropy considerably simpliﬁes the analyses that we are forced to undertake in our goal of characterizing the deformation ﬁelds associated with a dislocation. On the other hand, there are some instances in which it is desirable to make the extra effort to include the effects of elastic anisotropy. On the other hand, because the present work has already grown well beyond original intentions and because the addition of anisotropy is for the most part an elaboration of the physical ideas already set forth above, we refer the reader to the outstanding work of Bacon et al. (1979).

8.5 Interaction Energies and Forces

A

(a)

393

B

(b)

(c)

Fig. 8.19. Schematic illustration of breaking of translational invariance by (a) the presence of a free surfaces, (b) an internal interface between two dissimilar materials, and (c) a precipitate particle.

8.5 Interaction Energies and Forces Though the elastic theory of single dislocations is interesting in its own right, our elucidation of the elastic ﬁelds of such dislocations leaves us in a position to begin to explore what can be learned about the plastic deformation of crystalline solids on the basis of dislocations. At the very heart of the questions of both yield and hardening is the issue of how a given dislocation responds to the presence of a stress ﬁeld. Whether that stress ﬁeld has its origins in some remotely applied external load or from the presence of inhomogeneities such as point defects, surfaces and interfaces, voids or other dislocations themselves, ultimately we require a quantitative theory of how the dislocation will respond to such forces. We follow the lead of Eshelby already introduced in chap. 2 in our discussion of conﬁgurational forces. Recall that a small excursion δξi of the defect of interest will result in a change of the total energy of the system and attendant loading devices of the form δ E tot = −Fi δξi , where the conﬁgurational force Fi is the work-conjugate partner of the excursion δξi . As we noted earlier, the origin of such conﬁgurational forces is the breaking of translational symmetry. In the case of a single dislocation in an inﬁnite body that is treated within the conﬁnes of the theory of linear elasticity there is no such symmetry breaking, and this is manifested in the fact that translation of the dislocation core results in no energy change. This situation is to be contrasted with those shown in ﬁg. 8.19 in which we examine a dislocation in the presence of other defects. In these cases, it is clear that a small translation of the dislocation will result in a change in the total energy, signaling the presence of a nonzero conﬁgurational force on the dislocation. For the moment, we will restrict our attention to the general statements that can be made concerning such forces in the context of the linear theory of elasticity. In this case, the results simplify considerably in that we can think of such energetic

394

8 Line Defects in Solids

Fig. 8.20. Organization of surface integrals for computing the interaction energy between the ﬁelds of the defect of interest and all other ﬁelds.

forces as arising from the interaction terms between the separate stress systems. Let us parcel the stresses and strains into two groups, those of the singularity of interest which we will label σiSj and those from the remaining singularities and external ﬁelds, σiTj . Eshelby’s idea is to note that if we write the total elastic energy as 1 (σ S + σiTj )(iSj + iTj )d V, (8.41) E elastic = 2 ij then only the cross terms will be affected by the small excursions we intend to impose on the singularity S. Hence, we may rewrite the part of the total energy that is not translationally invariant as 1 E interaction = (σ S T + σiTj iSj )d V. (8.42) 2 ij ij Consideration of ﬁg. 8.20 suggests a strategy for rewriting the interaction energy. Note that within region I, the ﬁelds T are jump free while for region II, the same may be said of the ﬁelds S. Hence, we rewrite the interaction energy as σiTj u i,S j d V. (8.43) E interaction = σiSj u i,T j d V + I

II

This expression insures that our integrations are organized such that the integrands are well behaved in the regions of interest. If we use the fact that the stress ﬁelds satisfy the equilibrium equations (i.e. σi j, j = 0) in conjunction with the divergence theorem, this expression may be rewritten as E interaction = (σiSj u iT − σiTj u iS )n j d S, (8.44) ∂in

where the surface integral is evaluated on the dividing surface ∂in separating the

8.5 Interaction Energies and Forces

395

defect of interest from the rest of the crystal. This interaction energy is independent of the choice of ∂in so long as it encloses the singularity S. Though eqn (8.44) is abstract, it forms the basis of our calculation of the conﬁgurational forces on dislocations. In particular, on the basis of this expression we are now in a position to derive the Peach–Koehler formula which relates the force on a dislocation to the local stress ﬁeld and the geometric descriptors of the dislocation itself such as the Burgers vector b and the line direction ξ . 8.5.1 The Peach–Koehler Formula The expression derived above lays the foundation for much of our work on the forces on dislocations. In particular, we shall ﬁnd it convenient to direct our attention to the way in which an externally applied stress couples to the motion of a dislocation. This will culminate in the elucidation of the so-called Peach–Koehler force which explicitly reckons the force on a dislocation. Before invoking the Peach–Koehler formula, it is perhaps useful to ﬁrst examine the force between two screw dislocations from the perspective of the interaction energy. Our interest is in determining the force of interaction between these dislocations using the Eshelby philosophy espoused above. In particular, we must evaluate the interaction energy when the dislocations are separated by a distance d and when they are separated by a distance d + ξ , which reﬂects the existence of the small excursion which serves as the basis of our calculation of the conﬁgurational force. In this case, we note that the total energy is given by 1 1 1 1 (1) (1) (2) (2) (1) (2) (1) σi j i j d V + σi j i j d V + σi j i j d V + σi(2) E elastic = j i j d V. 2 2 2 2 (8.45) The last two terms, which are equal, represent the interaction energies, and are the only terms that will be affected by the excursion of the dislocation. Hence, we may write E int =

(2) σi(1) j i j d V,

(8.46)

which in terms of the particular dislocation ﬁelds for this case is y2 x(x − d) µb1 b2 d V. + E int = 4π 2 (x 2 + y 2 )[(x − d)2 + y 2 ] (x 2 + y 2 )[(x − d)2 + y 2 ] (8.47) The result of this integration may be derived after some calculations demanding algebraic care, with the result that R µb1 b2 E int (d) = , (8.48) ln 2π d

396

8 Line Defects in Solids

Fig. 8.21. Small excursion of dislocation segment.

where R is a large distance cutoff. In order to compute the conﬁgurational force, we require the difference between E int (d + ξ ) and E int (d) which to lowest order in ξ is given by E int = −

µb1 b2 ξ , 2πd

(8.49)

which implies that the interaction force is given by F=

µb1 b2 . 2πd

(8.50)

We see that in the case in which the Burgers vectors are equal, the force of interaction is repulsive, whereas in the case in which they are equal and opposite, the resulting force is attractive. In reality, all of this was vastly more work than was really needed to derive this elementary result. Our reason for pursuing this heavy-handed approach was not so much in the name of the particular result as to illustrate how the broken translational invariance induced by the presence of two dislocations manifests itself in the emergence of an interaction energy. The whole enterprise of computing the conﬁgurational forces can be worked out in explicit and gory detail in this case, although a more intelligent approach to the integrations would have been to compute the work done in bringing the second dislocation up to the ﬁrst one. The result derived above is but a special case of a more general formula which can be derived from eqn (8.44). In order to compute the more general result, we imagine a small excursion of the segment of dislocation as shown in ﬁg. 8.21. In

8.5 Interaction Energies and Forces

light of eqn (8.44), we must evaluate S T σi j (+)u i (+)n j (+)d S − E int (S, T ) = +

+ ∂in

− ∂in

σiSj (−)u iT (−)n j (−)d S

−

+ ∂in

− ∂in

397

σiTj (+)u iS (+)n j (+)d S

σiTj (−)u iS (−)n j (−)d S, (8.51)

where the label S refers to the ﬁelds associated with the dislocation that is bowing out and the label T refers to all other contributions to the stress. The labels + and − refer to the integration surfaces which are just above and just below the slip plane. We now use the fact that for the case in question, the stresses σiSj associated with the dislocation are continuous (i.e. σiSj (+) = σiSj (−)) and that the displacements associated with system T are continuous (i.e. u iT (+) = u iT (−)). Finally, upon noting that n i (+) = −n i (−), we may rewrite the expression above as bi σiTj n j (−)d S. (8.52) E int (S, T ) = ∂in

Recall that the deﬁnition of the Burgers vector is bi = u i (+) − u i (−), which has been used in writing the above expression in this ﬁnal form. For the special case of the inﬁnitesimal bow-out of a dislocation segment under the action of the stress σiTj , we note that δ E int = bi σiTj (dy × dl) j .

(8.53)

This equation is written on the basis of the observation that the inﬁnitesimal element of area swept out by the dislocation is characterized by the vector product dy × dl. Note that dy is the local excursion of the segment, while dl is a vector along the line at the point of interest. If we now recall that the conﬁgurational force is given as δ E int = −Fm δξm , then we may evidently write the conﬁgurational force in the present context as Fm = m jn bi σi j ζn , (8.54) dl where we have used dl = dlζζ . We apologize for temporarily denoting the local tangent vector as ζ , but note that had we not done so, the symbol ξ would be doing double time, serving to denote both the excursion of the dislocation as well as its local tangent vector. In vector form, we may write this as F σ b) × ζ . = (σ (8.55) dl The physical interpretation of this result is that it is the force per unit length of dislocation acting on a segment by virtue of the presence of the stress ﬁeld σ . This expression is the famed Peach–Koehler formula and will be seen to yield a host of interesting insights into the interactions between dislocations.

398

8 Line Defects in Solids

8.5.2 Interactions and Images: Peach–Koehler Applied In the discussion given above, we have resurrected the notion of an energetic force as ﬁrst described in chap. 2. The key point is the existence of a conﬁgurational force associated with energy changes that attend small excursions of the defect of interest. In the dislocation setting, we have shown that such arguments lead naturally to the Peach–Koehler formula. Presently, we use this formula to investigate the interactions between dislocations in different contexts. Part of our interest in this topic arises from our ultimate interest in explicating hardening in crystals as a consequence of dislocation interactions. Though the elastic theory will be found wanting once the dislocations in question are in too close a proximity, for larger distances of separation, the elastic theory offers an enlightening description of the types of dislocation interactions that are important. Interactions of Two Straight Edge Dislocations We begin with an analysis of the simple case of two parallel edge dislocations. Our aim in the present context is to compute the component of the force which will lead to gliding motion if it is sufﬁciently large as to overcome the intrinsic lattice resistance. The line directions of both dislocations are given by ξ 1 = ξ 2 = (0, 0, 1), and their Burgers vectors are b1 = b2 = (b, 0, 0). The Peach–Koehler formula instructs us to compute F = σ b × ξ . Further, we consider a geometry in which dislocation 1 is at the origin while dislocation 2 is to be found at (x, d). The state of stress at dislocation 2 due to the presence of dislocation 1 is given by d(3x 2 + d 2 ) x(x 2 − d 2 ) 0 − (x 2 + d 2 )2 (x 2 + d 2 )2 2 2 2 2 µb d(x − d ) x(x − d ) . σ = (8.56) 0 2π(1 − ν) (x 2 + d 2 )2 (x 2 + d 2 )2 dν 0 0 − 2 x + d2 By exercising the instructions dictated by the Peach–Koehler formula using the state of stress given above, the force on dislocation 2 is given by F1on2 =

µb2 {i[x(x 2 − d 2 )] + j[d(3x 2 + d 2 )]}. 2 2 2 2π(1 − ν)(x + d )

(8.57)

If we work in units in which x is measured as a fraction f of d (i.e. x = f d) then the glide force (i.e. the force in the x-direction) may be rewritten in dimensionless form as f ( f 2 − 1) 2π d(1 − ν)F = . (8.58) µb2 ( f 2 + 1)2

8.5 Interaction Energies and Forces

399

Fig. 8.22. Force of interaction between two dislocations on adjacent slip planes.

The normalized glide force is plotted in ﬁg. 8.22 where it is seen that there are two equilibrium points for the dislocations one of which is stable and the other of which is unstable. In fact, we have plotted the interaction force for the alternative case in which the dislocations have opposite Burgers vectors as well so as to contrast the resulting solutions. In preparation for our discussion of dislocation junctions, we now consider the case of two dislocations that are not parallel. This analysis is important as a ﬁrst step in evaluating the origins of ‘forest hardening’ in which it is presumed that dislocations gliding on one plane are blocked as a result of dislocations that are piercing their slip plane. The suggestive imagery of a forest of trees serves as a mnemonic for this blocking action and is taken up presently. For simplicity, consider the case depicted in ﬁg. 8.23 in which two screw dislocations characterized by ξ 1 = (0, 0, 1), ξ 2 = (0, 1, 0), b1 = (0, 0, b) and b2 = (0, b, 0), interact according to σ (1) b(2)

0 0 0 −y µb 0 0 s b . = 2π(s 2 + y 2 ) 0 −y s 0

(8.59)

Note that we denote the distance of closest approach of the dislocations (i.e. along the x1 -axis) as s. Carrying out the relevant algebra in conjunction with the Peach– Koehler formula leads to the result that F=−

µb2 s i. 2π(s 2 + y 2 )

(8.60)

This result yields the insight that everywhere along the dislocation line the force of interaction is attractive. However, we note that as a function of the perpendicular

400

8 Line Defects in Solids

Fig. 8.23. Interaction force between two perpendicular screw dislocations (adapted from Hartley and Hirth (1965)).

distance from the line of closest interaction, the interaction becomes weaker. The force proﬁle is indicated schematically in ﬁg. 8.23. Image Forces One of the key manifestations of the broken translational invariance resulting from the presence of a free surface is that of an image force. The presence of a free surface (or an internal interface) implies a breaking of the translational symmetry so that a small excursion of a dislocation will have an attendant energy cost and thereby an attendant conﬁgurational force. In the present section, we undertake an analysis of the image forces that emerge in the simplest of cases, namely that of a screw dislocation near a free surface. The geometry of interest is depicted in ﬁg. 8.24 which shows a screw dislocation a distance d below a free surface. From the standpoint of the elastic boundary value problem involving the dislocation and the free surface, the crucial additional requirement beyond the normal jump condition on the dislocations slip plane is the requirement that the free surface be traction free. What this means in particular is that tn = σ n = 0. If we begin our analysis by considering the ﬁelds due to the dislocation beneath the surface, pretending for the moment that the appropriate ﬁelds are those for a dislocation in an inﬁnite body, we have σ31 (x, y) = −

y+d µb , 2π x 2 + (y + d)2

(8.61)

8.5 Interaction Energies and Forces

401

S

d

d

S

Fig. 8.24. Subsurface screw dislocation and its image partner.

σ32 (x, y) =

x µb . 2 2π x + (y + d)2

(8.62)

These ﬁelds imply a surface traction of the form tn = (0, 0, σ32 ). This observation inspires the conclusion that if we could arrange for a compensating stress −σ32 at the free surface, then the boundary conditions would be satisﬁed. In particular, for this simple geometry it is well known that a parallel dislocation of Burgers vector −b at a distance d above the surface (as depicted in ﬁg. 8.24) accomplishes this end. The full ﬁelds for this problem are y+d y−d µb µb + , 2 2 2 2π x + (y + d) 2π x + (y − d)2 x x µb µb − . σ32 (x, y) = 2 2 2 2π x + (y + d) 2π x + (y − d)2

σ31 (x, y) = −

(8.63) (8.64)

A few remarks on the signiﬁcance of our assumptions are in order. First, we note that the linearity of our elasticity problem is central to the ability to write this solution. Because the sum of two solutions is itself a solution, we know that the elastic ﬁelds themselves are a solution to the problem. Furthermore, by construction, the ﬁelds satisfy the free surface boundary conditions, and hence these ﬁelds are the solution. In light of this result, we are now ready to pose the question concerning the conﬁgurational force induced by the presence of the free surface. We ask the question just how does the energy change if the subsurface dislocation makes a small excursion towards the free surface. However, we have already successfully carried out this calculation in an earlier section and the resulting force was given in eqn (8.50), although in the present case the signs of

402

8 Line Defects in Solids

the dislocations in question are opposite and hence there is an attractive force Fimage = −

µb2 . 4πd

(8.65)

Note that in contrast to the result in eqn (8.50), there is a factor of 4 rather than 2 in the denominator. This arises because the separation of the image dislocations themselves is 2d, not d. We have now seen that by virtue of the presence of a free surface, an image force is induced on a subsurface dislocation. In addition, the idea of an image force has further reinforced our use of conﬁgurational forces and their origins in the breaking of translational symmetry.

8.5.3 The Line Tension Approximation In many instances, the evaluation of the complete set of interactions between several dislocations can be prohibitive, at least at the level of the kind of analysis that one might wish to make with a stick in the sand. Indeed, though in the vast majority of this chapter we have been engaged in the development of the elastic theory of dislocations, we now undertake a different framework in which the complex interactions between various inﬁnitesimal segments of a given dislocation are entirely neglected. An alternative to the full machinery of elasticity that is especially useful in attempting to make sense of the complex properties of three-dimensional dislocation conﬁgurations is the so-called line tension approximation. The line tension idea borrows an analogy from what is known about the perturbations of strings and surfaces when they are disturbed from some reference conﬁguration. For example, we know that if a string is stretched, the energetics of this situation can be described via energy change = T δl.

(8.66)

Similarly, if the surface area of a particular interface is altered, the energetics may be handled through a similar idea, namely, energy change = γ A,

(8.67)

where γ is a surface energy. The analogy with the interfacial energy is more appropriate since dislocations, like free surfaces, have an anisotropy which leads to the conclusion that the energy cost for a small excursion from some ﬂat reference state depends upon the orientation of that reference state. However, the analogy between dislocations and interfaces is imperfect since models of this type have an inherent locality assumption which is exceedingly fragile. To explore this further, we note that in

8.5 Interaction Energies and Forces

403

the line tension approximation, the total energy of a dislocation line may be written as E disloc =

E[θ(s)]ds,

(8.68)

where we have written the dislocation line parameterically in terms of the parameter s, reminds us to integrate along the length of the dislocation of interest and θ is the angle between the local tangent vector and the Burgers vector. The subtlety of the assertion embodied in this equation is that of locality. The basic premise is that the contribution of a given segment to the total energy of the dislocation line depends only on one thing, namely, its local orientation, and is indifferent to the disposition of the remaining segments on the dislocation line. In the context of surfaces, this locality assumption may well be appropriate. On the other hand, because of the long-range elastic interactions between different segments, the energy of a given segment is patently not independent of the disposition of the remaining segments on the line. Nevertheless, as an approximate procedure for reckoning the total energy of some complex dislocation conﬁguration, we can make this locality assumption and use what we have learned earlier about the energetics of straight dislocations to build up a local line energy E(θ ) which depends only on the misorientation θ between the line direction and the Burgers vector. The most naive of all line tension models is that in which a single constant energy is assigned to all orientations. Based on what has been learned earlier (see eqns (8.19) and (8.39)), the assertion is made that E(θ) = T = 12 µb2 , independent of the angle θ . In this case, the line tension becomes a strictly geometric approximation and results in comparisons between different geometries predicated on the overall dislocation line length. In particular, in this approximation the energy is given by dx(s) dx(s) · ds. (8.69) E disloc = T ds ds Note that we have exploited a parameteric representation of the dislocation line in which the position of the line is given by x(s). A more sophisticated version of the line tension approximation is based upon the idea of using the energy per unit length that is obtained for a mixed dislocation in which the angle between the Burgers vector and the line direction is denoted by θ. In this case, the isotropic linear elastic results of section 8.4.4 can be used to obtain the energy per unit length of a mixed dislocation which is given by R µb2 sin2 θ E(θ ) . (8.70) = + cos2 θ ln L 4π 1 − ν r0 Once we are in possession of this result, we are then prepared to examine the

404

8 Line Defects in Solids

energetics of a given dislocation conﬁguration by exploiting it in conjunction with eqn (8.68). We will resort to the line tension approximation repeatedly since as was noted above, much may be learned about the key features of a given problem on the basis of such arguments, which are largely geometrical. Again, what is especially appealing about the line tension approach is the prospect for making analytic headway on fully three-dimensional problems.

8.6 Modeling the Dislocation Core: Beyond Linearity Our discussion of dislocations has thus far made little reference to the signiﬁcant role that can be played by the dislocation core. Whether one thinks of the important effects that arise from the presence of stacking faults (and their analogs in the alloy setting) or of the full scale core reconstructions that occur in materials such as covalent semiconductors or the bcc transition metals, the dislocation core can manifest itself in macroscopic plastic response. Our aim in this section is to take stock of how structural insights into the dislocation core can be obtained. Perhaps the simplest of those features of dislocations that may be thought of as core effects are those associated with the splitting of dislocations into partial dislocations which have associated Burgers vectors that do not correspond to lattice invariant shears. These ideas were already introduced in section 8.3.2. Though the slip associated with partial dislocations does not restore the lattice completely it is nevertheless energetically tolerable with an energy that scales with the stacking fault energy. A dislocation may undergo a splitting reaction into two dislocations that bound a stacking fault. In simple terms, we would describe the resulting dislocation as having a complex core structure. Our treatment in this section will cover three primary thrusts in modeling dislocation core phenomena. Our ﬁrst calculations will consider the simplest elastic models of dislocation dissociation. This will be followed by our ﬁrst foray into mixed atomistic/continuum models in the form of the Peierls–Nabarro cohesive zone model. This hybrid model divides the dislocation into two parts, one of which is treated using linear elasticity and the other of which is considered in light of a continuum model of the atomic-level forces acting across the slip plane of the dislocation. Our analysis will ﬁnish with an assessment of the gains made in direct atomistic simulation of dislocation cores.

8.6.1 Dislocation Dissociation In this section, our aim is to compute the core geometry associated with a dissociated dislocation in an fcc material. Our model will be founded upon a

8.6 Modeling the Dislocation Core: Beyond Linearity

405

Fig. 8.25. Geometry of dislocation splitting.

linear elastic analysis of the interactions between the partial dislocations, but supplemented with a constant energy cost γs f per unit area of stacking fault. To make the analysis eminently tractable, we restrict our attention to an isotropic material. The total energy of the system composed of two partials and the stacking fault they bound is E tot (d) = E self + E int (d) + γs f d.

(8.71)

What we have noted here is that the self-energies of the two Shockley partials are independent of their spacing. It is only the interaction energy between the partials and the stacking fault area itself that involves the splitting distance d. The equilibrium spacing is to be determined by minimizing this total energy with respect to d. We note that the interaction energy may be written as (2) σi(1) (8.72) E int = j i j d V,

where the labels 1 and 2 refer to the two partners in the dissociation reaction as shown in ﬁg. 8.25. The dislocation lines are characterized by ξ (1) = ξ (2) = (0, 1, 0), b(1) = (b sin θ, b cos θ, 0) and b(2) = (b sin θ, −b cos θ, 0). For the special case of elastic isotropy we note that the stress tensor decomposes as shown in eqn (8.40) where we have invoked the observation that the partial dislocations themselves are mixed dislocations. The signiﬁcance of this observation is that it implies that the interaction energy may be written as the sum of two interactions, edge screw . Using the interaction energies derived earlier, this result E int = E int + E int

406

8 Line Defects in Solids

may be rewritten as E int

µb2 cos2 θ d d µb2 sin2 θ + . ln ln =− 2π(1 − ν) R 2π R

(8.73)

The minimization of eqn (8.71) is effected by differentiating the total interaction energy with respect to d and leads to

sin2 θ µb2 deq = − cos2 θ . (8.74) 2π γs f (1 − ν) Thus we see that the splitting of dislocations into partials is characterized by a stacking fault width that is set by the magnitude of the stacking fault energy, with low stacking fault energy materials having larger splittings. As said above, the splitting of dislocations into partials can be thought of as the most elementary of core effects.

8.6.2 The Peierls–Nabarro Model Despite the signiﬁcant gains that have been made with atomistic models of the dislocation core (which we will take up in the next section), it remains of interest to produce analytical insights into the role of the core. One compelling strategy in this regard is that known as the Peierls–Nabarro model which is but one example of the general class of cohesive surface strategies that we will take up in more depth in chap. 12. The cohesive surface strategy in this context is an artiﬁcial mixture of conventional continuum thinking in the form of a linear elastic treatment of the vast majority of the body with a planar constitutive model whose aim it is to mimic the atomic-level forces that act across the slip plane of the dislocated body. This example serves as yet another reminder of the way in which information gleaned at one scale (in this case the interplanar potential) can be used to inform models of a different type. The basic idea of such thinking is embodied in ﬁg. 8.26, where the separation of the dislocated body into two elastic half-spaces joined by atomic-level forces across their common interface is shown. The formulation is aimed at determining the energy minimizing slip distribution on the slip plane. From a kinematic perspective the dislocation is characterized by the slip distribution δ(x) = u(x, 0+ ) − u(x, 0− ) which is a measure of the disregistry across the slip plane. In order to provide a proper variational setting within which to pose this problem we must ﬁrst identify the total energy itself as a functional of this unknown slip distribution. The total energy is built up of two distinct contributions that impose competing inﬂuences on the equilibrium slip distribution. One of the terms in the total energy accounts for the atomic-level interactions across the slip plane which reﬂect the fact that there is

8.6 Modeling the Dislocation Core: Beyond Linearity

407

Fig. 8.26. Schematic of key elements in Peierls–Nabarro dislocation model (courtesy of R. Miller). The key idea is the use of a nonlinear constitutive model on the relevant slip plane which is intended to mimic the atomic-level forces resulting from slip.

an energetic penalty for the disregistry across the slip plane. In particular, we may write −∞ φ(δ(x))d x, (8.75) E misﬁt = ∞

where φ is the interplanar potential which accounts for the disregistry mentioned above. This interplanar potential is the essence of the cohesive surface approach in this context. The most distinctive characteristic of the interplanar potential is the fact that it is nonconvex, implying the existence of multiple wells, and thereby, the possibility for the emergence of complex microstructures such as dislocations. The particular signiﬁcance of this feature in the present setting is that the multiple well character of the interplanar potential allows for a disregistry across the slip plane of a Burgers vector without any attendant energy cost. For the present purposes, the interplanar potential should be thought of as the energy cost associated with sliding two half-spaces with respect to one another by some slip vector. We have already encountered this idea in our discussion of the ideal strength, and in fact, will once again invoke the energetics of rigid sliding given in eqn (8.2). Note that the interplanar potential has the same periodicity as the lattice and that whenever atoms across the slip plane have suffered a relative translation equal to a lattice translation, there is no attendant energy penalty.

408

8 Line Defects in Solids

Fig. 8.27. Decomposition of slip distribution into a superposition of inﬁnitesimal dislocations.

The second contribution to the total energy, which also depends upon the as-yet undetermined slip distribution δ(x) is the elastic energy associated with the dislocation. As indicated schematically in ﬁg. 8.27, the Peierls–Nabarro dislocation may be thought of as a continuous distribution of inﬁnitesimal dislocations. These dislocations in turn are imagined to suffer the usual elastic interactions between dislocations that were described above. Because of our use of linear elasticity, the dislocation ﬁelds are obtained through the superposition principle by adding up the contribution from each inﬁnitesimal dislocation separately. Recall that for the case of two edge dislocations at positions x and x within the conﬁnes of isotropic linear elasticity, the interaction energy is given by E int =

1 µb2 . 2π(1 − ν) x − x

(8.76)

This result may be borrowed for the continuous distribution imagined here once we recognize that the Burgers vector of each such inﬁnitesimal dislocation is related to the local gradient in the slip distribution as is seen in ﬁg. 8.27. Hence, the elastic energy due to all such dislocations is given by dδ(x) dδ(x ) µ R d x d x ln . (8.77) E elastic = 2π(1 − ν) x − x dx dx In the equation given above, R is an inconsequential constant introduced as a large distance cutoff for the computation of the logarithmic interaction energy. Given the energy functional which depends upon the unknown slip distribution we are now set up to use standard techniques to ﬁnd the energy minimizing slip distribution. Evaluating the functional derivative of the total energy with respect to the function δ(x) (which amounts to balancing the atomic-level forces with those due to the elastic interactions) results in the Peierls–Nabarro integro-differential

8.6 Modeling the Dislocation Core: Beyond Linearity

409

equation which may be written as µb ∂φ(δ) = − ∂δ 2π(1 − ν)

1 dδ(x ) dx . x − x dx

(8.78)

For the special case in which we make the simplifying assumption that the interplanar potential takes the simple cosine form given in eqn (8.2) and advocated earlier in the context of the ideal strength model, this problem allows for direct analytic solution. In particular, the solution is b b −1 x δ(x) = − tan . (8.79) 2 π a One of the key features that emerges from this solution, and a crucial hint for the type of analyses we will aim for in the future, is the fact that the stresses implied by the Peierls–Nabarro solution do not suffer from the same singularities that plague the linear elastic solution. A detailed examination of this point may be found in Hirth and Lothe (1992) and is illustrated in their eqn (8-13). By introducing an element of constitutive realism in the form of a nonlinear (and in fact nonconvex) interplanar potential, the solution is seen to be well behaved. One of the outcomes we require of our analysis of dislocations is an insight into the value of the stress needed to move a dislocation. The Peierls–Nabarro model offers the possibility of examining this question. The key qualitative feature that will emerge from our calculations will be the idea that a straight dislocation may be thought of as living in an effective potential that is periodic. The periodicity of this potential reﬂects the fact that there are many degenerate wells within which we may place the dislocation, each separated by a fundamental length determined by the crystal symmetry. In order to induce dislocation motion, the applied stress must be sufﬁciently high so as to overcome the lattice resistance provided by the periodic Peierls potential. As usual, we hark back to the role of symmetry breaking terms in inducing conﬁgurational forces, of which the Peierls stress is but one example. One of the dominant objectives posed in the context of the theory of dislocations is how such models may assist us in the understanding of crystal plasticity. As noted earlier, one measure of our success is our ability to shed light on the tandem questions of yield and hardening. As yet, our focus has primarily centered on the behavior of single dislocations, and is hence at best only an initial foray into these type of problems. From the single dislocation perspective, one of the ﬁrst questions we might hope to answer is that of how a single dislocation responds to the presence of an applied stress. Our earlier efforts were based upon the linear elastic theory of dislocations, and revealed that even in the presence of a very small stress, a dislocation will experience a force compelling it to motion. On the other

410

8 Line Defects in Solids

hand, the phenomenology of plasticity teaches us that dislocation motion is one of many examples of a phenomenon that exhibits threshold behavior. Until a certain critical stress is reached, the dislocation remains sessile. Our task is to uncover the microscopic origins of this threshold response. One immediate route that allows for the examination of this question is offered by the Peierls–Nabarro model discussed above. Recall that the total energy of the Peierls dislocation was seen as arising from two distinct sources. On the one hand, there is an elastic contribution that arises from the two half-spaces that are adjacent to the slip plane. Secondly, we argued that there is an energy cost associated with the disregistry across the slip plane (the so-called misﬁt energy). Within the conﬁnes of the continuum description offered above, the energy of the Peierls dislocation is invariant under translations of the dislocation coordinate. This result emerges from the fact that we treat the misﬁt energy as an integral over the slip plane disregistry. To remedy this ﬂaw, it is necessary to make further concessions in the direction of atomistic realism. In particular, we must sample the interplanar potential at those discrete positions that are consonant with the underlying crystal lattice. In particular, to compute the Peierls stress, we make the transcription ∞ ∞ φ(δ(x − xc ))d x → φ(δ(nb − xc ))x, (8.80) E misﬁt (xc ) = −∞

n=−∞

where we have introduced the parameter xc to denote the position of the dislocation as measured by the position on the slip distribution where the slip is b/2, for example (i.e. δ(xc ) = b/2). The signiﬁcance of this replacement is that rather than evaluating the misﬁt energy at a continuum of points along the slip plane, the energy of disregistry is computed at a series of equally spaced points meant to mimic the atomic positions themselves. In this context, it is imagined that the dislocation core is translated with respect to the atomic positions. For the particular choice of interplanar potential suggested by Frenkel, this sum may be written as ∞ 2π b b µb2 −1 x c + nb 1 − cos E misﬁt (xc ) = . (8.81) − tan 4π 2 d n=−∞ b 2 π a All that we have done to arrive at this equation is to use eqn (8.2) to evaluate the energy at various points on the slip plane which have undergone slip characterized by eqn (8.79). After appropriate massaging using obvious trigonometric identities, this sum may be rewritten as E misﬁt (xc ) =

∞ µb2 a 2 1 , 2 2 2π d n=−∞ a + (xc + nb)2

(8.82)

which has the look of a sum that might be handled by the Poisson summation

8.6 Modeling the Dislocation Core: Beyond Linearity

formula. The Poisson summation formula states ∞ ∞ ∞ f (n) = f (x)e2πikx d x, n=−∞

k=−∞

411

(8.83)

−∞

and is predicated on the hope that the transformed sum in the variable k will be more directly amenable than was the sum in n. If we introduce the dimensionless variables γ = a/b and δ = x/b, the sum may be rewritten as ∞ 2πiku ∞ µa 2 d du −2πikδ e , (8.84) E misﬁt = 2 2 2 2π d k=−∞ −∞ γ + u which after performing the relevant integrations leads in turn to 2π xc − 2πa µab b 1 + 2 cos e E misﬁt (xc ) ≈ . 2πd b

(8.85)

In performing this sum, we have kept only the terms corresponding to k = 0 and k = ±1. What has been achieved thus far? Our claim is that the calculation just performed tells us the energy proﬁle for a straight dislocation as that dislocation is moved against the background of the ﬁxed lattice. That is, the straight dislocation is now seen to have a series of wells in which it has a minimum energy and in the act of passing from one well to the next it must cross a barrier known as the Peierls barrier which gives rise to the intrinsic lattice resistance to dislocation motion. Our next task is to use our newly found Peierls potential to estimate the stress to move a straight dislocation. The stress is essentially provided as the derivative of the energy proﬁle with respect to the coordinate x, and is given by µ 2π x −πd/(1−ν)b ∂ E(x) =− sin e , (8.86) ∂x 1−ν b where we have used the recollection that the parameter a is a measure of the core width and is given by a = d/2(1 − ν). By evaluating the derivative of this expression in turn, we ﬁnd that the maximum value of the stress occurs when x = b/4, yielding an estimate of the Peierls stress of µ −π d/(1−ν)b . (8.87) τP = e 1−ν Our analysis calls for a number of observations. First, we note that the formula for the Peierls stress leads to the expectation that the stress to move a dislocation will be lowest for those planes that have the largest interplanar spacing at ﬁxed b. In the case of fcc crystals, we note that the spacing √ between (001) planes is given by a0 /2, while for (110)√planes the spacing is 2a0 /4, and ﬁnally for the (111) planes this value is a0 / 3. A second observation to be made concerns

412

8 Line Defects in Solids

the magnitude of the Peierls stress. What we note is that the stress to move a dislocation is down by an exponential factor in comparison with the shear modulus. Recall that in our discussion of the ideal strength, the expectation was that aside from numerical factors, the ideal strength goes as the shear modulus itself. By way of contrast, we now see that the presence of the dislocation modulates this estimate. A ﬁnal observation that should be made is that even this case is too idealized. Real dislocation motion often takes place by kink mechanisms in which a bulge on the dislocation line brings a segment of the dislocation into adjacent Peierls wells, and the resulting kinks propagate with the end result being a net forward motion of the dislocation.

8.6.3 Structural Details of the Dislocation Core Thus far, our discussion of dislocation core effects has been built around those tools admitting of direct analytic progress such as is offered by the Peierls–Nabarro dislocation core model. This model has many virtues. However, it is also strictly limited, with one of its primary limitations being that without huge machinations, it may only be applied to dislocations with planar cores. To explore the full atomic-level complexity that arises in dislocation cores, we must resort to numerical techniques, and direct atomistic simulation in particular. The remainder of our discussion on dislocation cores will take up the question of how one goes about carrying out such simulations and what may be learned from them. One of the central conclusions derived from the Peierls–Nabarro analysis is the role of nonlinear effects in the dislocation core. From an atomistic perspective, the far ﬁeld atomic displacements could be derived just as well from linear elasticity as the full nonlinear function that results from direct atomistic calculation. By way of contrast, in the core region it is the nonlinear terms that give rise to some of the complex core rearrangements that we take up now. Our discussion will be built around two key examples: cores in fcc metals and the core reconstructions found in covalent semiconductors such as in Si. Before embarking on the speciﬁcs of these cores, we begin with an assessment of the basic ideas needed to effect an atomistic simulation of the dislocation core. We begin with a picture of lattice statics in which the core geometry is determined by energy minimization. To proceed, what is needed is an energy function of the type discussed in chap. 4 which may be written generically as E tot = E({Ri }),

(8.88)

which gives the total energy once the atomic positions have been speciﬁed. For the moment, we are indifferent to the particulars of the choice of total energy scheme. Later we will see that the detailed core geometry can depend critically on this

8.6 Modeling the Dislocation Core: Beyond Linearity

413

choice, and that not all choices are equally satisfying. On the other hand, since our present ambition is the description of how to perform such a simulation we leave these details aside. From the standpoint of energy minimization, we have said all there is to say except for the all important issue of boundary conditions. For the moment, we describe the most naive approach to this problem and will reserve for later chapters (e.g. chap. 12) more sophisticated matching schemes which allow for the nonlinear calculations demanded in the core to be matched to linear calculations in the far ﬁelds. As we have repeatedly belabored, the objective is to allow the core geometry to emerge as a result of the full nonlinearity that accompanies that use of an atomistic approach to the total energy. However, in order to accomplish this aim, some form of boundary condition must be instituted. One of the most common such schemes is to assume that the far ﬁeld atomic positions are dictated entirely by the linear elastic ﬁelds. In particular, that is xi = Xi + u(Xi ),

(8.89)

where xi is the position of the far ﬁeld atom i in the dislocated crystal, Xi is the position of the same atom in the perfect crystal and u(Xi ) is the displacement of that atom in the dislocated crystal as obtained using Volterra ﬁelds for a single straight dislocation like those described in section 8.4. To perform the energy minimization, the atoms in the far ﬁeld are rigidly ﬁxed to their linear elastic values. As an initial guess, it is often elected to assume that the initial positions even for the atoms that are being relaxed is well described by the linear elastic solution. The forces are computed using the total energy scheme and the local minimum is found by any of a number of schemes including conjugate gradient, Monte Carlo, Newton–Raphson, etc. Core structures in fcc materials A key example of the strategy for direct atomistic simulation of dislocation cores advocated above is that of fcc metals. In this case, we consider the atomic-level geometry of a perfect dislocation (which by virtue of the relaxation will split ¯ and Burgers vector (a0 /2)(110). ¯ into partials) with line direction (112) The Volterra ﬁelds associated with this geometry are introduced using the scheme suggested in eqn (8.89). For the case shown here, the atomic-level relaxation has been performed using the conjugate gradient method on an arrangement of Al atoms described by the embedded-atom potentials of Ercolessi and Adams. These potentials are of the traditional pair functional form. As noted above, the key structural rearrangement that occurs for this type of dislocation is the splitting of the perfect dislocation into Shockley partials. This result is shown in ﬁg. 8.28. We note that the resulting atomic-level geometry is a concrete realization of the arguments made earlier in this section concerning dislocation dissociation.

414

8 Line Defects in Solids

Fig. 8.28. Atomic-level geometry of the dislocation core for the conventional edge dislocation in Al (courtesy of Kedar Hardikar): (a) a view along the line direction of the dislocation showing two partials, and (b) a view looking down on the slip plane, revealing the stacking fault region bounded by the two partials.

Core reconstructions in Si A more substantial rearrangement in the dislocation core can be found in the case of a covalent material. Probably the single greatest inﬂuence on the structures adopted by defects in covalent materials is the severe energy penalty that attends dangling bonds. Free surfaces, grain boundaries and dislocation cores all have geometries that reconstruct in a manner that preserves (albeit in a distorted way)

8.7 Three-Dimensional Dislocation Conﬁgurations

415

Fig. 8.29. Atomic-level geometry of the dislocation core for the 30◦ partial dislocation in Si (adapted from Bulatov et al. (1995)). (a) Unreconstructed core structure and (b) reconstructed core structure with dimerization along line direction.

the fourfold coordination of the atoms in question. In the present discussion, we examine a manifestation of this antipathy for dangling bonds in the context of dislocation core structures. For concreteness, we consider the core geometry of the 30◦ partial in Si as computed using Stillinger–Weber potentials. Recall from the discussion of chap. 4 that the Stillinger–Weber potentials incorporate an angular term which penalizes deviations from the ideal tetrahedral angles found in the cubic diamond structure. For the present purposes, the key feature of the atomic-level relaxations is the presence of a dimerization reaction as seen in ﬁg. 8.29. Prior to relaxation, the Volterra ﬁelds leave each atom in the core region missing one of its full complement of four neighbors. The relaxation remedies this loss by pairing up the atoms along the core direction, restoring fourfold coordination and lowering the energy.

8.7 Three-Dimensional Dislocation Conﬁgurations To have any hope of honestly addressing the dislocation-level processes that take place in plastic deformation, we must consider fully three-dimensional geometries. Though we earlier made disparaging remarks about the replacement of understanding by simulation, the evaluation of problems with full three-dimensional complexity almost always demands a recourse to numerics. Just as the use of analytic techniques culminated in a compendium of solutions to a variety of twodimensional problems, numerical analysis now makes possible the development of catalogs of three-dimensional problems. In this section, we consider several very important examples of three-dimensional problems involving dislocations, namely, the operation of dislocation sources and dislocation junctions.

416

8 Line Defects in Solids

Fig. 8.30. Geometry associated with dislocation bow-out between two pinning points.

8.7.1 Dislocation Bow-Out A recurring theme in a number of different contexts is that of dislocation bow-out. In a number of different circumstances, a dislocation segment of ﬁnite extent, pinned at its two ends, is subjected to a resolved shear stress which has the effect of bowing out the segment in its slip plane. The simplest setting within which to view this process is the line tension approximation set forth earlier in this chapter. Dislocation pinning is a ubiquitous phenomenon. Pinning arguments arise in the context of solution and precipitate hardening as well as the discussion of dislocation sources. Our present discussion has as its aim the development of some of the theoretical apparatus needed to discuss the response of dislocations in this context, without giving any attention to the attributes of the pinning centers themselves. We simply imagine a geometry like that shown in ﬁg. 8.30 in which the dislocation is pinned at the two endpoints, leaving a segment of length l that is free to glide. The energetics of the bowed-out segment may be constructed simply on the basis of line tension arguments. We begin by adopting the simplest possible model of line tension, namely, that in which the angular dependence is ignored altogether. In this case, the energy of the bowed segment as a functional of its displacement proﬁle u(x) is given by l l 2 2 2 T 1 + u dx − σ bu(x)d x. (8.90) E[u(x)] = − 2l

− 2l

Our interest is in determining the energy minimizing conﬁguration of the bowedout segment. To do so, we note that this has become a simple problem in variational calculus, with the relevant Euler–Lagrange equation being

T u d = −σ b. (8.91) d x (1 + u 2 ) 12

8.7 Three-Dimensional Dislocation Conﬁgurations

417

Even at the level of the line tension approximation, this equation may be solved to various levels of approximation. In the limit in which the bow-out is small (i.e. |u | 1), the denominator in the expression given above can be neglected with the result that the equilibrium equation takes the form, σb d 2u =− . 2 dx T The solution to this equation can be written down by inspection as

(8.92)

σb 2 x + cx + d, (8.93) 2T where c and d are as-yet undetermined constants. Note that the solution we seek satisﬁes the boundary conditions u(−l/2) = u(l/2) = 0. Application of these boundary conditions results in the solution σ b l2 2 (8.94) −x , u(x) = 2T 4 u(x) = −

which may be recast in dimensionless terms if the stress is measured in units of σ = f (2T /bl), and f is what fraction of 2T /bl the stress has attained, and similarly, we take x = δ(l/2). In light of these notational simpliﬁcations, our expression for the bowed-out proﬁle may be rewritten as fl (8.95) (1 − δ 2 ). 4 The equation for bow-out may also be solved exactly without resorting to the approximation in which |u (x)| 1. In this case, the equation of equilibrium may be written (after performing the ﬁrst integration) 2 σ bx u 2 +c , = − (8.96) 1 + u 2 T u(x) =

where c is a constant of integration to be determined in light of the boundary conditions. This equation is separable and leads immediately to the solution T2 T2 l2 2 u(x) = . (8.97) − x − − σ 2 b2 σ 2 b2 4 Like its approximate partner derived above, this equation can be rewritten in dimensionless variables as 1 1 l 2− − δ − 1 . (8.98) u(δ) = 2 f2 f2 In the treatment above, we have used the line tension approximation to deduce both an exact and an approximate treatment of bow-out. The comparison between

418

8 Line Defects in Solids

Fig. 8.31. Comparison of the bow-out geometry resulting from exact (full line) and approximate (dashed line) treatment of the line tension approximation. f is a dimensionless stress such that f = σ bl/2T .

the resulting solutions is shown in ﬁg. 8.31. As expected, we note that in the small bow-out limit, the exact and approximate treatments are in very good accord, while for larger stresses, their correspondence is completely unsatisfactory. We have deemed it worthwhile to examine this comparison since in many instances, the treatment of curved dislocations is made not only in the constant line tension approximation, but also with the assumption that |u | 1, an assumption we are now in a better position to view skeptically.

8.7.2 Kinks and Jogs Our treatment thus far has centered on idealized geometries in which the dislocation is presumed to adopt highly symmetric conﬁgurations which allow for immediate insights from the linear elastic perspective. From the phenomenological standpoint, it is clear that we must go beyond such idealized geometries and our ﬁrst such example will be the consideration of kinks. The formation of kink–antikink pairs plays a role in the interpretation of phenomena ranging from plastic deformation itself, to the analysis of internal friction. For the purposes of our modeling efforts here, we will treat the formation energy of kinks via a hybrid scheme in which the elastic energy of the dislocation line that has adopted a conﬁguration like that shown in ﬁg. 8.32 is treated in the line tension approximation. The line tension picture supposes that the energy associated with perturbing a dislocation line can be accounted for in much the same way that one describes the potential energy of a stretched string. If we ignore the dependence of the line energy on the angle between the line and the Burgers vector, then the line

8.7 Three-Dimensional Dislocation Conﬁgurations

419

Fig. 8.32. Schematic of the geometry associated with the formation of a kink in the dislocation line (adapted from Sch¨ock (1980)).

tension may be treated as a scalar T and the energy associated with distorting the line is given by E elastic = T 1 + u 2 d x. (8.99) The kink conﬁguration emerges as the result of a competition between the elastic energy as characterized by the line tension which favors a straight dislocation line and a nonlinear term whose origins are crystallographic. By virtue of the translational periodicity of the underlying lattice the dislocation line may be thought of as riding in a periodic potential that we will call W p (u) and which is really nothing more than the result obtained in eqn (8.85). The idea here is that there are a series of wells that the line can occupy and the kink is a mechanism whereby the line can pass from one such well into another. As noted above, the nature of the kink reﬂects a competition between two different factors. Consideration of ﬁg. 8.32 illustrates that in the limit that the energy scale associated with the line tension is much larger than that of the multiple welled Peierls potential, the dislocation line will vary slowly with a resulting wide kink. Alternatively, in the limit that the peaks in the Peierls potential are high, the lowest-energy conﬁguration will correspond to a kink that has as little of its length on that peak as possible. The mathematical setting for examining this competition is the functional minimization of the energy E[u(x)] = T 1 + u 2 d x + W p (u)d x. (8.100) As seen in the ﬁgure, the function u(x) characterizes the displacement of the line from the well at the origin. The boundary condition of interest here is that u(−∞) = 0 and u(∞) = b. Our ambition is to ﬁnd the energy minimizing disposition of the dislocation as described by the function u(x). This function in the present context is a complete

420

8 Line Defects in Solids

characterization of the kink geometry. Evaluation of the variational derivative of the total energy given in eqn (8.100) leads to an Euler–Lagrange equation of the form u d − W p (u) = 0. T√ (8.101) dx 1 + u 2 If we further assume that |u | 1, then the equation simpliﬁes to T u − W p (u) = 0.

(8.102)

Upon multiplication by u , we are immediately led to a ﬁrst integral of the problem, which implies in turn that the proﬁle satisﬁes du 2 = W p (u). (8.103) dx T This equation may be integrated to yield a kink geometry of the form " Wp 2π x 2b −1 e b T . (8.104) tan u(x) = π Furthermore, we may determine the energy of the kinked conﬁguration in light of our solution in conjunction with the ﬁrst integral of the motion found above. The deﬁnition of the kink formation energy is f

E k = E kink − E straight .

(8.105)

This may be rewritten using our knowledge of the line energy and the periodic potential W p (u) as ∞ ∞ ∞ 2π u f 2 Ek = dx − T 1 + u dx + W p 1 − cos T d x. (8.106) b −∞ −∞ −∞ If we now expand the square root and recall from our ﬁrst integral that T u 2 /2 = W p [1 − cos(2π u/b)], the resulting kink energy is given by ∞ 2π u f E k = 2W p d x. (8.107) W p 1 − cos b −∞ If we now substitute the solution for the kink proﬁle (i.e. u(x)) obtained in eqn (8.104), the resulting integral is elementary and results in a kink energy 4b f T Wp . (8.108) Ek = π In addition to the insights that can be gleaned from continuum arguments, atomistic analysis has been used to shed light on some of the structural complexity that attends the motion of kinks. The basis for our case study will be the partial dislocations that are known to exist in covalent materials such as Si. In particular,

8.7 Three-Dimensional Dislocation Conﬁgurations

421

Fig. 8.33. Schematic of the computational cell used to model the structure and energetics of kinks using atomic-level analysis (adapted from Bulatov et al. (1995)).

there have been a variety of atomic-level calculations of the structure and energetics of kinks in Si using both empirical potentials such as the Stillinger–Weber potentials introduced in chap. 4, but also on the basis of tight-binding theory and density functional theory. The key insight that will emerge from our discussion of atomic-level calculations of the structure and energetics of kinks is that the kinks themselves are capable of supporting a number of defects within a defect which can alter the properties of the kinks and which may invalidate some of the ideas on kinks advanced in the continuum setting. As was shown in ﬁg. 8.29, partial dislocations in Si admit of a core reconstruction that includes dimerization along the line direction. It is that reconstructed geometry that will serve as our jumping off point for the calculation of the structure and energetics of kinks in Si. The calculations to be considered here were carried out using a computational cell of the form shown in ﬁg. 8.33 in which a kink–antikink pair are imposed on the dislocation line. The energy minimizing geometry was determined in this case by resorting to a simulated annealing algorithm. Since the kinked conﬁguration, and even the dislocation conﬁguration itself, is metastable, care had to be taken to ﬁnd only local minima and to guard against falling into the deeper well corresponding to a conﬁguration free of any vestiges of the dislocation. Though the issues that were confronted in achieving this are interesting in themselves, we leave them here for our more immediate concern, namely, the kink geometries themselves. As can be seen in ﬁg. 8.34,

422

8 Line Defects in Solids

Fig. 8.34. Series of conﬁgurations associated with motion of kink on the 30◦ partial in Si (adapted from Bulatov et al. (1995)).

in addition to the ability to determine the energy wells corresponding kinks, it is also possible to ﬁnd the transition pathways connecting one kink conﬁguration to another. In addition to the questions that can be raised about kink motion, the type of atomistic analysis being described here has also been used to examine the propensity for nucleation of kinks themselves. Though plausible mechanisms for

8.7 Three-Dimensional Dislocation Conﬁgurations

423

homogeneous nucleation of kink–antikink pairs exist, a more compelling argument can be made for heterogeneous nucleation off of in-core defects known as antiphase defects (APD). These antiphase defects arise from the fact that when the core of the partial dislocation like that under consideration here reconstructs, a given atom can form a partnership (i.e. dimerize) with its partners either to the left or to the right. If a sequence of partnerships is struck to the right and then changes to a partnership to the left, the point at which this transition occurs will bear the imprint of this transition in the form of a dangling bond. An especially interesting conclusion deriving from the atomistic analysis is that these antiphase defects can serve as the hosts for the nucleation of kink–antikink pairs. The mechanism for this nucleation is shown in ﬁg. 8.35. The atomic-level calculations described above were carried out using the Stillinger–Weber potentials. A step toward a higher level of realism in the description of the total energy can be made by accounting for the electronic degrees of freedom. As has already been made evident throughout the book, an intermediate position which strikes a compromise between computational tractability and accuracy is the tight-binding method. A series of tight-binding calculations have been carried out on the same systems described above (Nunes et al. 1998) resulting in the same sort of structural information. An example of these results is shown in ﬁg. 8.36. Our main objective in this section has been to illustrate the way in which continuum and several different atomistic schemes can be brought to bear on the same underlying problem.

8.7.3 Cross Slip Another important class of three-dimensional dislocation conﬁgurations are those associated with the cross slip process in which a screw dislocation passes from one glide plane to another. The most familiar mechanism for such cross slip is probably the Friedel–Escaig mechanism, which is illustrated schematically in ﬁg. 8.37. The basic idea is that an extended dislocation suffers a local constriction at some point along the line. This dislocation segment, which after constriction is a pure screw dislocation, can then glide in a different slip plane than that on which is gliding the parent dislocation. This mechanism, like those considered already, is amenable to treatment from both continuum and atomistic perspectives, and we take them each up in turn. Since it is presumed that the process of cross slip is thermally activated, to the extent that we are trying to explicate the unit processes that make up plasticity it is of great interest to come up with an estimate for the activation energy for cross slip. In broad terms, what this implies is a comparison of the energies between the unconstricted and constricted states. The simplest continuum estimate

424

8 Line Defects in Solids

Fig. 8.35. Nucleation of a kink–antikink pair from an antiphase defect (adapted from Bulatov et al. (1995)).

of this process derives from the line tension approximation. At a higher level of sophistication it is also possible to investigate this process from the point of view of full three-dimensional elasticity. An overview of some of the continuum thinking on these problems can be found in Saada (1991). On the other hand, the continuum treatment of cross slip is attended by a number of uncertainties. An

8.7 Three-Dimensional Dislocation Conﬁgurations

425

Fig. 8.36. Series of conﬁgurations associated with motion of kink on the 30◦ partial in Si as computed using the tight-binding model (adapted from Nunes et al. (1998)).

attractive feature of atomic-level calculations is that they allow for a systematic investigation of some of the complex questions that have earlier been attacked from the line tension or linear elastic perspective. The cross slip process has attracted attention with a resulting series of impressive calculations of the various intermediate conﬁgurations connecting the initial and ﬁnal states of a dislocation that has undergone cross slip as well as the energy barrier that separates them

426

8 Line Defects in Solids

Fig. 8.37. Schematic of the Friedel–Escaig cross slip mechanism (adapted from Bonneville et al. (1988)).

(Rasmussen et al. 1997a). These calculations were undertaken using a pair functional description of the total energy. Though there are a number of technical details associated with the calculations to be presented here, we will concentrate primarily on what these calculations have to say about cross slip itself without entering too much into the ﬁne points of the calculation. Sufﬁce it to say that like in any problem in which one is in search of an activation pathway, it is not always true that this pathway is that which presents itself to intuition, and hence a number of clever schemes have been set forth for ﬁnding the transition state. In the present setting, the series of steps taking a dislocation from one glide plane to another are shown in ﬁg. 8.38. From a visual perspective, what we wish to take away from this calculation is that the mechanism of cross slip in this case is largely similar to that indicated schematically above in ﬁg. 8.37. The energy of the intermediate state is ≈ 2.7 eV higher than that of the starting conﬁguration, which raises serious questions as to whether the homogeneous nucleation of a constriction is really plausible. Future work will have to explore the possible catalytic effect of heterogeneities which can induce cross slip. An interesting continuum model of cross slip induced by the presence of slip plane heterogeneities may be found in Li (1961). As an illustration of the type of observations that can be made on cross slip, we show a set of beautiful experimental pictures of the cross slip process in ﬁg. 8.39.

8.7.4 Dislocation Sources Frank–Read Sources. It is well known that with increasing deformation, the density of dislocations increases. This effect is illustrated in ﬁg. 8.40 in which the number of dislocations as a function of the strain is indicated schematically. The immediate conclusion from this observation is the fact that there are sources

8.7 Three-Dimensional Dislocation Conﬁgurations

427

Fig. 8.38. Series of intermediate conﬁgurations during the cross slip process as computed using atomistics (adapted from Rasmussen et al. (1997b)).

Fig. 8.39. Experimental image of the cross slip process (courtesy of I. Robertson).

of dislocations within solids which serve to increase the number of dislocations present. Though there have been a number of mechanisms postulated for the multiplication of dislocations, the most celebrated mechanism is known as the Frank–Read source and will serve as the cornerstone of the present discussion. The increase in the net dislocation density with increasing deformation illustrates that even with the passage of some fraction of the dislocations out of the crystal at the surface, there must be sources operating within the crystal. From an experimental perspective, the nature of these sources at the statistical level remains largely unexplored. On the other hand, speciﬁc mechanisms have been suggested, one of which we take up in quantitative detail here. An overview on the subject of dislocation sources can be found in Li (1981). The Frank–Read mechanism postulates the existence of some ﬁnite segment that can be bowed out in the same sense as was discussed earlier in this section. With increasing stress, the segment

428

8 Line Defects in Solids

Fig. 8.40. Illustration of the increase in dislocation density with deformation (adapted from Asaro (1983)).

continues to bow out until a critical stress is reached beyond which the dislocation’s line tension is no longer able to resist the bow-out and the segment continues to expand indeﬁnitely. The speciﬁc analytic ideas associated with the bowing-out of a pinned segment were already described earlier in this section. As a result of these arguments, we ﬁnd that the applied stress and the radius of curvature of the bowed-out segment are related by R=

T . τb

(8.109)

An additional insight may be garnered from this discussion which applies to the Frank–Read source. For a segment that is pinned between two points by a spacing d, and that will operate as a Frank–Read source, we now see that with increasing stress the radius of curvature will reduce. For a given pinning geometry, the maximum stress will occur when the radius of curvature is half the spacing between

8.7 Three-Dimensional Dislocation Conﬁgurations

429

obstacles or 2T . bd

τsource =

(8.110)

If we now invoke an approximate expression for the line energy, namely, T = 1 µb2 , then the critical stress may be rewritten as 2 b . L

τsource = µ

(8.111)

Thus we note that we have argued for a dislocation source which operates at a stress that is smaller than the shear modulus by a factor of b/L. Though the argument given above was offered in the spirit of the line tension approximation, the Frank–Read mechanism can be examined from the linear elastic perspective as well. The segment which is to serve as the Frank–Read source has a geometry that is determined by two competing effects. On the one hand, the applied stress has the tendency to induce glide in the various segments that make up the dislocation. On the other hand, the mutual interactions of the various segments (the effect giving rise to the line tension in the ﬁrst place) tend to maintain the dislocation line in its straight conﬁguration. The playing out of this balance can be carried out dynamically by supposing that a given dislocation segment glides with a velocity that is proportional to the force it experiences. That is, the n th segment on the dislocation line is attributed a velocity vn = M Fn ,

(8.112)

where M is a parameter characterizing the mobility of dislocations in the overdamped limit considered here. The main point behind a dynamics like that described here is that we are considering the limit in which dissipative effects are dominant and the dislocation is maintained in a steady state of motion with the work of the applied stress all going into feeding the relevant dissipative mechanisms such as phonon drag which results from the coupling of the dislocations center of mass motion to the vibrations of the atoms around it. The sequence of states reached by a dislocation subjected to a sufﬁciently large applied stress is shown in ﬁg. 8.41. A second view of the dislocation dynamics approach to Frank–Read sources is shown in ﬁg. 8.42. A further elaboration of this so-called ‘dislocation dynamics’ approach will be set forth in chap. 12. One of the more intriguing features of ﬁgure 8.42 is the realization that the full elasticity treatment conﬁrms our intuition about those parts of the bowing-out process which occur at stresses larger than the critical stress.

430

8 Line Defects in Solids

Fig. 8.41. Frank–Read source as obtained using dislocation dynamics (adapted from Zbib et al. (1998)).

Fig. 8.42. Three-dimensional rendering of a Frank–Read source as obtained using dislocation dynamics (adapted from Ghoniem et al. (1999)).

8.7.5 Dislocation Junctions From the standpoint of the phenomenology of plastic deformation, one of the most important classes of three-dimensional conﬁguration is that associated with dislocation intersections and junctions. As will become more evident in our

8.7 Three-Dimensional Dislocation Conﬁgurations

431

Fig. 8.43. Two different competing geometries (courtesy of D. Rodney): (a) Two dislocations with Burgers vectors b1 and b2 and (b) junction case in which the junction segment has Burgers vector b1 + b2 .

discussion of work hardening (see chap. 11), dislocations on one glide plane can pierce the glide plane of another slip system, with the result that the gliding dislocation must pass through a ‘forest’ of obstacles. From our present perspective, we are interested in examining the geometric and energetic characteristics of the intersection of two such dislocations. Our arguments will begin in generic terms with the aim being an overall assessment of the structure and energetics of dislocation junctions with special reference to the stress needed to break them. The simplest picture of junction formation is largely geometric and relies on the line tension approximation introduced earlier. Perhaps the most fundamental insight to emerge from these studies is the conclusion that the stress to break such junctions scales as (arm length)−1 . Important discussions of the line tension approach may be found in Saada (1960) and Hirth (1961). The basic idea concerning the structure of junctions is the assessment of the energetics of two competing states, one in which the two parent dislocations (with Burgers vectors b1 and b2 ) remain unattached and the other in which the two parent segments join along the line of intersection of the relevant slip planes to form a new dislocation segment with Burgers vector b1 + b2 . The competition being played out here in three dimensions is much like its two-dimensional analog in which a perfect dislocation dissociates to form two partial dislocations bounding a stacking fault. The two competing geometries are illustrated in ﬁg. 8.43. For the purposes of examining the energetics of junction formation, we will concentrate on a highly symmetric geometry such that the arm lengths l1 and l2 are equal, and similarly, such that the angles φ1 and φ2 between the two dislocations and the line of intersection of the two relevant glide planes are equal. Within the conﬁnes of this

432

8 Line Defects in Solids

Fig. 8.44. Schematic of the behavior of the arms of a dislocation before and after junction formation.

geometric setup the energy of the state in which the two lines have not formed a junction is given by 1 1 E lines = 2 µb12l0 + 2 µb22l0 . (8.113) 2 2 Similarly, within the line tension approximation, the energy of the state in which a junction of length l j has formed is given by 1 1 1 E junction = 2 µb12l1 + 2 µb22l1 + 2 µ|b1 + b2 |2l j . (8.114) 2 2 2 Because of the choice of the highly symmetric geometry, the junction geometry is characterized by a single parameter. In particular, the parameters l j and l1 may be rewritten purely in terms of the angle φ1 and the initial arm length l0 . These geometric relations are illustrated in ﬁg. 8.44. What we note is that by the law of sines, l j and l1 are given by lj =

sin(φ1 − φ0 ) l0 , sin φ1

(8.115)

sin φ0 l0 . sin φ1

(8.116)

and l1 =

Further, we choose a conﬁguration in which |b1 | = |b2 | = |b1 + b2 |, corresponding to the three edges of one of the faces of the Thompson tetrahedron. The signiﬁcance of this geometric choice is that it guarantees that the line tensions of all three dislocation segments of interest will be equal. To examine the structure and energetics of junction formation from the line tension perspective, we now seek the equilibrium angle φ1 corresponding to a given

8.7 Three-Dimensional Dislocation Conﬁgurations

433

Fig. 8.45. Dimensionless length of junction within the line tension approximation as a function of the initial angle.

choice of initial angle φ0 and arm length l0 . The equilibrium condition is equivalent to ﬁnding the energy minimizer, which for the symmetric geometry considered here results in a one-parameter optimization problem. From above, we note that the energy change relative to the junction-free state is given by E = E junction − E lines = 2µb2

sin φ0 sin(φ1 − φ0 ) l0 + µb2 l0 − 2µb2l0 , (8.117) sin φ1 sin φ1

where l j and l1 have been eliminated in favor of φ1 and we have used the fact that the magnitude of all relevant Burgers vectors are equal. If we now seek equilibrium with respect to the angle φ1 , we are led to the equilibrium condition sin φ0 1 ∂E = (−2 cot φ1 + cosec φ1 ) = 0. 2 µb l0 ∂φ1 sin φ1

(8.118)

Solution of this equation leads to the conclusion that for this particular choice of Burgers vectors (i.e. the Lomer–Cottrell junction) the equilibrium angle is 60◦ . Using this result, and in light of eqn (8.115), we can now plot the junction length as a function of initial angle, namely, π sin − φ0 lj 3 . (8.119) = π l0 sin 3 The result is plotted in ﬁg. 8.45.

434

8 Line Defects in Solids

(a)

(b)

Fig. 8.46. Junction results from atomistics as computed using atomic-level analysis (adapted from Rodney and Phillips (1999)).

Atomistic Models of Dislocation Junctions. As noted above, the line tension approximation is largely geometrical and it is clear that an assessment of the accuracy of these ideas can be addressed from an atomistic perspective. One of the questions that one hopes to address from the atomistic perspective is the extent to which dislocation core effects (including the presence of dislocation splittings) alter the basic picture set forth in the line tension approximation. In keeping with the arguments given above, we continue to consider the geometry of the junction in which |b1 | = |b2 | = |b1 + b2 |. When carrying out an atomistic calculation of a problem of this type, it is obviously necessary to impose some choice of boundary conditions. Often, the imposition of such boundary conditions has unwanted side effects, and that is the case thus far with regard to the structure and energetics of junctions. Fig. 8.46 shows a sequence of snapshots in the deformation history of a junction in fcc Al as computed using pair functionals of the embedded-atom variety. Fig 8.46(a) illustrates the junction geometry in the presence of zero applied stress, while ﬁg. 8.46(b) illustrates the evolution of the junction in the presence of an applied stress. Linear Elastic Models of Junction Formation. Yet another scheme for addressing the structure and energetics of dislocation junctions is using the machinery of full three-dimensional elasticity. Calculations of this type are especially provocative since it is not clear a priori to what extent elastic models of junction formation will be hampered by their inability to handle the details of the shortest range part

8.8 Further Reading

435

Fig. 8.47. Lomer–Cottrell junction as computed using three-dimensional elasticity representation of dislocation dynamics (adapted from Shenoy et al. (2000)).

of the dislocation–dislocation interaction. It is important to emphasize that these calculations include far more physics than do their line tension counterparts since within the elasticity framework the interactions between the various segments are taken into account. The calculations to be considered here, shown in ﬁg. 8.47, are built around a linkage of the type of dislocation dynamics models set forth earlier in the context of Frank–Read sources and the ﬁnite element method which is used to discretize the dislocation lines themselves. In addition, this elastic model explicitly treated the interaction energies (and corresponding forces) that arise from the presence of stacking faults.

8.8 Further Reading The entire series Dislocations in Solids edited by F. R. N. Nabarro, North Holland Publishing Company, Amsterdam: The Netherlands is replete with articles pertinent to all aspects of dislocations (and many other topics as well). Many of those articles are relevant to the discussion advanced here. In particular, with reference to the crystallographic aspects of dislocations and the complex dislocation arrangements that occur in three dimensions I strongly recommend the article by S. Amelinckx in volume 2.

436

8 Line Defects in Solids

Dislocations by J. Friedel, Pergamon Press, Oxford: England, 1964. One of the great classics in the ﬁeld, what makes Friedel’s book particularly appealing is that almost every time a new theoretical construct is introduced, it is done so with reference to a particular experimental question in mind. ‘Dislocations and Walls in Crystals’ by J. Friedel in Physique des D´efauts/Physics of Defects edited by R. Balian et al., North Holland Publishing Company, Amsterdam: The Netherlands, 1980 makes for very interesting reading as Friedel revisits the theory of dislocations after a twenty-year interlude. I recommend this article very highly. Dislocation Based Fracture Mechanics by Johannes Weertman, World Scientiﬁc, Singapore: Singapore, 1996. What I ﬁnd especially engaging about this book is its idiosyncratic treatment of a number of problems. Weertman shows repeatedly how in adopting the notion of dislocation solutions as being fundamental, many interesting concepts may be explained concerning cracks and dislocations. Introduction to Dislocations by D. Hull and D. J. Bacon, Butterworth-Heinemann Ltd, Oxford: England, 1984. Ostensibly, this book is aimed at an audience uninitiated in the subject of dislocations. However, this may be deceptive since there are a variety of interesting discussions that are of interest even to seasoned veterans. Theory of Dislocations by J. P. Hirth and J. Lothe, Krieger Publishing Company, Malabar: Florida, 1992. The classic treatise on the mathematical theory of dislocations. This is always the ﬁrst place I look when I want to ﬁnd out something about dislocations. Mathematical Theory of Dislocations and Fracture by R. W. Lardner, University of Toronto Press, Toronto: Canada, 1974. This book treats a variety of interesting problems in dislocation theory without shying away from mathematically sophisticated treatments using the elastic Green function. A reference that I return to repeatedly. Thermodynamics and Kinetics of Slip by U. F. Kocks, A. S. Argon and M. F. Ashby, Pergamon Press, Oxford: England. This book is volume 19 of the series Progress in Materials Science, edited by B. Chalmers, J. W. Christian and T. B. Massalski. This book reﬂects the considerable knowledge of three leaders in the ﬁeld. One of the key features that makes the book so useful is that rather than concentrating on elastic solutions it considers how dislocations give rise to observed macroscopic behavior. Micromechanics of Defects in Solids by T. Mura, Kluwer Academic Publishers, Dordrecht: The Netherlands, 1993. A highly nonconventional treatment of

8.9 Problems

437

dislocations built around the idea of eigenstrains. This perspective is quite valuable in that it calls special attention to the lattice invariant shears that make such defects possible. ‘Dislocations in Particular Structures’ by S. Amelinckx from the 1979 volume of Dislocations in Solids is an incredible achievement in which Amelinckx considers the peculiarities of dislocations that attend particular crystal structures. A truly incredible article!

8.9 Problems

1 Microscopic description of the ideal shear strength Use the Morse pair potential constructed in chap. 4 to compute the periodic energy proﬁle for sliding one half-space relative to another for the fcc crystal. In particular, consider the sliding of adjacent (111) planes along the [110]-direction. Make a plot of this periodic energy proﬁle and include for comparison the Frenkel sinusoid for the same slip system. You will need to be careful to insure that your program computes the distribution of neighbors of an atom of interest to large enough distances. Also, multiply your potential by some rapidly decaying function at large distances so as to eliminate the artifact of atoms going in and out of the cutoff radius.

2 Displacements associated with an edge dislocation In this chapter we derived the strain ﬁelds associated with an edge dislocation. In this problem your goal is to derive the displacement ﬁelds implied by those strains and to use them to generate a projected atomic view of an fcc lattice with such a dislocation. (a) Using the strains for an edge dislocation, derive an expression for the displacements associated with such a dislocation. Hint: You will want to integrate the strains with respect to speciﬁc variables, but bear in mind that when you integrate with respect to x, for example, you still have an unknown function of y that is unspeciﬁed. (b) Consider the fcc crystal with a conventional perfect edge dislocation with a line direction of the type [112]. Use the displacement ﬁelds to generate a plot of the displaced atoms resulting from the Volterra solution. Explain why the picture results in the addition of two additional planes of atoms.

438

8 Line Defects in Solids

3 Asymptotic ﬁelds for dislocation dipoles In this problem, our aim is to investigate the far ﬁelds produced by a dislocation dipole. For simplicity, begin by considering two screw dislocations, both situated on the x-axis at positions (δ, 0) and (−δ, 0). (a) Using linear superposition of the ﬁelds due to these two screw dislocations, write an analytic expression for the ﬁelds at an arbitrary position (x, y). Comment on how the solution depends upon the relative signs of the Burgers vectors at these two dislocations. (b) Consider both the case in which the dislocations have opposite signs and that in which they have the same signs, and ﬁnd the leading order expansion for the far ﬁelds for both components of the stress tensor (i.e. σx z and σ yz ) in terms of the parameter δ. Note the enhanced decay rate of the stresses with distance in the case in which the dislocations have opposite signs. Further, observe that for the case in which the dislocations have the same sign, the far ﬁeld behavior is equivalent to that of a single dislocation with Burgers vector 2b. (c) Make your observations from the end of the previous part of the problem concrete by making a plot of the far ﬁelds for the case in which the signs of the two dislocations are the same. In particular, plot the exact stress ﬁeld for this dipole conﬁguration (which you know from part (a)) and that of a dislocation with Burgers vector 2b. Make your plot with respect to the dimensionless parameter r/δ and for a line at 45◦ with respect to the x-axis.

4 Edge dislocation ﬁelds using the elastic Green function This problem is a bit nasty, but will illustrate the way in which the Volterra formula can be used to derive dislocation displacement ﬁelds. (a) Imitate the derivation we performed for the screw dislocation, this time to obtain the displacement ﬁelds for an edge dislocation. Use the Volterra formula (as we did for the screw dislocation) to obtain these displacements. Make sure you are careful to explain the logic of your various steps. In particular, make sure at the outset that you make a decent sketch that explains what surface integral you will perform and why. 5 Isotropic Line Tension We advanced the idea that the energy of a dislocation line could be written in a local approximation as E(θ)ds. (8.120) E line =

(a) Explain the meaning of ‘locality’ and reproduce the argument leading to

8.9 Problems

439

E(θ) given as eqn (8.70). (b) By averaging over all θ , derive a result for a θ -independent line energy. Compare this with the conventional use of 12 µb2 .

6 Bow-out in the Line Tension Approximation In this chapter, the bow-out of a dislocation segment of length a was derived on the basis of an isotropic line tension approximation. This derivation culminated in eqn (8.97). Derive this equation and its dimensionless counterpart by ﬁrst writing down the functional E[u(x)] and then deducing the corresponding Euler–Lagrange equation which will then be solved via separation of the resulting differential equation.

7 Energy of Curved Dislocation in Line Tension Approximation We wrote down the energy of a curved dislocation as L T 1 + u 2 (x)d x. E line =

(8.121)

0

The problem with this expression is that it assumes that the line can be parameterized in terms of x. In this problem I want you to write down a fully general version of this result such that the line can wander in any direction and we can still write the energy as an integral over the line. Hint: Consider a parameteric representation of the dislocation and write the arc length in terms of this parameter. Show that your new expression reduces to the expression given above in the case in which your curve is parameterized by x. In addition, sketch a winding line for which more than one part of the line corresponds to a given x (i.e. it has overhangs) and discuss why the form derived in this problem is still applicable while that given in the equation above is not.

8 Elastic Forces for Three-Dimensional Dislocation Conﬁgurations Use isotropic linear elasticity to compute the elastic forces of interaction between two dislocations oriented as: (a) two perpendicular screw dislocations, (b) two perpendicular edge dislocations.

9 Line Tension Model for Dislocation Junctions Reproduce the arguments culminating in eqn (8.119).

440

8 Line Defects in Solids

10 fcc Dislocation Core Structure using Pair Functional Description of Total Energy Using the Johnson potential, determine the structure of the dislocation core in an fcc material. Consider a conventional edge dislocation on the (111) plane ¯ line direction. For a computational cell use a large cylinder in with a [1¯ 12] which the atoms in an annular region at the edge of the cell are frozen in correspondence with the Volterra solution. 11 Displacements due to a Dislocation Loop In eqn (2.96) we obtained the displacements due to a distribution of eigenstrains. In this problem, show that the eigenstrain associated with a dislocation loop with Burgers vector b on a plane with normal n is given by 1 (8.122) i∗j = (bi n j + b j n i )δ(r · n). 2 By integrating eqn (2.96) by parts and substituting this experession for the eigenstrain into the resulting formula, show that the expression given in eqn (8.32) is recovered.

NINE

Wall Defects in Solids

9.1 Interfaces in Materials Much of materials science and engineering is played out at the level of a material’s microstructure. From a more reﬁned perspective, the quest to tune or create new microstructures may also be thought of as a series of exercises in interfacial control. Indeed, interfaces in materials are the seat of an extremely wide variety of processes ranging from the conﬁnement of electrons to the fracture of polycrystals. The character of the interfaces that populate a given material leaves an indelible imprint on that material’s properties. Whether we consider the susceptibility of a given material to chemical attack at its surfaces, the transport properties of complex semiconductor heterostructures, or the fracture of steels, ushered in by the debonding of internal interfaces, ultimately, interfaces will be seen as one of the critical elements yielding a particular material response. In some cases, the presence of such interfaces is desirable, in others, it is not. In either case, much effort attends the ambition of controlling such interfaces and the properties that they control. Until this point in the book we have concerned ourselves with defects of reduced dimensionality. The present chapter aims to expand that coverage by turning to two-dimensional wall defects. The analysis of these defects will serve as our jumping off point for the consideration of microstructures within materials. From the start, the notion of material interface will be broadly construed so as to encompass free surfaces which are the terminal interface separating a material from the rest of the world, stacking faults which are planar defects in the stacking arrangement of a given crystal, grain boundaries which separate regions with different crystalline orientations and the interfaces between chemically or structurally distinct phases. The plan of the chapter is to begin with an introductory commentary on the role of interfaces in materials. This will be followed by three primary sections which treat surfaces, stacking faults and grain boundaries in turn. 441

442

9 Wall Defects in Solids

9.1.1 Interfacial Conﬁnement One organizing paradigm for examining the signiﬁcance of material interfaces is to think of them in terms of their role in producing conﬁnement. For the purposes of the present discussion, conﬁnement refers to the localization of some process or object either to the vicinity of the interface itself, or to a region that is bounded by such interfaces. In this section, we will consider examples of such conﬁnement in the context of elastic waves, which in certain cases are conﬁned to the vicinity of interfaces (i.e. Rayleigh and Stoneley waves), mass transport, in which interfaces serve as short-circuit diffusion paths and sinks for chemical impurities, and as impediments to dislocation motion, thus conﬁning plastic action to certain favorably oriented grains. Finally, we will note the signiﬁcance of internal interfaces in their role in providing a localizing pathway for fracture. Interfacial Conﬁnement of Mass and Charge. One of the key forms of conﬁnement induced by interfaces is associated with mass transport. What we have in mind is the localization of the diffusion process to the immediate vicinity of the interface in question. In particular, the presence of interfaces can lead to wholesale alteration of the rate at which processes involving mass transport transpire with a huge enhancement in the rate of diffusion along interfaces relative to bulk values. The macroscopic evidence for this claim is presented in ﬁg. 9.1 in which the rate of diffusion is shown not only for the bulk processes considered in chap. 7, but also for the short-circuit diffusion pathways presented by dislocation cores, free surfaces and internal interfaces. The origins of such phenomena are the conﬁning properties of interfaces with respect to point defects such as vacancies and substitutional impurities. As will be seen in more detail later, the structure of interfaces (whether surfaces or internal interfaces) reduces the barrier to the activated processes that occur during diffusion. From the standpoint of the analytic machinery set up in chap. 7, these short-circuit diffusion pathways are characterized by an activation energy for diffusion that is smaller than that found in the bulk. In addition to the role of interfaces in serving as a conduit for easy diffusion, the chemical potential proﬁle near such interfaces also makes them an ideal sink for point defects. The existence of such sinks leads in turn to the emergence of precipitate-free zones, local regions near grain boundaries characterized by the conspicuous absence of second-phase particles such as those that riddle the remainder of the material which is more distant from boundaries. An example of this phenomenon is depicted in ﬁg. 9.2. Again, the explanation for this behavior is the argument that because of the strong driving force which encourages foreign atoms in the vicinity of boundaries to diffuse to those boundaries, these foreign atoms are unavailable to participate in the nucleation and growth of second-phase particles.

9.1 Interfaces in Materials

443

Fig. 9.1. Diffusion data revealing the alteration in diffusion rates as a result of short-circuit pathways provided by interfaces and other defects such as dislocations (adapted from Gjostein (1972)).

Fig. 9.2. Illustration of a precipitate-free zone in a Cr-3 at.% Nb alloy (courtesy of Sharvan Kumar). The grain boundary runs from left to right through the middle of the picture, and reveals the existence of Cr2 Nb precipitates along the boundary itself and in the Cr matrix and the absence of such precipitates in a band near the boundary.

444

9 Wall Defects in Solids

In addition to their role in conﬁning mass, in some cases interfaces also have the effect of conﬁning charge to certain regions. As will be discussed in greater detail below, one of the most signiﬁcant types of internal interface is that representing a boundary between chemically distinct phases. Such interfaces play a pivotal role in modern microelectronics, and can be understood in part as a result of their role in serving as potential barriers for electronic properties. In chap. 3, the problem of conﬁnement in this context was evident in our solution of both the particle in the box and the quantum corral. Our interest at this juncture is to call attention to three-dimensional analogs of those systems, with special emphasis on the ways in which the internal interface serves as such a potential barrier which can have the effect of conﬁning electrons. Interfacial Conﬁnement of Waves. A knowledge of the complex interactions between waves and interfaces is at least as old as the ﬁrst explanation of Snell’s law of refraction on the basis of the wave theory of light. Indeed, with the further insight that upon passing from a medium with larger index of refraction to one with a smaller index of refraction, light could suffer total internal reﬂection, we see the roots of the ideas of interest to the current discussion. Not only do interfaces serve as the basis of conﬁnement in the context of electromagnetic waves, but they similarly alter the behavior of elastic waves. As was already discussed in chap. 5, the theory of linear elasticity may be used in order to consider dynamics in solids, illustrating the possibility of elastic waves within a medium. From the perspective of bulk excitations, we have already seen (see section 5.3.1) the formalism involving the acoustic tensor, and the subsequent propagating solutions. This earlier work may be generalized to consider waves at interfaces. Such waves have been dubbed Rayleigh waves in the context of those elastic waves conﬁned to surfaces, and Stoneley waves for the case in which such propagation is conﬁned to internal interfaces. The basic argument is that the equations of elastodynamics already highlighted in eqn (5.55), for example, admit of solutions not only in the bulk context, but also those localized to a region near the interface of interest. To see this, a trial solution to the equations of elastodynamics of the form u i (x, t) = Ae−γ z ei(k·r−ωt) ,

(9.1)

is considered. The key feature of this trial solution is its property that the displacement ﬁelds decay in the direction z perpendicular to the interface substantiating the claim that the wave amplitude is nonzero only in the vicinity of the interface. Interfacial Conﬁnement of Plasticity and Fracture. From the perspective of the mechanical properties of materials, interfaces are key players as a result of their unequivocal role in dictating mechanical response. The role of such interfaces in

9.1 Interfaces in Materials

445

Fig. 9.3. Pile up of dislocations against a grain boundary in Ti (courtesy of Ian Robertson).

mechanical response is perhaps most evident in the context of intergranular fracture in which the crack path follows the grain boundaries. As the crack propagates, it traverses the medium in a manner such that it is internal interfaces themselves that are the victims of bond breaking. Such fracture processes jibe with our contention that by virtue of interfaces, there is a conﬁnement of processes to a spatial region localized about these interfaces. However, internal interfaces can manifest their presence in the mechanical properties of materials in more subtle ways. In particular, in the context of plasticity in polycrystals, grain boundaries serve as obstacles to dislocation motion, leading to either dislocation pile-ups or grain boundary absorption of these dislocations. An example of the piling up of dislocations against a grain boundary in Ti as revealed by transmission electron microscopy is shown in ﬁg. 9.3. The detailed accounting for the elastic ﬁelds associated with such pile-ups as well as their implications for plastic deformation is given in chap. 11, whereas at present we only wish to remark upon the obstacle to dislocation motion offered by the presence of interfaces.

446

9 Wall Defects in Solids

In the discussion given above, we have illustrated the sense in which interfaces can alter material properties. The entirety of all interfaces found within a given material forms one of the key backbones of that material’s microstructure. Indeed, much of the actual business of microstructural control takes place at interfaces, either by eliminating them through processes such as grain growth, or by intentionally creating them such as in processes like the carburization of steel. Having motivated the idea of the importance of material interfaces, we will begin our analysis of interfaces in much the same way we treated point and line defects. Our analysis will begin by examining interfacial phenomena from a geometric perspective with an attempt to consider not only the geometry at the level of atomic positions, but also with regard to the macroscopic geometries associated with interfaces. Particular attention will be directed ﬁrst towards surfaces which are largely the point of communication between a crystal and the external world. Once the geometric and energetic preliminaries have been dispensed with, the discussion will lead in the direction of increasing geometric complexity as we confront ﬁrst, the reconstructions that attend many surfaces, and then the step features and roughening that are present on most real surfaces. Surfaces will be followed by a discussion of stacking faults and twin boundaries. The point of this part of the discussion will be to examine how the structure and energetics of such interfaces may be determined, and once such features are known, how they may be used to provide insights into observed material behavior. Stacking faults and twins may perhaps be thought of as the least severe of internal interfaces in that they represent the smallest departure from the monotony of the perfect crystal. After having examined the fascinating structural polytypes that can occur as a result of repeated ‘mistakes’ in the packing sequence of various crystal planes, we will take up the geometric and energetic features of grain boundaries. Our discussion on grain boundaries will commence with bicrystallography. However, the ultimate aim of these conceptual notions will never be far from the fore: an analysis of grain boundaries should leave us poised to tackle the more difﬁcult problem of the structure and energetics of polycrystals.

9.2 Free Surfaces The crystal surface is the seat of the vast majority of interactions that take place between a material and the rest of the world. Catalysis, crystal growth, and degradation via corrosion are but a few of the key processes that take place at surfaces. In each case, it is the interaction between a crystal on the one hand and the atoms arriving at the surface on the other that leads to the properties of interest. Another way in which the crystal surface has emerged as one of the key players in the study of solids is by virtue of the recent development of a number

9.2 Free Surfaces

447

of experimental probes which allow the direct observation of the behavior in the vicinity of the surface. In addition to their importance to the enterprise of materials science itself, surfaces have been one of the central proving grounds in the quest to construct a viable computational materials science. Because of the experimental capacity for explicit determination of surface structure, many calculations have been aimed at establishing the nature of the atomic-level geometries that occur on a given surface. With the increasing sophistication of experimental and theoretical tools alike, not only have the geometries of an increasing number of metal, semiconductor and ceramic surfaces been determined unambiguously, but also a rich variety of new phases associated with adsorbates, islands and steps have been uncovered. Our starting point for the analysis of this class of problems will be to consider the structure and energetics of ideal crystal surfaces.

9.2.1 Crystallography and Energetics of Ideal Surfaces From a geometrical perspective, if one imagines terminating a crystal on some particular crystal plane, there is a well-deﬁned and unambiguous idealized geometry. By this we mean that by virtue of the simple conceptual act of terminating the repeated packing of crystal planes along a particular direction, we are left with an exposed surface whose structure is determined unequivocally by the particulars of the underlying crystal lattice. We adopt the standard characterization of the crystallographic features of such a surface by exploiting the Miller indices. Stated simply, the Miller indices of a given surface are determined by ﬁrst noting the points of intersection of the surface of interest and the Cartesian axes. These numbers are then inverted and multiplied by an appropriate integer such that all three fractions have been converted into integers. These integers are the Miller indices. For the purposes of the present argument, our intention is to convey a sense of the structure and energetics of ideal surfaces. The single most obvious feature of these geometries is the loss of neighbors to those atoms at the surface. In the case of a covalent material, such as Si, this loss will be most signiﬁcant as a result of the formation of dangling bonds in which the Si atom is left with fewer neighbors than is energetically favorable. Clearly, the creation of such surfaces has energetic consequences. As a starting point for our foray into the energetics and motion of surfaces, we will consider the energetics of such idealized geometries. These calculations will serve as our point of departure for more elaborate analyses involving reconstructions, surface steps and islands. For the sake of physical transparency, our calculations will begin on the basis of an idealized pair potential model. Once these calculations are in hand, a more general

448

9 Wall Defects in Solids

Fig. 9.4. Schematic of the (100) surface of an fcc crystal. Filled circles correspond to atoms on the top layer, open circles are those one layer beneath the surface.

discussion of computing surface energies will be undertaken, ﬁrst with respect to pair functionals, and then through consideration of the general concepts appropriate to all energetic descriptions. Our endeavor to uncover the energetic features of surfaces begins with a pair potential description. For convenience, we leave the speciﬁc details of the pair potential unspeciﬁed, noting only that the total energy of the solid is written as E tot =

1 V (Ri j ). 2 ij

(9.2)

Further, we restrict our attention to the simpliﬁed analysis in which it is assumed that only near-neighbor interactions contribute to the energy. Consider a slab of fcc material with periodic boundary conditions in two of the three Cartesian directions, and exposed (100) surfaces in the third direction with a geometry like that shown in ﬁg. 9.4. For concreteness, we imagine a total of N atoms in the slab with m atoms per layer. Once we have adopted the pair potential mindset, which will be our temporary preferred mode of thought, the determination of the surface energy is reduced to little more than a proper accounting of the number of bonds lost by those atoms in the vicinity of the surface. In this case, it is only those atoms on the surface itself that suffer any reduction in coordination number and hence have an altered energy. In particular, consideration of ﬁg. 9.4 reveals that surface atoms on the fcc (100) surface are deprived of four neighbors. As a result of this argument, the total energy of the slab of atoms is given by E tot = 6(N − 2m)V (Rnn ) + 8mV (Rnn ),

(9.3)

where the ﬁrst term on the right hand side corresponds to bulk atoms that are not

9.2 Free Surfaces

449

disturbed by the presence of the free surface, while the second term corresponds to the 2m atoms participating in the two free surfaces. One of the key linkages between continuum and microscopic descriptions of interfaces is the notion of an interfacial energy. Though the use of such energies is by now entirely routine, nevertheless, this exempliﬁes the type of information passage that is one of the hallmarks of multiscale modeling. Note that from the perspective of the continuum mechanics of materials with interfaces, the total energy is often written in the form W (F)d V + γ (n)d A, (9.4) E tot =

∂

where F is the deformation gradient and W (F) is the strain energy density accounting for the energy of bulk deformation and where we have included the possibility of an anisotropic surface energy through the dependence of the surface energy γ on the surface normal n. The question of current interest is the microscopic origins of such a surface energy. On the basis of the total energy for the slab considered above, we are in a position to evaluate the surface energy. The key point is that the surface energy is computed by evaluating the difference between the N -atom system including the free surfaces and that of N atoms in the perfect crystal, and then dividing by an area factor that reﬂects the amount of exposed surface. For the case of the (100) surface, this amounts to E N (surface) − E N (bulk) , (9.5) 2A where the factor of 2 in the denominator accounts for the fact that there are two exposed faces on the slab under consideration. Our notation calls for the energy of the N -atom system in the presence of free surface (i.e. E N (surface)) and the energy of an N -atom bulk solid (i.e. E N (bulk)). In this case, E N (surface) is given by eqn (9.3), while E N (bulk) = 6N V (Rnn ), our result for the energy of an fcc crystal in a near-neighbor pair potential approximation. Hence, we ﬁnd that the surface energy is given by √ 4V (a0 / 2) γ100 = − . (9.6) a02 γ100 =

Note that in deducing this result we have not allowed for the possibility of structural relaxations that might occur for surface and near-surface atoms. The type of calculation illustrated above can be elaborated by appeal to more sophisticated descriptions of the total energy. Regardless of choice of energy function, the fundamental concept is embodied in eqn (9.5). In preparation for our discussion of surface reconstructions, we will generalize the description given above to the case of pair functionals such as the embedded-atom method. We adopt

450

9 Wall Defects in Solids

the Johnson-type embedded-atom functions already described in chap. 4 which permit analytic progress in the context of questions such as that raised here. Recall that in this case, our task is to supplement the pair potential description of the surface energy (already deduced above) with the contribution due to the embedding energy. Following the discussion from chap. 4, recall that within a pair functional description the energy takes the form, 1 F(ρi ) + φ(Ri j ), (9.7) E tot = 2 ij i where the former term is the embedding energy and is a function of the density at site i (i.e. ρi ). The density at site i may be deduced in turn according to f (Ri j ), (9.8) ρi = j

where the function f (R) yields the contribution to the density at site i from a neighbor at a distance R. We will denote f (Rnn ) = ρnn , with the result that the energy of N atoms in a bulk fcc environment is given by E N (bulk) = N F(12ρnn ) + 6N φ(Rnn ). As with our evaluation of the surface energy in the strictly pair potential setting, the pair functional assessment of the total energy can be obtained essentially on the basis of bond counting. Again, if we assume a near-neighbor model in which not only is the pair potential range restricted to near neighbors, but so too is the function determining the electron density, then only atoms that are at the surface itself have environments that are distinct from the bulk. In particular, the total energy of the N -atom system in which there are two exposed (100) surfaces is given by, E N (surface) = (N − 2m)F(12ρnn ) + 6(N − 2m)φ(Rnn ) + 2m F(8ρnn ) + 8mφ(Rnn ),

(9.9)

where we have used the same geometry as that considered in the pair potential calculation. The ﬁrst two terms on the right hand side arise from the bulk atoms, while the second two terms reﬂect the presence of the free surface atoms. If we imitate the strategy used above in the pair potential context, it is found that the surface energy is given by γ100 =

2[F(8ρnn ) − F(12ρnn )] − 4φ(Rnn ) . a02

(9.10)

To put these expressions in perspective, we now examine the types of numerical values they imply for fcc surfaces. Using the analytic potentials of Johnson introduced in chap. 4, the surface energies of fcc Cu are γ111 = 0.99 J/m2 ,

9.2 Free Surfaces

451

γ100 = 1.19 J/m2 and γ110 = 1.29 J/m2 , which are nearly identical to the experimental values for this system, although we should recall that the potentials are ﬁtted to a number of important properties, though not the surface energies themselves. These results for the energy of free surfaces represent the ﬁrst in a hierarchy of interfacial energies that will be discussed in this chapter. As was already hinted at above, interfaces in solids come in a number of different forms resulting in several different energy scales. At the low end of the energy spectrum are the energies of twin boundaries and stacking faults. These are followed by the energies of grain boundaries which are superseded by the even higher energies associated with free surfaces. In the preceding parts of this section, our emphasis has been on the fundamental ideas associated with the energetics of ideal surfaces. Before embarking on the reﬁnement of our arguments to the consideration of surface reconstructions, we close this section with a few details related to the use of microscopic analysis to analyze in a systematic way the energies of free surfaces. First, we reiterate the importance of eqn (9.5), which is the basis of surface energy calculations whether one uses the lowliest of pair potentials or the most sophisticated ﬁrst-principles techniques. On the other hand, the details of implementation can differ depending upon the situation. One of the critical questions that must be faced when using more computationally expensive techniques is the thickness of the computational slab. On the one hand, one aims for carrying out such calculations using the fewest number of atoms possible. By way of contrast, failure to use a thick enough computational cell will result in interactions between the two surfaces. As with many of the ﬁrst-principles calculations that we have already described, there are a series of generic issues that must be faced in making a systematic analysis of features such as the surface energy. One useful class of calculations examines trends in important material parameters such as the surface energies. A systematic analysis of the surface energies of 60 metals has been carried out by Vitos et al. (1998) using a variant of the LMTO method. As we described in chap. 4, there are a number of different versions of the ﬁrst-principles solution to the Schr¨odinger equation which differ in the details of how they handle the ionic potential, the basis functions used to represent the wave function, and so on. The LMTO method is one of this set of methods. Periodic boundary conditions are employed with the added twist that vacuum layers separate surfaces along the stacking direction of interest. For example, in their analysis of fcc (111) surfaces, they use a slab that is four atomic layers thick with an associated vacuum layer that is two atomic layers thick. An example of the type of results that are obtained for the 4d transition metals is shown in ﬁg. 9.5. Note that as the number of d-electrons per atom (i.e. the band ﬁlling) increases, the surface energies exhibit a characteristic rise until the d-band is half-ﬁlled and then decline as the number

452

9 Wall Defects in Solids

Fig. 9.5. fcc (111) surface energies for 4d transition metals (adapted from Vitos et al. (1998)).

of d-electrons is further increased. This behavior is reminiscent of that associated with the cohesive energies reported in ﬁg. 4.18. Another way of representing the trends in surface energies is to examine the anisotropy in passing from one low-index surface to another. The surface energy anisotropy between the (100) and (111) surfaces is characterized by the ratio γ100 /γ111 . Fig. 9.6 reveals the surface energy anisotropies for the 4d transition metals where it is seen that there are systematic, but rather small, variations in the surface energy anisotropies. The discussion given above has concentrated on the energetics of metal surfaces. Though we could similarly enter into a description of the energetics of ideal semiconductor surfaces, such a discussion is much less revealing since in the case of semiconductor surfaces, the driving force for structural reconstruction is so high. As a result, we ﬁnd it convenient to await a discussion of semiconductor surfaces until we have introduced the next level of structural elaboration, namely, that of surface reconstructions.

9.2.2 Reconstruction at Surfaces The previous section highlighted the geometric aspects of surfaces that arise on carrying out the conceptual exercise of abruptly terminating the packing sequence along a given crystallographic direction. In the vast majority of cases, this ideal geometry is little more than a ﬁction and what is really found is a reconstructed geometry in which the atomic positions in the vicinity of the surface are distinct from those that are implied by merely truncating the crystal on a particular plane. Such reconstructions are the two-dimensional analog of the type of reconstructions

9.2 Free Surfaces

453

Fig. 9.6. Surface energy anisotropies for 4d transition metals (adapted from Vitos et al. (1998)).

described in the previous chapter as concerns dislocations in semiconductors (see section 8.6.3). The intention of this section is ﬁrst to provide plausibility arguments as to the origins of the structural rearrangements that attend the formation of free surfaces, several key examples of which are given in ﬁg. 9.7. The two key structural rearrangements to be considered here are: (i) structural relaxations in which the spacing between adjacent layers in the direction perpendicular to the surface is altered as is shown schematically in ﬁg. 9.7(a), and (ii) surface reconstruction in which there is a complete rearrangement of the surface geometry as shown schematically in ﬁgs. 9.7(b) and (c). In the case of these reconstructions, the symmetry of the surface can be completely altered relative to the bulk termination. Once we have spelled out the conceptual features of both surface relaxation and reconstruction we will give the particular details associated with a few different representative examples on both metal and semiconductor surfaces. We further idealize the discussion through the assumption that the various competing structures are thought of in a vacuum, since a further intriguing but difﬁcult complexity is introduced once foreign species are adsorbed on the surface. Plausibility Argument for Surface Relaxation. As already noted above, crystal surfaces are characterized by a wide range of structural rearrangements relative to the ideal surface. One such rearrangement is surface relaxation, with the entire surface layer moving either towards or away from the subsurface layers as shown

454

9 Wall Defects in Solids

Fig. 9.7. Schematic of some of the key rearrangement mechanisms at surfaces (adapted from L¨uth (1993)): (a) surface relaxation, (b) surface reconstruction and (c) missing-row reconstruction.

Fig. 9.8. Schematic illustrating the strengthening of back bonds at a free surface (adapted from Carlsson (1990)). Double and triple lines associated with surface atoms are meant to indicate the strengthening of bonds associated with those atoms that have lost neighbors due to the free surface.

in ﬁg. 9.7(a). One way to see the origins of this tendency is via the types of simple arguments we used earlier to justify the extra physics incorporated in pair functionals. In particular, we recall the essence of such models is in the fact that the bond strength is dependent upon the coordination number of the atom of interest. The coordination number dependence of the bond strength was illustrated in ﬁg. 4.5. In the context of free surfaces, as a result of the loss of neighbors to those atoms at the surface, there is a subsequent strengthening of back bonds between the surface atoms and their subsurface partners. This effect is indicated schematically in ﬁg. 9.8. Plausibility Argument for Surface Reconstruction. In addition to the types of relaxations discussed above, surfaces may also suffer massive rearrangements referred to as reconstructions. These reconstructions often represent a complete rearrangement of the underlying ideal geometry and may bear no resemblance to the subsurface structure. The crystallography of these symmetry breaking rearrangements is illustrated in ﬁg. 9.9. As is evident from the ﬁgure, there is some new notational baggage that goes along with the description of surface reconstructions. In particular, if we elect to denote the symmetry of the ideal

9.2 Free Surfaces

455

Fig. 9.9. Schematic of the symmetry changes that attend surface reconstruction for case of several surfaces (adapted from L¨uth (1993)).

surface in terms of two lattice vectors a and b, then the bulk termination of the surface is designated as having a (1 × 1) symmetry since the surface unit cell is bounded by the vectors a and b themselves. In the event that the surface undergoes a symmetry breaking reconstruction, the surface unit cell will be built up of larger multiples of the vectors a and b. In particular, if the surface unit cell is bounded by the vectors n 1 a and n 2 b, then the surface reconstruction is designated as the n 1 × n 2 reconstruction. Four distinct examples of this thinking are illustrated in ﬁg. 9.9 where frames (a) and (b) show a 2 × 2 reconstruction on a (100) surface, and frames (c) and (d) show examples from (111) surfaces. As we have already emphasized, the energy computed in the previous section is the ideal surface energy, and does not reﬂect the possible further energy reduction that attends a symmetry breaking surface reconstruction. On the other hand, we seek to understand the driving force towards such reconstruction in energetic terms. Perhaps the most immediate context within which to view the emergence of reconstructions is on semiconductor surfaces where simple arguments concerning

456

9 Wall Defects in Solids

Fig. 9.10. Representation of ideal and 2 × 1 reconstructed geometries for Si (001) (courtesy of Lloyd Whitman).

the necessity to saturate unfulﬁlled bonds give intuitive plausibility to such reconstructions. For example, in the case of the (001) surface in Si as depicted in ﬁg. 9.10, we see that the ideal surface is replete with dangling bonds. As in the case of the semiconductor dislocation cores discussed earlier, there is a driving force towards dimerization which has the effect of eliminating the dangling bonds through reconstruction. In particular, in this case we see that in the ideal 1×1 state, each surface atom has two dangling bonds. By virtue of the pairing up of adjacent surface atoms a 2 × 1 symmetry is induced which has the effect of reducing the number of dangling bonds on each atom. Computing Surface Reconstructions and Their Energies. Thus far, we have succeeded only in giving plausibility arguments for the emergence of reconstructions as structural competitors to the ideal bulk terminations. On the other hand, it is by now evident from preceding chapters that an analysis of the energetics and dynamics of such surfaces may be made through an appeal to the energetic methods of microscopic simulation. One difﬁculty faced in trying to carry out a systematic study of such reconstructions on the basis of energetic analyses is the biasing role played by the supercell dimensions. For example, if the overall lateral supercell size is 5 × 5, this implies that it is not possible to obtain structures with periodicities incommensurate with the underlying substrate, nor those structures with a surface unit cell larger than the 5 × 5 cell made available in the computation. One remedy to this difﬁculty is the construction of effective Hamiltonians from which it is possible to carry out not only much larger simulations, indeed with the

9.2 Free Surfaces

457

possibility for the emergence of long-period structures, but also to use the tools of statistical mechanics which in some cases allows for direct analytic progress to be made on the relevant Hamiltonian. We will give examples of this strategy in the pages that follow in the context of reconstructions on both the Au and W surfaces. Case Studies on Metal Surfaces We have already emphasized the revolution in surface science ushered in on the heels of high-quality vacuum technology and surface scanning probes. One subbranch of surface science that has been the beneﬁciary of these advances is the study of metal surfaces. The intention of this subsection is to consider two distinct case studies, namely, the surfaces of fcc Au and those of bcc W. These choices are inspired by the combination of high-quality experimental data, richness of surface phases, their diversity from the standpoint of the demands they place on atomistic simulation and their relevance to later generalizations to surfaces with steps, islands and even more extreme forms of roughness. Surface Reconstructions in Au. Gold is one of a number of systems that exhibits a wide range of fascinating surface reconstructions, which includes a host of orientational phases in the presence of steps. For our purposes, the Au system serves as a rich example not only for our arguments concerning surfaces and their reconstructions, but also as a basis for contrasting many of the different energetic arguments that have been set forth so far in the book. What we will ﬁnd is that the Au surfaces have been attacked from a wide variety of pair functional approaches, by recourse to ﬁrst-principles techniques and using different effective Hamiltonians. In fact, much of the theoretical effort on the Au(001) surface will be reminiscent of our earlier treatment of the Peierls–Nabarro model and treatments yet to come of cohesive zone models. Finally, the existence of a variety of X-ray, scanning tunneling microscopy and other experimental data makes the Au surfaces very appealing. For concreteness, we consider the (001) surface of Au. The unreconstructed geometry corresponds with the bulk termination along this direction and is nothing more than a square lattice, rotated at 45◦ with respect to the cubic directions. This geometry may be contrasted with a depiction of the reconstructed geometry, shown in ﬁg. 9.11. The key qualitative features of the reconstructed geometry are related, namely, a tendency towards close packing which is manifested as a nearly hexagonal arrangement of the surface atoms. As can be seen in the ﬁgure, the ideal bulk termination corresponds to the square grid, while the actual atomic positions form a pseudohexagonal arrangement. These structural insights have been garnered from a series of X-ray measurements as reported in Gibbs et al. (1990).

458

9 Wall Defects in Solids

Fig. 9.11. Reconstructed geometry for Au(001) surface (adapted from Gibbs et al. (1990)). The ﬁgure shows only the surface layer of atoms.

Fig. 9.12. Sequence of phases associated with Au(001). At high temperatures, distorted hexagonal phases are superseded by disordered phase with 1 × 1 symmetry. RDH refers to rotated–distorted hexagonal phase, DH refers to distorted hexagonal phase and DIS refers to disordered phase. Note that the schematic of the rotated hexagon associated with RDH exaggerates the rotation. In addition, the orientation relationship between the hexagonal structures and the subsurface atoms is not represented.

The experimental data associated with this surface are actually more revealing than we have suggested (Gibbs et al. 1990, Abernathy et al. 1992). On the basis of systematic X-ray reﬂectivity studies, it has been deduced that a sequence of phases are found as a function of temperature: these phases are shown schematically in ﬁg. 9.12. In particular, two related pseudohexagonal phases have been found which differ by a small relative rotation in addition to a high-temperature disordered phase in which the pseudohexagonal symmetry is lost. However, despite the apparent abruptness and reversibility of the transition between the two distorted hexagonal phases, it remains unclear whether or not these structures constitute true equilibrium phases. The mission of any energetic methods that might be brought to bear on the structure of this surface is to explicate the origins of its tendency towards close-packing, even at the cost of abandoning its epitaxial relationship with the subsurface layers. Our strategy is to contrast pair functional and ﬁrst-principles approaches to this reconstruction. In addition, we will examine the way in which ﬁrst-principles calculations may be used to construct an effective Hamiltonian for

9.2 Free Surfaces

459

this system and through which the competing inﬂuences governing the transition become more clear. A repeating theme that has been played out in modeling defects ranging from vacancies and interstitials, to dislocation cores and surface reconstructions is that of successive approximation. Often, the ﬁrst treatment of a new problem is put forth from the perspective of some empirical description of the total energy. The Au(001) surface is no different. The initial efforts to uncover the origins of this reconstruction were built on pair functional descriptions of the total energy (Ercolessi et al. 1986, Dodson 1987, Wang 1991). The argument was made that by virtue of the embedding term, the complex interplay of in-plane densiﬁcation and subsurface pinning could be considered. An example of the type of results that emerge from such simulations is shown in ﬁg. 9.13. The basic idea of the simulations was to construct a slab with some ﬁnite size and associated periodic boundary conditions. Note that the selection of a particular periodicity in the in-plane directions rules out symmetry breaking distortions whose periodicities (if any) are larger than these cells. The geometries are then relaxed, usually via some ﬁnite temperature annealing scheme (Monte Carlo or molecular dynamics) and are slowly cooled until the resulting energy minimizing conﬁguration is determined. The claim has been made that by carrying out molecular dynamics calculations at a sequence of increasing temperatures, pair functional schemes are sufﬁciently accurate to capture the series of transitions that are observed with increasing temperature. This claim is substantiated by appeal to calculations of the structure factor which provides a geometric signature of the surface geometry. Inspection of the results of such pair functional calculations of the Au(001) reconstructed geometry reveal a marked tendency towards the close-packed distorted hexagonal structures implied by experiment, though the precise surface periodicity probably remains out of reach of these methods. More accurate ﬁrst-principles calculations have also been undertaken with respect to the Au(001) reconstruction (Takeuchi et al. 1991). These calculations were conceptually identical in all essentials to those carried out using the pair functional description of the total energy. However, an important added feature was the additional task of considering the isoelectronic Ag system, with the aim of examining why the (001) surface of Au reconstructs while that of Ag does not. Further, by treating the subsurface layers of the Au crystal as a uniform electron gas, the ﬁrst-principles analysis was able to separate the competition between the surface atoms increasing their coordination number and the subsurface atoms locking the surface atoms into crystallographic positions. The desire for both computational tractability and physical transparency suggests the usefulness of effective Hamiltonians. We have emphasized the desirability of ﬁnding degree of freedom reducing strategies in which only those degrees

460

9 Wall Defects in Solids

Fig. 9.13. Several views of the (34 × 5) Au(001) surface reconstruction as obtained using a pair functional description of the total energy (courtesy of Furio Ercolessi). The atoms in the ﬁrst layer are colored in gray scale according to their z-coordinates: the lighter the color the larger z. The second layer atoms are colored black.

of freedom of real importance to the physical question at hand are considered. The Au(001) surface features two competing energetic factors: (i) the in-plane energy gain associated with a local increase in coordination number and favoring

9.2 Free Surfaces

461

a close-packed hexagonal arrangement, (ii) the subsurface pinning potential which favors a locking in of the surface atoms into registry with those beneath the surface. This competition suggests an effective Hamiltonian of the form 2π xi 2π yi V (Ri j ) + A cos , (9.11) E tot ({Ri }) = + cos a a ij i where the set {Ri } characterizes the entirety of atoms on the surface. The ﬁrst term on the right hand side represents the in-plane interactions between neighboring atoms, and for our purposes should be thought of as a pair potential that favors a near-neighbor distance smaller than that determined by the bulk termination of the surface. In particular, this term inclines the surface atoms to a two-dimensional close-packing geometry. The second term is a lock-in term and characterizes the interaction between the surface atom with coordinates (xi , yi ) and the atoms beneath the surface which have been buried in this effective potential. Note that this pinning term carries exactly the same sort of information as the interplanar potential introduced in the context of the Peierls–Nabarro model, and similarly, exploits the same sorts of locality assumptions favored there. In addition to the general theme of degree of freedom reduction, we have noted the objective of information transfer in which calculations at one scale are used to inform those used at a different scale. In the current context, we refer to the use of ﬁrst-principles calculations to inform the effective Hamiltonian of eqn (9.11). Like with the treatment of the interplanar potential associated with the Peierls–Nabarro model, the coefﬁcient A in eqn (9.11) is obtained on the basis of rigid sliding geometries in which the surface layer is slid with respect to the subsurface layer and the resulting energy is computed. In this case, it is the difference in energy between the conﬁguration in which all atoms have their bulk-terminated in-plane positions and that conﬁguration in which all surface atoms have slid by the vector δ = (a/2, a/2). The potential determined in this way is shown in ﬁg. 9.14. As usual, once the effective Hamiltonian is in hand, it is possible to investigate its implications for the equilibrium phases of the system. In this case, the outcome of examining the equilibrium structure associated with this Hamiltonian is shown in ﬁg. 9.15. Surface Reconstructions in W. In earlier sections, we have noted that the pair functional formalism is not always appropriate as the basis for an energetic description of metals. One case where this is evident is in the context of the surface reconstructions seen on certain bcc transition metals. In particular, the (001) surface of both W and Mo exhibits fascinating reconstructions, and as in the case of the Au(001) surface, the symmetry breaking distortions leave few vestiges of their crystallographic ancestry.

462

9 Wall Defects in Solids

Fig. 9.14. Representation of interplanar potential characterizing the locking in of surface atoms to their subsurface partners.

Fig. 9.15. Minimum energy conﬁguration for Au(100) as obtained using the effective Hamiltonian deduced from ﬁrst principles (adapted from Takeuchi et al. (1991)).

The ideal (001) surface of crystals with the bcc structure is illustrated in ﬁg. 9.16(a). We note that the ideal termination of this surface is a square lattice with a lattice parameter equal to that associated with the bulk crystal itself. This geometry may be contrasted with that of the reconstructed geometry in W in ﬁg. 9.16(b). The surface geometry can be continuously altered from the ideal bulk termination to the reconstructed state by imposing a series of surface displacements

9.2 Free Surfaces

463

Fig. 9.16. Schematic of the ideal bulk termination and reconstruction associated with certain bcc (001) surfaces: (a) ideal bulk termination for (001) surface of bcc crystal, (b) (001) reconstruction of W. The amplitude of the reconstruction is exaggerated for ease in viewing. Dark circles correspond to surface layer atoms and gray circles are associated with atoms in ﬁrst subsurface layer.

of the form umn = u0 cos(q · Rmn ),

(9.12)

where mn is a label for√the atom √ at surface position Rmn = mai+naj, u0 is a vector of the form u0 = δ(1/ 2, 1/ 2) and characterizes the amplitude and direction of the surface distortion and q is a wavevector that characterizes the periodicity of the surface reconstruction itself. For the reconstruction of interest here, the wavevector q is of the form q = (π/a)(1, 1, 0). The reconstructed surface is characterized by two distinct phases, one with c(2 × 2) symmetry (below ≈ 210 K) and one with (1 × 1) symmetry above that temperature, with the high-temperature phase thought to be a disordered state rather than the ideal bulk termination. The low-temperature ˚ phase is characterized by lateral displacements δ ≈ 0.25 A. The (001) surface reconstructions of bcc metals have become something of a proving ground for new total energy schemes. Our discussion in chap. 4 of angular potentials considered the role of angular forces in stabilizing certain characteristic geometric features of bcc crystals, and these features are revealed again in the context of the reconstruction. Instability of the surface with respect to a distortion of wavevector q can be considered via a series of static calculations in which the energy is repeatedly computed for increasing δ. An example of calculations of this sort is shown in ﬁg. 9.17. We note that the basic strategy adopted here is one that has done service for us repeatedly in a wide range of contexts. The basic idea is to compute (either analytically or numerically) the energies for the putative unstable state and to determine whether in fact there is an energy reduction associated with

464

9 Wall Defects in Solids

Fig. 9.17. Energy as a function of reconstruction amplitude for W(100) reconstruction as computed using angular potentials (adapted from Carlsson (1991)). The ﬁgure reveals the importance of the angular term in stabilizing the reconstruction. The units of δ are measured in a˚ ngstroms.

such an instability. The dynamic analog of this procedure is to consider the growth of the presumed unstable state in time and if the state does grow, then this is seen as evidence of an instability of the reference state. In the present setting, an angular force scheme similar to that presented in section 4.4 was used to examine the energetics of reconstruction. As shown in ﬁg. 9.17, the energetics of this instability may be decomposed into the part emerging from pair terms (E el(2) + Er ep ) and that due to four-body angular terms (E el(4) ). The energy is plotted as a function of the reconstruction amplitude δr ec and reveals a minimum at a nonzero value signaling the propensity for reconstruction. Further, we note that the driving force leading to this reconstruction can be traced to the angular terms. As we have already seen a number of times, empirical calculations can be supplemented and even supplanted by their ﬁrst-principles counterparts. The reconstructions on (001) surfaces have been explained not only on the basis of angular force schemes, but also using density functional theory. In this case, it is a brute force reckoning of the electronic structure and the associated energies that is used to probe the instability toward surface reconstruction. An analog of ﬁg. 9.17 obtained using electronic structure calculations is shown in ﬁg. 9.18. One of the advantages of calculations of this sort is that they can provide insight into the electronic features giving rise to a given phenomenon. In the present context, an intriguing distinction was made between the isoelectronic partners W and Ta, with the insight that emerged being that the propensity for reconstruction could be ascribed to particular structure in the electronic density of states.

9.2 Free Surfaces

465

Fig. 9.18. Energy as a function of reconstruction amplitude as computed using density functional √ theory (adapted from Singh et al. (1986)). The parameter δ is given by δ = δact / 2a0 , where δact is the actual displacement magnitude and a0 is the lattice parameter.

The type of ﬁrst-principles analysis presented above can serve an additional purpose which is tied to the creation of effective theories. In particular, it has been found possible to construct an effective Hamiltonian which represents the energetics of various surface distortions. The perspective adopted here is that the ﬁrst-principles calculations are used to inform the higher-level effective Hamiltonian. Extra importance attaches to the construction of effective Hamiltonians in cases like this since the use of ﬁrst-principles methods by themselves does not allow for a systematic investigation of the ﬁnite temperature aspects of the structural transformation. In particular, in the case of the W(001) surface of interest here, it is of interest to explore the nature of the structural transition at around 210 K. In the present setting, the functional form advanced for the effective Hamiltonian is

1 1 4 1 1 2 4 2 2 Au + Bu i + V4 u i cos(4θi ) + A z (z i − z 0 ) + Vz u i z i Heff = 2 i 4 2 2 i + [J1 ui · u j + K 1 Si j (u i x u j x − u i y u j y ) + R1 [u i x u j x (u i2x + u 2j x ) i j1

+ u i y u j y (u i2y + u 2j y )] +

J2 ui · u j .

(9.13)

i j2

There is a variety of notation associated with this model which includes the use of ui to represent the in-plane displacement of atom i, z i to represent the out-of-

466

9 Wall Defects in Solids

plane displacement of atom i, u i x as the x component of displacement of the i th atom, i jk to denote summing over k th neighbor pairs and the use of a variety of energetic coefﬁcients such as A, B, V4 , A z , Vz , J1 , J2 , R1 and K 1 . In addition, Si j is 1 if sites i and j are displaced from each other in the x-direction and −1 if they are displaced from each other in the y-direction. On the basis of a series of ﬁrst-principles total energy calculations, the various parameters that appear in this effective Hamiltonian can be deduced. An example of a set of calculations used to inform the effective Hamiltonian given above is shown in ﬁg. 9.19. As indicated in the ﬁgure, the basic idea is to carry out a family of distortions for which the energy can be computed ‘exactly’ on the basis of atomistics and approximately on the basis of the effective Hamiltonian. The parameters are then chosen so as to yield an optimal ﬁt to the ‘exact’ results on the basis of the effective Hamiltonian. Just as we saw in the context of phase diagrams (see section 6.5.5), once an effective Hamiltonian has been adopted, it becomes possible to carry out the associated statistical mechanical analysis which makes possible a systematic exploration of the phase diagram associated with that model. In the present case, Roelofs et al. (1989) carried out a series of Monte Carlo calculations on the W(001) surface using the effective Hamiltonian of eqn (9.13), all the while monitoring the diffraction amplitude associated with the superlattice peaks in the diffraction pattern emerging from the c(2 × 2) symmetry. At high temperatures (in fact at temperatures twice those of the observed transition temperature) the diffraction intensity in these satellite peaks was seen to decay, signaling the onset of the transition. The mismatch between observed and computed transition temperatures provides some idea of the challenges that still remain in the construction of material speciﬁc effective Hamiltonians. Case Studies on Semiconductor Surfaces Our discussion in the previous part of this section showed some of the variety associated with surface reconstructions on the surfaces of metals with both the fcc and bcc structures. Just as such surfaces have served as a proving ground for our understanding of metals, semiconductor surface reconstructions have played a similar role in the study of covalent systems. The starting point for the analysis in this section is a synthesis of a wide variety of experimental data in the form of a phase diagram for the Si surfaces. The objective in the remainder of the section will be to try to rationalize, even predict, such phases on the basis of microscopic analysis. Beyond their academic interest to surface science, the reconstructions in Si also impact the nature of the growth processes that occur when atoms are deposited on exposed surfaces.

9.2 Free Surfaces

467

Fig. 9.19. Calculations used in the construction of an effective Hamiltonian for the W(001) surface (adapted from Roelofs et al. (1989)). Panel (a) shows the surface Brillouin zone while panels (b)–(e) show the energy associated with various displacement patterns, with the solid lines corresponding to the energetics of the effective Hamiltonian while the discrete points are the energies associated with ﬁrst-principles total energy calculations.

468

9 Wall Defects in Solids

Fig. 9.20. Series of surface reconstructions associated with Si (adapted from Baski et al. (1997)). The graph depicts the stable planar reconstructions found between the (001) and (111) orientations and gives scanning tunneling microscopy images of the observed surface structures.

Si surface structures. The surfaces of Si present an entirely different set of challenges than do those of the metal surfaces considered thus far. As a prelude to the discussion to follow, we follow Baski et al. (1997) in pictorially representing the various stable planar surfaces between the (001) and (111) orientations as shown in ﬁg. 9.20. One of the key ideas to be conveyed by this ﬁgure is that each of the bold lines corresponds to a stable planar surface, and associated with each such surface is a corresponding scanning tunneling microscopy image of the associated reconstructions. The regions between the stable planar reconstructions are characterized by more complex structures involving steps or facets. For the purposes of the present discussion, we will consider the (001) and (111) surfaces as our representative case studies in semiconductor surface reconstruction. We note that from the point of view of intrinsic complexity, the Si(111) surface is characterized by a large unit cell and hence an intricate arrangement of atoms. The Si(001) Surface. Our analysis begins with perhaps the most studied of such surfaces, namely, the (001) surface. The ideal and reconstructed geometries were presented in ﬁg. 9.10 and are contrasted in more detail in ﬁg. 9.21 where it is noted that the presence of two dangling bonds per surface atom for the ideal bulk termination should provide a strong driving force for structural change. We have already remarked on the analogy between this tendency on the (001) surface and

9.2 Free Surfaces

469

Fig. 9.21. Schematic of the ideal and reconstructed (001) face of Si (adapted from Ramstad et al. (1995)).

that seen at the core of certain dislocations in Si. The presence of dangling bonds like this often manifests itself in structural rearrangements involving dimerization. However, the statement that the surface suffers such a dimerization reaction does not sufﬁce to fully characterize the reconstructed geometry. Though the original LEED (low-energy electron diffraction) experiments indicated the presence of a (2 × 1) symmetry on the reconstructed surface, more recent experiments indicated a phase with (4 × 2) symmetry as well. The presence of a series of such phases, each differing from the other by rather subtle geometric rearrangements poses serious challenges to efforts at modeling these surfaces. In particular, as shown in the ﬁgure (via open and ﬁlled circles for the surface layer) in addition to the lateral displacements related to dimerization, different atoms can suffer different out-of-plane displacements. Indeed, the ﬁlled and open circles correspond to

470

9 Wall Defects in Solids

Fig. 9.22. Comparison of the atomic-level displacements associated with the Si(001) (2 × 1) surface reconstruction as obtained using alternative total energy schemes (adapted from Balamane et al. (1992)). Arrows illustrate the atomic displacements in a˚ ngstroms in comparison with the (1 × 1) reference state. The numbers in each group correspond to the displacements as obtained using density functional theory and Biswas–Hamann, Stillinger–Weber and Tersoff potentials, respectively.

perpendicular displacements either up or down, resulting in a buckling in addition to the dimerization. One theoretical point of departure for examining the surface reconstructions seen on Si(001) is zero-temperature energy minimization using empirical descriptions of the total energy. Two key articles (Balamane et al. 1992, Wilson et al. 1990) have made systematic attempts at characterizing the extent to which empirical total energy schemes can be used to examine the energetics of semiconductor surfaces (as well as other defects). As shown already in ﬁg. 9.10, the distinctive feature of the Si(001) reconstruction is the dimerization of the surface layer atoms. A quantitative assessment of the propensity for such reconstruction as well as its extent is given in ﬁg. 9.22 which shows the computed atomic-level displacements associated with this reconstruction for both the Stillinger–Weber- and Tersoff-type potentials in addition to yet another empirical scheme (the Biswas–Hamann potentials) and the results of a full ﬁrst-principles analysis. The basic point to be made is that while the empirical potentials are unable to account for the subtleties of bond buckling once dimers have formed, the existence of the dimers themselves is well reproduced by the various alternative angular force schemes set forth to account for covalent bonding in semiconductors. In fact, the energy difference between the ideal (1 × 1) surface and the (2 × 1) reconstruction is also reasonably well reproduced.

9.2 Free Surfaces

471

Fig. 9.23. Energies for Si(001) surface. Energy obtained for both ideal and competing reconstructed geometries and illustrating errors (adapted from Ramstad et al. (1995)).

More reliable calculations of the energetic ranking of the various structural competitors on Si(001) have been performed using traditional ﬁrst-principles methods. In particular, a careful zero-temperature analysis has been performed with attention to the errors involved as a result of choice of both k-point sampling and plane wave cutoffs (Ramstad et al. 1995). This work attempts to discriminate between the energetics of the ideal unreconstructed surface and two different (2×1) competitors and the (4 × 2) reconstruction. In ﬁg. 9.23, we show the energy differences associated with the Si(001) reconstruction as well as the error bars associated with these energy differences. In particular, the four panels in the ﬁgure report the energy differences between various structural competitors and give the associated error bars in the calculations. For example, the upper left ﬁgure reports the difference in energy between the bulk terminated (1 × 1) surface and the symmetric dimerized (2 × 1) reconstruction. The label ‘This’ refers to the results from Ramstad et al. while the others (i.e. YC, DS, etc.) refer to the results of calculations of other groups. From a philosophical perspective, it is worth noting that while such calculations are highly tedious and lack glamor, they are also extremely instructive in that through them it is possible to quantify the level of conﬁdence that should be placed in the results. In this case, we see that the error bars associated with the (2 × 2)/(4 × 2) energy difference are so large as to render the result impotent since it was not possible even to conclude the sign of the energy difference. The structure and energetics of the Si(001) surface

472

9 Wall Defects in Solids

provide a series of interesting insights into the nature of surface reconstructions. Indeed, in addition to the simple question of dimerization considered above, there are fascinating issues that arise in conjunction with the presence of vacancies on these surfaces. The Si(111) Surface. As noted already at the beginning of the present subsection, the (111) surface is characterized by a complex (7 × 7) reconstruction which presents signiﬁcant challenges from both an experimental and theoretical point of view. Our current discussion is aimed at examining the structure of this surface in slightly more detail. A schematic depiction of the reconstructed (111) surface is shown in ﬁg. 9.24. The accepted reconstructed surface geometry is known as the dimer adatom stacking fault (DAS) model and is characterized by three distinctive structural features: in particular, the second-layer atoms undergo a dimerization rearrangement, the presence of twelve adatoms in an adatom layer on the surface (the twelve large ﬁlled circles in ﬁg. 9.24) and the existence of a stacking fault over part of the reconstructed area (seen in the left part of the surface cell in ﬁg. 9.24). Just as was possible with the Si(001) surface, a series of comparisons have been made for the energetics of various structural competitors on Si(111) using different total energy schemes. We appeal once again to the careful analysis of Balamane et al. (1992). In this case, the subtlety of the structural rearrangement leads largely to an inability on the part of various empirical schemes to correctly reproduce the energetics of this surface. In particular, as discussed by Balamane et al. (1992), only one of the Tersoff potentials leads to the conclusion that the 7 × 7 reconstruction is stable with respect to the ideal 1 × 1 surface. As a result, as yet the only reliable means whereby one can successfully explore energetic questions concerning these surfaces is through the use of electronic structure-based total energy methods. Surface Reconstructions Reconsidered In the preceding pages we have tried to convey a ﬂavor of the structure and energetics of surface reconstructions. We note that the great advances in this area have been largely experimentally driven and reﬂect the routine atomic-scale resolution that is now enjoyed in the analysis of surface structures. By dividing our analysis along the lines of material type (i.e. metals vs semiconductors) we have been able to contrast the relative merits of different schemes for computing the energetics of crystal surfaces. As a ﬁnal example of some of the exciting developments in considering surfaces, ﬁg. 9.25 shows a surface in amorphous Si with relaxed atomic positions obtained using density functional theory calculations. Now in keeping with our overall theme of examining the departures from the monotony of

9.2 Free Surfaces

473

Fig. 9.24. The 7 × 7 reconstruction of Si(111) in ultrahigh vacuum. Both empty and ﬁlled state constant-current scanning tunneling microscope images are shown for a 14 nm × 14 nm region (adapted from Whitman (1998)). The diamond shaped (7 × 7) unit cell is indicated in the scanning tunneling microscope images. The ﬁgure also gives a schematic of the reconstructed unit cell for both a top and a side view (through the long diagonal) with the topmost atoms largest and darkest. Some of the atoms are labeled to aid correlating the two views.

474

9 Wall Defects in Solids

Fig. 9.25. Surface geometry associated with amorphous Si as computed using density functional theory (courtesy of Martin Bazant and Tim Kaxiras). The surface layer is at the top of the ﬁgure and the atoms colored black are those having ﬁvefold coordination.

Fig. 9.26. Schematic of vicinal surface with low-index terraces bounded by surface steps (adapted from Poon et al. (1992)).

the perfect crystal, we push our analysis of crystal surfaces yet a step further in the form of an examination of steps on crystal surfaces.

9.2.3 Steps on Surfaces Despite our foray into the structure and energetics of surface reconstructions, the class of departures from the perfection of the bulk terminated surface that we have considered is still incomplete. In addition to the relaxations and symmetry breaking reconstructions that are present on surfaces, we must also consider the role of surface steps. Such steps arise from a variety of different sources: the inability to cut a crystal at exactly the face that is desired, the development of steps and islands during the growth process itself and the presence of thermal roughening. Surfaces with a slight misorientation relative to the conventional low-index surfaces are known as vicinal surfaces and are characterized by a series of terraces of the nearby low-index surface, separated by steps which accommodate the overall misorientation. Indeed, the relation between the step height (h), terrace width (lw ) and misorientation can be written as θ ≈ h/lw . A schematic of such a vicinal surface is given in ﬁg. 9.26.

9.2 Free Surfaces

475

Fig. 9.27. Scanning tunneling microscope image, 100 nm × 100 nm, of a stepped Si(001) surface (courtesy of A. Laracuente and L. J. Whitman).

We begin with a consideration of the experimental situation. The advent of scanning tunneling microscopy has made the examination of surface steps routine. In ﬁg. 9.27, we show a representative example of a stepped semiconductor crystal surface. There are a few key observations to be made about these scanning tunneling microscope results. First, we note that the presence of steps is a common occurrence on surfaces. In addition, we note that the morphology of the steps themselves (i.e. smoothly wandering or jagged) poses interesting challenges as well. Our strategy for examining the physics of such steps is to attend to a microscopic description of the energetics of steps. For the Si(001) surface, recall that the surface structure is characterized by dimer pairs. Depending upon which layer in the AB packing along this direction is exposed, these dimers will be oriented parallel to either the x-direction or the y-direction. This effect is indicated schematically in ﬁg. 9.28, where we see that if the surface is exposed on layer A, then the dimerization will occur with one orientation, while if it occurs on layer B, the dimerization will be rotated by 90◦ . This is precisely a schematic of the experimental situation shown in ﬁg. 9.27. The ﬁgure also reveals the presence of these different variants and shows the distinction between the two different step types that occur. The geometry of vicinal surfaces is extremely complex and gives rise to a richness in the series of resulting surface phases that was already foreshadowed in ﬁg. 9.20. In particular, that ﬁgure revealed that as a function of misorientation relative to stable planar surfaces, the surface geometry can range from terraces to facets.

476

9 Wall Defects in Solids

Fig. 9.28. Stepped Si(001) surface and different dimer orientations that result from different layers being exposed (adapted from Alerhand et al. (1990)).

As we have already noted a number of times, the analysis of defects in solids is served both by atomistic and continuum approaches. Like many of the other defects that we have already examined, surface steps are amenable to a description on the basis of atomistic analysis. Microscopic analysis is especially suitable for exploring the short-range contributions of these defects to the total energy that derive from the disruption of the atomic-level geometry at the surface. Without entering into a detailed description of what is involved in computing the energetics of steps, we note that many of the same ideas presented in this and earlier chapters are used. In particular, once a computational cell is in hand, one resorts to a computation of E tot ({Ri }). For our present purposes, we note that microscopic analysis has been invoked in order to carry out a systematic ﬁrst-principles analysis of step energies on metal surfaces as shown in ﬁg. 9.29. We note in closing that we have certainly not done justice to this important topic and a major omission in our discussion has been a failure to report on the continuum theory of surface steps. For a review, the reader is urged to consult Jeong and Williams (1999).

9.3 Stacking Faults and Twins In the previous section we highlighted some of the key issues that arise in considering free surfaces which are themselves one of the key wall defects found in solids. As noted in the introduction, in addition to free surfaces, there are a number of important internal interfaces that are found in solids. Perhaps the lowest-energy class of such internal interfaces are those associated with mistakes

9.3 Stacking Faults and Twins

477

Fig. 9.29. Step energies for 4d transition metals (adapted from Vitos et al. (1999)). The straight lines reﬂect the outcome of a model near-neighbor calculation for the step energies on these surfaces. The ﬁrst-principles calculations were done using the LMTO method.

in the stacking sequences that lead to a given crystal structure. The role of stacking faults as a key player in dislocation core phenomena has already been introduced in section 8.3.2. However, beyond their presence in dislocations, stacking faults can arise in the course of crystal growth, and in some cases form a part of the structural complexity in certain crystal phases. The goal of the current section is to make a deeper examination of the structure and energetics of stacking faults in crystalline materials. 9.3.1 Structure and Energetics of Stacking Faults Geometries of Planar Faults. In chap. 8 we introduced the geometric characteristics of stacking faults. One perspective for characterizing these faults is that they arise as the outcome of rigidly translating an entire set of (111) crystal planes ¯ That with respect to the rest of the crystal by vectors of the form (a0 /2)(211). is, we consider translating the entire half-space above some certain plane by the vector given above. The result is a stacking fault at this plane. Alternatively, these faults may be seen as disruptions in the regular ABCABC arrangement associated with packing of spheres. This perspective is taken up in ﬁg. 9.30. In keeping

478

9 Wall Defects in Solids

Fig. 9.30. Various stacking mistakes associated with (111) close packings (adapted from Rosengaard and Skriver (1993)).

with our earlier discussion concerning the transcription between microscopic and continuum descriptions of interfacial energies, these disruptions in the regular stacking sequence are characterized by an interfacial energy, γ S F . Once again, we see the emergence of a single material parameter which serves to characterize the behavior of materials and which is amenable to microscopic evaluation. We begin ﬁrst with an investigation of the geometric character of the atomiclevel geometry of stacking faults and then turn to the explicit numerical evaluation of their energies. Fig. 9.30 permits a comparative analysis of some of the key stacking fault geometries in fcc crystals. The ﬁrst two schematics illustrate the way in which the fcc and hcp structures can be generated by regular arrangements of either the ABCABC. . . (fcc) or ABABAB. . . (hcp) stacking sequence. The geometrically simplest of the possible faults in the stacking sequence is that of the twin boundary which results from a reversal in order of the stacking sequence and can be induced by a shearing transformation. In addition to the twinning fault introduced above, mistakes in the fcc stacking sequence can also be induced by either adding a plane in the sequence or by removing one. The former case is known as an extrinsic stacking fault and is characterized by a stacking sequence of the form ABCABCBABC. . . . The latter fault is known as an intrinsic fault and is characterized by a stacking sequence of the form ABCBCABC. . . . A systematic discussion of these geometries may be found in chap. 10 of Hirth and Lothe (1992). The ﬁrst geometric question we might pose concerning the stacking fault is how the bond lengths are redistributed by virtue of the presence of this defect. We note that in a perfect fcc crystals the twelve near neighbors of a given atom are associated with the vertices of a cube-octahedron, while the six second neighbors correspond to the vertices of an octahedron. What emerges in comparing the atomic conﬁgurations in the perfect crystal and in a crystal with a stacking fault is the recognition that at the near- and next near-neighbor level, the perfect and faulted

9.3 Stacking Faults and Twins

479

crystals have the same near-neighbor distributions. The details of this geometric analysis are taken up in the problems at the end of the chapter. This geometric fact has energetic consequences that will be taken up below. Energetics of Planar Faults. As shown in the previous chapter, the particulars of the dislocation reactions that will be found in a given material are determined by the numerical values of the relevant interfacial energies (i.e. stacking fault or antiphase boundary energies). One of the dominant philosophical thrusts of the book has been the idea that when it is possible, our aim should be to exploit insights from one level of modeling to inform models at a different scale. In this case, our aim will be to show how insights based upon atomistic calculations of the various interfacial energies can be used as the basis of the type of elasticity calculations that were carried out in the previous chapter in order to determine the dissociation width of dislocations that have undergone splitting reactions and which culminated in eqn (8.74). Our application of the continuum theory of dislocations required an external parameter, namely γ S F , which we now discuss from the perspective of microscopic analysis. Unlike the gross differences between a crystal with and without a free surface, the stacking fault constitutes a less severe perturbation and thereby, generically, has a lower energy than that of a free surface. Our discussion of the bond lengths in faulted regions given above provided a plausibility argument in favor of the relatively low energy of stacking faults in the hierarchy of interfacial defects. Both empirical and ﬁrst-principles methods have been used to evaluate stacking fault energies in crystals. For the purposes of numerical evaluation of the stacking fault energy, we must ﬁrst insure that the stacking fault itself is embedded in a box that is sufﬁciently large so as to mimic the presence of a stacking fault in an inﬁnite crystal. We will ﬁrst give an overview of how the stacking fault energy may be computed within the conﬁnes of empirical energy functionals, and will close our discussion with a representative example from the use of ﬁrst-principles methods for computing the stacking fault energy. Regardless of the choice of energy functional, the type of computational box that is used to evaluate the stacking fault energy is shown schematically in ﬁg. 9.31. The key elements of the simulation box are, evidently, the presence of the stacking fault itself, and the presence of a sufﬁcient distance between the stacking fault and the distant free surfaces, or periodic boundaries. Once the simulation box has been established, it is a routine matter to compute the stacking fault energy itself. The stacking fault energy may be computed on the basis of a generic total energy scheme according to E N (S F) − E N (bulk) . (9.14) γS F = A

480

9 Wall Defects in Solids

Fig. 9.31. Computational box used to compute the energy of an intrinsic stacking fault in Al (adapted from Wright et al. (1992)).

As with the surface energy as deﬁned in eqn (9.5), the stacking fault energy is obtained by computing the energy of two different N -atom conﬁgurations, one corresponding to the perfect crystal and the other corresponding to the N -atom supercell within which is a stacking fault. In practice, once the computational cell is in hand, the energy difference called for above can be evaluated in exactly the same way that we obtained the vacancy formation and surface energies earlier. From the perspective of a pair potential description of the total energy and in the context of the geometric distributions of neighbor environments shown above, the evaluation of stacking fault energies becomes an exercise in delicate choices about the long-range part of the potential of interest. As has been seen in earlier chapters, the introduction of higher-order terms in the energy functional can improve the pair potential treatment substantially. We note that in the case of stacking faults, even pair functionals are relatively ineffective at reproducing the energetics of stacking faults, suffering from routine underestimates of the stacking fault energy which lead in turn to unreasonably large dissociations for dislocations. On the

9.3 Stacking Faults and Twins

481

other hand, these results can be improved by incorporating angular terms in the energy functional. An example of the type of results that have been obtained in the empirical setting is shown in ﬁg. 9.32. The key idea being presented here is that the stacking fault energy can be thought of as being built up of both pair and four-body contributions. In particular, the total energy is written in the form E tot = E pair + E 4-body , where the four-body term is of the form ( f cc) α(µ(i) ). E 4-body = 4 − µ4

(9.15)

(9.16)

i

The four-body term is an application of exactly the ideas introduced in section 4.5.3 and culminating in eqn (4.95). Fig. 9.32 shows the relative contributions of different atoms in the faulted region to the overall fault energy. In particular, for a series of different metals the overall contribution to the stacking fault energy is decomposed layer by layer and each such contribution is itself decomposed into the relative contributions of the pair and four-body terms. The computation of stacking fault energies from ﬁrst principles is a more delicate matter. There are tedious questions that arise concerning convergence with respect to box size, energetic cutoffs and k-point sampling. Again, since we have repeatedly described the essential conceptual steps involved in carrying out a total energy calculation, we note here that the calculation of stacking fault energies involves the same basic elements such as building an appropriate computational cell, etc. An example of the types of results that emerge from these calculations is shown in ﬁg. 9.33. As was done in ﬁg. 9.32 (a calculation which was itself inspired by the present one) the stacking fault energies are decomposed into the contributions of the different layers in the faulted region. A rough rule of thumb which is substantiated by these calculations can be written in the form ≈ γ Sextrinsic ≈ 2γ Stwin γ Sintrinsic F F F .

(9.17)

Just as was found possible in the context of alloy phase diagrammatics and in the evaluation of surface energies, it is possible to exploit atomic-level calculations as the basis of effective Hamiltonians describing the energetics of stacking faults. Once again, the calculations are made on the basis of an Ising-like model of the stacking fault. Our development follows that of Hammer et al. (1992) in which the energy of a crystal with a stacking fault is written as E = ξ0 −

1

n max N atoms

Natoms

n=1 i=1

Jn σi σi+n .

(9.18)

The parameters Jn are the effective Ising parameters that are determined from

482

9 Wall Defects in Solids

Fig. 9.32. Systematics of stacking fault energy in different metals as computed using multiatom interactions (adapted from Stokbro and Jacobsen (1993)).

atomic-level analysis. The notation is such that σi = 1 if the atom in layer i + 1 maintains the integrity of ABC stacking whereas σi = −1 if the atom in layer i + 1 is part of CBA stacking. For example, if the i th layer is of C-type and the following layer is an A-type, then σi = 1. By way of contrast, if the i th layer is of the type C and the following layer in the stacking sequence is of the B-type, then σi = −1. To make the correspondence more concrete, the sequence ABCABCBABC, corresponding to an extrinsic stacking fault leads to

9.3 Stacking Faults and Twins

483

Fig. 9.33. Systematics of stacking fault energy in different metals as computed using ﬁrst-principles total energy methods (adapted from Crampin et al. (1990)).

the transcription ABCABCBABC = 1 1 1 1 1 −1 −1 1 1 1.

(9.19)

To compute the stacking fault energy, we must evaluate E = E faulted (N layers) − E perfect (N layers). For the extrinsic case given above only four layers (i.e. 1 1 −1 −1 have contributions that are different from the perfect crystal contribu-

484

9 Wall Defects in Solids

Fig. 9.34. Schematic of several polytypes occurring in SiC (adapted from K¨ackell et al. (1994)). Each polytype represents a different stacking of A, B and C layers.

tions, so the energy difference is of the form E = [−J1 + J2 + J1 + J2 − J1 + J2 + J1 + J2 ]−4(−J1 − J2 ) = 4J1 +8J2 . (9.20) The terms in square brackets come in pairs involving J1 and J2 correspond to working from left to right while the term involving 4(−J1 − J2 ) is the energy of four layers worth of perfect lattice on the assumption of one atom per layer. The use of these ideas is ﬂeshed out in problem 5 at the end of the present chapter. Once this effective Hamiltonian is in hand, it is possible to begin considering the distribution of such faults in crystals. One particularly interesting venue within which planar faults arise is in the context of some of the complex structures that arise in alloys. 9.3.2 Planar Faults and Phase Diagrams As noted above, stacking defects are relevant in the context of the phase diagrammatics of complex alloys. In this setting, there are a range of polytypes that a particular material may adopt depending upon the tuning of some control parameter such as the temperature or the chemical composition. For our present purposes, such polytpes represent different structural variants in which the regular packing of planes along a particular direction is disturbed relative to the stacking in some reference state. These mistakes in packing correspond in the fcc case to exactly the sort of stacking faults that have entered our discussion thus far. Example of

9.3 Stacking Faults and Twins

485

Fig. 9.35. Schematic of the different polytypic phases found in SiC (adapted from Trigunayat (1991)).

the types of structural rearrangements that occur in the SiC system are shown in ﬁg. 9.34. In addition, ﬁg. 9.35 gives a schematic indication of the stability ranges of the various structures. In addition to its importance in the type of covalent systems described above, the phenomenon of polytypism is also found in intermetallics. For example, in ﬁg. 9.36, we show a schematic rendering of the various structure types found in a series of Mg-based ternary alloys such as Mg(Znx Ag1−x )2 and Mg(Cux Al1−x )2 . The basic idea is that by varying x, and hence the proportions of the elements in the alloy, the mean electron/atom ratio (denoted as z in the ﬁgure) for the alloy can be altered. This ﬁgure reveals that depending upon the value of z, a whole range of different stacking sequences emerge. The notation presented in the ﬁgure is such that a given layer is labeled with an h if the two adjacent layers are of the same type and a given layer is labeled c otherwise. For example, the hcp structure (ABABABA. . . ) would be labeled as hhhhh. . . since every layer is such that the two adjacent layers are identical (i.e. A is sandwiched between two Bs and vice versa). The fcc structure, on the other hand, characterized by a stacking sequence ABCABC. . . , would be denoted as cccccc. . . in this notation since the two layers adjacent to a given layer are never the same. As shown in the ﬁgure, for the more complex case of interest here, different values of z, the electron per atom ratio (which is another way of saying for different compositions), the resulting stacking sequence will be a different arrangement of h and c layers. For our present purposes, all that we really aim to take away from this ﬁgure is a sense

486

9 Wall Defects in Solids

Fig. 9.36. Series of stable stacking sequences in Mg-based Laves phases as a function of the electron per atom ratio, z (Bruinsma and Zangwill 1985).

of the diversity of structural types that can be thought of from the ‘stacking fault’ perspective and to note the way in which control parameters such as the electron per atom ratio can govern structural stability. The emergence of the types of polytypes described above may be rationalized on the basis of a variety of different ideas. Rather than exploring the phenomenon of polytypism in detail, we give a schematic indication of one approach that has been used and which is nearly identical in spirit to the effective Hamiltonian already introduced in the context of stacking fault energies (see eqn (9.18)). In particular, we make reference to the so-called ANNNI (axial next-nearest-neighbor Ising) model which has a Hamiltonian of the form H = E0 −

1 1 J1 σi σi±1 − J2 σi σi±2 . 2 2 i i

(9.21)

The basic idea is to represent the energy of a given stacking sequence in terms of effective Ising parameters. The relative importance of ﬁrst (J1 ) and second (J2 ) neighbor interactions gives rise to a competition that can stabilize long-period

9.4 Grain Boundaries

487

10

∆E (meV)

5

0

SiC

ZnS

Si

Fig. 9.37. Ranking of structural energies associated with different polytypes using the Ising-like effective Hamiltonian described in the text (adapted from Engel and Needs (1990)).

equilibrium states. In particular, this competition is especially relevant in the case in which the magnitudes of the two terms are nearly equal and their signs are opposite. From the standpoint of the analysis of this model there are two different considerations. First, it is necessary to inform the effective Hamiltonian on the basis of atomic-level analysis. Secondly, the representation of polytypic energies in terms of an Ising parameterization like that described above opens up the possibility for a statistical mechanics analysis of the temperature dependence of phases. A representation of the ranking of polytype energies in three different material systems is shown in ﬁg. 9.37. In each of these cases, the energies shown in the ﬁgure are based upon the effective Hamiltonian, with the parameters in that Hamiltonian ﬁt on the basis of a ﬁrst-principles analysis of the total energy.

9.4 Grain Boundaries One of the dominant themes upon which much of our analysis has been predicated is the idea that a solid is populated by structures at many different scales. At the most fundamental level, a crystal may be thought of as an uninterrupted arrangement of atoms according to the simple decomposition Rm 1 ,m 2 ,m 3 = m 1 e1 + m 2 e2 + m 3 e3 ,

(9.22)

488

9 Wall Defects in Solids

where m i is a member of the integers, ei is a Bravais lattice vector and R(m 1 , m 2 , m 3 ) is the position of the lattice point indexed by the triplet (m 1 , m 2 , m 3 ). Here we are imagining the simplest of crystals in which there is only one atom per unit cell. At the next level of structure, we imagine this perfect regularity to be disturbed both by a distribution of point defects such as vacancies and interstitials as well as by arrangements of dislocations and possibly also by their attendant stacking faults. At even larger scales (i.e. the micron scale), there is yet another level of structure, namely, that of the multiple grains that make up a typical crystalline solid. Different regions within the crystal are tied to different orientations of the same fundamental Bravais lattice. These grains are bounded by interfacial defects known as grain boundaries which serve as an integral part of the geometry of crystalline solids and it is the business of the present section to examine the structure and energetics of such boundaries from the perspective of models of material behavior. As a reminder of the way interfaces, as key microstructural elements, can impact material response, we note one of the celebrated relations between a material’s microstructure and its physical response, namely, the Hall–Petch relation which holds that the yield strength of a material scales as 1

σ y = σ0 + kd − 2 ,

(9.23)

where d is the average ‘grain size’ and k and σ0 are constants. We have already exhibited pictorial evidence for this effect in ﬁgs. 1.3 and 8.2(c). We have elected to surround grain size in quotes as a reminder that despite the ease with which those words are used in everyday conversation in discussing materials, the geometric characterization of microstructure is subtle. Our reason for calling attention to the Hall–Petch relation is to anticipate some of the questions that are tied to the existence of grain boundaries. In the long history of efforts to piece together the connection between a material’s microstructure and its properties, one series of arguments has been built around a reductionist perspective. In these arguments, it is held that by building up an appropriate understanding of a single grain boundary perhaps it will be possible to bootstrap these insights to an analysis of microstructures themselves. As a result, not only has there been considerable effort in trying to ferret out the implications of polycrystalline structure on properties, but a great deal of effort has gone into examining the deformation and fracture of bicrystals. An entire hierarchy of geometric structures involving grain boundaries can be considered as illustrated in ﬁg. 9.38. As is evidenced by ﬁg. 9.38, there are a number of points of entry into a discussion of polycrystalline microstructures. In particular, ﬁg. 9.38 shows that at the simplest level (frame (a)) we can consider bicrystal geometries. In keeping with

9.4 Grain Boundaries

489

Fig. 9.38. Schematic of increasingly complex grain boundary distributions within materials (adapted from Randle (1994)): (a) bicrystal geometry with a single grain boundary, (b) bamboo-like distribution of grain boundaries in a one-dimensional array, (c) polycrystalline ﬁlm, and (d) three-dimensional polycrystal.

that suggestion and as a preliminary to investigating the physics of polycrystals, we begin by examining the geometry of bicrystals with an eye to examining such geometries from both a microscopic and continuum perspective.

9.4.1 Bicrystal Geometry In this section, we begin with consideration of the fundamental geometric degrees of freedom that characterize bicrystals and then turn to the descriptions of the structures themselves. The reference geometry around which the discussion of grain boundaries acquires meaning is the perfect lattice of eqn (9.22). Denote the Bravais lattice vectors of the ﬁrst grain by ei(1) , where 1 is a label denoting this grain, and the subscript ranges from one to three and labels the three linearly independent Bravais lattice vectors characterizing the crystalline state. The basic

490

9 Wall Defects in Solids

Fig. 9.39. Interpenetrating lattices used to consider grain boundary structure (courtesy of D. Pawaskar). Open and ﬁlled circles correspond to the two host lattices and ﬁlled squares correspond to those atoms that are common to both lattices (i.e. the lattice of coincident sites).

idea for describing the grain boundary structure is embodied in two fundamental geometric notions. First, we must characterize the orientation of the second grain with respect to the ﬁrst. Having done this, the boundary itself is not fully determined since we must also say which plane serves as the dividing surface between the two grains. Together, these two geometric descriptors, the relative orientations of the two grains and the identiﬁcation of the boundary plane, serve to completely specify the macroscopic grain boundary geometry. We now set ourselves the task of casting these geometric questions in a proper mathematical light. We begin by imagining ﬁlling space with two interpenetrating lattices, both built around the same Bravais lattice type, but with different orientations, and possibly a different overall origin. In particular, if we are given the two sets of Bravais lattice vectors, their relative orientations are connected via a rotation matrix Q by ei(2) = Qi j e(1) j .

(9.24)

In addition, as was mentioned above, it is possible that there is a shift of origin associated with some translation vector τ . The matrix Q imposes a linear transformation which, since it describes a rotation, may be characterized by three parameters. We now have two interpenetrating lattices as indicated in the simpliﬁed two-dimensional setting in ﬁg. 9.39. As yet, there is no grain boundary. The remainder of our work in identifying the macroscopic degrees of freedom is to select the boundary plane itself. This plane is characterized by a unit vector n

9.4 Grain Boundaries

491

Fig. 9.40. Schematic of degrees of freedom associated with choice of boundary plane (adapted from Wolf et al. (1992)). This ﬁgure illustrates the idea that once the relative orientation of the two grains has been chosen there is still a freedom to choose the grain boundary plane.

which can be identiﬁed by two additional degrees of freedom. The choice of boundary plane is illustrated in ﬁg. 9.40. We now imagine a shaving operation in which only one group of atoms is retained on each side of the boundary. For example, we might elect to keep those atoms associated with the Bravais lattice set ei(1) on one side and those from the other Bravais lattice set on the other side of the boundary. What we have learned is that with the speciﬁcation of ﬁve macroscopic degrees of freedom, the overall character of the boundary may be speciﬁed. For the special case in which the rotation axis is contained within the boundary plane, such a boundary is known as a tilt boundary, while for the other special case in which the rotation axis is perpendicular to the boundary plane, one speaks of a twist boundary. Just as the most generic dislocations are neither pure edge or pure screw, the generic grain boundary is neither pure tilt nor pure twist.

492

9 Wall Defects in Solids

The description of grain boundary geometry as given above is somewhat deceptive. In addition to the overall macroscopic descriptors of that boundary, there are also microscopic features that may be assigned to such boundaries. For example, even though we have selected the relative orientations and the boundary plane, it is possible that the two grains may have also suffered a relative translation. As will be seen in subsequent sections, the search for the particular energy minimizing translation is a tedious but important step in the analysis of grain boundary structure. Bicrystallography has been dominated by the analysis of special boundaries in which symmetry plays a pivotal role. In particular, the geometry of those boundaries with a high degree of symmetry is most easily captured through an appeal to certain important classiﬁcation schemes, such as that of the coincident site lattice (CSL). The qualitative idea behind this classiﬁcation is the insight that for certain choices of rotation matrix Q, there will be a fraction of the sites that are common to both lattices. The fraction of such overlapping sites serves as a measure of the boundary symmetry. This lattice of overlapping sites is known as the coincident site lattice. From a quantitative perspective, this degree of overlap of the two lattices is characterized by the ' number. To compute this number, we ﬁnd what fraction of the sites from a given lattice are coincident with those of the other. The reciprocal of this number is the ' number. For example, if one in every ﬁve sites is coincident, this would be referred to as a '5 boundary, precisely the case shown in ﬁg. 9.41. An example of a set of coincident site lattices is shown in ﬁg. 9.41. Interestingly, even in those cases in which a tilt boundary has relatively little symmetry, the boundary structure may be thought of as a limiting case in which the coincident site lattice has a very high ' number, where we note again that this number is deﬁned such that 1/' of the sites on a given lattice are common.

9.4.2 Grain Boundaries in Polycrystals In light of our characterization of the structures of individual grain boundaries, it is important to now undertake the statistical question of what the distribution of grain boundaries is like in real polycrystals. We have already noted that the important role of bicrystals was born of a reductionistic instinct in which it was argued that proper understanding of the structure and energetics of single boundaries must precede a fundamental understanding of the consequences of an assembly of such boundaries. Our task in the present section is to examine the geometric character of real polycrystals, paying special attention to the distribution of different boundary types within polycrystals. We have already seen that boundaries of high symmetry have been the workhorse of most research in examining the structure and energetics

9.4 Grain Boundaries

493

Fig. 9.41. Schematic of several representative grain boundaries with structures described by coincident site lattice model. This set of boundaries corresponds to a (001) rotation axis, and the atomic-level geometries have not been relaxed (courtesy of D. Pawaskar). The ﬁlled circles correspond to those sites (coincident sites) that are common to both lattices.

of grain boundaries. This raises the question of to what extent such boundaries are representative of those found in real microstructures. As pointed out in Randle (1997), there are two aspects to the statistics of grain boundary distributions. On the one hand, the question of how different grains are misoriented can be posed. This leads in turn to an analysis of the distribution of various coincident site lattice types. By way of contrast, it is also important to obtain quantitative insights into the distribution of grain boundary planes. Indeed, the character of the grain boundary plane is critically related to the nature of the underlying grain boundary structure. As a ﬁrst exercise in the statistics of grain boundaries, ﬁg. 9.42 shows the distribution of ' boundaries for an Fe–Si alloy. In this case, it is the relative frequency of different misorientations that is being reported. An example of this type of statistical distribution with regard to the boundary plane is shown in ﬁg. 9.43. In particular, this ﬁgure reveals the distribution of

494

9 Wall Defects in Solids

Fig. 9.42. Frequency of various coincident boundaries as a function of the ' number (adapted from Watanabe (1989)). The data are for a fully annealed Fe–6.5 wt% Si alloy. The two distributions (different color histograms) correspond to samples with different textures.

grain boundary plane types in annealed high purity Cu and Ni. All of the reported boundaries are for the same underlying crystal misorientation and correspond to '3 boundaries. The numbers on the left hand axis of the ﬁgure give the orientation of the grain boundary plane. Our intent in this section was not to give an exhaustive account of the nature of grain boundaries in real polycrystals. Rather, it was meant as a gentle reminder that despite the importance of bicrystals, they are but a ﬁrst step in understanding the deeper question of the nature of grain boundaries in real microstructures.

9.4.3 Energetic Description of Grain Boundaries We now take up the issue of how one goes about using microscopic calculation to determine grain boundary structure and energetics. The principles of these calculations will be essentially independent of whether or not empirical or ﬁrstprinciples schemes are adopted. However, the goodness of the results will clearly be inﬂuenced by that choice. As a preliminary, we recall the transcription between the microscopic and continuum description of grain boundary energies. As was noted in eqn (9.4), the introduction of interfacial energies in a continuum setting is effected via a scalar parameter (i.e. γsurf , γ S F or γG B ) which has a dependence on crystallographic features such as the interfacial normal and the relative orientations of adjacent grains in the case of grain boundaries. For grain boundaries, as

9.4 Grain Boundaries

495

Fig. 9.43. Distribution of grain boundaries in polycrystals (adapted from Randle (1997)). The numbers on the vertical axis refer to the coordinates of the boundary plane, while ATGB and TWGB refer to the asymmetric tilt boundaries and twist boundaries, respectively.

for surfaces and stacking faults, the transcription between the microscopic and continuum notions is based upon γG B =

E N (G B) − E N (bulk) . A

(9.25)

As with our previous treatments of interfacial energy, the fundamental idea is to make a comparison between an N -atom state in which all of the atoms are in their ideal bulk positions and an N -atom state in which the interface of interest is present. As an example of the type of supercell that can be used in this analysis, ﬁg. 9.44 shows a scheme in which the grain boundary is at the interior of a cell whose outer boundaries perpendicular to the boundary are treated as rigid slabs. In this case, the forces on the atoms in the region being relaxed are computed in exactly the

496

9 Wall Defects in Solids

Fig. 9.44. Schematic of the type of computational cell used in computing the energy of a grain boundary.

manner already emphasized repeatedly in the book, and the atoms are subsequently relaxed. Our thinking for the remainder of this section is to examine a few different case studies in grain boundary structure with the aim of seeing both how such calculations are done, and what can be learned from them. Semiempirical determination of grain boundary structure and energetics. Simple grain boundaries in metals have been exhaustively considered from the standpoint of empirical descriptions of the total energy. The logic of much of this work is founded on the contention that prior to understanding the susceptibility of boundaries to segregation and fracture or their role as short-circuit paths for diffusion, it is necessary to ﬁrst understand the structures themselves. The majority of this work has emphasized bicrystals. A series of studies in Ni have been made for tilt boundaries that elucidate the role of misorientation in boundary structure. The case study of interest to our present discussion (Rittner and Seidman 1996) involved the use of a pair functional description of the total energy to investigate 21 distinct symmetric tilt boundaries with a 110 tilt axis. Representative examples of the relaxed structures are shown in ﬁg. 9.45 and the corresponding grain boundary energies are shown in ﬁg. 9.46. One of the most important points of contact between models like those described above and experiment is the use of transmission electron microscopy to examine grain boundaries. In particular, there is a well-established tradition of effecting direct comparisons between the outcome of a given atomic-level simulation of

9.4 Grain Boundaries

497

Fig. 9.45. Series of grain boundary structures for 110 symmetric tilt boundaries as computed using a pair functional description of the total energy (adapted from Rittner and Seidman (1996)).

grain boundary structure and the corresponding images obtained on the basis of high-resolution transmission electron microscopy (HRTEM). The way such comparisons are effected is by taking the results of the atomic-level calculation and using them as input for image simulation tools which compute the nature of the high-resolution transmission electron microscopy image that would be expected on the basis of that collection of atoms. An example of this strategy is illustrated in ﬁg. 9.47 which shows the atomic-level structure for a tilt boundary in Al.

498

9 Wall Defects in Solids

Fig. 9.46. Grain boundary energy as a function of tilt angle for 110 symmetric tilt boundaries (adapted from Rittner and Seidman (1996)).

Fig. 9.47. Comparison of high-resolution images of a grain boundary with structures obtained from atomistic simulation (adapted from Mills (1993)).

First-principles determinations of grain boundary structure and energetics. We have repeatedly emphasized the complementary (and sometimes antagonistic) role of empirical and ﬁrst-principles calculations of the many structures that inhabit materials. The structure and energy of grain boundaries is clearly yet another defect

9.4 Grain Boundaries

499

Fig. 9.48. Computational cell used for computing energetics of '11 grain boundary in aluminum (adapted from Wright and Atlas (1994)). The numbering of atoms was used in the original work in order to describe electron densities. Atoms in different layers normal to the page (i.e. along the [110] direction) are shown with open and ﬁlled circles.

that is amenable to treatment within the ﬁrst-principles setting. The analysis is predicated on the creation of a computational cell of the sort shown in ﬁg. 9.48. In this case, a high-symmetry grain boundary in Al is of interest. All of the usual machinery is exploited in the usual way (i.e. periodic boundary conditions, computing energies and forces, structural relaxation), with the result that it is possible to obtain insights into the structure and energetics of grain boundaries with ﬁrst-principles accuracy. One of the interesting insights to emerge from the ﬁrst-principles calculations highlighted in ﬁg. 9.48 is that though there is reasonable accord between the structures obtained using ﬁrst-principles techniques and those using pair functionals to examine the same boundary, the grain boundary energies are underestimated in the pair functional calculations by a factor of the order of 2. The intent of the present section was to demonstrate that just as was the case in the context of point defects such as vacancies and interstitials and line defects such as dislocations, it is possible to bring a variety of microscopic methods to bear on the question of grain boundary structure and energetics. At this late stage in the book, the basic ideas behind such structural simulations have been illustrated repeatedly with the result that our discussion has aimed only to highlight via the device of case studies, the results of such calculations.

500

9 Wall Defects in Solids

Fig. 9.49. Schematic of grain boundary triple junction.

9.4.4 Triple Junctions of Grain Boundaries As we will discuss in chap. 10, the consideration of polycrystals demands an analysis not only of the grain boundaries that separate different grains, but also of the points at which several different boundaries intersect. The simplest model of a triple junction is of the type indicated schematically in ﬁg. 9.49. For our present purposes, the basic idea is to determine a condition for the stability of such triple junctions which will at once determine both the structure and energetics of these triple points. For the geometry considered in ﬁg. 9.49, we imagine three separate segments of grain boundary, all pinned at their extremeties as shown. Our aim is to write the total energy as a function of the as-yet undetermined position x. Once this energy has been set forth, we then minimize the energy with respect to the parameter x resulting in a condition for the optimal geometry. Before illustrating the details, we note that the calculation envisaged here constrains the class of possible triplejunction geometries and that a more general treatment requires an analysis of the variation in energy for both x and y displacement of the triple point. The more general calculation is considered in the problem section at the end of this chapter. The energy of the triple junction may be written by adding up the energy γ l which results from each interfacial segment of length l. Note that this calculation is the interfacial analog of the line tension calculations used to characterize the energetics of dislocations in the previous chapter. For the particular geometry of interest here, the energy may be written as (9.26) E(x) = γ x + 2γ h 2 + (d − x)2 ,

9.5 Diffuse Interfaces

501

where the ﬁrst term is the energy associated with the horizontal segment, while the second term is that associated with the two interfacial segments that are oriented at an angle φ = θ1 /2 with respect to the horizontal. Differentiation of this energy with respect to x provides us with the equilibrium condition which is

d−x

1 = . 2 h 2 + (d − x)2

(9.27)

Further, we note that the expression on the left hand side of this equation is nothing more than cos φ, resulting in the conclusion that the equilibrium angle is φ = θ1 /2 = 60◦ . This relatively simple calculation is aimed at illustrating the way in which energy minimization arguments may be used to deduce the structure and energetics of triple points which are yet another ingredient in our overall collection of defects used to build up material microstructures.

9.5 Diffuse Interfaces Our thinking on the treatment of interfaces has been largely inspired by atomiclevel understanding. In particular, we have acceded to the atomistically motivated picture of an interface as a sharp line of demarcation between distinct regions. On the other hand, as will become more evident in the next and subsequent chapters, there are advantages to adopting a continuum view of interfaces as regions over which certain continuum ﬁeld variables suffer rapid spatial variations. This idea will serve as the basis for the general class of phase ﬁeld models that have been used in settings ranging from the analysis of grain growth to the patterns that arise during the process of solidiﬁcation. To be concrete, though not detailed, we consider the case of a two-phase microstructure in which two distinct crystalline phases coexist. One way of characterizing the state of such a system is by recourse to an ‘order parameter’ ﬁeld which we denote η(x). Imagine that within one of the phases, this order parameter takes the value 1, while in the other phase it is assigned a value 0. The phase ﬁeld treatment of interfaces is indicated schematically in a simpliﬁed one-dimensional form in ﬁg. 9.50. What we note is that there are three distinct regions. First, there is a region in which η(x) = 1, second a region over which η(x) = 0 and most importantly for the purposes of the present discussion, there is a region over which the ﬁeld η(x) is making the transition from η(x) = 1 to η(x) = 0. Though we cannot necessarily assign a precise location to the interface, we can say that the interface occupies that region over which dη(x)/d x = 0. The discussion given above illustrates how the question of ‘structure’ at interfaces is handled within the phase ﬁeld setting. In addition to these structural questions, the phase ﬁeld concept allows for a treatment of interfacial energetics.

502

9 Wall Defects in Solids

Fig. 9.50. Schematic representation of the use of continuous ﬁelds to represent grain boundaries. In particular, the interfacial region is characterized by gradients in the order parameter η.

In particular, again in keeping with the simpliﬁed one-dimensional framework suggested above, these can ideas can be endowed with an energetic interpretation by introducing an energetics of the form E[η(x)] =

dη κ dx

2 d x.

(9.28)

This functional introduces an energetic penalty associated with those parts of the distribution of η(x) involving gradients. The parameter κ is a material parameter that characterizes the severity of the penalty associated with a given interface. The energy functional given in eqn (9.28) is a simpliﬁed version of one of the key terms in the overall free energy functional that is used in the derivation of the so-called Cahn–Hilliard equation which will be taken up in chap. 12. We note that the present section has only sketched some of the key ingredients in the phase ﬁeld approach to modeling interfaces and that a detailed description of these ideas will have to await later chapters.

9.6 Modeling Interfaces: A Retrospective This chapter has argued for the critical role of interfacial defects in solids. We have favored an artiﬁcial classiﬁcation into three primary types of interfacial defects, namely, surfaces, stacking faults and twins, and grain boundaries. In each of these cases, it has been argued that a continuum description of the energetics of such

9.7 Further Reading

interfaces may be marshaled through an appeal to equations of the form γ (n)d S, E int =

503

(9.29)

∂

where γ (n) is a generic interfacial energy which depends upon the particular interfacial plane. As evidenced by the various discussions throughout the present chapter, despite the seeming innocence of introducing quantities such as γ (n), the structure and energetics of interfaces is a complex problem when viewed from the atomic scale. In retrospect, it is clear that the energetics of the three different interfacial types considered here can be grouped. In particular, we have found an energetic ranking of the form γsurf > γgb > γ S F .

(9.30)

Ultimately, this ranking of energies could be rationalized on the basis of bond counting arguments in which we examine the extent to which atoms in the interfacial region have lost their partners. 9.7 Further Reading Generalities on Interfaces The Physics of Low-Dimensional Semiconductors by John H. Davies, Cambridge University Press, Cambridge: England, 1998. Chapter 4 of Davies’ book considers the properties of quantum wells and elaborates on some of the arguments concerning conﬁnement given earlier in the present chapter. Surfaces The literature on surface science is vast, and well represented in a number of different books and review articles. Here I give a few that have been most useful or enjoyable to me. Physics at Surfaces by A. Zangwill, Cambridge University Press, Cambridge: England, 1988. Zangwill’s book is thoughtfully constructed and wide in its coverage. He passes freely between questions of geometrical and electronic structure, the adsorption of atoms at free surface and the properties implied by the presence of surfaces. ‘Surface Reconstructions’ by D. King, in Physics World, 2, 45 (1989). This brief article is characterized by plain English and excellent pictures that take the reader right to the crux of the geometries that attend surface reconstruction. ‘Reconstructions and Relaxations on Metal Surfaces’ by J. E. Inglesﬁeld, in Prog. Surf. Sci., 20, 105 (1985). By now this article is somewhat dated, but still

504

9 Wall Defects in Solids

gives an introduction to issues faced in considering the reconstructions on Au, Pt and W surfaces. Inglesﬁeld’s article can be contrasted with ‘Scanning tunneling microscopy studies of metal surfaces’ by F. Besenbacher, in Rep. Prog. Phys., 59, 1737 (1996). This article is full of beautiful pictures substantiating our claim that the scanning tunneling microscope has revolutionized our knowledge of surface structure. Two complementary articles related to semiconductor surfaces are ‘Scanning tunnelling microscopy of semiconductor surfaces’ by H. Neddermeyer, in Rep. Prog. Phys., 59, 701 (1996) and ‘Theory of semiconductor surface reconstruction’ by G. P. Srivastava, in Rep. Prog. Phys., 60, 561 (1997). The article on scanning tunneling microscopy applied to semiconductor surfaces is replete with pictures of some of the huge variety of surfaces that have been considered in semiconductor systems. Physics of Crystal Growth by A. Pimpinelli and J. Villain, Cambridge University Press, Cambridge: England, 1998. This book is included here because it has an interesting discussion both of surface reconstructions and, more importantly, of the elastic theory of interactions between steps. Grain Boundaries Interfaces in Crystalline Materials by A. P. Sutton and R. W. Ballufﬁ, Oxford University Press, Oxford: England, 1995. An enormous compendium with broad coverage on interfacial structure, energetics, deformation, segregation and everything else. This book should be seen as doing for the study of interfaces what Hirth and Lothe (1992) did for the study of dislocations. This is the reference on interfaces. Materials Interfaces edited by D. Wolf and S. Yip, Chapman Hall, London: England, 1992. This book is a compilation consisting of articles by leading practitioners on all aspects of interfaces in solids. ‘The Inﬂuence of Grain Boundaries on Mechanical Properties’ by J. P. Hirth, Met. Trans., 3, 3047 (1972). Hirth offers a variety of insights on the role of grain boundaries in dictating mechanical properties. Miscellaneous Fractography – Observing, Measuring and Interpreting Fracture Surface Topography by Derek Hull, Cambridge University Press, Cambridge: England, 1999. Hull’s book is excellent whatever criterion is used to judge it. I include it here since fracture surfaces are another type of interface that emerges in considering solids.

9.8 Problems

505

9.8 Problems

1 Energetics of fcc Surfaces Using Pair Potentials In eqn (9.6) we revealed the surface energy for an fcc (100) surface in the near-neighbor pair potential approximation. Deduce analogous results for the (110) and (111) fcc surfaces.

2 Energetics of Surfaces Using Pair Functionals Use the Johnson embedded-atom analysis to compute the energies of the (111) and (110) surfaces in fcc materials. Carry out a ranking of the relative magnitudes of the (100), (110) and (111) surfaces using these potentials.

3 Energetics of Surfaces Using Stillinger–Weber Potentials Compute the energy of the unrelaxed and unreconstructed (100) surface in Si. Next, use either static energy minimization or molecular dynamics to relax this surface and examine the resulting reconstruction.

4 Geometry and energetics of stacking faults In this problem, you will investigate the geometry and energetics of stacking faults in fcc crystals. (a) Construct a histogram which shows the number of neighbors that a given atom has as a function of distance to these neighbors. ˚ Identify all neighbor First, make such a plot for fcc Cu (a0 = 3.61 A). ˚ (b) Next, repeat the same exercise for a shells out to a distance of 5.0 A. twinned conﬁguration. In particular, make two graphs, one for the atoms right at the twin plane, and one for the atoms one layer away from the twin plane. Compare the distribution of neighbors with those in the perfect crystal. Without doing any calculation, what will the twin fault energy be for the Morse potential for Cu that was derived in problem 2 of chap. 4? (c) Carry out the same procedure as in part (b), but now for the intrinsic stacking fault. Again, comment on the energy of such a fault as implied by the Morse potential. What do you conclude about the nature of the interactions that are responsible for the stacking fault energy? (d) Use an embedded-atom potential of the Johnson form (see chap. 4) and compute the stacking fault energy.

506

9 Wall Defects in Solids

5 Effective Hamiltonian for Stacking Fault Energy In the discussion culminating in eqn (9.18), we described the use of an Isinglike effective Hamiltonian for the description of fault energies. Show that if we use eqn (9.18) in the case when n max = 2 then the energy of a twin is given by E twin = 2J1 + 4J2 , the energy of an intrinsic stacking fault is given by E intrinsic = 4J1 + 4J2 and the energy of an extrinsic stacking fault is given by E extrinsic = 4J1 + 8J2 . Note that the extrinsic fault energy was worked out in the chapter to illustrate how to make such calculations. 6 Atomic-Level Simulation of Grain Boundary Structure Use the Johnson potential to simulate the structure of a '5 symmetric tilt boundary with a (001) rotation axis. In particular, ﬁnd the relaxed structure associated with the '5 boundary shown in ﬁg. 9.41. 7 Treatment of the Structure and Energetics of Triple Junctions (a) Our discussion of triple junctions in this chapter was intentionally simpliﬁed such that the equilibrium structure was presumed to depend only on a single geometric parameter. In this problem, generalize the treatment given in the chapter such that the triple junction has a position characterized by two parameters, namely, its x and y coordinates. (b) Write down the equilibrium condition in the case in which the interfacial energies differ for the three boundary segments.

TEN

Microstructure and its Evolution

We have made no secret of the pivotal role played by various geometric structures within materials in conspiring to yield observed properties. However, one of the abiding themes of our work thus far has been the observation that this notion of ‘structure’ is complex and scale-dependent. The properties of materials depend upon geometry not only at the microscopic scale, but at larger scales as well. Recall that the hierarchy of geometric structures that populate materials begins with the underlying atomic arrangements. Questions of structure at this level are answered through an appeal to phase diagrams in the way considered in chap. 6. These atomic-level geometries are often disturbed by the various defects that have served as the centerpiece of the previous three chapters, and which introduce a next larger set of length scales in the hierarchy. However, much of the effort in effecting the structure–properties linkage in materials science is carried out at a larger scale yet, namely, that associated with the various microstructures within a material. The current chapter has as its primary aim a discussion of some of the many types of microstructures that populate materials and how such microstructures and their temporal evolution can be captured from a theoretical perspective. This discussion will also serve as the basis of our later efforts to examine the connection between structure and properties in materials. We begin with an attempt at microstructural taxonomy with the aim being to give an idea of the various types of microstructures that arise in materials. Once we have built up an overall impression of the empirical backdrop concerning microstructures in materials, we will attempt to consider how modeling can be brought to bear on a few representative examples. Because of the vast diversity in different microstructures and materials, we will not attempt anything like an exhaustive discussion of microstructural evolution. Rather, through the device of considering a few well-placed examples, our hope is to give an impression of the types of questions that can be posed, and the theoretical machinery that might be used to address them. 507

508

10 Microstructure and its Evolution

10.1 Microstructures in Materials We begin with a brief overview that attempts to make sense of the wide variety of microstructures that are found in materials (primarily metallic). This part of our task should be seen as taxonomical: we aim to observe and classify with the hope that certain classes of microstructures will suggest broad classes of models. The observations of these structures will then be supplemented by an analysis of how by exploiting the twin strategies of heating and beating a material, microstructures can be tailored to a desired form. Microstructural taxonomy has reached a sufﬁcient level of sophistication that it is possible to identify certain broad classes of microstructure. Before beginning, however, it is necessary to reiterate what this chapter is not. Our primary emphasis will be on metals. The majority of experimental data to be highlighted will be drawn from the metallurgical literature with occasional reference to nonmetallic precipitates within such metals. This is not to say that other material systems are without interesting microstructures. On the contrary, the subject is so vast as to have escaped even a modicum of competency on the part of the author. 10.1.1 Microstructural Taxonomy Evidence for the existence of microstructures is often present even at those scales that can be discerned by the naked eye. This claim is substantiated in ﬁg. 10.1 which shows the microstructures of turbine blades associated with different generations of casting technology. The leftmost ﬁgure in the group reveals a series of grains that appear statistically homogeneous. The basic observation is that a generic crystalline solid will be composed of many different grains, each with a particular crystalline orientation and separated by grain boundaries. The entirety of these grains and the associated boundaries make up the polycrystalline microstructure. Polycrystals of this sort are but one example of the types of microstructures that can be found. The second picture in the sequence in ﬁg. 10.1 reveals an anisotropic microstructure in which the grains are elongated along a preferred direction. The ﬁnal picture in this sequence, though remarkable as a single crystal of enormous proportions, is perhaps less interesting as a representative example of a material with microstructure. Microstructure in Single Phase Polycrystals. We begin with a discussion of the simplest microstructure (at least to characterize geometrically) in which the grain size is the dominant microstructural parameter. We are all used to the idea that the technologies that surround us are constrained by various codes which attempt to standardize products and the processes used to realize them. Such codes exist for everything ranging from skyscrapers to microwave ovens. It is

10.1 Microstructures in Materials

509

Fig. 10.1. Microstructures for turbine blades produced using different casting technologies.

less evident, however, that there might exist codes that serve to standardize the discussion of microstructure as well. The ASM has standardized this ﬁeld in a way that is revealed in the Metals Handbook (ASM 1972) and which we show in ﬁg. 10.2. The frames of ﬁg. 10.2 show some representative examples of different grain structures in steel. The distinguishing feature from one frame to the next is the grain size. For the case shown here which is for a class of low-carbon steels, the grains range in size from roughly 10 µm to 250 µm. Recall that these observations are more than idle musings since, as was noted earlier (see ﬁgs. 1.3 and 8.2), the grain size normally has a direct impact on mechanical properties such as the yield strength. Already, there are many questions that might be asked concerning the microstructures shown in ﬁg. 10.2. First, we note that the two-dimensional cross sections shown here can be deceptive. One of the most frustrating features in studying solids and one of the largest challenges that must still be fully owned up to is the difﬁculty of attaining three-dimensional understanding of the various structures that populate materials. As a step in this direction, we interest ourselves in different ways of characterizing a material’s microstructure. As is evident from the ﬁgures discussed above, the microstructure is characterized by an element of randomness. On the other hand, there are also key elements of statistical regularity which may be exploited. Note that in the discussion given above, we have only made reference to the average grain size which is the simplest gross parameter for

510

10 Microstructure and its Evolution

Fig. 10.2. Representative examples of ASTM grain sizes in low-carbon steel: (a) grain size 2 (≈ 180 µm), (b) grain size 5 (≈ 60 µm), (c) grain size 7 (≈ 30 µm), (d) grain size 10 (≈ 10 µm). Mean grain sizes associated with each microstructure are given in parentheses.

characterizing a material’s microstructure, and that which enters into many of the simple empirical scaling models of material response. The microstructure described above may be seen as the most homogeneous limit of those we will consider here. A complementary set of information concerning microstructures of the type featured above can be obtained by mapping the orientations of the various grains making up the polycrystal. The basic idea is that one may determine the preponderance of different crystal orientations. The new technique of orientation imaging microscopy now allows for the determination of such orientational information with high spatial resolution. An example of the type of results that are obtained via this technique is shown in ﬁg. 10.3. Precipitates and Inclusions. The presence of more than a single species in a material makes it possible that a given microstructure will be far richer than that described above. In particular, by virtue of the presence of several species coupled

10.1 Microstructures in Materials

511

Fig. 10.3. Orientation imaging microscopy image of a partially recrystallized low-carbon steel. The leftmost ﬁgure is an image quality map in which the image quality obtained from the diffraction pattern is mapped onto a gray scale. The middle ﬁgure shows the orientation of the various grains with respect to the normal plane of the sample and the correspondence between colors and orientation is effected via the crystallographic triangle shown on the right of the ﬁgure (courtesy of Stuart Wright).

with the operation of diffusion giving the different atom types the possibility of redistributing, it is possible to have microstructures that are mixtures of different phases. The geometric framework that will serve as the basis of our analysis of these microstructures is that of a ‘matrix’ material that is punctuated by the presence of second-phase particles. In this section, our primary aim is to take stock of the qualitative features of such microstructures and to foreshadow some of the physical properties that are inherited because of them. One of the ﬁrst comments we must make in describing such structures from the standpoint of the modeler is the need to distinguish between coherent and incoherent second-phase particles. The key point is that the constraint of coherency (i.e. the two phases join up smoothly across the interface) implies an attendant possibility for signiﬁcant internal stresses. In ﬁgs. 10.4, 10.5 and 10.6, we show a few different examples of the microstructures involving second-phase particles that arise within different contexts. One feature of these examples that begs an explanation is that of the widely different morphologies exhibited in different cases. Second phase particle shapes range from nearly spherical, to faceted, to highly elongated rods and ultimately, plates and needles. A very useful compendium on some of the variety to be found in precipitate microstructures is Russell and Aaronson (1978). As will be seen later, the simplest model of the equilibrium shapes of such precipitates is based on an isotropic interfacial energy and leads to the expectation of spherical particles.

512

10 Microstructure and its Evolution

Fig. 10.4. Rod-shaped precipitates in Cr–Nb alloy (courtesy of Sharvan Kumar). The precipitates are Cr2 Nb and have the C15 Laves phase crystal structure.

Fig. 10.5. Al2 Cu (θ ) precipitates in Al (courtesy of Bob Hyland).

As the ﬁgures indicate, the most naive theoretical intuition is incomplete. Below we will take up the challenge of how to explain the origins and characteristics of these microstructures. In addition, in chap. 11, we will examine the way in which a distribution of second-phase particles can alter the mechanical properties of a material. Lamellar Microstructures. The precipitate microstructures described above have a geometric distribution such that a description in terms of a background matrix that is riddled with second-phase particles is appropriate. A second class of multiphase microstructure is lamellar microstructure like that shown in ﬁg. 10.7. To better

10.1 Microstructures in Materials

513

Fig. 10.6. As cast microstructure of Cu–O alloy with 0.78% oxygen content. The dendritic regions are Cu2 O. Micrograph 2257 from Metals Handbook (ASM 1972).

appreciate the nature of these microstructures, we begin by referring once again to the iron–carbon phase diagram as given in ﬁg. 1.5 in which it is seen that in the low-carbon concentration limit, we should expect the presence of both α-Fe (also known as ferrite) and Fe3 C. The presence of both of these constituents together gives rise to a lamellar microstructure like that considered here. The basic idea is the emergence of structure on a few different scales. At the larger scale are overall colonies (or grains) within which the α-Fe and Fe3 C have the same orientation relationship. The structure within such a grain is characterized by an alternation between α-Fe and Fe3 C regions. This characteristic morphology is revealed in ﬁg. 10.7. From the perspective of constructing models of such microstructures, both for their evolution and their impact on material properties, it is clear that this is a completely different class of problems than those built around second-phase particles. The diversity of the various microstructures we have considered thus far is depicted schematically in ﬁg. 10.8. From a structural perspective, these different structures permit interpretation crystallographically in terms of the various phases that make up the microstructure. A different class of microstructural feature can arise by virtue of the presence of dislocations. Organization and Patterning of Dislocations. As a result of deformation, the dislocations present in a given material form structures. These structures bear no resemblance to the featureless and homogeneous dislocation arrangements that might be thought of at ﬁrst blush. Nor, as remarked above, do these structures

514

10 Microstructure and its Evolution

Fig. 10.7. Lamellar pearlite microstructure of a hot rolled steel bar. Micrograph 354 from Metals Handbook (ASM 1972). This ﬁgure is at a magniﬁcation of 2000×.

Fig. 10.8. Classiﬁcation of various two-phase microstructures (adapted from Hornbogen (1984)).

10.1 Microstructures in Materials

515

Fig. 10.9. Transmission electron microscopy image revealing the organization of dislocations in single-crystal Cu into a labyrinthine pattern as a result of cyclic loading (adapted from Suresh (1998)).

admit of the relatively clear cut interpretation offered for the several microstructural types introduced above. The dislocation structures found in materials exhibit even more remarkable patterning as is evident when the loading to which the material is subjected is cyclic. In this case, the repeated loading allows the formation of yet sharper and more organized structures such as those shown in ﬁg. 10.9.

Microstructure at Surfaces. Our previous discussion has emphasized the microstructures that are present in generic bulk crystals. On the other hand, with the increasing reliance on layered materials in a variety of contexts including microelectronics (also revealed in ﬁg. 10.8) and in particular, on thin ﬁlms, a new generation of microstructures has grown up which are to a large extent two-dimensional. Though there is much that can be said on this point, we but mention them so as to signal the reader to the need for thinking in these areas as well. Because of the conﬂuence of high-quality growth systems and attendant surface probes, one area of especial interest is that of the variety of ‘self-organized’ microstructures that are seen during growth. A particular example in the Si–Ge system is shown in ﬁg. 10.10. Thus far, our discussion has centered on some of the qualitative geometric and chemical features of microstructures found in different classes of materials. Now that we have seen in broad brush strokes the classiﬁcations that are possible, we turn to the question of how such microstructures can be produced by appropriate processing strategies, and what the consequences of such microstructures are to the underlying physical properties of a material.

516

10 Microstructure and its Evolution

Fig. 10.10. Atomic force microscopy image of an island array in Si80 Ge20 alloy grown on Si(001) (courtesy of J. Floro and Eric Chason). The morphology is built up of pyramidal ‘hut’ clusters with (501) facets.

10.1.2 Microstructural Change Until now, our microstructural description has been geometric and qualitative without any real discussion of how such microstructures are prepared. Tuning microstructures is one of the oldest forms of engineering and may be traced to the historic ages when chemical impurities were used to harden metallic materials, though the microstructural understanding that went with these processes was clearly not present. The key insight, and the thrust of the present section, is the recognition that by subjecting a material either to deformation or heating or both, the underlying microstructure may be altered, another reminder that in dealing with microstructures we are treating nonequilibrium phenomena. As has already been mentioned, entire historic ages may be thought of as having emerged from particular types of microstructural control. Microstructural change occurs both intentionally and by accident. No doubt, most readers of this book have been confronted with the rusted remains of some favorite gadget – the terminal state of what was once a metastable arrangement. Despite the apparent permanence of many materials on everyday time scales, when viewed over longer times they are seen to be teeming with activity. Our present discussion aims to describe a few different processing histories, with an eye to explaining the way in which such processing steps alter a given microstructure. The particular modeling strategies for describing these processes will be taken up in turn as the chapter proceeds. Traditional metallurgy is sometimes derogatorily referred to as the science of ‘heat and beat’ where the tandem operations of annealing and working the material via a sequence of carefully selected, albeit often empirically derived,

10.1 Microstructures in Materials

517

processing steps are used to obtain some desired properties. On the other hand, the importance of thermomechanical processing to everyday materials technology cannot be underestimated. In addition, the processes that transpire under these circumstances provide a wide range of problems that any complete theory of nonequilibrium processes must answer to. Working a Material (Beat) Generically, beating a material refers to the act of subjecting a material to plastic deformation via processes such as systematic stretching or through cyclic loading. One of the particular means whereby materials are deformed in the name of reaching some desired ﬁnal shape or microstructure is that of rolling. The principal idea is to take the specimen and to subject it to preferential deformation which tends to elongate and squish it, for example. In ﬁg. 10.11, we show two snapshots in the deformation history of a sample of tungsten which has been subjected to such rolling processes. In this instance, it is seen that one of the primary outcomes of the deformation process is the elongation of the underlying grain structure. In addition, the working of the material is also attended by microstructural change at the dislocation level in that the dislocation density can be increased by orders of magnitude. The increase in dislocation density is attended by changes in the mechanical properties. An indication of the relation between plastic strain and dislocation density was already given in ﬁg. 8.40. What that ﬁgure showed was the way in which by virtue of the working of a material, dislocations are stored in that material. We have also already noted (see ﬁg. 8.2) that these microstructural changes are attended by concomitant changes in the properties of the material. Annealing a Material (Heat) In a worked material, the microstructure is characterized by a series of heavily dislocated grains. As was evidenced in our discussion of dislocations in chap. 8, such microstructures are inherently metastable. If the material is heated, a series of discernible changes will occur. An obvious example of this type of outcome is shown in ﬁg. 10.12 in which it is seen that in the vicinity of a weld, the grain structure is completely different than in those regions far from the heating. Systematic investigation of the properties of materials subject to annealing have resulted in a convenient classiﬁcation of the processes undergone within the solid. In particular, it has been found convenient to separate these changes into three separate processes, namely, recovery, recrystallization and grain growth. The onset of recovery can be discerned in electrical resisitivity measurements in which it is found that the resistivity decreases as a function of time, signaling a decrease in the number of scattering centers. There are a number of different mechanisms that can be associated with the recovery process, one of which corresponds to the removal

518

10 Microstructure and its Evolution

Fig. 10.11. Grain structure of tungsten polycrystals. Upper ﬁgure shows polycrystal with equiaxed grain structure while lower ﬁgure illustrates polycrystal that has suffered deformation via wire drawing (courtesy of Clyde Briant).

of point defects from the material. The recrystallization stage is characterized by a reduction of the net dislocation density, with the development of grains which are relatively dislocation-free. Finally, in the grain growth stage, the mean grain size increases with a corresponding reduction in the total grain boundary area. All of these processes are further elaborated in both Martin et al. (1997) and Humphreys and Hatherly (1995). In addition to processes involving the alteration of the defect structures within a material upon heating, it is also clear that by altering the temperature, phase changes can be induced as well. Indeed, the control of the relative proportions of different phases within a material is one of the primary ways that microstructural

10.1 Microstructures in Materials

519

Fig. 10.12. Illustration of changes in microstructure that attend the welding process in a copper cold rolled bar. Adapted from micrograph 2307 in Metals Handbook (ASM 1972).

control is exercised. As we have already mentioned, one of the scenarios in which phase transformations are sure to occur is that in which there is the potential for precipitation reactions due to an overabundance of some foreign atoms. With increasing temperature, the likelihood of diffusion increases and with it the possibility that atoms can organize into precipitates. With increasing time at elevated temperature, the size of such precipitates can increase due to coarsening effects.

10.1.3 Models of Microstructure and its Evolution We now wish to undertake an examination of various case studies in the analysis of microstructure. Perhaps the simplest example is that of a single second-phase particle in an otherwise homogeneous medium. For many purposes, this problem serves as the starting point for subsequent analyses, and ﬁnds its way into the analysis of problems ranging from two-phase microstructures to the effective properties of polycrystals. Our analysis will begin with one of the key elastic models of material microstructure, namely, the problem of the Eshelby inclusion. One direct route to the properties of this solution is to consider an elastically homogeneous medium (i.e. the same elastic properties throughout) but for which a certain region has undergone a transformation strain. Using the Green function techniques developed in earlier chapters, it is then possible to deduce the elastic ﬁelds associated with such an inclusion. Once we have deduced the elastic consequences of second-phase particles, we will be in a position to examine questions of both the nucleation and subsequent evolution of such particles, with special attention being given to the equilibrium sizes and shapes attained by these particles. The second modeling centerpiece considered in this chapter will be our discussion of martensitic microstructures. This work is offered on the basis of our

520

10 Microstructure and its Evolution

contention that this theory offers much of the analytic insight that one might hope to ﬁnd in models of more generic microstructures. In particular, by virtue of the conjunction of kinematic and energetic arguments, the theory of martensitic microstructure to be offered here is able to make detailed predictions about these microstructures, including the fractions of different martensitic variants that are to be expected. The discussion will be rounded out by our taking stock of microstructural evolution as seen from the more traditional metallurgical viewpoint. In particular, grain growth will be taken up from a theoretical perspective. This discussion should be seen as a continuation of those given in the previous chapter since the attempt to understand these phenomena rests heavily on a synthetic understanding of point, line and interfacial defects in concert. Our contention will be that despite the exertion of Herculean efforts, a number of key difﬁculties remain.

10.2 Inclusions as Microstructure As noted many times already, phase diagrams instruct our intuition concerning the temporal evolution of certain metastable states. In particular, for the case in which one has a supersaturation of foreign atoms, one is led to expect that if the atoms have sufﬁcient mobility, sooner or later they will ﬁnd each other out and colonize new phases, namely, precipitates. Examples of some of the resulting microstructures were shown in ﬁgs. 10.4, 10.5 and 10.6. We also note that by virtue of particular thermomechanical histories (i.e. by suitable processing) the nature and distribution of these precipitates may be tailored to yield desirable physical properties. For the purposes of the present discussion, one of our ambitions is to consider a class of second-phase microstructures in which the two phases are coherent. In these instances, the constraint of coherency carries with it an elastic penalty which results in elastic distortions in both the precipitate particle and the matrix material surrounding it. As a preliminary to the concrete mathematical investigation of such structures, we must ﬁrst learn something of the elastic consequences of a single inclusion.

10.2.1 Eshelby and the Elastic Inclusion The elastic solution upon which many approaches to the consideration of microstructure are built is that of the so-called Eshelby inclusion in which one considers a single ellipsoidal inclusion in an otherwise unperturbed material. From the standpoint of the linear theory of elasticity, this problem is analytically tractable

10.2 Inclusions as Microstructure

521

Fig. 10.13. Schematic of an ellipsoidal inclusion within an elastic medium.

and provides valuable insights concerning the stresses in adjacent grains and the compatibility issues that must be faced at the interfaces between such grains. Our intention in the present section is to examine the elasticity solution to the problem of a single elastic inclusion and to attempt to use the insights afforded by this solution to learn something about that class of microstructures that can be thought of in terms of inclusions. Our starting point is the notion of an eigenstrain as discussed already in chap. 2. We picture an elastically homogeneous medium (i.e. the elastic moduli are the same throughout) with some spatial region that has undergone a strain ∗ as indicated schematically in ﬁg. 10.13. The philosophy espoused in the method of eigenstrains is that the presence of these eigenstrains may be thought of as giving rise to some distribution of body forces. However, as we have already shown repeatedly, once such a distribution is speciﬁed, the elastic Green function may be invoked to write down the displacement ﬁelds as an integral over this distribution. In the present setting, this argument proceeds as follows. The equilibrium equations of elasticity may be written as ∇ · σ e = 0,

(10.1)

where the superscript e refers to the fact that it is only the elastic part of the strain that gives rise to stresses. However, this statement of equilibrium may be rewritten on the basis of the observation that the total strain is given by tot = e + ∗ . In particular, we have tot ∗ Ci jkl kl, j − C i jkl kl, j = 0.

(10.2)

Recall that the distribution of eigenstrains is prescribed and hence the term

522

10 Microstructure and its Evolution

∗ ∗ Ci jkl kl, j is known. If we make the transcription C i jkl kl, j = − f i , where f i is the th i component of a ﬁctitious body force ﬁeld, then our problem has been mapped onto a boundary value problem for the unknown total displacement,

Ci jkl u tot k,l j = − f i .

(10.3)

For the particular case of interest below, we imagine an inﬁnite body and an associated condition that the ﬁelds vanish at inﬁnity. As already remarked, once the body force distribution has been speciﬁed, by invoking the elastic Green function, the displacement ﬁelds are immediately obtained as the integral tot ∗ 3 (10.4) u k (x) = − Cmjpl pl, j G km (x − x )d x .

For our present purposes, we assume that the eigenstrain of interest is uniform throughout the region . Using integration by parts, the differentiation on the eigenstrain itself can be pushed onto the Green function with the result that tot ∗ u k (x) = Cmjpl pl G km, j (x − x )d 3 x . (10.5)

Note that the differentiation of the Green function is with respect to the primed variables. We can now use the relation ∂ ∂ G km (x − x ), (10.6) G km (x − x ) = − ∂ xj ∂ xj to rewrite our expression for the displacements as tot ∗ G km, j (x − x )d 3 x , u k (x) = −Cmjpl pl

(10.7)

where in this instance the differentiation of the Green function is with respect to the unprimed variables. Thus far, our results are primarily formal. As an exercise in exploiting the formalism, we will ﬁrst examine the ﬁelds associated with spherical inclusions, and then make an assessment of the elastic strain energy tied to such inclusions. These results will leave us in a position to consider at a conceptual level the nucleation, subsequent evolution and equilibrium shapes associated with inclusion microstructures. To compute the displacements and strains associated with an inclusion explicitly, we must now carry out the operations implied by eqn (10.7). To make concrete analytic progress, we now specialize the analysis to the case of an elastically isotropic solid. As a preliminary to the determination of the elastic ﬁelds, it is necessary to differentiate the elastic Green function which was featured earlier as

10.2 Inclusions as Microstructure

523

eqn (2.91). In particular, if we evaluate the derivative of G km with respect to x j , we ﬁnd G km, j (x − x ) =

(x j − x j ) 1 −(λ + 3µ)δkm 8π µ(λ + 2µ) |x − x |3 (xk − xk ) (xm − xm ) + (λ + µ)δk j + (λ + µ)δ m j |x − x |3 |x − x |3

(xm − xm )(xk − xk )(x j − x j ) , − 3(λ + µ) |x − x |5

(10.8)

a mess that can be simpliﬁed considerably if we follow Mura (1987) in adopting the notation li = (xi −xi )/|x−x |. In particular, contracting this expression to form ∗ G km, j as is demanded by our expression for the displacements, eqn (10.7), Cmjpl pl we ﬁnd that the displacements can be written as ∗ pl

d 3 x (µδkl l p + µδkp ll − µδ pl lk + 3(λ + µ)lk l p ll ). 4π(λ + 2µ) |x − x |2 (10.9) Our ﬁrst exercise in computing the displacements themselves will be to consider the ﬁelds due to a spherical inclusion with a dilatational eigenstrain of the form i∗j = 0 δi j and with radius a. In this case, the contraction implied by the presence of the δi j simpliﬁes considerably such that u tot k (x)

=

∗ Cmjpl pl G km, j

0 3λ + 2µ (xk − xk ) =− , 4π λ + 2µ |x − x |3

(10.10)

and hence the computation of the displacements reduces to the evaluation of the integral (xk − xk ) 3 0 3λ + 2µ tot d r. (10.11) u k (x) = 3 4π λ + 2µ |x − x | For the sake of checking the correspondence of our present results with those favored by others where the elastic constants µ and ν are used, we note the identity (3λ + 2µ)/(λ + 2µ) = (1 + ν)/(1 − ν). Note that in light of these results, the determination of the elastic displacements has been reduced to the evaluation of a geometric integral over the inclusion itself. For an isotropic solid with a spherical inclusion, the displacements ﬁelds are themselves spherically symmetric. As a consequence, without a loss of generality, we can evaluate the u 3 component of displacement along the z-axis, resorting to spherical coordinates to simplify the integrals. By symmetry, this is equivalent to the radial component of displacement,

524

10 Microstructure and its Evolution

Fig. 10.14. Radial displacements associated with a spherical inclusion for which the eigenstrain is given by i∗j = 0 δi j . Displacements have been cast in dimensionless terms.

u r (r ). In particular, the expression for the displacements reduces to a π 0 3λ + 2µ r − r cos θ tot 2 r dr sin θ dθ . u r (r ) = 3 2 λ + 2µ 0 0 (r 2 + r 2 − 2rr cos θ ) 2 (10.12) For a point outside of the inclusion, evaluation of the requisite integrals results in 0 a 3 3λ + 2µ tot u r (r ) = . (10.13) 3r 2 λ + 2µ Similarly, if we are to evaluate the displacements within the inclusion, it is found that 0r 3λ + 2µ tot , (10.14) u r (r ) = 3 λ + 2µ indicating that within the inclusion the strain is constant, as was hinted at earlier. The displacement as a function of the radial coordinate is shown in ﬁg. 10.14. From the point of view of our efforts to examine the energetics of microstructures, our assessment of the elastic ﬁelds due to inclusions must be supplemented with insights into their energies. In light of our success in deducing the elastic ﬁelds, it is relatively straightforward to compute the strain energy associated with such an inclusion and the most naive approach is to add up the elastic energy throughout the entire medium via 1 E elastic = σi j iej d V, (10.15) 2 where denotes the entire region of matrix and inclusion. (A simpler scheme for carrying out this evaluation of the elastic strain energy is reserved for the problem

10.2 Inclusions as Microstructure

525

section at the end of this chapter.) Note that the integral demands a knowledge of the elastic strain. Since our calculations have yielded the total displacement, there is a bit of work needed to recast our results in a form that is suitable for the determination of the elastic energy. In particular, we ﬁnd it most convenient to work with an alternative form for the strain energy density, namely, ν 1 ∗ tot ∗ 2 tot ∗ 2 . (10.16) σi j (itot [tr( − ) = µ ( − ) + − )] j ij ij ij 2 1 − 2ν Note that we have resorted to the use of µ and ν for our description of the elastic properties for ease of comparison with many of the expressions that appear elsewhere. In order to compute the total elastic energy, we separate the volume integral of eqn (10.15) into two parts, one which is an integral over the inclusion, and the other of which is an integral over the matrix material. The reason for effecting this separation is that, external to the spherical inclusion, the displacements we have computed are the elastic displacements. On the other hand, within the inclusion, it is the total ﬁelds that have been computed and hence we must resort to several manipulations to deduce the elastic strains themselves. For the particular eigenstrain chosen here, note that we have i∗j = 0 δi j . Within the inclusion this led to the displacement given in eqn (10.14) which can be differentiated to yield the strain 0 1 + ν in i j = δi j . (10.17) 3 1−ν As a consequence, we ﬁnd that the elastic strain is given by 20 1 − 2ν elastic ∗ δi j . = i j − i j = − i j 3 1−ν

(10.18)

In light of this result, we are now prepared to evaluate the strain energy within the inclusion, which using eqn (10.16) is in = E strain

16πa 3 02 µ (1 − 2ν)(1 + ν) . 9 (1 − ν)2

(10.19)

We are also interested in the elastic energy external to the inclusion. To compute this, we demand the strains outside of the inclusion, which can be simply evaluated on the basis of eqn (10.13) with the result that 20 a 3 1 + ν (10.20) rr = − 3r 3 1 − ν 0 a 3 1 + ν . (10.21) θθ = φφ = 3r 3 1 − ν The elastic energy stored in the region outside of the inclusion may now be

526

10 Microstructure and its Evolution

evaluated in a fashion similar to that invoked to evaluate the energy stored within the inclusion with the result that out = E strain

8πa 3 02 µ (1 + ν)2 . 9 (1 − ν)2

(10.22)

Hence, the total strain energy of the medium is arrived at by summing the contributions from within and outside of the inclusion, and leads to E strain =

8πa 3 02 µ (1 + ν) . 3 (1 − ν)

(10.23)

What we have learned is that the elastic energy associated with a spherical inclusion characterized by an eigenstrain i∗j = 0 δi j scales in a simple way with the volume of the inclusion itself. Similar analytic progress can be achieved for other simple geometries such as ellipsoidal and cube-shaped inclusions. The main point of the efforts described above is that we are now in a position to evaluate the elastic consequences of coherent precipitates as will be necessary in our consideration of equilibrium shapes in coming sections. What we note now is that by virtue of our knowledge of the features of this highly idealized problem and its corresponding solution, we are prepared to make inroads on a variety of problems including that of the coarsening of two-phase microstructures and the effective properties of multiphase media. Despite the insight provided by analytic solutions like those given above, there are many instances in which the geometries, materials and loads are sufﬁciently complex as to defy useful analytic description. Indeed, note that our solution was predicated on the use of a Green function which was itself derived on the assumption of material homogeneity, an assumption which is manifestly not warranted in many cases of interest. In these cases, one must resort to numerical calculation. We have already noted that there is both a synergy and tension between analytic and numerical results. On the one hand, analytic results are highly instructive in that they provide insights into the qualitative dependence of solutions on material and geometric parameters. On the other hand, such solutions are limiting in that they usually do not allow for a treatment of a wide range of geometries. Though the analytic solution set forth here will be of great use for providing insights into the nature of elastic ﬁelds surrounding inclusions, our ultimate discussion of the temporal evolution of precipitate microstructures and their equilibrium shapes will be largely predicated upon numerical schemes for solving the types of elastic boundary value problems posed above.

10.2 Inclusions as Microstructure

527

10.2.2 The Question of Equilibrium Shapes Having now developed a feel for the elastic consequences of the presence of a second-phase particle in a given material, we are poised to investigate the equilibrium morphologies of second-phase particles as well as their temporal evolution. We begin with the question of the equilibrium shapes of coherent second-phase particles which will be expressed as the playing out of a competition between the types of elastic terms considered above and other energetic inﬂuences such as the energy of the interface between the two particles. This type of reasoning is ubiquitous and ultimately rests on the variational character of thermodynamic equilibrium. Of course, such arguments skirt the question of whether or not the particular situation of interest is really an equilibrium state or not. Stated simply, our initial foray into these questions will be predicated upon the idea that in certain cases, microstructures of interest may be thought of as energy minimizers. For the problem at hand, the competition of interest may be expressed in its simplest incarnation with relative ease. If we are to return to the experimental circumstances of interest, our starting point is a situation in which an alloy has been cooled to the point that there is an overabundance of foreign atoms within the host matrix. As a result of the process of diffusion, these foreign atoms collect and begin to form precipitates. However, because of the difference in structure between the matrix and precipitate (this difference in structure may mean nothing more than a different chemical distribution on the same underlying lattice), there is an energy penalty for both the interface between the matrix and the precipitate as well as for the elastic strains induced by this difference in structure. Both of these energies depend, in turn, upon the particle shape as well as upon the arrangements of the precipitates with respect to each other. If we are to consider the simplest case in which a ﬁxed quantity of mass is assigned to the second-phase particle of interest and demand what shape results in the lowest free energy, it is easily imagined that the free energy depends upon those parameters characterizing the shape through a number of different terms. The conceptual underpinnings of our investigation of equilibrium shapes is represented by the formula 1 γ (n)d A + σi j i j d V. (10.24) E tot (shape) = 2 ∂ The ﬁrst term on the right hand side represents the energy cost associated with the interface between the particle and the matrix, and for generality we have assumed (temporarily) that the interfacial energy is anisotropic, a fact that is revealed by the dependence of this energy on the normal n as γ (n). The second term is the elastic energy of the medium by virtue of the presence of the second-phase particle. Note that both of these terms are functionals of the particle shape and our ambition is to

528

10 Microstructure and its Evolution

minimize the energy with respect to the various possible shapes. We note that in the discussion that follows, the use of the term anisotropy will do double service to characterize both the morphological anisotropy of the particles themselves, as well as the crystallographic anisotropy of the various material parameters such as the interfacial energy and the elastic moduli.

10.2.3 Precipitate Morphologies and Interfacial Energy The simplest picture that can be considered for describing equilibrium shapes is predicated entirely on the presence of the interfacial energy. In particular, the elastic energy given in eqn (10.24) is dropped all together and instead, we are left with minimizing γ (n)d A + λ d V, (10.25) E tot (shape) = ∂

where the second term on the right hand side introduces a Lagrange multiplier λ with the constraint of ﬁxed volume. Note that we have ignored the complicating inﬂuence of ﬁnite temperatures. Before continuing with our discussion of the minimizers of this functional, it is important to recall the extent to which the physics it entails can be informed on the basis of microscopic insights. In particular, in light of the discussion of chap. 9, it is clear that microscopic analysis can be used to construct the interfacial energy γ (n). Indeed, both ﬁgs. 9.46 and 11.9 illustrate the dependence of interfacial energy upon the relative orientation of the different crystallites which the interface separates. In the present case, it is the relatively simple generalization of these results to the case in which the interface separates two different phases that is of interest, and we conclude this comment by noting that the microscopic evaluation of these quantities offers no compelling new twists on what we have done before. Though it would take us too far aﬁeld to provide a detailed discussion, we at least mention the idea of the Wulff construction in which the equilibrium shapes of particles are inherited from the properties of the interfacial energy as a function of orientation. The starting point of an analysis of the equilibrium shapes associated with minimizing the interfacial energy is made by appealing to a Wulff plot (or γ -plot) in which a three-dimensional closed surface is constructed with the property that the distance of a given point on that surface from the origin is equal to the interfacial energy associated with the orientation of that point. That is, the surface is speciﬁed as the collection of points r of the form r = γ (n)n. The set of points corresponding to all of the unit vectors n corresponds to the unit sphere. The idea of the γ -plot is to take each such point and to scale its distance from the origin by the corresponding γ (n). Once we are in possession of the

10.2 Inclusions as Microstructure

529

γ -plot, we are then prepared to determine the equilibrium shape itself by recourse to Wulff’s construction which instructs us to convexify the γ -plot with the result that the equilibrium shape corresponds precisely with the resulting polygon (in two dimensions) or polyhedron (three dimensions). Concretely, what this means is that we are to visit each and every normal vector n and to construct a perpendicular plane which passes through the intersection of that normal with the γ -plot. The equilibrium shape corresponds to the inner envelope of this collection of planes. We also make the important point that the resulting equilibrium shape has no dependence on particle size, a conclusion that is at marked odds with observed microstructures. These ideas are elaborated further in the problem section at the end of the chapter. An excellent discussion of these ideas may be found in section 5.4 of Martin et al. (1997). An alternative discussion with more emphasis on the statistical mechanical underpinnings of this problem may be found in Rottman and Wortis (1984). The construction described above now permits us to hint at the relevance of the interfacial energy to the question of equilibrium shapes. Indeed, an example of the outcome of such reasoning in the context of a Cu–Zn alloy is shown in ﬁg. 10.15. The precipitates being evaluated here arose as a result of isothermal heat treatment of supersaturated β phase which resulted in the formation of faceted polyhedra of the γ phase of composition Cu5 Zn8 . The ﬁgure shows various sections through the precipitate centroids associated with γ phase precipitates in the Cu–Zn system. In particular, note that these sections are made through the (100), (111) and (110) planes. The dotted curves in the ﬁgures reveal the Wulff plots associated with these measured particle morphologies. In fact, the reasoning is really run in reverse relative to the usual Wulff argument since in this case it is the shapes that are observed and the γ -plots that are backed out. Nevertheless, our main point in bringing up these issues was to call attention to the ideas used in addressing the case in which the interfacial energy dominates the equilibrium shape.

10.2.4 Equilibrium Shapes: Elastic and Interfacial Energy A more complete description of the question of equilibrium shapes than that given above must account for both of the terms indicated in eqn (10.25). Our strategy in this section is to consider models which synthesize the effects of both interfacial and elastic energy from ever increasing levels of sophistication. As usual, these formulations will illustrate the tension between analytic tractability and physical realism, with the most realistic models almost entirely defying analytic progress. Two-Dimensional Analysis of Johnson and Cahn. For starters, we consider the equilibrium shape for second-phase particles in a two-dimensional setting.

530

10 Microstructure and its Evolution

Fig. 10.15. Series of equilibrium shapes as observed in γ Cu–Zn (solid lines) and estimated values of the interfacial energy vs orientation (dashed lines) (adapted from Stephens and Purdy (1975)). The precipitate sizes are roughly 60 µm for all but the 500 ◦ C case, in which the precipitates have a size on the order of 500 µm.

In particular, we consider a single such particle with a dilatational misﬁt (i.e. i∗j = 0 δi j ) with the restriction that the particle shape derives from only a family of such shapes that can be parameterized in terms of a few simple geometric quantities. In essence, we adopt the Rayleigh–Ritz variational procedure in which the energy function of interest depends upon a ﬁnite set of parameters and with respect to which the energy function is minimized. We follow Johnson and Cahn (1984) in considering the family of elliptical shapes characterized by their area A = πab and aspect ratio a/b. Though it is a point we have raised repeatedly, it is worth reiterating that the space of energy minimizing solutions has been shrunk to include only those that are elliptical. From the standpoint of the quantitative model used to describe this system, we assume that both the matrix and precipitate are elastically isotropic and characterized by the same elastic moduli and that the misﬁt strain associated with the precipitate is purely dilatational and is given by 0 . Further, it is assumed that the interfacial energy γint (n) is isotropic (i.e. γint (n) = γ0 ). Recall from

10.2 Inclusions as Microstructure

531

our discussion in chap. 9 that interfacial energies can vary signiﬁcantly from one crystal face to the next. What is being assumed here is that this variability can be suppressed without losing the essential features of the competition being played out. Of course, these restrictions can be relaxed, and it is interesting to do so. On the other hand, as a tool for illustrating the fundamental ideas being considered here, the simpliﬁcations that attend these assumptions make them highly attractive. As a prelude to writing the dependence of the energy on the particle shape and size, Johnson and Cahn found it convenient to carry out a change of variables which respected important symmetries that this energy must satisfy. For example, the energy should be indifferent to an interchange of the major and minor axes of the ellipse. That is, the energy associated with an ellipse with its long axis along the (10) direction and its short axis along the (01) direction should be no different from the reverse circumstance. These symmetries imply that a more useful set of coordinates are (a − b) √ , 2 (a + b) v= √ . 2

u=

(10.26) (10.27)

In terms of these new variables, the geometric description of the elliptical particles is given by π (10.28) A = (v 2 − u 2 ), 2 which is the area of the particle and U=

a−b u = , v a+b

(10.29)

which provides a measure of the departure of the ellipse from a circle. In order to determine the lowest-energy shape for a given particle size, it is necessary to express the energy in terms of the variables U and A. In principle, what we have learned from the previous two sections permits the construction of an exact energy as a function of these parameters. On the other hand, an alternative idea is to map the exact energy onto an approximate surrogate which has the form of a Landau free energy, well known from the study of phase transitions, which permits us to exploit what is known about such free energies from other contexts. The strategy is to seek an expansion of the energy in powers of U in which the expansion coefﬁcients depend upon the parameter A. Much can be said about the energy minimizing structure on the basis of general symmetry considerations which we will discuss shortly. However, we ﬁrst examine the detailed character of

532

10 Microstructure and its Evolution

these energies themselves. The interfacial contribution to the total energy in the isotropic approximation contemplated here is given by E int = γ0l,

(10.30)

where l is the circumference of the ellipse. For an ellipse with semimajor axis a and semiminor axis b, the circumference can be evaluated through the integral a a2 − ξ 2 x 2 l(a, b) = 4 d x, (10.31) a2 − x 2 0 where we have deﬁned the dimensionless parameter ξ 2 = 1 − (b/a)2 . This result is a special case of an elliptic integral and may also be written as √ 2 a − b2 π , , (10.32) l = 4a E a 2 where E is an elliptic function. By resorting to Taylor expansion, the interfacial energy term may be rewritten as √ 3 33 (10.33) E int (A, U ) = 2 π Aγ0 1 + U 2 + U 4 + · · · . 4 64 In addition to the interfacial energy, the competition at play here depends also on the elastic energy associated with the second-phase particle. Using ideas quite similar to those introduced already in the context of the Eshelby inclusion the elastic energy may be written as 1 + κδ − (1 − δ)U 2 , (1 + κδ)(1 + δ − 2ν ∗ ) + (1 − δ)(κδ − 1 + 2ν ∗ )U 2 (10.34) where the precipitate is characterized by elastic constants µ∗ and ν ∗ , while the matrix has elastic constants µ and ν. The dimensionless ratio δ = µ∗ /µ characterizes the difference in shear moduli between the two media and κ = 3−4ν. Like the interfacial energy, this term may be expanded in powers of U yielding 2A02 µ∗ δ(1 − δ)(1 + κ) 1− U2 E elastic (A, U ) = ∗ 1 + δ − 2ν (1 + κδ)(1 + δ − 2ν ∗ )

δ(1 − δ)2 (1 + κ) 4 + U ··· . (10.35) (1 + κδ)2 (1 + δ − 2ν ∗ )2 E elastic (A, U ) = 202 µ∗ A

Given our knowledge of both the elastic and interfacial energies, the total energy as a function of the particle size and shape parameters now has the character of a Landau expansion like that seen in the theory of phase transitions. In particular, we

10.2 Inclusions as Microstructure

533

have 1 1 E tot (A, U ) = E int (A, U )+ E elastic (A, U ) = F0 (A)+ F2 (A)U 2 + F4 (A)U 4 · · · , 2 4! (10.36) the minima of which will tell us the optimal U for a given A. If we truncate the expansion at fourth order, the minima are realized by those U satisfying

∂ E tot 1 (10.37) = 0 = U F2 (A) + F4 (A)U 2 . ∂U 6 On physical grounds, F4 (A) will be seen to be positive, leading to the conclusion that the energy minimizing U is given by 0 if F2 > 0 √ . (10.38) U= ± −6F2 /F4 if F2 < 0 Hence, within this approximate model, the entire question of equilibrium shape has been reduced to the dependence of F2 on A which is gotten by adding the quadratic contributions to the energy from both the interfacial and elastic terms and is given by 2A02 µ∗ δ(1 − δ)(1 + κ) 3 √ F2 (A) = γ0 π A − . (10.39) 2 (1 + κδ)(1 + δ − 2ν ∗ )2 By setting F2 (A) to zero we can obtain the critical particle size, Ac , which also √ permits the deﬁnition of a size parameter λ = A/Ac . Recall that in the present model, the parameter A has the role of characterizing the particle size, and hence suggests that with increasing particle size there could be a transition from the U = 0 regime (i.e. circular particles) to the broken symmetry regime in which the particles exhibit elliptical shapes. This transition is most simply described in considering the ratio F2 /F4 as a function of the parameter λ. Note that the transition can only occur in the case in which δ < 1 which is the limit in which the particles are softer than the matrix. The results of our analysis of the question of equilibrium shapes may be depicted graphically as shown in ﬁg. 10.16. This graph is shown for the speciﬁc case in which ν = ν ∗ = 1/3 and δ = 1/2. The key point is that with increasing particle size (measured by the dimensionless parameter λ), there is a transition from circular to elliptical shapes as the energy minimizing geometry. Note that the onset of this transition in the graph is observed by monitoring the value of U , the parameter which measures the deviation about the limit of circular particles, as a function of the particle size as measured by λ. An additional remark is to note the physical competition that is being played out. For small particle sizes, the surface to volume ratio is such that the particle shapes will be dominated by the interfacial energy while in the large-particle-size limit, the elastic terms will

534

10 Microstructure and its Evolution

Fig. 10.16. Representation of energy minimizing U as a function of a dimensionless representation of the particle size (adapted from Johnson and Cahn (1984)).

have an increasing importance. Because the interfacial energy is isotropic, it favors circular geometries while the elastic energy prefers the elongated geometries found at larger particle sizes. Numerical Calculation of Two-Dimensional Equilibrium Shapes. To go beyond the relative simplicity of the set of shapes considered in the analysis presented above it is necessary to resort to numerical procedures. As a preliminary to the numerical results that will be considered below and which are required when facing the full complexity of both arbitrary shape variations and full elastic anisotropy, we note a series of ﬁnite-element calculations that have been done (Jog et al. 2000) for a wider class of geometries than those considered by Johnson and Cahn. The analysis presented above was predicated on the ability to extract analytic descriptions of both the interfacial and elastic energies for a restricted class of geometries. More general geometries resist analytic description, and thus the elastic part of the problem (at the very least) must be solved by recourse to numerical methods. Jog et al. use a two-dimensional numerical implementation of an iterative scheme in which the geometry of the interface is parameterized by a set of nodes which serve as the conﬁgurational degrees of freedom associated with the question of the equilibrium shape. Their scheme is predicated on computing the elastic ﬁelds at ﬁxed geometry and then these ﬁelds are used ﬁrst to compute the energy and then to compute the conﬁgurational forces on those same nodes (i.e. the derivatives of the energy with respect to the interfacial coordinates) providing a search direction

10.2 Inclusions as Microstructure

535

Fig. 10.17. Comparison of analytic and numerical results for the critical size at which the circle– ellipse bifurcation takes place as a function of particle size (adapted from Jog et al. (2000)).

for the next increment in the quest for the equilibrium structure. The signiﬁcance of this implementation is that it imposes no requirements on the particle shape. As a result, the search for the energy minimizers is over a much larger space of possible shapes. One way of testing such numerical implementations is to recover known results. In the present setting, this means recovering the results of Johnson and Cahn for the transition from circular to elliptical shapes. In ﬁg. 10.17 we show the results for the critical size (the inverse of this size is actually plotted) at which the bifurcation from circular to elliptical shapes takes place as a function of the inhomogeneity factor δ = µ∗ /µ, where µ∗ and µ are the shear moduli for the precipitate and the matrix, respectively. Of course, we should note that in the case of the analysis by Jog et al., the shape transition is from circular to nearly elliptical shapes, since their geometries are no longer constrained to the single degree of freedom geometry (at ﬁxed particle size) considered by Johnson and Cahn. The numerical results beautifully complement those resulting from the Johnson and Cahn analysis since they allow for an examination of the way in which elastic anisotropy and different forms of misﬁt other than dilatational can alter the equilibrium shapes. Equilibrium Shapes in Three Dimensions. The analyses described above have illustrated the fundamental competition between interfacial energies and elastic energies in governing the outcome of the question of equilibrium shapes. These calculations were introduced in the setting of reduced dimensionality with the

536

10 Microstructure and its Evolution

Fig. 10.18. Series of equilibrium shapes for three-dimensional particles (adapted from Mueller and Gross (1998)). The parameter L is a measure of the particle size and governs the competition between the surface energy terms (dominant at small L) and the elastic terms (dominant at large L).

result that analytic progress could be made. On the other hand, the importance of the answer to the question of equilibrium shapes is much greater in the context of three dimensions and it is for that reason that we also sketch the application of ideas like those described above in their full three-dimensional generality. As before, the fundamental competition being played out in selecting equilibrium shapes in three dimensions is between interfacial and elastic energies. In the analysis of Mueller and Gross (1998), energy minimizing geometries are searched for by recourse to a boundary element treatment of the elastic energies of a given three-dimensional shape. Their treatment is fully anisotropic and relies conceptually on exactly the same eigenstrain ideas introduced earlier (see section 2.5.3) in conjunction with the elastic Green function, but now tailored to problems involving elastic anisotropy. Because their methods are numerical, the elastic ﬁelds for a given conﬁguration can be computed directly, and the driving forces on the conﬁgurational coordinates describing the interfacial position are computed in exactly the same spirit as those introduced in our discussion of conﬁgurational forces in chap. 2. The three-dimensional equilibrium shapes found in their analysis are shown in ﬁg. 10.18. The elastic parameters chosen in these calculations were meant to mimic those of Ni, with the result that in the elastically dominated large-particle limit, there is a tendency for the particles to be cube-like. The arguments given above were concerned more with the terminal privileged state that would be arrived at by a particular second-phase particle than with the dynamical trajectory by which these equilibrium states are attained. In addition, we ignored the possible interactions between different particles, which in addition to interacting elastically can exchange matter via mass transport. All of these complaints can be remedied by recourse to a more computationally intensive approach in which the dynamical evolution of a given particle is considered as

10.2 Inclusions as Microstructure

537

a function of time and the equilibrium shape is a ﬁxed point of this dynamical system. This approach will be taken up later in this chapter. However, we should note that it is also possible to go beyond the types of continuum analyses introduced here and rather to use the type of effective Hamiltonian introduced in chap. 6 in conjunction with Monte Carlo simulation to revisit the question of equilibrium shapes. Using these methods, there are no restrictions concerning particle shapes, elastic homogeneity, isotropy of interfacial energies, nor is there even any restriction to linear elasticity. These ideas will be described in chap. 12 (see section 12.4.4 in particular). 10.2.5 A Case Study in Inclusions: Precipitate Nucleation As noted above, the question of equilibrium shapes is essentially a static one and can be answered without recourse to an analysis of the temporal processes that occur in conjunction with microstructural evolution. On the other hand, we are interested in examining the theoretical apparatus that has grown up around problems in which time is considered explicitly. One of the ﬁrst questions we can address in light of our elastic solution for the energetics of an inclusion and the ﬁrst step in our attempt to understand the temporal evolution of such particles is that of nucleation of second-phase particles. As with many questions concerning an instability toward the development of some new phase, the discussion centers on a competition between two different effects, each of which tends to favor a different terminal state. In the present setting, it is the competition between a term which scales as the volume of the second-phase particle and tends to favor the formation of the second-phase particle, and an interface term which carries an energy penalty associated with the interface between the inclusion and the matrix and thus favors removal of the second-phase particle. So as to permit analytic progress, we consider the restricted class of spherical geometries. The volume term is of the form 4 (10.40) E V = πr 3 E b , 3 where E b is an energy density such that E b < 0, and r is the particle radius. On the basis of arguments made in this and earlier chapters, we are in a position to seek an interpretation of the term E b . First, we note that there is a contribution to E b that arises from the fact that the second-phase particle has a different structure and hence a different structural energy than the matrix. Our use of the term ‘structure’ here is meant to include even the difference between ordered and disordered states on the same underlying lattice. The microscopic route to computing the energy lowering represented by a second-phase particle was described in chap. 6. However, we note that this energy will be renormalized by the energy penalty

538

10 Microstructure and its Evolution

Fig. 10.19. Schematic of the bulk and interfacial energies as a function of particle size.

arising from the elastic strains as was computed in section 10.2.1. As a result, in the present model, E b can be thought of as arising from two terms, one negative and essentially a structural energy difference, the other positive and representing the elastic strain energy associated with the inclusion. The volume term described above is balanced against an interfacial energy of the form E surf = 4πr 2 γint ,

(10.41)

where for the present purposes we have assumed an isotropic interfacial energy. The generalization to the anisotropic case introduces no new physical ideas. Again, because of the types of arguments made in previous chapters, it is now clear how to appeal to microscopic calculations in order to compute γint . The energy balance to be considered here is familiar and is depicted graphically in ﬁg. 10.19. The key observation is that with increasing particle size, a certain critical particle radius r ∗ is reached such that a further increase in particle size leads to an energy reduction. From the standpoint of our discussion of conﬁgurational forces (see section 2.3.3), we see that the sign of the driving force (i.e. ∂G(r )/∂r ) depends upon the size of the particle. For small particles, the driving force is in the direction of particle shrinkage, while for particles greater than the critical size, the driving force results in growth of the particle. To cast these ideas in mathematical form, we note that the total free energy in the present model may be written as 4 (10.42) G(r ) = 4πr 2 γint + πr 3 E b . 3 To determine the critical radius r ∗ , we need to satisfy the condition ∂G(r )/∂r = 0. The consequence of performing the relevant differentiation and solving for the

10.2 Inclusions as Microstructure

539

critical radius is r∗ = −

2γint . Eb

(10.43)

Though the results of nucleation theory are well worn, it is worth emphasizing the way in which a number of disparate threads have been woven into the discussion. First, armed with the results of the previous chapter, we are now well placed to understand the microscopic origins of γint . Similarly, because of our earlier discussion of structural energies, the structural contribution to E b is also clear. Finally, the elastic solution to the problem of a spherical inclusion given earlier in this chapter has instructed us concerning the strain energy penalty that arises on forming the inclusion which has been modeled as carrying a transformation strain. The model developed above serves as a convenient starting point for carrying out a dynamical analysis of the nucleation problem from the perspective of the variational principle of section 2.3.3. A nice discussion of this analysis can be found in Suo (1997). As with the two-dimensional model considered in section 2.3.3, we idealize our analysis to the case of a single particle characterized by one degree of freedom. In the present setting, we restrict our attention to spherical particles of radius r . We recall that the function which presides over our variational statement of this problem can be written generically as ˙ r ; r ), (˙r ; r ) = (˙r ; r ) + G(˙

(10.44)

and speciﬁcally in the present context as r˙ 2 + G˙ int (˙r ; r ) + G˙ bulk (˙r ; r ). (10.45) 2M We recall that M is the mobility of the interface between the two phases as the particle changes size. To compute the rate of change in the interfacial contribution to the free energy, we evaluate G int (r + r˙ t) − G int (r ), recognizing that G int (r ) = 4πr 2 γint . This amounts to computing the difference in the interfacial energy at an initial instant when the radius of the particle is r and at a time t later when the radius of the particle is r + r˙ t. As a result of these arguments, we ﬁnd (r, r˙ ) = 4πr 2

G int (r + r˙ t) − G int (r ) = 8πr r˙ γint . G˙ int = lim t→0 t

(10.46)

A similar argument is made in the case of the rate of change of the bulk contribution to the free energy. In this case, we interest ourselves in the free energy when the particle has radius r (i.e. G bulk (r ) = 43 πr 3 E b ) and when the particle has radius r + r˙ t. In this case, the result is G bulk (r + r˙ t) − G bulk (r ) = 4πr 2r˙ E b . G˙ bulk = lim t→0 t

(10.47)

540

10 Microstructure and its Evolution

Fig. 10.20. Flows for the differential equation describing evolution of a spherical particle with growth (or dissolution) dictated by the balance of interfacial and bulk energy. The particle size (f) and time (τ ) are plotted in the same dimensionless form used in the text.

If we now invoke the variational principle (i.e. ∂/∂ r˙ = 0), then it is found that 2Mγint . (10.48) r As seen earlier, there is a natural length scale in this problem, namely, rc = 2γint /|E b |, and it is similarly convenient to introduce the dimensionless time t0 = 2γint /M E b2 . In light of these deﬁnitions, the radius may be written in dimensionless form as f = r/rc , with a similar dimensionless time given by τ = t/t0 . Using these deﬁnitions, eqn (10.48) may be rewritten as r˙ = M|E b | −

df f −1 = . dτ f

(10.49)

This equation is separable and has the solution, f − f 0 + ln |

1− f | = −τ. 1 − f0

(10.50)

The temporal evolution of particles starting with different fractions of the critical size is shown in ﬁg. 10.20. Note that as expected, if a particle happens to start with an initial size equal to the critical radius, it will remain invariant in time. On the other hand, particles smaller than the critical size will shrink while those larger than the critical size will grow indeﬁnitely.

10.2.6 Temporal Evolution of Two-Phase Microstructures Though the calculation given above was both fun and interesting, it suffered from a number of defects. First, the class of intermediate shapes was entirely restrictive

10.2 Inclusions as Microstructure

541

since we assumed that the only possible shape was spherical. This assumption ignores all possibile instabilities of spherical particles to other shapes. In addition, our treatment of the mechanism of interfacial migration was implicit and was referenced only through the parameter M without any appeal to an underlying mechanism. To remedy these deﬁciencies, we now resort to schemes that can be spelled out in analytic terms, but for which one must have recourse to numerics to make any real progress in explicitly examining the particle shapes. Diffusional Dynamics. In the present analysis, we consider the explicit treatment of diffusion as the mechanism of interfacial migration, with the rate of such diffusion inﬂuenced in turn by the elastic ﬁelds implied by a particular particle shape. As a result, the problem of the temporal evolution of particles is posed as a coupled problem in elasticity and mass transport. The particles are given full scope to develop in any way they want. Our treatment of the temporal evolution of inclusion microstructures will be predicated on the following physical ideas. First, we note that the mechanism of microstructural change that is envisioned is that of mass transport. A given particle, by virtue of its shape and attendant elastic ﬁelds induces a local chemical potential. This chemical potential serves as a boundary condition in our solution of the diffusion equation for the entire medium. The update of the particle shape is based, in turn, upon the concentration gradients resulting from the solution of the diffusion equation with the local velocity increment scaling as vn ∝ ∇c · n. The logic behind this form for the velocity is the claim that the ﬂux of mass to or from the interface is of the form j ∝ ∇c and hence that the normal motion of the interface as a result of this mass ﬂux should scale as ∇c · n. The strategy is essentially iterative since once the particle shape has been altered, the elastic ﬁelds are also changed which demands another solution of the elasticity problem so that the chemical potential can be redetermined and from it, the next shape increment computed. The conceptual philosophy of these calculations is one of instantaneous equilibrium in which it is assumed that at every instant in the temporal history, the equations of mechanical equilibrium are instantaneously satisﬁed. The physical reasoning that is attached to this assumption has the same spirit as the Born–Oppenheimer approximation introduced in section 4.2.2. In particular, there is the expectation of a separation of time scales with the rearrangements (i.e. displacements) that maintain mechanical equilibrium taking place essentially inﬁnitely fast in comparison with the diffusion time. In addition to statements about mechanical equilibrium, it is also assumed that there is an instantaneous chemical equilibrium across the interface. Our discussion follows in a conceptual way (with different notation) that of Voorhees et al. (1992). These statements of equilibrium are imposed as follows.

542

10 Microstructure and its Evolution

Mechanical equilibrium is imposed by demanding that the elastic ﬁelds satisfy ∇ · σ = 0.

(10.51)

We note that just as with our analytic solution for the Eshelby inclusion, the equilibrium equations within the inclusion will have a ‘source’ term (i.e. an effective body force ﬁeld) associated with the eigenstrain describing that inclusion. In addition, we require continuity of both displacements, uin = uout , and tractions, tin = tout , at the interface between the inclusion and the surrounding matrix. The point of contact between the elastic problem and the diffusion problem is the observation that the interfacial concentration depends upon the instantaneous elastic ﬁelds. These interfacial concentrations, in turn, serve as boundary conditions for our treatment of the concentration ﬁelds which permits the update of our particle geometries in a way that will be shown below. The concentration at the interface between the inclusion and the matrix may be written as

1 σ : ]] − σ [[ ]] + γint κ . C = C0 + B [[σ (10.52) 2 Note that C0 is the equilibrium concentration associated with a ﬂat interface, B is a constant term, the two jump terms correspond to the jump in the Eshelby tensor across the interface and the ﬁnal term corresponds to the Gibbs–Thomson term and depends upon the interfacial curvature κ. Having solved the elastic boundary value problem and from it obtained the relevant interfacial concentrations, we are then prepared to obtain the concentration ﬁelds throughout the solid from which we compute the ﬂux to or away from the various particles. Since we are assuming the situation to be quasistatic, the instantaneous concentration ﬁelds must satisfy an equilibrium condition, namely, ∇ 2 c = 0.

(10.53)

This equation follows from our discussion of chap. 7 in which it was shown that in the simplest model of diffusion the concentration ﬁelds must satisfy the diffusion equation, which in the time-independent setting of interest here, reduces to Laplace’s equation. Once the concentration ﬁelds have been obtained we are ﬁnally positioned to update the conﬁguration of the system by recourse to vn = (∇c) · n,

(10.54)

where vn is the velocity of the interface. When the particle shapes have been updated, the procedure is repeated anew. To elaborate on the signiﬁcance of the interfacial concentrations as implied by eqn (10.52), we examine the playing out of these ideas in the context of a spherical particle. The question we pose is how to determine the chemical potential at

10.2 Inclusions as Microstructure

543

the interface between the spherical precipitate and the matrix and from it, the corresponding interfacial concentration. The essential idea is that this chemical potential can be written as µ=

∂G ∂a ∂G = . ∂N ∂a ∂ N

(10.55)

That is, we must compute the free energy change associated with a small excursion of the radius a. The relevant energy is built up of both interfacial and elastic terms as well as a chemical energy that we will ignore. In particular, we can write the free energy as 8πa 3 02 µ 1 + ν 2 , (10.56) G(a) = 4πa γint + 3 1−ν where the ﬁrst term is the interfacial energy associated with a spherical inclusion of radius a and the second term is the elastic energy associated with such an inclusion, as already computed in eqn (10.23). As a result of this insight, the chemical potential is immediate by effecting the derivative ∂G/∂a and exploiting it in the context of eqn (10.55), resulting in

2γint 1+ν , (10.57) + 202 µ µ = at a 1−ν where we have used the fact that for a small excursion of the radius a, the change in the number of particles is d N = ρ4πa 2 da and we introduce the deﬁnition of the atomic volume, ρ = 1/at . Note that the ﬁrst term on the right hand side is the conventional Gibbs–Thomson term relating the chemical potential to interfacial curvature, while the second term represents a purely mechanical effect due to the strain ﬁelds that are present in the system. If we now use the relation between chemical potential and concentration that corresponds to an ideal solution, namely, µ = kT ln(c/c0 ), and expand the resulting exponential, we are left with

c0 at 2γint 1+ν 2 + 20 µ , (10.58) c = c0 + kT a 1−ν a relation precisely of the form of that given in eqn (10.52). We note again that the key point here is that by virtue of solving a problem concerning the instantaneous mechanical equilibrium, we can compute interfacial concentrations which then permit the solution of the diffusion and the calculation of the resulting ﬂuxes which lead to the shape changes of interest. Equilibrium Shapes Revisited. In section 10.2.4, we described the examination of equilibrium shapes. Though the question of equilibrium shapes is one of terminal privileged states, nevertheless, the ideas introduced here which can in

544

10 Microstructure and its Evolution

Fig. 10.21. Series of equilibrium shapes for particles (adapted from Thompson et al. (1994)). The parameter L is a measure of the particle’s size, while a2R is one of the Fourier coefﬁcients that deﬁnes the shape of the particle and is a measure of the deviation away from the circular shape.

principle tell us about temporal evolution, can be used just as well to ﬁnd those terminal states. An example of the type of results that have been achieved with this type of method in two dimensions is shown in ﬁg. 10.21 (Thompson et al. 1994). This result should be contrasted with that of ﬁg. 10.16 which showed the analytic results of Johnson and Cahn in the restricted search over elliptical particle shapes. For the set of calculations shown in ﬁg. 10.21, the elastic anisotropy ratio is chosen to correspond to that of Ni, resulting in elastically soft 100 directions. The eigenstrain associated with the inclusion is assumed to be purely dilatational (i.e. i∗j = δi j ). In the limit of vanishingly small particles, the equilibrium shapes are circular reﬂecting the dominance of the interfacial energy term. With increasing particle size, the solution acquires a fourfold symmetry signaling the increasing relevance of the elastic energy. For yet larger particles, a critical size is reached at which the symmetry is broken resulting in particles with twofold symmetry. Coarsening of Two-Phase Microstructures. As yet, we have made reference to the formulation involving mass transport only in the context of the problem of equilibrium shapes. The method has deeper signiﬁcance in the context of problems involving real temporal evolution such as that of coarsening. Coarsening refers to the increase in size of certain particles at the expense of others. This additional elaboration on the problem of the temporal evolution of a single particle is intriguing since it introduces yet another interesting physical effect, namely, the elastic interactions between different particles which can affect their morphology as well. An example of this process from the experimental perspective is revealed in ﬁg. 10.22 in which Ni3 Si precipitates in a Ni–Si alloy are shown at various times, revealing the marked tendency of certain particles to increase in size while

10.2 Inclusions as Microstructure

545

Fig. 10.22. Series of snapshots of the coarsening of Ni3 Si precipitates in a Ni–Si alloy (adapted from Cho and Ardell (1997)).

others disappear. In addition to changes in particle size, the temporal evolution of this system is also attended by changes in shape as well. In particular, at short times the particles are nearly spherical while at later times they acquire a deﬁnite cuboidal shape. A more quantitative spin on results of the kind noted above can be given such as that shown in ﬁg. 10.23 in which the average particle radius as a function of time is revealed. These data suggest that the particle radius grows via a scaling law of the form r ∝ t 1/3 . In addition to well-developed theoretical ideas such as the theory of Lifshitz–Slyozov–Wagner, understanding of this phenomenon can be developed on the basis of numerical simulations involving a formalism like that described above in which mass transport is treated explicitly, and elastic effects are given full scope to drive the relevant rearrangements of matter. In principle, the coarsening phenomenon was included implicitly in the treatment of temporal evolution given above, though when posed in the numerical terms given above, it is perhaps difﬁcult to attain the sort of understanding that might be wished for blackboard level discussion. Using methods that solve for the same basic physics as has been described earlier in this section, Jou et al. (1997) have carried out a series of two-dimensional studies on the temporal evolution of a distribution of precipitates. Mediated by mass transport that is driven in turn

546

10 Microstructure and its Evolution

Fig. 10.23. Average particle radius as a function of time for coarsening of γ precipitates in Ni–13.23 at.% Al alloy aged at 750 ◦ C (adapted from Ardell (1997)).

by the elastic ﬁelds, their analysis allowed for a numerical examination of the coarsening process with results like those shown in ﬁg. 10.24. Qualitatively, the coarsening process as revealed by the diffusional dynamics introduced above has all the features expected of the coarsening phenomenon, namely, large particles grow at the expense of the small particles which eventually disappear. We close by noting that this section on the microstructure in two-phase solids has illustrated a number of key ideas that can be brought to bear on the question of the spatial and temporal evolution of these structures. The foundational statement for our analysis was given in eqn (10.24) which asserts that the instantaneous conﬁgurational forces derive from both interfacial and elastic energies. We should note that our treatment of the elastic effects in these systems has ignored stresses that are induced by composition variations, though such terms can be included. Similarly, we have also ignored the way in which externally applied stresses can tip the energy balance in favor of particular orientations, breaking the degeneracies between different crystallographically equivalent versions of a given second-phase particle. Finally, we note that some ideas that invoke the diffuse interface concepts introduced in section 9.5 have not been introduced with regard to two-phase microstructures and we alert the reader that concepts like these, with precisely this application in mind, will be featured in our discussion of bridging scales in section 12.4.4. 10.3 Microstructure in Martensites In the previous section, we showed one quantitative scheme for treating microstructure and its evolution. Earlier in the chapter we discussed the geometrical

10.3 Microstructure in Martensites

547

Fig. 10.24. Coarsening of particles in two-dimensional simulation (adapted from Jou et al. (1997)).

characterization of grain structures, and noted the want of a quantitative theory of such microstructure that at the same time admits of analytic progress. One area in which considerable progress has been made is in the study of microstructure in systems which undergo reversible martensitic transformations. What is found in this setting is that on the basis of kinematical constraints and fairly simple nonconvex models of the energetics of the competing phases, a quantitative theory of martensitic microstructure may be laid down which makes veriﬁable predictions. We give special attention to this theory in that it provides an inspirational example of the type of theoretical description that is desirable within the setting of more general microstructures.

10.3.1 The Experimental Situation The class of transformations known as martensitic are those cases in which upon cooling, the system undergoes a spontaneous change of lattice from a high-symmetry parent phase to some lower-symmetry ‘martensite’. These transfor-

548

10 Microstructure and its Evolution

Fig. 10.25. Change in Bravais lattice and well structure associated with the cubic–tetragonal transformation (adapted from Bhattacharya (1991)). U1 , U2 and U3 are the matrices that map the original cubic Bravais lattice into the three tetragonal variants.

mations are distinctive since they occur in a diffusionless manner (sometimes also called ‘displacive’) in which the atoms undergo only local rearrangements while preserving the same distribution of near neighbors. Perhaps the most well-known example of such transformations is that offered by the case of steel. Similar transformations occur in other intermetallic systems such as the cubic–tetragonal transformation in the Ni–Al system and the cubic–orthorhombic transformation in the Al–Cu–Ni system, to name but two. In addition to the geometric signature of these transformations at the lattice scale, even more fascinating (and beautiful) geometric changes are evinced at the microstructural scale. Martensitic microstructures are those in which a partnership has been struck between different variants of a given structure, and possibly the parent phase as well. For the sake of concreteness, consider ﬁg. 10.25 which depicts a transformation between a parent (austenite) phase that is cubic and a tetragonal (martensite) product phase. One of the ﬁrst observations that emerges from the schematic is the presence of multiple degenerate realizations of the martensitic phase. This degeneracy arises from the fact that any of the choices of the original cubic axes serves, by symmetry, as an appropriate axis along which to carry out the tetragonal distortion. As seen in the ﬁgure, the transformation matrices which map the original Bravais lattice vectors onto the transformed Bravais lattice vector are denoted by U1 , U2 and U3 . If our only interest were in the equilibrium crystal structures, our work would already be done. However, if we further interest ourselves in the actual geometric arrangements that are realized in a crystal that has undergone such a transformation, it is evident that the possibility of peaceful coexistence of the different variants results in a richness of structures at the microstructural level.

10.3 Microstructure in Martensites

549

Fig. 10.26. Fine structure at martensite interface (courtesy of Richard James).

An example of the type of martensitic microstructure that can arise when there is more than one degenerate well is given in ﬁg. 10.26. For the moment, we interest ourselves in a particular aspect of these microstructures, namely, the ﬁne structure at twinned interfaces. In particular, this ﬁgure demonstrates the geometry adopted in the Cu–Al–Ni system as the various twins arrive at a second internal interface. The alternating light and dark regions in the ﬁgure correspond to different variants separated by twin boundaries. For the moment, our interest is more in what takes place between these interfaces. To illustrate the types of quantitative questions that can be addressed by the theory of ﬁne-phase microstructures, we ﬁrst elaborate further on the character of these microstructures. As seen above, the martensitic microstructure is characterized by the presence of different variants. However, in the presence of an applied stress, the relative proportion of the different variants can be changed. The experiments are carried out in a biaxial loading apparatus like that shown schematically in ﬁg. 10.27. If we align our Cartesian axes with the two loading directions, then the state of stress to which the sample is subjected can be characterized by the scalars σ1 and σ2 which are a measure of the magnitudes of the load in these two loading directions. A compelling series of snapshots in the type of loading program that can be attained in this biaxial machine are shown in ﬁg. 10.28. What is noted is that, indeed, the stress has the effect of biasing one variant over another. In the ﬁrst frame, the volume fraction of the dark variant is much higher than the lighter one. However, we see that with the decrease in the load σ2 , the light variant begins to grow at the expense of its darker partner. Consequently, one class of questions that

550

10 Microstructure and its Evolution

Fig. 10.27. Schematic of biaxial loading apparatus used to examine stress-induced transformations and resulting microstructures in martensites (courtesy of R. James).

Fig. 10.28. Sequence of snapshots of martensitic microstructure corresponding to different load levels (courtesy of R. James and C. Chu) as obtained using polarized light. Different shades correspond to different variants of the Cu–Al–Ni martensite. Biaxial stress state applied using ¯ directions: (a) σ1 = machine shown in ﬁg. 10.27, with stresses applied along (011) and (011) 7.4 MPa, σ2 = 11.1 MPa, (b) σ1 = 7.4 MPa, σ2 = 9.1 MPa, (c) σ1 = 7.4 MPa, σ2 = 8.3 MPa, (d) σ1 = 7.4 MPa, σ2 = 7.4 MPa, (e) σ1 = 7.4 MPa, σ2 = 6.9 MPa, (f) σ1 = 7.4 MPa, σ2 = 6.2 MPa. Field of view in pictures is roughly 2.5 mm.

10.3 Microstructure in Martensites

551

Fig. 10.29. Illustration of deformation satisfying the rank-one connection condition.

can be posed about these microstructures is how do the volume fractions of the different variants depend upon the state of stress?

10.3.2 Geometrical and Energetic Preliminaries Much of the action associated with the emergence of martensitic microstructures can be traced to kinematic constraints. In particular, on purely geometric grounds, we can identify what types of interfaces are permitted between the austenite and martensite phases, and between the different variants of the martensite itself. It is the aim of the present section to describe these geometric preliminaries in preparation for the theory of ﬁne-phase microstructures which will be given below. Our treatment closely parallels that of Bhattacharya (1998) who in addition to discovering much of what we will say here has codiﬁed a wealth of insights on martensitic microstructure in review article form. We begin by considering the compatibility we will demand across a particular interface. The fundamental physical statement is our insistence on a certain invariant plane such that whether we approach the plane from below or above, when we reach the plane, our prescription for displacing the atoms on that plane will be the same. The reasoning here is illustrated graphically in ﬁg. 10.29. We imagine transformations speciﬁed by the deformation gradients F1 and F2 and ask what constraints must be placed on them in order that the crystals maintain their continuity across the interface between the two transformed regions. As said above, the physical requirement is the existence of a certain invariant plane such that whether or not we use F1 or F2 to compute the transformation on the plane itself we will ﬁnd the same result. The solution to this demand is that the two

552

10 Microstructure and its Evolution

deformation gradients be related by F1 − F2 = a ⊗ n,

(10.59)

the so-called rank-one connection of the pertinent deformation tensors. The vector n is the normal to the putative invariant plane in the reference conﬁguration and a is a vector to be determined. Indeed, another way to see what we have wrought with this equation is to rewrite eqn (10.59) as F1 = F2 + a ⊗ n,

(10.60)

and to note that the action of F1 is the same as F2 except that it picks off the components of vectors normal to the invariant plane. That is, if we take our origin of coordinates somewhere on the invariant plane and ask how F1 acts on the vector r = r# e# +r⊥ n, we see that it is only if r has a nonzero component perpendicular to the invariant plane that the deformation gradients F1 and F2 have a different action on that vector. This guarantees that whether we approach the interface from above or below, the deformation gradients F1 and F2 will agree as to the displacements of atoms (or more generally, of points) on the invariant plane. These ideas are further elaborated in the problem section at the end of the chapter. Part of the beauty of the theory of martensite is the far-reaching implications of the simple geometric constraint represented by eqn (10.59). One of the key results that emerges from this constraint is the nature of the allowed twinning planes that can coexist between different variants of the same underlying martensite. To see this, we must ﬁrst examine in a bit more detail the symmetries present in the energy landscape. For the time being, we interest ourselves in the properties of afﬁne deformations characterized by the deformation gradient F. On the basis of the known transformation strains and the invariances implied by crystal symmetry and overall rotational symmetry, much can already be said about the nature of the energy landscape, φ(F, T ), connecting the austenite and martensite phases. In schematic terms, we know that the energy as a function of the deformation gradient F has the basic character depicted in ﬁg. 10.30. Note that this energy is something that can in principle be evaluated directly on the basis of microscopic calculation. Indeed, we have already shown an example of such a calculation in ﬁg. 4.1. The basic point of a free energy like that mentioned above is that at high temperatures, the energy landscape is characterized by a global minimum for F = I (i.e. the austenite is the most stable structure). On the other hand, below the critical temperature, there are a number of degenerate wells corresponding to the different variants of martensite, F = Ui . Of course, in the ﬁgure, the set of possible deformations has only been indicated schematically since we have represented the deformation gradient as a scalar, and in reality, such deformations are characterized by the nine parameters needed to specify the full deformation gradient. From the

10.3 Microstructure in Martensites

553

Fig. 10.30. Schematic representation of the relative positions of competing minima in the energy landscape as a function of temperature (courtesy of K. Bhattacharya). φ(F, T ) is the free energy function, which depends upon both the deformation gradient F and the temperature T , U1 and U2 are the deformation gradients associated with the two martensite variants considered in this ﬁgure and the identity I is associated with the austenite well.

present standpoint, the key feature of the energy function φ that gives rise to the existence of microstructures is the presence on its energy landscape of multiple wells. As was said before, it is the degeneracy of different martensitic variants that makes it possible for one region of the microstructure to have selected one variant and some other region to have selected another. An alternative way to characterize the various wells is through the device of the James diagram in which each well is characterized by a circle like those shown in ﬁg. 10.31. The point of such diagrams is to represent a crucial feature of the symmetry of the stored energy function φ(F, T ). Material frame indifference requires that φ(F, T ) = φ(RF, T ), the meaning of which is that if we ﬁrst apply the deformation gradient and then rotate the resulting crystal, the energy is the same as if we had only applied the deformation gradient itself. The signiﬁcance of this insight is that the additional freedom associated with the ability to apply rotations broadens our scope to ﬁnd compatible interfaces between the different variants. As shown in the ﬁgure, each well is identiﬁed by a different circle, with the circle meant to indicate the entire group of allowable rotations R, namely, S O(3). Though F1 and F2 themselves may not satisfy the rank-one connection, material frame indifference illustrates that it is possible to ﬁnd a rotation R such that RF1 and F2 do satisfy the rank-one condition, and it is this additional freedom that is conveyed by the James diagram.

554

10 Microstructure and its Evolution

Fig. 10.31. Schematic illustration of deformation gradients in different wells for the cubic to tetragonal transformation that satisfy the rank-one connection condition (adapted from Ball and James (1992)).

As was shown in ﬁg.10.25, for the case of the cubic–tetragonal transformation there are three distinct wells to be considered, each corresponding to the tetragonal distortion occurring along a different Cartesian direction. Recall that our discussion of compatibility culminated in eqn (10.59). Part of the virtue of the James diagrams is that they provide a geometrical representation of part of the information content of eqn (10.59). What we note is that compatible deformations on different wells can be signiﬁed by connecting them with a line as shown in ﬁg. 10.31. In particular, what ﬁg. 10.31 tells us is that while there is no rank-one connection between U1 and U2 , for example, there is a rank-one connection of the form U2 − Rα U1 = a ⊗ n, where we have introduced the notation Rα to signify the particular choice of R on the U1 well that results in a rank-one connection to well U2 . The dotted lines in the ﬁgure connect two rank-one connected deformation gradients on different wells. To see all of these ideas in action, we now turn to a consideration of some of the many different types of compatible interfaces that can be found in martensitic systems.

10.3.3 Twinning and Compatibility The questions we will pose in this section concern the ability of different energetically favorable structures to coexist geometrically. We have already seen that the conﬂuence of two key ideas gives rise to the possibility for diverse microstructures. In particular, the identiﬁcation of a series of degenerate energy wells makes it possible that, for example, a cubic crystal will transform into several different (but

10.3 Microstructure in Martensites

555

Fig. 10.32. Schematic of interface between structures characterized by deformation gradients F1 = R1 U1 and F2 = U2 .

energetically equivalent) variants. On the other hand, we have also seen that it is not evident a priori that a compatible interface can be formed between both the different variants and the host austenite. To explore this question further, we require compatibility equations which specify under what conditions a compatible interface may be formed between two structures, each characterized by its own well. In ﬁg. 10.32, we indicate the type of interface we have in mind. On one side of the interface, the structure is characterized by a deformation gradient R1 U1 while on the opposite side of the interface the deformation is characterized by a deformation gradient U2 . Note that without loss of generality, we have rewritten the compatibility condition in terms of the stretch tensors U1 and U2 and a single rotation R1 . For a given set of structures characterized by the matrices U1 and U2 our question may be posed as: can we ﬁnd a rotation R1 as well as vectors a and n such that the condition R1 U1 − U2 = a ⊗ n,

(10.61)

is satisﬁed? Recall that in formal terms this is precisely the compatibility condition developed earlier and identiﬁed as the rank-one connection. We answer this question in the form of a theorem which asserts that if the eigenvalues of the matrix −1 T U−T 2 U1 U1 U2 may be ordered as λ1 ≥ 1, λ2 = 1 and λ3 ≤ 1, then there exists a rank-one connection. For details, see Proposition 4 of Ball and James (1987). From a physical perspective, we note that the signiﬁcance of this result is that the compatibility condition introduced above can only be satisﬁed for certain special choices of lattice parameters, a theme that will recur repeatedly in our discussion of martensitic microstructures.

556

10 Microstructure and its Evolution

−1 T If the eigenvalues of the matrix C = U−T 2 U1 U1 U2 satisfy the conditions described above, then we may go further and compute the vectors a and n as well as the rotation matrix. In particular, we assert that the vector a is given by

λ3 (1 − λ1 ) λ1 (1 − λ3 ) (10.62) e1 ± e3 , a=c λ3 − λ1 λ3 − λ1

while the vector n is given by √ √ λ3 − λ1 (− 1 − λ1 U2T e1 ± λ3 − 1U2T e3 ). n= √ c λ3 − λ1

(10.63)

Note that there are two solutions corresponding to the ± sign in our equations. In addition, the requirement that n be normalized is satisﬁed by exploiting the as-yet undetermined constant c. To determine the rotation matrix, we substitute the values for a and n back into eqn (10.61) and solve for R1 . Our intention in the remainder of this section is to build up a picture of some of the various interfaces that are present in martensitic systems. Our approach will be to consider microstructural elements of increasing complexity, beginning ﬁrst with the case of the simple austenite–martensite interface and culminating in the investigation of martensitic wedges within the host austenite. In all of these cases, the primary theoretical engine in our analysis will be the compatibility conditions and their outcome as typiﬁed by eqns (10.62) and (10.63). Austenite–Martensite Interfaces. As a ﬁrst exercise in the machinery set forth above, we pose the question of whether or not a simple interface can exist between a cubic crystal and its tetragonal offspring. Without loss of generality, this situation can be represented via the condition RU − I = a ⊗ n, where the matrix U is of the form

α 0 0 U = 0 β 0 . 0 0 β

(10.64)

(10.65)

For the special choice of stretch matrix U made here, all we are saying is that to produce the tetragonal crystal, all one need do is stretch by a factor α along the x-direction and by a factor β along the y- and z-directions. That is, the crystal axes of the cubic and tetragonal variants are parallel. Note that in light of the theorem set forth above, all that remains is to ask how the eigenvalues of the matrix C = U2 are ordered. However, since the matrix is already diagonal, we know that its eigenvalues are λ1 = α 2 , λ2 = λ3 = β 2 .

10.3 Microstructure in Martensites

557

For concreteness, we assume that α > 1 > β as is the case in systems such as In–Tl (α = 1.0221 and β = 0.9889) and Ni–Al (α = 1.1302 and β = 0.9392). As a result, we note that there is not an ordering of the eigenvalues of the form λ1 ≥ λ2 = 1 ≥ λ3 , which immediately lends itself to the conclusion that in the case of a cubic–tetragonal transformation, there is no simple interface between the host austenite and a single variant of the tetragonal martensite except in the unlikely event that the parameter β takes the value 1.0. Martensite–Martensite Interfaces. At the next level of complexity, we consider the nature of the interfaces that characterize the coexistence of different martensitic variants. In this case, the compatibility condition takes the more general form given earlier in eqn (10.61) where for explicitness we choose α 0 0 U1 = 0 β 0 (10.66) 0 0 β and

β 0 0 U2 = 0 α 0 . 0 0 β

(10.67)

Once again, our exercise is reduced to that of determining the eigenvalues of the matrix C. In the case in which the different variants in question are described by U1 and U2 as given above, the matrix C is of the form 2 2 0 0 α /β (10.68) C= 0 β 2 /α 2 0 . 0 0 1 In this case, we ﬁnd that the eigenvalues are precisely arranged so as to allow for the existence of a martensitic interface between the two variants in question. The question of the martensitic interface can be further explored by recourse to the equations that determine the vectors a and n themselves. In particular, by exploiting the results spelled out in eqns (10.62) and (10.63), we see that in the cubic–tetragonal case under consideration here, the vectors a and n are given by a=

√ β 2 − α2 2 2 (β, ±α, 0) β + α2

(10.69)

and 1 n = √ (−1, ±1, 0). 2

(10.70)

What we have learned from this analysis is that the invariant plane allowing for

558

10 Microstructure and its Evolution

Fig. 10.33. Schematic of interface between twinned martensite and the parent austenite (adapted from James and Hane (2000) and Chu (1993)).

the development of an interface between two different variants of the tetragonal martensite is of the (1, 1, 0)cubic -type. Austenite in Contact with Twinned Martensite. An even more interesting example is that of an interface between austenite and a twinned version of the martensite. In this case, the strategy is to satisfy the conditions of compatibility across the austenite–martensite interface in an average sense. The geometry of interest is indicated schematically in ﬁg. 10.33. Recall that in the case of the cubic–tetragonal system, we could ﬁnd no interface between the host austenite and a single variant of martensite. In the present context, the idea is to seek an average deformation gradient F = λF1 + (1 − λ)F2 that satisﬁes the compatibility condition. Note that here λ is not an eigenvalue of the matrix C, but is rather the volume fraction of F1 . For simplicity, we take the deformation gradient in the austenite to be the identity I, while the two variants of martensite are characterized by RU1 and U2 . The compatibility condition within the twinned martensite region is nothing more than was written earlier and takes the speciﬁc form RU1 − U2 = a ⊗ n.

(10.71)

In addition to this constraint, we must also satisfy compatibility across the austenite–martensite interface which in light of the deformation gradients speciﬁed

10.3 Microstructure in Martensites

559

above may be written R (λRU2 + (1 − λ)U1 ) − I = b ⊗ m.

(10.72)

The latter of these equations is sometimes referred to as the habit-plane or austenite–martensite equation. This equation imposes the rank-one connection across the austenite–martensite interface, with the rotation R governing the overall orientation of the twinned martensite with respect to the austenite across the austenite–twinned-martensite interface. We also note that this equation embodies the classic results of the crystallographic theory of martensite as expounded in Wayman (1964), though now interpreted energetically in terms of the various energy wells available to the system. As it stands, we must determine the matrices R and R , as well as the vectors a, b, n and m and the mixing parameter λ, given our knowledge of the tensors U1 and U2 . To do so, we resort to a divide and conquer strategy in which ﬁrst we solve eqn (10.71) using exactly the same technique described earlier and culminating in the solutions of eqns (10.62) and (10.63). Once these solutions are in hand, we then turn to a solution of eqn (10.72). The key point concerning this solution for our present purposes is that it depends critically on particular choices of the relevant lattice parameters. In particular, as shown in Ball and James (1987) and explained in James and Hane (2000), necessary and sufﬁcient conditions for the existence of a solution are δ ≡ a · U2 (U22 − I)−1 n ≤ −2

(10.73)

and |a|2 ≥ 0. 2δ The resulting volume fraction λ of variant 1 is given by 2 1 1− 1+ . λ= 2 δ η ≡ tr(U22 ) − det(U22 ) − 2 +

(10.74)

(10.75)

The dependence of the volume fraction λ on the parameter δ shows that it too is material speciﬁc and depends upon the particular values of the various lattice parameters. Wedge Structures. As our ﬁnal exercise in examining the conjunction of energetic and compatibility arguments, we consider the case of wedge-like structures in which a series of twins are arranged in such a way that a wedge of martensite can be embedded within austensite. The situation we have in mind is depicted schematically in ﬁg. 10.34. We also note again that our discussion leans heavily on that of Bhattacharya (1991) who considered the issue of wedges in martensite in detail.

560

10 Microstructure and its Evolution

Fig. 10.34. Schematic of a martensite wedge embedded within an austenite structure (adapted from Bhattacharya (1991)).

From the standpoint of the kinematic arguments introduced earlier, the additional complexity that attends situations such as the wedge microstructure considered here is the fact that we no longer have only a single interface on which to satisfy the conditions of compatibility. Our calculations on the austenite–twinnedmartensite interface served as a warm up exercise for the present case. Each and every interface of the type in ﬁg. 10.35 must itself satisfy conditions such as that of eqn (10.59). As a result, the imposition of compatibility across all of the interfaces takes the form of the collection of equations A − B = a1 ⊗ n1 ,

(10.76)

C − D = a 2 ⊗ n2 ,

(10.77)

λ1 A + (1 − λ1 )B − λ2 C − (1 − λ2 )D = a3 ⊗ m,

(10.78)

λ1 A + (1 − λ1 )B − I = a4 ⊗ m1 ,

(10.79)

λ2 C + (1 − λ2 )D − I = a5 ⊗ m2 .

(10.80)

Like in the simpler case of the interface between an austenite region and twinned martensite, this set of equations can be solved by recourse to a divide and conquer policy. Our main interest in showing these equations is to show the reader what is involved in setting up such a problem and to inspire him or her to read Bhattacharya’s beautiful 1991 paper.

10.3.4 Fine-Phase Microstructures and Attainment We have now structured the problem of martensitic microstructre in accordance with key geometric and energetic notions. What we have seen is that once the

10.3 Microstructure in Martensites

561

Fig. 10.35. Detailed schematic of the variants within a martensite wedge which is itself embedded within an austenite structure (adapted from Bhattacharya (1991)).

energy wells have been identiﬁed, largely on the basis of geometric arguments it is possible to classify the various types of interfaces that can be realized within a given microstructure. We now pose the deeper question of the character of the overall microstructure itself. For example, what are the volume fractions of the different variants, and what features of the problem determine the typical length scale associated with these variants? The answer to such questions demands a discussion of the subtlety that can attend the notion of minimization of the type of nonconvex energies introduced above. For the present purpose, our ﬁrst observation is that under certain circumstances, it is possible that the minimizer will be represented as the limit of a sequence of increasingly ﬁne microstructures. Alternatively, this can be stated by noting that in some cases there are no smooth deformations that minimize the energy. Instead, we extend the space of possible minimizers by including those deformations which are piecewise continuous and are allowed to have a vanishingly small thickness. A two-dimensional model problem described in depth by Bhattacharya (1998) which illustrates this idea is built around the idea of trying to ﬁnd a scalar ﬁeld y(x1 , x2 ) that minimizes the free energy functional φ(∇ y(x1 , x2 ))d x1 d x2 , (10.81) E[y(x1 , x2 )] =

subject to the boundary condition that y = 0 on the boundary ∂ of the body . To make the problem interesting, the free energy itself is chosen to have two wells,

562

10 Microstructure and its Evolution

and is of the form

φ(∇ y(x1 , x2 )) =

∂y ∂ x1

2

2 −1

+

∂y ∂ x2

2 .

(10.82)

The free energy density given above has two wells, corresponding to ∂ y/∂ x1 = ±1 and ∂ y/∂ x 2 = 0. In addition to the speciﬁcation of the free energy itself, our problem is supplemented with the boundary condition that the deformation vanish on the boundary of the region. We see that this free energy functional and the associated boundary conditions pose contradictory demands on the deformation mapping y(x1 , x2 ), resulting in a lack of ‘attainment’, a word that signiﬁes that the class of continuous deformations is unable to provide a minimizer, even though the free energy is bounded from below. To see this, we note that on the boundaries we would like to choose y = 0. On the other hand, within the ‘volume’ , the choice y = 0 is energetically unfavorable since it corresponds to a choice of ∇ y that deﬁnitely does not occupy either of the wells. Hence, we are unable to attain the minimum with any continuous deformation. On the other hand, using the construction to be described below, we can get as close as we like to the state of zero energy by considering ever ﬁner mixtures of the two variants. It is evident at the outset that there is no continuous deformation that minimizes this energy function. On the other hand, we can also note that by adopting the approach of setting up a series of piecewise continuous deformations with a corresponding energetic boundary layer near the boundaries, we can construct structures that approach the lowest energy to within arbitrary accuracy. This construction is revealed pictorially in ﬁg. 10.36, and illustrates the enlargement of our space of solutions to include so-called minimizing sequences. The idea is to build up the overall microstructure by considering strips with ∇ y = (1, 0) and ∇ y = (0, 1). In each of these strips, the contribution to the overall energy is zero. On the other hand, these strips fail to satisfy the boundary condition (y = 0) at x2 = 0 and x2 = L, where L is the dimension of the region of interest. As seen in ﬁg. 10.36, the remedy to this problem is to cut the strips off at the ends so they vanish at x2 = 0 and x2 = L. Of course, in so doing, we must pay an energy penalty for this boundary layer since in these regions ∇ y is not associated with either of the energy wells. In fact, as shown in Bhattacharya (1998), the energy associated with this boundary layer is of the form E layer = L 2 /2n, where n is an integer that characterizes how many strips are present in our microstructure. This demonstrates that the boundary layer contribution to the energy goes to zero in the limit that the ﬁneness of our microstructure is increased without bound. As a result of the arguments set forth in this part of the chapter, we are now prepared for the job of evaluating the structure and energetics of martensitic microstructures. The fundamental idea is to construct arrangements of the different

10.3 Microstructure in Martensites

563

Fig. 10.36. Illustration of two members of the minimizing sequence for two-dimensional problem posed in the text (adapted from Bhattacharya (1998)).

variants that simultaneously satisfy the geometric constraints associated with the rank-one connection and the energetic constraints introduced by presence of the pertinent free energy function. The discussion given above centered on the use of analytic reasoning to deduce the general characteristics of martensitic microstructures. Such analytic investigations have been complemented successfully using numerical solutions in which minimizers of the relevant free energy functional are sought after by recourse to a ﬁnite element description of the deformation ﬁelds (see Luskin (1996) for example). An example of the type of results that emerge upon implementing the ideas of the previous few sections in a numerical sense is

564

10 Microstructure and its Evolution

Fig. 10.37. Outcome of numerical calculation of the energy minimizers associated with martensite (adapted from Luskin (1996)): (a) an example of a ﬁnite element mesh used to model the martensitic microstructure, (b)–(d) the results of microstructure computations using different levels of mesh reﬁnement.

shown in ﬁg. 10.37. These calculations were made for a two-dimensional model free energy which is intended to mimic the energetics of the three-dimensional orthorhombic to monoclinic transformation. The calculations are made for a square geometry in which the boundary deformation gradient is prescribed and corresponds to neither of the competing wells. Like in the model problem resulting in ﬁg. 10.36, this choice of boundary condition guarantees the type of nonattainment described above. Though we will not elaborate on this point in any great detail, it is important to note that on physical grounds there is a lower cutoff to the type of runaway reﬁnement of the microstructure described above. Recall that our assessment of the free energy has until now been predicated entirely upon searching for a means to minimize the elastic contributions to this energy subject to particular boundary conditions. On the other hand, it is clear that the increased level of reﬁnement

10.3 Microstructure in Martensites

565

is accompanied by energy penalties associated with the various interfaces, terms which we have so far ignored. As said above, the physical consequence of these terms is to regularize the problem and to impose a length scale resulting from the balance of the surface energy and the elastic energy associated with the boundary layers in which the deformations are not associated with either the austenite or martensite wells.

10.3.5 The Austenite–Martensite Free Energy Reconsidered In ﬁg. 10.30, we gave a schematic description of the free energy as a function of deformation gradient for various temperatures above, below and at the transformation temperature. This discussion was built upon an intuition of what the basic character of the free energy must be in order to give rise to the phenomenology of these systems. We now reconsider the question of the alloy free energy from the perspective of chap. 6, with the aim of trying to explicate such free energies on the basis of microscopic calculation rather than on the phenomenological grounds introduced earlier in this chapter. For the present purposes, we write the free energy φ(F, T ) as a sum of two terms: φ(F, T ) = Fel (F, T ) + Fvib (F, T ),

(10.83)

where the ﬁrst term is the electronic contribution to the free energy of structures characterized by the deformation gradient F, while the second term is the vibrational contribution to the free energy, and it too depends upon the state of deformation. This equation is essentially an imitation of that given already as eqn (6.2). For an assessment of the ﬁrst term, we turn to a discussion of the so-called Cauchy–Born rule introduced in section 5.4.2, while for the second, we will revisit experiments on the free energy of structural transformations. For the purposes of computing Fel (F, T ), we can exploit the Cauchy–Born rule, as was done in the calculations leading to ﬁg. 4.1. Such calculations are conceptually simple in comparison with some of the more complex defect calculations introduced elsewhere throughout the book. All that one need do is take the original Bravais lattice (i.e. the reference state), deform the relevant basis vectors according to the prescription given above and compute the resulting energy using one’s favorite total energy scheme. We will not belabor the point other than by noting that the basic character of the results will resemble those of ﬁg. 4.1 in the sense that there can be more than one local minimum.

566

10 Microstructure and its Evolution

To compute the vibrational contribution to the free energy, we remind the reader of the results of chap. 6 in which we argued that entropy contributions can arise from vibrations (both harmonic and anharmonic) as well as electronic excitations. For the moment, we will advance the hypothesis, supported in some cases by experiment (see ﬁg. 10.38), that in the context of martensitic transformation the contribution of harmonic lattice vibrations to the entropy will tell most of the story. Further, our interest is in sketching ideas, in suggesting possible origins for effects rather than being exhaustive, and hence perhaps an overly facile representation of a rather complex problem can be forgiven. In the context of the Cu–Zn–Al system, a series of measurements were undertaken (Ma˜nosa et al. 1993) with the aim of sorting out the relative importance of the various contributions mentioned above to the overall entropy of transformation. In a word, their method was to use calorimetric techniques to obtain the total entropy. Using magnetic susceptibility measurements it is possible to independently pick off the electronic contribution to the total entropy which is known already from the calorimetric measurements. Finally, by taking the difference between this electronic contribution and the total entropy it is possible to compute the vibrational contribution to the entropy. Fig. 10.38 shows both the electronic (Se ) and vibrational (Sv ) contributions to the entropy in a series of different Cu–Zn–Al alloys. As is seen in ﬁg. 10.38, the magnitude of the vibrational entropy (and this is itself almost all harmonic) is quite large in comparison with that due to electronic degrees of freedom as is evidenced by comparing the scales of the two contributions. The conclusion to be drawn from these experiments is that in this case we can go a long way towards deducing the type of free energy function shown in ﬁg. 10.30 by combining what we know about the zero-temperature part of Fel (F, T ) (i.e. the zero-temperature structural energies) and the free energy of harmonic vibrations.

10.4 Microstructural Evolution in Polycrystals Our third and ﬁnal microstructural example centers on the question of polycrystals and their temporal evolution. Here we imagine the perfect crystal disturbed not by the presence of other phases, but rather by a series of grain boundaries separating crystalline regions each having a different orientation. We have already hinted at the implications of such a polycrystalline microstructure for the mechanical properties of a material. The aim of the present section is to examine how such microstructures evolve in time. We will begin with an examination of the observations that have been made on such microstructures, with an emphasis on the quantitative features of their temporal evolution. This will be followed by a reexamination of the driving forces that induce grain boundary motion as well as the mechanisms whereby such motion is realized.

10.4 Microstructural Evolution in Polycrystals

567

Fig. 10.38. Entropy difference between austenite and martensite in Cu–Zn–Al alloys (adapted from Ma˜nosa et al. (1993)). Different values of the electron per atom ratio correspond to different concentrations of the three alloy constituents.

10.4.1 Phenomenology of Grain Growth One of the palpable effects of annealing a polycrystal is a systematic change in the mean grain size, a phenomenon known as grain growth. A quantitative view of this process is evoked by plotting the mean grain size as a function of time as shown in ﬁgs. 10.39 and 10.40. Though we will not enter into the debate (for further details see Atkinson (1988)), the question of how to characterize three-dimensional microstructures on the basis of two-dimensional cuts is a subtle one. A more satisfying kinematic framework for characterizing polycrystalline microstructures, and grain growth in particular, is offered by considering the entire grain size distribution rather than just the mean grain size itself. In particular, consider the function F(R, t) which is the probability density for ﬁnding grains of size R within the microstructure. In particular, F(R, t) gives the number of grains per unit volume with size between R and R + d R at time t. Just as the mean grain size is amenable to experimental evaluation, so too is the grain size distribution function as shown in ﬁg. 10.41. One of the claims associated with these distribution functions is that they can nearly be thought of as lognormal

568

10 Microstructure and its Evolution

Fig. 10.39. Evolution of grain size as a function of time during the annealing process (adapted from Rhines and Craig (1974)). The vertical axis reveals the average grain volume as obtained by taking the reciprocal of the number of grains per cubic centimeter.

distributions. Perhaps more important yet is the assertion of a scaling property of the grain size distribution function. In particular, if the grain size is plotted, not in terms of the absolute size of the various grains, but rather in terms of the normalized grain size R/R (where R is the mean grain size, labeled by R¯ in the ﬁgure), then the distribution is statistically invariant. Exactly this point is made in ﬁg. 10.41 which shows the grain size distribution using scaled variables for various times in the temporal history of the microstructure. The process of grain growth bears some resemblance to the coarsening process discussed earlier in the context of precipitate microstructures. From the point of view of the driving force for such structural change, as we have repeatedly emphasized, such microstructures are metastable. A state of lower free energy may be reached by eliminating grain boundary area. By virtue of the presence of a variety of grain boundaries, it is plausible to imagine a state of lower free energy in which there are fewer such boundaries, and hence a lower overall boundary energy. One of the challenges posed by such microstructures is the way in which such metastable systems evolve in time.

10.4.2 Modeling Grain Growth As noted above, ostensibly, part of the empirical background concerning grain growth that demands explanation is the power law growth in time of the grain size. One of the justly famous contributions in that regard is the work of Burke

10.4 Microstructural Evolution in Polycrystals 99.9999% Cd

569

240 C

1.4 1.2

D (mm)

1.0 0.8 0.6 0.4 0.2

(a)

25

75

175

225

240 C

D2-D2 (mm2) 30

99.9999% Cd

125

(b)

Fig. 10.40. Evolution of grain size as a function of time during the annealing process (adapted from Simpson et al. (1971)). The parameter D is a measure of the grain size. In the lower frame the grain growth data are plotted with respect to t − t0 , where t0 is the time from which the subsequent grain growth is measured.

and Turnbull (1952) in which a parabolic growth law in which the mean grain 1 size scales as R ∝ t 2 was deduced on the grounds of arguments much like those leading to our eqn (10.48). The basic hypotheses behind the Burke–Turnbull argument are that the properties of the distribution itself can be understood by concentrating on the properties of one grain only, and that this one grain evolves under the action of curvature-induced forces. Recalling the variational statement of ˙ the variational eqn (10.45), but now treating only the interfacial contribution to G,

570

10 Microstructure and its Evolution

Fig. 10.41. Scaled grain size distribution function for various times in annealing history of sample of Fe (adapted from Pande and Marsh (1992)). In addition to the experimental results, the ﬁgure also shows the lognormal and Rayleigh distributions thought to be relevant to describing the distribution F(R, t).

principle can be written as ˙2 ˙ R). ˙ R) = 4π R 2 R + G˙ int ( R; ( R; 2M

(10.84)

On the assumption of an isotropic interfacial energy γint , G˙ may be written ˙ int . Following the usual procedure (i.e. (see eqn (10.46)) as G˙ int (R) = 8π R Rγ ∂/∂ R˙ = 0) results in an equation for the evolution of R of the form 2Mγint dR =− , dt R which when integrated yields the grain size scaling relation

(10.85)

1 2 1 2 R − R0 = −2Mγint t. (10.86) 2 2 Highly idealized arguments like that given above have been complemented by more realistic numerical simulations in which the various interfaces move in conjunction. Since our aim is the illustration of ideas rather than to exhaustively detail the ultimate solution to particular problems, we will take up three distinct schemes for considering the problem of microstructural evolution in the grain growth setting. The three paradigmatic examples to be considered here are shown in ﬁg. 10.42. Our intention is to consider in turn the Potts model approach to grain growth, phase ﬁeld models for grain growth and their sharp interface

10.4 Microstructural Evolution in Polycrystals

571

Fig. 10.42. Schematic of various paradigms for considering the evolution of polycrystal (adapted from Frost and Thompson (1996)). The upper panel shows the representation of the polycrystal from the perspective of each of the different models and the lower panel illustrates the way in which the interfaces between different grains migrate.

counterpart. As will be seen in the coming sections, each of these schemes has a different underlying philosophy, though they all attempt to capture the energy penalty associated with the presence of interfacial areas. Potts Models of Microstructural Evolution. Perhaps the simplest representation of the energetics of grain growth is provided by the so-called kinetic Monte Carlo models of grain growth. Here a model Hamiltonian is set forth that provides an energy penalty for all interfaces within the microstructure. The basic idea is to exploit the Potts model which is highly reminiscent of the Ising model. In concrete terms, the model is set up as follows. An order parameter σi is introduced which labels the orientation of the i th grain. Each possible orientation within the model is assigned a different integer. This kinematic scheme allows for each different orientation within the polycrystal to be represented by a different integer, though clearly the continuous set of misorientations has been replaced with a discrete (and ﬁnite) approximation. Note that the lattice considered here is not a crystalline lattice but rather a modeler’s lattice and represents a spatial discretization of the microstructure that is presumed ﬁne enough to capture the essential features of grain growth while at the same time being coarse on the scale of the lattice parameter. One scheme for deciding upon a length to associate with the lattice in the model is through reference to the typical curvatures that must be accounted

572

10 Microstructure and its Evolution

Fig. 10.43. A Potts microstructure in which different grains are identiﬁed by different values of the occupation number σ (adapted from Anderson et al. (1984)).

for in the lattice model of the microstructure. A Potts microstructure using the kinematic description of the microstructure described above is shown in ﬁg. 10.43. One means to generate such a microstructure is to select a series of grain centers, each of which will have a different orientation, set up the corresponding Voronoi tiling and then specify each grain according to its occupation label. As yet, the model is purely descriptive and says nothing about the possible subsequent evolution of the microstructure. To endow this geometric model with an underlying ‘dynamics’, we ﬁrst require a statement of the energetics. One conventional choice is a Hamiltonian of the form Ji j (1 − δσi ,σj ), (10.87) H= ij

where the sum is over lattice sites in the model and Ji j is an energy parameter that essentially mimics the grain boundary energy. A given grain is made up of many lattice sites, and the energy penalty implied by eqn (10.87) is associated with changes in the local spin variables from one lattice site to the next corresponding to the presence of a grain boundary. What the Hamiltonian tells us is that if two neighboring lattice sites i and j are identical (i.e. δσi ,σj = 1) then there is no associated energy penalty. On the other hand, if the neighboring sites have different values of σ , then there will be an energy cost parameterized by Ji j . In the general form with which the Hamiltonian was written above, each type of interface characterized by a different pair i j potentially has a different energy Ji j . However, a simpler realization of the model is to consider a single value J of the Potts coupling parameter which is equivalent to attributing an isotropic interface energy to the grain boundaries.

10.4 Microstructural Evolution in Polycrystals

573

The temporal evolution of a microstructure (i.e. grain growth) is examined by recourse to Monte Carlo methods. A trial change in occupation number is selected. If the move results in a net reduction of the energy, it is accepted. If not, it is accepted with a probability given by a Boltzmann weight. As a result of this ‘dynamics’, the trend is towards states of lower overall energy which in the context of the present model of energetics means less overall grain boundary area. A series of snapshots in a Potts microstructure as computed in this manner is shown in ﬁg. 10.44. One of the ways in which these results can be examined is from the perspective of the types of experiments on grain growth described earlier in this section. In particular, it is possible to monitor the grain size as a function of time.

Phase Field Models for Grain Growth. One of the complaints that can be registered about the type of analysis given above is the fact that the underlying dynamics is not really tied to the physics of interfacial motion. A partial remedy for this problem is provided by a second class of models that we will feature several times, namely, phase ﬁeld models. Note that these models are the logical extension of the ideas introduced in section 9.5. In this setting, the set of orientations corresponding to the polycrystalline microstructure is associated with a collection of ﬁeld variables (i.e. order parameters) ηi (r, t), with each ηi corresponding to a different orientation. The total energy of the system is written in such a way that its minimizers (i.e. there is only a single orientation present) are of the form that either ηi = 1 or ηi = −1 and all the other η j s are zero. Further, there is an energy penalty associated with spatial variations in the ﬁelds ηi which can be construed as an interfacial energy. Note that in this setting the interface is endowed with a ﬁnite width of the type described in the previous chapter and shown in ﬁg. 9.50. It is also worth noting that there are signiﬁcant similarities between the continuum model set forth here and the Potts model described above. To be concrete, one scheme that has been used to model grain growth in the phase ﬁeld setting is to identify a set of N ﬁeld variables (η1 (r, t), η2 (r, t), . . . , η N (r, t)) corresponding to 2N distinct orientations (since each ηi can assume the values ±1). The kinematic idea of such models is illustrated in ﬁg. 10.45 which shows the ‘interface’ between two different grains. As said above, the generalization to the situation involving more orientations is built around having a larger number of ﬁelds. Once these kinematic preliminaries have been settled, the total free energy functional is then written as the integral f [{ηi (r, t)}] =

[ f 0 ({ηi (r, t)}) +

κi i

2

(∇ηi (r, t))2 ]d 3 r.

(10.88)

574

10 Microstructure and its Evolution

Fig. 10.44. Series of snapshots in the life history of a Potts microstructure (courtesy of E. Holm): (a)–(d) represent various stages of the time evolution of this system.

The term f 0 is written explicitly as f 0 ({ηi (r, t)}) = −

α 2 β 4 ηi + ηi + γ ηi2 η2j , 2 i 4 i i j>i

(10.89)

which has energy wells corresponding to a given ηi being ±1 while all of its competitors are zero. The interpretation of the gradient term is relatively straightforward and imposes an energetic penalty for variations in the ﬁelds {ηi (r, t)} with a length scale set by the parameters {κi }. To summarize, the energetics set forth

10.4 Microstructural Evolution in Polycrystals

575

Fig. 10.45. Representation of the ‘interface’ region between different grains, one characterized by η1 (x) and the other by η2 (x).

above has two key features. First, there is a preference for one of the ηi s to be ±1 with all others zero. The demonstration of this point is taken up in the problem section at the end of the chapter. Secondly, the gradient term assigns an energy penalty to the ‘interfaces’ between regions in which the order parameter ﬁeld is different. That is, in passing from one grain (say ηi = 1) to another (say η j = 1), the order parameter ﬁeld will vary smoothly between 1 and 0 with a corresponding energy penalty for this interface. The basic idea of the phase ﬁeld approach is to play out this competition in a continuum setting. In addition to the deﬁnition of the energy functional, it is necessary to institute a dynamics associated with a model of this sort. In the present setting, the dynamics is obtained by asserting that the temporal evolution of a given ﬁeld variable is linear in the driving force, namely, δf ∂ηi (r, t) = −L i + ζi (r, t), ∂t δηi (r, t)

(10.90)

where the parameter L i is a kinetic coefﬁcient that modulates the driving force. ζi is a noise term which is intended to mimic the effects of thermal ﬂuctuations. We will return to the subject of gradient ﬂow dynamics like that introduced here in more detail in chap. 12. Notice that one of the challenges of a model of this type is that there are as many equations as there are components to the order parameter. As a result, for the simulation of a polycrystal with many different grains, there will be as many ﬁeld variables as there are grains resulting in both conceptual and computational

576

10 Microstructure and its Evolution

Fig. 10.46. Phase ﬁeld model for two-dimensional grain growth (adapted from Chen and Wang (1996)). Figure shows grain distribution at various times in the evolution of the grain structure with: (a) t = 1000, (b) t = 3000, (c) t = 5000 and (d) t = 8000. Time is measured in units of how many integration steps have taken place.

complexity. An example of the type of grain growth that occurs in a model like that sketched above is shown in ﬁg. 10.46 (Chen and Wang 1996). One of the outcomes of these calculations is the ability to characterize the kinetics of grain growth. In particular, it is possible to address the question of the mean grain size R as a function of time as well as the distribution of grain sizes. The temporal evolution of the average grain area is shown in ﬁg. 10.47 An outcome of this analysis is that it is found that the mean grain size scales with time with an exponent of 1/2. It should be noted that we have only outlined one of the many different diffuse interface approaches to the problem of grain growth. For the present purposes, our main point has been to call attention to the possibility of a strictly continuum model of grain growth in which the interfaces are endowed with a ﬁnite width and the kinematics of the polycrystal is encoded in a series of continuum ﬁelds. We

10.4 Microstructural Evolution in Polycrystals

577

7.5

7.0

6.5

(

ln A − Ao

) 6.0

5.5

5.0

4.5 6.0

6.5

7.0

7.5

8.0

8.5

9.0

9.5

ln(t)

Fig. 10.47. Temporal evolution of mean grain size in phase ﬁeld model of grain growth (adapted from Chen and Yang (1994)). Plots are of logarithm of average grain area as a function of time, with the two curves corresponding to four (crosses) and thirty-six (circles) different order parameter ﬁelds.

will see later that this class of models (i.e. phase ﬁeld models) has a much wider application than that of its particular incarnation in the context of grain growth. Sharp Interface Models of Grain Growth. An alternative paradigm for considering grain growth is offered by the class of sharp interface models. From a kinematic perspective, the polycrystal may be thought of as a series of lines (in two dimensions) or a series of interfaces (in three dimensions), the positions of which may be parameterized continuously or discretely. This class of models is especially appealing since the full kinematic complexity of the polycrystal has been collapsed onto nothing more than a discrete set of nodal coordinates which identify the interfacial position. The kinetics of the system is built around the idea of considering the various interfaces that make up the polycrystal of interest as being subjected to an array of driving forces of different physical origins. For example, driving forces can be present because of curvature of the boundary plane or because of differences between the stored strain energy in adjacent grains, or because of chemical inhomogeneities, or yet further mechanisms. These ideas may be put on a more formal basis by resorting to the variational arguments set forth in section 2.3.3 in which the power associated with the various driving forces is balanced with the various dissipative mechanisms that are present.

578

10 Microstructure and its Evolution

The application of this theoretical framework to the problem of grain growth is instructive, both as a case study in the use of the variational approach, and for the insights it provides into the grain growth process itself. Recall that the variational formulation is indifferent to the number of different dissipative mechanisms that are incorporated in the analysis. On the other hand, for the purposes of the present discussion we will only consider grain boundary motion induced by curvature without reference to the variety of other possible mechanisms. The driving force for microstructural change is the energy reduction that attends the elimination of grain boundary area and is given by γgb κvn d, (10.91) G˙ = G Bs

with κ the curvature of the boundary at the point of interest, γgb the grain boundary energy and vn the interfacial normal velocity. The overall variational function can be written as Nb Nb Nt 3 vn2 j ds + γb κvn ds + γb vk · sk . (10.92) [vn (s); r (s)] = 2D L L i i i=1 i=1 k=1 j=1 The ﬁrst two terms have already been discussed in several other contexts (see eqns (2.46) and (10.45)) with the new twist that now we have a summation over all of the different interfaces. The third term, on the other hand, is a new feature and reﬂects the extra attention that must be given to triple points within the polycrystalline microstructure when attacked from the sharp interface perspective. In order to turn the variational scheme given above into a calculational scheme, the various interfaces are discretized, thus turning the functional given in eqn (10.48) into a corresponding function which depends only upon the nodal coordinates that deﬁne the boundaries. The variational statement is then invoked in order to determine a set of nodal velocities which are used to update the microstructure. The results of this type of sharp interface treatment of grain growth is shown in ﬁg. 10.48. As noted above, the temporal evolution of the microstructure in this case is the result of a driving force that emerges from the reduction in grain boundary energy by reducing the overall length of such boundaries. Our treatment of grain growth was intentionally diverse, with the aim being to show some of the different paradigms that have been put forth for the consideration of grain growth. In broad terms, the key ideas can be divided between those having to do with computing the driving force on a given interface, and those whose aim it is to attribute a kinetics with these driving forces. The Potts model offered a very simple energetic description of grain boundaries in which the thermodynamic driving force was seen to be associated with the reduction in energy that attends the overall grain boundary area. Phase ﬁeld models

10.4 Microstructural Evolution in Polycrystals

Time = 0.00

Number of cells = 1024

Time = 8.54

Number of cells = 269

Time = 1.95

Number of cells = 707

Time = 30.0

Number of cells = 85

Time = 4.21

Number of cells = 464

Time = 336

Number of cells = 10

579

Fig. 10.48. Series of snapshots from simulation of temporal evolution of two-dimensional polycrystal (courtesy of S. Gill).

could be interpreted as the continuous partners of Potts-type models in that they assign an energy penalty to the presence of interfaces which translates into a driving force for grain boundary migration. Our treatment of the sharp interface

580

10 Microstructure and its Evolution

approach to grain growth illustrated the effects of curvature driven boundary motion.

10.5 Microstructure and Materials The root level argument set forth in this chapter has been that in light of the critical role played by structures at the microstructural scale in determining material properties, a crucial prerequisite to a fuller understanding of materials demands an analysis of the factors governing microstructural evolution. The treatment given in this chapter has in no sense been exhaustive. Our discussion has been heavily biased in favor of metallic materials and has made no reference to the rich microstructures found in polymeric materials, for example. On the other hand, our aim has been to illustrate some of the key methodologies (primarily geometric and energetic) which have been brought to bear on the question of microstructure and its evolution. One of the important unanswered questions at the foundation of the approaches provided here concerns the general principles giving rise to the kinetics of microstructural evolution, and whether or not it is appropriate to express microstructures (as in the martensite case) as energy minimizers. A further query that must be posed is that of how best to synthetically couple approaches to the evolution of microstructures and the effect of these microstructures on properties. Part of the quest of the remaining chapters will be to spell out in several case studies how microstructural features manifest themselves in macroscopic properties.

10.6 Further Reading The Structure of Materials by S. M. Allen and E. L. Thomas, John Wiley and Sons, New York: New York, 1999. This text is part of an excellent MIT series on materials science. This particular volume considers structure in materials from the hierarchical perspective considered here as well. Chap. 6 on microstructure provides a number of interesting discussions and ﬁgures to illuminate the nature of microstructure in wide classes of materials. The Theory of Transformations in Metals and Alloys by J. W. Christian, Pergamon Press, Oxford: England, 1965. This classic text provides a deﬁnitive account of many of the key ideas that attend the study of microstructure. Unfortunately, the book has not been reissued in an updated form, but still makes for excellent reading. Theory of Structural Transformations in Solids by A. G. Khachaturyan, John Wiley & Sons, New York: New York, 1983. I haven’t spent as much time with Khachaturyan’s book as I would have liked, but I can say that it is full of insights into a variety of topics covered in the present chapter.

10.6 Further Reading

581

Microstructure and Properties of Materials edited by J. C. M. Li, World Scientiﬁc, Singapore: Singapore, 1996. This work has a number of interesting articles on the implications of microstructure for material behavior. Stability of Microstructure in Metallic Systems by J. W. Martin, R. D. Doherty and B. Cantor, Cambridge University Press, Cambridge: England, 1997. This book gives a deep coverage to many of the ideas raised in the present chapter. Recrystallization and Related Annealing Phenomena by F. J. Humphreys and H. Hatherly, Pergamon Press, Oxford: England, 1996. A useful discussion of the connection between observed macroscopic changes in microstructure and the underlying defect mechanisms that engender it. Introduction to Engineering Materials: The Bicycle and the Walkman by C. J. McMahon, Jr and C. D. Graham, Jr, published by C. J. McMahon, Jr, 1994 (available from author: http://www.seas.upenn.edu/mse/fac/mcmahon.html). This is one of my favorite books. Despite the claimed low level of the book, the discussion of recovery, recrystallization and grain growth is highly instructive as are many other topics covered by the authors. ‘Modeling of Phase Separation in Alloys with Coherent Elastic Misﬁt’ by P. Fratzl, O. Penrose and J. L. Lebowitz, J. Stat. Phys., 95, 1429 (1999) is one of a series of outstanding papers collected in a volume honoring John Cahn on his 70th birthday. This paper provides an outstanding treatment of many of the ideas that have been put forth from both the sharp and the diffuse interface perspective for thinking about two-phase microstructures. ‘Modeling Microstructure Evolution in Engineering Materials’ by A. C. F. Cocks, S. P. A. Gill and J. Pan, Advances in Applied Mechanics, Vol. 36, edited by E. van der Giessen and T. Y. Wu, Academic Press, San Diego: California, 1999. This article gives a unifying perspective on the role of the variational principle associated with conﬁgurational forces as the basis for numerical investigations of microstructural change. ‘Theory of Martensitic Microstructure and the Shape-Memory Effect’ by Kaushik Bhattacharya, unpublished (1998) (a huge pity!) – available from author: [email protected] Bhattacharya’s article gives a complete and thorough discussion of the many ideas that have been brought to bear on the problem of microstructure in martensites. ‘On the computation of crystalline microstructure’ by Mitchell Luskin, Acta Numerica, pg. 191, Cambridge University Press, Cambridge: England, 1996. Luskin’s article covers many similar issues to those found in the article of

582

10 Microstructure and its Evolution

Bhattacharya and provides an alternative view on some of the issues related to energy minimization. ‘The Analytical Modeling of Normal Grain Growth’ by C. S. Pande and S. P. Marsh, JOM, Sept., 25 (1992). Though brief, this article provides an interesting overview of many of the issues involved in modeling grain growth. ‘Theories of Normal Grain Growth in Pure Single Phase Systems’ by H. V. Atkinson, Acta Metall., 36, 469 (1988). A thorough review that mixes insights on both the experimental situation and the models that have been put forth to confront these experiments. ‘Some Fundamentals of Grain Growth’ by D. Weaire and S. McMurry, in Solid State Physics edited by H. Ehrenreich and F. Spaepen, Vol. 50, Academic Press, San Diego: California, 1997. This article is full of interesting ideas on the geometrical aspects of grain growth and includes a discussion of key theoretical ideas as well.

10.7 Problems

1 Details in the Eshelby Inclusion One of the fundamental solutions from which much is made in the evaluation of microstructure is that of the elastic ﬁelds due to ellipsoidal inclusions. (a) In this part of the problem, revisit the problem of the elastic ﬁelds due to inclusions by deriving the expression given in eqn (10.12). Further, perform the integrations required to determine the displacements, and show that the displacements external to the inclusion are given by a 3 3λ + 2µ (10.93) u r (r ) = 2 3r λ + 2µ while those internal to the inclusion are given by r 3λ + 2µ . (10.94) u r (r ) = 3 λ + 2µ Hint: Recall that (r − r )2 = sgn(r − r ). (b) Imitate our analysis of the ﬁelds due to a spherical inclusion, but now deducing the ﬁelds for a cuboidal inclusion.

10.7 Problems

583

2 Elasticity and Diffusion for a Circular Inclusion In this problem we try to imitate in analytic terms the various arguments that have been set forth coupling mechanics and diffusion in the context of microstructural evolution. Consider a single circular precipitate of initial radius R0 . (a) Solve for the elastic ﬁelds of such a circular inclusion on the assumption that it has the same elastic properties as the matrix, but is characterized by an eigenstrain i∗j = 0 δi j . (b) Using the results of part (a) in conjunction with the expression for the concentration given in eqn (10.52) to obtain the instantaneous concentration at the interface between the particle and the matrix. (c) Use this concentration to solve the diffusion equation for a circular region of outer radius Rout with the far ﬁeld boundary condition, c = C0 . (d) Compute ∇c · n at the interface between the particle and the matrix and update the radius of the particle accordingly. (e) What is the ﬁnal size of the particle? 3 Compatibility at Martensite Interfaces Earlier we introduced the compatibility condition F1 = F2 + a ⊗ n,

(10.95)

and noted that the action of F1 is the same as F2 for points within the invariant plane. Prove this assertion in detail by examining the effect of F1 and F2 on points characterized by the vector r = r# e# + r⊥ n. Show that only if r has a nonzero component perpendicular to the invariant plane will the deformation gradients F1 and F2 have a different action on that vector. 4 Rank-One Connection for Model Deformations Examine the deformation mapping given by x1 = X 1 ± γ X 2 ,

(10.96)

x2 = X 2 ,

(10.97)

x3 = X 3 ,

(10.98)

with the ± sign signifying that we are to take + if the region of interest is above the invariant plane, and − if below. First, sketch the outcome of applying this mapping to points lined up along vertical lines, and then compute the deformation gradients in the two regions. Finally, show that the deformation gradients in question satisfy the rank-one condition, and ﬁnd the vectors a and n.

584

10 Microstructure and its Evolution

5 Different Paradigms for Motion of a Curved Interface Implement the Potts, phase ﬁeld and sharp interface descriptions for the motion of a curved interface. In particular, in ﬁg. 10.42, we showed schematically how these three classes of models are used to describe the evolution of the same microstructure. In this problem, use these three schemes to obtain the ﬂattening of an initially curved interface. Assume an initial parabolic proﬁle and examine the time evolution predicted by these three schemes as the interface becomes ﬂat.

Part four Facing the Multiscale Challenge of Real Material Behavior

ELEVEN

Points, Lines and Walls: Defect Interactions and Material Response

11.1 Defect Interactions and the Complexity of Real Material Behavior In previous chapters, we have begun the attack on the problem of the observed thermomechanical properties of materials from a number of different perspectives. One of our key realizations has been the conspiratorial role of defects in governing the response of materials. Thus far, we have largely concentrated on the structure and energetics of individual defects with less attention given to the implications of these defects for material response. Our efforts have been primarily divided along dimensional lines, with point defects, line defects and interfacial defects each being treated as an end unto itself. The concern of the present chapter is to make evident the claim that such divisions are a theorist’s artiﬁce and that, in general terms, it is the synthetic response of all of these different types of defects in concert that gives rise to the observed complexity of materials. We begin our discussion with the consideration of diffusion. In earlier chapters, we noted that diffusion is mediated by the presence of point defects. However, until now, we have not given any quantitative analysis of the lubricating effect of other defects in the context of diffusion. We have already seen in ﬁg. 9.1 that bulk diffusion can be negligible in comparison with the diffusion that takes place along surfaces, grain boundaries and dislocations. As a particular realization of this class of problem, we consider the case of surface diffusion with special reference to some of the counterintuitive diffusion mechanisms that take place at surfaces. A second fundamental theme that will be taken up in this chapter in which there is an interplay between the various types of defects introduced earlier is that of mass transport assisted deformation. Our discussion will build on the analysis of diffusion at extended defects. We will begin with an examination of the phenomenology of creep. A third example in which there is a mutual interplay between the different types of defects that we have discussed in previous chapters is that provided by the 587

588

11 Points, Lines and Walls: Defect Interactions and Material Response

dislocation–grain boundary interaction. In the context of polycrystal plasticity, it is clearly of interest to determine the conditions under which plasticity in one grain can be communicated to adjacent grains. Experiments indicate that under certain conditions, dislocations may pass from one grain into neighboring grains. Clearly, the presence of grain boundaries can have the effect of impeding dislocation motion, and we will take up this topic in section 11.4. The next example that will be set forth as an example of a problem in which multiple defect types can be present simultaneously is that of fracture. Our discussion will begin with an examination of the way in which cracks can be built up as superpositions of dislocations. This leads naturally to questions of the interaction of dislocations and cracks and culminates in the analysis of the intriguing problem of crack tip nucleation of dislocations. An age old observation around which entire revolutions took place is that if a pure metal is mixed with small amounts of some other metal, the resulting strength of the material will be altered. Witness the Bronze Age. These observations will be codiﬁed in quantitative terms in section 11.6 where we show how the yield stress varies as a result of obstacles to dislocation motion. These observations, once again, drive home the potency of the synthetic effect of different types of defects in tandem. We will sketch some of the key qualitative ideas that have been elucidated with respect to both solution and precipitate hardening which are the technical names for the area of study that has arisen in response to the simple observations that made the Bronze Age possible. The development in this part of the chapter will culminate in certain scaling arguments which reveal how the yield stress scales with various microstructural parameters. In keeping with the theme of the present chapter, our basic argument will be that although dislocations are the key players in plastic deformation, it is their interactions with each other and other obstacles that gives rise to much of the observed richness of plastic deformation. The basic aim of this chapter is to illustrate the way in which the various defects we have introduced in previous chapters can form partnerships that enrich the properties of materials and the processes that transpire within them. The logic of the chapter is to provide evidence for this viewpoint through the medium of case studies. As usual, we have not been exhaustive. 11.2 Diffusion at Extended Defects 11.2.1 Background on Short-Circuit Diffusion In chap. 7, we discussed the fundamental role of point defects in diffusion. We also hinted at the serious amendment to diffusion rates that is mediated by the presence of extended defects such as dislocations and grain boundaries (see ﬁg. 9.1). As was noted above, diffusion rates along defects can often be so much larger than those in

11.2 Diffusion at Extended Defects

589

the bulk that the bulk mechanisms can be rendered almost irrelevant. As a result of this insight, it is evident that we must reconsider diffusion more carefully in light of the presence of line and interfacial defects. Our present task is to build on the foundations laid in chap. 7, but now with special reference to the diffusive processes that take place at extended defects. The basic argument will be that by virtue of the more open atomic-level environments near extended defects, the activation energy both for point defect formation and migration will often be reduced relative to bulk values. We will build our case around a fundamental case study through the consideration of diffusion at surfaces. The surface diffusion example will illustrate not only how diffusive processes are amended at extended defects, but will also illustrate the shortcomings of the transition state formalism when the detailed atomic-level mechanisms are not known a priori.

11.2.2 Diffusion at Surfaces Because of the widespread interest in growth of material systems by deposition, the subject of surface diffusion is one of enormous current interest. The example of surface diffusion being taken up here is of interest to our overall mission for several different reasons. First, as noted above, surfaces are one of the most important sites of communication between a given material and the rest of the world. Whether we interest ourselves in oxidation and corrosion, catalysis, the crystal surface is the seat of tremendous activity, most of which is mediated by diffusion. A second reason that we have deemed it important to consider the role of surface diffusion is that our analysis will reveal the dangers that attend the use of transition state theory. In particular, we will appeal to the existence of ‘exchange mechanisms’ for diffusion that reveal that the diffusion pathways adopted on some crystal surfaces are quite different than those that might be suggested by intuition. Exchange Mechanisms for Surface Diffusion. Our discussion of transition state theory in chap. 7 showed that in those cases when we are lucky enough to know the details of the transition pathway associated with a given diffusion mechanism, atomic-level analysis can shed important light on the process of diffusion. On the other hand, as we have already emphasized, the successful application of the ideas of transition state theory ultimately requires a knowledge of the transition pathway. Field-ion microscopy in conjunction with ﬁrst-principles analysis of the energetics of metal surfaces has led to a convincing picture of surface diffusion in some instances that is entirely contrary to the ideas built around intuition. The simplest picture of diffusion on the (001) surface of an fcc metal such as Al or Pt would hold that atomic jumps take place from one binding site to the next via

590

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.1. Competing surface diffusion mechanisms on an fcc (001) surface (adapted from Feibelman (1990)): (a) intuitive mechanism in which adatom moves from one fourfold site to another by passing across bridge site, and (b) exchange mechanism in which diffusion occurs by concerted motion both of adatom and its subsurface partner.

the pathway illustrated in ﬁg. 11.1(a). The contention in this case would be that diffusion takes place by the simple motion of the atom from one fourfold binding site to the next through the intermediate twofold bridge site. On the other hand, observations on Pt and Ir (001) determined that diffusion takes place by hopping exclusively along 100 and 010 directions as opposed to the 110 direction that would correspond to crossing the bridge site. Reconciliation of the simplest intuitive notions concerning diffusion with these observations would require that the adatom pass through an intermediate state in which it is onefold coordinated and sits directly above one of the surface atoms. This mechanism is associated with an unphysically high activation energy. Because of the failure of the mechanism suggested above to account for observed diffusion, alternative mechanisms must be sought. To quote Feibelman (1990), ‘The key to developing a correct model of surface diffusion is to think of it as a chemical phenomenon rather than in terms of a hard sphere moving on a bumpy plane.’ In terms of what we have learned about the energetics of atomic-level bonding in previous chapters, Feibelman’s exhortation is a reminder that there may be alternative mechanisms in which the adatom does not suffer the signiﬁcant loss of coordination implied by the intuitive diffusion mechanism involving bridge sites suggested above. In particular, an alternative ‘exchange mechanism’ in which the adatom burrows into the surface at the same time that the atom previously at one of the surface sites vacates its position has led to a plausible explanation for all of the observations. This mechanism is illustrated in ﬁg. 11.1(b). In the case of Al, Feibelman (1990) found that this mechanism was associated with an activation energy of only 0.20 eV, in contrast with the 0.65 eV associated with the naive but intuitive mechanism discussed earlier. As a result, the exchange mechanism explains both the orientational preferences observed in ﬁeld-ion microscopy experiments as well as the corresponding activation energies. One of the key reasons we have considered the exchange mechanism for surface diffusion is as a reminder of the inherent difﬁculties in using transition state theory.

11.2 Diffusion at Extended Defects

591

While it is true that once there is conﬁdence that the correct mechanism has been identiﬁed that transition state theory will usually yield a reasonable description of the energetics, it is also true that ignorance of the correct pathway can lead to results that are completely misleading. As a result, work has concentrated on important new developments in the area of determining the relevant reaction pathways in complex systems. In particular, sophisticated techniques have been set forth that are aimed at uncovering the optimal reaction pathway in cases where intuition does not sufﬁce as a guide. Surface Steps and Diffusion. Recall from our discussion of surfaces in chap. 9, there are a series of structures at increasing levels of complexity that may be found on crystal surfaces. Beyond the reconstructions that attend ﬂat surfaces, we also noted the important role of surface steps as key structural components of generic surfaces. These steps are interesting not only from the perspective of their geometry, but also from the point of view of their role in altering the nature of the diffusive processes that take place on surfaces. In this section, our intention is to examine a particular feature of such diffusion, namely, the existence of a barrier resulting from surface steps. The evidence for reﬂecting barriers at the edge of surface terraces derives from a number of different sources, one important example of which is ﬁeld-ion microscopy. For example, it has been found that there is an enhancement in the likelihood of ﬁnding an adatom just adjacent to the top edge of a surface step. From the standpoint of the simple random walk analysis put forth earlier, one way to interpret the results of the types of experiments sketched above is via the random walker with reﬂecting walls. The basic idea in this case is the presumption that the random walker can exercise excursions within the conﬁnes of some ﬁnite region, but whenever the walker reaches the boundary of the region it is reﬂected from the walls. These phenomenological ideas have been lent quantum mechanical credibility through consideration of the energetics of adatoms near steps. In particular, examination of the energetics of adatoms near a surface step has led to the elucidation of the concept of the Schwoebel barrier. The total energies of adatoms in the vicinity of a surface step have been computed using both empirical and ﬁrst-principles techniques though for the present purposes we will consider but one example of a calculation of this barrier from the empirical perspective. The rough physical expectation is that as an adatom approaches a surface step from above, in the immediate vicinity of that step it will suffer an even greater loss of coordination than that it already experiences on a free surface, with a concomitant energy penalty. A series of energetic snapshots for the (111) surface of Pt are shown in ﬁg. 11.2 and reveal the energetics of different conﬁgurations of the adatom near

592

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.2. Illustration of energetics of an adatom near a surface step on the (111) surface of Pt (adapted from Jacobsen et al. (1995)).

a step. As claimed above, the key remarkable qualitative feature of the near-step energetics is the existence of both a barrier to adatom motion across the step from above, and an enhanced bonding for those adatoms arriving at the step edge from below. From the overall perspective of the present chapter, our ambition in brieﬂy describing the energetics of surface diffusion has been to illustrate the additional complexity that is ushered in as a result of the simultaneous action of more than one type of defect. In particular, we have shown that via a counterintuitive exchange mechanism, the activation energy for surface diffusion can be lowered by 0.4 eV relative to the intuitive motion associated with an imagined random walker on a surface. In addition, we have also shown that the presence of surface steps can have signiﬁcant implications for the nature of diffusion on surfaces.

11.3 Mass Transport Assisted Deformation In chap. 7 we laid the foundations for the analysis of mass transport in solids. In the current section, our aim is to examine the ways in which mass transport can assist the deformation that occurs in a given material. As a preliminary, we remind the reader of one of the key features of the deformation mechanism map introduced in ﬁg. 7.7. We refer to the fact that in many instances for stresses well below the putative yield stress, permanent deformation is still observed. Such deformation usually occurs at temperatures which are larger than, say, 0.3TM ,

11.3 Mass Transport Assisted Deformation

593

Fig. 11.3. Schematic of strain as a function of time in a constant-stress creep test (adapted from Courtney (1990)).

where TM is the melting temperature. These high-temperature mechanisms are referred to generically as creep and will be our present concern.

11.3.1 Phenomenology of Creep The phenomenology of creep is best illustrated through the vehicle of the so-called creep test in which a specimen is subject to either a constant load or a constant stress, and the deformation is monitored as a function of time. The generic outcome of such a test is illustrated in ﬁg. 11.3 and suggests that the creep behavior may be divided into three distinct regimes, denoted primary, secondary and tertiary creep. The primary regime is characterized by an initially high strain rate which decreases with increasing time until a so-called ‘steady-state’ regime is entered in which the strain rate is roughly constant. The tertiary regime is characterized by an increase in the strain rate and terminates with the failure of the material. In considering creep, there are several different control parameters that are known to inﬂuence the resulting deformation. Clearly, with increasing stress, the strain rate ˙ will be increased. Similarly, an increase in temperature also serves to increase ˙ . We continue our discussion by examining these two different parameters in turn. Before embarking upon that discussion, we note that our analysis will highlight the signiﬁcant empirical insights that have been gained into the creep process, with less emphasis on the models that have been advanced to rationalize these empirical gains.

594

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.4. Schematic of strain rate ˙s as a function of normalized stress (adapted from Nabarro and de Villiers (1995)). D refers to the bulk diffusion constant and b is a measure of the lattice parameter.

One of the elemental empirical insights into the creep process concerns the stress dependence of the creep rate. A broad range of experimental data can be captured on the assumption of a power law relation between the strain rate ˙ and the stress σ . In particular, the strain rate can be written in the form n σ , (11.1) ˙ ∝ µ where the exponent n varies depending upon the situation. This behavior is illustrated qualitatively in ﬁg. 11.4. Another critical question is how the creep rate depends upon temperature. As hinted at in the title of this section, creep is in many instances mediated by the presence of mass transport. Part of the basis of this insight is the observed temperature dependence of the creep rate. In particular, it has been found that creep is thermally activated. Indeed, one can go further than this by noting the relation between the activation energy for diffusion and that of the creep process itself. A plot of this relation is shown in ﬁg. 11.5. As a result, we see that the temperature dependence of the creep rate may be written in the form ˙ = const.e−E/kT .

(11.2)

Our insights on both the stress and temperature dependence of the strain rate may thus be uniﬁed in a single phenomenological equation of the form n σ ˙ = A e−E/kT . (11.3) µ

11.3 Mass Transport Assisted Deformation

595

Fig. 11.5. Plot of activation energies for creep and bulk diffusion (adapted from Courtney (1990)).

From a theoretical perspective, what we are left with is the ambition of explaining the stress and temperature dependence of the strain rate evoked in eqn (11.3) from a mechanistic perspective. As we will see, the problem is not so much a shortage of ideas in this regard, but rather an embarrassment of choices, without any clear scheme which will permit the falsiﬁcation of these models. In the remainder of our discussion on mass transport assisted deformation, the plan is to sketch the ideas associated with Nabarro–Herring and Coble creep. I should note that this discussion is little more than a report on the party line as regards the modeling of creep phenomena and further that we have not done justice to both what is known and what remains unknown in this important ﬁeld. In particular, we omit all reference to an important alternative mechanism related to the mass transport assisted climb of dislocations, thus allowing them to breach obstacles to their further glide.

11.3.2 Nabarro–Herring and Coble Creep The class of creep mechanisms of interest here are those that are mediated by stress-biased diffusion. If we are to consider the vacancy ﬂux in a given grain within a material that is subjected to an applied stress, it is argued that the vacancy formation energy differs in different parts of the grain, and hence that there should be a gradient in the vacancy concentration leading to an associated ﬂux. This

596

11 Points, Lines and Walls: Defect Interactions and Material Response

ﬂux of vacancies (or atoms) can, with the accumulated weight of time, lead to a macroscopic change in the shape of the material. This mechanism results in a strain rate that is linear in the applied stress and with an activation energy that is identical to that for self-diffusion. The distinction between the Nabarro–Herring and Coble mechanisms is one of variety rather than form. In particular, the Nabarro–Herring mechanism is associated with lattice diffusion within the grains, while the Coble mechanism is built around diffusion along the grain boundaries. In both cases, however, the key point is the presence of a gradient in the vacancy concentration induced by the applied stress. Our ambition in the paragraphs to follow is to illustrate an approximate heuristic model which shows how the presence of an applied shear stress can result in mass transport mediated deformation. We begin with the notion that the crystal of interest is subjected to a shear stress. From a two-dimensional perspective, for example, we then make use of the fact that the shear stress 0 σ σ = , (11.4) σ 0 may be rewritten in principal coordinates as σ 0 . σ = 0 −σ

(11.5)

In principle, we are thus faced with solving a boundary value problem for a region like that shown in ﬁg. 11.6 with the aim being to evaluate the mass transport that arises by virtue of the spatially varying chemical potential, and hence, mass currents, that arise in response to the nonuniform stress. In practice, since we are only interested in an estimate of the effect, we resort to an approximate analysis in which the relevant chemical potentials and mass ﬂux, and attendant strain rate are all evaluated heuristically. The argument begins with reference to ﬁg. 11.6 with the claim that the vacancy formation energy for the faces subjected to tensile stresses differs from that on the faces subjected to compressive stresses. Again, a rigorous analysis of this effect would require a detailed calculation either of the elastic state of the crystal or an appeal to atomistic considerations. We circumvent such an analysis by asserting that the vacancy concentrations are given by f

c(T ) = e−(vac −σ )/kT ,

(11.6)

and f

c(C) = e−(vac +σ )/kT ,

(11.7)

where the superscripts T and C refer to tensile and compressive, respectively. To

11.3 Mass Transport Assisted Deformation

597

MACROSCOPIC STRESS

Fig. 11.6. Schematic of how stress assisted mass transport results in a net strain rate (adapted from Herring (1950)).

really understand this result, we need to reﬂect further on the deﬁnition of the vacancy formation energy given in section 7.3.3. In particular, we need to see how those arguments should be amended to account for the presence of a stress. A simple plausibility argument can be constructed as follows. From an atomistic perspective, the vacancy formation energy associated with plucking a near-surface f atom out and placing it on the surface can be represented approximately as vac ≈ f¯b, where f¯ is the mean force exerted by neighboring atoms as the atom is plucked to the surface. In the presence of the tractions imagined above, there is either a suppression (tensile case) or enhancement (compressive case) in this energy cost, which can now be written as f f vac (stress) = vac ± σ Aatom b,

(11.8)

f f vac (stress) = vac ± σ ,

(11.9)

or

where we have deﬁned Aatom as the area over which the traction is working during the plucking process. The next step in the argument is to estimate the amount of mass transported from one face to the other by virtue of the concentration gradient embodied in eqns (11.6) and (11.7). In particular, the ﬂux is given by j = −D(∂c/∂ x), where the gradient term is estimated as ∂c c(T ) − c(C) ≈ , ∂x l

(11.10)

598

11 Points, Lines and Walls: Defect Interactions and Material Response

where the parameter l is a measure of the size of the region in question. We note that our objective is to compute the strain rate which is deﬁned as ˙ =

1 dl , l dt

(11.11)

and may be written in terms of the amount of volume arriving on the face of interest per unit time as a result of the relation 1 dV dl = 2 . dt l dt

(11.12)

The rate d V /dt can be evaluated by recourse to the relation dV = l 2 j, dt

(11.13)

with the result that when all the pieces of our analysis are assembled, we have ˙ =

f 2D0 σ −(vac m )/kT +vac . e 2 l kT

(11.14)

At this point, several comments are in order. First, we note that we have recovered an expression for the strain rate which jibes with the empirical result presented in eqn (11.3). In this case, the stress exponent is unity. Our discussion of creep given above implicitly assumed that the mass transport resulting in an overall shape change took place through the crystalline region itself. An alternative diffusion mechanism, founded upon the same principles as the discussion of Nabarro–Herring creep given above is based on reconsidering those arguments when the mass transport is mediated by grain boundary diffusion rather than bulk diffusion. The result of this analysis is a change in the way that eqn (11.14) scales with grain size. In particular, in the context of the Coble mechanism, the strain rate is written ˙ =

2Dgb σ δ . l 3 kT

(11.15)

The new features of this result in comparison with that of eqn (11.14) are the presence of the grain boundary diffusion constant, Dgb , and the introduction of a parameter δ which is a measure of the thickness of the region over which diffusion is enhanced in the vicinity of the grain boundary. Note that in the context of both the Nabarro–Herring analysis and that of Coble, the strain rate is found to vary linearly with the applied stress. In particular, this result is consistent with dubbing this process ‘diffusional viscosity’ as did Herring (1950) in his original work. Indeed, the identiﬁcation of a material parameter such as the ‘viscosity’ and its associated scaling properties with grain size and temperature represents another example of the type of micro–macro connection

11.4 Dislocations and Interfaces

599

Fig. 11.7. Examination of the success of the hypothesis of linear stress dependence of the creep strain rate in the high-temperature regime (adapted from Nabarro and de Villiers (1995)).

which is at the heart of the viewpoint taken in the present work. The question of how such models jibe with experience is partially addressed in ﬁg. 11.7 which reveals that the linear stress dependence is well obeyed for a range of materials. It bears repeating that our discussion has been little more than a caricature of this important ﬁeld.

11.4 Dislocations and Interfaces In the previous chapter we took preliminary steps to examine grain boundary motion. However, in the absence of considerations of dislocations in the vicinity of such grain boundaries, this description is incomplete. In the present section, we begin by examining the way in which dislocations and grain boundaries merge. In particular, for the special geometric case of low-angle grain boundaries, the boundary may be thought of as nothing more than a superposition of dislocations, with tilt boundaries being built up of edge dislocations and pure twist boundaries being built up by screw dislocations. However, our analysis can go further than this. In addition, we pose the question of how dislocations that impinge on a grain

600

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.8. Representation of grain boundary as an array of dislocations (adapted from Amelinckx (1979)).

boundary are greeted by the boundary which serves as an obstacle. Such processes can lead to both dislocation pile-ups and slip transmission in which crystal slip in one grain passes to adjacent grains.

11.4.1 Dislocation Models of Grain Boundaries We begin our geometric discussion with the case of pure tilt boundaries on the grounds that the connection between dislocations and the boundary is most evident visually in this case. As was discussed in some detail in chap. 9, a tilt grain boundary is characterized by a simple misorientation between the two grains as was discussed in chap. 9. The intent of this section is to illustrate that a simple superposition of the elastic displacements implied by the Volterra solution for straight dislocations discussed in chap. 8 can lead to exactly the same type of misorientation. First, we consider the most elementary geometrical arguments that can be set forth in this regard. The question we pose at this moment is what is the relation between the dislocation spacing and the misorientation. For concreteness, consider a series of uniformly spaced edge dislocations with Burgers vector of length b such as is shown in ﬁg. 11.8. What we note immediately is that this geometry may be thought of as the introduction of an extra half-plane each time we traverse the distance D along the boundary plane. As a result, the dislocation spacing and the

11.4 Dislocations and Interfaces

601

misorientation angle are related by D=

b . 2 sin(θ/2)

(11.16)

Although a length scale tied to the underlying discrete lattice is present in this equation, there is no clear selection mechanism that distinguishes between those geometries that have a special relation to the underlying crystalline lattice and those that do not. What we are noting is that not all dislocation spacings are equal and that for certain special choices of this spacing the lattice and the dislocations are locked into a commensurate relationship. One of the immediate questions that arises in the context of such a model of grain boundaries is what it might have to say about the stress ﬁelds and energies of that boundary. An immediate reaction to the claim that grain boundaries may be thought of as arrays of dislocations is that this must mean that boundaries have long-range stress ﬁelds. However, as will be shown in short order, the long-range dislocation stress ﬁelds when superposed in the special way demanded by a grain boundary lead to cancellations that leave exponentially decaying ﬁelds. For simplicity, consider the isotropic linear elastic description of the problem. The total stress is obtained by summing up the contributions of the constituent dislocations. If we consider the shear stress components for concreteness, then the total stress for the boundary with dislocation spacing D is ∞ µb 1 x3 σx y (x, y) = 2 2 2 2π(1 − ν) n=−∞ [x + (y − n D) ] ∞ (y − n D)2 . −x 2 2 2 n=−∞ [x + (y − n D) ]

(11.17)

All this formula instructs us to do is to take the contribution to the total stress of each dislocation using the results of eqn (8.38) and to add them up, dislocation by dislocation. We follow Landau and Lifshitz (1959) in exploiting the Poisson summation formula to evaluate the sums. Note that while it would be simple enough to merely quote the result, it is fun to see how such sums work out explicitly. If we use dimensionless variables α = x/D and β = y/D, then the sum may be rewritten as σx y (x, y) =

∞ µbx α 2 − (β − n)2 . 2π D 2 (1 − ν) n=−∞ [α 2 + (β − n)2 ]2

(11.18)

The next step in the thrust to beat the sum into submission is to recognize that if

602

11 Points, Lines and Walls: Defect Interactions and Material Response

one deﬁnes J (α, β) =

∞ n=−∞

α2

1 , + (β − n)2

then the expression for the stresses is given in turn as

∂ J (α, β) µbx J (α, β) + α . σx y = − 2π D 2 (1 − ν) ∂α

(11.19)

(11.20)

With these clever algebraic machinations behind us, the original problem has been reduced to that of evaluating the sum J (α, β). Recall that the Poisson summation formula tells us ∞ ∞ ∞ f (n) = f (x)e2πikx d x. (11.21) n=−∞

k=−∞

−∞

For the problem at hand, the Poisson summation formula allows us to rewrite our sum as ∞ −2πiku ∞ e 2πikβ e du. (11.22) J (α, β) = 2 2 −∞ α + u k=−∞ Evaluation of the relevant integrals is immediate and results in J (α, β) =

∞ π 2π + e−2πkα cos 2πkβ. α α k=1

(11.23)

Consultation of Gradshteyn and Ryzhik (1980) or some other reference permits −kt cos kx = sinh t/(cosh t − cos x), the exact evaluation of the sum 1 + 2 ∞ k=1 e which for our case leads to the stress 2π x 2π y cosh −1 cos µbπ x D D σx y (x, y) = 2 (11.24) . D (1 − ν) 2π x 2 2π y − cosh cos D D However, we could have made more immediate progress with eqn (11.23) by recalling the signiﬁcance of the parameter α. In dimensionless terms this parameter is a measure of the distance from the boundary and for large distances we could safely keep only the term associated with k = 1. In this case, we ﬁnd σx y (x, y) =

2π µbx − 2π x 2π y e D cos . D 2 (1 − ν) D

(11.25)

Having attained our end, namely, the determination of the grain boundary stresses (note that the computation of σx x and σ yy proceeds similarly), what may be learned about boundaries themselves? We begin with a simple, but profound

11.4 Dislocations and Interfaces

603

observation concerning the solution. Because of the exponential dependence of the stresses on the distance from the boundary, we see that the elastic perturbation due to a boundary is short-ranged. Though dislocations have their characteristic long-range elastic signature, grain boundaries lead only to a localized inﬂuence. As we have already remarked in earlier discussions on interfaces in materials, there is a hierarchy of energies associated with such interfaces commencing with surfaces, which have the highest energies, passing through grain boundaries, which are intermediate in energy, and ﬁnishing with stacking faults, which are usually at the bottom of the energy scale. One issue of interest that our dislocation model of grain boundary permits us to revisit is that of the energies of grain boundaries. The simple argument that is made in exploiting the dislocation model for an estimate of the grain boundary energy is that the boundary may be thought of energetically as the sum of the energies of the isolated dislocations, where the long-range cutoff is taken to be determined by the dislocation spacing itself. To make this argument more plausible, consider the stress at the boundary in the immediate vicinity of a particular dislocation. Note that the total stress is given by eqn (11.24), and we are interested in a point (x, y) in the immediate vicinity of a particular dislocation. Expansion of the relevant cos and cosh factors to quadratic order in their arguments results in σx y (x, y) =

x 2 − y2 µbx , 2π(1 − ν) (x 2 + y 2 )2

(11.26)

which is seen to be exactly the shear stress component for a single dislocation at the origin. This result suggests the plausibility of treating the boundary as a series of single dislocations, each with an energy E disl =

D µb2 ln . 4π(1 − ν) 2r0

(11.27)

To obtain this result, all we have done is to use the results from chap. 8 for the energy of a single dislocation within isotropic linear elasticity. We may make an approximate evaluation of the grain boundary energy on the grounds that each dislocation speciﬁes the energy of its local neighborhood on the boundary. Hence, the energy per unit depth of boundary is given by E gb =

D µb2 ln , 4π D(1 − ν) 2r0

(11.28)

which if we recall that θ = b/D may be rewritten as E gb = θ(A − B ln θ),

(11.29)

with A = [µb/4π(1 − ν)] ln(b/2r0 ) and B = [µb/4π(1 − ν)]. This is the

604

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.9. Energy of tilt grain boundary as a function of misorientation angle (adapted from Sutton and Ballufﬁ (1995)).

noted result of Read and Shockley for the energy of a grain boundary, and is plotted in comparison with experimental values in ﬁg. 11.9. As was remarked earlier, one of the serious shortcomings of the present model, and a fact which is revealed in considering the experimental numbers, is that there is no provision for the possible commensurability of the lattice parameter and the dislocation spacing D. In particular, for certain choices of the misorientation angle, very special geometries arise as was noted in our earlier discussion on coincidence site lattices. By way of contrast, the dislocation model holds that the parameter D may be varied continuously without prejudice.

11.4.2 Dislocation Pile-Ups and Slip Transmission Dislocations and grain boundaries form partnerships other than the one described above. Another intriguing mechanism involving dislocations and grain boundaries arises when dislocations, during the process of their gliding motions, impinge on a grain boundary in their pathway which serves as an obstacle. Our thinking in the current section will be founded upon two alternative approaches to the question of dislocation pile-ups. We will begin with a discrete analysis of such problems. However, it will be seen to be mathematically more convenient to assume that the set of dislocations piled up against a boundary are continuously distributed, unleashing the powerful machinery of integral equations to make analytic headway. We begin with a consideration of the relevant phenomenology. Fig. 11.10 shows a number of different possible outcomes of the interaction between an array of

11.4 Dislocations and Interfaces

605

Fig. 11.10. Schematic of interactions between dislocations and grain boundaries (courtesy of Ian Robertson).

piled-up dislocations and a grain boundary. Several of the mechanisms feature the development of plastic deformation (i.e. dislocation motion) in the adjacent grain. On the other hand, the pile up of dislocations against a boundary can result in processes within the grain boundary plane itself. As shown in the ﬁgure, two possible outcomes are the development of dislocation motion within the grain boundary plane or wholesale fracture along the grain boundary. The advent of transmission electron microscopy opened the doors to the direct observation of processes such as the pile-up of dislocations at a grain boundary and the subsequent commencement of dislocation motion in adjacent grains. The process of slip transmission described above may be seen from the perspective

606

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.11. Slip transmission process (taken from Lee et al. (1990)).

of transmission electron microscopy in ﬁg. 11.11. What we note in inspecting this ﬁgure is that the geometric positions of the dislocations adopt a pleasing disposition which suggests a regular mathematical relation governing the spacings of the piled up dislocations. Two central questions that arise in the context of this geometry are: (i) what governs the distribution of pile-up dislocations, and (ii) what are the implications of such a pile-up, especially in terms of the stresses it produces in adjacent grains? Our fundamental assertion concerning the geometry of pile-ups is that they reﬂect the equilibrium spacing of the various dislocations which are participants in such a pile-up. From a discrete viewpoint, what one imagines is an equilibrium between whatever applied stress is present and the mutual interactions of the dislocations. In simple terms, using the geometry depicted schematically in ﬁg. 11.12, we argue that each dislocation satisﬁes an equilibrium equation of the form 1 = 0. (11.30) τapp (x) + A x − xi i= j j

11.4 Dislocations and Interfaces

607

Fig. 11.12. Schematic representation of pile-up geometry (adapted from Smith (1979)).

This equation considers the equilibrium of the j th dislocation. In particular, it is nothing more than a dislocation-by-dislocation statement of Newton’s ﬁrst law of = 0, which says that the total force on the j th dislocation motion, namely, F(tot) j is zero. The factor A is determined by the elastic moduli and differs depending upon whether we are considering dislocations of edge (A = µb/2π(1 − ν)), screw(A = µb/2π ) or mixed character. The problem of determining the equilibrium distribution of the dislocations in the pile-up has thus been reduced to one of solving nonlinear equations, with the number of such equations corresponding to the number of free dislocations in the pile-up. For further details see problem 3 at the end of the chapter. A more elegant (and mathematically tractable) description of the problem of dislocation pile-ups is to exploit the representation of a group of dislocations as a continuous distribution. This type of thinking, which we have already seen in the context of the Peierls–Nabarro model (see section 8.6.2), will see action in our consideration of cracks as well. The critical idea is that the discrete set of dislocations is replaced by a dislocation density ρb (x) such that dn(x) = ρb (x)d x.

(11.31)

What this equation tells us is the number of dislocations between x and x + d x. The key constraint on the function ρb (x) is that it be properly normalized so that xmax n tot = ρb (x)d x, (11.32) xmin

where n tot is the number of dislocations in the pile up. Once we have taken this step, the equilibrium condition for the dislocations is represented by an integral equation ∞ ρb (x )d x µb + τext (x) = 0. (11.33) P 2π −∞ x − x This equation should be seen as the continuous analog of eqn (11.30). It expresses the equilibrium of the inﬁnitesimal dislocation at position x with the applied stress, τext (x) and the remaining inﬁnitesimal dislocations in the distribution ρb (x ). The P refers to the principal value integral and eliminates the self-interaction of the dislocation at x with itself.

608

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.13. Representation of dislocation pile-up as a continuous distribution of dislocations.

As a concrete example of such a problem, we follow Lardner (1974) in considering n screw dislocations, each with Burgers vector of magnitude b in the region x > 0, driven to the left by a constant shear stress −τ and bounded by a barrier at x = 0 (in mentioning the barrier, we have a grain boundary in mind, for example). Furthermore, if we assume that the pile-up has a width a, then the solution to this problem which we quote without derivation (for details see Lardner (1974)) is 2τ a − x . (11.34) ρb (x) = µb x To determine the width a, recall eqn (11.32) which in this instance yields a πτa n= , (11.35) ρb (x)d x = µb 0 with the implication that a = µnb/π τ . The dislocation density associated with this proﬁle is shown in ﬁg. 11.13, and demonstrates the same qualitative features as noted in the observed pile-ups. The next question we pose is how such a dislocation distribution affects the stress state in its neighborhood. The pertinence of this question to broader issues in the mechanics of materials is that a quantitative understanding of dislocation pile-ups has been invoked to explain the dependence of the yield stress on the grain size as canonized in the Hall–Petch relation and depicted in ﬁg. 8.2. One hypothesis put forth with the aim of explaining the Hall–Petch behavior is that the presence of such pile-ups reduces the stress needed to inspire slip in adjacent grains. As we will show below, the grain size enters as the characteristic dimension by which the pileup size is measured, and larger pile-ups lead to larger stresses in adjacent grains and thus smaller stresses are needed to induce slip within them. The geometry we have

11.5 Cracks and Dislocations

609

Fig. 11.14. Schematic of the pile-up of dislocations at a grain boundary. Enhancement in the stress ﬁeld in an adjacent grain as a result of the presence of the pile-up is also indicated schematically.

in mind is depicted in ﬁg. 11.14 In attempting to explain the Hall–Petch behavior, the argument has been advanced that once slip has commenced in the grain that is favorably oriented for slip, dislocations will pile-up against the boundary that is the terminus of the slip plane. The presence of this pile-up has the effect of increasing the stress in the adjacent grain which is itself less favorably oriented for slip. The pile-up is thought to catalyze slip in the adjacent grain by virtue of the increased stress there. The total stress ahead of the pile-up is given by µb a ρb (x )d x . (11.36) τ (x) = −τ + 2π 0 x − x This equation reﬂects the addition of the externally applied shear stress, −τ , as well as the contribution of the pile-up itself as embodied in the integral. Substitution of the dislocation density determined above yields x −a τ (x) = −τ . (11.37) x What this result demonstrates is the presence of an enhanced stress in front of the pile up (x < 0). We forego a discussion of the implications of such stress enhancements for dislocation nucleation until section 11.5.3.

11.5 Cracks and Dislocations In chap. 2, we noted that linear elastic fracture mechanics offers powerful insights into the continuum description of fracture processes. On the other hand, we also noted that the occurrence of fracture ultimately depends upon mechanisms that take place in the vicinity of the crack tip, some of which depend upon atomic-level

610

11 Points, Lines and Walls: Defect Interactions and Material Response

details. It is the aim of the present section to recount some of the issues that arise in trying to bring atomic-level insights to bear on the problem of fracture especially in the context of crack tip dislocation nucleation. Our reason for including this discussion in the present chapter is the fact that our understanding of cracks and the fracture process can be signiﬁcantly extended once we adopt a broader view in which cracks and dislocations are considered simultaneously. In coming sections we undertake a discussion of the conspiracy that arises once dislocations and cracks are taken into consideration jointly. In particular, the goal is to examine two key issues related to dislocation–crack interactions. First, we wish to consider the notion of crack tip shielding in which, by virtue of the presence of a dislocation in the neighborhood of a crack tip, the crack tip ﬁelds are amended locally. In particular, we will interest ourselves in the renormalization of the crack tip stress intensity factor by virtue of the presence of dislocations. Once we have built up the tools for handling dislocations and cracks simultaneously, we aim to consider the competition between cleavage and nucleation of dislocations at a crack tip. Our fundamental argument will be that the elastic energy release rate can be balanced either against the creation of new free surface or in the installation of crystalline slip in the form of dislocations.

11.5.1 Variation on a Theme of Irwin In chap. 2 the central role of cracks in fracture mechanics was discussed. One of the universal features of such cracks from the standpoint of the theory of linear √ elasticity is the characteristic 1/ r signature of their stress ﬁelds. In the present section we wish to revisit these ﬁelds with an eye to examining how such ﬁelds may be deduced using arguments from dislocation theory. The approach adopted here will be to use the same superpositions of dislocations already discussed in the context of dislocation pile-ups. The fundamental argument is that by using the dislocation ﬁeld of a single dislocation as a fundamental solution (i.e. a Green function), the ﬁelds due to cracks may be constructed by superposition. Cracks as a Superposition of Dislocations. A scheme that will suit our aim of building a synthetic description of cracks and any allied dislocations is to think of a crack as an array of dislocations. Indeed, the majority of our work has already been done earlier in the context of our consideration of dislocation pile-ups in section 11.4.2. In fact, our present analysis will do little more than demonstrate that the solutions written down there are relevant in the crack context as well. The more fundamental signiﬁcance of the perspective to be offered here is that we will soon want to build up solutions in which cracks and dislocations are equal partners,

11.5 Cracks and Dislocations

611

and it will be seen that the dislocation ideas developed here provide a useful basis for doing so. One of the key points to be made in the present discussion is the substantiation of the claim that a continuous distribution of inﬁnitesimal dislocations can be assembled in a way that respects the traction-free boundary conditions associated with crack faces. In particular, we consider a crack which runs from −a to a, with a remotely applied stress of the form σx y = τ0 . In this mode II setting (see ﬁg. 11.16), we insist that on the crack faces σ yy = σx y = 0. Our claim is that such a crack can be represented by a distribution of inﬁnitesimal dislocations with a density of the form ρb (x) =

x 2(1 − ν)τ0 . √ 2 µb a − x2

(11.38)

This distribution is determined by insisting that the traction-free condition, a µ ρb (x )d x , (11.39) τ0 = − 2π(1 − ν) −a x − x be imposed along the crack, |x| < a. As pointed out by Weertman (1996), the solution to this problem is reached via recourse to a table of Hilbert transforms and is of the form reported in eqn (11.38). In light of this distribution, we may then write the stresses at an arbitrary point (x, y) as the superposition a tot ρb (x )σi(disl) (x − x , y)d x . (11.40) σi j (x, y) = j −a

We denote the stress ﬁeld due to a single Volterra dislocation at position (x , y ) by σi(disl) (x − x , y − y ). We also note that the original interpretation of the elastic j energy release rate offered in section 2.4.4 can be reinterpreted in terms of the driving forces on the various dislocations making up the crack. Now that we have seen how the crack itself may be written in terms of dislocations, we turn to the question of how to think about such a crack when there are other dislocations in its vicinity. 11.5.2 Dislocation Screening at a Crack Tip From the standpoint of the linear theory of elasticity, the problem of crack tip shielding may be seen as a question of solving the boundary value problem of a crack in the presence of a dislocation in its vicinity. As indicated schematically in ﬁg. 11.15, the perspective we will adopt here is that of the geometrically sterilized two-dimensional problem in which both the crack front and the dislocation line are inﬁnite in extent and perfectly straight. As we will see, even this case places mathematical demands of some sophistication. The basic question we

612

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.15. Conformal transformation from wedge + dislocation to the problem of a half-space containing dislocation (adapted from Ohr et al. (1985)).

pose concerns the nature of the stress ﬁelds in the neighborhood of the crack tip, in particular, as a result of the presence of the dislocation. From a physical perspective, what is found is that the presence of the dislocation inspires the introduction of a local stress intensity factor which may be thought of as an effective stress intensity and may be reduced relative to the bare stress intensity that would be present in the absence of the dislocation. In order to perform the mathematical manipulations that allow for the solution of this problem, we turn to the powerful tools of complex analysis. Of course, the moment we take such a step, it is clear that our methods will be impotent once we pose questions concerning more interesting three-dimensional geometries. We begin with a problem of antiplane shear in which the crack of interest has a mode III geometry, as indicated schematically in ﬁg. 11.16, and the associated dislocation is a screw dislocation. In this instance, the problem is that of ﬁnding a harmonic function u 3 (x, y) such that the relevant boundary conditions are satisﬁed. One particularly elegant scheme for solving this problem is the use of conformal mapping. Geometrically, the problem of wedge + dislocation shown in ﬁg. 11.15 is mapped onto a half-space with a subsurface dislocation, a problem we have already encountered in section 8.5.2, and which culminated in the introduction of an image dislocation. Through the device of determining a potential function that satisﬁes the free surface boundary conditions and subsequent inversion of the mapping so that we recover the original problem of a crack in the presence of a dislocation, the solution is rather immediate. To be concrete, we note that we seek a potential function η(z) such that u(z) = (2/µ) Im[η(z)]. Note that the factor of 2 here is consonant with the convention

11.5 Cracks and Dislocations

613

Fig. 11.16. Three independent modes of crack tip loading and associated dislocations (adapted from Ohr (1985)).

used in Ohr et al. (1985). Once this potential function is in hand, the corresponding stresses may be found using the isotropic linear elastic constitutive relation which in the case of antiplane shear reduces to σi j = 2µi j . In terms of the potential η(z), this may be rewritten as σ (z) = σ yz + iσx z = 2η (z).

(11.41)

In general, for complex geometries, direct determination of the function η(z) cannot be carried out simply. The trick with conformal mapping is to map the originally complex problem onto a simpler geometry for which the corresponding solution is known. In particular, if the mapping that effects this transformation is of the form w = g(z) and the potential for the transformed problem is χ (w), then the stresses for the original problem are obtained as dw . (11.42) dz Note that in this case, the function χ(w) is presumed to be known (usually by virtue of the symmetric geometry of the transformed problem), and dw/dz is a geometric derivative determined strictly by the transformation between the two geometries. For the case of interest here, namely, the ﬁelds that arise for a crack in the presence of a dislocation, the procedure described above is disarmingly simple. Through a suitable choice of transformation, the problem of a crack and dislocation can be mapped onto the problem of a single subsurface dislocation beneath a traction-free surface already solved by the method of images in section 8.5.2. σ (z) = 2χ (w)

614

11 Points, Lines and Walls: Defect Interactions and Material Response

Before writing down the solution we must ﬁrst broach the subject of the geometric transformation relating the wedge crack problem to the allied problem of a free surface. If we consider a wedge crack with opening angle α, all points on the line α π z = r ei(π− 2 ) must be mapped onto the line z = r ei 2 . The transformation that effects this mapping is w = z q , with q = π/(2π − α). Given the transformation, all that remains is to determine the potential χ(w) which characterizes the ﬁelds due to the subsurface dislocation and its image. This solution, which we state without derivation, is given by µb w−δ χ(w) = . (11.43) ln 4π w + δ¯ √ The dislocation of interest is at position δ in the w plane (i.e. δ = ξ , where ξ ¯ For is the dislocation position in the z plane) while its image is at position −δ. √ the special case of a sharp crack of interest here, w = z. If we now apply the prescription of eqn (11.42), we ﬁnd that the stresses are given by 1 1 µb . (11.44) σ (z) = √ √ √ −√ 4π z z− ξ z + ξ¯ The signiﬁcance of the result of eqn (11.44) is that it tells us how to account for the stresses in the context of problems in which a crack and a dislocation coexist. A particularly interesting feature of solutions like that given above is their interpretation as providing a source of screening for the crack tip. The use of the word screening in this context refers to the fact that the local stress intensity factor is modiﬁed by the presence of the dislocation and can result in a net reduction in the local stresses in the vicinity of the crack tip. In particular, the total stress intensity factor is a sum of the form K tot = K I I I + K disl ,

(11.45)

where K I I I is the stress intensity factor for the mode III crack in the presence of remote loading. If we imagine the special case in which the screw dislocation is on the prolongation of the crack plane at a distance d, then the contribution due to the dislocation to the stress intensity factor is given by µb . K disl = − √ 2πd

(11.46)

The key qualitative observation to be made is that the sign of K disl can be negative resulting in the local screening effect alluded to earlier. We note that while the analysis presented here centered on the mathematically simplest case of antiplane shear, there are analogous situations to be found for other modes of crack tip loading as seen in ﬁg. 11.16.

11.5 Cracks and Dislocations

615

Fig. 11.17. Competition at a crack tip between the emission of a dislocation and cleavage (adapted from Beltz et al. (1999)).

11.5.3 Dislocation Nucleation at a Crack Tip The solution constructed above provides the necessary tools from elasticity theory in order to consider nucleation of a dislocation at a crack tip. The philosophical perspective adopted here is that due to Rice (1992) in which a comparison is made between the work needed to create new free surface and that needed to create a slip distribution corresponding ultimately to a dislocation. We present this model not so much with the hope that it will deliver quantitative insights but on the grounds that it is highly instructive concerning the atomic-level processes near a crack tip. In particular, the model is appealing because the treatment of dissipative processes such as dislocation nucleation is endowed with atomic-level realism, while still maintaining an overall continuum description. For an atomically sharp crack subjected to remote mode I loading we may imagine a variety of irreversible mechanisms that might transpire once the load is sufﬁciently large. Two of these processes are the creation of new free surface (cleavage) and the nucleation of dislocations. We have already discovered that the energy release rate tied to the opening displacement discontinuities is that accounted for in the Grifﬁth model of the fracture toughness. Our present task is to ﬁnd the analogous description for dislocation nucleation and to do so, we follow the development of Rice. The basic idea is to express these two processes as a competition and to determine which one will commence at a lower stress level. This competition can be couched in terms of the energy release rates of the two competing processes as shown in ﬁg. 11.17. As noted in the ﬁgure, if the creation of new free surface can occur with a smaller energy release rate than the process of dislocation nucleation, it will be the winner in the competition. Alternatively, if the energy release rate to create a dislocation is the smaller of the two, it will be

616

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.18. Mode II crack with an incipient dislocation along prolongation of the crack plane (adapted from Rice and Beltz (1994)).

the process that transpires. As a result, the question becomes one of obtaining a measure of how much energy is fed to each of these processes during incremental crack extension, with G cleave and G disl being the relevant energy release rates for these two processes. Our preliminary analysis centers around the geometry shown in ﬁg. 11.18 in which an atomically sharp crack is subjected to mode II loading and the slip distribution is assumed to occur along the prolongation of the crack plane. Borrowing from the Peierls–Nabarro analysis described in section 8.6.2, it is assumed that the atomic-level forces across the slip plane may be characterized in terms of an interplanar potential φ(δ). This description asserts that the tractions which arise on account of the sliding discontinuity are given by τ = −∂φ/∂δ. The implementation of the Peierls–Nabarro analysis in the crack tip context is really quite similar to that advanced already in the analysis of dislocations (see section 8.6.2), with the added complication that the energy functional must now account not only for the energy on the slip plane and the interactions between dislocations, but also for the terms resulting from the presence of a crack tip. We begin by writing down an energy functional which features the as-yet undetermined slip distribution. The total energy of the system of crack with its attendant incipient dislocation is a sum of terms representing the energy cost for the slip, the energy associated with the elastic ﬁelds of the crack, and a part reﬂecting the energy associated with the crack interacting with the dislocations. In particular, we have ∞ ∞ KI I δ(r )dr φ[δ(r )]dr − E[δ(r )] = √ 2πr 0 0 ∞ ∞ ρ 1 dδ(ρ) µ δ(r )dr dρ. (11.47) + 4π(1 − ν) 0 r r − ρ dρ 0 Functional differentiation of this equation with respect to the slip distribution

11.5 Cracks and Dislocations

results in the equilibrium equation ∞ dφ µ ρ 1 dδ(ρ) KI I dρ = . − √ 2π(1 − ν) 0 r r − ρ dρ dδ 2πr

617

(11.48)

From a numerical perspective, the critical load for dislocation nucleation can be obtained by repeatedly solving this equation for increasing loads (as reﬂected in the value of K I I ) and seeking that load at which solutions fail to exist. An alternative appealing numerical approach is to map the continuous variational problem described above onto a corresponding discrete problem by parameterizing the solution in terms of a ﬁnite set of variational parameters (i.e. the Rayleigh–Ritz method) and solving the resulting coupled equations. This approach is described in Sch¨ock (1996). On the other hand, Rice has shown through an ingenious application of the J -integral how this problem may be solved analytically. The fundamental philosophy adopted in computing the energy spent in building up the incipient slip distribution is to use the J -integral, the path independence of which allows for a remote and near ﬁeld determination of the energy release rate. The far ﬁeld reckoning of this quantity is given in terms of Irwin’s stress intensity factor introduced in section 2.4.4. By way of contrast, the near ﬁeld evaluation of J reduces to an integral along the slip plane. In particular, we have ∞ − ∂(u + x − ux ) d x, (11.49) τ J =− ∂x 0 This integral may be rewritten as

δti p

J=

τ dδ,

(11.50)

0

which, because the shear stress is known in terms of the interplanar potential may = be directly evaluated yielding J = φ(δti p ). Thus, we have found that K Icrit I 2µφ(δti p )/(1 − ν). What we have learned is that dislocation nucleation will occur once φ(δti p ) reaches its maximum allowable value. This idea is depicted graphically in ﬁg. 11.19 where it is seen that instability to dislocation nucleation occurs when φ(δti p ) = γus , where γus is a material parameter that Rice has christened the unstable stacking energy. This idea is intriguing since it posits that the competition between cleavage and dislocation nucleation has been reduced to consideration of the relative values of two simple material parameters, both of which admit of ﬁrst-principles determination, and relevant geometrical factors. One of the problems with the analysis we have made thus far is its geometric simplicity. For the mode I case of primary interest here, the assumption that dislocations will be nucleated on the prolongation of the slip plane is overly

618

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.19. Potential energy for sliding adjacent crystal planes across one another (adapted from Rice (1992)).

severe. The type of geometry that is more appropriate in this setting is such that dislocations will be nucleated on slip planes that are at an angle θ with respect to the crack plane. In fact, to treat this problem with full generality, it is necessary to consider the role of oblique planes as possible contenders and will be considered further in section 12.6.3. As was hinted at in the previous section, the ease with which dislocations may be produced at a crack tip can clearly alter the mechanical response of a solid containing such a crack. In particular, for the special case of the clean geometry and samples that can be found in a material such as Si, the consideration of the cleavage–dislocation emission dichotomy may encompass all of the relevant mechanisms to attempt model building. As we have done so often before, we look to Ashby for a revealing systemization of the data around which the micromechanical study of fracture is built. In ﬁg. 11.20 a summary of the various fracture mechanisms is presented. One idea that emerges is that often at low temperatures, the sample undergoes virtually no plastic deformation before fracture, while at high temperatures, the material is seen to deform enormously. In addition, examination of the fracture surfaces reveals that different mechanisms are at play in the different results.

11.5 Cracks and Dislocations

619

Fig. 11.20. Schematic of a variety of different fracture mechanisms (adapted from Ashby et al. (1979)).

Despite the overwhelming complexity of real fractures processes, it is possible to discern dominant failure mechanisms under different conditions. However, we should bear in mind that in most instances many different processes transpire simultaneously. In ﬁg. 11.20, the different mechanisms are elucidated schematically. For high loads and low temperatures, we see that our intuition about failure by cleavage is correct, although the crack path can travel either along or through grains depending upon speciﬁc details of a given material. On the other hand, at higher temperatures, other mechanisms such as void nucleation and coalescence can assume a dominant role. The energy expended in such processes deﬁes description in simple Grifﬁth terms in which it is held that all of the elastic energy loss goes to the creation of new free surface. Those mechanisms involving appreciable plastic deformation require the expenditure of greater quantities of energy. This energy increase is revealed in the increased toughness of the material, with typical toughnesses far exceeding their Grifﬁth values. Fracture toughness data are shown in ﬁg. 11.21. The challenge grappled with in the current section

620

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.21. Schematic representation of data on fracture toughness of different materials (adapted from Ashby and Jones (1996)).

is that of explaining the dramatic increase in fracture toughness that can occur, sometimes after a temperature change of only a few degrees. The beginnings of an answer to that question can in some cases be tied to the type of analysis undertaken here, namely, to the energetics of dislocation nucleation at a crack tip.

11.6 Dislocations and Obstacles: Strengthening The fact that we refer to entire historic periods in terms of the names of certain metals is a powerful indirect testimony to the role played by chemical disorder in altering the mechanical properties of materials. Indeed, the appellation Bronze Age refers to precisely that moment in a civilization’s development when it was learned that the addition of tin to copper not only lowers the melting temperature of the resulting alloy relative to pure copper, but increases its strength as well. The goal of the present section is to set the stage for understanding why the addition of tin to copper can change its mechanical properties, and more generally, to recount the role of various strengthening mechanisms in the understanding of the mechanics of materials, and to seek the microscopic origins of hardening

11.6 Dislocations and Obstacles: Strengthening

621

phenomena in their roots in dislocation theory. After describing certain generic features of strengthening mechanisms related to the interactions of dislocations with obstacles, we will take up solution, precipitate and work hardening in turn. A visit to a steel mill results in the immediate recognition that there is more to a given steel than just iron and carbon. This is not accidental. Various chemical elements are introduced in a material with a wide variety of aims including the hardening effects to be considered here. Similarly, entire classes of Al alloys are described on the basis of the impurities that populate them. Beyond the capacity to raise the ﬂow stress by populating the material with either foreign atoms or particles, the stress to induce permanent deformation can be raised by working a material. The key point to be made is the recognition that what all of these hardening mechanisms reﬂect is the fact that some form of microstructural control has been exercised on the material. In that sense, the present section is a follow up on our earlier discussion of microstructure itself (see chap. 10) since we now attempt to explicate the ‘properties’ part of the structure–properties paradigm by tracing the inﬂuence of microstructure on dislocations. As an explicit reminder of the signiﬁcance of microstructural control in the context of strengthening, we recall ﬁg. 8.2 in which the variation in ﬂow stress with various microstructural parameters is shown. For example, ﬁg. 8.2(a) shows the way in which the ﬂow stress increases with the increasing concentration of foreign atoms. From a mechanistic perspective, what transpires in the context of all of these strengthening mechanisms when viewed from the microstructural level is the creation of obstacles to dislocation motion. These obstacles provide an additional resisting force above and beyond the intrinsic lattice friction (i.e. Peierls stress) and are revealed macroscopically through a larger ﬂow stress than would be observed in the absence of such mechanisms. Our aim in this section is to examine how such disorder offers obstacles to the motion of dislocations, to review the phenomenology of particular mechanisms, and then to uncover the ways in which they can be understood on the basis of dislocation theory. This program to understand hardening involves two distinct parts. First, we examine the interaction between a single dislocation and a localized elastic perturbation such as is offered either by an impurity atom or a foreign particle. This analysis demonstrates the force on a dislocation induced by such particles and hints at the possibility that a group of such impurities acting in concert could harden the material. Inspired by the insights gained by considering the role of a single obstacle to dislocation motion, the second part of our argument will be built around the statistical question of how to compute the average effects of a distribution of such obstacles. We begin with a conceptual overview of the hardening process as viewed from the dislocation perspective, followed by a systematic quantitative analysis of both the one-body interaction between a given dislocation and an associated

622

11 Points, Lines and Walls: Defect Interactions and Material Response

obstacle as well as the statistical question of how many such obstacles act in unison. We round out the discussion with an application of these ideas to three of the prominent hardening mechanisms, namely, solution, precipitate and work hardening.

11.6.1 Conceptual Overview of the Motion of Dislocations Through a Field of Obstacles As noted above, our working hypothesis concerning the various hardening mechanisms is that chemical impurities, second-phase particles and even other dislocations serve as obstacles to the motion of a given dislocation. As a result of the presence of these obstacles, the intrinsic lattice resistance τ p is supplemented by additional terms related to the various strengthening mechanisms. We further assume that the ﬂow stress can be written as τc = τ p + τ,

(11.51)

where τc signiﬁes the overall critical ﬂow stress, τ p is the intrinsic lattice friction (i.e. the Peierls stress) and τ is the change in the critical stress resulting from the presence of the obstacles. For simplicity, we will carry out our analysis in the limit in which τ p is negligible and hence use τc and τ interchangeably. As our ﬁrst step in the attempt to model the various strengthening mechanisms within crystals, we consider a problem in the abstract: what is the stress needed to induce glide of a dislocation through an array of obstacles? For the moment, we leave unspeciﬁed the particulars concerning the origins of such obstacles, since our present thinking will aid us in considering a variety of different speciﬁc mechanisms. A pictorial representation of the situation of interest is given in ﬁg. 11.22 in which the dislocation moves through an array of obstacles. As was already noted in chap. 8, much of the business of the metallurgical use of dislocation theory takes place at the level of the line tension approximation. To make our arguments deﬁnite, we consider the case in which the dislocation line tension is assumed to be orientation-independent. We next suppose that the dislocation, which is pinned at two points separated by the distance L, has bowed out under the action of an applied stress τ resulting in an equilibrium at the pinning point between the line tension and the pinning force F of the obstacle itself. As shown in the free-body diagram for the pinning point in ﬁg. 11.23, the equilibrium of the pinning point may be written as F = 2T cos

φ . 2

(11.52)

Recall from the discussion on line tension and dislocation bow-out given in

11.6 Dislocations and Obstacles: Strengthening

623

Fig. 11.22. Dislocation in a random array of obstacles (adapted from Foreman and Makin (1967)).

section 8.7.1, the radius of curvature is related to the applied stress and the line tension via T τb = . (11.53) R We recall the signiﬁcance of this result by noting that it tells us that in the isotropic line tension approximation, the segment bows out into a circular arc with the radius determined by a competition between the line tension and the applied stress. The next step in the general argument being set forth here is to unite eqns (11.52) and (11.53) in such a way that R and φ are replaced by the more metallurgically accessible parameter L which characterizes the mean spacing between obstacles. To do so, we note on the basis of ﬁg. 11.23 that R = L/[2 sin(θ/2)]. Hence, if we rewrite eqn (11.53) using the fact that T = F/[2 cos(φ/2)] and on the grounds that the angles θ and φ are related by sin(θ/2) = cos(φ/2), we ﬁnd the simple and central relation, F (11.54) τc b = . L This equation serves as the foundation of all that we will have to say about hardening. We begin by noting that the numerator is a reﬂection of the interaction between a single obstacle and a single dislocation. As a result, it is something that we can expect to understand on the basis of local calculations that concern themselves only with the properties of a single such interaction. By way of contrast, the denominator reﬂects the statistical properties related to the distribution of obstacles. As we will see below, there are a number of different ways of

624

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.23. Free-body diagram for the interaction of a dislocation and an obstacle characterized by a pinning force F.

constructing approximate models of the mean dislocation spacing, a fact which we signify by adopting the notation L eff which reminds us that the obstacles are distributed throughout the solid, and that to use an equation like eqn (11.54) to describe the yield properties of the solid as a whole (as opposed to describing the properties of a single segment of length L between two pinning points) we will have to determine L eff using some sort of statistical arguments. There are two scenarios which can develop in the context of the type of bow-out considered here. Either, the line tension forces become so large that they exceed the maximum resistance of the pinning point, or the pinning force is so strong that two adjacent bowed-out segments rejoin through a process known as Orowan looping. In the context of the former process, breakaway of the dislocation can be seen to occur when the applied stress reaches the critical value corresponding to the maximum resistance that can be offered by the obstacle, Fmax . Hence, eqn (11.54) may be rewritten in the form Fmax . (11.55) τc = bL eff By way of contrast, the resisting force offered by the obstacle at the moment of breakaway corresponding to the Orowan process is dictated by the equilibrium equation written above as eqn (11.52). In particular, since φ = 0 in this case, we have Fmax = 2T , and therefore the critical stress is τc =

2T . bL eff

(11.56)

11.6 Dislocations and Obstacles: Strengthening

625

The beauty of this result is that it requires no particular insight into the details of the pinning force, only requiring a bound on its net strength. We will see in our discussion of precipitate hardening that both bow-out scenarios are possible and result in different conclusions as to the way in which τ scales with the particle size and distribution. There are a number of different complaints that can be registered concerning our arguments. First, our results are cast in the abstract language of the modeler, without any reference to the more important microstructural parameters that are experimentally accessible. For example, we would clearly prefer a statement of the critical stress in terms of parameters such as the volume fraction of obstacles and their mean size. In addition, there is a distinctly approximate ﬂavor to our treatment of the distribution of obstacles which appears only through the parameter L eff . In coming sections, we will see just how far we might go in remedying these shortcomings. As yet, we have made no reference to the physical origins of the obstacle force Fmax . In the next section, we examine the way in which insights may be borrowed from the linear theory of elasticity in order to develop plausible models of these forces.

11.6.2 The Force Between Dislocations and Glide Obstacles Our current ambition is to elucidate one of the microscopic mechanisms that has been charged with giving rise to solution and precipitate hardening. The argument is that by virtue of the elastic ﬁelds induced by an obstacle there will be a force on a dislocation which the dislocation must overcome in its motion through the crystal. As a ﬁrst step towards modeling this phenomenon, we imagine the obstacle to be a spherical disturbance within the material. As was already demonstrated in chap. 7, such an obstacle produces spherically symmetric displacement ﬁelds of the form u r = Ar + b/r 2 . Once again invoking arguments about conﬁgurational forces, our expectation is that the force of interest is given by the derivative in the interaction energy as a function of some small excursion of the dislocation line. In generic terms, to ﬁnd the interaction energy we must evaluate the integrals 1 disl obs obs disl σ dV + σi j i j d V , (11.57) E int = 2 ij ij where the superscripts refer to the ﬁelds of the dislocation (disl) and obstacle (obs). This equation derives from the recognition that the total elastic energy is given by an integral 1 E tot = σ tot tot d V, (11.58) 2 ij ij

626

11 Points, Lines and Walls: Defect Interactions and Material Response

and the observation that by linearity, the total ﬁelds can be written as a superposition of the separate obstacle and dislocation ﬁelds. Furthermore, if we note that both the dislocation and obstacle stress ﬁelds are obtained using the same elastic modulus tensor, then eqn (11.57) collapses to disl σiobs (11.59) E int = j i j d V,

which will serve as the starting point for the remainder of our analysis. In principle, eqn (11.59) is all that we need to go about computing the interaction force between an obstacle and a dislocation. However, we will ﬁnd it convenient to rewrite this equation in a more transparent form for the present discussion. Using the principle of virtual work, we may rewrite the interaction energy as f obs · udisl d V. (11.60) E int =

Recall that the obstacle elastic ﬁelds may be arrived at by solving a boundary value problem in which three force dipoles are superposed as we did in chap. 7. In particular, we had

3 a a obs F δ x − x − ei − δ x − x + ei ei . (11.61) f (x) = 2 2 i=1 Substituting this expression into eqn (11.60), we are led to

3 a a F u idisl x + ei − u idisl x − ei . E int = 2 2 i=1

(11.62)

If we now go about expanding the displacement ﬁelds about the point x , then we are left with E int ≈ Fa∇ · udisl .

(11.63)

Recall from our review of continuum mechanics that the divergence of the displacement ﬁeld is a measure of the volume change associated with a given deformation. In this case, it is the volume change associated with the dislocation ﬁelds at the obstacle that gives rise to the interaction energy. At this level of description, only an edge dislocation will have any interaction with our spherical obstacle since tr( ) = 0 for a screw dislocation. On the other hand, for an edge dislocation we have ∇ · u = tr( ) = −

b 1 − 2ν sin θ . 2π 1 − ν r

(11.64)

With this result in hand, the interaction force between the dislocation and the

11.6 Dislocations and Obstacles: Strengthening

627

Fig. 11.24. Schematic of the geometry of interaction between a spherically symmetric obstacle and an edge dislocation.

obstacle may be computed by differentiating the interaction energy with respect to the coordinates of the dislocation. In particular, if we consider the case depicted schematically in ﬁg. 11.24, and interest ourselves only in the component of the force acting along the glide direction of the dislocation, we have Fx = −

x ∂ E int = −C 2 , ∂x (x + d 2 )2

(11.65)

where we have absorbed all of the material and geometric constants describing the dislocation and√obstacle themselves into the constant C. The maximum force occurs for x = d/ 3. To complete this model, we must return to an explicit reckoning of the quantity Fa which appears in the discussion above. In particular, recall that this product is the dipole moment associated with the obstacle and we wish to reconcile this quantity with the geometric features of the spherical inclusion such as its radius and the displacement at its surface. To do so, we recall from our earlier discussion that the displacement induced by such a collection of force dipoles is given by u(x) =

r Fa . 4π(λ + 2µ) r 3

(11.66)

Hence, if we insist that the displacement at the surface of this hole (i.e. for r = a0 /2) is δ, then we ﬁnd Fa = 4π δa02 (λ + 2µ).

(11.67)

If we rewrite λ + 2µ in terms of µ and ν and substitute the resulting expression

628

11 Points, Lines and Walls: Defect Interactions and Material Response

into our equation for the interaction force, we are left with E int = −4µδa02 bd

d , x2 + d2

(11.68)

and Fx = −8µδa02 bd

(x 2

x . + d 2 )2

(11.69)

As yet, our analysis has concerned itself with the total interaction force between the dislocation and the obstacle to its motion. However, a deeper understanding of the pinning process itself can be reached if we compute the force on the dislocation segment by segment. The geometry of interest is indicated in ﬁg. 11.24. We are now interested in obtaining the force on a segment at the point shown in the ﬁgure with coordinates (x, y, 0). The calculation amounts to nothing more than computing the Peach–Koehler force df = (σ b) × dl. The glide component of that bdl, where the stress ﬁeld is that due to the obstacle. force is given by −σxobstacle z Recall from our earlier discussion that the displacements for the obstacle (assumed spherically symmetric for the moment) are u r = δ(a0 /r )2 . Such displacements imply a strain x z = −

3δa02 xh 5

(x 2 + y 2 + h 2 ) 2

,

(11.70)

where the parameter h is the distance of the obstacle beneath the slip plane. As a result of this analysis, we ﬁnd that the localized force on the dislocation segment due to the obstacle is 6µbδa02 dh Fglide = . (11.71) 5 dl (d 2 + h 2 + y 2 ) 2 Although there are a number of interesting features of this analysis, it also leaves us with serious concerns about the formulation of an elastic theory of the obstacle forces that impede dislocation motion. In particular, this analysis suggests that for an obstacle on the slip plane itself, there is no interaction with the dislocation. Despite this elastic perspective, it seems certain that core effects will amend this conclusion.

11.6.3 The Question of Statistical Superposition In the previous subsection, we considered the emergence of the parameter F in eqn (11.54) on the basis of an elastic treatment of the interaction between a single dislocation and a single obstacle. In order to complete the analysis associated with eqn (11.54) we must now determine the parameter L eff which characterizes the distribution of obstacles. To do so, we will invoke statistical arguments of varying

11.6 Dislocations and Obstacles: Strengthening

629

Fig. 11.25. Schematic of the random forces exerted on a dislocation by virtue of the presence of point disorder such as is induced by foreign particles (adapted from Mott and Nabarro (1948)).

levels of sophistication. Our key approach will be that of localized point obstacles which Nabarro (1972) points out ‘provides an anchor in the sea of uncertainty.’ In light of our understanding of the interaction between a single localized obstacle and a dislocation, we next take up the question of how many such interactions conspire to yield observed hardening behavior. Again, we begin with a qualitative discussion aimed at examining some of the generic issues that must be addressed in tackling the question of statistical superposition of interest here. To that end, ﬁg. 11.25 shows a schematic from one of the famed early papers of hardening (Mott and Nabarro, 1948) in which an attempt was made to show the sort of random assemblage of forces that would act on a dislocation in the presence of a statistical distribution of obstacles. For our present purposes, what we wish to note is that unlike the ideal situation considered in our discussion of the Peierls stress which culminated in eqn (8.87), the intrinsic lattice friction must be supplemented by the statistical superposition of the random forces considered here. A more sophisticated consideration of the forces that are exerted upon a dislocation as it glides through a medium populated by a distribution of obstacles is depicted in ﬁg. 11.26. In this case, the fundamental idea that is being conveyed is to divide the character of various obstacles along the lines of whether or not they are localized or diffuse and whether or not they are ‘strong’ or ‘weak’. These different scenarios result in different scaling laws for the critical stress to induce dislocation motion.

630

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.26. Four distinct regimes suggested for the interactions between a dislocation and the disorder distributed throughout the body (adapted from Nabarro (1972)). The four regimes of interest are: (a) weak, localized obstacles, (b) strong, localized obstacles, (c) weak, diffuse obstacles and (d) strong, diffuse obstacles.

Periodic Array of Point Obstacles. The simplest picture that can be developed, and one for which our analysis leading up to eqn (11.54) is essentially exact, is one in which it is imagined that the obstacles are arranged periodically in the slip plane. One argument that we might set up to compute the areal density in terms of the known volume concentration c of obstacles, is to note that if we assign a slip plane of area A a volume Ab, then the number of obstacles found in that plane will be c Ab. We have used the discrete packing of atomic planes to obtain a volume per plane c Ab. As a result of this argument, we see that the areal density may be written either as c Ab/A or in terms of L eff as 1/L 2eff . What we have said is that the c Ab obstacles which ﬁnd themselves in the slip plane of interest are arranged on a square lattice with lattice parameter L eff . By equating our two expressions for the areal density, we are left with the relation 1 L eff = √ . bc

(11.72)

If we take the result given above and exploit it in the context of eqn (11.54) we obtain one of the crucial scaling relations for obstacle limited motion of dislocations, namely, √ (11.73) τc ∝ c.

11.6 Dislocations and Obstacles: Strengthening

631

Fig. 11.27. Schematic of two consecutive conﬁgurations in the unpinning history of a given dislocation.

This result is one which Kocks (1977) goes so far as to note already contains ‘the most important result of dislocation theory: namely, that the ﬂow stress is proportional to the square root of concentration’. Indeed, to the extent that we are interested in understanding the observed macroscopic plastic properties of materials, scaling relations involving the concentration of obstacles are pivotal. Random Array of Point Obstacles. At the next level of sophistication we imagine the opposite extreme in which the distribution of point obstacles is taken to be completely random. As was mentioned above, there are a variety of circumstances √ in which the τc ∝ c scaling is obtained, and we will see that in the present setting this same scaling is found. Our strategy is to compute the so-called Friedel length, which is a stress-dependent measure of the effective spacing between obstacles. In this case, the argument is altogether more subtle. The basic idea is to consider two consecutive pinned conﬁgurations such as are shown in ﬁg. 11.27. Physically, the idea is that as the stress increases, the number of pinning points that the dislocation joins up with will vary. As a result, even though the areal density of such pinning points is unchanged, the mean spacing between such pinning points along the dislocation (i.e. L eff ) will change. Our aim is to estimate L eff and in particular, its stress dependence. The key physical assumption made in the Friedel argument√is that once the dislocation becomes unpinned it will sweep an area l 2 = 1/ bc before encountering another pinning point. Comparison of the two conﬁgurations shown in ﬁg. 11.27 √ shows that in passing from the initial to the ﬁnal 2 conﬁguration, an area l = 1/ bc is swept out. To make these arguments concrete, we note that we are insisting that the area A swept out be given by the relation 2L eff L eff 1 A = = u 2 (x)d x − 2 u 1 (x)d x. (11.74) bc 0 0 We have introduced the function u 1 (x) to characterize the dislocation position

632

11 Points, Lines and Walls: Defect Interactions and Material Response

of the initial conﬁguration and u 2 (x) to characterize the dislocation of the ﬁnal conﬁguration. Note that the as-yet undetermined (and desired) parameter L eff appears in the limits of integration and will be determined in the end as a function of the concentration and the applied stress. In fact, to obtain the functions u 1 (x) and u 2 (x) we use what we already learned about dislocation bow-out in section 8.7.1. In particular, in the limit of weak driving force (which corresponds to the presumed weakness of the obstacles) generically, the dislocation proﬁle is of the form u(x) = −

τb 2 x + cx, T

(11.75)

where the constant c is determined by appealing to the boundary conditions. In the present case, we have u 1 (0) = u 1 (L eff ) = 0 and u 2 (0) = u 2 (2L eff ) = 0. Application of these boundary conditions results in the solutions τb (L eff x − x 2 ) 2T

(11.76)

τb x2 L eff x − . T 2

(11.77)

u 1 (x) = and u 2 (x) =

With these results in hand we may evaluate the integrals demanded in eqn (11.74) with the result that τ bL 3eff . (11.78) A = 2T Note that as a result of these arguments we may now determine L eff as L eff =

2T τ b2 c

13

.

(11.79)

This result is now in a form that may be fed back into eqn (11.55) with the result that 1 Fmax τc b2 c 3 , (11.80) τc = b 2T which may be solved for τc with the result that τc =

3 Fmax 2T b

12

1

c2.

(11.81)

We note that even in the context of this more roundabout description of the superposition of the effect of different obstacles, we once again recover the τc ∝ c1/2 scaling discussed earlier.

11.6 Dislocations and Obstacles: Strengthening

633

Continuously Distributed Disorder. Our treatment until this point has treated the disordering effect of the obstacles on the basis of a picture in which the homogeneous medium is punctuated by localized forces. An alternative viewpoint is one in which the disordering effect is imagined to be distributed continuously throughout the medium resulting in a local contribution to the resistance at every point on the dislocation. As a result of this picture, rather than attempting to assert equilibrium conditions only at pinning points, equilibrium is represented in integral form along the entire length of the dislocation. For the present purposes, the crucial conclusion of this analysis which we quote without derivation is the assertion that the critical stress to induce dislocation glide scales as τc ∝ c2/3 . Our reason for bringing this result up at all is mainly to serve as a point of comparison when we consider the actual data on solution hardening to be taken up in the next section.

11.6.4 Solution Hardening The use of impurities to alter the behavior of materials is a technique of great signiﬁcance, and solution hardening is but one of many ways in which this is carried out. Our intention in this section is to present a few experimental highlights which reveal the level of the quantitative understanding of solution hardening which will serve to catalyze the modeling discussion to follow. Having introduced the experimental backdrop, the remainder of our discussion will be ﬁxed on how well the ideas introduced in the previous few subsections rise to the challenge of the data. An example of the type of data associated with solution hardening it is the mission of our models to explain was shown in ﬁg. 8.2(a). For our present purposes, there are questions to be posed of both a qualitative and quantitative character. On the qualitative side, we would like to know how the presence of foreign atoms dissolved in the matrix can have the effect of strengthening a material. In particular, how can we reconcile what we know about point defects in solids with the elastic model of dislocation–obstacle interaction presented in section 11.6.2. From a more quantitative perspective, we are particularly interested in the question of to what extent the experimental data permit a scaling description of the hardening effect (i.e. τ ∝ cn ) and in addition, to what extent statistical superposition of the presumed elastic interactions between dislocations and impurities provides for such scaling laws. The metallurgical approach to coming to terms with data like that considered above is by virtue of an appeal to various parameters that signal the presence of foreign atoms and which can be used as the basis of contact with the elastic theory of interaction forces. Indeed, although results like that revealed in eqn (11.81) are extremely provocative, our work will only be done once plausible strategies are

634

11 Points, Lines and Walls: Defect Interactions and Material Response

found for linking quantities such as Fmax to underlying parameters of metallurgical signiﬁcance. In particular, two of the most immediate parameters that measure the extent to which a given set of foreign atoms will make their presence known to the dislocation elastically are the size misﬁt parameter deﬁned by δ=

1 da , a dc

(11.82)

η=

1 dµ . µ dc

(11.83)

and the modulus misﬁt parameter

The symbols introduced here include the lattice parameter a, the concentration c and the shear modulus µ. The purpose of these parameters is to provide a measure of the extent to which the presence of foreign atoms within the matrix will result in elastic interactions between these impurities and dislocations present in the material. My own take on these ideas is that they are largely inspired by the desire to make contact with the ideas on elastic ﬁelds of inclusions developed by Eshelby. We remind the reader that in that setting (see section 7.3.2), a foreign particle can make its presence known by virtue both of a difference in size and of a difference in moduli between the matrix and the particle. Of course, when speaking of a single foreign atom, these continuum notions become highly suspect. Nevertheless, what our elastic models have shown us is that if we are to install an inclusion within a continuum, the distinction between that particle and the surrounding matrix material can be introduced either by attributing a different size to that particle or by asserting that it is characterized by different moduli than that of the matrix material. The parameters δ and η introduced in eqns (11.82) and (11.83) measure the strength of these two effects. In addition to the two mechanisms introduced above, there are a variety of other mechanisms that have been invoked to explain the origins of solution hardening, including contributions due to the presence of stacking faults, the difference in valence of the matrix and solute and ordering effects. The key point to be taken away from this part of the discussion is the recognition that there are a wide variety of different ways in which we can construct elastic models of the interaction between foreign atoms and dislocations. We have seen that if we model a given foreign atom as a source of dilatation, a dislocation–obstacle interaction arises that depends upon the parameter δ. Similarly, if a given foreign atom is modeled as a source of elastic inhomogeneity (i.e. a region of different elastic constants than the matrix) then a dislocation–obstacle interaction arises that depends upon parameters like η introduced above. In addition to these models, it is also possible to imagine more sophisticated effects related to elastically induced redistribution

11.6 Dislocations and Obstacles: Strengthening

635

2 √ Fig. 11.28. Illustration of ﬁt to c and c 3 scaling to observations on solid solution hardening in Au–Al (adapted from Haasen (1979)).

of the foreign atoms around the dislocations. All of these models share the feature that they inhibit the motion of dislocations. Though the qualitative ideas introduced above are instructive, to really make contact with experiment we must calculate something. In particular, we need to ﬁnd a way to average over the types of disorder described schematically in ﬁg. 11.26 so as to obtain a concrete result for the scaling of the ﬂow stress with the concentration of foreign atoms, for example. Indeed, this is precisely what was done in various approximations in section 11.6.3. For the present purposes what we wish to really note about the outcome of the arguments given there is the emergence of two different scaling laws for how the critical stress scales with the concentration √ of impurities, namely, τc ∝ c and τc ∝ c2/3 . A provocative representation of experimental data on solution hardening is shown in ﬁg. 11.28. What we see on the basis of these data is that although clearly increasing the concentration increases the critical stress, identifying the particular scaling relation is a more challenging proposition. In addition to the attempt to link observed solution hardening with ideas on the scaling with concentration, efforts have been put forth on examining how the strengthening effect scales with the parameters δ and η. A particular example which reveals the magnitude of the hardening effect as a function of the size of the foreign atoms is shown in ﬁg. 11.29. The reader is encouraged to examine these issues in the article of Haasen (1979). A second facet to this discussion that we have omitted but which is immensely important is the temperature dependence of the ﬂow stress. As it stands, our discussion really only attempts to answer to the challenge of the zero-temperature contribution to the ﬂow stress.

636

11 Points, Lines and Walls: Defect Interactions and Material Response 20

c, MN m-2/at -%

16

Cu

Mn

12 Mg 8

4

Ag

Ge

Li Zn 0

10

20

30 40 50 * [( s- A)/ A] x 100

60

70

Fig. 11.29. Magnitude of solution hardening effect in Al alloys as a function of the size mismatch of the foreign atoms (adapted from Embury et al. (1989)).

11.6.5 Precipitate Hardening In the previous section, we saw that we can arrange that a particular material be endowed with a supersaturation of impurities by quenching some concentration of foreign atoms in the material beyond the solubility limit. On the other hand, the resulting microstructure is metastable. The equilibrium phase that is preferred in this part of the phase diagram is two-phase coexistence between the pure phase and a second phase, which is often an ordered alloy built up from the two components. For example, in the context of the Fe–C phase diagram, this coexistence is struck between α-Fe (bcc) and an orthorhombic phase of Fe3 C. From a modeling perspective for considering the mechanics of such two-phase microstructures, the simplest picture we might imagine is that the nuclei of these precipitates are spherical and that their radii increase with time. The presence of such second-phase particles makes itself known through a substantive change in the mechanical properties of the material, a speciﬁc example of which is shown in ﬁg. 8.2(b) Observations on precipitation hardening make it evident that in certain cases the key microstructural features in this context are the mean particle radius and the

11.6 Dislocations and Obstacles: Strengthening

637

Fig. 11.30. Illustration of the variation in ﬂow stress as a function of precipitate radius (adapted from Reppich (1993)).

volume fraction of such precipitates. In particular, the type of generic results that emerge are indicated schematically in ﬁg. 11.30 in which the variation in the ﬂow stress is shown as a function of particle size. Our present ambition is to explain this behavior on the basis of the type of simple models developed above. In simplest terms, the key feature of the ﬂow stress increment as a function of particle size is the fact that there is an ‘optimal’ particle size. What we will ﬁnd is that this maximum reﬂects a change in mechanism from particle cutting, which is dominant at small radii, to the Orowan process, which is easier at large particle radii. Our discussion in section 11.6.1 culminated in two possible outcomes to the encounter of a dislocation with an array of pinning points. On the one hand, we found that if the obstacles are sufﬁciently weak (characterized by a maximum force Fmax ), they will be breached at a critical stress of τc = Fmax /bL eff as shown in eqn (11.55). On the other hand, if the obstacles are strong enough, they will be traversed by an alternative mechanism in which the dislocations loop around the obstacle and rejoin on the opposite side, a mechanism known as Orowan looping and characterized by a strength τc = 2T /bL eff as shown in the derivation leading up to eqn (11.56). These two different eventualities are illustrated schematically in ﬁg. 11.31. We now undertake a systematic analysis of these two mechanisms, with special emphasis being placed on how to rewrite eqns (11.55) and (11.56) in terms of the metallurgical parameters relevant to two-phase microstructures.

638

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.31. Schematic of the Orowan looping and particle cutting mechanisms that arise from interaction of dislocations with foreign particles (adapted from Gerrold (1979)).

Particle Cutting For small radii, the mechanism of dislocation interaction with the foreign particles is that of particle cutting in which after a certain maximum force is reached, the dislocation shears the foreign particles themselves. As a result, in this context the relevant equation for the critical stress is eqn (11.55) and our charter is to reﬂect once again on Fmax and L eff from the perspective of the microstructure itself. Without entering into details, we note that L eff can be obtained using exactly the same arguments given in section 11.6.3 with the proviso that we replace bc with the areal density ρArea . If we carry out this substitution, eqn (11.55) may be rewritten as 3

2 Fmax √ ρArea . τc = √ b 2T

(11.84)

At this point our task is to relate the areal density ρArea to the volume fraction of second-phase particles, denoted by f , and to the particle radius R. To convert the result given above into these more usable terms, we make a highly simpliﬁed argument based on the following assumptions. (1) The particles are all of the same size and are characterized by a radius R. (2) The estimate of the mean particle spacing is determined by assuming full correlation between the particles positions. For simplicity, we imagine them arranged on a three-dimensional cubic

11.6 Dislocations and Obstacles: Strengthening

639

Fig. 11.32. Schematic of the geometry of the precipitate particles.

lattice. Note that despite the seeming artiﬁcial nature of these assumptions, in some cases the distribution of precipitates can indeed be highly regular. To determine the mean spacing between obstacles, we begin with the modeling assumption that any particle whose center lies within a distance R of the slip plane of interest is considered to provide a glide obstacle on that slip plane. Further, we assert that the volume fraction of such particles is given by the parameter f . The geometrical ideas are depicted in ﬁg. 11.32. The volume occupied by the precipitate particles in this slab of thickness 2R and area A is 2A f R. Hence the number of particles in this slab volume can be estimated by dividing the volume occupied by particles within the slab by the volume per particle, resulting in # particles in slab = 3A f /2π R 2 . This result may be used to compute the area per obstacle (Aobstacle ). Note that the area per obstacle is related to the areal density by ρArea = 1/Aobstacle . The area per obstacle is found by dividing the total area of the slip plane by the number of such particles and yields the estimate 3f . (11.85) 2π R 2 In light of these arguments, the critical stress for particle cutting is of the form 3/2 Fmax 3 f 1 τc = √ . (11.86) b 2T 2π R ρArea =

In order to complete the discussion, we must say something about how Fmax depends upon the mean particle radius. It is crucial to note that a wide variety of different Fmax s associated with particle cutting have been determined. For a broad discussion of this topic see section 2.3 of the article by Gerrold (1979) and

640

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.33. Schematic cross section of a precipitate particle as it is being cut by a gliding dislocation.

the discussion in section IV of the article by Embury et al. (1989). Rather than entering into the particulars of these different mechanisms, we note that much can be learned by examining the scaling of τc with f and R for different choices of Fmax . In particular, we note that if we make the assumption that Fmax s

Crystals, Defects and Microstructures Materials science has emerged as one of the central pillars of the modern physical sciences and engineering, and is now even beginning to claim a role in the biological sciences. A central tenet in the analysis of materials is the structure–property paradigm, which proposes a direct connection between the geometric structures within a material and its properties. The increasing power of high-speed computation has had a major impact on theoretical materials science and has permitted the systematic examination of this connection between structure and properties. In this textbook, Rob Phillips examines the various methods that have been used in the study of crystals, defects and microstructures and that have made such computations possible. The author presents many of the key general principles used in the modeling of materials, and punctuates the text with real case studies drawn from recent research. A second key theme is the presentation of recent efforts that have been developed to treat problems involving either multiple spatial or temporal scales simultaneously. This text is intended for graduate students and researchers in science and engineering with an interest in the theoretical constructs that have been devised to undertake the study of materials.

Crystals, Defects and Microstructures Modeling Across Scales ROB PHILLIPS Brown University, Providence RI

The Pitt Building, Trumpington Street, Cambridge, United Kingdom The Edinburgh Building, Cambridge CB2 2RU, UK 40 West 20th Street, New York, NY 10011-4211, USA 477 Williamstown Road, Port Melbourne, VIC 3207, Australia Ruiz de Alarcón 13, 28014 Madrid, Spain Dock House, The Waterfront, Cape Town 8001, South Africa http://www.cambridge.org © Robert B. Phillips 2004 First published in printed format 2001 ISBN 0-511-04108-X eBook (netLibrary) ISBN 0-521-79005-0 hardback ISBN 0-521-79357-2 paperback

Dedicated to Sonic’s accomplices

Contents

Preface Acknowledgements Notes on Units, Scales and Conventions

page xv xxi xxiv

Part one: Thinking About the Material World 1 1.1

1.2

1.3 2 2.1 2.2

2.3

2.4

1

Idealizing Material Response A Material World 1.1.1 Materials: A Databook Perspective 1.1.2 The Structure–Properties Paradigm 1.1.3 Controlling Structure: The World of Heat and Beat Modeling of Materials 1.2.1 The Case for Modeling 1.2.2 Modeling Deﬁned: Contrasting Perspectives 1.2.3 Case Studies in Modeling 1.2.4 Modeling and the Computer: Numerical Analysis vs Simulation Further Reading

3 3 3 8 12 14 14 15 18 25 26

Continuum Mechanics Revisited Continuum Mechanics as an Effective Theory Kinematics: The Geometry of Deformation 2.2.1 Deformation Mappings and Strain 2.2.2 Geometry of Rigid Deformation 2.2.3 Geometry of Slip and Twinning 2.2.4 Geometry of Structural Transformations Forces and Balance Laws 2.3.1 Forces Within Continua: Stress Tensors 2.3.2 Equations of Continuum Dynamics 2.3.3 Conﬁgurational Forces and the Dynamics of Defects Continuum Descriptions of Deformation and Failure 2.4.1 Constitutive Modeling

29 29 31 32 35 36 37 39 39 41 44 51 51

vii

viii

2.5

2.6 2.7 2.8 3 3.1 3.2

3.3

3.4 3.5

Contents

2.4.2 Linear Elastic Response of Materials 2.4.3 Plastic Response of Crystals and Polycrystals 2.4.4 Continuum Picture of Fracture Boundary Value Problems and Modeling 2.5.1 Principle of Minimum Potential Energy and Reciprocal Theorem 2.5.2 Elastic Green Function 2.5.3 Method of Eigenstrains 2.5.4 Numerical Solutions: Finite Element Method Difﬁculties with the Continuum Approach Further Reading Problems

51 54 60 64 64 66 69 72 75 76 78

Quantum and Statistical Mechanics Revisited Background Quantum Mechanics 3.2.1 Background and Formalism 3.2.2 Catalog of Important Solutions 3.2.3 Finite Elements and Schr¨odinger 3.2.4 Quantum Corrals: A Finite Element Analysis 3.2.5 Metals and the Electron Gas 3.2.6 Quantum Mechanics of Bonding Statistical Mechanics 3.3.1 Background 3.3.2 Entropy of Mixing 3.3.3 The Canonical Distribution 3.3.4 Information Theoretic Approach to Statistical Mechanics 3.3.5 Statistical Mechanics Models for Materials 3.3.6 Bounds and Inequalities: The Bogoliubov Inequality 3.3.7 Correlation Functions: The Kinematics of Order 3.3.8 Computational Statistical Mechanics Further Reading Problems

81 81 82 82 87 94 101 103 109 115 115 119 122 126 129 135 137 139 142 144

Part two: Energetics of Crystalline Solids

147

4 4.1 4.2

149 149 152 152

Energetic Description of Cohesion in Solids The Role of the Total Energy in Modeling Materials Conceptual Backdrop for Characterizing the Total Energy 4.2.1 Atomistic and Continuum Descriptions Contrasted

Contents

4.2.2

4.3

4.4

4.5

4.6

4.7 4.8 4.9 5 5.1 5.2

The Many-Particle Hamiltonian and Degree of Freedom Reduction Pair Potentials 4.3.1 Generic Pair Potentials 4.3.2 Free Electron Pair Potentials Potentials with Environmental and Angular Dependence 4.4.1 Diagnostics for Evaluating Potentials 4.4.2 Pair Functionals 4.4.3 Angular Forces: A First Look Tight-Binding Calculations of the Total Energy 4.5.1 The Tight-Binding Method 4.5.2 An Aside on Periodic Solids: k-space Methods 4.5.3 Real Space Tight-Binding Methods First-Principles Calculations of the Total Energy 4.6.1 Managing the Many-Particle Hamiltonian 4.6.2 Total Energies in the Local Density Approximation Choosing a Description of the Total Energy: Challenges and Conundrums Further Reading Problems

ix

154 156 156 158 164 164 165 172 176 176 184 189 197 198 200 203 204 206

5.5 5.6

Thermal and Elastic Properties of Crystals Thermal and Elastic Material Response Mechanics of the Harmonic Solid 5.2.1 Total Energy of the Thermally Fluctuating Solid 5.2.2 Atomic Motion and Normal Modes 5.2.3 Phonons 5.2.4 Buckminsterfullerene and Nanotubes: A Case Study in Vibration Thermodynamics of Solids 5.3.1 Harmonic Approximation 5.3.2 Beyond the Harmonic Approximation Modeling the Elastic Properties of Materials 5.4.1 Linear Elastic Moduli 5.4.2 Nonlinear Elastic Material Response: Cauchy–Born Elasticity Further Reading Problems

229 231 231 239 244 244 248 250 251

6 6.1 6.2

Structural Energies and Phase Diagrams Structures in Solids Atomic-Level Geometry in Materials

253 253 254

5.3

5.4

210 210 213 214 216 228

x

6.3

6.4

6.5

6.6 6.7 6.8

Contents

Structural energies of solids 6.3.1 Pair Potentials and Structural Stability 6.3.2 Structural Stability in Transition Metals 6.3.3 Structural Stability Reconsidered: The Case of Elemental Si Elemental Phase Diagrams 6.4.1 Free Energy of the Crystalline Solid 6.4.2 Free Energy of the Liquid 6.4.3 Putting It All Together 6.4.4 An Einstein Model for Structural Change 6.4.5 A Case Study in Elemental Mg Alloy Phase Diagrams 6.5.1 Constructing the Effective Energy: Cluster Expansions 6.5.2 Statistical Mechanics for the Effective Hamiltonian 6.5.3 The Effective Hamiltonian Revisited: Relaxations and Vibrations 6.5.4 The Alloy Free Energy 6.5.5 Case Study: Oxygen Ordering in High TC Superconductors Summary Further Reading Problems

Part three: Geometric Structures in Solids: Defects and Microstructures 7 7.1 7.2 7.3

7.4

7.5

Point Defects in Solids Point Defects and Material Response 7.1.1 Material Properties Related to Point Disorder Diffusion 7.2.1 Effective Theories of Diffusion Geometries and Energies of Point Defects 7.3.1 Crystallographic Preliminaries 7.3.2 A Continuum Perspective on Point Defects 7.3.3 Microscopic Theories of Point Defects 7.3.4 Point Defects in Si: A Case Study Point Defect Motions 7.4.1 Material Parameters for Mass Transport 7.4.2 Diffusion via Transition State Theory 7.4.3 Diffusion via Molecular Dynamics 7.4.4 A Case Study in Diffusion: Interstitials in Si Defect Clustering

260 261 264 265 268 268 275 277 278 280 282 283 291 297 299 300 304 304 305

309 311 311 312 318 318 326 327 328 332 341 344 345 346 351 353 356

Contents

xi

7.6 7.7

Further Reading Problems

356 359

8 8.1

Line Defects in Solids Permanent Deformation of Materials 8.1.1 Yield and Hardening 8.1.2 Structural Consequences of Plastic Deformation 8.1.3 Single Crystal Slip and the Schmid Law The Ideal Strength Concept and the Need for Dislocations Geometry of Slip 8.3.1 Topological Signature of Dislocations 8.3.2 Crystallography of Slip Elastic Models of Single Dislocations 8.4.1 The Screw Dislocation 8.4.2 The Volterra Formula 8.4.3 The Edge Dislocation 8.4.4 Mixed Dislocations Interaction Energies and Forces 8.5.1 The Peach–Koehler Formula 8.5.2 Interactions and Images: Peach–Koehler Applied 8.5.3 The Line Tension Approximation Modeling the Dislocation Core: Beyond Linearity 8.6.1 Dislocation Dissociation 8.6.2 The Peierls–Nabarro Model 8.6.3 Structural Details of the Dislocation Core Three-Dimensional Dislocation Conﬁgurations 8.7.1 Dislocation Bow-Out 8.7.2 Kinks and Jogs 8.7.3 Cross Slip 8.7.4 Dislocation Sources 8.7.5 Dislocation Junctions Further Reading Problems

362 362 363 365 367 369 371 372 375 382 382 388 391 392 393 395 398 402 404 404 406 412 415 416 418 423 426 430 435 437

Wall Defects in Solids Interfaces in Materials 9.1.1 Interfacial Conﬁnement Free Surfaces 9.2.1 Crystallography and Energetics of Ideal Surfaces 9.2.2 Reconstruction at Surfaces 9.2.3 Steps on Surfaces

441 441 442 446 447 452 474

8.2 8.3

8.4

8.5

8.6

8.7

8.8 8.9 9 9.1 9.2

xii

9.3

9.4

9.5 9.6 9.7 9.8

Contents

Stacking Faults and Twins 9.3.1 Structure and Energetics of Stacking Faults 9.3.2 Planar Faults and Phase Diagrams Grain Boundaries 9.4.1 Bicrystal Geometry 9.4.2 Grain Boundaries in Polycrystals 9.4.3 Energetic Description of Grain Boundaries 9.4.4 Triple Junctions of Grain Boundaries Diffuse Interfaces Modeling Interfaces: A Retrospective Further Reading Problems

476 477 484 487 489 492 494 500 501 502 503 505

10 Microstructure and its Evolution 10.1 Microstructures in Materials 10.1.1 Microstructural Taxonomy 10.1.2 Microstructural Change 10.1.3 Models of Microstructure and its Evolution 10.2 Inclusions as Microstructure 10.2.1 Eshelby and the Elastic Inclusion 10.2.2 The Question of Equilibrium Shapes 10.2.3 Precipitate Morphologies and Interfacial Energy 10.2.4 Equilibrium Shapes: Elastic and Interfacial Energy 10.2.5 A Case Study in Inclusions: Precipitate Nucleation 10.2.6 Temporal Evolution of Two-Phase Microstructures 10.3 Microstructure in Martensites 10.3.1 The Experimental Situation 10.3.2 Geometrical and Energetic Preliminaries 10.3.3 Twinning and Compatibility 10.3.4 Fine-Phase Microstructures and Attainment 10.3.5 The Austenite–Martensite Free Energy Reconsidered 10.4 Microstructural Evolution in Polycrystals 10.4.1 Phenomenology of Grain Growth 10.4.2 Modeling Grain Growth 10.5 Microstructure and Materials 10.6 Further Reading 10.7 Problems

507 508 508 516 519 520 520 527 528 529 537 540 546 547 551 554 560 565 566 567 568 580 580 582

Part four: Facing the Multiscale Challenge of Real Material Behavior

585

Contents

11 Points, Lines and Walls: Defect Interactions and Material Response 11.1 Defect Interactions and the Complexity of Real Material Behavior 11.2 Diffusion at Extended Defects 11.2.1 Background on Short-Circuit Diffusion 11.2.2 Diffusion at Surfaces 11.3 Mass Transport Assisted Deformation 11.3.1 Phenomenology of Creep 11.3.2 Nabarro–Herring and Coble Creep 11.4 Dislocations and Interfaces 11.4.1 Dislocation Models of Grain Boundaries 11.4.2 Dislocation Pile-Ups and Slip Transmission 11.5 Cracks and Dislocations 11.5.1 Variation on a Theme of Irwin 11.5.2 Dislocation Screening at a Crack Tip 11.5.3 Dislocation Nucleation at a Crack Tip 11.6 Dislocations and Obstacles: Strengthening 11.6.1 Conceptual Overview of the Motion of Dislocations Through a Field of Obstacles 11.6.2 The Force Between Dislocations and Glide Obstacles 11.6.3 The Question of Statistical Superposition 11.6.4 Solution Hardening 11.6.5 Precipitate Hardening 11.6.6 Dislocation–Dislocation Interactions and Work Hardening 11.7 Further Reading 11.8 Problems 12 Bridging Scales: Effective Theory Construction 12.1 Problems Involving Multiple Length and Time Scales 12.1.1 Problems with Multiple Temporal Scales: The Example of Diffusion 12.1.2 Problems with Multiple Spatial Scales: The Example of Plasticity 12.1.3 Generalities on Modeling Problems Involving Multiple Scales 12.2 Historic Examples of Multiscale Modeling 12.3 Effective Theory Construction 12.3.1 Degree of Freedom Selection: State Variables, Order Parameters and Conﬁgurational Coordinates 12.3.2 Dynamical Evolution of Relevant Variables: Gradient Flow Dynamics and Variational Principles 12.3.3 Inhomogeneous Systems and the Role of Locality

xiii

587 587 588 588 589 592 593 595 599 600 604 609 610 611 615 620 622 625 628 633 636 642 644 647 649 651 652 653 655 658 668 669 674 685

xiv

12.4

12.5

12.6

12.7 12.8

Contents

12.3.4 Models with Internal Structure 12.3.5 Effective Hamiltonians Bridging Scales in Microstructural Evolution 12.4.1 Hierarchical Treatment of Diffusive Processes 12.4.2 From Surface Diffusion to Film Growth 12.4.3 Solidiﬁcation Microstructures 12.4.4 Two-Phase Microstructures Revisited 12.4.5 A Retrospective on Modeling Microstructural Evolution Bridging Scales in Plasticity 12.5.1 Mesoscopic Dislocation Dynamics 12.5.2 A Case Study in Dislocations and Plasticity: Nanoindentation 12.5.3 A Retrospective on Modeling Plasticity Using Dislocation Dynamics Bridging Scales in Fracture 12.6.1 Atomic-Level Bond Breaking 12.6.2 Cohesive Surface Models 12.6.3 Cohesive Surface Description of Crack Tip Dislocation Nucleation Further Reading Problems

688 697 701 701 709 711 715 718 719 720 728 731 732 732 734 735 736 738

13 Universality and Speciﬁcity in Materials 13.1 Materials Observed 13.1.1 What is a Material: Another Look 13.1.2 Structural Observations 13.1.3 Concluding Observations on the Observations 13.2 How Far Have We Come? 13.2.1 Universality in Materials 13.2.2 Speciﬁcity in Materials 13.2.3 The Program Criticized 13.3 Intriguing Open Questions 13.4 In Which the Author Takes His Leave

742 743 743 744 746 748 749 750 751 752 754

References Index

757 771

Preface

Materials science as a formal discipline has quietly emerged as one of the central pillars of the physical sciences. Whether one interests oneself in the creation of lighter, more durable surfboards, or in the invention of new technologies to free up the trafﬁc jam on the world wide web, in the end, these questions will always imply demands which must be met by new classes of materials. Though the study of materials is largely rooted in the enlightened empiricism of traditional metallurgy, the advent of high-speed computers and the emergence of robust quantum simulations suggests new engineering strategies in which mechanism-based understanding might be hoped to lead to new materials. As a result of the maturation of theoretical materials science, it has become increasingly possible to identify a corpus of central results which serve as the basis for the analysis of materials. In addition, increasingly complex materials with structures at many different scales have led to the emergence of methods built around the explicit consideration of multiple scales simultaneously. As a result of these advances, this book attempts to take stock of the present capacity for modeling materials, with the word modeling used in the broadest sense. The book is divided into four basic parts. It opens with an overview of some of the key issues concerning materials that one might hope to succeed in modeling. Special reference is made to the notion of material parameters as characterized by the broad variety of data about materials that may be found in any databook. Though my comments on material response will be rather generic, my efforts to model such response will be restricted almost exclusively to crystalline solids. Though I am ashamed to have ignored so many classes of important and interesting materials, in the end, even restricting myself to crystalline materials left me with a project that exceeds my competence. After the introduction to material response, I present something like a modelers toolkit with a review of the key ideas from continuum mechanics, quantum mechanics and statistical mechanics that one might want to bring to the evaluation of a particular problem in the mechanics of materials. My argument here is that these three broad ﬁelds of study serve as the cornerstone for the rest of what we will do. The second main section of the xv

xvi

Preface

book is entitled ‘Energetics of Crystalline Solids’ and aims to describe the various tools that may be brought to bear on the problem of understanding the properties of perfect crystals. The argument made here is that the understanding we will require later concerning the role of defects in materials will have more impact when measured against the backdrop of the perfect solid. Particular emphasis in chaps. 4–6 is placed on computing the total energies of a given solid and using these energies to deduce the thermal and elastic properties of solids and the structural stability of different materials as revealed by phase diagrams. It should be noted that though I have restricted my attention to crystalline solids, much of what we will say in these chapters can be borrowed without alteration in the context of noncrystalline solids (and even liquids). Part 3, ‘Geometric Structures in Solids: Defects and Microstructures’ is organized according to the dimensionality of the various defects that populate materials and considers point defects (chap. 7), line defects (chap. 8) and interfacial defects (chap. 9). The organization of the material along dimensional lines is in the end somewhat artiﬁcial, but provides an organizational thread which has been useful to me if not the reader. Once an understanding of these various defects is in hand, I make an attempt at describing the assembly of these defects into a material’s microstructure (chap. 10). The ﬁnal part of the book, ‘Facing the Multiscale Challenge of Real Material Behavior’, should be seen as the culmination of the efforts set forth in the preceding chapters with the aim being to see just how far the modeler can go in the attempt to concretely consider material behavior. In addition, I have had a go at trying to seek the generic features of those models in which a deliberate attempt has been made to eliminate degrees of freedom. Indeed, my contention is that the enormous current interest in ‘multiscale modeling’ is born in large part of a self-conscious attempt to construct theories in a way that will lend them computational efﬁciency. Though there has been an incontrovertible increase in computational power, it has carried with it an attendant perception that almost always our appetite will outstrip our abilities. As a result, modelers throughout the physical sciences have had to seek to reformulate existing theories and to create new ones in a way that is ever mindful of the need to reduce computational burden. My reasons for writing this book are primarily selﬁsh. I have found that the only way I can really learn something is by self-study, and in particular, by seeking understanding at the level of the details – factors of 2 and π included. I consider myself one of the lucky few, namely, those who are able to earn a living as a college professor. Indeed, my privileges are greater yet. Almost daily I count my good fortune for having landed in the Solid Mechanics group at Brown University. One of the challenges in entering such a group has been to grope my way to some modicum of understanding in the area of the mechanics of materials. This book represents one part of that groping and reﬂects my own sense of some of the key

Preface

xvii

strategies that may be brought to bear on modeling material behavior. As part of the process of bringing myself up to speed for attempting to write this book, I have also undertaken the writing of a number of review articles with which the perceptive reader will undoubtedly see some overlap. This process was intentional in the hope that by working with various coauthors a useful vision of much of the material included here could be built up. Similarly, many of the ideas set forth here have been tested out in courses given at Brown, Caltech, the National University of Singapore and the Institut National Polytechnique de Grenoble. My intention in writing this book has not been to produce an encyclopedic compendium of all that is known concerning the modeling of materials and their properties. Rather, I have attempted to consider a sufﬁciently diverse set of problems to reveal the habit of mind that can be brought to the study of materials. Indeed, the book is largely anecdotal, with what I perceive to be fundamental ideas punctuated by more speculative ‘case studies’ that may not stand the test of time. As a result, the book has mixed character, alternating back and forth between text and monograph mode. In his outstanding book The Gift of Fire, Richard Mitchell notes the distinction between knowing and knowing about. The aims of the present work move back and forth between these objectives, with my hope being that after reading those sections having to do with general principles (and working the corresponding problems), the reader will ‘know’ these ideas. By way of contrast, the case studies are put forth more in the spirit of ‘knowing about’ with the hope that such studies will familiarize the reader with the implementation of the general ideas as well as the attendant literature, and will embolden him or her to set out to carry through a detailed case study themselves. I should also note that although many a preface emboldens the reader with the claim that various chapters can be read independently, I have written the present work very much as narrative, with the same idea presented in a different light several (or even many) different times, each contrasted with the other. For example, the discussion on Bridging Scales in Microstructural Evolution in chap. 12 presupposes a knowledge of what has gone before in chap. 10. Though it is true that one can read one without the other, it is certain that the message I wish to convey about microstructure and its evolution can only be gleaned by reading them both. For me, the book was written as a single entity and its logic is intertwined accordingly. In keeping with this general philosophy, the book is populated by a minimum of numerical tables in which speciﬁc data are presented. Rather, I have opted for pictorial and graphical representation of numerical results with the aim being the presentation of trends rather than detailed quantitative insights. On the other hand, there are a number of instances in which I present tables of data, but in the more sympathetic form of pictures. The calculations of the group of Skriver come to mind in this regard since they have done the service of providing the energies of

xviii

Preface

a number of defects (vacancies – ﬁg. 7.15, surfaces – ﬁg. 9.5 and step energies – ﬁg. 9.29) for a whole host of different materials, using the same theoretical analysis in each instance raising the possibility of a meaningful assessment of the trends. In addition, at times I have resorted to presenting collages of experimental data since I often feel it is beyond my competence to bring expert judgement to one experiment vs another and thus leave it to the reader to explore several sources and thereby decide for his or herself. My selection of material is also based in part upon a sinking feeling I sometimes get both while attending meetings and while cranking out the next calculation at my desk: it seems that so much of ‘research’ (mine included) is slated for obsolescence from the moment of its inception. It has always seemed to me that pedagogy is an ideal litmus test of signiﬁcance. Is a particular piece of work something that I would want to tell my students? The difﬁculty in answering this question is further exacerbated by the pedagogical uncertainties that attend the increasing reliance on numerical solutions and computer simulation. How exactly are we to communicate what is being learned from computational approaches? I have tried to follow a basic formula in many of the later chapters in the book. An attempt is ﬁrst made to illustrate the fundamental principles involved in contemplating a given class of material properties. These generic ideas, which are assumed to be largely uncontroversial, are then illustrated in an iterative fashion with a given case study examined from as many different angles as possible. For example, in discussing structural stability of Si, I make a point of showing how these questions can be addressed both from the perspective of empirical potentials and using ﬁrst-principles quantum mechanical treatments. Similarly, in my treatment of grain growth, I show how the Potts model, phase ﬁeld models and sharp interface models may all be used to examine the same basic process. My logic in these instances is to encourage a breadth of perspective ﬁltered by a critical eye that sees the shortcomings of all of these approaches. In the end, this book reﬂects my quest to unearth some of the exciting developments in the modeling of thermomechanical properties which have the power to either instruct or predict or entertain. In addition to commenting on what is in this book, it is with a trace of sadness that I also note what is not. With the narrowing of time between a given day of writing and the date of my self-imposed deadline, as well as with the increasingly swollen zip disks and hard copies of my book, it became increasingly clear that I must abandon many of my original intentions and resort to wholesale slashing. It is with particular regret that I eliminated my discussions of thermal conductivity, electromigration, the use of path integral methods to study diffusion and the electronic structure of quantum dots. In the end, I came to the view that I must stop and return to more active daily participation in family, sleep and my own research. I should also note that despite its length, in the end experts will recognize that my

Preface

xix

book has provided only a caricature of their ﬁelds. My aim was to highlight what seemed to me to be either the most general ideas or the most intriguing from each broad area. A word of explanation concerning references and further reading is in order. Ultimately, I decided to reference the works of others in only two ways. First, the Further Reading sections at the end of each chapter make reference only to those books or articles that form a part of my working and thinking vocabulary. Each time reference is made to one of these works, I attempt to provide some editorial comment as to why it has appeared on my list. My taste is idiosyncratic: if given the choice, I will always seek out that author who tells me something other than the party line, who has forged his or her own vision. I hold to this same mean in graduate teaching with the conviction that students are not interested in a watered down regurgitation of what they can read in the textbook – a unique perspective is what interests me. In addition to the suggestions for further reading, I have also compiled a single bibliography at the end of the book. This list serves an entirely different purpose and there is only a single way to get on it. These books and articles are those from which I have borrowed ﬁgures, followed derivations or turned the analysis into a ‘case study’. One of my abiding aims has been to try to ﬁgure out which part of the work on modeling has earned some level of permanence. Certain models (for example the quantum corral discussed in chap. 2) are pedagogically satisfying and at the same time permit immediate comparison with experiment. This is the ideal situation and, wherever possible, I have attempted to include them. In addition, I have also sought those steps forward that illustrate a certain approach that, in my opinion, should be imitated. As is evident from the preceding paragraphs, my bibliographic acumen is severely limited. The reference list is not encyclopedic and reﬂects my taste for browsing the index in a few favorite journals such as Physical Review B and Physical Review Letters, Journal of Mechanics and Physics of Solids, Metallurgical Transactions A, Philosophical Magazine and Acta Metallurgica. I am a particular fan of the ‘Overview’ sections in Acta Metallurgica and the articles written by award recipients in Metallurgical Transactions. Further, my choice of references is biased in favor of friends and acquaintances, due largely to the fact that in these instances I have had the beneﬁt of private discussions in order to learn what really happened. This is especially true in those cases where I sought a picture to illustrate a concept such as, for example, a polycrystalline microstructure. In these cases, it was most convenient to tap acquaintances, resulting in an over representation of work carried out at Brown. Hence, while my choice of references should be seen as something of an endorsement for those that are here, it should not be seen as a rejection of those that are not.

xx

Preface

Another feature of the book deserving of comment is the problem sets that are to be found at the end of each chapter. Many of these problems have already had a tour of duty in the various courses that I have taught at Brown and Caltech. On the other hand, there is a reasonable fraction of these problems that have not seen the light of day before now and thus risk having bugs of various types. The problems come in all types ranging from the ﬂeshing out of material covered in the chapters themselves to the construction of full-ﬂedged computational solutions to problems that are otherwise not tractable. A few stylistic comments are also in order. For the most part, I have written the book in the ﬁrst person plural, making constant reference to ‘we’ this and ‘we’ that. My reason for selecting this language is an honest reﬂection of my presumed relation with the reader – I imagine us both, you the reader and me, side by side and examining each question as it arises, almost always in a questioning tone: can we do better? I have reserved the more personal and subjective ‘I’ for those places where it is really my opinion that is being espoused as, for example, in the sections on Further Reading. In addition, the book is written in an informal (and at times light) style with various asides and observations. I fear that I will probably be charged with both ﬂippancy and arrogance, but wish to note at the outset that my hope was to produce a book that was to some extent fun to read. But even more importantly, I have tried to have fun in its writing. Three hours a morning for four years is a lot of hours to sit by oneself and I confess that on many occasions I could not resist certain turns of phrase or observations that amused me. Rob Phillips Barrington RI 2000

Acknowledgements

As a voracious reader myself, I am a veteran of many a preface and its attendant list of acknowledgements. What I realize now that it is my turn to make such a list is that for one such as me, who owes so much to so many, acknowledgements are deeply felt and yet are probably irrelevant to the anonymous reader. As said above, I wrote this book largely for myself in the hope that I would learn something in the act of so doing. This learning can be divided along two main lines, one emanating from the isolated groping I did at my desk, and the other from the pleasant meaningful interactions I have had with the people it is the business of this section to acknowledge. These paragraphs are for me and my family, my friends and my teachers. To all of you who have taught, tolerated, scolded, encouraged, discouraged, challenged and befriended me, let me state it simply: thank you for enriching my life. I now see the dangers inherent in making a list of names, but have decided to risk it on the grounds that I wish to express my indebtedness to some people publicly. I am grateful to William Martin and Andrew Galambos who literally opened up a new world of scientiﬁc thinking to my teenage mind, and life has never been the same. I am also grateful to Solomon Deressa, Chuck Campbell and Anders Carlsson, all of whom gave me a chance when I probably didn’t deserve one, and from whom, I have learned much. It is a pleasure to acknowledge my various friends at Brown from whom I have taken the vast majority of the courses offered in our Solid Mechanics curriculum (B. Freund – Stress Waves, Thin Films; R. Clifton – Advanced Continuum Mechanics; K.-S. Kim – Foundations of Continuum Mechanics; A. Bower – Plasticity; F. Shih – Finite Element Method; C. Briant – Mechanical Properties of Materials; and Mig Ortiz who taught Dislocations in Solids and much else through private consultation). Indeed, the inimitable Professor Ortiz has been the kind of friend and collaborator that one is lucky to ﬁnd even once. My good fortune at Brown has also been built around the chance to learn from a series of outstanding graduate students and postdocs. Ellad Tadmor, Ron Miller, Vijay Shenoy, David Rodney and Harley Johnson all were a key part of my ﬁrst ﬁve years at Brown and I can only hope they learned a fraction as much xxi

xxii

Acknowledgements

from me as I did from them. More recently, I have beneﬁted enormously from my interactions with Nitin Bhate, Dan Pawaskar, Kedar Hardikar and David Olmsted. As I said above, much of the fun in writing this book came from the interactions I had with others. I must single out Kaushik Bhattacharya, Rick James, Art Voter, Mig Ortiz, Chris Wolverton, Vivek Shenoy and Mark Asta, all of whom need special acknowledgement for running a veritable intellectual babysitting operation. I have also beneﬁted from expert advice on a number of different chapters from Janet Blume, Jane Kondev, Craig Black, Saryn Goldberg, Deepa Bhate, Anders Carlsson, K.-J. Cho, John Jameson, Tim Kaxiras, Stephen Foiles, Fabrizio Cleri, Mark Asta, Chris Wolverton, Art Voter, Luciano Colombo, Ladislas Kubin, Lyle Roelofs, Lloyd Whitman, Clyde Briant, Ben Freund, Dan Pawaskar, Karsten Jacobsen, Perry Leo, Kaushik Bhattacharya, Rick James, Simon Gill, Kevin Hane, T. Abinandanan, Peter Gumbsch, Long-Qing Chen, Georges Saada, Peter Voorhees, Alan Ardell, Emily Carter, Alan Needleman, Sam Andrews, Didier de Fontaine, Jakob Schiotz, Craig Carter, Jim Warren, Humphrey Maris, Zhigang Suo, Alan Cocks, Gilles Canova, Fred Kocks, Jim Sethna, Walt Drugan, Mike Marder, Bob Kohn, and Bill Nix and Mike Ashby indirectly as a result of a series of bootlegged course notes from excellent courses they have given. My book has also been read cover to cover by a number of hearty souls (Ron Miller, David Rodney, David Olmsted, Rob Rudd, Nitin Bhate, Walt Drugan and Bill Curtin) who made immensely useful suggestions that took my manuscript from an infantile performance to something that might be considered presentable. Of course, any errors that remain are strictly my own responsibility and indeed, at several junctures throughout the text, my arguments are suspect. It is also my great pleasure to thank Maryam Saleh who literally sketched, traced, drew and redrew over 300 ﬁgures, and Lorayn Palumbo who took care of everything from making sure I didn’t forget to teach my class to taking care of all manner of miscellaneous tasks. I am happy to extend my warmest thanks also to Amy Phillips who submitted literally hundreds of requests for permission to reprint ﬁgures. I would also like to thank Florence Padgett from Cambridge University Press who has supported me through the various stages of frustration that attended the writing of this book and, similarly, Simon Capelin. I would also like to acknowledge the outstanding editorial efforts of Maureen Storey who suggested all manner of improvements. The opportunity to write this book was supported generously through my wonderful NSF Career Award. As will be evident to any reader of my book, I have tried to present as many of my conclusions as possible in pictorial form. The task of amassing the various ﬁgures that form the backbone of this work was lightened enormously by the generous help of many friends, namely, Sharvan Kumar, Mike Mills, Peter Voorhees, Dan Fridline, Allan Bower, Alan Schwartzman, Harley Johnson,

Acknowledgements

xxiii

Karsten Jacobsen, Jakob Schiøtz, Rolf Heid, Rajiv Kalia, Sanjay Kodiyalam, Rick James, Kedar Hardikar, Dan Pawaskar, Charles McMahon, Vasily Bulatov, David Vanderbilt, Ralf Mueller, Lindsey Munro, Luciano Colombo, Tomas de la Rubia, George Gilmer, Christophe Coupeau, Marc Legros, Kevin Hemker, Sean Ling, Ian Robertson, Torben Rasmussen, Nasr Ghoniem, Klaus Schwarz, Marc Fivel, Bill Gerberich, David Rodney, Vivek Shenoy, Hans Skriver, Lloyd Whitman, Furio Ercolessi, Martin Bazant, Dieter Wolf, David Seidman, Craig Carter, Eric Chason, Stuart Wright, Brent Adams, Bob Hyland, Subra Suresh, Clyde Briant, Alan Ardell, Mitch Luskin, Liz Holm, Simon Gill, T. Abinandanan, Long Chen, Michael Ortiz (da Mig), Eberhard Bodenschatz, Art Voter, Chris Roland, Chris Wolverton, Charles-Andre Gandin, Michel Rappaz, Nik Provatas, John Hamilton, Farid Abraham, Harry Bhadesia and David Clarke. Thank you all again. My parents and sisters provided me a rich and interesting family life for which I count my blessings more each day and for which I thank them. Though the writing of this book took much time and effort spent in solitude to the sounds of Santana, Yehudi Menuhin, Bobby Caldwell, Eric Clapton, Sarah Brightman and others, in the end, it is but a small thing when measured against the things that really count such as a family. Many authors close their acknowledgements with accolades for their families who tolerated their absence and fatigue, etc. My temptations are different and can be stated succinctly by noting that it is my greatest pleasure to round out this list of acknowledgements by thanking Amy, Casey and Molly, who make coming home even more fun than going to work.

Notes on Units, Scales and Conventions

In the chapters to follow, one of our aims is to try to recast many of our results in numerical form, giving an impression of the many interesting scales (length, time, energy, stress, etc.) that arise in discussing solids. A prerequisite to such discussions is to make sure that a correspondence has been constructed between the units favored here and those encountered in the everyday experience of the reader. Geometric and Structural Notions. One of the most signiﬁcant single ideas that will appear in what follows is the important role played by geometric structures at a number of different scales within materials. Indeed, the coupling between structure and properties is an element of central orthodoxy in materials science. In characterizing the structures within materials, it is clearly overly pedantic to hold to any single set of units for characterizing such structures, and we will comfortably interchange between a few different units of measure. The smallest scales that we will touch upon are those tied to the existence of atoms and their arrangements to form crystalline solids. Two fundamental units of length are ˚ = 10−10 m) and the most popular in this setting, namely, the a˚ ngstrom (1 A −10 Bohr radius (a0 ≈ 0.529 177 × 10 m). The a˚ ngstrom should be seen as a member in the series of scales which are all simple factors of 10 away from the meter itself. On the other hand, the Bohr radius arises as a natural unit of length in assessing atomic-scale processes since it is built up as a combination of the fundamental constants characterizing these processes, namely, a0 = h¯ 2 /m e e2 , where h¯ is Planck’s constant, m e is the mass of the electron and e is the charge on an electron. We will also occasionally resort to the use of nanometers (1 nm = 10−9 m) as an alternative unit of length when characterizing atomic-scale processes. When characterizing structures at the microstructural level, we will try to hold to a single unit of length, the micron (1 µm = 10−6 m). Note that a human hair has dimensions on the order of 50 µm. The use of both nanometers and microns will be seen as characteristic of the dimensions of many structural features such as precipitates xxiv

Notes on Units, Scales and Conventions

xxv

and inclusions as well as the grains making up polycrystals. In our ambition of providing meaningful geometric classiﬁcations of solids, it will also be necessary to make reference to units of area and volume, both of which will be reported either ˚ 2 or m2 for areas using a˚ ngstroms or meters as the base unit, resulting in either A ˚ 3 or m3 for volumes. and A Time Scales and Temporal Processes. One of our recurring themes in the pages to follow will be the role of disparate scales in characterizing processes and structures within materials. In addition to the diversity of spatial scales, there are a host of processes in solids which are themselves characterized by widely different time scales. As a result, we will be forced to adopt a series of different measures of the passage of time. One of the elemental processes in solids that will occupy much of our attention is that of the vibrations of solids. As will become evident in later chapters, atomic vibrations are characterized by frequencies on the order of 1013 –1014 Hz, which corresponds to a time scale on the order of one-tenth of a picosecond. As a result, we will make use of both 1.0 fs = 10−15 s and 1.0 ps = 10−12 s in describing atomic motions. Force and Energy. Just as with the characterization of the various geometric structures that populate solids we will stick to a few standard units of measure: we will adopt a strategy of characterizing the various measures of force, stress and energy in terms of a few basic units. The two units of force that will occupy centerstage in the pages that follow are the standard MKS unit, the newton, ˚ (eV is a unit of energy) which is much and the less familiar choice of eV/A more representative of the types of forces that arise in characterizing atomic-scale motions. When translated into units of stress, we will ﬁnd it advantageous again to adopt two distinct sets of units, namely, the MKS unit of stress, the pascal ˚ 3 . In addition, we will ﬁnd (1 Pa = 1 N/m2 ) and the atomic-scale analog, eV/A it convenient to interchange between units of energy reported in both joules and electron volts (eV). In particular, we recall that the conversion between these two sets of units is given by 1.0 eV ≈ 1.602 × 10−19 J. On the other hand, from time to time we will also invoke the rydberg as a unit of energy. This unit of energy arises naturally in characterizing the energy levels of atoms and can be expressed in terms of fundamental constants as Ry = me4 /2h¯ 2 . Note that the conversion between Ry and eV is, 1 Ry = 13.6058 eV. In our analysis of activated processes, we will repeatedly ﬁnd it advantageous to reckon our energies in dimensionless form, where the energy scale is determined by k B T , here k B ≈ 1.38 × 10−23 J/K is Boltzmann’s constant. We note that a useful rule of thumb is that for room temperature, k B T ≈ 1/40 eV. For the remainder of the book, we will suppress the subscript on k B .

xxvi

Notes on Units, Scales and Conventions

Material Parameters. The key means whereby material speciﬁcity enters continuum theories is via phenomenological material parameters. For example, in describing the elastic properties of solids, linear elastic models of material response posit a linear relation between stress and strain. The coefﬁcient of proportionality is the elastic modulus tensor. Similarly, in the context of dissipative processes such as mass and thermal transport, there are coefﬁcients that relate ﬂuxes to their associated driving forces. From the standpoint of the sets of units to be used to describe the various material parameters that characterize solids, our aim is to make use of one of two sets of units, either the traditional MKS units or those in which the eV is the unit of energy and the a˚ ngstrom is the unit of length. Conventions. During the course of this work we will resort to several key conventions repeatedly. One important example is that of the summation convention which instructs us to sum on all repeated indices. For example, the dot product of two vectors may be written a · b = a1 b1 + a2 b2 + a3 b3 = ai bi .

(1)

A second key notational convention that will be invoked repeatedly is the deﬁnition of the dyadic product given by (a ⊗ b)v = a(b · v). Another key convention that will be used repeatedly is the notation that {ai } refers to the set a1 , a2 , . . . , a N . When carrying out integrations, volumes will typically be denoted by while the boundary of such a volume will be denoted as ∂.

Part one Thinking About the Material World

ONE

Idealizing Material Response

1.1 A Material World Steel glows while being processed, aluminum does not. Red lasers are commonplace, while at the time of this writing, the drive to attain bright blue light is being hotly contested with the advent of a new generation of nitride materials. Whether we consider the metal and concrete structures that ﬁll our cities or the optical ﬁbers that link them, materials form the very backdrop against which our technological world unfolds. What is more, ingenious materials have been a central part of our increasing technological and scientiﬁc sophistication from the moment man took up tools in hand, playing a role in historic periods spanning from the Bronze Age to the Information Age. From the heterostructures that make possible the use of exotic electronic states in optoelectronic devices to the application of shape memory alloys as ﬁlters for blood clots, the inception of novel materials is a central part of modern invention. While in the nineteenth century, invention was acknowledged through the celebrity of inventors like Nikola Tesla, it has become such a constant part of everyday life that inventors have been thrust into anonymity and we are faced daily with the temptation to forget to what incredible levels of advancement man’s use of materials has been taken. Part of the challenge that attends these novel and sophisticated uses of materials is that of constructing reliable insights into the origins of the properties that make them attractive. The aim of the present chapter is to examine the intellectual constructs that have been put forth to characterize material response, and to take a ﬁrst look at the types of models that have been advanced to explain this response. 1.1.1 Materials: A Databook Perspective What is a material? The answer to this seemingly nonsensical question strikes right to the heart of some of the key issues it is the aim of this book to examine. 3

4

1 Idealizing Material Response

From the most naive of perspectives, questions surrounding the deﬁning qualities of a particular material are easily answered in terms of our everyday perceptions: weight, luster, color, hardness, susceptibility to heating. However, these simple notions are a reﬂection of a deeper underlying identity, an identity that is revealed quantitatively the moment one poses the question of precisely how a given material replies when affected by some external probe. If we subject a material to a force, it changes shape. If we apply a potential difference, electrical current might ﬂow. And if the temperatures of the two ends of a sample are different, a ﬂow of heat results. In each of these cases, these experiments reveal something further about the identity of the material in question. One of the overarching conceptual themes that has emerged from such simple experiments and that rests behind the quantitative description of materials is the idea of a material parameter. For example, Hooke’s original efforts, which were aimed at uncovering the relation between a body’s extension and the applied force that engendered it, led to the recognition that there exist a series of numbers, namely the elastic moduli, that characterize the elastic response of that material under different loading conditions. Similarly, there is a well established tradition of subjecting materials to applied ﬁelds which result in the emergence of various ﬂuxes such as the electrical and thermal currents mentioned above. Allied with these ﬂuxes are material parameters that link the response (i.e. the ﬂux) to the applied ﬁeld. In these cases and many more, the central idea is that a particular material can be identiﬁed in terms of the speciﬁc values adopted by its material parameters. In fact, for some purposes, a particular material may be idealized completely in terms of a set of such parameters. For the elastician, single crystal Al is characterized by a density and three elastic constants, namely, C11 = 106.78 GPa, C12 = 60.74 GPa and C44 = 28.21 GPa (data for Al at 300 K taken from Simmons and Wang (1971)). By way of contrast, to the engineer concerned with the application of Al in thermal environments, Al is speciﬁed in terms of a density and a thermal conductivity κ = 2.37 W/(cm K) (data for Al at 300 K taken from Shackelford et al. (1995)). This type of idealization of a material in which its entire identity is represented by but a few numbers is one of far-reaching subtlety. In the context of the elastic constants, all of the relevant atomic bond stretching and bending has been subsumed into the three material parameters introduced above. Similarly, the full complexity of the scattering of phonons giving rise to the thermal properties of a material has also been subsumed into just one or a few numbers. One of our primary missions in the coming chapters will be to explore how such effective theories of material behavior may be built strictly on the basis of such material parameters and to examine what gives rise to the difference in these parameters from one material to the next.

1.1 A Material World

5

From the standpoint of the idea given above, a particular material is characterized by a set of numbers that can be unearthed in a databook. For example, important parameters include the density ρ, the yield stress σ y , the fracture toughness K I C and the diffusion constant D. We note that in each case there is a number that can be looked up that characterizes the weight of a material in some normalized terms (i.e. the density), the resistance of the material to permanent deformation and fracture (yield strength and toughness), the ease with which mass can be transported within the material at elevated temperatures (diffusion constant) and any of a number of other possibilities. Our main point is to illustrate the way in which a given number (or set of numbers) can be used to introduce material speciﬁcity into continuum treatments of material response. For example, in considering the continuum treatment of mass transport, it is held that the ﬂux of mass is proportional to the gradient in concentration, with the constant of proportionality being the diffusion constant. This same basic strategy is exploited repeatedly and always hinges on the fact that the complexity of the atomic-level processes characterizing a given phenomenon can be replaced with a surrogate in the form of material parameters. The signiﬁcance of the notion of a material parameter is further clariﬁed by putting the properties of different materials into juxtaposition with one another. In ﬁgs. 1.1 and 1.2, we follow Ashby (1989) with some representative examples of the range of values taken on by a few prominent material properties, namely the Young’s modulus, the yield strength, the fracture toughness and the thermal conductivity. The basic idea adopted in Ashby’s approach is to allow the contrasts between the properties of different materials to speak for themselves. One of our aims in the chapters that follow will be to develop plausible explanations for the range of data indicated schematically in ﬁg. 1.1, with special attention reserved for thermomechanical properties. Despite the power of the idea of a material parameter, it must be greeted with caution. For many features of materials, certain ‘properties’ are not intrinsic. For example, both the yield strength and fracture toughness of a material depend upon its internal constitution. That is, the measured material response can depend upon microstructural features such as the grain size, the porosity, etc. Depending upon the extent to which the material has been subjected to prior working and annealing, these properties can vary considerably. Even a seemingly elementary property such as the density can depend signiﬁcantly upon that material’s life history. For a material such as tungsten which is often processed using the techniques of powder metallurgy, the density depends strongly upon the processing history. The signiﬁcance of the types of observations given above is the realization that many material properties depend upon more than just the identity of the particular atomic constituents that make up that material. Indeed, one of our central themes will

6

1 Idealizing Material Response

Fig. 1.1. Elastic and plastic properties of a wide class of materials (adapted from Ashby (1989)).

1.1 A Material World

7

Fig. 1.2. Fracture and thermal properties of a wide class of materials (adapted from Ashby (1989)).

8

1 Idealizing Material Response

be the argument that microstructural features such as point defects, dislocations and grain boundaries can each alter the measured macroscopic ‘properties’ of a material. One of our primary concerns in the pages that follow is to understand the emergence of material properties on the basis of the geometric structures that populate materials. This critical link between structure and properties has been canonized through the structure–properties paradigm which elevates the analysis of structure as a prerequisite to understanding properties. We have tried, in this section, to present something of the backdrop against which we will develop models of material behavior, especially with reference to thermomechanical properties. As an introduction to such models we ﬁrst examine the role played by geometric structure in dictating material properties, followed by an overview of the ways in which materials may be tailored to yield particular values of these material parameters.

1.1.2 The Structure–Properties Paradigm In the previous section we noted that, in the abstract, Al (or any other material) may be characterized by a series of numbers, its material parameters, to be found in a databook. However, as we already hinted at, because of the history dependence of material properties, the description of such properties is entirely more subtle. There is no one aluminum, nor one steel, nor one zirconia. Depending upon the thermomechanical history of a material, properties ranging from the yield strength to the thermal and electrical conductivity can be completely altered. The simplest explanation for this variability is the fact that different thermomechanical histories result in different internal structures. A fundamental tenet of materials science hinted at in the discussion above is the structure–properties paradigm. The claim is that by virtue of a material’s structure many of its associated properties are determined. Structure is an intrinsically geometric notion and one of the abiding themes in this book will be the constant reminder that it is structure on a variety of different length scales that gives rise to many of the well-known properties of materials. From the atomic-scale perspective we will constantly return to the implications of the fact that a material has a given crystal structure, whether it be for its role in dictating the properties of interfacial defects such as antiphase boundaries or the elastic anisotropy that must enter elasticity theory if the crystal symmetries are to be properly accounted for. Next, we will devote repeated attention to the lattice defects that disturb the uninterrupted monotony of the perfect crystal. Vacancies, interstitials, dislocations, stacking faults, grain boundaries and cracks will each claim centerstage in turn. At yet lower resolution, it is geometry at the microstructural scale that comes into relief and will occupy much of our attention. At each of these scales we will return to

1.1 A Material World

9

Fig. 1.3. Yield strength data for steel as a function of grain size d (adapted from Leslie (1981)). Plot shows dependence of yield stress on inverse power of grain size. The legends at the top of the ﬁgure show the actual grain size as measured in both µm and using the ASTM units for grain size.

the question of the structure–properties paradigm, always with a critical eye, to see just how far it may take us in our desire to unearth the behavior of real materials. A celebrated example of the coupling of structure and properties is exhibited in ﬁg. 1.3 in which the relation between the yield strength and the grain size is depicted. In particular, the Hall–Petch relation √ posits a relation between the yield stress and the grain size of the form σ y ∝ 1/ d, where d is the grain size of the material. The Hall–Petch relation leads us to two of the most important notions to be found in contemplating materials: the existence of microstructure and its implications for material properties, and the development of scaling laws for characterizing material response. An immediate consequence of the results depicted here is the insight that not only are structures at the atomic scale important, but so too are the geometric structures found at the microstructural scale. We have noted that the attempt to understand materials demands that we confront a hierarchy of geometric structures, starting with the atomic-level geometries presented by the crystal lattice and increasing in scale to the level of the isolated defects that exist within materials to their assembly into the material’s microstructure itself. The quest to understand the structure of a given material inevitably commences with the phase diagram. Phase diagrams are one of the primary road maps of the materials scientist. Such diagrams represent a summary of a series of tedious analyses aimed at determining the equilibrium atomic-scale structure of a given element or mixture of elements for a series of temperatures (and possibly

10

1 Idealizing Material Response

Fig. 1.4. Phase diagram of elemental sulfur (adapted from Young (1991)).

pressures). In ﬁgs. 1.4 and 1.5, we show the equilibrium phase diagrams of elemental sulfur and the iron–carbon system. The particular choices of materials shown here are meant to give a feel for the existence of the rich atomic-level complexity that is found in both elemental systems and their alloy counterparts. Note that in the case of elemental sulfur, there are not less than ten different equilibrium structures corresponding to different values of the temperature and pressure. These structures are built around molecular S8 and range from orthorhombic to monoclinic lattices. The iron–carbon phase diagram illustrates a similar structural diversity, with each phase boundary separating distinct structural outcomes. Phase diagrams like those discussed above have as their primary mission a succinct description of the atomic-level geometries that are adopted by a given system. However, as we have already mentioned, there is structure to be found on many different length scales, and one of the surprises of deeper reﬂection is the realization that despite the fact that phase diagrams reﬂect the equilibrium state of a given material, they can even instruct us concerning the metastable microstructures that occur at larger scales. The simplest example of such thinking is that associated with precipitation reactions in which an overabundance of substitutional impurities is frozen into a system by quenching from high temperatures. If the material is subsequently annealed, the phase diagram leads us to expect a two-phase

1.1 A Material World

11

Fig. 1.5. Phase diagram for the iron–carbon system (adapted from Ashby and Jones (1986)).

microstructure in which the overabundance of substitutional impurities is now taken up in the relevant equilibrium phase. What this suggests is that strategies can be concocted for preparing particular metastable states with desirable properties. It is this insight that has led to many of the heat and beat strategies that have attracted pejorative attention to the materials engineer. A broad description of the signiﬁcance of phase diagrams to materials science may be found in Massalski (1989). As noted above, the phase diagram instructs our intuitions concerning the atomic-level geometries of materials. At the next level of geometric complexity in the hierarchy of structures that exist within a material, we must confront the defects that populate materials. Indeed, one of the key realizations that we will revisit from a number of different perspectives is that of the role of defects in the determination of material response. What this means is that the structure–properties paradigm makes an ambiguous use of the word ‘structure’ since in different situations, the structures being referenced can range all the way from atomic-scale structure to that of the nature of the grains making up a polycrystal. At the level of the defect

12

1 Idealizing Material Response

geometries found within materials, our present argument is that if we trace yield in crystals to the mechanisms which engender it for example, it is the motion of dislocations which will be implicated. Similarly, if we pursue the stress–strain curve to its limits, the material will fail either through crack propagation or void coalescence or some other defect mechanism. The implication of this insight is that much of the work of modeling the thermomechanical behavior of materials can be reduced to that of carrying out the structure–properties linkage at the level of defect structures within materials. In later chapters, we will adopt a hierarchical approach to constructing models of material response. First, we will examine the way in which atomistic models can be used to uncover the structural rearrangements in defect ‘cores’ which are a signature of the nonlinear interatomic interactions that are difﬁcult to capture within continuum theory. Once these tools are in hand, we will turn to an analysis of the dominant defect types themselves, with a classiﬁcation scheme centered on the dimensionality of these defects. Having successfully captured the structure and energetics of single defects, our next mission will be to understand the role of defects as conspiratorial partners in the emergence of observed macroscopic behavior. The uncovering of this conspiracy will in the end always lead us to questions of averaging. The challenge here is in forging the connection between the behavior of single defects, on one hand, and the macroscopic material response, on the other, which often emerges as a synthetic response of many defects in concert.

1.1.3 Controlling Structure: The World of Heat and Beat In the previous section we considered the critical role played by structures at a number of different scales in determining material properties. From the standpoint of the materials engineer this insight may be recast as a challenge: how may the various structures within a material be tailored so as to yield desired properties? Metallurgy has a longstanding reputation as an empirical subject founded upon the twin pillars of heating and beating a material to some desired form. Whether one resorts to cold working a material or subjecting it to a high-temperature anneal, the outcome of these processes is a change in the internal constitution of that material at one or more scales. Because of these structural changes, there is a concomitant change in the properties of the material. Indeed, these strategies for altering the structure of materials should be seen as the answer to the challenge posed above. By carefully selecting the thermal and mechanical history of a material, it is possible to tailor a number of different features of that material. Low-temperature anneals can induce precipitate reactions that increase the yield stress. Cold working changes the dislocation density, and this too alters the yield stress. If the material

1.1 A Material World

13

Fig. 1.6. Schematic of the different microstructures for the Ni–Al system that are obtained using different thermomechanical processing schedules (adapted from Kumar et al. (1992)). The ﬁgure illustrates precipitation at grain boundaries and within grains.

is exposed to a particular chemical atmosphere it can result in a thin surface layer that can increase the material’s hardness, a strategy that is adopted in the production of carburized steels. In each of these examples, through annealing (heat) or deformation (beat) or both, the internal structures within the material are changed and as a result, so too are the macroscopic properties. As an explicit example of how a material changes when subjected to the type of processing program introduced above, ﬁg. 1.6 shows a schematic of the microstructures that arise from slightly different chemical compositions and for different thermal histories for Ni-rich Ni–Al alloys. The ﬁgure illustrates the signiﬁcant variety in microstructure as a function both of slight ( 0, E˙ surf is the increase in surface energy and may be written down directly as E˙ surf = 4γ a, ˙ where γ is the surface energy and (a, ˙ a) is the dissipative potential and is of the form (a, ˙ a) = a˙ 2 /2M. The factor of 4 in the expression for E˙ surf results from the fact that for a crack of length 2a such as that under consideration here, there is both a top and bottom face contributing to the overall surface energy. To proceed with the calculation, we must still determine the rate of change of E elastic . For a crack of length 2a under plane strain conditions and subject to a remote load σ0 , the elastic energy is given by (a result which we apologize for quoting without proof, see Lawn (1993)) E elastic (a) = −

πa 2 σ02 (1 − ν 2 ) , E

(2.71)

˙ a) is given by implying that E˙ elastic (a, 2πaσ02 (1 − ν 2 ) E˙ elastic (a, a. ˙ ˙ a) = − E

(2.72)

Note that E is the Young modulus and ν is the Poisson ratio for the material of interest. We are now ready to turn to the concrete implementation of the variational statement of eqn (2.70). Evaluation of ∂/∂ a˙ results in the equation of motion 2πaσ02 (1 − ν 2 ) a˙ = − 4γ . M E

(2.73)

Grifﬁth sought the criticality condition at which a˙ = 0. That is, his argument (which was carried out completely differently than we have done here) was to determine the precise condition under which the elastic energy release rate would just compensate for the energy that must be donated to create new free surface. Regardless of the route taken to get the result, this condition results in a critical

2.4 Continuum Descriptions of Deformation and Failure

63

stress for crack initiation of the form σ0crit

=

2Eγ . πa(1 − ν 2 )

(2.74)

Much of the discussion given above can be recast in the language of section 2.3.3. In particular, we see that the question posed above was how does the total potential energy of the system change during incremental crack extension? This may be recast in mathematical form as G=−

∂ E elastic , ∂a

(2.75)

where G is the mechanical energy release rate. The key point to be made presently is the observation that the quantity −∂ E elastic /∂a is exactly the type of conﬁgurational force introduced earlier and, as a result, we may invoke the ideas presented there. In particular, in the fracture context, eqn (2.45) is of such importance it is digniﬁed with a special name, namely, the J -integral and given by ∂u l Ji = W n i − σlm n m ds. (2.76) ∂ xi The integral is framed in the context of a two-dimensional geometry with the contour parameterized by s. The key point is that by evaluating this integral it is possible to reproduce exactly the type of result given in eqn (2.71). For the purposes of the present discussion, there were three main ideas that we wished to put forth concerning fracture. First, we noted that if fracture is imagined to be a homogeneous process in which bonds in the perfect crystal are stretched until they break, this leads to a critical stress for fracture (the ideal tensile strength) known to be completely out of line with experimental values. As a remedy to this paradox, it was realized that ﬂaws such as cracks could have the effect of locally magnifying the remotely applied stress to levels consonant with that needed to break atomic-level bonds. The linear elastic theory of fracture mechanics teaches us how to assess the elastic consequences of these defects, a subject we will return to in chap. 11. Finally, we wished to illustrate how using energetic arguments like those of Grifﬁth, which we have reformulated in the language of conﬁgurational forces and the associated variational principle presented in section 2.3.3, the critical stress for crack initiation may be determined on the basis of microscopic parameters such as the surface energy. It bears emphasizing again that it is particularly interesting how far a linear elastic analysis can take us in evaluating what is an intrinsically nonlinear process.

64

2 Continuum Mechanics Revisited

2.5 Boundary Value Problems and Modeling From the standpoint of the continuum simulation of processes in the mechanics of materials, modeling ultimately boils down to the solution of boundary value problems. What this means in particular is the search for solutions of the equations of continuum dynamics in conjunction with some constitutive model and boundary conditions of relevance to the problem at hand. In this section after setting down some of the key theoretical tools used in continuum modeling, we set ourselves the task of striking a balance between the analytic and numerical tools that have been set forth for solving boundary value problems. In particular, we will examine Green function techniques in the setting of linear elasticity as well as the use of the ﬁnite element method as the basis for numerical solutions.

2.5.1 Principle of Minimum Potential Energy and Reciprocal Theorem In many of the cases in which we resort to the theoretical analysis of a particular problem from a continuum perspective, it will be from the point of view of the linear theory of elasticity. Though we have already introduced the fundamental governing equations of continuum mechanics as well as their linear elastic incarnation, in many instances it will be useful to assign these ideas a variational character. In the context of linear elastic solids, the global principle presiding over equilibrium states (which we assert without proof, for details see Gurtin (1981), for example) is the fact that they are privileged states characterized by the property that they minimize the total potential energy. In particular, in the context of linear elastic boundary value problems, the equilibrium displacement ﬁelds are minimizers of the potential energy functional W ({u i, j })d V − t · ud A − f · ud V, (2.77) [u(x)] =

∂

where the ﬁrst term on the right hand side yields the elastic energy stored in the body, the second term is associated with the potential energy of external loads that are communicated to the body at its surface and the third term provides a measure of the work associated with body forces. The formal statement of the principle is that of all the kinematically admissible ﬁelds (i.e. those ﬁelds that are sufﬁciently smooth and satisfy the displacement boundary conditions), the equilibrium ﬁelds will minimize the functional of eqn (2.77). The importance of this theorem will be especially felt in two separate contexts. First, in a number of instances, it will be most natural to construct models of a given problem which are couched in the language of energetics. In many such instances, the total energy will be parameterized in terms of one or several conﬁgurational coordinates, and the resulting minimization will seek their optimal conﬁguration. The principle

2.5 Boundary Value Problems and Modeling

65

of minimum potential energy will also see action as the basis of many of the approximation strategies that are adopted to solve linear elastic boundary value problems, and in particular, the ﬁnite element method. To illustrate the equivalence of the energy minimization principle advanced above and the linear elastic equilibrium equations of section 2.4.2, we resort to evaluating the functional derivative of eqn (2.77) and setting it equal to zero, or in mathematical terms δ/δu i = 0. Equivalently, working in indicial notation, we ﬁnd 1 1 Ci jkl δi j kl d V + Ci jkl i j δkl d V − f i δu i d V − ti δu i d A. δ = 2 2 ∂ (2.78) Exploiting the symmetries of the elastic modulus tensor and the strain tensor, the ﬁrst two terms may be joined to form σi j δi j d V . Rewriting the integrand σi j δi j as ∂ ∂ δu i = (σi j δu i ) − σi j, j δu i , (2.79) σi j ∂ xj ∂ xj and plugging this result back into the expression given above followed by an application of the divergence theorem leaves us with (σi j n j − ti )δu i d A = 0. (2.80) δ = (σi j, j + f i )δu i d V +

∂

The signiﬁcance of this result emerges once it is recalled that δu i itself is arbitrary except for the fact that δu i = 0 on that part of the boundary for which u is prescribed, and hence that the integrands themselves must vanish. But in the case of the integral over , this results in Ci jkl u k,l j + f i = 0 which is nothing more than the original linear elastic equilibrium equations for a homogeneous material. Further, applying the same reasoning to the surface integrals compels us to accept that σi j n j = ti on that part of the boundary characterized by traction boundary conditions. Again, what all of this means is that there is an equivalence between the original equilibrium equations for linear elasticity and insisting that the potential energy [u(x)] be minimized. As remarked above, in most instances in fact, we will favor the energetic interpretation of equilibrium. In addition to the theoretical advantages offered by the principle of minimum potential energy, our elastic analyses will also be aided by the reciprocal theorem. This theorem is a special example of a more general class of reciprocal theorems and considers two elastic states (u(1) , (1) , σ (1) ) and (u(2) , (2) , σ (2) ), where each state satisﬁes the equilibrium equations and boundary conditions associated with body force ﬁelds f1 and f2 , respectively. The theorem asserts that the work done by the external forces of system 1 on the displacements of system 2 is equal to the work done by the external forces of system 2 on the displacements of system 1.

66

2 Continuum Mechanics Revisited

Mathematically, this is written as t(1) · u(2) d A + f (1) · u(2) d V = ∂

∂

t(2) · u(1) d A +

f (2) · u(1) d V. (2.81)

The signiﬁcance of this result will be appreciated later (for example in section 8.4.2) when we see that it can be used for the construction of fundamental solutions for the elastic displacement ﬁelds of defects such as dislocations. The proof of the reciprocal theorem is based upon two fundamental realizations. First, we note the relation (1) (2) (1) (2) t ·u dA + f · u dV = (1) : C (2) d V. (2.82) ∂

The veracity of this expression can be shown by running the divergence theorem in reverse, basically turning the argument given above to prove the principle of minimum potential energy around. This result in conjunction with the application of symmetries of the tensor of elastic moduli allows us to note (1) : C (2) d V = (2) : C (1) d V. (2.83)

Based on this latter result, the reciprocal theorem is immediate.

2.5.2 Elastic Green Function One of the most powerful means for solving boundary value problems in linear elasticity is that of Green functions. The Green function approach offers the possibility of building up solutions to complex problems on the basis of insights garnered from the solution to the problem of a unit point load. The pivotal assumption exploited in this context is that of linearity which allows us to use the fact that a sum of solutions to a given problem is itself a solution, a result known as the superposition principle. As a result of this principle and a knowledge of the Green function, solutions to generic problems are written as integrals over a kernel provided by the fundamental solution itself. As noted above, the elastic Green function yields the elastic ﬁelds induced by a point load. The ideas here resemble those from the setting of electrodynamics where point sources of charge are the basis of the Green function approach. Recall from earlier that the equilibrium equations that govern the continuum are given by σi j, j + f i = 0,

(2.84)

where σi j is the i j th component of the Cauchy stress and f i are the components of the body force. In the special case of an isotropic linear elastic solid, we have seen that these equations reduce to the Navier equations shown in eqn (2.55).

2.5 Boundary Value Problems and Modeling

67

To construct the elastic Green function for an isotropic linear elastic solid, we make a special choice of the body force ﬁeld, namely, f(r) = f0 δ(r), where f0 is a constant vector. In this case, we will denote the displacement ﬁeld as G ik (r) with the interpretation that this is the i th component of displacement in the case in which there is a unit force in the k th direction, f0 = ek . To be more precise about the problem of interest, we now seek the solution to this problem in an inﬁnite body in which it is presumed that the elastic constants are uniform. In light of these deﬁnitions and comments, the equilibrium equation for the Green function may be written as (λ + µ)

∂2 ∂ ∂ G m j (r) + µ G i j (r) = −δi j δ(r). ∂ xi ∂ xm ∂ xl ∂ xl

(2.85)

Interesting strategies have been adopted for explicitly determining G(r) both in real space as well as Fourier space. Here we follow de Wit (1960) in adopting the Fourier space scheme, leaving the real space solution for the ambitious reader. To ﬁnd the Green function, we exploit our Fourier transform convention: ˜ (2.86) G i j (k) = G i j (r)e−ik·r d 3 r, and G i j (r) =

1 (2π )3

G˜ i j (k)eik·r d 3 k.

(2.87)

Upon Fourier transforming eqn (2.85) as dictated by the deﬁnitions given above, we ﬁnd (2.88) (λ + µ)ki km G˜ m j (k) + µk 2 G˜ i j (k) = δi j , where ki is the i th component of the wavevector k. The k-space Green function can be found by multiplying the previous equation by ki and summing on the repeated index i, which yields the result, km G˜ m j =

kj , (λ + 2µ)k 2

(2.89)

which may be substituted into eqn (2.88). After carrying out the resulting manipulation, the explicit expression for the Green function in Fourier space is

1 (λ + µ) ki k j ˜ δi j − . (2.90) G i j (k) = µk 2 (λ + 2µ) k 2 This result will serve as the cornerstone for many of our developments in the elastic theory of dislocations. We are similarly now in a position to obtain the Green function in real space which, when coupled with the reciprocal theorem, will allow for the determination of the displacement ﬁelds associated with various defects.

68

2 Continuum Mechanics Revisited

Following the procedure used in electrostatics where it is found that the Fourier transform of the Coulomb potential yields a k −2 dependence, we can invert the expression found above rather easily as

δi j xi x j 1 (2.91) (λ + 3µ) + (λ + µ) 3 . G i j (r) = 8π µ(λ + 2µ) r r As a result of these various algebraic machinations, we are now prepared to construct solutions to problems in isotropic elasticity through superposition of the fundamental solution constructed above. The Green function enables us to ﬁnd the displacements at point x given the presence of a point force at point x . However, because of the linearity of the underlying governing equations, the solution for an arbitrary force distribution can be built up as a superposition over a collection of such point forces. That is, we claim that the solution to Ci jkl u k, jl = − f i is u k (x) = G km (x − x ) f m (x )d 3 x . (2.92)

The proof of this claim can be sketched in abstract terms as follows. If we are to write the original governing equation for the displacements as L(x)u(x) = −f(x), where L is the linear operator associated with the various differentiations in the equilibrium equations, then the equation satisﬁed by the Green function may be written as L(x)G(x −x ) = −Iδ(x − x ). Our assertion is that the displacements are given by u(x) = G(x − x )f(x )d 3 x . Application of the operator L to this equation for the displacements results in 3 L(x)u(x) = L(x)G(x − x )f(x )d x = − f(x )δ(x − x )d 3 x = −f(x),

(2.93) demonstrating that when we write the displacements as a convolution inte gral, namely, u(x) = G(x − x )f(x )d 3 x , the original governing equations are satisﬁed. Eqn (2.92) is the culmination of our efforts to compute the displacements due to an arbitrary distribution of body forces. Although this result will be of paramount importance in coming chapters, it is also important to acknowledge its limitations. First, we have assumed that the medium of interest is isotropic. Further reﬁnements are necessary to recast this result in a form that is appropriate for anisotropic elastic solids. A detailed accounting of the anisotropic results is spelled out in Bacon et al. (1979). The second key limitation of our result is the fact that it was founded upon the assumption that the body of interest is inﬁnite in extent. On the other hand, there are a variety of problems in which we will be interested in the presence of defects near surfaces and for which the half-space Green function will be needed. Yet another problem with our analysis is the assumption that the elastic constants

2.5 Boundary Value Problems and Modeling

69

Fig. 2.13. Four schematic examples of eigenstrains: (a) spherical inclusion, (b) eigenstrain due to thermal expansion, (c) dislocation loop and (d) eigenstrain due to wedge of martensite.

are the same throughout the material. On the other hand, when it comes time (see chap. 10) to investigate the elastic consequences of second-phase particles, the moduli of the inclusion can differ from those of the matrix, and again, the particulars (though not the concept) of our Green function analysis will have to be amended.

2.5.3 Method of Eigenstrains A very powerful technique in conjunction with that of elastic Green functions is the method of eigenstrains. The eigenstrain concept allows us to solve elasticity problems for a continuum with internal heterogeneities such as dislocations or inclusions, by replacing these heterogeneities by effective body force ﬁelds. An eigenstrain is deﬁned as a strain without any attendant internal stresses. The deﬁnition is abstract without the clariﬁcation afforded by particular examples. In ﬁg. 2.13, we show four distinct examples of elastic media in the presence of eigenstrains. For example, as shown in ﬁg. 2.13(a), an inclusion may be characterized by a strain i∗j which carries the information about how the inclusion differs structurally from the matrix material. In addition, we should note that in the absence of the constraining effect provided by the matrix, the eigenstrain i∗j has

70

2 Continuum Mechanics Revisited

Fig. 2.14. Energy as a function of shear for a generic crystalline solid. The periodicity of the energy proﬁle reﬂects the existence of certain lattice invariant shears which correspond to the ‘stress-free strains’ considered in the method of eigenstrains (adapted from Tadmor et al. (1996)).

no associated stress. Similarly, as shown in ﬁg. 2.13(b), if a crystal is to undergo thermal expansion, the associated strains can be thought of as eigenstrains since they imply no internal stresses. Dislocations can also be characterized in terms of eigenstrains since the region of the crystal that has slipped (see ﬁg. 2.13(c)) has suffered a lattice invariant shear. In ﬁg. 2.13(d) we imagine the case of a solid, part of which has undergone a phase transformation. Like in the inclusion example introduced above, the phase transformed region is characterized by an eigenstrain. Further insights into the eigenstrain concept can be obtained on the basis of energetic arguments. We imagine an energy landscape which characterizes the energy of the continuum as a function of the relevant kinematic measure such as the strain. In many cases of interest, the energy landscape is nonconvex, with different wells corresponding to different structural alternatives. The eigenstrain concept allows for the emergence of structures in which one part of the continuum corresponds to one well in the energy landscape while some other part of the continuum corresponds to a different well. In computing stresses, we appeal not to the total strain, but rather the departure of the strain from the well of interest. In many problems, different parts of the body are characterized by different eigenstrains. Clearly, in making a transition from one eigenstrain to another, speciﬁc regions will not be associated with a well in the energy landscape, and it is largely these incompatibilities that give rise to internal stresses. A concrete example of these energetic arguments can be made through consideration of simple shear. In generic terms, if a particular crystal is subject to a monotonically increasing shear, the energy as a function of this shear will have qualitative features such as those shown in ﬁg. 2.14. The existence of the periodicity in the energy

2.5 Boundary Value Problems and Modeling

71

proﬁle reﬂects the fact that there exist certain lattice invariant shears that map the Bravais lattice onto itself. The fundamental idea of the method of eigenstrains is the argument that if the system is sheared such that it occupies one of the minimum energy wells, there will be no associated stress. In mathematical terms, the implementation of the eigenstrain concept is carried out by representing the geometrical state of interest by some distribution of ‘stress-free strains’ which can be mapped onto an equivalent set of body forces, the solution for which can be obtained using the relevant Green function. To illustrate the problem with a concrete example, we follow Eshelby in thinking of an elastic inclusion. The key point is that this inclusion is subject to some internal strain i∗j , such as arises from a structural transformation, and for which there is no associated stress. The outcome of the hypothesis advanced above is that the stress is computed as ∗ σi j = Ci jkl (u tot k,l − kl ),

(2.94)

where u tot k,l is the displacement gradient of the total displacement ﬁeld. Note that the physical meaning of this equation corresponds to our statement above that it is only the departure of the strain from the nearest energy well that leads to the generation of stresses, and not the total strain. The imposition of the condition of equilibrium, namely, σi j, j = 0 in this context is then equivalent to ∗ Ci jkl u tot k,l j = C i jkl kl, j .

(2.95)

Since the eigenstrain itself is prescribed, eqn (2.95) can be interpreted as corresponding to a homogeneous elastic body, now in the presence of an effective body eff ∗ force f i = −Ci jkl kl, j . Note that in the context of the effective theory concept which we will return to repeatedly throughout this book, the eigenstrain idea allows us to replace some heterogeneity within a continuum by a series of effective body forces resulting in a tractable (sometimes) elasticity problem. As a result of the deﬁnition of the effective body force ﬁeld, the Green function machinery elucidated above may be exploited. In particular, recall eqn (2.92) which expresses the displacement ﬁelds as an integral over the force distribution. In the present setting, the unknown displacements may be written as a convolution integral of the elastic Green function and the effective body force distribution as ∗ u k (x) = − G km (x − x )Cmrst st,r (x )d 3 x . (2.96)

Of course, there are a number of manipulations (integration by parts, for example) that can be carried out in order to restate this result in a more convenient fashion. On the other hand, our intention at this point is to introduce the conceptual framework, and to reserve the explicit use of the method of eigenstrains until later.

72

2 Continuum Mechanics Revisited

2.5.4 Numerical Solutions: Finite Element Method Despite the existence of powerful analytical tools that allow for explicit solution of certain problems of interest, in general, the modeler cannot count on the existence of analytic solutions to most questions. To remedy this problem, one must resort to numerical approaches, or further simplify the problem so as to reﬁne it to the point that analytic progress is possible. In this section, we discuss one of the key numerical engines used in the continuum analysis of boundary value problems, namely, the ﬁnite element method. The ﬁnite element method replaces the search for unknown ﬁelds (i.e. the solutions to the governing equations) with the search for a discrete representation of those ﬁelds at a set of points known as nodes, with the values of the ﬁeld quantities between the nodes determined via interpolation. From the standpoint of the principle of minimum potential energy introduced earlier, the ﬁnite element method effects the replacement [u(x)] → ({ui }),

(2.97)

where [u(x)] is a functional of the unknown displacement ﬁelds and ({ui }) is a function of a discrete set of nodal displacements indexed by the integer i which runs from 1 to N , where N is the number of nodes. We note that the ﬁnite element method is in no way restricted to elasticity problems, but that such problems will serve as a convenient vehicle for our discussion. The central ideas associated with the ﬁnite element approach may be summarized as follows. First, the original boundary value problem is stated in weak form (i.e. the relevant partial differential equations are restated in integral form). Next, the continuum is parceled up into discrete regions known as elements, with the unknown ﬁeld variables considered at the points of intersection of these elements known as nodes. The net result of this discretization is that we have now replaced a problem in which we are searching for an unknown function u(x) with a search for discrete set of 3N variables {ui } (i.e. the three components of displacement for each of the N nodes). One crucial observation at this juncture is that the elements need not be uniform, thereby allowing for mesh design in which near rapidly varying parts of the solution, one uses high resolution, while in regions of slow variation larger elements can be supported. From the perspective of variational principles, the idea embodied in the ﬁnite element approach is similar to that in other schemes: identify that particular linear combination of basis functions that is ‘best’ in a sense to be deﬁned below. The approximate solution of interest is built up as linear combinations of basis functions, and the crucial question becomes how to formulate the original boundary value problem in terms of the relevant expansion coefﬁcients.

2.5 Boundary Value Problems and Modeling

73

Fig. 2.15. Replacement of a continuous body with a set of ﬁnite elements. In this case, the unknown displacement ﬁeld has been replaced by a discrete set of unknown nodal displacements, un .

Recall that within the continuum mechanics setting set forth in section 2.3.2, the equations of equilibrium may be written as σi j, j + f i = 0.

(2.98)

Our present task is to rewrite these equations in integral (or weak) form which will simplify the formulation in terms of ﬁnite elements. We introduce a series of ‘test functions’ wi (x) that satisfy the relevant displacement boundary conditions which are hence denoted as admissible ﬁelds and now contract these test functions with the equation given above and integrate over the spatial region of interest. This strategy results in wi σi j, j d V + wi f i d V = 0. (2.99)

If we now use integration by parts on the ﬁrst term in this equation, we are left with wi, j σi j d V = ti wi d A + f i wi d V, (2.100)

∂

where we have used ti = σi j n j . As yet, our exercise corresponds to nothing more than a statement of the principle of virtual work. On the other hand, if we now proceed with the concrete consideration of the test functions wi (x), it is possible to construct a numerical framework. As yet, our statements have been general and do not reﬂect our wish to replace the continuous problem with a discrete analog. We now imagine that the body is discretized into a set of elements which meet at vertices denoted as nodes and indicated in ﬁg. 2.15. Within each element, the value of the displacement is

74

2 Continuum Mechanics Revisited

Fig. 2.16. Schematic illustration of the three triangular shape functions tied to the different nodes of a triangular element.

obtained via interpolation according to u(x) = ui Ni (x),

(2.101)

i

where the subscript i refers to nodes and Ni (x) is the ‘shape function’ attached to the i th node and deﬁned through Ni (x j ) = δi j . That is, the i th shape function is 1 at the i th node and vanishes at neighboring nodes. These shape functions are illustrated in ﬁg. 2.16 in the case of linear triangular elements. In essence what we are saying is that the solution is determined at a discrete set of nodal values, and if we interest ourselves in the solution elsewhere, it is to be determined by interpolation in terms of those nodal values via a series of interpolation functions which are commonly referred to as shape functions. If we substitute the interpolated displacements as denoted above into the integral statement of the equilibrium equations, and furthermore, we take as our test functions the Ni s themselves (i.e. wi (x) = Ni (x)), we ﬁnd a series of equations in the unknown coefﬁcients of the form Ku = f,

(2.102)

where K is known as the stiffness matrix (and for nonlinear problems can depend upon u itself) and f is the force matrix. To make the treatment given above more than just an abstraction, we now consider the case of one-dimensional elasticity. We imagine our one-dimensional elastic medium to have length a and to be characterized by an elastic stiffness k. The traction vector, t (x), is directly related to the gradients in displacements by t = kdu/d x. Our weak statement of the equilibrium equations may be written as a a dw du dx = k f wd x + [t (a)w(a) − t (0)w(0)]. (2.103) dx dx 0 0 At this point, we are primarily confronted with a series of algebraic manipulations founded upon the ﬁnite element edicts described above. First, we approximate the solution u(x) in terms of the ﬁnite element shape functions, u(x) = i u i Ni (x). Secondly, we make the correspondence between the test functions w(x) and the

2.6 Difﬁculties with the Continuum Approach

75

shape functions themselves. For example, the equation resulting from the assertion w(x) = N j (x) is a a d N j (x) d Ni (x) dx = ui k f (x)N j (x)d x + [t (a)N j (a) − t (0)N j (0)]. dx dx 0 0 i (2.104) This equation may now be rewritten as K ji u i = f j (2.105) i

if we make the correspondence

K ji =

k 0

a

d N j (x) d Ni (x) d x, dx dx

(2.106)

a

fj =

f (x)N j (x)d x + [t (a)N j (a) − t (0)N j (0)].

(2.107)

0

The result of this analysis is a series of coupled algebraic equations in the unknown nodal displacements. For the linear problem we have considered here, these equations are themselves linear (though they are not in general) and our problem reduces to little more than diagonalization of the relevant stiffness matrix which, as seen above, can be computed as products of material parameters and geometric factors. In this section, we have seen how one may formulate numerical strategies for confronting the types of boundary value problems that arise in the continuum description of materials. The key point is the replacement of the problem involving unknown continuum ﬁelds with a discrete reckoning of the problem in which only a discrete set of unknowns at particular points (i.e. the nodes) are to be determined. In the next chapter we will undertake the consideration of the methods of quantum mechanics, and in this setting will ﬁnd once again that the ﬁnite element method offers numerical ﬂexibility in solving differential equations. 2.6 Difﬁculties with the Continuum Approach One of the key beneﬁts provided by the types of approaches advocated in this chapter is that the mathematics associated with solving for three unknown ﬁelds (for example) is more sympathetic than that of solving coupled ordinary differential equations in a number of variables of Avogradrian dimensions. On the other hand, continuum approaches have their disadvantages as well. We have noted earlier that one of the primary difﬁculties tied to the use of continuum models is their reliance on constitutive assumptions. In some instances, we will see that the constitutive models adopted are often selected as much for their theoretical convenience as

76

2 Continuum Mechanics Revisited

for their phenomenological realism. It is on these grounds that we will appeal to microscopic theories as the proper basis for informing higher-level constitutive strategies. A second difﬁculty that attends the use of continuum models is the fact that such models are indifferent to the presence of a minimum length scale as dictated by the typical separation between atoms. This absence of small scale resolution within the continuum framework can have a souring inﬂuence on the success of such theories in predicting features in the immediate vicinity of defects. One of our main objectives will be to show how, via the device of incorporating nonlinear information into our models, many of these difﬁculties may be sidestepped. As a result of the evident appeal of microscopic insights into the ultimate origins of continuum behavior, in the next chapter we undertake a review of the theoretical foundations of microscopic modeling, the partnership of quantum and statistical mechanics.

2.7 Further Reading Continuum Mechanics Continuum Mechanics by P. Chadwick, Halsted Press, New York: New York, 1976. My personal favorite, Chadwick’s book is direct and to the point, and full of clever insights and interesting examples. An Introduction to Continuum Mechanics by M. Gurtin, Academic Press Inc., San Diego: California, 1981. Gurtin’s book is a classic among solid mechanicians and gives a thorough treatment of much of the material found in the present chapter. ‘Mechanics of Solids’ by J. R. Rice in Encyclopedia Britannica Vol. 23, pg. 734 (1993) is an outstanding overview of the entire realm of solid mechanics, giving coverage not only of the principles of continuum mechanics, but also their applications to deformation and fracture with interesting historical and philosophic commentary. Nonlinear Continuum Mechanics for Finite Element Analysis by J. Bonet and R. D. Wood, Cambridge University Press, Cambridge: England, 1997. This book provides an interesting discussion of many of the concepts discussed in the present chapter and includes commentary on the numerical implementation of these same concepts. Mathematical Theory of Elasticity by I. S. Sokolnikoff, Krieger Publishing Company, Malabar: Florida, 1983. One of the classic texts on elasticity theory. Theory of Elasticity by S. P. Timoshenko and J. N. Goodier, McGraw Hill Book

2.7 Further Reading

77

Company, New York: New York, 1970. My personal taste for this book is founded on the fact that it is full of solutions to elasticity problems of interest. Theory of Elasticity by L. D. Landau and E. M. Lifshitz, Pergamon Press, Oxford: England, 1970. Written in the terse style that the Landau and Lifshitz series is famous for, the book is full of solutions and insights. Micromechanics of Defects in Solids by T. Mura, Kluwer Academic Publishers, Dordrecht: The Netherlands, 1993. Mura’s book is a neglected classic which features an enormous number of examples on the use of Green functions in conjunction with the method of eigenstrains. Plasticity The Mathematical Theory of Plasticity by R. Hill, Clarendon Press, Oxford: England, 1967. The deﬁnitive work on the mathematical theory of plasticity. This book goes well beyond our treatment regarding continuum descriptions of plasticity without entering into the question of how plasticity emerges as the result of defect motion. Continuum Theory of Plasticity by A. S. Khan and S. Huang, John Wiley and Sons, New York: New York, 1995. The subject of plasticity is lacking in texts that are directed at interpreting plastic deformation on the basis of the underlying mechanisms. This book provides an overview of much of the machinery that is invoked in current considerations of plasticity. Fracture ‘Mathematical Analysis in the Mechanics of Fracture’ by James R. Rice, from Vol. II of Fracture edited by G. Sih, Academic Press, New York: New York, 1968. Rice’s account of fracture remains, in my opinion, one of the deﬁnitive statements of many of the key ideas in the subject. Section E on Energy Variations and Associated Methods is especially pertinent to our discussion on conﬁgurational forces and gives an in depth application of these ideas in the fracture context. Dynamic Fracture Mechanics by L. B. Freund, Cambridge University Press, Cambridge: England, 1990. A careful account of many of the fundamental ideas of interest in the analysis of fracture with special reference to dynamics. Fracture of Brittle Solids by Brian Lawn, Cambridge University Press, Cambridge: England, 1993. I have found Lawn’s book quite readable and a useful place to become acquainted not only with much of the phenomenology of fracture, but also with some of the key ideas in that ﬁeld. Elementary Engineering Fracture Mechanics by D. Broek, Martinus Nijhoff

78

2 Continuum Mechanics Revisited

Publishers, The Hague: Holland, 1982. A readable account of many of the central ideas in the analysis of fracture.

The Finite Element Method The Finite Element Method by T. J. R. Hughes, Prentice Hall Inc., Englewood Cliffs: New Jersey, 1987. An exhaustive coverage of the mathematical formalism of ﬁnite elements. Computational Differential Equations by K. Eriksson, D. Estep, P. Hansbo and C. Johnson, Cambridge University Press, Cambridge: England, 1996. A wonderful book with many interesting historical sidelights that describes the numerical tools that arise in the solution of boundary value problems using continuum mechanics. A First Course in the Numerical Analysis of Differential Equations by A. Iserles, Cambridge University Press, Cambridge: England, 1996. This book, especially in the later chapters, treats many of the numerical issues of interest to those practicing ﬁnite elements. An Introduction to the Finite Element Method by J. N. Reddy, McGraw-Hill, New York: New York, 1993. A readable introduction to the conceptual foundations of the ﬁnite element method.

2.8 Problems

1 Deformation Gradient and Volume Change An additional insight into the signiﬁcance of the deformation gradient tensor can be gleaned by evaluating the scalar triple product of three noncoplanar vectors a, b and c both before and after a homogeneous deformation. In the undeformed conﬁguration, the vectors a, b and c span a region whose volume is given by a · (b × c). In the deformed conﬁguration, the transformed region has a volume given by Fa · (Fb × Fc). Show that the reference and deformed volumes are related by Fa · (Fb × Fc) = (det F)a · (b × c).

(2.108)

Interpret this result and demonstrate that for a pure shear there is no volume change.

2.8 Problems

79

2 Finite and Inﬁnitesimal Strains Consider a deformation mapping that is nothing more than a rigid rotation about the z-axis. First, explicitly write down the deformation mapping and then compute both the Green strain and the inﬁnitesimal strain tensors associated with this deformation mapping. In general, the inﬁnitesimal strains are nonzero. Why? 3 Cauchy Tetrahedron and Equilibrium In this problem, use the balance of linear momentum to deduce the Cauchy stress by writing down the equations of continuum dynamics for the tetrahedral volume element shown in ﬁg. 2.7. Assign an area S to the face of the tetrahedron with normal n and further denote the distance from the origin to this plane along the direction n by h. Show that the dynamical equations may be written as Dv V. (2.109) t(n) S + fV − t(e1 ) S1 − t(e2 ) S2 − t(e3 ) S3 − = ρ Dt Rewrite S1 , S2 , S3 and V in terms of S, h and the components of the vector n normal to S and then evaluate the limiting value of the expression given above as h → 0. Now, by adopting the convention that the traction vector on the i th Cartesian plane can be written as t(ei ) = σ ji e j ,

(2.110)

show that t(n) = σ n. 4 Isotropic Elasticity and Navier Equations Use the constitutive equation for an isotropic linear elastic solid given in eqn (2.54) in conjunction with the equilibrium equation of eqn (2.84), derive the Navier equations in both direct and indicial notation. Fourier transform these equations and verify eqn (2.88). 5 Elastic Green Function for an Isotropic Solid The elastic Green function is a useful tool in the analysis of a variety of problems in the elasticity of defects in solids. In this problem, we consider the various steps in the derivation of the elastic Green function for an inﬁnite, isotropic solid. In particular, ﬂesh out the details involved in the derivation of eqn (2.90) and carry out the Fourier inversion to obtain eqn (2.91).

80

2 Continuum Mechanics Revisited

6 Displacements for an Elastic Inclusion using the Method of Eigenstrains Consider a spherical inclusion characterized by an eigenstrain i∗j = δi j . (a) For an isotropic linear elastic solid, write the effective body forces associated with this eigenstrain. (b) Use the effective body force derived in part (a) in conjunction with eqn (2.96) to obtain an integral representation for the displacements due to the spherical inclusion. 7 Airy Stress Function and the Biharmonic Equation The biharmonic equation in many instances has an analogous role in continuum mechanics to that of Laplace’s equation in electrostatics. In the context of two-dimensional continuum mechanics, the biharmonic equation arises after introduction of a scalar potential known as the Airy stress function φ such that ∂ 2φ , ∂ x22 ∂ 2φ σ22 = 2 , ∂ x1 ∂ 2φ . σ12 = − ∂ x1 ∂ x2 σ11 =

(2.111) (2.112) (2.113)

Given this deﬁnition of the Airy stress function, show that the equilibrium equations are satisﬁed. The compatibility condition for inﬁnitesimal strains for planar problems may be written as ∂ 2 yy ∂ 2 x y ∂ 2 x x . (2.114) + = 2 ∂ y2 ∂x2 ∂ x∂ y Compatibility conditions address the fact that the various components of the strain tensor may not be stated independently since they are all related through the fact that they are derived as gradients of the displacement ﬁelds. Using the statement of compatibility given above, the constitutive equations for an isotropic linear elastic solid and the deﬁnition of the Airy stress function show that the compatibility condition given above, when written in terms of the Airy stress function, results in the biharmonic equation ∇ 4 φ = 0.

THREE

Quantum and Statistical Mechanics Revisited

3.1 Background In the previous chapter we examined the central tenets of continuum mechanics with an eye to how these ideas can be tailored to the modeling of the mechanical properties of materials. During our consideration of continuum mechanics, we found that one of the key features of any continuum theory is its reliance on some phenomenological constitutive model which is the vehicle whereby mechanistic and material speciﬁcity enter that theory. As was said before, the equations of continuum dynamics are by themselves a continuous representation of the balance of linear momentum and make no reference to the particulars of the material in question. It is the role of the constitutive model to inform the equations of continuum dynamics whether we are talking about the plastic deformation of metals or the washing of waves across a beach. A key realization rooted in the microscopic perspective is the idea that the constitutive response, used in the continuum settings described in the previous chapter, reﬂects a collective response on the part of the microscopic degrees of freedom. It is the business of quantum and statistical mechanics to calculate the average behavior that leads to this collective response. In addition to our interest in effective macroscopic behavior, one of our primary aims is to produce plausible microscopic insights into the mechanisms responsible for observed macroscopic behavior. For example, is there a microscopic explanation for the difference in the Young’s modulus of lead and silicon? Or, under what conditions might one expect to see creep mediated by grain boundary diffusion as opposed to bulk diffusion? Or, how does the yield strength depend upon the concentration of some alloying element? As noted above, microscopic modeling is founded upon the two complementary ediﬁces of quantum and statistical mechanics. From the present perspective, quantum mechanics allows us to capture the electronic origins of many of the internal energy differences that accompany processes central to the mechanics of 81

82

3 Quantum and Statistical Mechanics Revisited

materials. Similarly, statistical mechanics provides a venue within which it is possible to effect a quantitative treatment of the many degrees of freedom that conspire to yield observed macroscopic response. Our purpose in this chapter is to revisit some of the key ideas associated with these two disciplines, with emphasis on features of these theories that will ﬁnd their way into our later thinking.

3.2 Quantum Mechanics Quantum mechanics is the appropriate fundamental theory for describing phenomena ranging from bonding in fullerenes to superconductivity to the behavior of neutron stars. For our purposes, quantum mechanics should be seen in its role as the theory which describes the electronic origins of bonding in solids. In many cases, it is found that the very existence of solids is the result of a collective response on the part of the electronic degrees of freedom. In particular, the free energy is lower when the atoms conspire to form a solid than when they remain in isolation, and a key contribution to the total free energy arises from the electronic degrees of freedom. In the previous chapter, we noted that the principle of linear momentum balance leads to the central ‘governing equation’ of continuum mechanics. Similarly, within the context of nonrelativistic quantum mechanics, there is another such governing equation, namely that of Schr¨odinger. Though the conceptual origins of the Schr¨odinger equation are tied to a long and fascinating history, here we opt for the axiomatic approach in which the governing equation is asserted without derivation and is instead queried for its implications.

3.2.1 Background and Formalism Quantum mechanics represents one of the cornerstones of modern physics. Though there were a variety of different clues (such as the ultraviolet catastrophe associated with blackbody radiation, the low-temperature speciﬁc heats of solids, the photoelectric effect and the existence of discrete spectral lines) which each pointed towards quantum mechanics in its own way, we will focus on one of these threads, the so-called wave-particle duality, since this duality can at least point us in the direction of the Schr¨odinger equation. Though classical electromagnetic theory as embodied in Maxwell’s equations led to an interpretation of light in terms of waves, the photoelectric effect inspired Einstein to the view that in its interactions with matter, light might be better thought of from a corpuscular perspective. A complementary view of matter which took quantitative form in the hands of de Broglie was the contention that in some cases matter should be thought of in wave-like terms. In most naive

3.2 Quantum Mechanics

83

terms, the idea is that one should attribute a wavelength λ = h/ p to a particle with momentum p, where h is Planck’s constant. Indeed, the discovery that electrons form interference patterns provided further impetus towards the discovery of a mathematical description of these ‘matter waves’. Schr¨odinger was inspired by an analogy between classical mechanics and the ray theory of light, and hoped that a mechanics could be found that would stand in the same relation to wave optics that classical mechanics does to ray optics. The result of this inspiration is the famed Schr¨odinger equation. This equation determines the features of the electronic wave function, ψ(r). In turn, the wave function itself has a kinematic character and serves to characterize the ‘state’ of the system. A convenient analogy is that the wave function characterizes the state of a system within the quantum framework in a fashion that is analogous to the way that the coordinates and momenta characterize the state of a system within classical mechanics. Just as in classical descriptions, once the coordinates {qi , pi } are determined, all observables that depend upon those coordinates can be evaluated, so too in quantum mechanics, once the wave function is determined, there are well-deﬁned prescriptions for determining the expected values of quantities of interest. The interpretation of the wave function (here given in the one-dimensional setting, though the generalization to higher dimensions is clear) is that |ψ(x)|2 d x = ψ ∗ (x)ψ(x)d x is the probability that a particle will be found between x and x + d x. Note that we have introduced the notation ψ ∗ (x) which instructs us to use the complex conjugate of the wave function ψ(x). When written in time-independent form for a single particle interacting with a potential V (r), the Schr¨odinger equation takes the form −

h¯ 2 2 ∇ ψ(r) + V (r)ψ(r) = Eψ(r). 2m

(3.1)

The quantity E is the energy eigenvalue associated with a given wave function, while m is the mass of the particle of interest. In its role as the governing equation of quantum systems, the Schr¨odinger equation for a given problem amounts to the solution of a boundary value problem. Depending upon the nature of the potential V (r) that the particle experiences and the associated boundary conditions, one ﬁnds different solutions ψn (r) with associated stationary energy states, E n . Unlike the governing equations of continuum mechanics, these solutions involve a fundamental physical parameter with dimensions of action, namely, Planck’s constant, which is denoted here by h¯ = h/2π . Later we will see that Planck’s constant sets the energy scale of interest for many problems relating to electrons in solids. As noted above, the Schr¨odinger equation yields not only the electronic wave functions, but also the spectrum of energy eigenvalues E n which are available to the system. These eigenvalues, in turn, are the basis for the determination of the

84

3 Quantum and Statistical Mechanics Revisited

total energy of the system, whether it be an atom, a molecule or a solid. It is upon reckoning the relative distributions of eigenvalues for different conﬁgurations that we can construct a picture of why some conﬁgurations are more favorable than others. For example, if our aim is to determine the ground state geometry of a particular molecule, this question can be unambiguously answered by comparing the total energies of the geometric alternatives. The relation between a given classical Hamiltonian and its quantum counterpart depends upon the transcription between classical dynamical variables and certain operators that act upon the space of wave functions. The basic idea is to take the classical Hamiltonian, replace the relevant dynamical variables by their operator analogs, and then to solve the resulting differential equation, Hˆ ψ = Eψ.

(3.2)

This equation is a restatement of eqn (3.1) and we have introduced the notation that aˆabove a quantity signals that quantity as an operator. Note that we are considering the time-independent setting and for now have made reference only to a single particle. To make the classical–quantum transcription more complete, the recipe is to replace classical dynamical variables by their operator analogs according to p → −i h¯ ∇

(3.3)

r → r.

(3.4)

and

The Schr¨odinger equation corresponding to a given classical Hamiltonian is then obtained by replacing all of the dynamical variables in the original Hamiltonian with their operator analogs. With our realization that dynamical variables are represented as operators, we can also raise the question of how to compute observed quantities within the framework of quantum mechanics. The essential rule is that if we are interested ˆ p) when the system is in in obtaining the expectation value of the operator O(r, the state ψ, then this is evaluated as ˆ ˆ p) = ψ| O|ψ ˆ (3.5) O(r, = d 3 rψ ∗ (r) Oψ(r). Here we have introduced the bra (ψ|) and ket (|ψ) notation of Dirac which for us will serve as a shorthand way of representing certain integrals. This assertion is of special importance in our enterprise in the context of the energy for which the relevant expectation value may be written ˆ E = ψ| H |ψ = d 3 rψ ∗ (r) Hˆ ψ(r). (3.6)

3.2 Quantum Mechanics

85

Indeed, one sense in which this expression will be seen again is in its role as the basis of variational approximations for the wave function. Rather than solving for ψ itself, our idea will be to represent it as a linear combination of some set of basis functions, and to choose the coefﬁcients in the linear combination that minimize E. To explicitly solve a problem using the machinery of quantum mechanics, one speciﬁes the potential experienced by the particle within the Schr¨odinger equation which results in a corresponding boundary value problem. Upon solving this problem one ﬁnds the spectrum of allowed energy eigenvalues. The paradigmatic example of this program is the hydrogen atom, wherein one speciﬁes the Coulombic potential that characterizes the interaction between the nucleus and the electron and ﬁnds that the energy eigenvalues are consonant with the well-known Balmer formula of nineteenth century spectroscopy. In addition to the hydrogen problem, there are a variety of model problems that can also be solved analytically. For less tractable problems one can resort to perturbative treatments wherein more complicated potentials can be treated systematically. In the sections that follow, we undertake the solution of a few of these problems that are of particular interest in our attempt to build plausible models of material behavior. Not only will these models illustrate the fundamental concepts of quantum mechanics, but they will indeed prove useful in our quest to build models of materials. As a quick example to set notation and illustrate a few more points concerning formalism, we consider the problem of a single particle in a one-dimensional box. In this problem, the potential that acts on the particle is of the form 0 if 0 < x < a V (x) = (3.7) ∞ otherwise. If we like, we can think of this potential as the simplest model of the conﬁning effect of a free surface. The meaning of the potential is that the particle is ‘bound’ to the region 0 < x < a. As a result, all that we really need do is solve the equation −

h¯ 2 d 2 ψ = Eψ(x), 2m d x 2

(3.8)

subject to the boundary condition ψ(0) = ψ(a) = 0. These boundary conditions guarantee that the probability of ﬁnding the particle outside of the box is zero. By inspection, the solutions are of the form πnx 2 sin , (3.9) ψn (x) = a a a √ where the constant 2/a is chosen to guarantee that 0 |ψ(x)|2 d x is normalized to unity for reasons that we will see shortly and n is an integer that insures that

86

3 Quantum and Statistical Mechanics Revisited

Fig. 3.1. Ground state and ﬁrst excited state wave functions associated with particle in a box problem. The wave functions are drawn such that their zeroes correspond to the energy of the corresponding state.

the boundary conditions are satisﬁed. In addition to the wave functions, the energy eigenvalue corresponding to the n th wave function is En =

h¯ 2 π 2 n 2 . 2ma 2

(3.10)

The ground state and ﬁrst excited state wave functions for this problem are shown in ﬁg. 3.1. Each wave function has been plotted such that the zeroes of the wave function occur at the value on the vertical energy axis corresponding to that particular state. Thus, in the dimensionless units favored in the ﬁgure, ψ1 (x) has an energy E 1 = 1, while ψ2 (x) is associated with the energy E 2 = 4. As yet, our quick tour of quantum mechanics has featured the key ideas needed to examine the properties of systems involving only a single particle. However, if we are to generalize to the case in which we are asked to examine the quantum mechanics of more than one particle at a time, there is an additional idea that must supplement those introduced above, namely, the Pauli exclusion principle. This principle is at the heart of the regularities present in the periodic table. Though there are a number of different ways of stating the exclusion principle, we state it in words as the edict that no two particles may occupy the same quantum state. This principle applies to the subclass of particles known as fermions and characterized by half-integer spin. In the context of our one-dimensional particle in a box problem presented above, what the Pauli principle tells us is that if we wish to

3.2 Quantum Mechanics

87

put two electrons in the box, then in reckoning the total energy we say that one of the particles occupies the ground state and the second occupies the ﬁrst excited state with a resulting total energy E tot = E 1 + E 2 = 5, where the energy is written in the dimensionless units already introduced in ﬁg. 3.1. We confess to ignoring the extra subtleties associated with an explicit inclusion of spin.

3.2.2 Catalog of Important Solutions The solutions to a few different problems within the quantum mechanical setting will serve as the backdrop for many of the models of materials that will be set forth in later chapters. The quantum mechanical oscillator will serve as our jumping off point for the analysis of the thermodynamics of solids, while the solution to the problem of the hydrogen atom will give us a basis within which to discuss bonding in solids. Consequently, we take up the solution of these problems presently. Harmonic Oscillator. One exercise that proves central to modeling the thermal properties of materials is that of a particle bounded by a quadratic potential well. Our interest in the harmonic oscillator arises from the following observation. The particles that make up an N -atom solid may be thought of as spanning a 3N -dimensional conﬁguration space with the potential energy of interaction given by U (x 1 , x2 , . . . , x3N ). This function gives the potential energy of a given atomic conﬁguration, and regardless of the exact details of the potential energy surface, one may imagine representing this surface in the vicinity of points of equilibrium in terms of a collection of quadratic wells. It is on this basis that the harmonic oscillator serves as a jumping off point for an analysis of the vibrations of solids and reveals itself as of special interest to the modeling of materials. In anticipation of our use of this model in chaps. 5 and 6, we recount the quantum mechanical treatment of a particle in a quadratic potential. For the case of the one-dimensional harmonic oscillator the potential energy is given by V (x) = 12 kx 2 , which is parameterized in terms of a stiffness constant k. After some manipulation, the Schr¨odinger equation associated with this potential may be written as d 2ψ + (α − βx 2 )ψ = 0, dx2

(3.11)

where α = 2m E/h¯ 2 and β = m 2 ω2 /h¯ 2 , and with the constant ω2 = k/m corresponding to the classical frequency of vibration. Equations of this generic form suggest a rescaling of the variables motivated by the attempt to isolate the term quadratic in x. In particular, this equation can be further simpliﬁed if we 1 make the change of variables y = β 4 x which results in a restatement of the original

88

3 Quantum and Statistical Mechanics Revisited

Schr¨odinger equation in terms of natural coordinates as 2E d 2φ 2 − y φ = 0, + h¯ ω dy 2

(3.12)

where we have deﬁned a new function φ(y) which reﬂects the change of variables. 2 Asymptotic analysis suggests a trial solution of the form φ(y) = f (y)e−y /2 . 2 This form is suggested by the fact that e−y /2 satisfactorily describes the large-y behavior of the solution, namely, that the particle is bound within the quadratic well. Substitution of this trial solution into the original differential equation results in an auxiliary equation for the unknown function f (y). In particular, we ﬁnd 2E − 1 f (y) = 0. (3.13) f (y) − 2y f (y) + h¯ ω The details of the solution to this equation are of less immediate interest to us than the nature of the solutions themselves. Sufﬁce it to note that this equation admits of a solution in power series form, and that these solutions guarantee the vanishing of the wave function as y → ∞ only if the series is truncated after a ﬁnite number of terms. This large y boundary condition meets with our intuition that the solutions must ultimately vanish at large distances. That is, we expect the particle to be bound by the oscillator potential. The polynomials that result upon truncating the series are the so-called Hermite polynomials. Our requirement that the series solution be truncated after a ﬁnite number of terms is imposed by insisting that 2E = 2n + 1, (3.14) h¯ ω where n is an integer. Imposition of the boundary condition results in quantization of the allowed energy levels which can be labeled as E n = (n + 12 )h¯ ω. Note that even for the ground state (n = 0), the energy is nonzero (the so-called zero point energy). The wave functions that are associated with these various energies are themselves labeled by the integer n (n is known as a quantum number) and can be written as 1 mω 4 − mωx 2 1 mω 2h¯ H e x , (3.15) ψn (x) = n n 1 h¯ 2 2 (n!) 2 π h¯ where Hn (x) is a Hermite polynomial of order n. The ﬁrst few eigenfunctions and their associated energy levels are indicated schematically in ﬁg. 3.2. One of the key observations concerning our solution is that the probability of ﬁnding a particle in the classically forbidden region is nonzero. For example, if we consider the state labeled by n = 0, the maximum classical amplitude of vibration is given by equating the ﬁxed total energy, namely 12 h¯ ω, and the

3.2 Quantum Mechanics

89

Fig. 3.2. Schematic illustrating the harmonic oscillator potential and the associated wave functions. The wave functions are plotted such that the zeroes of ψi (x) intersect the energy axis at that energy corresponding to the energy of the i th state. 2 classical expression for the energy, which is given by 12 mω2 xmax , where xmax is the maximum displacement. This operation implies a maximum classical amplitude √ of vibration of x max = h¯ /mω. As is evident from the ﬁgure, the wave function bleeds out of the classical region with nonzero amplitude even at values of x in excess of the classical turning point. Many of the features of nonrelativistic quantum mechanics have revealed themselves in this problem. First, we have seen that as a result of imposition of the boundary conditions the allowed energy states are discrete. Secondly, we note a progression of associated wave functions, those tied to higher energies having more nodes, and all of which allow the particle to penetrate into the classically forbidden region. For the harmonic oscillator in particular, we have found a series of equally spaced energy levels that will loom important in our quest to understand the entropy of vibration of crystalline solids. In fact, when we undertake our analysis of the thermal motions of crystals, we will need exactly the spectrum of eigenvalues we have uncovered in examining what may at ﬁrst blush seem an unduly artiﬁcial example.

The Hydrogen Atom. The hydrogen atom is the problem against which many other models are measured. In confronting a new subject, often one seeks the ‘hydrogen atom’ of that ﬁeld, that is, the illustrative example that at once contains sufﬁcient complexity to capture the key ingredients of the problem without at the same time exacting too high an analytic toll. In this section our aim is to highlight the key features of the quantum mechanical investigation of the hydrogen atom. Our reason for doing so is derived in part from the fact that in attempting to build up models of the bonding in solids, we will ﬁnd ourselves appealing repeatedly to the

90

3 Quantum and Statistical Mechanics Revisited

hydrogenic wave functions to build intuition concerning the interactions between neighboring atoms. As with the harmonic oscillator, our starting point is the Schr¨odinger equation itself. In this case, the equation may be written in the form −

h¯ 2 2 ∇ ψ(r) + V (|r|)ψ(r) = Eψ(r), 2m

(3.16)

where for the moment we have speciﬁed the potential only to the extent that we note it is of the central force form. There is virtue in continuing our analysis in generic terms without yet specifying which central potential will be of interest, though we will do well to anticipate our eventual appeal to the special case of the Coulomb potential pertinent to the hydrogen atom. There are a number of ways to proceed at this point, and we will pursue the classic description in terms of the solution to a differential equation. By virtue of the presumed spherical symmetry of this problem, we carry out a separation of variables, with the result that the radial and angular terms are decoupled. This may be seen by starting with the Laplacian operator in spherical coordinates which leads to a Schr¨odinger equation of the form,

1 ∂ ∂ 1 ∂2 h¯ 2 1 ∂ 2 ∂ r + 2 sin θ + ψ(r) − 2m r 2 ∂r ∂r r sin θ ∂θ ∂θ r 2 sin2 θ ∂φ 2 + [V (|r|) − E]ψ(r) = 0. (3.17) We now seek a solution of the form ψ(r, θ, φ) = R(r )Y (θ, φ) which may be inserted into the equation above. Upon so doing and after the requisite reorganization of terms, we ﬁnd that our problem is reduced to

∂Y 1 h¯ 2 1 1 ∂ ∂ 2Y −h¯ 2 1 ∂ 2∂R 2 r +r [V (r )−E] = sin θ + . 2m R ∂r ∂r 2m Y sin θ ∂θ ∂θ Y sin2 θ ∂φ 2 (3.18) The result is an equation in which one side depends upon one set of variables while the other side depends upon a different set of variables and leads us to conclude that both sides are equal to a constant which, with feigned insight, we call l(l + 1). We now further assume that the angular solution may be factored into the form, Y (θ, φ) = P(θ)u(φ). Substituting this solution into the angular equation results once again in a decoupling of the θ and φ dependence and a second separation constant, namely, 1 d 2u dP sin θ d − sin θ + l(l + 1) sin2 θ = m 2 . = (3.19) u dφ 2 P dθ dθ As a result of these manipulations, the problem of solving the Schr¨odinger equation

3.2 Quantum Mechanics

91

for a particle in the presence of a central force potential has been reduced to the solution of three ordinary differential equations which may be written as

and

d 2u = −m 2 u, dφ 2

(3.20)

dP m2 1 d sin θ + l(l + 1)P − 2 P = 0, sin θ dθ dθ sin θ

(3.21)

d R 2mr 2 d2 R + 2 [E − V (r )] − l(l + 1) = 0. + 2r dr 2 dr h¯

(3.22)

and r2

The φ equation is routine and has solutions of the form u(φ) = eimφ . The requirement of periodicity of the wave function, namely that u(φ) = u(φ + 2π), restricts m to integer values. The θ equation is simpliﬁed by making the change of variables z = cos θ, resulting in the associated Legendre equation

2 m2 dF 2 d F (1 − z ) 2 − 2z F = 0, (3.23) + l(l + 1) − dz dz 1 − z2 which can be tackled via series solution. Rather than examining the strategy for solving the equation, we merely quote the solutions and attempt to learn something of their nature and signiﬁcance. The general solution to the associated Legendre equation may be written in the form F(z) = a Plm (z) + bQ lm (z), where the functions Plm (z) and Q lm (z) are known as associated Legendre polynomials. The solution Q lm (z) is rejected on the grounds that it is singular when z = ±1, and hence we keep only the Plm s. The compositions of the solutions to the θ and φ equations, by virtue of their relevance to all problems with spherical symmetry, are so important as to merit a special name, the spherical harmonics. These solutions bear the same relation to spherical problems that the Bessel functions do to those with cylindrical symmetry. The spherical harmonics, Ylm (θ, φ), may be written as Ylm (θ, φ) = Plm (cos θ)eimφ .

(3.24)

In the present context, their importance attaches to their role in describing the angular dependence of the hydrogenic wave functions. When we take up bonding in solids, we will see that the angular character implied by the spherical harmonics makes itself known in macroscopic observables as fundamental as those of the elastic moduli. We now take up the speciﬁc nature of the radial wave function. From eqn (3.18), we see that to make further progress requires the speciﬁcation of a particular form for V (r ). For the case of the hydrogen atom, V (r ) is of

92

3 Quantum and Statistical Mechanics Revisited

the Coulomb form. A choice must be made with regard to units in treating the electrostatic interaction, and we adopt the esu units within which the Coulomb potential is of the form V (r ) = e2 /r and results in a radial equation of the form

2 e2 h¯ 2l(l + 1) d R 2mr 2 2d R R = 0. (3.25) + 2 E+ − + 2r r dr 2 dr r 2mr 2 h¯ The radial equation can be further simpliﬁed into a recognizable form if one makes the substitution f (r ) = r R(r ), leading to

d2 f e2 l(l + 1) 2m f = 0. (3.26) − f + 2 E+ dr 2 r2 r h¯ What we have succeeded in doing is to rework the radial equation into exactly the form of a one-dimensional Schr¨odinger equation in the presence of an effective potential e2 h¯ 2 l(l + 1) . (3.27) + r 2m r 2 As in our analysis of the θ equation, rather than bothering with the niceties of solving this radial equation, we will quote its solutions and consider their signiﬁcance. The strategy that is adopted in solving this equation is in many respects similar to that used in solving the problem of the harmonic oscillator. One assumes on the basis of asymptotics that the solution may be written as a product of a term of the form e−βr and some as yet undetermined function. What results is a new differential equation, analogous to the Hermite differential equation we confronted in solving the harmonic oscillator, and this equation may be solved in terms of special functions known as the associated Laguerre polynomials, which depend upon the quantum numbers n and l and result in a radial wave function of the form r l 2l+1 2r −r/na0 . (3.28) L n−l−1 Rnl (r ) = e na0 na0 Veff (r ) = −

Here we have denoted the associated Laguerre polynomials as L 2l+1 n−l−1 . A few of these radial functions are shown in ﬁg. 3.3. In anticipation of the fact that we will later invoke hydrogen-like orbitals in the context of our discussion of electronic structure in chap. 4, we note that it is conventional to label orbitals using both their principal quantum number, n, and their orbital angular momentum number l. In particular, a hierarchy of states at a given n is built running from l = 0 to l = n − 1. For example, for n = 4 we have 4s, 4p, 4d and 4f states, where l = 0 is labeled s, l = 1 is labeled p, l = 2 is labeled d and l = 3 is labeled f. Like in the case of the harmonic oscillator, our insistence that the wave functions be bounded for large-r forces a truncation of the series in the form of

3.2 Quantum Mechanics

93

Fig. 3.3. Radial probability distributions for various low-lying states of hydrogen (adapted from Condon and Shortley (1935)).

polynomials. Further, this condition that the wave functions vanish at inﬁnity imposes restrictions on the allowed values of the energy which are En = −

me4 , 2h¯ 2 n 2

(3.29)

where n assumes only integral values. We note that the energies depend only upon the principal quantum number n. The implication of this result is that the various states of different angular momenta (labeled by l and m) are degenerate. In

94

3 Quantum and Statistical Mechanics Revisited

numerical form, the series of energy states introduced above is of the form 13.6 eV, (3.30) n2 providing a clear idea of the energy scale associated with problems of this type. We have found that the generic hydrogenic wave function takes the form En ≈ −

ψnlm (r) = Rnl (r )Ylm (θ, φ),

(3.31)

with associated energy eigenvalues of the form given in eqn (3.29). This solution will prove of great utility in our later development of the linear combination of atomic orbitals (or tight-binding) method.

3.2.3 Finite Elements and Schr¨odinger Recall from chap. 2 that often in the solution of differential equations, useful strategies are constructed on the basis of the weak form of the governing equation of interest in which a differential equation is replaced by an integral statement of the same governing principle. In the previous chapter, we described the ﬁnite element method, with special reference to the theory of linear elasticity, and we showed how a weak statement of the equilibrium equations could be constructed. In the present section, we wish to exploit such thinking within the context of the Schr¨odinger equation, with special reference to the problem of the particle in a box considered above and its two-dimensional generalization to the problem of a quantum corral. Our preliminary exercise will state the problem in one dimension, with the generalization to follow shortly. The one-dimensional Schr¨odinger equation may be written h¯ 2 d 2 ψ + V (x)ψ = Eψ. (3.32) − 2m d x 2 In the present case, the weak form is obtained by multiplying eqn (3.32) by some test function and integrating the ﬁrst term by parts. For the purposes of concreteness in the present setting, we imagine a problem for which the domain of interest runs from the origin to point x = a, and for which the wave functions vanish at the boundaries. We note that the Schr¨odinger equation could have been stated alternatively as the Euler–Lagrange equation for the functional a a h¯ 2 a dψ 2 2 dx + V (x)|ψ(x)| d x − E |ψ(x)|2 d x. (3.33) [ψ(x)] = 2m 0 d x 0 0 The ﬁnite element strategy is to replace this functional with a function of the N unknown values ψn (not to be confused with wave functions related to the hydrogen

3.2 Quantum Mechanics

95

atom from the previous section) of the wave function at the nodes of the ﬁnite element mesh. That is, we imagine a discretization of the region [0, a] by N distinct points which are taken to be the nodes of the ﬁnite element mesh. The problem of solving the Schr¨odinger equation then becomes one of determining not the entire function ψ(x), but rather for the values of ψ (i.e. ψn ) at the nodal positions, with the understanding that the value of the wave function at points between the nodes is obtained by ﬁnite element interpolation. Speciﬁcally, as with our earlier treatment of the ﬁnite element method, we imagine shape functions Ni (x) centered at each node, with the subscript i labeling the node of interest. It is then asserted that the wave function is given as ψ(x) =

N

ψn Nn (x),

(3.34)

n=1

and similarly the potential (which is known) is expanded in terms of the shape functions via N V (x) = Vn Nn (x). (3.35) n=1

What this means is that to write down the interpolated potential V (x), we ﬁnd the values of the potential at the nodes, Vn = V (xn ) and interpolate elsewhere using eqn (3.35). By virtue of the ﬁnite element ansatz, we may now effect a mapping between the functional [ψ(x)] and the function ({ψn }). In particular, upon substituting ψ(x) and V (x) from eqs (3.34) and (3.35) into eqn (3.33) and simplifying to the case in which we drop all reference to the fact that the wave function can be complex rather than real, we have h¯ 2 a d Ni (x) d N j (x) [ψ(x)] → ({ψn }) = dx ψi ψ j 2m i j 0 dx dx a Vk ψi ψ j Ni (x)N j (x)Nk (x)d x + i

−E

j

0

k

i

j

a

ψi ψ j Ni (x)N j (x)d x. 0

This result may be simpliﬁed considerably if we invoke the deﬁnitions h¯ 2 a d Ni (x) d N j (x) d x, Ki j = 2m 0 dx dx a Vi j = Vk Ni (x)N j (x)Nk (x)d x, k

0

(3.36)

96

3 Quantum and Statistical Mechanics Revisited

Mi j =

a

Ni (x)N j (x)d x. 0

Note that these matrices are functions only of known quantities, namely, the potential V (x) and the shape functions N (x). It is convenient to further simplify by introducing Hi j = K i j + Vi j , with the result that the function of interest is [Hi j − E Mi j ]ψi ψ j . (3.37) ({ψn }) = ij

At this point, we need to implement our original variational statement by seeking those ψn s that minimize the function ({ψn }). Imposition of this condition via ∂ = 0, ∂ψn results in the reformulation of the original problem as [Hn j − E Mn j ]ψ j = 0.

(3.38)

(3.39)

j

As a speciﬁc realization of these ideas, consider the celebrated problem of the one-dimensional particle in a box already introduced earlier in the chapter. Our ambition is to examine this problem from the perspective of the ﬁnite element machinery introduced above. The problem is posed as follows. A particle is conﬁned to the region between 0 and a with the proviso that within the well the potential V (x) vanishes. In addition, we assert the boundary condition that the wave function vanishes at the boundaries (i.e. ψ(0) = ψ(a) = 0). In this case, the Schr¨odinger equation is d 2 ψ(x) 2m E + 2 ψ(x) = 0. (3.40) dx2 h¯ We are searching for the wave functions and associated energy eigenvalues. From an analytic perspective, this problem is entirely routine with the result that the n th eigenfunction is of the form given in eqn (3.9) and the corresponding eigenvalues as given in eqn (3.10). Our objective is to see to what extent we can recover these results using the ﬁnite element method. Further, the relevant ﬁnite element analysis can be carried out almost entirely by hand. We imagine discretizing the region between 0 and a with N + 1 nodes as illustrated in ﬁg. 3.4. The representation of the wave function is now restricted entirely to the values of the wave function at the nodes, ψi , with the value between nodes determined by interpolation via ψ(x) = i ψi Ni (x). The particular choices of shape functions used in the present analysis are shown in ﬁg. 3.4 as well. Because of the fact that the shape functions are highly localized, the matrices K i j and Mi j introduced above will be nonzero only for the cases in which j = i or

3.2 Quantum Mechanics

97

Fig. 3.4. Schematic illustration of the nodes used to discretize the particle in a box problem and the corresponding ﬁnite element shape functions.

j = i ± 1. For a given level of approximation (as represented by the number of elements used in the analysis), the solution of the Schr¨odinger equation has been reduced to the construction of the matrix Hi j − E Mi j and the determination of the associated energy eigenvalues. In abstract terms, the relevant matrix elements may be evaluated as follows. Consider the case in which there are N + 1 nodes as shown in ﬁg. 3.4. First, we note that since within the region of interest there is no potential V (x), Hi j = K i j . The matrix element K ii is found as xi

xi + a N d Nil (x) 2 d Nir (x) 2 h¯ 2 dx + dx , (3.41) K ii = 2m xi − Na dx dx xi where we have introduced the notation Nir (x) to represent the shape function facing to the right of the i th node and Nil (x) to represent the shape function facing to the left of the i th node. These shape functions are written as N (xi − x) + 1, a N Nil (x) = (x − xi ) + 1, a

Nir (x) =

(3.42) (3.43)

and are characterized by the property that Ni (x j ) = δi j . In light of these deﬁnitions, the integrals in eqn (3.41) may be evaluated with the result K ii =

h¯ 2 N . ma

(3.44)

In a similar way, the matrix element K i,i+1 (which by symmetry is equal to K i,i−1 ) may be written as a l (x) h¯ 2 xi + N d Nir (x) d Ni+1 d x. (3.45) K i,i+1 = 2m xi dx dx The region of integration is determined by the fact that the only nonzero overlap between the i th and (i + 1)th shape functions is in the element sharing the i th and

98

3 Quantum and Statistical Mechanics Revisited

(i + 1)th nodes which is the region between xi and xi + a/N . Again, in light of the deﬁnition of the shape functions, it is easily shown that K i,i±1 = −

h¯ 2 N . 2ma

(3.46)

We also require the various matrix elements of the form Mi j which reﬂect the overlap of adjacent shape functions. The diagonal matrix elements may be written as xi xi + a N l 2 Mii = [Ni (x)] d x + [Nir (x)]2 d x. (3.47) xi − Na

xi

Performing the requisite integrals results in Mii =

2a . 3N

Similarly, the off-diagonal matrix elements may be written xi + a N l Nir (x)Ni+1 (x)d x, Mi,i+1 =

(3.48)

(3.49)

xi

with the result Mi,i±1 =

a . 6N

(3.50)

Once the various matrix elements are in hand, we can now search for the eigenvalues associated with a given ﬁnite element approximation. As a starting point, consider the case N = 2 in which there is only a single unconstrained nodal degree of freedom. In this case, the matrix of eqn (3.39) reduces to (K 11 − E M11 )ψ1 = 0. As a result, we see that our ﬁrst approximation to the ground state energy for the particle in the box is given by E 1(N =2) = K 11 /M11 = 6h¯ 2 /ma 2 . At the next level of approximation, we consider the case in which N = 3. If we adopt the notation that K ii = α and Mi,i±1 = β, then K i,i±1 = −α/2 and Mii = 4β. For the case N = 3, therefore, the resulting condition for the eigenvalues is α α − 4Eβ − − Eβ 2 = 0. (3.51) det α − − Eβ α − 4Eβ 2 The resulting energy eigenvalues are E 1(N =3) = α/10β and E 2(N =3) = α/2β and are represented in terms of h¯ 2 /2ma 2 in table 3.1, as are increasing levels of approximation. The act of taking our analysis to the next level of approximation (i.e. the use of more elements) requires neither further physical nor mathematical

3.2 Quantum Mechanics

99

Table 3.1. Eigenvalues associated with ﬁnite element approximation to solutions for Schr¨odinger equation for a particle in a one-dimensional box. Energies are reported in units of h¯ 2 /2ma 2 . Approximation

E1

E2

E3

E4

N =2 N =3 N =4 N =5 Exact

6.000 5.400 5.098 5.048 4.935

27.000 22.44 21.6 19.739

58.057 54.0 44.415

113.91 108.0 78.896

elaboration. The generic form of the secular equation, the roots of which are the energy eigenvalues, is tridiagonal and takes the form α 0 0 ··· 0 α − 4Eβ − − Eβ 2 α α 0 ··· 0 − − Eβ α − 4Eβ − − Eβ 2 2 α α ··· 0 0 − − Eβ α − 4Eβ − − Eβ 2 2 det .. .. .. .. .. .. . . . . . . . . . . α .. .. .. .. ··· − − Eβ 2 α 0 0 0 ··· − − Eβ α − 4Eβ 2 = 0.

(3.52)

The fact that the matrix is nonzero only in a strip near the main diagonal is an immediate consequence of the locality of the shape functions which implies that the overlap between different shape functions vanishes except in the case of neighboring elements. The result of carrying out calculations with increasing numbers of elements are summarized in table 3.1, and give a feel for the rate of convergence of the results. In addition to questions concerning the distribution of energy eigenvalues for this problem, we can also demand the implications of our ﬁnite element analysis for the wave functions. As a result of our knowledge of the energy eigenvalues, eqn (3.39) can be exploited to determine the wave functions themselves. By substituting the eigenvalues into these coupled equations, we can then solve for the corresponding ψi s. The simplest realization of this program is for the case N = 2 introduced above in which there is only a single free nodal degree of freedom. In this case, the value of ψ1 is determined entirely by the constraint of normalization. That is, we

100

3 Quantum and Statistical Mechanics Revisited

Fig. 3.5. Illustration of the ﬁnite element interpolated approximate wave functions: (a) ground state wave function for the N = 2 approximation; (b) ground state and ﬁrst excited state wave functions for the N = 3 approximation.

require that we have

a 0

ψ 2 (x)d x = 1. In this case, because of ﬁnite element interpolation, a 2 if x ≤ ψ1 x a 2 . ψ1(N =2) (x) = a 2 if x > ψ1 2 − x a 2

(3.53)

Our notation ψm(N =P) (x) indicates the m th eigenstate associated with the ﬁnite element approximation in which N = P. In the case above, the constraint of √ normalization requires that ψ1 = 3/a. The ground state wave function as obtained from our N = 2 approximation is illustrated in ﬁg. 3.5. A more instructive example of the ﬁnite element approximation to the wave function is provided by the case N = 3. In this case, by substituting the values of the energy eigenvalues back into eqn (3.39), we obtain equations for determining the ratio ψ1 /ψ2 . In particular, we ﬁnd that ψ1 K 12 − E M12 =− . ψ2 K 11 − E M11

(3.54)

For the ground state energy, this results in ψ1 /ψ2 = 1 while for the ﬁrst excited state we have ψ1 /ψ2 = −1. Again, in conjunction with the requirement that the

3.2 Quantum Mechanics

101

Fig. 3.6. Successive steps in the construction of a quantum corral using the tip of a scanning tunneling microscope (courtesy of D. Eigler).

wave functions be normalized, ψ1 and ψ2 can be unambiguously determined, with the result being shown in ﬁg. 3.5.

3.2.4 Quantum Corrals: A Finite Element Analysis Quantum mechanics is a subject that is well endowed with a series of enlightening schoolboy exercises. However, one of the fascinating features that has accompanied the attainment of atomic-level experimental probes is the ability to carry out experiments that attempt to mimic these very same problems. In this section we will examine the issues surrounding the solution of the problem of the ‘quantum corral’, in which a series of atoms are brought together on a crystal surface into a closed circular conﬁguration. The presence of these surface atoms has the effect in turn of conﬁning electrons, the states of which can be probed experimentally using scanning tunneling microscopy. In ﬁg. 3.6 a sequence of images is shown that represents the stages in constructing the quantum corral itself. From the standpoint of the Schr¨odinger equation, this is another example of a ‘particle in a box’ problem which in this case is effectively two-dimensional. In particular, the potential within the corral region is assumed to be zero, while the

102

3 Quantum and Statistical Mechanics Revisited

ring of atoms at the boundary is treated in the model as the source of an inﬁnite potential barrier. The inﬁnite barrier is translated into a boundary condition for the wave function at the boundary of the corral (r = a), namely, ψ(a, θ ) = 0. We begin by writing the Schr¨odinger equation in polar coordinates, 1 ∂2 1 ∂ h¯ 2 ∂ 2 (3.55) + 2 2 ψ(r, θ ) = Eψ(r, θ ), + − 2m ∂r 2 r ∂r r ∂θ and immediately attempt a solution in the separated form, ψ(r, θ ) = R(r )u(θ ). The differential equation can then be rearranged into two terms, one of which depends only upon r while the other depends only upon θ . As we noted in the case of the hydrogen atom, the equality of two independent functions to one another implies that both must, in turn, be equal to a constant which we denote m 2 in anticipation of the resulting differential equation. As a result of our separation of variables strategy, the problem of solving the Schr¨odinger equation for the quantum corral is reduced to that of solving two ordinary differential equations. In particular, we have 2m E d2 R 1 d R n2 + + − R = 0, (3.56) dr 2 r dr r2 h¯ 2 and d 2u + m 2 u = 0. (3.57) dθ 2 The r equation can be massaged into the form of a Bessel equation while the θ equation is elementary. As a result of these insights, the solution may be written as Jn ( 2m E/h¯ 2 r )eimθ . It now remains to impose our boundary conditions. We require that the solution be periodic in the angular coordinate, which implies that m is restricted to integer values, and that the wave function vanish when r = a. This second condition means that 2m E nl a = z nl , (3.58) h¯ 2 where z nl is the l th zero of the n th Bessel function. We see that each energy eigenvalue E nl is labeled by two quantum numbers, n and l. A more interesting perspective on the quantum corral problem is garnered from a ﬁnite element analysis. Since we have already carried through a detailed implementation of the ﬁnite element strategy with regard to the one-dimensional particle in a box, here we only note the salient features of the problem. To illustrate the character of two-dimensional ﬁnite elements, the circular region over which the solution is sought is discretized into a series of ﬁnite elements. An example of the type of mesh that is generated is shown in ﬁg. 3.7. We should also note

3.2 Quantum Mechanics

103

Fig. 3.7. Finite element mesh used to compute the eigenstates of the quantum corral (courtesy of Harley Johnson).

that a full two-dimensional treatment of this problem is an overkill since, as was already shown, the original problem can be reduced to the search for solutions of a one-dimensional radial equation. On the other hand, the two-dimensional solution is enlightening from the ﬁnite element perspective. As with the one-dimensional case described earlier, the unknowns are the nodal values of the wave function, ψn . To determine the wave functions between nodes, ﬁnite element interpolation is used, in this case with the relevant shape functions taking the form of triangular sheets such that the value of the shape function is 1 at one of the three nodes making up a given triangle, and 0 at the other two nodes and varying linearly in between. Once again, the Hamiltonian matrix is constructed and the resulting secular equation is solved with the result being a series of eigenvalues. In addition, the nodal values of the wave functions associated with the various states are determined as a result of this analysis, and two of the ﬁnite element wave functions are shown in ﬁg. 3.8. 3.2.5 Metals and the Electron Gas So far, our quantum mechanics examples have been rather far aﬁeld from questions of immediate interest to our study of solids. In particular, we aim to see what light quantum mechanics sheds on the origin of bonding and cohesion in solids. To do so, in this introductory chapter we consider two opposite extremes. Presently, we consider the limit in which each atom is imagined to donate one or more electrons to the solid which are then distributed throughout the solid. The resulting model is the so-called electron gas model and will be returned to repeatedly in coming

104

3 Quantum and Statistical Mechanics Revisited

Fig. 3.8. Two different eigenfunctions for the quantum corral as obtained by using a two-dimensional ﬁnite element calculation (courtesy of Harley Johnson).

chapters. The other limit that will be considered in the next section is that in which it is imagined that the formation of the solid results in a small overlap between the atomic orbitals associated with different atoms. This picture will lead to the so-called tight-binding method (or linear combination of atomic orbitals). With our interest in the bonding of solids, we undertake an analysis of the electron gas, which in simplest terms is nothing more than a three-dimensional version of the particle in a box problem which we have already seen in both its one- and two-dimensional guises. Here the physical idea is that some subset of electrons is donated from some host atoms such as sodium or aluminum, and can be thought of as being distributed within a box, with the only conﬁning potential they experience arising from the presence of the boundaries of the solid themselves. In addition, for the time being we advance the assumption that the positive charge associated with the ions is distributed uniformly so as to guarantee charge neutrality. This approximation is the basis of the free electron theory of metals. However, in considering this idealized model, we are immediately confronted with one of the intriguing paradoxes of the electronic theory of solids, namely, the surprising efﬁcacy of independent particle models. Note that we have said nothing of the interactions between electrons. We will revisit this conundrum in later chapters, while for now maintaining our assumption that the electrons behave as though they are independent. Within the model of a metal proposed above, the Schr¨odinger equation becomes −

h¯ 2 2 ∇ ψ(r ) = Eψ(r ), 2m

(3.59)

3.2 Quantum Mechanics

105

with the additional proviso that the wave functions satisfy boundary conditions to be elaborated below. The solution in this is immediate and is seen to take the √ case ik·r familiar plane wave form, ψ(r) = (1/ )e . Here we have adopted the notation box. This factor appears in the = L 3 , where L is the edge length of the conﬁning wave function as a result of our demand that |ψ(r)|2 d 3 r = 1, a normalization condition. Note that in light of our probabilistic interpretation of the wave function, we see that the electron can be thought of as uniformly spread out throughout the conﬁning box. Associated with a plane wave characterized by a wavevector k, is an energy eigenvalue given by E k = h¯ 2 k 2 /2m. Note that the dependence of the energy on the wavevector k is isotropic. The choice of a ﬁnite-sized box imposes restrictions on the allowed values of the wavevector. In particular, if we impose periodic boundary conditions of the form ψ(x, y, z) = ψ(x + L , y, z), we ﬁnd that the wavevectors can only take the values ki = 2πm i /L, where m i is an integer. Note that we could just as well have chosen boundary conditions in which the wave functions vanish at the boundary, with no change in our conclusions concerning the energetics of the electron gas. If we wish to characterize these eigenvalues geometrically it is convenient to think of a discrete lattice of allowable points in ‘k-space’. Each set of integers (m 1 , m 2 , m 3 ) labels a point in this space and is tied to a particular energy eigenvalue Em1m2m3 =

2π 2 h¯ 2 2 (m 1 + m 22 + m 23 ). m L2

(3.60)

The set of allowed points in k-space is depicted schematically in ﬁg. 3.9. The isotropy of the energy spectrum implies a wide range of degeneracies which are of interest as we ﬁll these states. To probe the implications of our solution, we now need to implement the Pauli principle described earlier. The goal is to assign to the various energy states their relevant occupancies, that is, how many electrons are to be assigned to each state? The Pauli principle demands that only one electron be assigned to each state (or two electrons for each k-vector if we acknowledge the two possible states of spin). This requirement is tied at a deeper level to the existence of certain symmetry requirements for the electronic wave function. For the case of electrons (fermions), one insists that the electron wave function be antisymmetric. In the context of our problem, this demand is equivalent to the assertion that only one electron be allowed to occupy each energy state. The prescription that emerges for computing the total electronic energy of our system, then, is to sum up the energies associated with the lowest eigenvalues, until all of the electrons have been suitably assigned to an associated energy. For the sake of concreteness, we assume that the conﬁning box has cube edges of dimension L. Further, we assume that N atoms occupy this box and that each has

106

3 Quantum and Statistical Mechanics Revisited

Fig. 3.9. Depiction of allowed k-points associated with energy eigenvalues for particle in a threedimensional box. The series of k-points shown in the ﬁgure are those in the positive octant of k-space falling within a spherical shell of such k-points.

donated a single valence electron which results in an electron density ρ = N /L 3 . The total electronic energy in our noninteracting electron model can then be found N by evaluating the discrete sum over the energy eigenvalues (i.e. 2 i=1 E i , where the energies are rank ordered E 1 < E 2 < · · · < E N and the factor of 2 accounts for spin) and terminating this sum once N states have been occupied. However, in the limit that our box is sufﬁciently large, the energy levels are so closely spaced we can just as well evaluate this energy by replacing the discrete sum with an integral over a continuous distribution of eigenvalues. To see this, note that adjacent energy levels have an energy difference of order 2π 2 h¯ 2 /m L 2 . The integration that arises in replacing the discrete summation is most conveniently realized in k-space. To effect this integration, it is ﬁrst necessary to identify the number of states per unit volume of k-space. Recall that the points in k-space are of the form km 1 ,m 2 ,m 3 = (2π/L)(m 1 , m 2 , m 3 ), and hence occupy the vertices of a simple cubic lattice in k-space. As a result, each such point may be assigned a volume (2π/L)3 . This observation comes from the recognition that the lattice parameter in k-space is 3 3 2π/L. Hence we make the identiﬁcation N = (L/2π) d k and it is seen that the total energy is given by 3 L h¯ 2 k 2 3 (3.61) d k, E tot = 2 2π k 2m

3.2 Quantum Mechanics

107

where the factor of 2 accounts for the fact that each k-point can accommodate two electrons, one for each component of spin. Here we have done nothing more than replace the sum over occupied states with the integral given above, where the prefactor serves as a density of states and insures that our volume element d 3 k is properly weighted. Because of the isotropy of the energy spectrum when viewed from the k-space perspective, this integration can be carried out in spherical coordinates, where the radius of the resulting sphere is denoted as the Fermi wavevector, k F . It is clear that the magnitude of the Fermi wavevector is intimately tied to the electronic density, but how? Here, we see that the total number of states contained within this k-space sphere is the same as half the total number of electrons (again the factor of 2 arising because of spin). The volume of the Fermi sphere is k = 4π k 3F /3, while the volume per state is (2π/L)3 . Hence, the ratio of these numbers must yield the total number of electrons and 1 leads to the conclusion that k F = (3π 2 ρ) 3 . Given the radius of the Fermi sphere, we are now in a position to evaluate the total energy of our electron gas. Upon explicitly writing the integral given above in spherical coordinates, we ﬁnd 3 k F 2π π 2 4 L h¯ k sin θk dkdφk dθk , (3.62) E tot = 2 2π 2m 0 0 0 where we include the subscript k as a reminder that our integration is carried out over a sphere in k-space. Performing the relevant integrations leads to the conclusion that h¯ 2 k 5F E tot = , (3.63) V 10π 2 m which can in turn be converted into an average energy per electron of 3 h¯ 2 k 2F 3 E tot = = F . (3.64) N 5 2m 5 Here we have introduced the notion of the Fermi energy which is denoted by F . This energy, like the Fermi wavevector, can be obtained explicitly in terms of the electron density. In fact, since shortly we will use the energy of the electron gas to obtain the optimal density, it is convenient to rewrite eqn (3.64) in terms of the 1 density, recalling that k F = (3π 2 ρ) 3 as E tot =

3 h¯ 2 2 (3π 2 ρ) 3 , 5 2m

(3.65) 2

illustrating that this part of the electron gas energy scales as ρ 3 . If we take a typical ˚ −3 , the associated Fermi energy is roughly 7 eV, some 300 density such as 0.1 A times larger than the thermal energy scale at room temperature, for example.

108

3 Quantum and Statistical Mechanics Revisited

The results for the electron gas obtained above can be pushed much further. In particular, the rudimentary calculation developed thus far can serve as a jumping off point for an evaluation of the lattice parameter and bulk moduli of simple metals. As it stands, the energy we have determined for the electron gas is a monotonically increasing function of the density and thus there is as yet no provision for an optimal density. However, we can now supplement the analysis given above by treating the effect of electron–electron interactions perturbatively. In this case, the details of the calculation will take us too far aﬁeld, so we will have to be satisﬁed with sketching what is involved in making the calculation and in quoting the results. The basic idea is that we wish to evaluate the expectation value of the perturbed Hamiltonian H =

1 e2 , 2 i= j |ri − r j |

(3.66)

which characterizes the electron–electron interaction. Physically what this means is that we are trying to determine the correction to the energy of eqn (3.65) as a result of putting the electron interaction back into the problem. This correction is determined by using the ground state wave function of the unperturbed electron gas (this is the normal rule of ﬁrst-order perturbation theory), which we already know from the previous section is a product of plane waves that have been appropriately antisymmetrized to respect the Pauli principle. In particular, we must evaluate E ee = ψtot |H |ψtot , where ψtot (r1 , . . . , r N ) is of the form 1 ik ·r √ e 1 1 1 ik ·r 1 √ e 2 1 ψtot (r1 , . . . , r N ) = √ .. N! . 1 ik ·r √ e N 1

1 √ eik1 ·r2 1 ik2 ·r2 √ e .. . 1 √ eik N ·r2

(3.67)

··· ··· .. . ···

1 √ eik1 ·r N 1 ik2 ·r N √ e .. . 1 √ eik N ·r N

, (3.68)

a construction known as the Slater determinant that instructs us how to build up a properly antisymmetrized wave function as a product of one-electron wave functions. Note that we have been slightly sloppy by omitting the added dependence on the spin coordinates in the wave function. For full details, see chap. 3 of Pines (1963) or chap. 1 of Fetter and Walecka (1971). As is evident from the form of the integrals that will result from evaluating the expectation value demanded in eqn (3.67), the outcome of this analysis depends upon the Fourier transform

3.2 Quantum Mechanics

109

of the Coulomb potential itself. Careful evaluation of the integrals demanded by eqn (3.67) results in a contribution to the total energy of the electron gas of the form 3 h¯ 2 1 E interact = − (3π 2 ρ) 3 , (3.69) 2π 2ma0 where a0 is the Bohr radius and is given by a0 = h¯ 2 /me2 . Note that the sign of this contribution to the energy is negative, resulting in a competition between the two terms we have found and a consequent emergence of an optimal density. The result of adding together the two contributions to the energy of the electron gas is E egas =

3 h¯ 2 3 h¯ 2 2 1 (3π 2 ρ) 3 − (3π 2 ρ) 3 . 5 2m 2π 2ma0

(3.70)

This energy has a minimum at a certain optimal density which may be found by evaluating ∂ E egas /∂ρ = 0, resulting in ρopt =

125 . 192π 5 a03

(3.71)

This density may be converted in turn to an estimate for the lattice parameter by assuming that the atom at each lattice site of the bcc lattice has donated a single electron. In particular, the lattice parameter implied by these arguments is 1 384π 5 3 ˚ aeg = a0 ≈ 5.2 A. (3.72) 125 This number should be contrasted with the experimental lattice constant of a typical ˚ In free electron metal such as sodium, for which the lattice parameter is 4.23 A. addition to the lattice parameter, this model may also be used to estimate the bulk modulus of free electron metals by resorting to the deﬁnition B = V (∂ 2 E/∂ V 2 ). This is left as an exercise for the reader. In the present context, this example was intended to serve as a reminder of how one formulates a simple model for the quantum mechanics of electrons in metals and, also, how the Pauli principle leads to an explicit algorithm for the ﬁlling up of these energy levels in the case of multielectron systems. In addition, we have seen how this model allows for the explicit determination (in a model sense) of the cohesive energy and bulk modulus of metals.

3.2.6 Quantum Mechanics of Bonding As we hinted at in the section on the hydrogen atom, when we turn our attention to the origins of bonding in molecules and solids, a useful alternative to the

110

3 Quantum and Statistical Mechanics Revisited

Fig. 3.10. Disposition of wave functions of neighboring atoms during the process of bond formation.

electron gas physics described above is to build our picture around the simple ideas suggested by the H2 molecule. As shown in ﬁg. 3.10, the hydrogenic wave functions on the atoms of interest begin to overlap once these atoms are sufﬁciently close. Conceptually, we see that once this happens, the nuclear potential on one of the atoms begins to amend the wave function tied to the other. In this section, our task is to compute this interaction and to demonstrate how it makes possible the reduction in energy more commonly known as bonding. We begin with a discussion of bonding in the abstract, and then turn to an explicit treatment of the H2 molecule itself, and show how what is learned there can be generalized to systems of increasing size. The ideas developed here provide the conceptual foundations for our development of the tight-binding method in chap. 4. The intuition leading to this approach is best coached by an analogy. If we are to consider a system of masses and springs such as is shown in ﬁg. 3.11, our various oscillators will vibrate independently, each at its own natural frequency. If we now imagine connecting the oscillators, as also shown in the ﬁgure, it is immediate that the vibrational frequencies are altered by the interaction. In particular, if we consider the simple case where the masses and spring constants are all equal, we ﬁnd that the frequencies are split in the manner indicated in the ﬁgure. The quantum mechanical analog of the spring problem, also illustrated schematically in ﬁg. 3.11, is the idea that when two atoms are sufﬁciently far apart, their respective atomic energy levels at energy E a are undisturbed, and the atoms should be thought of as independent. On the other hand, when the atoms are in sufﬁciently close proximity, the potential due to one nucleus begins to inﬂuence the electron centered on the other. This interaction has the effect of splitting the original energy levels as indicated in the ﬁgure. For a two-atom molecule in which each atom

3.2 Quantum Mechanics

111

Fig. 3.11. Analogy between problem of coupled oscillators and that of bonding in molecules.

donates one electron, the difference in energy between the original isolated atoms and the molecule is E bond = −2|h|, the bonding energy. From a physical perspective, our strategy in thinking about bonding has certain key similarities to our treatment of the free electron gas. In particular, we assume that the properties of the molecule (or solid) can be obtained by solving a oneelectron Schr¨odinger equation and then ﬁlling up energy levels in accordance with the Pauli principle. This means that we completely ignore the interaction between the electrons themselves. Hence, for the two-atom molecule of interest here, the Schr¨odinger equation may be written h¯ 2 2 ∇ ψ + V1 (r)ψ + V2 (r)ψ = Eψ. (3.73) 2m In this equation, the total potential experienced by the electron is obtained by −

112

3 Quantum and Statistical Mechanics Revisited

summing up the separate nuclear potentials emanating from the two nuclei, V1 and V2 . Rather than trying to ﬁnd those functions which satisfy the Schr¨odinger equation written above, we adopt a simpler variational approach in which the search for unknown functions is replaced by the search for unknown coefﬁcients. The basis for this strategy is a variational argument. We represent the wave function for the molecule as a linear combination of the atomic orbitals centered on the two nuclei, that is, ψ = a1 φ1 + a2 φ2 ,

(3.74)

where φ1 and φ2 are the atomic orbitals on sites 1 and 2, and the ai s are the coefﬁcients we aim to determine. We have adopted a minimalist approach in which rather than using a basis consisting of all of the atomic orbitals associated with each site, we just borrow a single 1s orbital (i.e. |1, 1s and |2, 1s, where the ﬁrst index labels the site and the second labels the orbital type) from each atom and assume that the molecular wave function can, to a ﬁrst approximation, be represented as a linear combination of these functions. A more sophisticated treatment could include more basis functions such as the 2s and 2p states, and so on. The basis of the determination of the unknown coefﬁcients is the recognition that the expectation value of the energy can be written as E = ψ| Hˆ |ψ,

(3.75)

and our task is to ﬁnd those ai s that minimize this expression. In fact, this is exactly the same argument we adopted in our description of the ﬁnite element approach to the Schr¨odinger equation, with the difference being the choice of basis functions. As a result of the arguments given above, we write the function to be minimized as (a1 , a2 ) = a1 φ1 + a2 φ2 | Hˆ |a1 φ1 + a2 φ2 − Ea1 φ1 + a2 φ2 |a1 φ1 + a2 φ2 , (3.76) in perfect analogy with eqn (3.36). If we write this out explicitly term by term, the result is (a1 , a2 ) = a1∗ a1 φ1 | Hˆ |φ1 + a1∗ a2 φ1 | Hˆ |φ2 + a2∗ a1 φ2 | Hˆ |φ1 + a2∗ a2 φ2 | Hˆ |φ2 − E(a1∗ a1 φ1 |φ1 + a1∗ a2 φ1 |φ2 + a2∗ a1 φ2 |φ1 + a2∗ a2 φ2 |φ2 ),

(3.77)

an equation which can be further simpliﬁed if we adopt the notation E 1 = φ1 | Hˆ |φ1 , E 2 = φ2 | Hˆ |φ2 , and h = φ1 | Hˆ |φ2 = φ2 | Hˆ |φ1 . Applying these deﬁnitions to the result given above, and exploiting the assumption of orthonormality (i.e. φi |φ j = δi j ), which is, strictly speaking, not true, we now

3.2 Quantum Mechanics

113

Fig. 3.12. Solutions for H2 molecule using the two-orbital basis.

ﬁnd (a1 , a2 ) = a1∗ a1 E 1 + a1∗ a2 h + a2∗ a1 h + a2∗ a2 E 2 − E(a1∗ a1 + a2∗ a2 ).

(3.78)

For simplicity, we now assume that the two atoms are identical (i.e. E 1 = E 2 ) and further, choose our zero of energy such that E 1 = 0. If we now minimize this function with respect to the ai s, in particular by enforcing ∂/∂ai∗ = 0 for i = 1, 2, we can ﬁnd the optimal choice for these coefﬁcients. Effecting the minimization suggested above results in two coupled algebraic equation that are more conveniently written in matrix form as a1 0 −|h| a1 =E . (3.79) a2 a2 −|h| 0 Note that we have used our knowledge of the sign of h to rewrite it as h = −|h|, a result of the fact that the potential energy of interaction represented by this parameter is negative. The result of solving these √ equations is two solutions, one with energy E = −|h| and wave function ψ1 =√(1/ 2)(φ1 +φ2 ) and the other with energy E = |h| and wave function ψ1 = (1/ 2)(φ1 − φ2 ). These two solutions are shown in ﬁg. 3.12.

114

3 Quantum and Statistical Mechanics Revisited

Fig. 3.13. Series of molecules of increasing size and associated molecular eigenstates. The wave functions are indicated schematically with shaded atoms corresponding to one sign of relevant atomic orbital and unshaded atoms corresponding to opposite sign for relevant orbital (adapted from Hoffmann (1988)). Note that the spacing of energy levels is schematic and there is no relation indicated between the energy scales for different size molecules.

Recall that the question we originally posed was that of the origin of bonding. As a result of the solution worked out above, we are now in a position to address this question. With the zero of energy chosen above, the energy of the two isolated atoms is E atoms = 0. For the molecule, we ﬁll energy levels according to Pauli’s principle, which for the two-electron problem of interest here means one spin-up electron and one spin-down electron are both assigned energy −|h| with the result that the energy difference between the molecule and the free atoms is E bond = −2|h|. The energy is lowered by virtue of the partnership struck up between the two free atoms: a bond has formed. This idea is illustrated graphically in ﬁg. 3.12 where it is seen that there is an enhancement in the probability distribution in the region between the two atoms, a signature of the formation of bond charge. The generalization of this problem to the case of increasingly larger collections of atoms is straightforward and is founded upon the construction of larger matrices of the variety described above. For example, if we consider the problem of three atoms which occupy the vertices of an equilateral triangle, a 3 × 3 matrix emerges with three resulting eigenvalues. The distribution of energy eigenvalues for increasing system sizes is indicated schematically in ﬁg. 3.13. This ﬁgure demonstrates the way in which the energy can be lowered as a result of atoms conspiring to form bonds. In chap. 4, we will undertake a systematic analysis

3.3 Statistical Mechanics

115

of bonding in solids, using what we have learned of quantum mechanics in the preceding pages. In this part of the chapter, we have seen that quantum mechanics provides the microscopic foundations for evaluating the disposition of the electronic degrees of freedom. Just as continuum mechanics provides the setting within which one solves the boundary value problems related to the deformation of solids, quantum mechanics provides a scheme for attacking the boundary value problems associated with electrons in solids. Of course, quantum mechanics has a much wider scope than we have hinted at here, but our aim has been to couch it in terms of the subject at hand, namely, the modeling of materials. In this case, it is the role of quantum mechanics in instructing us as to the nature of bonding in solids that is of most importance, and as will be seen in coming chapters, these ideas will be an indispensable part of our modeling efforts.

3.3 Statistical Mechanics 3.3.1 Background Thermodynamics provides the conceptual cornerstone upon which one builds the analysis of systems in equilibrium. The elemental theoretical statement that can be made about such systems is embodied in Gibbs’ variational principle. This asserts that a certain function of state, namely the entropy, is a maximum in equilibrium so long as the system is subject to the additional constraint of constant total energy. The usual intuitive notions one attaches to the analysis of systems in contact with each other such as equality of temperature, pressure and chemical potential emerge from this principle quite naturally. For example, if we consider the box shown in ﬁg. 3.14 with an internal partition that is rigid and impermeable, the variational principle noted above can be used to determine the privileged terminal state (i.e. the state of equilibrium) that results from removing the constraints offered by the wall. The argument is that for the overall closed system, the total energy is given by E tot = E 1 + E 2 = const., implying that d E 1 = −d E 2 . On the assumption that the entropy S is additive, we note that ∂ S1 ∂ S2 d Stot = d E1 + d E2. (3.80) ∂ E 1 V ,N ∂ E 2 V ,N 1

1

2

2

These derivatives are evaluated at ﬁxed volumes V1 and V2 as well as ﬁxed particle numbers N1 and N2 . If we now replace d E 2 with −d E 1 , we see that the condition of maximum entropy is equivalent to the statement that ∂ S2 ∂ S1 = , (3.81) ∂ E1 ∂ E2

116

3 Quantum and Statistical Mechanics Revisited

Fig. 3.14. Partitioning of the system under consideration into two boxes which may freely exchange energy.

which because of the deﬁnition of temperature as 1/T = (∂ S/∂ E)|V,N , we recognize as the condition of equality of temperature between the two subsystems. If we consider in turn the case in which the wall is permeable (d N1 = −d N2 ) or may move (d V1 = −d V2 ), the conditions of equal chemical potential and pressure result. As it stands, the type of thermodynamic assertions ﬂeshed out above are indifferent to microscopic considerations, though it is certainly of great interest to unearth their microscopic origins. In this part of the chapter our aim is to investigate statistical mechanics. A key insight that emerges from these ideas is the probabilistic nature of equilibrium states. We take the view that statistical mechanics is the microscopic partner of equilibrium thermodynamics. While equilibrium thermodynamics does not concern itself with the mechanistic underpinnings of observed behavior, statistical mechanics teaches how one may deduce macroscopic features of a system as the result of a postulated microscopic model. Such models are widespread, doing service in problems such as the calculation of electric and magnetic susceptibilities, the analysis of the equilibrium concentrations of point defects in solids and the determination of the vibrational entropy of solids and its connection to phase transformations. Our treatment begins on a philosophical note with an attempt to elucidate the business of statistical mechanics. Next, we will turn to an analysis of the formal apparatus of statistical mechanics with a view of the partition function and how

3.3 Statistical Mechanics

117

it may be used in the evaluation of quantities of thermodynamic interest. The harmonic oscillator will loom large in our discussion as a result of the contention that this model may serve as a basis for the analysis of material properties, such as the speciﬁc heat, the vibrational entropy and the microscopic origins of the diffusion constant. This discussion will then be couched in the alternative language of information theory. These arguments will identify the role of inference in statistical mechanics, and will make more evident how we treat systems in the face of incomplete knowledge of that system’s microscopic state. This will be followed by a computational view of statistical mechanics. Here the task will be to see how the use of computing lends itself to a numerical statement of the program of statistical mechanics, with a brief overview of molecular dynamics and the Monte Carlo method. Our starting point is an assessment of the meaning of a macroscopic observable state. Thermodynamic states are parameterized by a small number of relevant macroscopic variables such as the energy, E, the volume, V , the pressure, p, and the various mole numbers, n α . As Callen (1985) has eloquently noted in the introductory sections of his book, it is well nigh miraculous that despite the ostensible need of 1023 degrees of freedom to fully characterize the state of a system, all but a few of them ‘are macroscopically irrelevant.’ Indeed, a key outcome of the statistical mechanical approach is an insight into how macroscopic parameters arise as averages over the microscopic degrees of freedom. Our fundamental contention is that a given macroscopic state is consistent with an enormous number of associated microscopic states. This observation lends itself to a nomenclature which distinguishes between macrostates and microstates. For the moment, we do not distinguish between the classical and quantum versions of these microstates, though we will see later that in some cases, such as that of the speciﬁc heat of solids, there are dramatic differences in the outcome of classical and quantum analyses. Classical physics envisions a continuum of microscopic states parameterized by the conjugate variables qi and pi , where these are the coordinates and momenta of the i th particle, respectively. For a system composed of N particles, each microstate corresponds to a particular point in a 6N -dimensional space referred to as ‘phase space’, with the dynamical variables varying continuously as the system winds about on its trajectory through this space. A given point within the classical phase space corresponds to a particular realization of the coordinates (q1 , p1 , q2 , p2 , . . . , q N , p N ) = ({qi , pi }). On the other hand, within quantum mechanics, these states are discretely reckoned and each microstate is parameterized by distinct quantum numbers. The notion of a microstate is perhaps most easily understood by virtue of an example. We imagine a closed box containing an ideal gas. Our use of the term ‘closed’ is meant to imply that in this case the volume, the number of particles and

118

3 Quantum and Statistical Mechanics Revisited

Fig. 3.15. Comparison of two possible microstates for particles in a box.

the energy of the system are all held constant and assume the values V, N and E, respectively. Within either the classical or quantum settings we may immediately identify the nature of the microstates available to the gas. The speciﬁcation of a particular point in phase space implies knowledge of a geometrical character. In particular, the speciﬁcation of the 3N coordinates qi identiﬁes the locations of all of the particles while the 3N momenta pi characterize their motions. The momenta of the molecules of the gas are imagined to be distributed in some way that is consistent with the assumed total energy, E. In addition, there is a conﬁgurational part of the microstate. One possible geometric conﬁguration which corresponds to an allowable microstate of the gas would have all of the molecules bunched in one corner of the box. Intuitively, such a state seems unlikely. On the other hand, there are many more microstates in which the molecules are distributed evenly throughout the box. These two alternatives are contrasted in ﬁg. 3.15. We can estimate the probability of the state in which the particles are bunched in one corner as (Vc /Vtot ) N , where Vc is the volume of the region where the particles are assumed to be bunched. In keeping with the assumption of noninteracting particles that is the essence of the ideal gas, we have assumed that the probability that a given particle will be in any subregion is given by the ratio of the volume of that subregion to the whole volume. The key feature of interest for the calculation given above is that all such microstates (including the unlikely state in which all the molecules are localized in some small region) are consistent with the overall macrostate characterized by the observables V, N and E. The postulate that rests behind the explicit calculation of macroscopic observables is that such observables are averages that emerge as a result of the system ranging over the allowed microstates. For our purposes, the central assumption upon which the rest of our development is ﬁxed is that all such microstates

3.3 Statistical Mechanics

119

consistent with the overall macrostate are equally likely. This statement is sometimes referred to as the principle of equal a priori probabilities or the principle of insufﬁcient reason. At ﬁrst sight, it may seem odd that this statement has calculable consequences. But as will be shown below, this postulate provides a logical basis for statistical mechanics and is used to derive the analytic machinery which makes the theory so powerful. The quantitative basis for the linkage between macro- and microstates is provided by the prescription for computing the entropy S(E, V, N ) in terms of the number of microstates, namely, S(E, V, N ) = k B ln (E, V, N ),

(3.82)

where (E, V, N ) is the number of microstates available to the system when it has energy, E, occupies a volume, V , and consists of N particles. This equation is a key example of the type of link between the microscopic and macroscopic perspectives that is our aim. In this case, it is the entropy, S, a property of the macrostate that is related to (E, V, N ), the associated microscopic quantity which characterizes the number of ways of realizing the macroscopic state of interest. The constant that links these two quantities is Boltzmann’s constant and will hereafter be referred to simply as k. The immense signiﬁcance of this equation is tied to the fact that it provides a mechanistic interpretation of the notion of entropy, while at the same time rooting the notion of equilibrium in probabilistic ideas. In particular, the assertion that emerges from this equation in conjunction with Gibbs’ variational statement, is that the equilibrium state (the state of maximum entropy) is really the macrostate corresponding to the largest number of microscopic realizations. As a result, we see that the primary business of statistical mechanics has been reduced to that of counting the number of microstates accessible to the system once the energy, volume and particle number have been ﬁxed.

3.3.2 Entropy of Mixing In this section, we take up the view of the statistical origins of entropy and equilibrium that was introduced in the previous section. We advance the view that equilibrium can no longer be viewed as a matter of certainty, but rather only as a matter of enormous likelihood. An example which is at once simple, enlightening and useful is related to the entropy of mixing, where it is imagined that two constituents are randomly distributed among N sites subject to the constraint that N A + N B = N , as depicted in ﬁg. 3.16. The analysis of the entropy of mixing serves as a viable starting point for the consideration of problems such as the conﬁgurational entropy of a two-component alloy, the distribution of vacancies within a single crystal at equilibrium and the arrangements of magnetic spins.

120

3 Quantum and Statistical Mechanics Revisited

Fig. 3.16. Two-dimensional schematic representation of two distinct alloy conﬁgurations where different atom types are represented by different colors: (a) disordered state, (b) ordered state.

We note that if we have a total of N sites to occupy, there are N ! different ways of occupying these sites on the assumption that each conﬁguration is distinct. However, in our case this logic must be amended on the basis of the realization that there are N A equivalent A objects and N B equivalent B objects. This implies that in reality there are N! = (3.83) N A !N B ! distinct conﬁgurations. The denominator in this expression eliminates the redundancy which results from the fact that the A objects are indistinguishable among themselves as are the B objects. Following Boltzmann’s equation linking the entropy and the number of microstates, the entropy that follows from this enumeration is N! . (3.84) S = k ln N A !N B ! As we can see in this instance, the calculation of the entropy of mixing has been reduced to the combinatorial problem of identifying the number of distinct microstates consistent with our overall macrostate which is characterized by a ﬁxed number of A and B objects. Further insights into this conﬁgurational entropy can be gleaned from an attempt to reckon the logarithms in an approximate fashion. We note that our expression for the entropy may be rewritten as S = k(ln N ! − ln N A ! − ln N B !).

(3.85)

Following Reif (1965), these sums may be written explicitly as ln N ! = ln 1 + ln 2 + · · · + ln N .

(3.86)

3.3 Statistical Mechanics

121

Fig. 3.17. Approximations associated with Stirling approximation.

This sum may be represented graphically as shown in ﬁg. 3.17, which suggests the approximate expression N ln x d x = N ln N − N . (3.87) ln N ! ≈ 1

Here it must be noted that we have made an imprecise description of what under more formal terms is known as the Stirling approximation. Within the context of our characterization of the conﬁgurational entropy, the Stirling approximation of ln N ! allows us to rewrite the entropy as S = k[(N A + N B ) ln(N A + N B ) − N A ln N A − N B ln N B ].

(3.88)

If we now deﬁne the variable c = N A /N and rearrange terms it is found that S = −k N [(1 − c) ln(1 − c) + c ln c].

(3.89)

This entropy is shown in ﬁg. 3.18 as a function of the concentration variable. In chap. 7, it will be shown that this result is one piece of the free energy that reﬂects the competition between the energy cost to increase the number of vacancies in a solid and the free energy lowering increase in entropy that attends an increase in the number of such vacancies. The arguments given above were built around the idea of an isolated system. However, there are both mathematical and physical reasons to favor a treatment in which we imagine our system as being in contact with a reservoir at ﬁxed temperature. For example, our later discussion of annealing is a realization of this claim. A particular sample of interest (a chunk of metal, for example), is subjected to external heating with the aim of examining the change in its microstructure. In this case, the model of an isolated system is inappropriate. Rather, we should model

122

3 Quantum and Statistical Mechanics Revisited

Fig. 3.18. Entropy of mixing associated with binary conﬁgurations.

the system as being in contact with a reservoir with which it exchanges energy. This scenario leads to the canonical distribution which will form the substance of the next section. 3.3.3 The Canonical Distribution For many problems, consideration of the isolated system envisioned above is inadequate. In particular, it is often of interest to consider a subsystem in contact with a reservoir. Such reservoirs can either be a source of energy or particles, and one imagines free communication between the subsystem of interest and its associated reservoir. The conceptual trick introduced to allow for rigorous treatment of this problem, without advancing assumptions beyond those made already, is to treat the entire universe of subsystem plus reservoir as a closed system unto itself. Within this setting, we once again carry out the same sort of counting arguments introduced in the previous section for an isolated system. However, unlike the previous case, we will derive expressions for the underlying thermodynamics which can be couched purely in terms of the degrees of freedom of only the subsystem. As a ﬁrst example, we consider the problem in which the subsystem and reservoir are free to exchange only energy, as is indicated schematically in ﬁg. 3.19. In this case, the number of microstates available to the subsystem is s (E s ), where the subscript s refers to the subsystem. Similarly, the number of microstates available to the reservoir is given by r (E − E s ). From the perspective of the composite universe made up of the system and its reservoir, the total energy is

3.3 Statistical Mechanics

123

Fig. 3.19. Composite system composed of a subsystem and a reservoir with which it is free to exchange energy.

constant, and the number of microstates available to that composite system when the subsystem has energy E s is given by composite (E; E s ) = s (E s )r (E − E s ). Here we have noted that the total number of states available to the composite system at a given E s is the product of the number of states available to the reservoir and those available to the subsystem. Note that the total number of microstates available to the composite system is gotten as tot (E) = s composite (E; E s ). Equilibrium between the reservoir and the subsystem is attained when the entropy is maximized, which corresponds to ﬁnding that distribution of energy between the subsystem and reservoir which corresponds to the largest number of total microstates. Within the microcanonical formalism presented in the previous section we asserted that all microstates are equally likely. In the present situation, we center our interest just on the subsystem. The price we pay for restricting our interest to the nonisolated subsystem is that we no longer ﬁnd all states are of equal probability. Though the states of the composite universe are all equally likely, we will ﬁnd that there is a calculable energy dependence to the probability for a given energy state for the subsystem. To make our analysis concrete, we begin by noting that if we consider the circumstance in which the subsystem is in a nondegenerate state of energy, E a (i.e. s (E a ) = 1), then the total number of states available to the composite universe of system plus reservoir is composite (E) = r (E − E a ). What we have done here is to identify the subset of states of the composite system that is consonant with the subsystem having deﬁnite energy E a . We continue with the observation that the probability P(E a ) of ﬁnding the system in this state is proportional to the number of microstates available to the reservoir. That is, P(E a ) ∝ r (E − E a ). The speciﬁc dependence of this probability on the energy E a can be garnered from the

124

3 Quantum and Statistical Mechanics Revisited

following argument. First, we note that as a consequence of the assertion made above we have r (E − E a ) eln[r (E−Ea )] P(E a ) = = ln[ (E−E )] . (3.90) b P(E b ) r (E − E b ) e r This equation notes that the ratio of the probabilities of ﬁnding the subsystem with two particular energies is equal to the ratios of the corresponding number of states available to the reservoir at the two energies of interest. The remainder of our analysis can be built around the presumed smallness of E a with respect to E itself, which affords an opportunity for Taylor expansion of the slowly varying logarithms in the form ∂ ln r (3.91) Ea . ln r (E − E a ) ln r (E) − ∂E Coupled with the thermodynamic identity that relates the temperature to the energy dependence of the entropy, namely, 1 ∂S 1 ∂ ln = = , (3.92) ∂E k ∂E kT we are left to conclude that 1 −(Ea /kT ) e , (3.93) Z where Z is an as-yet undetermined constant. In fact, for the practical purposes of everyday calculation, it is the ‘constant’ Z that depends on parameters such as T and V which is the basis of many calculations. This quantity, known as the partition function, is found by insisting that our probability distribution be suitably normalized, namely, 1 −(En /kT ) P(E n ) = e = 1. (3.94) Z n n P(E a ) =

This expression states that the partition function itself can be determined from knowledge of the energy levels via Z= e−(En /kT ) . (3.95) n

Our notation is meant to argue that the subsystem can have any of a number of different energies, labeled by the set of integers n. We would do well at this point to reﬂect on the preceding argument. Throughout, our derivation has rested on the central assertion upon which the microcanonical distribution is built, namely, that of the equal likelihood of all microstates consistent with the given macrostate. In this case, however, we have seen ﬁt to examine a subsystem in contact with a thermally rigid reservoir which can freely donate and receive energy

3.3 Statistical Mechanics

125

without altering its temperature. By examining, within a microcanonical setting, the properties of the composite universe of subsystem plus reservoir, we have been able to identify the unequal probabilities attached to the subsystem’s energy levels. What has emerged is a scheme in which only the parameters characterizing the subsystem need be considered. Having established the probability distribution that characterizes our subsystem when in contact with a reservoir, we now seek insights into the thermodynamic implications of this solution. As a ﬁrst example, suppose we are interested in determining the average energy of the subsystem. On the basis of the familiar notion of determining averages associated with a given probability distribution, it is immediate that 1 E n P(E n ) = E n e−(En /kT ) . (3.96) E = Z n n This expression may be considerably simpliﬁed on the recognition that we may deﬁne a variable β = 1/kT , and that

E n e−β En = −

n

1 ∂Z . Z ∂β

(3.97)

Hence, we have that E = −

∂ ln Z . ∂β

(3.98)

This result supports our contention that it is the partition function that serves as the analytic engine for calculating quantities of thermodynamic interest. The speciﬁc heat, which is a measure of the stiffness of the system to thermal ﬂuctuations, will emerge later as an additional material parameter which looks to microscopic models for its origins. Within the statistical mechanical formalism we have set up here, the speciﬁc heat may be easily determined on the recognition that C V = ∂E/∂ T |V . Upon exploiting the deﬁnition of β, this may be rewritten as C V = kβ 2

∂ 2 ln Z . ∂β 2

(3.99)

An alternative and more streamlined approach to the types of results described above emerges once we have made contact between the partition function and the Helmholtz free energy. Recall that thermodynamic quantities such as the pressure and entropy may be evaluated simply as derivatives of the Helmholtz free energy as ∂F ∂F , S=− . (3.100) p=− ∂V T ∂T V

126

3 Quantum and Statistical Mechanics Revisited

The connection of the partition function to the Helmholtz free energy is effected via the expression F = −kT ln Z .

(3.101)

This result is yet another example of an equation (like the Boltzmann expression for the entropy) which connects macroscopic and microscopic quantities. The origins of this equation can be obtained on the basis of thermodynamic reasoning and to probe these details the reader is encouraged to examine chap. 16 of Callen (1985) or the ﬁrst sections of Feynman (1972). In the following section we will examine how this machinery may be brought to bear on some model problems.

3.3.4 Information Theoretic Approach to Statistical Mechanics Until now, our treatment of statistical mechanics has been founded upon the assumption that this theory reﬂects the average treatment of the coupled microscopic degrees of freedom that make up a material. However, in this section we follow an alternative view in which it is held that statistical mechanics is not a physical theory at all, but is rather an example of a calculus of uncertainty in which inference in the face of incomplete information is put on a rigorous footing. Indeed, the Boltzmann factor introduced above has been used in problems ranging from image reconstruction to the analysis of time series data lending support to the claim that the fundamental ideas transcend their historical origins in physics. The central idea is that the algorithm of statistical mechanics is but one example of how reasoning should proceed when we are confronted with incomplete knowledge. The ideas associated with the information theoretic approach to statistical mechanics may be sketched as follows. We begin with the observation that our task is to infer the probability of the various microstates that the system is capable of adopting. From the macroscopic perspective, all that we may know about a system might be its mean energy, E. Given so little information about the distribution of microstates it seems brash to assume that anything deﬁnitive may be argued for. However, such problems form the province of probabilistic reasoning, and in conjunction with the ideas of information theory, much progress can be made. We follow Shannon in attaching a measure to the quality of our knowledge of a system’s disposition as revealed by the probability distribution that describes it. For an overview of these ideas, we refer the reader to Jaynes (1983). For example, if we consider the rolling of a die, the best we might do is to enumerate the six possible outcomes and to attribute to each an equal likelihood. This is low-quality information. On the other hand, if the die were loaded and we could say with certainty that only the face with a one would be revealed, our state of knowledge is of the highest quality.

3.3 Statistical Mechanics

127

Associated with a discrete probability distribution with N outcomes Shannon identiﬁes an entropy, H ( p1 , p2 , . . . , p N ), which lends quantitative weight to our intuitive notions about the quality of information associated with that distribution. The derivation of the particular functional form taken by H ({ pi }) is based on a few fundamental desiderata. First, given N possible outcomes, the case in which all such outcomes are equally likely will maximize the function H . This statement corresponds to our intuition that the case of equal likelihood of all outcomes corresponds to maximal ignorance. The probability distribution is featureless and there is nothing about it that inclines us to favor one outcome over any other. Secondly, if we now imagine increasing the number n of equally likely outcomes, the function H ({1/n}) should be a monotonically increasing function of n. This too jibes with our intuition that as the number of outcomes is increased, our knowledge is degraded. The ﬁnal requirement of the function H is based upon its additivity. If we specify the state of the system in two steps (i.e. there are n rooms, each of which contains m boxes), the reckoning of the information entropy must be consistent with the result of specifying all of the information at once (i.e. there are n ×m outcomes). On the basis of these few basic requirements, the claim is that the function H ( p1 , p2 , . . . , p N ) is uniquely determined and that it provides a measure of the information content of the probability distribution it characterizes. The outcome of the reasoning hinted at above is the claim that the function H is given by pi ln pi . (3.102) H ( p1 , p2 , . . . , p N ) = −k i

That is, if we are given a discrete probability distribution { pi }, the function H ({ pi }) provides a unique measure of the information content of that distribution. The beauty of this result is that it provides a foundation upon which to do inferential reasoning. In particular, when faced with the question of determining a probability distribution (such as, for example, in the context of constructing a statistical ensemble which gives the probabilities of various microstates), it gives us a way to determine the best distribution. As yet, we have said nothing of statistical mechanics, and it is just this fact that makes the information theoretic approach to inference of utility to X-ray crystallographers, radio astronomers attempting to decipher noisy data and statistical mechanicians alike. In light of the developments described above, the Gibbsian variational principle may be seen in a different light. The idea is that the maximization of entropy may be alternatively viewed as a statement of unbiased inference: choose that probability distribution that assumes nothing that is not forced on us by the data themselves. To see the workings of the maximum entropy approach, we begin with the trivial example of N outcomes with our only knowledge being the enumeration of the

128

3 Quantum and Statistical Mechanics Revisited

states themselves. In this case, our intuition anticipates the probability distribution in which all outcomes are equally likely. To see how this arises from the principle of maximum entropy, we maximize the augmented function pi ln pi + λ pi − 1 , (3.103) S = − i

i

where λ is a Lagrange multiplier used to enforce the constraint that the distribution be normalized. Also, we have absorbed the constant k into the Lagrange multiplier. Maximizing this function with respect to the pi s results in pi = eλ−1 , independent of i, revealing that all outcomes are equally likely. The determination of the constant is based on the recognition that i pi = 1, and yields pi = eλ−1 = 1/N . Note that we have provided theoretical justiﬁcation for the principle of equal a priori probabilities that was adopted earlier. We see that this is the best guess that can be made on our very limited data. The key point is that rather than asserting equal a priori probabilities as an article of faith we have shown that it is the best distribution that we can possibly assign in the sense that it most faithfully represents our degree of ignorance concerning the various outcomes. A more enlightening example is that in which not only is the constraint of normalization of the probability distribution imposed, but it is assumed that we know the average value of some quantity, for example, E = i E i pi (E i ). In this case, we again consider an augmented function, which involves two Lagrange multipliers, one tied to each constraint, and given by pi ln pi − λ pi − 1 − β pi E i − E . (3.104) S = − i

i

i

Note that once again the ﬁrst constraint imposes normalization of the distribution. Maximizing this augmented function leads to the conclusion that p j = e−1−λ−β E j . Imposition of the normalization requirement, j p j = 1, implies that 1 e−1−λ = e−β E j ,

(3.105)

j

which is consonant with our expectation that we should recover the partition function as the relevant normalization factor for the canonical distribution. A deeper question concerns the Lagrange multiplier β which is formally determined via the nonlinear equation E = −

∂ ln Z . ∂β

(3.106)

3.3 Statistical Mechanics

129

3.3.5 Statistical Mechanics Models for Materials Statistical Mechanics of the Harmonic Oscillator. As has already been argued in this chapter, the harmonic oscillator often serves as the basis for the construction of various phenomena in materials. For example, it will serve as the basis for our analysis of vibrations in solids, and, in turn, of our analysis of the vibrational entropy which will be seen to dictate the onset of certain structural phase transformations in solids. We will also see that the harmonic oscillator provides the foundation for consideration of the jumps between adjacent sites that are the microscopic basis of the process of diffusion. In light of these claims, it is useful to commence our study of the thermodynamic properties of the harmonic oscillator from the statistical mechanical perspective. In particular, our task is to consider a single harmonic oscillator in presumed contact with a heat reservoir and to seek the various properties of this system, such as its mean energy and speciﬁc heat. As we found in the section on quantum mechanics, such an oscillator is characterized by a series of equally spaced energy levels of the form E n = (n + 12 )h¯ ω. From the point of view of the previous section on the formalism tied to the canonical distribution, we see that the consideration of this problem amounts to deriving the partition function. In this case it is given by 1 ] ¯ e−[(n+ 2 )hω/kT . (3.107) Z= n

The contribution of the zero point energy can be factored out of the sum leaving us with ¯ ¯ e−n hω/kT , (3.108) Z = e−hω/2kT n ¯ which upon the substitution x = e−hω/kT is seen to be a simple geometric series and can be immediately summed to yield

Z=

¯ e−hω/2kT . ¯ 1 − e−hω/kT

(3.109)

As a result, we are left with the insight that the free energy of such an oscillator is given by h¯ ω ¯ + kT ln(1 − e−hω/kT ). (3.110) F= 2 This equation will arise in chap. 6 in the context of structural transformations in solids when it comes time to evaluate the contribution made by vibrations to the total free energy of a solid. As shown earlier, the thermodynamic properties of this system can be reckoned as derivatives of the logarithm of the partition function with respect to the inverse

130

3 Quantum and Statistical Mechanics Revisited

temperature. For example, the mean energy is given by E = −

h¯ ω h¯ ω ∂ ln Z = + hω/kT . ∂β 2 e¯ −1

(3.111)

This result should be contrasted with expectations founded on the classical equipartition theorem which asserts that an oscillator should have a mean energy of kT . Here we note two ideas. First, in the low-temperature limit, the mean energy approaches a constant value that is just the zero point energy observed earlier in our quantum analysis of the same problem. Secondly, it is seen that in the high-temperature limit, the mean energy approaches the classical equipartition result E= kT . This can be seen by expanding the exponential in the denominator ¯ −1 of the second term to leading order in the inverse temperature (i.e. ehω/kT h¯ ω/kT ). As a result, the mean energy is thus E (h¯ ω/2) + kT . With the presumed largeness of the temperature as revealed in the inequality h¯ ω/kT 1, this yields the classical equipartition result. These results will all make their appearance later in several different contexts including in our discussion of phase diagrams in chap. 6. Statistical Mechanics of the Ising Model. A tremendously important model within statistical mechanics at large, and for materials in particular, is the Ising model. This model is built around the notion that the various sites on a lattice admit of two distinct states. The disposition of a given site is represented through a spin variable σi which can take the values ±1, with the two values corresponding to the two states. With these ‘kinematic’ preliminaries settled, it is possible to write the energy (i.e. the Hamiltonian) as a function of the occupations of these spin variables as E Ising = Ji j σi σ j . (3.112) i j

In its simplest form, we can take the coupling constants Ji j as being equal so that the energy may be rewritten as E Ising = J i j σi σ j and further we restrict our attention to the near-neighbor variant of this model in which only spins on neighboring sites interact. At this point, we see that the physics of this model is determined in large measure by the sign of J , with J > 0 favoring those states in which adjacent sites are unlike, whereas when J < 0, the energy favors alignment of neighboring spins. The statistical mechanics of this model surrounds the question of the competition between the energy which favors an ordering of the various spins and the entropy term in the free energy which favors a disordering of the arrangement of spins. Before entering into questions concerning the ‘solution’ of this model, we should ﬁrst recount some of the uses to which it has been put and to foreshadow its

3.3 Statistical Mechanics

131

signiﬁcance to our endeavor. The Ising model has enormous signiﬁcance beyond the limited range of applications it has in modeling materials. Nevertheless, even for what we will want to say, the Ising model will often serve as a paradigm for the analysis of a wide range of problems in materials modeling. In chronological terms, the Ising model will see duty as the basis for our analysis of phase diagrams, the various stacking arrangements that arise in the so-called polytypes, some of our discussion of surface reconstructions and will provide a foundation for the use of the Potts model in the analysis of grain growth. Though the Ising model is amenable to full analytic solution in one and two dimensions, we will make use of it in the more general three-dimensional setting and will therefore have to resort to either analytic approximations or full numerics to really probe its implications. On the other hand, examination of this model in the reduced dimensionality setting can be very revealing to illustrate the various tools of statistical mechanics in action. In addition, the reduced dimensionality problems will also help foreshadow the difﬁculties we shall face in confronting the three-dimensional problem that will arise in the consideration of phase diagrams, for example. As has already been noted throughout this chapter, the engine for our analysis of the thermodynamic properties of a given model is the partition function, which for the Ising model may be written as ··· exp(−β Ji j σi σ j ). (3.113) Z= σ1 =±1

σ N =±1

ij

The sums in front of the exponential are an instruction to consider all possible 2 N conﬁgurations of the N -spin system. For the one-dimensional case, there are a variety of possible schemes for evaluating the partition function, and thereby the thermodynamics. One appealing scheme that illustrates one of the themes we will belabor repeatedly is that of degree of freedom thinning in which degrees of freedom are eliminated by integrating over particular subsets of the full set of degrees of freedom. Indeed, in chap. 12, we will attempt to make generic comments on strategies for eliminating degrees of freedom. In the present case, the idea is to evaluate the partition sum explicitly for half the spins. For example, we can elect to integrate over the even-numbered spins, resulting in an effective Hamiltonian in which only the odd-numbered spins appear explicitly, though at the price of introduction of new coupling parameters in the model. An instructive description of this procedure may be found in Maris and Kadanoff (1978), whom we follow below. To see the idea in practice, the partition function of eqn (3.113) is reorganized as ··· e K (σ1 σ2 +σ2 σ3 ) e K (σ3 σ4 +σ4 σ5 ) · · · , (3.114) Z= σ1 =±1

σ N =±1

132

3 Quantum and Statistical Mechanics Revisited

where the constant K = J/kT has been introduced. We may now sum over the spins with even labels, resulting in · · · (e K (σ1 +σ3 ) + e−K (σ1 +σ3 ) )(e K (σ3 +σ5 ) + e−K (σ3 +σ5 ) ) · · · . (3.115) Z= σ1 =±1 σ3 =±1

The goal is to seek a scheme to rewrite this result that takes precisely the same form as the original partition function. In concrete terms, this implies that we seek an f (K ) such that

e K (σi +σi+2 ) + e−K (σi +σi+2 ) = f (K )e K σi σi+2 .

(3.116)

Note that this equation involving the unknown function f (K ) must be true whatever our choices for σi = ±1 and σi+2 = ±1 may be. In particular, for σi = σi+2 = 1, this becomes

e2K + e−2K = f (K )e K ,

(3.117)

while for σi = −σi+2 , eqn (3.116) becomes

2 = f (K )e−K .

(3.118)

Eqns (3.117) and (3.118) may now be solved for f (K ) and K with the result that 1 f (K ) = 2 cosh 2 2K and K = 12 ln cosh 2K . Note that in the more formidable setting in higher dimensions, the degree of freedom thinning procedure leads to equations for the ‘renormalized’ coupling constant (i.e. K ) that may be treated only approximately. The result obtained above leads now to the key insight of the analysis, namely, the relation between the partition functions of the system with N degrees of freedom and that of the thinned down model involving only N /2 degrees of freedom. Using our new found results for the constant K and the function f (K ), we may relate these partition functions as N

Z (N , K ) = [ f (K )] 2 Z (N /2, K ),

(3.119)

where the dependence of the partition function on both the number of degrees of freedom and the the coupling constant has been made explicit. The next step in the argument is the recognition that the free energy (i.e. F = −kT ln Z ) scales with the system size and thus we may write, ln Z = N ζ (K ). Taking the logarithm of eqn (3.119) and using the fact that ln Z (N , K ) = N ζ (K ), results in 1

ζ (K ) = 2ζ (K ) − ln[2 cosh 2 (2K )].

(3.120)

What is the good of this set of results? The key point is the identiﬁcation of a recursive strategy for obtaining the partition function. In particular, in the present setting, we note that in the high-temperature limit, Z = 2 N resulting in the

3.3 Statistical Mechanics

133

observation that ζ (K → 0) = ln 2. On the basis of the knowledge of ζ (K ) at this particular point, we can now iterate to determine the functions of interest at other points in parameter space. Our discussion of the Ising model was primarily intended to introduce the physics of the model itself. However, because of its conceptual relevance to many of the strategies to be adopted later in the book, we have also illustrated the use of real space renormalization group ideas for degree of freedom thinning. We note again that our later uses of the Ising model will be for problems in which exact analytic progress is presently unavailable, and for which either approximate or numerical procedures will be resorted to. Statistical Mechanics of Electrons. Later in the book, we will repeatedly require insights into the generalization of the arguments made earlier in the context of the electron gas for ﬁlling up energy states at ﬁnite temperatures. Recall our discussion of the electron gas given earlier in which all states with wavevectors |k| ≤ k F were unequivocally occupied and those with |k| > k F were unequivocally not occupied. This picture must be amended at ﬁnite temperatures, since in this case, by virtue of thermal excitation, some fraction of electrons will ﬁll states of higher energy. The distribution which governs the ﬁnite temperature distribution of electrons is the so-called Fermi–Dirac distribution, and it is that distribution (both its derivation and signiﬁcance) that occupies our attention presently. The ﬁrst question we pose is of wider generality than is needed to consider the question of electron occupancies. In particular, we ask for the relevant probability distribution for those problems in which not only is the average value of the energy prescribed, but so too is the average number of particles, N . In this case, using the maximum entropy ideas introduced above, the entropy and its associated constraints may be written as pi ln pi − λ pi − 1 − β pi E i − E − α pi Ni − N . S =− i

i

i

i

(3.121) The index i is a superindex that refers to a particular realization of both E and N . If we now follow the same procedure used earlier to derive the canonical distribution by maximizing the entropy, it is found that the resulting probabilities are of the form 1 (3.122) pi = P(E, N ) = e−β(E−µN ) . Z In this case, we have introduced the Gibbs sum deﬁned as e−(E−µN )/kT . Z= states

(3.123)

134

3 Quantum and Statistical Mechanics Revisited

Fig. 3.20. Fermi–Dirac distribution for several different temperatures.

Note that the passage from the formal result based on information theoretic reasoning to the physical setting of interest here involved the recognition of the Lagrange multiplier α being related to the chemical potential through α = µ/kT . The results obtained above are of such general importance when applied to the case of electrons (more generally to fermions) that the resulting distribution has its own nomenclature and is referred to as the Fermi–Dirac distribution. To see how eqn (3.122) is applied to determine the average number of particles in a given quantum state when the particles themselves obey the Pauli principle, we consider a particular electronic state with energy . In this case, the Gibbs sum is of the form Z = 1 + e−β(−µ) .

(3.124)

The reasoning behind this assertion is the statement that there are only two allowed states to consider: the state is unoccupied (E = 0, N = 0) and the state is occupied by a single particle (E = , N = 1). As a result, the mean occupancy of this state is obtained as 1 e−β(−µ) = β(−µ)+1 , (3.125) N () = −β(−µ) 1+e e which is the sought after Fermi–Dirac distribution which presides over questions of the occupancy of electron states at ﬁnite temperatures. In ﬁg. 3.20, we show this distribution for several different temperatures. For ease of plotting, we have rescaled variables so that the Fermi–Dirac distribution is written in the form 1 , (3.126) N ( f, βµ) = βµ( f −1) e +1

3.3 Statistical Mechanics

135

where f has been introduced as a way of characterizing what fraction the energy of interest is of the energy µ. It is evident from the ﬁgure that at low temperatures (i.e. βµ 1) we recover the results of our earlier analysis, namely, that all states with energy lower than F (note that F is the zero temperature µ, i.e. F = µ(0)) are occupied while those above this energy are not. On the other hand, we also see that at higher temperatures there is a reduction in the mean occupancy of states with energy below F and a corresponding enhancement in the occupancy of those states just above F . 3.3.6 Bounds and Inequalities: The Bogoliubov Inequality There are many instances in which an exact analytic solution for the partition function (or the free energy) will be beyond our reach. One notable example that will arise in chap. 6 is that of the free energy of a liquid. In such instances, there are several related strategies that may be adopted. It is possible to adopt perturbative approaches in which the statistical mechanics of the unperturbed state is in hand, and approximations for the problem of interest are arrived at through a series of systematic corrections. A related approach is the attempt to bound the exact free energy through the use of robust inequalities such as the Bogoliubov inequality to be introduced below. With this principle in hand, the bounds can be variationally improved by introducing free parameters in the ‘reference’ Hamiltonian, which are then chosen to yield the best possible bound. The basic idea is as follows: we assume that the free energy of real interest is that associated with a Hamiltonian H , for which the exact calculation of the free energy is intractable. We then imagine an allied Hamiltonian, denoted H0 , for which the partition function and free energy may be evaluated. The inequality that will serve us in the present context asserts that Fexact ≤ F0 + (H − H0 )0 ,

(3.127)

where the average on the right hand side is evaluated with respect to the distribution that derives from the Hamiltonian H0 . What this inequality teaches us is that if we can ﬁnd an approximate Hamiltonian for which we can evaluate the partition function, then we can provide bounds on the free energy of the system described by the full H = H0 + H1 , where we have introduced the notation H1 to describe the perturbation that is added to the original H0 . Presently, we consider a few of the details associated with the derivation of the Bogoliubov inequality. Our treatment mirrors that of Callen (1985) who, once again, we ﬁnd gets to the point in the cleanest and most immediate fashion. As said above, we imagine that the problem of real interest is characterized by a Hamiltonian H which may be written in terms of some reference Hamiltonian H0

136

3 Quantum and Statistical Mechanics Revisited

Fig. 3.21. Schematic of the free energy as a function of the parameter λ discussed in the context of the Bogoliubov inequality.

as H (λ) = H0 + λH1 ,

(3.128)

where λ is a tunable parameter which weights the contribution of the perturbation to the reference Hamiltonian. We introduce the notation Z = tr e−β H , with the symbol tr referring to the trace operation, though it should be read as ‘sum over all conﬁgurations’. Evaluation of the derivatives of the exact free energy Fexact (λ) = −kT ln tr e−β H with respect to λ reveal that d Fexact = H1 , dλ

(3.129)

d 2 Fexact = −β(H1 − H1 )2 . dλ2

(3.130)

The signiﬁcance of the latter equation is that it demonstrates that for all λ, the curvature of the function Fexact (λ) is negative. Why should this observation ﬁll us with enthusiasm? The relevance of this insight is revealed graphically in ﬁg. 3.21, where it is seen that we may construct an approximate free energy (a ﬁrst-order Taylor expansion in powers of λ) of the form d Fexact λ, (3.131) Fapprox (λ) = Fexact (λ = 0) + dλ λ=0 which is guaranteed to satisfy the inequality Fexact (λ = 1) ≤ Fapprox (λ = 1), by virtue of what we have learned about the curvature of the function Fexact (λ).

3.3 Statistical Mechanics

137

What has been done, in essence, is to exploit our certainty about the sign of the curvature of the free energy with respect to λ to carry out a Taylor expansion of that free energy with respect to λ on the hope that the leading order expansion will be sufﬁciently accurate. Note that when the slope of Fexact (λ) is evaluated explicitly, we ﬁnd tr H1 e−β(H0 +λH1 ) d Fexact = , (3.132) dλ tr e−β(H0 +λH1 ) which for the special case of λ = 0 yields d Fexact = H1 0 , dλ

(3.133)

where H1 0 signiﬁes the evaluation of the average value of H1 (or H − H0 ) with respect to the distribution function arising only from the reference Hamiltonian. The implication of these results is that with only a knowledge of the distribution function for the reference state, we are able to put bounds on the exact free energy. To see this mathematically, we plug the result of eqn (3.133) into eqn (3.131) with the result that Fexact ≤ Fexact (λ = 0) + H − H0 0 .

(3.134)

Recall that Fexact (λ = 0) is nothing more than the free energy associated with the Hamiltonian H0 which, by hypothesis, we know how to compute. As a result, we have demonstrated the existence of the sought after bound on the exact free energy. The ﬁnishing touches are usually put on the analysis by allowing the reference Hamiltonian to have some dependence on adjustable parameters that are determined to minimize the right hand side of eqn (3.134). We note that as a result of this scheme, the better the choice of H0 , the higher will be the quality of the resulting variational estimate of the free energy.

3.3.7 Correlation Functions: The Kinematics of Order Conventional kinematic notions are built around the idea that the system of interest can be characterized by a series of simple states without any reference to microscopic ﬂuctuations or disorder. On the other hand, in the analysis of systems at ﬁnite temperature or in the presence of the effects of disorder, it is essential to build up measures that characterize the disposition of the system while at the same time acknowledging the possibility of an incomplete state of order within that system. Just as strain measures served as the primary kinematic engine used in our analysis of continua, the notion of a correlation function will serve to characterize the disposition of those systems that are better thought of statistically. Indeed, we will ﬁnd that in problems ranging from the ‘spins’ introduced earlier in conjunction

138

3 Quantum and Statistical Mechanics Revisited

with the Ising model, to the density (and its ﬂuctuations), and even to the heights on fracture surfaces, correlation functions provide a quantitative language for describing the statistical state of systems with many degrees of freedom. As is already evident from the discussion of this chapter, many-particle systems are often described in terms of averages over microscopic variables. For example, the net magnetization M of a spin system can be thought of as an average of the form M = N µσi , where N is the total number of spins per unit volume, µ is the magnetic moment per spin and σi is the spin variable at site i. The notion of the correlation function is introduced in light of the knowledge that by virtue of the dynamics of the microscopic variables, the macroscopic variables themselves are subject to ﬂuctuations. The extent of these ﬂuctuations is conveniently quantiﬁed using the notion of the correlation function which achieves a greater signiﬁcance because of its relation to the response of a system to external probes, including the scattering of X-rays, electrons or neutrons. The basic idea is to quantify the extent to which the behavior of a particular microscopic quantity such as the spin at site i, σi , is correlated with that of the spin σ j at site j. By deﬁnition, the pair correlation function of σi and σ j is deﬁned by Ci j = σi σ j − σi σ j .

(3.135)

What we note is that if the joint probability distribution P(σi , σ j ) is of the form P(σi , σ j ) = P(σi )P(σ j ), then σi σ j = σi σ j , the spins are uncorrelated, and correspondingly, the correlation function Ci j vanishes. The importance of correlation functions as a way of characterizing systems with many degrees of freedom can be argued for from a number of different angles, but here we simply note that a knowledge of such functions serves as a basis for computing ‘susceptibilities’ of various types in a number of different systems, and can be thought of as providing a kinematics of order. From a structural perspective, these ideas can be couched in slightly different terms by considering the two-particle distribution function deﬁned by ρ (2) (r1 , r2 ) = δ(r1 − ri )δ(r2 − r j ) . (3.136) i= j

The two-particle distribution tells us the probability that particles will be found at r1 and r2 and will thereby serve as the basis for determining the energy of interaction between different pairs of particles when the best statements we can make about the system are statistical. For example, when describing the energetics of liquids our statements about the structure of that liquid will be couched in the language of distribution functions. In preparation for our later work on the free energy of liquids (see chap. 6), we ﬁnd it convenient to introduce an auxilliary

3.3 Statistical Mechanics

139

quantity, the pair correlation function g(r1 , r2 ), which is deﬁned through ρ (2) (r1 , r2 ) = ρ(r1 )ρ(r2 )g(r1 , r2 ).

(3.137)

This deﬁnition simplifes considerably in the case of an isotropic liquid for which the single particle density is a constant (i.e. ρ(r) = N /V ), resulting in the radial distribution function g(r ). As said above, these deﬁnitions will form a part of our later thinking.

3.3.8 Computational Statistical Mechanics As yet, we have described some of the analytic tools that are available to forge a statistical connection between macroscopic observables and the microstates that lead to them. The advent of high-speed numerical computation opened up alternative strategies for effecting this connection which permitted a literal interpretation of the notion of an average. The key idea is to allow the system to visit a sequence of microscopic ‘realizations’ of the macroscopic state of interest. By effecting an average for the quantity of interest over the various members in this set of realizations, the statistical average of interest is performed explicitly. On the one hand, molecular dynamics obtains average quantities by repeatedly evaluating the dynamical variable of interest as it takes on a succession of values as the system winds through phase space. Alternatively, Monte Carlo methods allow for construction of copies of a particular system that one envisions in speaking of the ‘ensemble averages’ of Gibbs. In this case, rather than explicitly tracking the system along some trajectory through phase space, we imagine an ensemble of copies of the system of interest, each corresponding to some different microstate and which are representative members of the set being averaged over. In both the molecular dynamics and Monte Carlo methods, the mentality is to construct explicit microscopic realizations of the system of interest in which once the microscopic degrees of freedom have been identiﬁed and the nature of their interaction understood, one explicitly constructs some subset of the allowable microstates and performs averages over them. In this part of the chapter, our aim is to describe a few of the highlights of both the molecular dynamics and Monte Carlo approaches to computational statistical mechanics. We begin with a review of the notion of microstate, this time with the idea of identifying how one might treat such states from the perspective of the computer. Having identiﬁed the nature of such states, we will take up in turn the alternatives offered by the molecular dynamics and Monte Carlo schemes for effecting the averages over these microstates. As noted in the preface, the availability of computers has in many cases changed the conduct of theoretical analysis. One of the ﬁelds to beneﬁt from the emergence

140

3 Quantum and Statistical Mechanics Revisited

Fig. 3.22. Wandering of a Ag adatom on the Ag(111) surface as revealed using molecular dynamics (adapted from Boisvert and Lewis (1996)).

of powerful computational alternatives to traditional analytic approaches is that of statistical mechanics. If we follow the line of reasoning suggested by molecular dynamics, the argument is made that the averages of interest can be realized by following the system in its trajectory in phase space via the expression 1 T At = A({ p(t), q(t)})dt. (3.138) T 0 In this case, our notation indicates that we are considering the time average ( t ) of the quantity A which itself is a function of the dynamical variables. Those variables are represented here generically by q(t) and p(t),with q a conﬁgurational coordinate and p the associated momentum. The averaging process is tied to the type of trajectory indicated schematically in ﬁg. 3.22, where we have artiﬁcially reduced the problem to a two-dimensional scenario that allows for visualization. Molecular dynamics provides a scheme for explicitly evaluating these averages by computing A at various time intervals while allowing the particles to range over the trajectories resulting from their respective equations of motion. In the simplest classical terms, carrying out a molecular dynamics simulation involves a few key steps. First, it is necessary to identify some force law that governs the interactions between the particles which make up the system. The microscopic origins of the force laws themselves will be taken up in chap. 4, and for the moment we merely presuppose their existence. It is then imagined that these particles evolve under their mutual interactions according to Newton’s second law of motion. If we adopt the most naive picture in which all of the atoms are placed in a closed box at ﬁxed energy, we ﬁnd a set of 3N coupled second-order ordinary

3.3 Statistical Mechanics

141

differential equations of the form d 2 ri = Fi . (3.139) dt 2 A host of clever schemes have been devised for integrating these equations of motion in a manner that is at once efﬁcient and stable. One well-known integration scheme is that of Verlet (though we note that more accurate methods are generally used in practice). One notes that for a sufﬁciently small time step, the position at times t ± δt may be expressed as mi

1 d 2 ri 2 dri δt + δt . dt 2 dt 2 By adding the two resulting expressions and rearranging terms, we ﬁnd ri (t ± δt) ≈ ri (t) ±

(3.140)

d 2 ri 2 δt . (3.141) dt 2 Though there are a variety of sophisticated schemes for carrying out the integrations required here, we choose to emphasize the physical insights gained thus far. The choice of a time step δt strikes to the heart of one of the key difﬁculties in carrying out the types of simulations advocated here. The processes of interest to the mechanics of materials involve a broad range of time scales. At the smallest end of that spectrum, we have the time scale associated with atomic vibrations. Clearly, if we are to simulate the thermal properties of solids, the time step must be a small fraction of the vibrational period. By way of contrast, if our aim is the investigation of deformation processes that are slaved to mass transport, the time scale can be many orders of magnitude larger than the picosecond scale associated with thermal vibrations, resulting in a gross mismatch between the time step required for carrying out temporal integrations, and the time scale associated with the process of interest. This question will be addressed in chap. 12 when we describe the hyperdynamics method. In addition to questions surrounding the treatment of multiple time scales, another intriguing problem is posed by simulating a system in contact with a thermal reservoir. Until now, we have envisaged a system that is maintained at ﬁxed total energy. In many cases, one would rather mimic a system at ﬁxed temperature. One of the more interesting aspects of molecular dynamics is the role of effective theories for mimicking the presence of either thermal or pressure reservoirs. The point is that through the trick of incorporating a single extra set of conjugate variables, the effect of a thermal reservoir may be accounted for rigorously while maintaining the Hamiltonian description of the underlying dynamics. The approach we will follow here was pioneered by Nos´e (1984) and Hoover (1985). ri (t + δt) = −ri (t − δt) + 2ri (t) +

142

3 Quantum and Statistical Mechanics Revisited

Nos´e argues that the presence of the thermal reservoir may be accounted for in the Hamiltonian context by incorporating an additional set of conjugate variables, {s, ps }. The Hamiltonian for the extended system is given by H=

p2 ps2 i + gkT ln s. + V ({q }) + eff i 2ms 2 2Q i

(3.142)

For the present purposes, all that we really wish to note is that in light of this Hamiltonian, it becomes possible to carry out averages that are effectively those associated with a canonical ensemble, or said differently, with a system maintained at a temperature T . These ideas are described very nicely in Frenkel and Smit (1996). As already mentioned, an alternative to the explicit contemplation of microscopic trajectories is the construction of a stochastic approach in which various microscopic realizations of a system are constructed so as to respect the underlying distribution. Much has been made of the necessity of ergodic assumptions in statistical mechanics which allow for a replacement of the type of temporal average described above by the alternative ensemble averages immortalized by Gibbs. Here the idea is that rather than following the system on its excursions through phase space, one generates a series of macroscopically equivalent copies of the system, and averages over the members of this ‘ensemble’. For example, if our interest is in the thermodynamic properties of an alloy with constituents A and B, we can imagine generating alternative occupations of the various crystal lattice sites on the basis of random occupancy. Two snapshots corresponding to different members of the ensemble under consideration here were shown in ﬁg. 3.16. The underlying physical contention is the equivalency of the averaging process when effected either via the ensemble trick introduced above or by following the system as it ranges over its dynamic trajectory. Besides providing the foundation on which Monte Carlo methods are built, we have seen that the ensemble picture serves as the basis for much of the analytic machinery which is used to conduct the investigations of statistical mechanics. if one generates a sequence of states based upon the rule that a given state is ‘accepted’ with probability 1 if the new state lowers the energy and with probability e−βE is the new state increases the energy, then the resulting distribution will be canonical. For further details, I am especially fond of the discussion of Frenkel and Smit (1996). 3.4 Further Reading Quantum Mechanics Principles of Quantum Mechanics by R. Shankar, Plenum Press, New York: New York, 1980. A personal favorite on the subject of quantum mechanics. Shankar

3.4 Further Reading

143

does a ﬁne job of integrating the mathematical formalism and physical principles of quantum mechanics with their roots in many of the historical ideas of classical mechanics. His discussion of path integral methods is enlightening and readable. Quantum Theory by David Bohm, Prentice-Hall, Inc., Englewood Cliffs: New Jersey, 1951. Bohm’s book brings both clarity and completeness to many of the features of quantum mechanics that are of importance for the work carried out in the present book. Quantum States of Atoms, Molecules and Solids by M. A. Morrison, T. L. Estle and N. F. Lane, Prentice-Hall, Inc., Englewood Cliffs: New Jersey, 1976. Not a well-known book, but one I like very much as it has much that is practical to offer concerning the application of quantum mechanics to understanding bonding in solids. Thermodynamics and Statistical Mechanics E. T. Jaynes: Papers on Probability and Statistics edited by R. D. Rosenkranz, D. Reidel Publishing Company, Dordrecht: The Netherlands, 1983. The presence of this work on the list reﬂects my enormous prejudice in favor of the information theoretic approach to statistical mechanics as pioneered by Edwin T. Jaynes. This book is one of my prize possessions and at the time of this writing has no trace of its original hardback cover as a result of the many trips the book has made. Statistical Mechanics by R. P. Feynman, The Benjamin/Cummings Publishing Company, Inc., Reading: Massachusetts, 1972. This book bears the usual stamp of Feynman’s idiosyncratic approach to physics. There are many perspectives to be found here that will not be found elsewhere. States of Matter by D. L. Goodstein, Prentice-Hall, Inc., Englewood Cliffs: New Jersey, 1975. This often humorous book is full of insights into everything from the meaning of the partition function to the origins of Bragg scattering. Principles of Statistical Mechanics by A. Katz, W. H. Freeman and Company, San Francisco: California, 1967. This book remains virtually unknown, but again reﬂects my own taste for the information theoretic perspective. This book offers some hints as to the possible uses of this perspective to build more complete theories of nonequilibrium processes. Thermodynamics and an Introduction to Thermostatics by H. B. Callen, John Wiley and Sons, New York: New York, 1985. The perceptive reader will recognize on short order my own afﬁnity for the book of Callen. His treatment of the central ideas of both thermodynamics and statistical mechanics is clean and enlightening, and I share the author’s view that classical thermodynamics is primarily a theory of thermostatics.

144

3 Quantum and Statistical Mechanics Revisited

Fundamentals of Statistical Mechanics, Manuscript and Notes of Felix Bloch, prepared by John Dirk Walecka, Stanford University Press, Stanford: California, 1989. I have found this book eminently readable and interesting. ‘The Expanding Scope of Thermodynamics in Physical Metallurgy’ by J. W. Cahn, Materials Transactions, JIM, 35, 377 (1994). Cahn’s article is full of interesting ideas concerning both the signiﬁcance of previous thermodynamic achievements and the possible expansion of thermodynamic ideas to novel ways of treating interfaces and lattice effects.

Computational Statistical Mechanics Understanding Molecular Simulation by Daan Frenkel and Berend Smit, Academic Press, San Diego: California, 1996. An extremely serious book written at a high level and full of detailed insights. The Art of Molecular Dynamics Simulation by D. C. Rapaport, Cambridge University Press, Cambridge: England, 1995. This book gives a modern introduction to the subject of computer simulation, with special reference to molecular dynamics. ‘The Virtual Matter Laboratory’, M. J. Gillan, Contemporary Physics, 38, 115 (1997) provides an overview of some of the key ideas associated with the use of the ideas presented in this chapter as the basis of simulations of the properties of matter.

3.5 Problems

1 Particle in a Box by the Finite Element Method Flesh out the details of the discussion of the use of the ﬁnite element method to solve the problem of a particle in a box. In particular, derive eqns (3.44), (3.46), (3.48), (3.50) and table 3.1.

2 Finite Elements and the Schr¨odinger equation In this chapter, we discussed the use of the ﬁnite element method to solve the Schr¨odinger equation. Use the same formalism to solve the Schr¨odinger equation for a quantum corral of elliptical shape.

3.5 Problems

145

Fig. 3.23. Two three-atom conﬁgurations to be considered in problem 4.

3 Two-Dimensional Electron Gas Construct a two-dimensional analog of the electron gas model developed in this chapter. Begin by solving the relevant Schr¨odinger equation and obtaining the set of discrete energy eigenvalues. Assume that in the square box of area A there are N free electrons. Obtain the electronic energy by ﬁlling up the various energy states. How does the resulting energy depend upon the density?

4 Tight-Binding Model of Three-Atom Molecules Using the arguments introduced earlier for considering the H2 molecule, consider two separate three-atom conﬁgurations and their associated binding energies. In particular, consider both a three-atom chain with near-neighbor interactions as well as an equilateral triangle geometry as shown in ﬁg. 3.23. Use the same basis (i.e. one s-orbital per atom) and maintain the notation introduced earlier, namely, that i|H | j = h. Construct the appropriate 3 × 3 Hamiltonian matrices for these two different geometries and ﬁnd their corresponding eigenvalues. Fill up the lowest lying energy states and thereby ﬁnd the electronic contribution to the binding energies of both conﬁgurations in the case in which there is one electron per atom.

5 The Stirling Approximation Revisited To obtain an explicit analytic expression for the entropy of mixing as shown in eqn (3.89), we exploited the Stirling approximation. Plot both the exact and the approximate entropy (as gotten from the Stirling approximation) for systems of size N = 10, 100 and 1000.

6 Statistical Mechanics of a Two-Level System Consider a system characterized by two distinct energy levels, 0 and 0 + . Write down the partition function and compute the average energy and speciﬁc heat for this system.

146

3 Quantum and Statistical Mechanics Revisited

7 Entropy Maximization and the Dishonest Die In this problem we will examine the way in which maximum entropy can be used to confront a problem in incomplete information. The basic idea is that we are told that the mean value that emerges after many rolls of a die is 4.5. On this information, we are urged to make a best guess as to the probability of rolling a 1, 2, 3, 4, 5 and 6. Apply the principle of maximum entropy in order to deduce the probability p(n) by applying the constraint 4.5 = n np(n). 8 Partition Function for the One-Dimensional Ising Model For the one-dimensional Ising model with near-neighbor interactions with a Hamiltonian of the form (i.e. zero ﬁeld) J σi σ j , (3.143) H= i j

compute the partition function, the free energy and the average energy. 9 Statistical Mechanics of the Harmonic Oscillator In the text we sketched the treatment of the statistical mechanics of the harmonic oscillator. Flesh out that discussion by explicitly obtaining the partition function, the free energy, the average energy, the entropy and speciﬁc heat for such an oscillator. Plot these quantities as a function of temperature. 10 Monte Carlo Treatment of the Ising Model Write a computer program that allows for the Monte Carlo simulation of the two-dimensional Ising model. The program should use periodic boundary conditions. Generate representative conﬁgurations at a number of different temperatures and attempt to deduce the nature of the phase transition found as a function of temperature. To monitor the state of the system, evaluate the average spin on each site as a function of temperature. In addition you may wish to monitor the values of spin correlation functions such as were described in section 3.3.7.

Part two Energetics of Crystalline Solids

FOUR

Energetic Description of Cohesion in Solids

4.1 The Role of the Total Energy in Modeling Materials A recurring theme in the study of materials is the connection between structure and properties. Whether our description of structure is made at the level of the crystal lattice or the defect arrangements that populate the material or even at the level of continuum deformation ﬁelds, a crucial prerequisite which precedes the connection of structure and properties is the ability to describe the total energy of the system of interest. In each case, we seek a function (or functional) such that given a description of the system’s geometry, the energy of that system can be obtained on the basis of the kinematic measures that have been used to characterize that geometry. As we have discussed earlier (see chap. 2), the geometry of deformation may be captured in a number of different ways. Microscopic theories are based upon explicitly accounting for each and every atomic coordinate. Alternatively, a continuum description envisions a sort of kinematic slavery in which the motion of a continuum material particle implies the associated evolution of large numbers of microscopic coordinates. From the standpoint of microscopic theories, the computation of the total energy requires a description in terms of the atomic positions. In this instance, we seek a reliable function E tot ({Ri }), where {Ri } refers to the set of all nuclear coordinates and serves to describe the geometry at the microscale. For a more complete analysis, this picture should reﬂect the electronic degrees of freedom as well. By way of contrast, a description in terms of a continuum model often results in a phenomenological treatment of the total energy in which the energy is postulated to vary in accordance with some functional of the relevant strain measures. Here we seek a functional E tot [F] which relates the spatially varying deformation ﬁeld and the attendant energy. Note that in accordance with the distinction made between interesting and uninteresting motions in chap. 2, the energy of deformation should depend only on relative motions of material particles. As will become evident 149

150

4 Energetic Description of Cohesion in Solids

in this and subsequent chapters, there are a variety of means for describing the energetics of deformation, each with its own merits and advantages. It is of special interest to uncover the way in which insights at the microscopic scale can be bootstrapped for use at scales normally reserved for continuum approaches. As mentioned above, the total energy often serves as the point of entry for the analysis of material behavior. To whet our appetite for subsequent developments and to illustrate how the total energy impacts material properties we consider three different examples; the elastic moduli, the diffusion constant and the so-called gamma surface. As was already made clear in chap. 2, the elastic moduli are the phenomenological cornerstone of the linear theory of elasticity. Given these parameters, one is positioned to evaluate the stored energy of an arbitrary state of deformation so long as the displacement gradients are not too large. In chap. 5, we will show how by exploiting an analogy between the microscopic and macroscopic descriptions of the total energy the elastic moduli themselves may be computed strictly on the basis of microscopic considerations such as those that form the backbone of this chapter. The basic idea is founded on the recognition that for small deformations, the stored energy is quadratic in the appropriate strain measure. In addition to their ability to probe the energy cost for small excursions from some reference state, microscopic calculations can also be used to examine the energetics of large homogeneous deformations. This type of behavior is indicated schematically in ﬁg. 4.1. By exploiting a series of total energy calculations at the microscopic scale, each associated with a different overall state of strain, the curvature of the energy about the minimum may be determined and thus the moduli. Just as the elastic moduli characterize the properties of a material in the context of elastic boundary value problems, the diffusion coefﬁcient serves as the phenomenological basis for solving boundary value problems involving mass transport. In chap. 7, we will explicitly evaluate the diffusion constant on the basis of microscopic arguments. To do so, we will require an energetic analysis of certain saddle point conﬁgurations on a multi-dimensional potential energy surface. To compute them one must have solved the problem posed in this chapter: given a certain geometric conﬁguration, what is the total energy? For the problem of diffusion, it is the energy as a function of the diffusing atom’s position, also known as the ‘reaction coordinate’, that determines the diffusion rate. This type of analysis is indicated in ﬁg. 4.2 where the energy of a Pb adatom on a Ge surface is computed for a series of different adatom positions. These calculations were carried out using the types of ﬁrst-principles techniques to be described at the end of this chapter. In section 12.3.4, we will discuss a wide class of constitutive models that are broadly known as cohesive surface models. These models postulate the existence of an elastic potential that can be used to describe sliding and opening of interfaces.

4.1 The Role of the Total Energy in Modeling Materials

151

Fig. 4.1. Energy as a function of shear deformation in Al (adapted from Mehl and Boyer (1991)). The lattice parameter a is ﬁxed during the deformation and hence the energy characterizes a oneparameter family of deformations of the fcc lattice, with the members of the family parameterized by b.

Fig. 4.2. Energy of a diffusing adatom as a function of reaction coordinate (after Kaxiras and Erlebacher (1994)).

In the context of the mechanics of materials, such analyses are of value in describing both plasticity and fracture. What will be required in the determination

152

4 Energetic Description of Cohesion in Solids

of these elastic potentials, like for the problems described above, is the relative energies of a number of different conﬁgurations. Our reason for calling attention to these models at this point is to drive home the signiﬁcance of the total energy, whether that energy is being considered in the context of elasticity, mass transport or fracture. The aim of the present chapter is to give examples of the broad classes of microscopic energy functionals that are available to make such calculations. 4.2 Conceptual Backdrop for Characterizing the Total Energy 4.2.1 Atomistic and Continuum Descriptions Contrasted One of the key questions posed in this chapter is how best to reconcile microscopic descriptions, which are presumed to represent the true mechanistic underpinnings of a given process, and phenomenological descriptions, whose aim is to capture the essential physics of a particular process, and to use this reduced description as a predictive tool. The philosophies of these two types of calculations are strikingly different. The microscopic viewpoint champions a complete description of the ‘relevant’ degrees of freedom, with an explicit reckoning of the interactions and evolution of all of them. The total energy may then be written in the form E tot ({Ri , rn }) which highlights the dependence of the total energy on each and every microscopic degree of freedom. Note that here we have explicitly acknowledged the presence not only of the nuclei {Ri }, but also the electrons which are characterized in a classical description by coordinates {rn }. We note that in some instances, such as in density functional theory, the dependence on the electronic degrees of freedom is effected via a dependence of the total energy on the electron density, ρ(r ), which may be written as E tot [ρ(r); {Ri }]. Continuum descriptions are built around energy functionals which depend upon kinematic measures such as displacement ﬁelds as opposed to atomic coordinates, and the neglected atomic-level degrees of freedom make their appearance only implicitly through the presence of material parameters such as the elastic moduli. Whether the description of the total energy is based upon microscopic or continuum notions, ultimately, all such energy functionals represent a reduction in complexity relative to the full microscopic Hamiltonian. The type of degree of freedom reduction we have in mind can be illustrated on the basis of an analogy borrowed from statistical mechanics. If we begin with a system of spins on a lattice which interact according to a near-neighbor Ising model, the total energy may be written E tot ({σi }) = i J σi σi+1 . If we now use the dodge of constructing block spins by adding up the spins in small groups, the total energy may be rewritten in terms of the new block spin variables mediated by some new effective coupling constant Jeff . That is, the reduced description of the total block . In this case, the missing degrees of energy is E tot ({σiblock }) = i Jeff σiblock σi+1

4.2 Conceptual Backdrop for Characterizing the Total Energy

153

freedom only make their presence known through the effective coupling constant Jeff . The simplest example of this type of degree of freedom as pertains to the energy of solids emerges through consideration of the meaning of the elastic moduli. From the continuum perspective, the elastic moduli are material parameters whose values cannot be determined by the continuum theory itself. Within such a framework, the moduli represent the energy cost associated with special afﬁne deformations of the solid. For example, a pure breathing mode has an energy that scales with the bulk modulus B. Thus, we write the energy change upon altering the volume by an amount V as 1 (V )2 . (4.1) E = B 2 V One then makes a bolder assertion. It is hypothesized that even in the presence of some inhomogeneous deformation, the total energy may be obtained as an integral over the strain energy density which is itself obtained by appealing only to the local state of deformation. This leads to the form described in chap. 2: 1 E tot = Ci jkl i j (x)kl (x)dx. (4.2) 2 On the other hand, the microscopic view of such elastic distortions reﬂects the modiﬁcation of a multitude of atomic bonds. The energy cost associated with a given deformation is nothing more than the outcome of evaluating the energies of the distinct atomic constituents. Remarkably, these two perspectives merge in the form of the elastic moduli. That is, the energetics of the complex arrangements of atomic bonds that result from some complicated inhomogeneous deformation can in the end be represented (at least in the case of small deformations) via the relevant elastic moduli. In subsequent chapters, we will reﬁne this description by demonstrating the nature of the coupling between microscopic and continuum descriptions of elasticity by explicitly computing a microscopic expression for the moduli using a simple model potential. However, bonding in solids is an inherently quantum mechanical process and thereby, at least in principle, requires a consideration of the electronic degrees of freedom. In the remainder of this chapter we will investigate the ways in which the total energy can be evaluated from the microscopic perspective. First, we will examine those methods in which the electronic degrees of freedom are subsumed in some effective description. The result of adopting this strategy is that the total energies we will write can only be considered as approximations. We begin by considering pair potential models of bonding in solids. Such models provide a transparent scheme for evaluating the total energy, though they are often of limited quantitative value. In this case, the idea is that the pair potential is an effective

154

4 Energetic Description of Cohesion in Solids

representation of the underlying electronic degrees of freedom which enter only through a parametric dependence of the potentials on the electron density. A more thorough analysis of the electronic degrees of freedom suggests a class of total energy functionals known as effective medium and angular force schemes in which additional features of the physics of bonding are incorporated. These methods are evaluated in turn, with a summarizing commentary on the limitations inherent in all of these methods. Subsequently, we will highlight the key ideas involved in extending the microscopic analysis to permit incorporation of the electronic degrees of freedom. The crowning achievement here is the Hohenberg–Kohn theorem which shows how the total energy may be evaluated as a functional of the electronic density. Further, this scheme allows for a variational treatment of the total energy which amazingly leads to a set of effective single particle equations that are an exact description of the complex many-body system encountered when thinking about electrons in solids. 4.2.2 The Many-Particle Hamiltonian and Degree of Freedom Reduction From a quantum mechanical perspective, the starting point for any analysis of the total energy is the relevant Hamiltonian for the system of interest. In the present setting, it is cohesion in solids that is our concern and hence it is the Hamiltonian characterizing the motions and interactions of all of the nuclei and electrons in the system that must be considered. On qualitative grounds, our intuition coaches us to expect not only the kinetic energy terms for both the electrons and nuclei, but also their mutual interactions via the Coulomb potential. In particular, the Hamiltonian may be written as p2j Z e2 Z 2 e2 P2 e2 1 i + + − + . 2M 2m 2 i j |ri − r j | |ri − R j | |Ri − R j | i j ij ij

(4.3)

The terms in this Hamiltonian are successively, the kinetic energy associated with the nuclei, the kinetic energy associated with the electrons, the Coulomb interaction between the electrons, the electron–nucleus Coulomb interaction and ﬁnally, the nuclear–nuclear Coulomb interaction. Note that since we have assumed only a single mass M, our attention is momentarily restricted to the case of a one-component system. As an antidote to the nearly hopeless complexity presented by the problem of the coupling of degrees of freedom revealed in eqn (4.3), a number of different strategies have been constructed. Such strategies can be divided along two main lines, although this division is in the end an oversimpliﬁcation. One set of ideas surrounds the attempt to remove the electronic degrees of freedom altogether,

4.2 Conceptual Backdrop for Characterizing the Total Energy

155

electing to bury them in effective interactions between the ions. Note that in these approaches, the exact energy is replaced by an approximate surrogate via E exact ({Ri , rn }) → E approx ({Ri }).

(4.4)

As will be shown in coming sections, wide classes of total energy descriptions fall under this general heading including traditional pair potential descriptions, pair functionals, angular force schemes and cluster functionals. The second general class of schemes, which almost always imply a higher level of faithfulness to the full Hamiltonian, are those in which reference to the electrons is maintained explicitly. In this case, the mapping between the exact and approximate descriptions is of the form, E exact ({Ri , rn }) → E approx ({Ri , rn }),

(4.5)

E exact ({Ri , rn }) → E approx [ρ(r), {Ri }],

(4.6)

or as was said already

where the second expression highlights the use of a function ρ(r) to characterize the disposition of the electronic degrees of freedom. Later in the present chapter, we will discuss both tight-binding models (section 4.5) and the use of density functional theory (section 4.6) as ways to effect this type of approximate mapping between the full Hamiltonian and more tractable approximations. The ideas embodied in eqns (4.5), (4.6) and (4.7) constitute profound exercises in effective theory construction. Though considerable hype surrounds the use of the term ‘multiscale modeling’, efforts to confront the difﬁculties inherent in the many-body problem that is cohesion in solids provide a perfect example of the philosophy behind systematic degree of freedom elimination which is itself at the heart of multiscale modeling. The ﬁrst step taken in the attempt to pare down the problem is to exploit the so-called Born–Oppenheimer approximation. Though this approximation will not enter into our calculations in any material way, it is crucial to our enterprise from a philosophic perspective since it illustrates the way in which degrees of freedom can be unlinked, and thereby, problems can be rendered more tractable. The central physical idea is to separate the nuclear and electronic motions on the basis of the smallness of the ratio m/M, where m is the electron mass and M is that of the relevant nuclei. Indeed, from a multiscale perspective, the Born–Oppenheimer approximation represents the simplest of cases in which there is a natural separation of scales, upon which may be founded the scale-bridging ansatz. The physical argument that is made is that the electronic motions are so fast relative to the nuclear motions that we may imagine the electrons to respond to an essentially static set of nuclear positions. The outcome of adopting this view is

156

4 Energetic Description of Cohesion in Solids

that the ionic coordinates only appear parametrically in the Schr¨odinger equation for the electrons. The key observations may be summarized as follows. The Schr¨odinger equation we are faced with solving in the context of the Hamiltonian of eqn (4.3) is of the form H ψ({Ri , rn }) = Eψ({Ri , rn }),

(4.7)

where our notation highlights the dependence of the wave function on all of the nuclear and electronic coordinates. The strategy at this point is to attempt a solution of the form ψ({Ri , rn }) = ψe ({rn }; {Ri })ψn ({Ri }),

(4.8)

where ψe and ψn refer to the solutions to the electron and nuclear problems, respectively. To be more precise, ψe ({rn }; {Ri }) is a solution to the problem (Te + Vee + Ven )ψe ({rn }; {Ri }) = E e ψe ({rn }; {Ri }),

(4.9)

where we have introduced the notation Te to describe the electron kinetic energy, Vee is the electron–electron interaction and Ven is the interaction between the electrons and the nuclei. In addition, this problem is solved with respect to ﬁxed nuclear coordinates {Ri } on the grounds that the nuclei are effectively frozen on the time scale of electronic motions. The ﬁnal step in the approximation is to solve the Schr¨odinger equation for the nuclei of the form (Tn + Vnn + E e )ψn ({Ri }) = E n ψn ({Ri }),

(4.10)

where it is to be noted that the energy eigenvalue from the electron problem ends up as part of the effective potential for the nuclear problem.

4.3 Pair Potentials 4.3.1 Generic Pair Potentials As said earlier, almost the entire business of the present chapter will be to examine the various ways in which the overwhelming complexity presented by the full Hamiltonian of eqn (4.3) has been tamed. Perhaps the simplest example of simplifying the total energy is via an approximation of the form 1 E exact ({Ri , rn }) → E approx ({Ri }) = V (Ri j ), (4.11) 2 ij where V (Ri j ) is the pair potential, and Ri j is the distance between the i th and j th particles. Examples of the pairwise decomposition of the total energy are as old as Newtonian physics itself. Both the gravitational and Coulomb problems exhibit

4.3 Pair Potentials

157

Fig. 4.3. Lennard–Jones pair potential plotted in dimensionless units.

such additivity. Indeed, the ability to write the gravitational potential of a given mass distribution with density ρ(r) as ρ(r )d 3 r (4.12) φ(r) = G |r − r | may be traced directly to such pairwise additivity. To understand the origins of pair potentials, we begin by reﬂecting on their nature in a generic sense, and then turn to an explicit evaluation of quantum mechanically based pair potentials from the standpoint of perturbation theory. As noted above, the total energy within a pair potential setting may be written as E tot = (1/2) i j Veff (Ri j ), where Ri j is the distance between the i th and j th atoms. The logic in this case is that the total energy may be decomposed into a number of distinct contributions, one from each of the bonds that make up the system. Perhaps the most familiar example of such potentials is that of the Lennard–Jones potentials which are intended to reﬂect the polarization interactions that occur in closed-shell systems in which the charge distribution on a given atom may be rearranged as a result of the presence of the neighboring atoms. Within the context of the Lennard–Jones potentials, the energy of interaction between atoms at sites separated by a distance r is 12 6

σ σ , (4.13) − V (r ) = V0 r r where V0 is a parameter determining the depth of the potential well and σ is a length scale that determines the position of the minimum. An example of a Lennard–Jones potential, plotted in dimensionless units, is shown in ﬁg. 4.3.

158

4 Energetic Description of Cohesion in Solids

Once the pair potential has been speciﬁed, it is a straightforward exercise given the atomic positions to compute the total energy. For simplicity, consider a pair potential Veff (r ) whose form is left unspeciﬁed. Further, consider the simplifying assumption that this potential reﬂects a coupling only between ‘nearest neighbors’. To compute the total energy of a given conﬁguration, all that is required is that we sum up the independent contributions of all distinct bonds. For example, if we consider an fcc crystal with lattice parameter a0 , the total energy within the context of a generic potential in which only near-neighbor atoms are presumed to interact is given by a0 N E tot = (4.14) Veff (rnn ) = 6N Veff √ . 2 neighbors 2 In the previous expression we have exploited the fact that in the fcc crystal, each atom is surrounded by an identical √ environment that is composed of twelve near neighbors at a distance of a0 / 2. Because of the high symmetry of the perfect fcc geometry, it was possible to carry out the total energy computation analytically. The basic idea associated with a pair potential calculation of the total energy is to sum over the entirety of bonds between each atom and its ‘neighbors’. When confronted with a more complex geometry, it is likely that we will be reduced to numerical computation, but the concept remains unchanged.

4.3.2 Free Electron Pair Potentials Though simple analytic expressions such as the Lennard–Jones form adopted above (at least the attractive part) may be constructed on the basis of a sound quantum mechanical plausibility argument, the derivation of pair potentials for free electron systems is even more enlightening and strikes to the heart of bonding in metallic systems. An even more important reason for the current discussion is the explicit way in which the effective description of the total energy referred to in eqn (4.4) is effected. As will be shown below, the electronic degrees of freedom are literally integrated out with the result that 1 ¯ = V (Ri j ; ρ). ¯ (4.15) E exact ({Ri , rn }) → E approx ({Ri }; ρ) 2 ij Note, however, that there is a remnant of the electronic degrees of freedom in the form of a dependence of the potentials on the mean electron density. The starting point for our free electron analysis is the assertion that to a ﬁrst approximation, simple metallic systems may be thought of as consisting of a uniform electron gas with a density determined by how many electrons each atom has donated to the ‘electron sea’. The underlying conceptual model is that

4.3 Pair Potentials

159

described in chap. 3 for electrons in a three-dimensional box. That model is now supplemented by imagining the box to contain not only the free electrons, but also the ions that have donated them. Our task is to compute the total energy of such a system. The presence of the ion cores which have donated the free electrons to the electron gas is then imagined to impose a weak periodic perturbation on the quiescent electron gas. For the present purposes, the key result is that within the conﬁnes of perturbation theory, if the effect of these ion cores is carried to second order in the weak perturbing potential, the total energy of the system may be written in real space in exactly the form of a pair potential. We have now advanced the view that the effect of the ionic cores may be treated as a weak perturbating potential Vp (r) on the free electron states discussed earlier. The presence of the perturbing potentials will have the effect of altering the free electron E k = h¯ 2 k 2 /2m, √ energies, (0) and the free electron wave functions, ψk (r ) = (1/ )eik·r . We begin by recalling that within quantum mechanical perturbation theory, the ﬁrst- and second-order corrections to the energy of the n th eigenstate, E n(1) and E n(2) , may be written as (1) E n = ψn(0)∗ (r)Vp (r)ψn(0) (r)d 3 r (4.16) and E n(2)

=

| ψ (0)∗ (r)Vp (r)ψ (0) (r)d 3 r|2 n k E n(0) − E k(0)

k=n

,

(4.17)

where Vp (r) is the perturbing potential derived from the ionic potentials, ψn(0) (r) is the n th wave function of the unperturbed system and E n(0) is the n th energy eigenvalue in the absence of the perturbation. The results written above should be thought of in the following context. Our preliminary investigation of the electrons in a metal was restricted to the assumption that the presence of the ionic cores is completely irrelevant. We solved this problem in the introductory sections on quantum mechanics in the last chapter. We have now introduced a periodic array of ionic potentials and have included their contribution to the total energy perturbatively. The picture at this point is that the total potential experienced by an electron in the box as a result of the presence of the ionic cores may be written as Vps (|r − Rn |). (4.18) V (r) = n

We have introduced the notation Vps to denote the atomic pseudopotentials. These pseudopotentials are meant to characterize the interaction of the valence (i.e. outer) electrons with the nucleus and its associated tightly bound core electrons. Our aim now is to assess the corrections to the total energy of the electron gas as a result of

160

4 Energetic Description of Cohesion in Solids

the perturbation due to the ionic cores. To begin with, we consider the alteration of the energy in ﬁrst-order perturbation theory. The change in energy of a plane wave state with √ wavevector k is obtained using eqn (4.16) with wave functions ψk(0) (r) = (1/ )eik·r and is given by 1 e−ik·r V (r)eik·r d 3 r. (4.19) E k(1) = We see immediately that this results in an energy shift E = (1/ ) V (r)d 3 r that is independent of the wavevector. As a result, the conclusion is that to ﬁrst order, the presence of the ionic cores does nothing more than impose a uniform shift on the energies of all of the free electron states. It is thus uninteresting as concerns different structural arrangements but contributes to the overall cohesive energy. We now look to second-order pertubation theory for a determination of a nontrivial change in the energy. Our strategy will be to ﬁrst compute the energy change associated with a state of a particular wavevector and, subsequently, to sum the change over all occupied states. The net result is the second-order energy change for the electron gas in the presence of a particular ionic conﬁguration. The second-order shift to a state with wavevector k is obtained using eqn (4.17), again √ (0) ik·r with wave functions ψk (r) = (1/ )e and energies E k(0) = h¯ 2 k 2 /2m and is given by 2 1 −ik·r i(k+q)·r 3 e V (r)e d r . (4.20) E k(2) = h¯ 2 2 q=0 2 (k − |k + q| ) 2m We now use eqn (4.18) to obtain 2 2 1 iq·Rn 1 iq·r 3 e Vps (r)e d r a N n . E k(2) = h¯ 2 2 q=0 2 (k − |k + q| ) 2m

(4.21)

We have used a simple relation between the total volume and the atomic volume a , namely, = N a . Note that the factors in the numerator are both of particularly simple forms, with the term involving Vps clearly revealed as the Fourier transform of the atomic pseudopotential. It is convenient to invoke the notational convention 1 iq·Rn S(q) = e , (4.22) N n

4.3 Pair Potentials

161

which is the structure factor and is only dependent upon the geometry of the ionic positions. If we replace the sum overq with the corresponding integral, using the well-worn identity q → (V /2π )3 d 3 q, our expression for the energy change to second order for the state with wavevector k is |S(q)|2 |Vps (q)|2 V (2) 3 . (4.23) d q Ek = (2π )3 h¯ 2 2 2 (k − |k + q| ) 2m Our claim is that this expression may now be manipulated in such a way that when it is time to sum the energy change over all of the occupied states, the total energy change will be seen as a sum over effective pair potentials. With the Fourier transform of the atomic pseudopotential in hand, it is possible to evaluate the energy change explicitly. However, rather than concerning ourselves with the particulars associated with the speciﬁc choice of pseudopotential, we will work in the abstract, holding a course that will reveal the emergence of the pair potential as an effective theory for the electronic degrees of freedom as quickly as possible. To demonstrate that the energy shift described above may be written as a sum over pair terms, we proceed as follows. Note that what we have done above is to identify the energy change to second order for the free electron state of wavevector k. In order to assess the total energy change of the free electron gas in the presence of the potentials due to the ionic cores, we must now sum over all of the occupied free electron states. This results in a second-order change in the band structure part of the total energy per atom of |S(q)|2 |Vps (q)|2 2 V band 3 d . (4.24) q E tot = N |k|≤k F (2π )3 h¯ 2 2 2 (k − |k + q| ) 2m Note that everything except for S(q) is structure-independent. By expanding the structure factor explicitly in terms of its deﬁnition given in eqn (4.22), it is evident that the energy has decomposed into a series of pair terms as 1 band E tot = φeff (Rm − Rn ), (4.25) 2N m,n with the effective pair interaction given by

iq·(Rm −Rn ) 4V |Vps (q)|2 3 e d q . (4.26) φeff (Rm − Rn ) = (2π )3 |k|≤k F h¯ 2 2 2 (k − |k + q| ) 2m We now note that in addition to the electronic contribution to the structural part of the energy, the term computed above must be supplemented by the repulsion between the ions. We should also note that if our emphasis had been on computing

162

4 Energetic Description of Cohesion in Solids

Fig. 4.4. Pair potentials for Al as computed using perturbation analysis (adapted from Hafner (1987)). The four separate potentials shown here reﬂect different treatments of the electron–electron interaction, where RPA, IU, LDA and VS refer to the names of different approximations used in the construction of potentials.

the potential itself, rather than on demonstrating the way in which the electronic degrees of freedom are subsumed in an effective potential, we could have worked out expressions in which the Fourier transform of the pseudopotential is used explicitly and in which the sums over k and q are performed explicitly leaving in the end a single one-dimensional integral. As a ﬁnal word of caution, it should be noted that we have been lax in our treatment of screening effects which would modify the quantitative details of what we have said, though not the overall argument concerning the integrating out of the electronic degrees of freedom. For further details, the reader is encouraged to consult Harrison (1980) or Hafner (1987). The outcome of a calculation such as that given above is not entirely unambiguous. In particular, the choice of atomic pseudopotential and the treatment of screening effects can lead to potentials with different qualitative features. For the sake of discussion, in ﬁg. 4.4 we show a series of pair potentials for Al developed using different schemes for handling these effects. For our purposes, the key insight to emerge from this analysis is that we have seen how, on the basis of a free electron picture of metals, one may systematically construct effective pair potentials. Though our primary emphasis will center on the calculation of energies, it is also worth remembering that the total energy serves as the basis for the determination of forces as well. In many instances (i.e. static relaxation or molecular dynamics), the

4.3 Pair Potentials

163

calculation of forces is a prerequisite to the performance of structural relaxation. If we are to consider a generic pair potential of the form 1 φ(Rmn ), (4.27) E tot = 2 mn then the force in the α th Cartesian direction on particle i is given by f iα = −

∂ E tot , ∂ Riα

(4.28)

where we have introduced the notation Riα to characterize the α th component of the position vector Ri . Explicit evaluation of the derivative we are instructed to perform results in the force (Riα − Rmα ) φ(Rim ) . (4.29) f iα = − Rim m Despite the virtues inherent in using pair potentials, they also exhibit certain physical features that are troubling. Once the total energy has been written in the pair potential form, we note that the bond strength is explicitly independent of the environment. What this means is that no matter how many neighbors atom i may have, its bond with atom j has energy φeff (Ri j ). In the next section, we will see that ab initio calculations suggest that the environmental independence presumed in pair potential models is a faulty assumption. In addition to this fundamental qualitative shortcoming, there are other quantitative problems as well. When we undertake an analysis of elastic properties in ensuing chapters, the conceptual foundations for the microscopic evaluation of the moduli will be laid in terms of pair potentials. This development will be made not so much out of necessity, but rather because the pair potential description lays bare the central idea behind the evaluation of the moduli. One of the outcomes of such an analysis will be the realization of just how restrictive is a pair potential description of the total energy (especially in those cases in which volume-dependent terms are neglected). We will show, for example, that for cubic crystals, the elastic moduli C12 and C44 are equal, in contradiction with observation. Though there are ways to soften this blow, fundamentally, the pair description is left wanting. A second difﬁculty with the pair potential description is manifest when we attempt to consider defect formation energies. Speciﬁcally, we will also show that the pair potential description implies a formation energy for vacancies that is a vast overestimate relative to the numbers found in experiment. As is true for the elastic moduli, there are modiﬁcations that can be considered, but not without a sense that the crucial physics is being ignored. In response to these difﬁculties, and others, concerted efforts have been made to extend our description of the energetics of

164

4 Energetic Description of Cohesion in Solids

solids without paying the full price of ab initio calculation. We undertake such analyses now.

4.4 Potentials with Environmental and Angular Dependence As we have noted above and will see in more detail later, the pair potential description is littered with difﬁculties. There are a few directions which can be taken that will be seen to cure some of them. We begin with a qualitative discussion of these issues, and turn in what follows to the development of both angular force schemes and effective medium theories that patch some of these troubles, primarily through the device of incorporating more of what we know about the nature of bonding in solids.

4.4.1 Diagnostics for Evaluating Potentials We begin with a few qualitative insights into where the pair potential description might be lacking. One question we might pose that could expose a particularly problematic assumption of a pair potential description would be: how does the strength of a given bond depend upon whether or not the atom is participating in other bonds? Using ﬁrst-principles calculations one can address this question systematically by repeatedly evaluating the strength of bonds for a range of different geometries. By ﬁrst-principles calculations, we mean fully quantum mechanical calculations that are, at least in principle, parameter-free. An example of this strategy is revealed in ﬁg. 4.5 where it is seen that the strength of the bond goes roughly inversely as the square root of the coordination number. That is, as the number of neighbors to a given atom increases, the energy associated with each bond goes down. The ﬁrst-principles calculations were performed by considering a number of different structures, some observed, others hypothetical, which have near-neighbor environments that differ considerably in terms of coordination number. For example, the diamond cubic structure features only four near-neighbor bonds while the fcc structure is characterized by twelve. The energies of each of these structures were computed using the type of ﬁrst-principles techniques to be described later in the chapter, and then the resulting energies were plotted in a normalized form that revealed the energy per bond. In the context of pair potentials, what do these results teach us? Stated simply, the conclusion is that the bond strength has a certain environmental dependence. As will become evident in what follows, this environmental dependence can be mimicked by a class of energy functionals that are known variously as effective medium theories, Finnis–Sinclair potentials, glue models, the embedded atom method and pair functionals.

4.4 Potentials with Environmental and Angular Dependence

165

Fig. 4.5. Energy per atom for a variety of different structures in Al having different coordination 1

numbers (after Payne et al. (1996)). The curve is a ﬁt to the functional form E = E 0 + α Z 2 + β Z , where Z refers to the coordination number of a given atom.

A second perspective on the weakness of pair potentials comes from a consideration of bond angles. For example, if we are to consider a simple pair potential of the Morse or Lennard–Jones form in which there is a minimum associated with the near-neighbor separation, it is difﬁcult to imagine how open structures such as those found in the covalent semiconductors could be stabilized. The argument in this case might go as follows: twelve bonds taking advantage of the near-neighbor separation is better than only four. As a result, we are inclined to the view that there must be something particularly energetically important about the existence of certain bond angles.

4.4.2 Pair Functionals At the next level of sophistication beyond pair potentials, a variety of methods which can broadly be classiﬁed as pair functionals have been developed. In keeping with the various surrogates for the full Hamiltonian introduced in eqns (4.4), (4.5) and (4.30), the total energy in the pair functional setting is given by 1 φ(Ri j ) + F(ρi ), (4.30) E exact ({Ri , rn }) → E approx [ρ(r), {Ri }] = 2 ij i as will be seen below. Pair functionals can be motivated in a number of different ways, a few of which will be taken up here. One route to pair functionals is to

166

4 Energetic Description of Cohesion in Solids

Fig. 4.6. Energy cost to embed ion in electron gas of particular density ( from Jacobsen et al. (1987)).

revisit the electron gas, seen in a different light from that discussed in the context of free electron pair potentials. The physical picture that we will adopt here may be summarized as follows. The question that is posed is what is the energy cost to deposit an ion into a homogeneous electron gas of density ρ? What is found and will be discussed at some level of detail below is that there is an optimum electronic density (i.e. an energy minimizing density), and that optimal density depends upon the identity of the ion being placed in the electron gas. Consideration of ﬁg. 4.6 reveals the outcome of a series of numerical calculations made using density functional theory for a host of elements. What is learned from these calculations is that an ion of a particular type has a taste as to what the optimal local electron density should be. This insight provides the opportunity to construct a new class of energy functional which overcomes some of the limitations of the pair potential description. The philosophy of the pair functional approach is perhaps best illustrated via a concrete example. Consider fcc Ni. In this case, we know on the basis of the results shown above, that the Ni atom prefers to live in a certain equilibrium electron density. As yet, we have not seen how to exploit this insight in the context of particular geometric arrangements of a series of Ni atoms. We may see our way through this difﬁculty as follows. If we center our attention on a particular Ni atom, we may think of it as being deposited in an electron gas, the density of which is dictated by the number and proximity of its neighbors. The hypothesized energy

4.4 Potentials with Environmental and Angular Dependence

167

functional that captures that dependence may be written as E embedding = F(ρ),

(4.31)

where we further suppose that the electron density of the electron gas that the Ni atom ﬁnds itself in is given by f (Ri j ). (4.32) ρi = j=i

This equation tells us how to determine the ‘density’ of the electron gas at the site of interest which we denote ρi in terms of the geometric disposition of the neighboring atoms. In particular, f (R) is a pairwise function that characterizes the decay of electronic density from a given site. Hence, if we wish to ﬁnd the contribution of atom j to the density at site i, the function f (R) evaluated at the distance R = |Ri − R j | tells us exactly how much electronic density bleeds off from site j onto its neighbors. To bring the development of the pair functional approach to its completion, we assume that the total energy may be divided into two parts; one part whose aim is to mimic the type of electron gas embedding terms envisaged above and another whose intent is to reﬂect the Coulombic (possibly screened) interactions between the various nuclei. As yet, we have examined the embedding energy on the basis of the quantum mechanics of the electron gas. We have argued that on the basis of legitimate numerical evidence from quantum calculations one can construct the functional F(ρ). On the other hand, a large body of work has been built around the idea of taking one’s cue from the quantum mechanical foundations laid above, but instead to assume a pragmatist’s position and to ﬁt the various functional forms on the basis of known data. The embedded atom method is predicated on the latter alternative, and posits a total energy of the form, 1 φ(Ri j ) + F(ρi ), (4.33) E tot = 2 ij i where the density on site i is given in turn by an equation of the form of eqn (4.32) above. Our appeal that pair potentials were inadequate for capturing many of the energetic features of real materials was founded in part upon the environmental dependence of the bond strengths, captured in ﬁg. 4.5. It is of interest to revisit this question in light of the simple embedding form adopted above. As with our discussion of the free electron pair potentials, our aim at the moment is not to discuss the optimal choice of embedding functions but rather to identify the extra physics that makes such energy functionals an improvement over pair potentials. For the sake of argument, consider the same near-neighbor model discussed earlier

168

4 Energetic Description of Cohesion in Solids

Fig. 4.7. Model geometries used to illustrate computation of total energy within pair functional formalism: (a) linear chain, (b) square lattice.

in which the density due to a single neighbor at the equilibrium distance Rnn is given by f 0 . Our aim now is to consider the energy/atom for a few distinct structures in order to explicitly exhibit the environmental dependence that was claimed to be of interest above, and to build facility in using this functional form. For the linear chain of atoms (see ﬁg. 4.7), the total energy per atom within the embedded atom context is given by E chain = φ(Rnn ) + F(2 f 0 ).

(4.34)

This result reﬂects the fact that every atom on the chain has an identical environment with two near neighbors at the equilibrium distance. If we continue along the lines set above and consider the total energy of the square lattice depicted in ﬁg. 4.7, it is seen to have a total energy of E square = 2φ(Rnn ) + F(4 f 0 ).

(4.35)

The analysis precedes similarly for other cases of interest, such as, for example, the fcc structure, which has a total energy of E f cc = 6φ(Rnn ) + F(12 f 0 ).

(4.36)

Note that in the absence of the embedding term the total energy per bond is constant √ as expected. However, if we adopt the form F(ρ) = ρ which will be motivated

4.4 Potentials with Environmental and Angular Dependence

169

Fig. 4.8. Universal binding energy relation (adapted from Rose et al. (1984)).

after we have introduced the tight-binding method, the energy per bond is clearly not constant. One of the cleanest routes to determining embedding functions is by invoking the universal binding energy relation (UBER) (Rose et al. 1984). On the basis of a vast collection of experience with ﬁrst-principles calculations of a range of materials, it was found that the total energy as a function of lattice parameter may be ﬁtted to

r −α( r −1) E tot (r ) = −E c 1 + α − 1 e r0 , (4.37) r0 where r is a measure of the interatomic separation and α and r0 are scaling parameters which collapse the speciﬁc material data onto the universal curve. An example of this scaling behavior as a function of the lattice parameter for a range of materials is shown in ﬁg. 4.8. This form for the total energy suggests a strategy for constructing embedding functions via the following argument. We assume the pair potential is of some speciﬁed form. Once this form is adopted, the embedding function may be deduced as the difference between the total energy as given by the universal binding energy relation and the total contribution to the pair potential. To illustrate this procedure, we follow Johnson (1988) by assuming a nearneighbor only interaction. Hence, as was shown in eqn (4.36), the energy of a given atom is E i = F(ρi ) + 6φ(Rnn ). If we now assert that the left hand side

170

4 Energetic Description of Cohesion in Solids

of this equation is determined by the universal binding energy relation, then the embedding function is F[ρ(R)] = E UBER (R) − 6φ(R).

(4.38)

Johnson makes the explicit choice of density function ρ(r ) = f e

−β( rr −1) 0

,

(4.39)

and deﬁnes the pair potential as φ(r ) = φ0 e

−γ ( rr −1) 0

.

(4.40)

Note that we have imitated Johnson’s notation in which the quantity f is a constant factor that appears in the determination of the density ρ, and the parameters r0 , β, γ and φ0 are other parameters that are determined through the ﬁtting procedure. Once the density function and the pair potential have been speciﬁed, the determination of the embedding function is complete in principle. In this case, because of the choice of functions, the relevant equations can be solved analytically with the result that the embedding energy is given by βα γβ α ρ ρ ρ F(ρ) = −E c 1 − ln − 6φ0 . (4.41) β ρ0 ρ0 ρ0 The basic strategy used in deriving this form for the embedding function is the recognition that the density function ρ(r ) may be inverted to yield 1 ρ(r ) r − 1 = − ln , r0 β ρ0

(4.42)

where ρ0 is the density when the interatomic separation is r0 . This form for the embedding energy is contrasted with others in ﬁg. 4.9. The central importance of this particular embedding strategy is that now that the analytic form is in hand, it is possible to examine a range of secondary quantities such as the elastic moduli, surface energies and point defect formation energies analytically. Of course, there exist signiﬁcantly more sophisticated (and accurate) schemes for carrying out pair functional calculations. While such functions may be preferable in the attempt to calculate real material properties, the Johnson potential serves as an ideal pedagogic vehicle for discussing embedding energies. From the standpoint of ‘back of the envelope’ exercises, one may use analytic near-neighbor models such as that proposed by Johnson to estimate quantities ranging from the (111) surface energy to the vacancy formation energy. In addition to the importance of energies, a number of situations demand a knowledge of the forces between atoms. We have already seen in eqn (4.29) how forces are computed within the pair potential setting. The presence of the

4.4 Potentials with Environmental and Angular Dependence

171

Fig. 4.9. Various representations of the embedding energy for Cu (adapted from Johnson (1988)). The solid curve is the embedding function for Cu derived from UBER as described in text, the dashed curve is a ﬁt for the embedding function and the dotted curve corresponds to an embedding function √ of the Finnis–Sinclair form in which F(ρ) ∝ ρ.

embedding term in the pair functional setting leads to additional subtlety in the computation of forces. In particular, the expression for the force on the i th atom due to the embedding term is given by ˆ ji , fi = − (F (ρ j )ρi + F (ρi )ρ j )R (4.43) j=i

ˆ ji is the unit vector pointing from the j th to the i th atom. It is left to the where R reader to derive this result explicitly in the problems at the end of the chapter. A ﬁnal intriguing point about energy functionals like those described in this section is that they may be transformed into an effective pair potential description of the total energy. This claim is an interesting example of the various layers in effective theory construction and reﬂects a transformation of the form 1 E approx [ρ(r), {Ri }] → E approx ({Ri }; ρref ) = Veff (Ri j ; ρref ), (4.44) 2 ij where ρref denotes the dependence of the resulting pair potential on a reference density. Thus, the effective pair potential developed to describe bulk environments will differ considerably from that derived to account for free surfaces. Indeed, these potentials will reﬂect exactly the environment-dependent bond strengthening that is the hallmark of the pair functional approach. The reader is asked to ﬁll in the details of this development in the problem section at the end of the chapter.

172

4 Energetic Description of Cohesion in Solids

4.4.3 Angular Forces: A First Look There are some circumstances in which the inclusion of the ‘many-body’ terms present in pair functionals is insufﬁcient and recourse must be made to angular terms. As yet, our discussion has been dominated by metals. On the other hand, more than ﬁfty different potentials have grown up around the question of how best to model covalent materials, with Si as the dominant example. One of the remarkable features of Si in the solid state is its open structure, characterized by only four neighboring atoms in the ﬁrst neighbor shell in contrast with the twelve neighbors found in close-packed structures. As a result of this structural clue, it seems that the insistence on the coupling between bond lengths and energy must be supplemented by consideration of the energetics of bond angles. As will be seen below, both angular potentials and cluster functionals have been developed to characterize materials such as Si. Our aim here is to give a ﬂavor of these developments by recourse to two of the most celebrated total energy schemes used in semiconductors: the Stillinger–Weber angular potentials and the Tersoff cluster functional. The Stillinger–Weber potentials were developed with the mind of explaining the condensed phases of Si, including the fact that in the liquid state, the coordination number of Si atoms increases. The basic structure of the Stillinger–Weber potential is revealed in the expression for the total energy which is 1 1 V2 (Ri j ) + V3 (Ri , R j , Rk ), (4.45) E tot ({Ri }) = 2 i, j 3! i, j,k with the ﬁrst term corresponding to a pair potential of the type with which we are already familiar, and the second term is an angular term which imposes penalties when the angles in three-atom triangles deviate from particularly stable values. The potentials themselves are represented as Ri j , (4.46) V2 (Ri j ) = f 2 σ and

V3 (Ri , R j , Rk ) = f 3

Ri R j Rk , , . σ σ σ

The functions f 2 (Ri j ) and f 3 (Ri , R j , Rk ) are deﬁned by −1 A(B R − p − R −q )e[(r −a) ] if r < a f 2 (R) = 0 otherwise

(4.47)

(4.48)

and f 3 (Ri , R j , Rk ) = h(Ri j , Rik , θ jik ) + h(R ji , R jk , θi jk ) + h(Rki , Rk j , θik j ). (4.49)

4.4 Potentials with Environmental and Angular Dependence

173

Fig. 4.10. Stillinger–Weber angular term.

The novel feature associated with the Stillinger–Weber potentials is this angular term. To be more speciﬁc, the three-body terms have an angular dependence of the form 1 2 −1 −1 , (4.50) h(Ri j , Rik , θ jik ) = λe[γ (Ri j −a) +γ (Rik −a) ] cos θ jik + 3 where only the angle-dependent part of this function is shown in ﬁg. 4.10. Recall that in our discussion of pair potentials, structural stability was attributed to the fact that particular structures have bond lengths that take advantage of minima in the pair potential. On the other hand, the existence of angular potentials paves the way for a second form of correspondence between structure and energetics. In particular, now not only must bond length constraints be satisﬁed, but bond angle constraints as well. In this case, we see that the angular term is minimized in the case that θ ≈ 109.47◦ , corresponding to the favorability of the tetrahedral angles that characterize the sp3 bonding in many covalent materials. The computation of the total energy in the context of a total energy scheme involving angular forces is quite analogous to that considered in the pair potential setting. Indeed, that part of the energy due to the pair potential terms is identical to those considered earlier. However, the angular terms involve a more careful analysis of the neighbor environment for a given atom. In particular, these terms require that a three-body contribution to the total energy be made for each and every triplet of atoms in which the distances between neighbors are smaller than the range of V3 . To illustrate the reckoning of these three-body contributions

174

4 Energetic Description of Cohesion in Solids

Fig. 4.11. Schematic of the triangular lattice used in computing the total energy using angular forces.

to the total energy, we consider the simple case of the perfect two-dimensional triangular lattice shown in ﬁg. 4.11, and we further assume that the range of V3 is chosen such that only near-neighbor atoms are considered. Given these simplifying assumptions, the total energy per atom may be computed as E tot = 3V2 (Rnn ) + 6h(Rnn , 60◦ ) + 6h(Rnn , 120◦ ) + 3h(Rnn , 180◦ ),

(4.51)

where we have used the notation h(Rnn , θ) = h(Rnn , Rnn , θ ). The contribution of the angular term was arrived at by noting that by translational invariance, each and every atom has an identical local environment. In more complicated geometrical situations, the strategy required is similar. Essentially, it is necessary to ﬁnd all three-atom clusters that are within the required proximity and to sum up their contributions separately. Note that our example is especially artiﬁcial in the context of the Stillinger– Weber potential since for the triangular lattice it is 60◦ angles, and not the tetrahedral angles, that form the central angular motif. However, our reason for including this example is not to argue for the stability of the triangular lattice in the Stillinger–Weber context, but rather to show how calculations are made using this potential. We also note that in the remainder of the book, the Stillinger–Weber potential will often be invoked as the model of choice for discussing empirical treatments of Si in much the same way that the Johnson potential will serve as one of our key paradigms for pair functionals. The Stillinger–Weber scheme lacks the explicit environmental dependence that was argued to be of importance in our discussion of pair functionals. However, environmental dependence has been accounted for in covalent materials as well. Tersoff (1988) was one of the ﬁrst to suggest such a scheme, and his total energy

4.4 Potentials with Environmental and Angular Dependence

175

takes the form E tot =

1 r [V (Ri j ) + bi j V a (Ri j )], 2 ij

(4.52)

where V r (Ri j ) is a repulsive potential of the form Ae−λ1 Ri j and, similarly, V a (Ri j ) is an attractive potential of the form Be−λ2 Ri j . As Tersoff notes, the key novelty is buried in the function bi j . Indeed, it is via this function that both the environmental and angular dependences enter the potential. The form adopted by Tersoff is bi j = (1 + β n ζinj )(−1/2n) ,

(4.53)

where the function ζi j is in turn given by f c (Rik )g(θi jk ). ζi j =

(4.54)

k=i j

The function f c (R) is a cutoff function and passes quickly but smoothly from unity to zero as R → Rc , where Rc is a cutoff distance. The function g(θi jk ) is an angular term of the form g(θ ) = 1 +

c2 c2 − . d 2 d 2 + (h − cos θ )2

(4.55)

While these potentials are notationally complex, they are conceptually simple in terms of the basic physics they incorporate. In particular, potentials of this type invoke both of the new physical ideas presented in this section: environmental dependence and angular forces. In particular, the quantity denoted bi j guarantees that the interaction between two given atoms will depend upon both the number and disposition of neighboring atoms. For our purposes, the key advantage of the Tersoff potential is its attempt to capture effects which are outside of the purview of more traditional potentials. The Stillinger–Weber and Tersoff schemes as introduced above are essentially ad hoc. In forthcoming chapters, we will describe some of the successes and shortcomings of models like these. These examples will show that it is important to build intuition concerning the bonding in solids in order to formulate a clear idea as to when a particular empirical description of the energy is suitable and when it can be expected to fail. One way to service this ambition is to develop a more systematic scheme for deriving such potentials, or if not deriving them, then at least developing plausibility arguments for their functional form. The tack adopted here is to appeal to an understanding of the electronic structure of a material with special reference to the electronic density of states and its moments (which will be deﬁned shortly).

176

4 Energetic Description of Cohesion in Solids

4.5 Tight-Binding Calculations of the Total Energy Thus far, our emphasis has been on methods in which no explicit reference is made to the electronic degrees of freedom. In the present section we make our ﬁrst concession in the direction of incorporating electronic structure information into the total energy in the form of the tight-binding method. From the perspective of the general discussion given at the beginning of the chapter, the tight-binding total energy can be thought of in terms of the replacement E exact ({Ri , rn }) → E approx ({Ri , αi }),

(4.56)

where the coefﬁcients {αi } are expansion coefﬁcients that characterize the electronic wave function. That is, the tight-binding scheme represents an approximate treatment of the electronic structure of the material. The rudiments of the tight-binding method can be spelled out as follows. First, we take our cue from the discussion of the H2 molecule given in chap. 3, where we noted that the total molecular wave function could be written as a linear combination of atomic wave functions centered on the various sites making up the molecule. In the case of a solid, we will adopt the same strategy, this time with the electronic wave function of the entire solid being built up as a linear combination of the atomic wave functions centered on the various sites that make up the solid. The coefﬁcients in the linear combination of these basis functions will then be thought of as variational parameters, chosen so as to obtain the lowest possible energy. Finally, the resulting Hamiltonian matrix is diagonalized with the resulting eigenvalues serving as the basis for the calculation of the electronic contribution to the total energy. The tight-binding method will be exploited in two distinct senses. The ﬁrst main thrust of this section will be to show how the tight-binding method can be used to compute the total energy directly without recourse to some reduced description in terms of pair functionals or angular forces. Secondly, tight-binding arguments will be invoked in order to provide a plausibility argument for the form of both the pair functionals and angular potentials introduced in previous sections. Ultimately, the potentials will be seen to inherit the angular features of the moments of the electronic density of states. Prior to undertaking either of these objectives, we must ﬁrst describe the tight-binding method itself. 4.5.1 The Tight-Binding Method The tight-binding method is based upon the same set of observations that inspired the approach to molecular bonding introduced in chap. 3. We imagine that in the act of assembling the solid, the wave functions that characterize the isolated atoms are viable building blocks for describing even the complex wave function appropriate to the solid. When atoms are brought into one another’s proximity, the

4.5 Tight-Binding Calculations of the Total Energy

177

atomic energy levels associated with the outer valence electrons are disturbed as a result of the overlap of wave functions on adjacent atoms. This simple observation leads to a naive picture of the formation of the chemical bond. In particular, by summing up the occupied one-electron eigenvalues, one determines the electronic part of the total energy. As was shown in ﬁg. 3.13, as the number of atoms participating in the molecule increases, the resulting electronic spectrum becomes increasingly complex. Our discussion of the tight-binding method is intended to set forth in quantitative detail the recipe for computing the one-electron eigenvalues for solids. As noted already, the starting point of the analysis is an approximation to the total electronic wave function for the solid. In particular, we seek a wave function of the form n N aiα φα (r − Ri ), (4.57) ψ(r) = i=1 α=1

which we will write more compactly as |ψ =

N n

aiα |i, α.

(4.58)

i=1 α=1

The sum over i in eqns (4.57) and (4.58) runs over the number of atoms N in the solid, while the sum on α is over the number of orbitals per site. The atomic-like orbital of type α centered on site i is written as |i, α = φα (r − Ri ). Indeed, the nature of these orbitals and the size of the parameter n strikes right to the heart of the minimalist character of the semiempirical tight-binding method. As an example of the characteristics of the type of basis |i, α that might be used in a tight-binding calculation, we consider two distinct cases, that of Si, a covalently bonded semiconductor with an energy gap, and W, a transition metal with an electronic structure that is dominated by its d-electrons. We consider both examples, since each sheds different light on the questions that arise in the tight-binding context. As mentioned above, the basic spirit of tight-binding theory is minimalist in the sense that one searches for the smallest possible basis for expanding the total wave function. For the case of W, this might mean considering only ﬁve d-orbitals per atom. Recall from the discussion of chap. 3 that the solution of the atomic hydrogen problem resulted in a series of energy eigenvalues and their associated wave functions. These solutions could be organized along the lines of their angular momenta, with the possibility of s-orbitals (l = 0), p-orbitals (l = 1), d-orbitals (l = 2) and so on. For the case at hand, it is the 5d orbitals of W that serve as our basis. That is, each W atom has electrons from the 5d shell which contribute to the overall electronic wave function for the solid. We also observe that if we are interested in Si, for example, rather than

178

4 Energetic Description of Cohesion in Solids

W, our expansion will center on the outer 3s and 3p electrons. In this case, the total wave function is built up out of the four such basis functions at each site which for the i th site we label as |i, 3s, |i, 3px , |i, 3p y and |i, 3pz . Note that in keeping with our aim to shed unnecessary degrees of freedom, all reference to core electrons has been omitted; they are assumed to be unchanged by the proximity of neighboring atoms. In addition, the basis itself is incomplete in the mathematical sense, since we have not included higher energy atomic states such as |i, 4s, etc. in the basis. Having identiﬁed the nature of our approximation to the wave function, the next step in the argument concerns the evaluation of the energy. In particular, we aim to determine the series of coefﬁcients aiα which state with what weight the α th orbital on site i (i.e. |i, α) contributes to the total wave function |ψ. The scheme is to construct an energy function that depends upon the set of coefﬁcients aiα and to ﬁnd the values of those coefﬁcients that minimize that energy. Just as was done in our ﬁnite element treatment of the Schr¨odinger equation in chap. 3, we have replaced the problem of ﬁnding unknown functions (i.e. the wave functions) with that of ﬁnding unknown coefﬁcients through the device of writing the energy function ({aiα }) = ψ| Hˆ |ψ − Eψ|ψ,

(4.59)

where it is understood that the wave function ψ depends explicitly on the as-yet undetermined coefﬁcients aiα . Substitution of the total wave function given in eqn (4.58) into eqn (4.59) results in ({aiα }) =

N n

αβ

αβ

∗ (h i j − E Si j )aiα a jβ ,

(4.60)

i, j=1 α,β=1

where we have introduced the notation αβ ˆ φα∗ (r − Ri ) Hˆ φβ (r − R j )d 3 r, h i j = i, α| H | j, β =

(4.61)

and αβ Si j

= i, α| j, β = αβ

φα∗ (r − Ri )φβ (r − R j )d 3 r. αβ

(4.62)

The nature of the matrices h i j and Si j is subtle and as a result has been tackled from a number of different perspectives. Since our aim is to present ideas rather than to give an exhaustive description of each and every alternative approach to a given problem, the present discussion will try to highlight some of αβ the distinguishing features of these quantities. The matrix Si j provides a measure of the overlap of wave functions on adjacent sites, and is often described as the ‘overlap matrix’. For the purposes of the present discussion, we adopt the simplest

4.5 Tight-Binding Calculations of the Total Energy

179

approximation of orthonormality which is characterized mathematically as αβ

Si j = δi j δαβ ,

(4.63)

with the proviso that nonorthogonal tight-binding methods have much to recommend them and hence, the interested reader should pursue this matter further. αβ We make equally strong approximations in the context of the matrix h i j as well by resorting to the so-called two-center approximation. The basic idea of this approximation may be understood in qualitative terms by noting that the total Hamiltonian is constructed as a sum of potentials arising from the different atoms N (i.e. V (r) = i=1 Vatom (r − Ri )). The essence of the two-center approximation αβ is to say that the only terms from V (r) contributing to h i j are those arising from Vatom (r − Ri ) or Vatom (r − R j ). Within this approximation, a given matrix element depends upon both the separation and relative orientation of atoms i and j. The interactions between orbitals on different sites can be parameterized in terms of certain energetic factors Vssσ , Vppσ , etc. and the direction cosines l, m, n of the vector connecting the i th and j th atoms. As yet, however, our discussion has been generic and has not revealed insights into the nature of the tight-binding matrix elements themselves. To best see in qualitative terms where these matrix elements come from, we return to the simpler molecular setting. Recall that the orbitals of different angular momentum character have wave functions characterized by different numbers of lobes. An s-orbital is spherically symmetric, while p-orbitals have single lobes. As a result, the matrix elements which parameterize the interactions between orbitals on different sites depend exclusively on geometric/symmetry characteristics of the participating orbitals and, in particular, on the symmetry of these orbitals about the axis joining the two sites of interest. For example, for s-orbitals, the symmetry about the bond axis is such that we can rotate the orbitals about the bond axis with impunity (i.e. there is axial symmetry). Such bonds are labeled as σ bonds, and lead to the coupling Vssσ . However, axial symmetry bonds can also occur for p-orbitals. For example, if we have two atoms aligned along the z-axis, and consider the interaction between the pz -orbital on the ﬁrst atom and the pz -orbital on the second atom, this too has azimuthal symmetry and is parameterized by the coupling Vppσ . On the other hand, if we consider the coupling of pz -orbitals between two atoms that are neighbors along the x-axis, then the symmetry of their coupling is denoted by π, and leads to couplings of the form Vppπ . The geometry of orbitals associated with these couplings is depicted in ﬁg. 4.12. We take up the question of how precisely parameters such as Vssσ , Vppσ , Vppπ , Vddσ , etc. are determined later in this section. p p For example, for two p y -orbitals, the matrix element h i jy y can be split up into a term involving Vppσ and a second term involving Vppπ . As a result of these

180

4 Energetic Description of Cohesion in Solids

s Vss px

s Vsp -Vsp px states

px Vpp px

py Vpp py

states pz Vpp pz

Fig. 4.12. Schematic indication of the different symmetry types associated with couplings between orbitals on different sites (adapted from Harrison (1980)).

4.5 Tight-Binding Calculations of the Total Energy

181

Fig. 4.13. Radial dependence of the tight-binding coupling parameters for Si (adapted from Kwon et al. (1994)).

arguments, the calculation of the Hamiltonian matrix is reduced to a series of simple geometric operations (i.e. the determination of the direction cosines of the vector joining the two atoms of interest) in conjunction with a table known as the Slater–Koster table which illustrates how two orbitals are coupled. In addition to the dependence of the coupling between two sites on the relative orientation of the vector joining them, there is also a strong dependence of these couplings on the distance between the two sites. An example of the radial dependence of these couplings is shown in ﬁg. 4.13. Once the Hamiltonian matrix is in hand, the next step in the procedure is to seek the energy minimizing coefﬁcients {aiα }. This minimization is effected by ∗ computing ∂/∂aiα = 0 for all i and α, and results in a series of coupled algebraic equations that may be written in matrix form as (Hpp − Eδ pp )a p = 0, (4.64) p

where we have introduced the superindex p that runs from 1 to n N , with each p corresponding to a different one of the n N choices of i and α. This implies that we will have n N equations in the unknowns {aiα }. The result of solving these equations will be n N different energy eigenvalues and their corresponding set of expansion coefﬁcients which in turn determine the wave function itself. What has been learned thus far? We have noted that in the context of our truncated basis, built from the atomic orbitals characterizing the free atoms, the

182

4 Energetic Description of Cohesion in Solids

solution of the Schr¨odinger equation is mapped onto the equivalent problem of ﬁnding that set of expansion coefﬁcients that minimize the total energy. Like in the ﬁnite element context discussed earlier, minimization problems of this type lead to coupled equations such as that found in eqn (4.64). From the point of view of that set of equations, our problem has been reduced to a series of coupled linear algebraic equations and to ﬁnd the undetermined coefﬁcients we must diagonalize the Hamiltonian matrix. The result of this exercise is a series of energy eigenvalues that represent, within the conﬁnes of the present model, the allowed energy states of the solid. The spectrum of energy eigenvalues that emerge from the type of calculation spelled out above can be complex in the sense that there can be a large number of such eigenvalues spread across a wide range of energies. One way to tame this complexity is by virtue of the electronic density of states (DOS). The density of states is essentially a histogram that characterizes the distribution of eigenvalues which arise from solving problems concerning either the vibrational or electronic states of solids. In particular, the electronic density of states is deﬁned as δ(E − E i ), (4.65) ρ(E) = i

where the sum i is over the energy eigenvalues. Our present objective is to develop an understanding of the physical origins of these eigenvalues in the context of the electronic structure of a material. We already saw a schematic example of such a density of states in ﬁg. 3.13 which shows the densities of states for a series of model problems treated in the one-electron framework adopted in chap. 3. The vertical axis in that ﬁgure speciﬁes the energy of a given eigenstate. The more complex tight-binding analysis introduced here results in n N eigenvalues which may be used within the context of eqn (4.65) to obtain the density of states. Once the density of states has been determined, the electronic contribution to the energy may be obtained by summing the energies of all the occupied states. In terms of the density of states itself, this amounts to an evaluation of the integral F ρ(E)Ed E, (4.66) E el = 2 −∞

where the factor of 2 accounts for the fact that each state may be occupied by an electron of two different spins. The equation written above is the continuum limit of the discrete sum over energy eigenvalues (i.e. E el = 2 i i ) that we adopted earlier. In order to compute the total energy, the electronic term introduced above must be supplemented by a phenomenological treatment of those terms left out of the tight-binding description including the interactions between the various nuclei.

4.5 Tight-Binding Calculations of the Total Energy

183

This extra piece of the energy is often represented as a pair potential resulting in a total energy of the form F 1 Veff (Ri j ) + 2 Eρ(E)d E. (4.67) E tot ({Ri }) = 2 ij −∞ The effective pair potential can be determined by insisting that certain properties such as the lattice parameter, the cohesive energy and the bulk modulus are accurately reproduced. Of course, more sophisticated ﬁtting schemes are also possible. From a more concrete perspective, the application of eqn (4.67) is carried out as follows. A computational cell is considered in which the set of nuclear coordinates {Ri } is known. Given these coordinates, it is then possible to determine the various αβ matrix elements h i j which characterize the coupling of the α th orbital on site i to the β th orbital on site j. By assembling all such matrix elements, the full Hamiltonian matrix is thus known, and one can resort to either k-space or real space methods to determine the all-important density of states, ρ(E). Given this density of states, the electronic contribution to the total energy is determined by carrying out the integration indicated in eqn (4.67). The Fermi level itself (i.e. the upper limit of the integral) is determined by insisting that the atoms have the appropriate number of electrons. By tuning the Fermi energy, one tunes between the empty band and full band limits. In addition to the electronic term, we are also required to consider the pair term which demands lattice sums no different than those undertaken in our discussion of pair potentials. This procedure, therefore, gives an unambiguous transcription between a set of atomic positions and a corresponding total energy, thus paving the way for the investigation of questions relating to the coupling of structure and material properties. In chap. 6, we will return to the types of total energy analysis discussed here with special reference to the ability of tight-binding models to capture the relative energetics of competing crystal structures. In addition, in subsequent chapters, we will repeatedly make reference to the application of these methods for examining the energetics of a wide range of processes and mechanisms. The tight-binding method is a convenient entry level way to undertake calculations of the total energy in which reference to the electronic degrees of freedom is made explicitly. In addition, it has the added virtue that the calculations are computationally less demanding than those involving a more faithful treatment of the electronic degrees of freedom. Despite our ability to now write down with some level of conﬁdence the tight-binding description, our treatment has been overly cavalier in that we have as yet not stated how one might go about determining the Hamiltonian matrix αβ elements, h i j . Note that in precise terms these matrix elements describe the

184

4 Energetic Description of Cohesion in Solids

coupling between orbitals of character α and β on sites i and j, respectively. The basic thrust of the type of semiempirical tight-binding theories that it is our aim to discuss here is to assume that the interactions between orbitals on different sites may be empirically parameterized (through the parameters Vssσ , Vspσ , etc.) without ever really entering the debate as to the fundamental interactions between nuclei and electrons. The question of how to go about determining these ﬁtting parameters will be taken up once we have seen how the tight-binding description is carried out in the context of periodic solids. 4.5.2 An Aside on Periodic Solids: k-space Methods The description of tight binding introduced above advanced no assumptions about the symmetries present in the atomic-level geometry. As a result, the Hamiltonian matrix and the symmetries of the eigenfunctions deﬁed any generic classiﬁcation of the states along lines of their symmetries. On the other hand, in crystalline solids, the existence of translational symmetry leads to the expectation that the wave functions will have very special properties that guarantee that the charge density is the same in every unit cell. In particular, the existence of translational symmetries gives rise to so-called k-space methods which are the thrust of the present discussion. We specialize our discussion to periodic solids with the recognition that there are a wide variety of problems for which translational symmetry is lacking and that will therefore demand the more general perspective introduced above. Because of the presence of the regularity associated with a crystal with periodicity, we may invoke Bloch’s theorem which asserts that the wave function in one cell of the crystal differs from that in another by a phase factor. In particular, using the notation from earlier in this section, the total wave function for a periodic solid with one atom per unit cell is 1

|ψk = √ nN

n N

aα eik·Ri |i, α.

(4.68)

i=1 α=1

The ﬁrst sum is over cells, the i th of which is speciﬁed by the Bravais lattice vector Ri , while the second sum is over the set of orbitals α which are assumed to be centered on each site and participating in the formation of the solid. If there were more than one atom per unit cell, we would be required to introduce an additional index in eqn (4.68) and an attendant sum over the atoms within the unit cell. We leave these elaborations to the reader. Because of the translational periodicity, we know much more about the solution than we did in the case represented by eqn (4.58). This knowledge reveals itself when we imitate the procedure described earlier in that instead of having n N algebraic equations in the n N unknown

4.5 Tight-Binding Calculations of the Total Energy

185

coefﬁcients aiα , translational symmetry collapses the problem into a series of n coupled algebraic equations in the n unknowns aα , where n is the number of orbitals on each site. Imitating the treatment given in eqn (4.60), we can once again elucidate our variational strategy, but this time with the added knowledge that the wave function takes the special form given in eqn (4.68). In particular, the function we aim to minimize is (4.69) periodic ({aα }) = ψk | Hˆ |ψk − E k ψk |ψk , which in light of eqn (4.68) may be rewritten as periodic ({aα }) =

N n n j=1 α=1 β=1

αβ

eik·Rj aα∗ aβ h i j − E k

n α=1

aα∗ aα .

(4.70)

The energy eigenstates in the periodic case are labeled by the wave vector k. If we now seek those aα s that minimize eqn (4.70), and introduce the notation Hαβ (k) =

N

αβ

h i j eik·Rj ,

(4.71)

j=1

then the resulting problem may be rewritten as (Hαβ (k) − E k δαβ )aβ = 0.

(4.72)

β

The structure of our result is identical to that obtained in eqn (4.64) in the absence of any consideration of crystal symmetry. On the other hand, it should be remarked that the dimensionality of the matrix in this case is equal to the number of orbitals per atom, n, rather than the product n N (our statements are based on the assumption that there is only one atom per cell). As a result of the derivation given above, in order to compute the eigenvalues for a periodic solid, we must ﬁrst construct the Hamiltonian matrix H(k) and then repeatedly ﬁnd its eigenvalues for each k-point. Thus, rather than carrying out one matrix diagonalization on a matrix of dimension n N × n N , in principle, we carry out N diagonalizations of an n × n matrix. To complete the description, it is also necessary to understand the nature of the k-vectors themselves. For the purposes of the present discussion, we consider a one-dimensional periodic chain along the x-direction of N atoms with a spacing a between the atoms on the chain. One statement of Bloch’s theorem, which we set forth in one-dimensional language, is the assertion that the wave function in the n th cell ψn and that in the (n + 1)th cell, ψn+1 is given by ψn+1 = eika ψn .

(4.73)

186

4 Energetic Description of Cohesion in Solids

The periodicity of this one-dimensional crystal implies that ψ1 = ψ N +1 , or eik N a = 1,

(4.74)

which illustrates that the allowed k-vectors are of the form kn =

2πn , Na

(4.75)

where the integer n can assume the values 0, 1, . . . , N − 1. This collection of vectors deﬁnes a ﬁnite region in k-space known as the ﬁrst Brillouin zone. For the one-dimensional case being discussed here, it is convenient to consider the N vectors that run between −π/a and π/a. The three-dimensional analogs of the concepts introduced here involve no particular subtlety and are left to the reader as an exercise. In addition, further elaboration of these concepts can be found in Ashcroft and Mermin (1976). To illustrate the ideas presented above in concrete form, we now consider two separate one-dimensional examples of increasing sophistication. In the ﬁrst case, we consider a one-dimensional periodic solid and examine a tight-binding basis that consists of one s-orbital per site. As seen from the deﬁnition of the matrix H(k) given in eqn (4.71), this case is elementary since the Hamiltonian matrix itself is one-dimensional and may be written as H (k) = heika + he−ika ,

(4.76)

where we have introduced the parameter h to characterize the coupling between orbitals on neighboring sites. All interactions beyond those at the near-neighbor level are neglected and we have assumed that the ‘on-site’ coupling (i.e. i|H |i) is zero. Hence, the outcome of this calculation is a dispersion relation for the electronic states of the form E(k) = 2h cos ka.

(4.77)

This dispersion relation is plotted in ﬁg. 4.14. A more revealing example is provided by that of a linear chain in which each atom has four-basis functions, namely, s, px , p y and pz . This basis is of the same variety as that which is often used in the analysis of Si. In the present setting, the Hamiltonian matrix H(k) is obtained by recourse to the deﬁnition of eqn (4.71). In particular, we note that in the one-dimensional setting considered here, there p p p p ss are only six nonvanishing matrix elements, namely, h i,i = s , h i,ix x = h i,iy y = p p pz pz p p sp y y x x x ss h i,i = p , h i,i±1 = Vssσ , h i,i±1 = Vppσ , h i,i±1 = Vspσ and h i,i±1 = Vppπ . As a

4.5 Tight-Binding Calculations of the Total Energy

187

Fig. 4.14. Dispersion relation for a one-dimensional s-band tight-binding model.

result, the Hamiltonian matrix can be written down immediately as H(k) = s + 2Vssσ cos ka

2Vspσ cos ka 0 0

2Vspσ cos ka

0

0

p + 2Vppσ cos ka

0

0

0

p + 2Vppπ cos ka

0

0

0

p + 2Vppπ cos ka

.

(4.78) Because the structure of this matrix involves only a 2 × 2 subblock that is nondiagonal, two of the four energy bands are already determined and are degenerate with the form E(k) = p + 2Vppπ cos ka.

(4.79)

To ﬁnd the remaining two energy bands, we diagonalize the remaining 2 × 2 piece with the result that s + p + (Vssσ + Vppσ ) cos ka E ± (k) = 2 1 1 2 ) cos2 ka] 2 , ± [()2 + 4(Vσ )() cos ka + (4(Vσ )2 + 16Vspσ 2 (4.80) where we have introduced the notation = s − p and Vσ = Vssσ − Vppσ .

188

4 Energetic Description of Cohesion in Solids

Given our discussion of the band structures that arise on the basis of tightbinding arguments, we are now prepared to look a little more deeply into the logic behind the ﬁtting of tight-binding parameters. It is not really possible to provide any deﬁnitive statement which encompasses the diversity of ideas that have been brought to bear on the question of how best to determine tight-binding parameters. Evidently, there are any of a number of different schemes, many of which are founded on a sensible rationale. On the one hand, it is possible to imagine constructing parameterizations on the basis of the goodness of the ﬁt to the band structure itself. In these cases, one notes that the values of the energy at certain k-points within the Brillouin zone can be determined simply in terms of the unknown tight-binding parameters, with the result that a ﬁt is possible. However, in another sense, it is often the total energy that is of concern, so one can imagine determining the tight-binding parameters on the basis of energetic criteria. In either case, the central idea is more or less to determine the tight-binding expressions for a series of properties of interest a1 , a2 , . . . , an . In each case, from the tight-binding perspective, these properties are functions of the unknown parameters, and one’s task is to determine these parameters on the basis of these constraints. In mathematical terms, we are noting that f 1 (Vssσ , Vspσ , . . .) = a1 , f 2 (Vssσ , Vspσ , . . .) = a2 , .. . f n (Vssσ , Vspσ , . . .) = an .

(4.81)

Depending upon the strategy that has been adopted, it is possible to have as many equations as there are unknown coefﬁcients, in which case one is reduced to solving n equations in n unknowns. On the other hand, the number of equations could conceivably outnumber the number of unknowns in which case one resorts to solving these equations in the least-squares sense. An example of the type of success that can be attained by exploiting the tight-binding framework in the context of periodic solids is shown in ﬁg. 4.15, where the result of a tight-binding characterization of the band structure of Mo is contrasted with that determined from a full ﬁrst-principles calculation. For the present purposes, the key recognition is that once this type of ﬁtting procedure has been undertaken, it is possible to carry out calculations on both the electronic and structural properties of essentially arbitrary geometric conﬁgurations as long as the number of atoms is not so large as to be beyond the capacity to calculate.

4.5 Tight-Binding Calculations of the Total Energy

189

1

1

Fig. 4.15. Band structure for Mo as obtained from tight-binding calculations and from density functional theory (from Mehl and Papaconstantopoulos (1996)). The notation , N, H, etc. refers to particular k-points within the Brillouin zone.

4.5.3 Real Space Tight-Binding Methods Earlier in this chapter, we introduced pair and cluster functionals as approximate effective theories in which explicit reference to the electronic degrees of freedom had been removed. In each case, we introduced these total energy schemes on

190

4 Energetic Description of Cohesion in Solids

heuristic grounds without giving any strong arguments as to the origins of their particular functional forms. In the present section, we will see how tight-binding theory may be used to motivate both pair and cluster functionals, yielding both of the essential pieces of new physics represented by these schemes: environmental and angular dependence. As a preliminary to our discussion of the emergence of both pair functionals and angular forces from tight-binding theory, we ﬁrst discuss the moments of the density of states which serve as a useful basis for these developments. We begin with the recognition that every distribution has its moments. In particular, the n th moment of the density of states is deﬁned by ∞ µn = E n ρ(E)d E. (4.82) −∞

The moments of the density of states can be seen to be related to the electronic structure itself through the following argument. The shape of the electronic density of states determines the outcome of the one-electron sum embodied in eqn (4.66). The shape of the density of states is in turn determined by its moments. The connection between geometry and the electronic structure in the moments’ setting is revealed when we note that the moments may be written as products of matrix elements over directed paths starting and ending on the same atom. For the purposes of the present discussion we will consider an s-band tight-binding method in which our notation is collapsed in the form |i, s → |i. The elaboration to the more general situation in which there is more than one orbital per site can be carried out relatively painlessly. If we are interested in the second moment associated with a particular site, a more useful but equivalent deﬁnition to that given in eqn (4.82) is µ2 (i) = i|H 2 |i. Making use of the identity I = j | j j|, we see that the second moment may be written in the form µ2 (i) = h(Ri j )h(R ji ), (4.83) j

where h(Ri j ) = i|H | j. What this means is that to ﬁnd the second moment associated with a given site, we sum up all the products called for in eqn (4.83). For example, for an fcc crystal in which the matrix elements are assumed to vanish for distances greater than the near-neighbor distance, the second moment is 12h(Rnn )2 . For the higher-order moments, we have µ3 (i) = h(Ri j )h(R jk )h(Rki ) (4.84) jk

and µ4 (i) =

jkl

h(Ri j )h(R jk )h(Rkl )h(Rli ).

(4.85)

4.5 Tight-Binding Calculations of the Total Energy

191

These are the two lowest-order moments beyond the second moment itself. In this expression, the quantities h(R) characterize the strength of interaction between orbitals that are separated by a distance R. Yet higher-order moments can be obtained by recourse to the same basic ideas. Rectangular Band Model and Pair Functionals. As stated earlier, the ‘derivation’ of the pair functional ansatz may be approached from a variety of different viewpoints. One particularly revealing avenue which is relevant to understanding the emergence of pair functional descriptions of cohesion in transition metals such as Pd or Cu is to adopt the rectangular band model . This model density of states is shown in ﬁg. 4.16(a), and is contrasted with a rigorous density functional calculation of a transition metal density of states in ﬁg. 4.16(b). Despite the presence of a range of detail in the ﬁrst-principles density of states, the rectangular band model is very useful in elucidating qualitative trends in quantities such as the electronic contribution to the cohesive energy that depend upon integrated properties of the density of states. The rectangular band model posits that the density of states is constant over some range of energies and zero otherwise. The constant value associated with the density of states is chosen such that W/2 ρ(E)d E, (4.86) Nfull = 2 −W/2

where Nfull is the total number of electrons that can be accommodated in the band (including spin). This implies that the density of states within our rectangular band ansatz is given by ρ(E) = Nfull /2W . We may use this density of states to evaluate the electronic contribution to the total energy as a function of the ﬁlling of the band (i.e. the number of electrons, Ne ). The electronic contribution to the energy is given by Nfull F E el = Ed E, (4.87) W −W/2 where the Fermi energy, F , is dependent upon the band ﬁlling Ne through Nfull F d E, (4.88) Ne = W −W/2 yielding

Ne 1 F = W . − Nfull 2

(4.89)

In light of these insights, it is seen then that the electronic contribution to the

192

4 Energetic Description of Cohesion in Solids

Fig. 4.16. Comparison of ‘exact’ and rectangular band densities of states for osmium (adapted from Harrison (1980)): (a) density of states for osmium as computed using density functional theory and (b) density of states constructed by superposing a rectangular band model with a free-electron-like density of states. Rising lines in the two curves are a measure of the integrated density of states.

bonding energy is given by Nfull W E el = − 2

Ne Nfull

Ne 1− . Nfull

(4.90)

4.5 Tight-Binding Calculations of the Total Energy

193

Fig. 4.17. Band energy associated with rectangular band density of states. Energy is plotted in dimensionless units, scaled by the width of the band, W . Similarly, the band ﬁlling is plotted as a fraction of the full band.

The parabolic bonding proﬁle revealed above is shown in ﬁg. 4.17 and may be contrasted with the measured cohesive energies shown in ﬁg. 4.18, which in the case of the transition metals reveal just the same trends. The picture that we have advanced here is one of rigid bands in which it is imagined that in passing from one element to the next as we traverse the transition series, all that changes is the ﬁlling of the d-band, with no change in the density of states from one element to the next. It is also important to note that the bonding energy scales with the bandwidth, an observation that will makes its appearance shortly in the context of pair functionals. The rectangular band model developed above may be used as a tool to gain insights into the type of functional form that should be presumed in pair functionals such as those introduced earlier. In particular, if we consider a particular choice of band ﬁlling (i.e. ﬁx our attention on describing the energetics of a particular element), then the electronic contribution to the total energy of eqn (4.90) scales with the second moment of the density of states, since eqn (4.90) can be rewritten √ on the basis of the observation that W ∝ µ2 . To see that the bandwidth and the second moment of the density of states are indeed related, a plausibility argument can be made by appealing to a calculation of the second moment of the rectangular band density of states. In this case, the second moment is µ2 = 5W 2 /12, showing that the bandwidth scales with the square root of the second moment. Thus, if we consider as an example the case of a half-ﬁlled d-band (i.e. Ne /Nfull = 1/2) then √ eqn (4.90) tells us that E el = − 15µ2 /4. On the basis of the reasoning given

194

4 Energetic Description of Cohesion in Solids

Fig. 4.18. Experimental energies of cohesion as a function of the number of d-electrons (n d ) for the three transition metal series (adapted from Young (1991)).

above, the rectangular band model suggests a total energy that is written as the sum of the electronic contribution and a pair potential term that accounts for the interactions between nuclei, resulting in 1 φ(Ri j ) − α µ2 (i), (4.91) E tot = 2 ij i where the constant α is a parameter that depends upon the band ﬁlling and can be deduced on fundamental grounds or used as a ﬁtting parameter. To ﬁnish the argument, we need to know the way in which the second moment itself depends upon the geometric arrangement of atoms. At this point, it sufﬁces to note that if we are interested in the second moment associated with a particular site, it may be determined using eqn (4.83). The fact that the second moment can be written in pairwise form immediately suggests the correspondence between the pair functionals presented earlier and our present argument. Because the second moment is itself of the pairwise additive form, it is now seen that, like in the embedded atom description explored earlier, the energy per bond depends upon the coordination number. Moments and Angular Forces. Our aim in the present setting is to exploit the geometry of the densities of states in order to construct effective potentials for describing the bonding in solids which go beyond the pairwise forms considered thus far. We follow Carlsson (1991) in formulating that description. First, we reiterate that our aim is not the construction of the most up-to-date potentials that

4.5 Tight-Binding Calculations of the Total Energy

195

may be imagined. Rather, we wish to understand the microscopic origins of the angular terms which might appear in a total energy functional. For example, the total energy can take the form 1 eff 1 eff V2 (Ri , R j ) + V (Ri , R j , Rk ) 2 ij 3! i jk 3 1 eff V (Ri , R j , Rk , Rl ) + · · · . + 4! i jkl 4

E tot =

(4.92)

Our aim at this point is an analysis of the quantum mechanical underpinnings for the angular terms introduced above. We begin by assuming the existence of some reference state, the energy of which shall serve as our zero and from which all other energies are measured. In this state, if we assume that only n moments of the density of states are known, the electronic contribution to the total energy is given by ref

ref

E el = E(µ2 , µ3 , . . . , µref n ).

(4.93)

By way of contrast, if we interest ourselves in a particular conﬁguration and aim to determine its energy relative to the reference state, that energy may be written ref

ref

E el = E(µ2 + δµ2 , µ3 + δµ3 , . . . , µref n + δµn ),

(4.94)

where the δµi s reﬂect the difference between the moments of the reference state and the structure of interest. We now adopt the usual dodge of Taylor expanding in the presumed small deviations from the reference environment, resulting in an expression for the total energy change of the form ∂E E el = (µn − µref (4.95) n ). ∂µ n ref n This expression is enlightening in that it reveals that the effective interatomic potentials have inherited the explicit angular dependence of the moments and, further, that the potentials have an environmental dependence that is dictated by the ‘susceptibility’ ∂ E/∂µn . By absorbing the constant terms involving the reference state into our deﬁnition of the potentials, the energy of a given state may now be written as n ∂ E E el = µ(k) (4.96) n . ∂µ n ref k=1 n We have adopted the notation µn(k) to signify the contribution to the n th moment arising from paths connecting k atoms. We now seek a correspondence between eff eqns (4.92) and (4.96). In particular, Vk (R1 , . . . , Rk ) is obtained by adding up all

196

4 Energetic Description of Cohesion in Solids

the terms in eqn (4.96) involving atoms 1, 2, . . . , k. For example, the effective pair potential is given by eff V2 (Ri , R j )

=2

Nm ∂E n=2

∂µn

µ(2) n (Ri , R j ),

(4.97)

ref

th where we have deﬁned µ(2) n (Ri , R j ) as the two-atom contribution to the n moment involving atoms i and j. Note that we are considering two-atom contributions to all moments between the 2nd moment and the Nmth moment. Similar expressions are obtained in the case of the higher-order potentials. As said before, the key observation is that the potentials inherit the angular dependence of the moments. Though the notation used above is admittedly cumbersome, the basic idea associated with the development of these potentials is relatively straightforward. The idea was to expand the energy about a reference environment and to adopt a functional form for the potentials that is a direct inheritance from the moments of the density of states which themselves are deﬁned as directed paths involving the atoms in a given cluster. We must maintain the insight that the energies are measured relative to a reference environment. In particular, the susceptibilities are evaluated for the reference environment. As a result, depending upon the choice of reference environment, the relative strengths of the potentials will vary. To see this explicitly, consider the effective pair potential tied to the rectangular band model √ √ discussed above. Since E el scales as µ2 , we see that ∂ E el /∂µ2 ∝ 1/ µ2 . The implication of this result is that for a reference environment with a small µ2 (i.e. the atoms have fewer neighbors, such as at a surface) the effective potential is stronger. An example of the type of potentials that result upon adopting a strategy like that given above is shown in ﬁg. 4.19. We focus attention on the effective interactions involving clusters of four atoms The four-body terms are based upon a slightly more sophisticated scheme than that used here involving a basis more complex than the simple tight-binding basis considered here, but the basic concepts are identical. In this case, we see that for a metal such as Mo, four-body planar clusters with 90◦ angles are energetically costly and point to a substantial lowering of the energy of the bcc structure (which has no such clusters based on ﬁrst neighbors) and the fcc structure. As we have seen in the preceding sections, the development of empirical potentials is a mixture of plausibility arguments and sound guesswork. Despite their successes in accounting for the features of defects in a range of materials, even the best of potentials at times suffer from fatal weaknesses. Our aim now is to give a ﬂavor of the many attempts that have been put forth to build satisfactory interatomic descriptions for the direct simulation of problems of interest concerning real materials. One perspective has been offered by Heine et al. (1991) who note

4.6 First-Principles Calculations of the Total Energy

197

Fig. 4.19. Four-body potential for Mo (adapted from Moriarty (1990)).

“The success of the ‘glue’ models, which take many-atom forces speciﬁcally into account, has been impressive particularly in accounting for subtle effects such as the reconstructions of the Au surface. By way of contrast, one can point to the sad history of attempts to ﬁnd a satisfactory force model for Si. There has been a whole succession of models, each ﬁtted to experimental data plus the computed energies of a range of unstable structures covering quite a variety of bonding geometries. Yet each model failed when confronted a year or so later by the energy of some new structure.” At the time of this writing it remains an open question whether or not any satisfactory scheme can be developed for treating covalent materials. For the moment, the most reliable scheme is to use the full quantum mechanical description described in the next section. 4.6 First-Principles Calculations of the Total Energy As yet, our discussion has focused on the attempt to construct energy functionals in which there is some level of empiricism that mimics to a greater or lesser extent the presumed exact results of a full quantum mechanics calculation. Our reason for shying away from the full quantum mechanical calculations themselves was founded upon the fact that these methods are computationally intensive, and hence must be undertaken with the foresight to insure that they are used only when really necessary. It is the purpose of the present section to sketch the way in which ﬁrst-principles calculations are constructed.

198

4 Energetic Description of Cohesion in Solids

As our starting point, we begin by reminding ourselves of the basic facts that make the full many-electron problem so difﬁcult. A useful starting point is the Hamiltonian that describes both the electrons and the nuclei from which they are derived. The full many-particle Hamiltonian made its appearance in eqn (4.3), where it was shown that the various particle coordinates are linked in an exceedingly complicated way. If we adopt the purists’s perspective, we demand the full wave function which is a function not only of the electronic degrees of freedom, but of the nuclear degrees of freedom as well. As is clear from the full Hamiltonian, the Schr¨odinger equation corresponding to this many-body description is a coupled problem of enormous proportions. Nevertheless, through a combination of path-breaking theorems and numerical inventiveness, the calculation of electronic structure and associated total energies has still become routine. 4.6.1 Managing the Many-Particle Hamiltonian Density Functional Theory and the Local Density Approximation Even in light of the insights afforded by the Born–Oppenheimer approximation, our problem remains hopelessly complex. The true wave function of the system may be written as ψ(r1 , r2 , r3 , . . . , r N ), where we must bear in mind, N can be a number of Avogadrian proportions. Furthermore, if we attempt the separation of variables ansatz, what is found is that the equation for the i th electron depends in a nonlinear way upon the single particle wave functions of all of the other electrons. Though there is a colorful history of attempts to cope with these difﬁculties, we skip forth to the major conceptual breakthrough that made possible a systematic approach to these problems. In the language of the beginning of the chapter, the basic idea used in the density functional setting is to effect a replacement E exact ({Ri , rn }) → E approx [ρ(r), {Ri }].

(4.98)

In particular, Hohenberg and Kohn advanced the view that the total energy of the many-electron system may be written as a unique functional of the electron density of the form, ρ(r )ρ(r ) 3 3 1 d rd r + Vext (r)ρ(r)d 3 r, E[ρ(r )] = T [ρ(r)] + E xc [ρ(r)] + 2 |r − r | (4.99) and that the ground state energy of the system is attained on minimizing this functional. The various terms in this equation shape up as follows. T [ρ(r)] is the kinetic energy term, while the term E xc [ρ(r)] is the so-called exchange-correlation energy and refers to parts of the many-electron interaction whose origin is quantum mechanical. The remaining terms correspond to the direct electron–electron

4.6 First-Principles Calculations of the Total Energy

199

interaction and the interaction of electrons with an external potential (which can include the ions). In the problem section at the end of the chapter, we take up the question of how a simple model for the kinetic energy functional can be built up using what we have already learned about the electron gas. As it stands, the statement given above is exact. The profundity of the insight buried in the density functional given above is related to the fact that it allows for an exact mapping of our perceived hopeless many-electron problem onto a set of effective single particle equations. The only difﬁculty is that the functional itself is unknown. However, the strategy suggested in eqn (4.98) is to use a local approximation to the exchange-correlation functional which results in a series of approximate, but highly accurate, one-electron equations. We also note that local approximations like those introduced here will reveal themselves of relevance in other continuum settings. As said above, the key assertion is that the ground state energy corresponds to that density that minimizes the functional of eqn (4.99). Of course, until something can be said about the form of T [ρ(r)] and E xc [ρ(r)], we don’t have a practical scheme for obtaining the total energy. The next key step in the analysis was the introduction of an approximation which converted the original problem into a corresponding problem for a ﬁctitious system involving noninteracting electrons in the presence of an effective potential. The key approximation is known as the local density approximation and consists in the statement E xc [ρ(r)] = xc (ρ(r))d 3 r. (4.100) As we said above, in the absence of knowledge of the exchange-correlation functional E xc [ρ(r)] itself, our results were only suggestive. The key additional insight that makes this formulation a viable calculational scheme is the local density approximation in which, once again, appeal is made to the properties of the electron gas. In this instance, the idea is to presume that the exchange-correlation functional may be approximated by the electron gas exchange-correlation functional xc (ρ), which is known. The use of this functional in the solid is based upon the assumption that the local behavior of the electrons in the solid mimic those of the corresponding homogeneous electron gas at the same density. In light of this approximation, we are now prepared to seek the energy minimizing density ρ(r) which is obtained by minimizing this functional, that is by effecting the functional derivative δ E[ρ(r)]/δρ(r) = 0.

(4.101)

This results in a set of single particle equations, known as the Kohn–Sham

200

4 Energetic Description of Cohesion in Solids

equations given by h¯ 2 2 ∇ ψi (r) + Veff (r)ψi (r) = i ψi (r). 2m The effective potential is given in turn as δ E xc ρ(r )dr + . Veff (r) = Vext (r) + |r − r | δρ(r) −

(4.102)

(4.103)

Note that at this point we have turned the original (hopeless) many-body problem into a series of effective single particle Schr¨odinger equations. As will become increasingly evident below, there are a number of different particular realizations of the general ideas being set forth here. For example, in the context of the exchange-correlation energy itself, there are several popular parameterizations of the density dependence of the exchange-correlation energy that are in use. Recall that the exchange-correlation energy is representative of those parts of the electron–electron interaction which are purely quantum in nature. Part of the variety that attends the various computer implementations of density functional theory in the local density approximation surrounds the different parameterizations for this term. The key point is that from an analytic perspective, even after making the simplifying assumption that it is the exchange-correlation energy of the uniform electron gas that is needed, xc (ρ) cannot be described fully. Often, one resorts to parameterizations which satisfy known constraints in the limits that the density of the electron gas is either very high or very low, and then searches for interpolation formulae in the intervening density regime which can be informed on the basis of quantum Monte Carlo calculations of this property. A detailed discussion of many of the popular parameterizations for this term can be found in table 7.1 of Dreizler and Gross (1990) and the attendant prose. 4.6.2 Total Energies in the Local Density Approximation Once the effective single particle equations have been derived, there are almost limitless possibilities in terms of the different schemes that have been invented to solve them. By way of contrast, the assertion is often made that if the calculations in these different realizations of the ﬁrst-principles methodology are made correctly, then the predictions of these different implementations should be the same. Interactions Between Nuclei and Electrons Note that in our treatment of the Kohn–Sham equations, we assume the existence of an external potential Vext (r) which characterizes the interactions of the nuclei and the electrons. Given our interest in modeling the properties of solid materials,

4.6 First-Principles Calculations of the Total Energy

201

Vext will arise as a superposition of the potentials associated with each of the nuclei making up the solid. In the most direct of pictures, one can imagine treating the solid by superposing the ‘bare’ nuclear potentials for each atom, and subsequently solving for the disposition of each and every electron. This approach is the basis of the various ‘all-electron’ methods. As an alternative to the explicit treatment of each and every electron, a variety of methods have grown up around the use of effective potentials in which Vext is meant to mimic the nucleus and its complement of core electrons which are presumed to be indifferent to the changes in environment in going from the free atom to the solid. Indeed, much of the spirit of this book centers on the idea of reduced descriptions in which degrees of freedom are eliminated in the name of both conceptual simplicity and computational tractability and the use of pseudopotentials like those described above is a compelling example of this strategy. It is crucial to realize that in the process of formation of the solid, many of the low-lying atomic states (i.e. those electrons that are tightly bound to the nucleus in inner shells) are disturbed very little by the formation of the solid. As a result, pseudopotential schemes attempt to exploit this observation by creating an effective potential in which the nucleus and the core electrons together serve to inﬂuence the outer electrons. The key idea is a choice of pseudopotential that reproduces known properties such as atomic wave functions or the scattering properties associated with the full potential. An example of a pseudopotential is given in ﬁg. 4.20. For our purposes our interest in this idea is as observers rather than practitioners, with the key insight gleaned from the observation being the formal way in which degrees of freedom are eliminated. Choosing a Basis In our statement of the Kohn–Sham equations, nothing has been said about the way in which ψ(r) itself will be determined. Many methods share the common feature that the wave function is presumed to exist as a linear combination of some set of basis functions which might be written generically as αn bn (r), (4.104) ψ(r) = n

where αn is the weight associated with the n th basis function bn (r). Just as with the earlier statement of tight-binding theory, solving the relevant equations becomes a search for unknown coefﬁcients rather than unknown functions. Part of the variety associated with the many different incarnations of density functional codes is associated with this choice of basis functions. For example, in the spirit of the earlier tight-binding discussion, one can imagine a basis constructed out of functions localized about each atomic site. Alternatively, we can

202

4 Energetic Description of Cohesion in Solids

pseudo

rc

r

v Vpseudo

Z/r

Fig. 4.20. Schematic of pseudopotential and associated pseudowave function (adapted from Payne et al. (1992)).

take our cue from the physics of the electron gas and attempt to expand the total wave function in terms of a free-electron-like basis. If one is to use the so-called plane wave basis set, then the generic wave function for a state characterized by wave vector k is represented as ak+G ei(k+G)·r . (4.105) ψk (r) = G

In this case, the vectors G are members of the set of reciprocal lattice vectors and eqn (4.105) really amounts to a three-dimensional Fourier series. The task of solving the Kohn–Sham equations is then reduced to solving for the unknown coefﬁcients ak+G . The only difﬁculty is that the potential that arises in the equation depends upon the solution. As a result, one resorts to iterative solution strategies. Computing the Electronic Structure and the Total Energy Once the Kohn–Sham equations have been solved, we are in a position to evaluate energies, forces and the electronic structure of a material itself. In particular, with the eigenvalues i and corresponding wave functions ψi (r) we can compute the energy of the system explicitly. As can be seen from the discussion given above, and as has been true with each of the total energy methods introduced in this chapter, in the end we are left with a scheme such that once the nuclear

4.7 Choosing a Description of the Total Energy: Challenges and Conundrums 203

Fig. 4.21. Densities of states for several bcc transition metals as computed using density functional theory (adapted from Eriksson et al. (1992)).

coordinates have been provided, one can compute the corresponding energy. From the perspective of computational materials science, this step is of primary importance since it is the key to ﬁrst examining the structure and energetics of the various defects that populate materials, and ultimately to explicating how those structures conspire to give rise to the properties of materials. Part of the added value of using methods in which the electronic degrees of freedom are treated explicitly is the insights that may be garnered concerning the electronic properties of a material. To provide some feel for the types of results that emerge, an example of the densities of states for several materials is shown in ﬁg. 4.21.

4.7 Choosing a Description of the Total Energy: Challenges and Conundrums This chapter has emphasized the microscopic approach to computing the total energy of solids. We have seen that there are a number of different schemes for computing the total energy, each with its own advantages and difﬁculties. In simplest terms, the largest conundrum faced in the selection of a total energy description concerns the compromise that must usually be made between computational tractability and accuracy. Treatments featuring the electronic degrees of freedom explicitly are often plagued by the inability to treat system sizes capable of

204

4 Energetic Description of Cohesion in Solids

resolving the problem of interest without the contaminating inﬂuences of nearby boundaries. On the other hand, empirical schemes, while able to handle much larger system sizes, suffer a shortcoming of similar magnitude in that the results can often be charged with lacking physical realism. In subsequent chapters, we will show how the types of energy functionals described here may be used as a tool for computing the properties of materials. Part of our approach will be to attempt to tackle particular case studies from the perspective of several different total energy methods. Our intention in adopting this approach is to illustrate the way in which some methods provide a clearer physical picture of the problem at hand, while others are to be noted for their physical accuracy. 4.8 Further Reading ‘Beyond Pair Potentials’ by A. E. Carlsson, in Solid State Physics edited by H. Ehrenreich and D. Turnbull, Academic Press, San Diego: California, Vol. 43, pg. 1, 1990. This article gives a thorough discussion of the conceptual underpinnings associated with efforts to build effective potentials as a way to eliminate explicit reference to electronic degrees of freedom. ‘Many-atom interactions in solids’ by V. Heine, I. J. Robertson and M. C. Payne, Phil. Trans. Roy. Soc. Lond., A334, 393 (1991) gives a thoroughly thoughtful overview of the difﬁculties that must be faced in trying to create effective theories of interatomic interactions in which explicit reference to the electronic degrees of freedom has been renounced. Electronic Structure and the Properties of Solids by W. A. Harrison, W. H. Freeman and Company, San Francisco: California, 1980. Harrison’s book espouses the tight-binding perspective in a way that reveals how this method may be applied to consider materials ranging from Si to Ta. I have learned much from this book. ‘Tight-binding modelling of materials’ by G. M. Goringe, D. R. Bowler and E. Hern´andez, Rep. Prog. Phys., 60, 1447 (1997). This article gives an up-to-date review of the continued uses of the tight-binding formalism. Solids and Surfaces: A Chemist’s View of Bonding in Extended Structures by R. Hoffmann, VCH Publishers, New York: New York, 1988. This book reﬂects the chemist’s intuition as regards bonding in solids. Hoffmann has a special talent for constructing plausible models of the electronic structure of solids on the basis of insights strictly in terms of the crystalline geometry and the character of the underlying atomic orbitals. Another book that espouses the chemical perspective on bonding in solids is

4.8 Further Reading

205

Chemical Bonding in Solids by J. K. Burdett, Oxford University Press, Oxford: England, 1995. One of the key features that I enjoy in looking at the work of both Hoffmann and Burdett is their willingness to confront systems not only with a high level of structural complexity, but chemical complexity as well. Bonding and Structure of Molecules and Solids by D. Pettifor, Clarendon Press, Oxford: England, 1995. A superb contribution aimed at explaining the fundamental physical reasoning associated with constructing models of bonding in solids. Primary emphasis is placed on metals and covalent materials. The Electronic Structure and Chemistry of Solids by P. A. Cox, Oxford University Press, Oxford: England, 1987. Like the book by Hoffmann, this book takes a more chemical perspective of bonding in solids. Though the mathematical sophistication demanded of the reader is fairly low, this does not imply that there is not much to be learned here. A book I have returned to repeatedly. ‘Iterative minimization techniques for ab initio total energy calculations: molecular dynamics and conjugate gradients’, by M. C. Payne, M. P. Teter, D. C. Allan, T. A. Arias and J. D. Joannopoulos, Rev. Mod. Phys., 64, 1045 (1992). Despite the title which makes it appear highly specialized, this article has much to offer on everything from the LDA formalism itself, to issues of convergence and the use of LDA calculations (rather than classical potentials) as the basis of molecular dynamics. ‘Modern Electron Theory’ by M. W. Finnis in Electron Theory in Alloy Design edited by D. G. Pettifor and A. H. Cottrell, Institute of Materials, London: England, 1992. This is my favorite article on ﬁrst-principles calculations. Finnis spells out all of the key points involved in carrying out ﬁrst-principles calculations of the total energy. ‘Understanding quasi-particles: observable many-body effects in metals and 3 He’ by J. W. Wilkins in Fermi Surface edited by M. Springford, Cambridge University Press, New York: New York, 1980. Wilkins’ article describes many of the issues that arise in thinking about the many-body aspects of the total energy in solids. Density Functional Theory by R. M. Dreizler and E. K. U. Gross, Springer-Verlag, Berlin: Germany, 1990. This book concerns itself primarily with the formalism of density functional theory and less with the speciﬁcs of a given computer implementation. It has much to offer on the origins of the Kohn–Sham equations, the treatment of the exchange-correlation energy and on reﬁnements such as gradient corrections.

206

4 Energetic Description of Cohesion in Solids

4.9 Problems

1 Fitting parameters in the Lennard–Jones potential In this chapter, we introduced the Lennard–Jones potential given by 12 6

σ σ . − V (r ) = V0 r r

(4.106)

Determine the constants V0 and σ for fcc Xe by using the fact that the cohesive ˚ Energy energy of Xe is 0.17 eV/atom and the lattice parameter is 6.13 A. ˚ Carry out the units for the potential should be in eV and length units in A. solution to this problem both analytically (by ﬁtting these energies only for a near-neighbor model) and numerically, by using six-neighbor shells. For further details see Kittel (1976).

2 Morse Potential and Cohesion in Cu The Morse potential is given by V (r ) = V0 (e−2a(r −r0 ) − 2e−a(r −r0 ) ), where V0 , a and r0 are parameters to be determined by ﬁtting to experimental data. Using the experimental data for the cohesive energy of fcc Cu (E coh = 336 kJ/mole), ˚ and the bulk modulus the fcc Cu equilibrium lattice parameter (a0 = 3.61 A) ˚ −1 ) and r0 (in (B = 134.3 GPa), determine the parameters V0 (in eV), a (in A ˚ under the assumption that only near-neighbor atoms interact. A)

3 Forces within the Pair Functional Formalism Given the prescription for the total energy as deﬁned within the pair functional formalism, compute the expression for the force on atom i as a result of its interactions with its neighbors. In particular, compute Fi = −∂ E tot /∂ xi , remembering that there is implicit dependence on xi through the density. Use your result to demonstrate that if the cutoff range of the interactions is denoted as Rcut , then the motion of an atom at a distance of 2Rcut from the atom of interest can result in a force on that atom. The result of this calculation is given in eqn (4.43).

4 Effective Pair Interactions from Pair Functionals The pair functional formalism may be recast in the language of pair potentials by computing an effective pair potential which is valid for environments close

4.9 Problems

207

to some reference environment. In this problem, starting with eqn (4.33), consider small deviations about some reference environment characterized by an electron density ρref . By writing the total density at a given site as ρref + δρ and Taylor expanding the embedding term, show that the resulting expression for the total energy takes the form of a pair potential. Using Johnson’s analytic embedded-atom functions introduced in this chapter, obtain and plot the effective pair potentials valid for both the bulk environment and for the (100) surface of an fcc crystal.

5 Stillinger–Weber Energy for Si in Diamond Cubic Structure In eqn (4.51) we derived an expression for the total energy of a twodimensional triangular lattice. That expression was for a geometrically unrealistic structure for a covalently bonded material. Derive an analogous expression for the total energy of Si when in the diamond cubic structure.

6 Forces Associated with Stillinger–Weber Potentials Obtain an expression for the forces between atoms in a system characterized by the Stillinger–Weber potential. An explicit expression may be found in Wilson et al. (1990).

7 Electronically Driven Structural Transformations Consider an s-band tight-binding Hamiltonian with matrix elements i|H | j = h 0 /r , where r is the distance between atoms i and j. The goal of this problem is to examine the electronic driving force for dimerization of a linear chain of atoms by examining the electronic structure and resulting cohesive energy for a chain of atoms with nominal lattice parameter a0 as shown in ﬁg. 4.22. Consider a dimerization reaction in which the new lattice is characterized by alternating spacings a0 − δ and a0 + δ with the result that there are two atoms per unit cell with a lattice parameter of 2a0 . Assume that each atom has one electron (i.e. the case of half-ﬁlling) and obtain the electronic contribution to the energy as a function of the parameter δ. Note that each atom is coupled only to its near neighbors on the left and right, though the strength of that coupling is scaled by 1/r as described above. Plot the electronic energy as a function of δ and comment on the implications of your result.

208

4 Energetic Description of Cohesion in Solids

Fig. 4.22. Chain geometries to be considered in problem 7 corresponding to: (a) the undimerized state and (b) the dimerized state.

8 d-Band Tight-Binding Model for fcc Metal In this problem you are asked to obtain an expression for the dispersion relation along the (100) direction in k-space for fcc Ni. The calculation should be done using a basis of ﬁve d-orbitals per atom, with the parameters Vddσ , Vddπ and Vddδ chosen in the ratio Vddσ : Vddπ : Vddδ = −6 : 4 : −1.

9 Tight-Binding for Crystals with Multiple Atoms per Unit Cell In eqn (4.68), we developed the tight-binding formalism for periodic systems in which there was only one atom per unit cell, with each such atom donating n basis functions to the total electronic wave function. Generalize the discussion presented there to allow for the presence of more than one atom per cell. In concrete terms, this means that the basis functions acquire a new index, |i, J, α, where the index i speciﬁes the unit cell, J is a label for the atoms within a unit cell and α remains the label of the various orbitals on each site.

10 Density of States for Electron Gas In the previous chapter we described the physics of the electron gas. Using the ideas described there, deduce the density of states, ρ(E) for the one-, two- and three-dimensional electron gas. In particular, show how the density of states scales with the energy and plot your results. Recover the expression for the cohesive energy of the electron gas by evaluating integrals of the form F E el = 2 ρ(E)Ed E. (4.107) 0

4.9 Problems

209

11 Simple Model for the Kinetic Energy Functional The density functional introduced in eqn (4.99) featured a kinetic energy term denoted T [ρ(r)]. In this problem, derive an expression for a kinetic energy functional based upon the simple electron gas physics described in chap. 3. In particular, if the total kinetic energy per atom is of the form 3 h¯ 2 E eg 2 = (3π 2 ρ) 3 , (4.108) N 5 2m then what form should the kinetic energy density t(ρ(r)) take in writing a kinetic energy functional of the form T [ρ(r)] = t (ρ(r))d 3 r? Now that this kinetic energy functional is in hand, write an approximate functional for thetotal energy of the form ρ(r )ρ(r ) 3 3 1 3 d rd r + Vext (r)ρ(r)d 3 r, E T F [ρ(r)] = t (ρ(r))d r + 2 |r − r | (4.109) subject to the constraint that ρ(r)d 3 r = N , (4.110) where N is the total number of electrons. Note that we have introduced the notation E T F [ρ(r)] to refer to the fact that we are making the Thomas–Fermi approximation. By computing the functional derivative of the Thomas–Fermi functional subject to the constraint given above, obtain the equation satisﬁed by the ground state density.

FIVE

Thermal and Elastic Properties of Crystals

5.1 Thermal and Elastic Material Response As yet, our discussion of modeling the energetics of crystalline solids has centered on the analysis of atomic conﬁgurations that are undisturbed by deformation, by the thermal vibrations that are inevitably present at ﬁnite temperatures or by defects. Before embarking on an analysis of the full-ﬂedged defected solid, we begin with a consideration of geometric states that may be thought of as relatively gentle perturbations about the perfect crystal. In particular, the aim of the present chapter is to assess the energetics of both thermal vibrations and elastic deformations, with a treatment that is uniﬁed by the fact that in both cases the energy can be expanded about that of the perfect crystal which serves as the reference state. Prior to examining the ways in which the methods of chap. 4 can be used to examine the energetics of both thermal vibrations and elastic deformations, we consider the signiﬁcance of these excitations to the properties of materials at large. The methods of the present chapter feed into our quest to understand the properties of materials in several distinct ways. First, as will be described in the following paragraphs, a variety of important material properties involve the energetics of thermal vibration or elastic deformation directly, including the speciﬁc heat, the thermal conductivity, the thermal expansion and the elastic moduli themselves. However, in addition to the direct signiﬁcance of the ideas to be presented here to the analysis of thermal properties, much of what we will have to say will form the methodological backdrop for our discussion of the thermodynamic ideas invoked to understand phase diagrams, diffusion and microstructural evolution. In chap. 4 we argued that much can be learned by comparing the energetics of different competing states of a crystalline solid. One set of material parameters that can be understood on the basis of total energy methods like those presented in the previous chapter in conjunction with the methods of statistical mechanics are those related to the thermal response of materials. Indeed, one of the workhorses 210

5.1 Thermal and Elastic Material Response

211

Fig. 5.1. Speciﬁc heat for Cu as obtained from Debye model contrasted with experimental results (adaptation of Debye’s original results by Reif (1965)).

of the statistical mechanics curriculum is the evaluation of the speciﬁc heat of crystalline solids as a function of the temperature. A representative example of the experimentally observed speciﬁc heat of solids is shown in ﬁg. 5.1. Our discussion of the theoretical apparatus that is needed to understand these data will provide a variety of lessons in the use of total energy methods in conjunction with statistical mechanics. A second class of material parameters associated with the thermal behavior of solids is more traditionally thought of as those associated with ‘anharmonic effects’ in solids and includes the thermal conductivity and the coefﬁcient of thermal expansion. As already shown in ﬁg. 1.2, the thermal conductivity of different material classes ranges over a number of orders of magnitude and involves a variety of different mechanisms including the scattering of phonons by point defects as will be brieﬂy described in chap. 7. The coefﬁcient of thermal expansion also looms as an important material parameter, with an increasingly important technological role as a result of the reliance on complex heterostructures in which many different materials are joined together. In these cases, it is the mismatch in thermal expansion coefﬁcient which is of particular signiﬁcance since this mismatch results in thermal stresses that can lead to mechanical failure. The use of thermal expansion mismatch as an engineering tool in the form of the bimetallic strip dates at least as far back as the creation of the famed clocks of John Harrison described in Dava Sobel’s Longitude (1995). It is amusing to note that the application of thermal mismatch preceded its understanding on the basis of statistical mechanics by nearly 250 years.

212

5 Thermal and Elastic Properties of Crystals

In addition to the thermal properties mentioned above, the present chapter also has as its charter the investigation of the elastic (both linear and nonlinear) properties of solids. We begin by noting that the linear theory of elasticity is one of several prototypical continuum theories and is at the heart of analyses of problems ranging from the formation of dislocations in Six Ge1−x to the deformation of bridges subjected to loads from wind and earthquakes. As noted earlier, continuum theories such as the linear theory of elasticity are silent on the values of the material parameters used to characterize solids. As a result, it is the business of subscale analysis, such as is offered by the types of microscopic energy functionals described in the previous chapter, to evaluate the elastic response of different materials. An example of the diversity of elastic properties as measured by the Young modulus is shown in ﬁg. 1.1. In the preceding paragraphs, we have given a sketch of some of the material parameters that are explicitly tied to the thermal and elastic response of solids. However, as we already noted, the tools developed to examine these material parameters are of much broader importance to the generic aim of modeling materials and their response. Indeed, the ideas to be presented in the present chapter serve as the backbone for an analysis of thermostatics (i.e. the study of equilibria) and of kinetics in solids. The discussion above was meant to highlight the various material parameters related to the thermal properties of solids. In the following paragraphs we also show the origins of the methodological relevance of the material in the present chapter to our later examination of both equilibria and kinetics in solids. One of the central points of contact between the methods of the present chapter and an analysis of material response will be the application of these methods to the construction of free energies. Whether our aim is the investigation of phase diagrams or the driving forces on interfaces, one of the elemental challenges that will be faced will be that of the construction of the relevant free energy. For example, in the context of phase diagrams, we will see that a central part in the competition between different phases is played by the vibrational entropy of these competing phases. In addition to the consideration of equilibrium problems, the treatment of thermal excitations is also important to the investigation of kinetics. An intriguing insight into kinetics is that in many cases, the tools for treating thermal excitations to be described in this chapter can be used to consider driven processes such as diffusion. As will be noted in chap. 7, models of kinetics are tied to the idea that as a result of the random excursion of atoms from their equilibrium positions, a system may occasionally pass from one well in the multi-dimensional potential energy surface to another. Indeed, this eventuality has already been rendered pictorially in ﬁg. 3.22 where we saw an adatom hopping from one energy well to the next in its

5.2 Mechanics of the Harmonic Solid

213

excursion across a crystal surface. As will be seen below, the treatment of these excursions, at least in the case of small displacements, can be put on a formal basis that allows for the construction of explicit models of thermal activation. A less explicit way in which the methods of the present chapter are of paramount importance is the way in which they can instruct us in our aim of building effective theories based on some reduced set of degrees of freedom. As we have emphasized repeatedly, one of our central tasks is the construction of effective theories in which the degrees of freedom used in the model subsume the full set of microscopic degrees of freedom. For instance, in chap. 8, we will see that despite the complicated atomic-level motions which attend plastic deformation, it is possible to construct models based on defect-level entities, namely, dislocations, without mandating the consideration of atomic positions or motions explicitly. These dislocations represent the collective motion of huge numbers of atoms which have suffered relative displacements across a common slip plane. An interesting side effect of our construction of such effective models is that they require that we institute some notion of dissipation. For example, as the dislocation traverses the crystal some of the energy associated with its center of mass motion is transferred to the microscopic degrees of freedom which are disguised from the effective theory that interests itself only in the overall dislocation motion. The methods of the present chapter begin to teach us how to think of the coupling of the center of mass motions of defects to atomic-level motions, and thereby to construct models of dissipation. The plan of the following sections is as follows. First, we undertake an analysis of the energetics of a solid when the atoms are presumed to make small excursions about their equilibrium positions. This is followed by a classical analysis of the normal modes of vibration that attend such small excursions. We will see in this case that an arbitrary state of motion may be speciﬁed and its subsequent evolution traced. The quantum theory of the same problem is then undertaken with the result that we can consider the problem of the speciﬁc heat of solids. This analysis will lead to an explicit calculation of thermodynamic quantities as weighted integrals over the frequencies of vibration.

5.2 Mechanics of the Harmonic Solid As noted in the introduction to the present chapter, the contemplation of thermal and elastic excitations necessitates that we go beyond the uninterrupted monotony of the perfect crystal. As a ﬁrst concession in this direction, we now spell out the way in which the energy of a weakly excited solid can be thought of as resulting from excursions about the perfect crystal reference state. Once the total energy of such excursions is in hand, we will be in a position to write down equations of

214

5 Thermal and Elastic Properties of Crystals

motion for these excursions, and to probe their implications for the thermal and elastic properties of solids.

5.2.1 Total Energy of the Thermally Fluctuating Solid Our starting point for the analysis of the thermal and elastic properties of crystals is an approximation. We begin with the assertion that the motions of the i th atom, will be captured kinematically through a displacement ﬁeld ui which is a measure of the deviations from the atomic positions of the perfect lattice. It is presumed that this displacement is small in comparison with the lattice parameter, |ui | a0 . Though within the context of the true total energy surface of our crystal (i.e. E tot (R1 , R2 , . . . , R N )) this approximation is unnecessary, we will see that by assuming the smallness of the excursions taken by the atoms of interest, a well-deﬁned and tractable formulation of the thermal properties of the solid may be made. As in chap. 4, we posit the existence of a total energy function of the form E tot (R1 , R2 , . . . , R N ) = E tot ({Ri }), where {Ri } denotes the entire set of ionic coordinates. For simplicity, the total energy is allowed to depend only upon the ionic positions (i.e. we have ignored the explicit dependence of the total energy function on the electronic degrees of freedom thus assuming that the system remains on the Born–Oppenheimer energy surface). Since our interest is in ref excursions about the equilibrium positions Ri , we now advance an expansion of the total energy about the reference conﬁguration in powers of the small displacements ui . In particular, the total energy of the instantaneous ﬂuctuating ref snapshot of the solid characterized by atomic positions {Ri + ui } is written as ref

ref

E tot ({Ri + ui }) = E tot ({Ri }) +

∂ E tot i,α

+

∂ Riα

u iα

1 ∂ 2 E tot u iα u jβ + · · · . 2 iα jβ ∂ Riα R jβ

(5.1)

The α th component of displacement of the i th ion is denoted u iα . The rationale for our strategy is cast in geometric terms in ﬁg. 5.2 which shows the quadratic approximation to a fully nonlinear energy surface in the neighborhood of the minimum for an idealized two-dimensional conﬁguration space. This ﬁgure allows us to contrast the energy in both its exact and approximate guises. It is clear that in the vicinity of the minimum, the total energy is well characterized by what will shortly be revealed as a far-reaching but tractable model. Further progress can be made in trimming down the various terms embodied in the equation above by recognizing that the expansion is built around

5.2 Mechanics of the Harmonic Solid

215

Full Nonlinear Potential

Quadratic Potential

Fig. 5.2. Nonlinear potential energy V (x1 , x2 ) and corresponding quadratic approximation to that potential. The cutaway in the upper left hand corner shows one quadrant of the two potentials to illustrate their correspondence in the limit of small displacements.

the equilibrium conﬁguration and hence the terms linear in u iα can be eliminated since at equilibrium we have ∂ E tot /∂ Riα = 0. Furthermore, since the ﬁrst term is an uninteresting constant it is found convenient to deﬁne our zero of energy as ref E tot ({Ri }) = 0 leaving us with the result that ref

E tot ({Ri + ui }) =

1 αβ K u iα u jβ , 2 iα jβ i j

(5.2)

where the stiffness matrix (more conventionally known as the force constant matrix) is deﬁned by αβ

Ki j =

∂ 2 E tot . ∂ Riα ∂ R jβ

(5.3)

Note that the expressions we have written thus far are entirely generic. All that we have assumed is the existence of a total energy function that is dependent upon the set of ionic positions. Our analysis is thus indifferent to the microscopic energy functional used to compute E tot and hence the results are equally valid for total energy methods ranging from pair potentials to fully quantum mechanical E tot s. On

216

5 Thermal and Elastic Properties of Crystals

the other hand, the ease with which we can expect to determine the stiffness matrix is signiﬁcantly different, with pair potentials allowing for analytic determination of K and density functional calculations demanding a signiﬁcant computational effort. From the standpoint of our consideration of effective theories, it is especially interesting to note that regardless of our choice of microscopic energy functional, the result embodied in eqn (5.2) is nothing but a sophisticated model of atoms coupled with springs.

5.2.2 Atomic Motion and Normal Modes Having identiﬁed our approximation to the total energy associated with small vibrations about equilibrium, we are now in a position to construct the classical equations of motion which dictate the ionic motions. If we make the simplifying assumption that we are concerned with an elemental material (i.e. all the masses are identical, etc.), thus surrendering some of the possible generality of our treatment, the equation of motion for the α th component of displacement associated with the i th ion is given by m

αβ ∂ E tot d 2 u iα = − = − K i j u jβ . dt 2 ∂ Riα jβ

(5.4)

We note, however, that the added complication of including different masses at different sites does not change any of the key physical ideas. For further details the reader is urged to consult Maradudin et al. (1971). What has emerged from our analysis is a series of coupled linear differential equations in which the accelerations at one site are coupled to the displacements at the other sites. Though clearly our ambition at this point is to solve these coupled differential equations, we may recast this objective in different terms. In particular, we are after the appropriate linear combinations of the atomic-level displacements which will render the matrix K diagonal and lead to independent ‘modes’ of vibration. We anticipate the nature of the desired result by insisting that the solution take the form of a normal mode solution (which in the quantum setting we will refer to as phonons) in that each and every atom is imagined to vibrate with the same frequency ω but with different amplitudes. This conjectured behavior calls for the trial solution u iα (t) = u iα eiωt ,

(5.5)

where u iα is the amplitude of the displacement and where the physical motion is obtained by considering the real part of this expression. We hope the reader will forgive our notation in which the letter i serves both as a label of atomic positions as well as the unit imaginary number. Note that as yet we have presumed nothing

5.2 Mechanics of the Harmonic Solid

217

Fig. 5.3. Mass–spring system consisting of two point masses used in normal mode analysis considered in eqn (5.9).

about the possible geometric symmetries of the atomic positions. On the assumed solution given above, we ﬁnd that the equations of motion may be rewritten as αβ K i j u jβ . (5.6) −mω2 u iα = − jβ

This series of coupled linear equations in the unknowns u iα may be seen in a different light if written in direct form as the matrix equation, [K − mω2 I]u = 0,

(5.7)

where I is the identity matrix. Here we use the compact notation in which the displacements u iα are contained in the vector u 11

u 12 u 13 u= u 21 . ..

.

(5.8)

uN3 When our problem is recast in this form it is clear that we are reconsidering it as one of matrix diagonalization. Our task is to ﬁnd that change of variables built around linear combinations of the u iα s that results in a diagonal K. Each such linear combination of atomic displacements (the eigenvector) will be seen to act as an independent harmonic oscillator of a particular frequency, and will be denoted as ‘normal coordinates’. Before undertaking the formal analysis of vibrations in solids, it is worthwhile to see the machinery described above in action. For concreteness and utter simplicity, we elect to begin with a two-degrees-of-freedom system such as that depicted in ﬁg. 5.3. Displacements in all but the x-direction are forbidden, and we assume that both masses m are equal and that all three springs are characterized by a stiffness k. By inspection, the total potential energy in this case may be written as 1 1 1 V (u 1 , u 2 ) = ku 21 + ku 22 + k(u 2 − u 1 )2 , 2 2 2

(5.9)

218

5 Thermal and Elastic Properties of Crystals

where u i refers to the x-component of displacement of mass i. Following the prescription outlined in eqn (5.4), the two equations of motion become m u¨ 1 + 2ku 1 − ku 2 = 0,

(5.10)

m u¨ 2 + 2ku 2 − ku 1 = 0.

(5.11)

and

These equations can be rewritten in the more sympathetic matrix form as u1 u1 2k −k = mω2 . −k 2k u2 u2

(5.12)

This equation may be rewritten as the requirement 2k − mω2 −k det = 0, (5.13) −k 2k − mω2 √ √ which results in the vibrational frequencies ω− = k/m and ω+ = 3k/m. In fact, we could have arrived at the lower of these frequencies without calculation by noting that this mode corresponds to the motion of the two masses in unison without any stretching of the spring that couples them. In effect, they are vibrating as if they are only attached to the springs that are tied to the walls. The eigenvectors that are allied with our two frequencies correspond precisely to the motion in unison described above and the opposite mode in which the two masses are exactly out of phase. The general solution in this instance may then be written as 1 1 u 1 (t) = A1 cos ω− t + B1 sin ω− t 1 1 u 2 (t) 1 1 (5.14) + A2 cos ω+ t + B2 sin ω+ t. −1 −1 The undetermined coefﬁcients Ai and Bi allow for the speciﬁcation of the relevant initial data in the form of the initial positions and velocities of the two masses. In the more general setting in which we imagine 3N degrees of freedom, our analysis goes through in the same way. As mentioned earlier, the strategy remains one of ﬁnding independent normal modes in which every ion is presumed to vibrate at the same frequency. As with our two-masses problem, in principle all that remains is a diagonalization of the stiffness matrix K. If we consider the generalization to a fully three-dimensional situation, then the α th component of displacement of the i th ion may be represented in general terms as (s) u iα (t) = u iα (As cos ωs t + Bs sin ωs t), (5.15) s

where As and Bs are as-yet undetermined constants that insure that our solution has

5.2 Mechanics of the Harmonic Solid

219

(s) the full generality needed to capture an arbitrary state of displacement, u iα is that th part of the eigenvector associated with the s normal mode that is tied to the α th component of displacement of atom i and the sum over s is a sum over the various normal modes. As yet, we have illustrated that the mechanics of harmonic vibrations can be reduced to the consideration of a series of independent normal modes. This normal mode decomposition is an especially powerful insight in that it points the way to the statistical mechanical treatment of the problem of the thermal vibrations of a crystal. The Hamiltonian for the problem of harmonic vibrations can be written as

H=

p2 1 αβ iα + K u iα u jβ , 2m 2 i j αβ i j iα

(5.16)

where piα is the α th component of momentum associated with atom i and the second term is the harmonic part of the potential energy of the system as introduced in eqn (5.2). The key result we will highlight presently is that when this Hamiltonian is rewritten in terms of the normal modes, it reduces to a series of uncoupled harmonic oscillators which from the point of view of both quantum and statistical mechanics may each be treated independently. As it stands, the Hamiltonian as written in eqn (5.16) represents a coupled problem since the equation of motion for the i th atom depends upon the coordinates of the remaining atoms. Again in keeping with our contention that much of the business of effective theory construction is about ﬁnding the right degrees of freedom, we note that in the present context by adopting the correct linear combinations of the original coordinates {u iα }, the original problem can be recast in much simpler terms. To simplify the analysis, we introduce the notation ηr (t) = Ar cos ωr t + Br sin ωr t. In terms of this notational convention, eqn (5.15) may be rewritten as (s) u iα ηs (t), (5.17) u iα (t) = s

and hence the original Hamiltonian may similarly be rewritten as 1 αβ (r ) (s) 1 (r ) (s) u iα u iα η˙r (t)η˙ s (t) + K u u ηr (t)ηs (t). (5.18) H= m 2 iα r s 2 i j αβ r s i j iα iβ This expression may now be cast in its most useful form by recourse to certain (s) . In particular, key orthogonality relations satisﬁed by the eigenvectors u iα (r ) (s) we assert without proof (see Marion (1970)) that iα u iα u iα = δr s and that αβ (r ) (s) 2 i K i j u iα u ibeta = ωr δr s . In light of these orthogonality relations, our Hamiltonian reduces to 1 1 2 2 2 η˙ (t) + ωr ηr (t) . (5.19) H= 2 r 2 r

220

5 Thermal and Elastic Properties of Crystals

What we have learned is that our change to normal coordinates yields a series of independent harmonic oscillators. From the statistical mechanical viewpoint, this signiﬁes that the statistical mechanics of the collective vibrations of the harmonic solid can be evaluated on a mode by mode basis using nothing more than the simple ideas associated with the one-dimensional oscillator that were reviewed in chap. 3. We have already learned a great deal about the atomic-level treatment of vibrations in solids and in the paragraphs that follow intend to consolidate our gains by invoking the known translational periodicity of crystals. Let us examine what more can be said about the vibrational spectrum without actually doing any calculations. First, we note that for a generic conﬁguration of N atoms, there will be 3N vibrational modes, corresponding to the dimensionality of the stiffness matrix itself. We have found that the eigenvectors associated with the stiffness matrix may be constructed to form an orthonormal set, and that we can determine coefﬁcients such that arbitrary initial data may be matched. However, as yet there has been a serious oversight in our reasoning. We have forgotten that in the case of crystalline solids, the repetitive nature of the geometry implies special symmetry relations that lead to vast simpliﬁcations in the analysis of both their electronic and vibrational states. At this point we are poised to replace our problem of diagonalization of a 3N × 3N matrix by N diagonalizations of a 3 × 3 matrix. The crucial insight that makes this further simpliﬁcation of our problem possible is known as either Bloch’s theorem or Floquet analysis. As was already shown in chap. 4 (see eqn (4.68)), the basic idea is the assertion that on account of the translational periodicity, the solution in one unit cell can differ from that in other cells by at most a phase factor. The physical content of the statement above can be translated into mathematical terms by recognizing that this extra piece of information about the solution allows us to go beyond the trial solution of eqn (5.5), to suggest u iα (t) = u α eiq·Ri −iωt .

(5.20)

Note that we have presumed something further about the solution than we did in our earlier case which ignored the translational periodicity. Here we impose the idea that the solutions in different cells differ by a phase factor tied to the Bravais lattice vector Ri . The result is that the eigenvector u α has no dependence upon the site i; we need only ﬁnd the eigenvectors associated with the contents of a single unit cell, and the motions of atoms within all remaining cells are unequivocally determined. Substitution of the expression given above into the equations of motion yields αβ K i j u β (q)eiq·Rj = 0. (5.21) −mωq2 u α (q)eiq·Ri + jβ

By virtue of the crystal’s periodicity we can, without loss of generality, take Ri =

5.2 Mechanics of the Harmonic Solid

0. The equation given above may consequently be rewritten Dαβ (q)u β (q) = 0, −mωq2 u α (q) +

221

(5.22)

β

where we have deﬁned the ‘dynamical matrix’ as αβ K 0 j eiq·Rj . Dαβ (q) =

(5.23)

j

As a result of these deﬁnitions, eqn (5.22) may be rewritten in matrix form as [D(q) − mω2 I]u(q) = 0.

(5.24)

Just as was found in the discussion prior to eqn (4.75), the set of allowed q vectors is restricted because of the condition that the crystal is periodic. Indeed, because of this restriction, the q vectors are of the form qx = 2πm 1 /N a, q y = 2πm 2 /N a and qz = 2π m 3 /N a, where m 1 , m 2 and m 3 take only integer values. We have thus reduced our original problem which demanded the diagonalization of a 3N × 3N matrix to a problem in which we diagonalize a 3 × 3 matrix N times, where q adopts N different values and labels the different vibrational states. Here we have trimmed our analysis down such that we consider only the case in which there is one atom per unit cell. Aside from index gymnastics, the extension to more atoms in each cell is relatively uneventful. Note also that the present discussion parallels, even in the details, that already given in the context of the electronic structure of periodic solids in chap. 4. What we have learned is that our solutions may be labeled in terms of the vector q, which is known as the wavevector of the mode of interest. Each such mode corresponds to a displacement wave with wavelength λ = 2π/|q|. This interpretation makes it clear that there is a maximum |q| above which the oscillations are associated with lengths smaller than the lattice parameter and hence imply no additional information. This insight leads to an alternative interpretation of the signiﬁcance of the ﬁrst Brillouin zone relative to that presented in chap. 4. As an aside, we also note that had we elected to ignore the translational periodicity, we could just as well have solved the problem using the normal mode idea developed earlier. If we had followed this route, we would have determined 3N vibrational frequencies (as we have by invoking the translational periodicity), but our classiﬁcation of the solutions would have been severely hindered. The standard textbook exercise for illuminating the ideas discussed above in their full generality is that of the linear chain of atoms. The simplest variant of this exercise assumes that all the masses are the same as are all of the springs joining them. In this case, the dynamical matrix itself is one-dimensional and hence its

222

5 Thermal and Elastic Properties of Crystals

eigenvalues are immediate. From above, we note that K 011j eiq R j , D11 (q) =

(5.25)

j

where in our case we have K 00 = 2k, and K 01 = K 0,−1 = −k. To see this, recall that the total potential energy of our one-dimensional chain can be written in simplest terms as 1 ki j (u i − u j )2 . (5.26) E tot = 2 ij If we make the simplifying assumption of only nearest-neighbor interactions via springs of stiffness k, then the only terms involving atom 0 are 1 (5.27) E 0 = k (u 0 − u −1 )2 + (u 1 − u 0 )2 . 2 In light of this insight, it follows that the elements of the stiffness matrix are those assigned above. Explicitly evaluating the sums demanded by the dynamical matrix, yields the spectrum 4k qa sin . (5.28) ω(q) = m 2 This spectrum of vibrational frequencies is shown in ﬁg. 5.4. We note again that the signiﬁcance of this result is that it tells us that if we are interested in a particular displacement wave characterized by the wavevector q, the corresponding frequency associated with that wave will be ω(q). One of the key outcomes of this calculation is that it shows that in the limit of long wavelengths (i.e. small qs) the conventional elastic wave solution is recovered (i.e. ω = Cq, where C is the relevant sound velocity), while at the zone edges the waves are clearly dispersive. The use of the word dispersive is intended to convey the idea that the wave speed, dω/dq, depends explicitly on q. An additional way in which the outcome of the normal mode analysis may be analyzed is by recourse to the distribution of vibrational frequencies. This distribution of modes is captured most succinctly via the vibrational density of states deﬁned by ρ(ω) =

N modes

δ(ω − ωn ).

(5.29)

n=1

The idea here is that the Nmodes vibrational frequencies may be bunched up over certain frequencies, and will have some maximum frequency. Just as the electronic density of states introduced in chap. 4 succinctly encompassed much of the key information about the electronic spectrum, the vibrational density of states will

5.2 Mechanics of the Harmonic Solid

223

Fig. 5.4. Dispersion relation, ω vs q, for a linear chain of atoms.

play an analogous role in our analysis of the thermodynamics of solids. In the case of the linear chain, we may arrive at the vibrational density of states analytically. Before venturing our analytic solution for the vibrational density of states, we examine the ideas pictorially. In ﬁg. 5.4 we examine the dispersion relation. Note that each region of q-space of width 2π/N a corresponds to a single mode. (In fact, we need to be slightly cautious on this point since in addition to the mode with wavevector q there is a partner mode with wavevector −q.) However, we have interested ourselves in the distribution of states as a function of frequency ω. The correspondence is made in the ﬁgure where we note that in regions where ∂ω/∂q ≈ 0, there are many q-vectors per unit interval in ω while for those regions where ∂ω/∂q is large, there are but a few. To compute the vibrational density of states explicitly, we make the correspondence ρ(ω)dω = (N a/π )dq. What we have noted is that in a region of q-space of width dq, there are 2dq/(2π/N a) states since the uniform spacing between q-points is 2π/N a and the factor of 2 in the numerator accounts for the q and −q degeneracy. We may reorganize this statement as ρ(ω) =

1 Na . π |dω/dq|

(5.30)

For the dispersion relation given above for the linear chain, we have ω0 a qa dω = cos , dq 2 2

(5.31)

√ where we have deﬁned ω0 = 4K /m. We must now rewrite the right hand side of this equation in terms of ω. We note that qa −1 ω . (5.32) = sin 2 ω0

224

5 Thermal and Elastic Properties of Crystals

Fig. 5.5. Vibrational density of states associated with linear chain.

This is nothing more than an inversion of the dispersion relation. In geometric " 2 2 terms, what we have learned is that cos(qa/2) = ω0 − ω /ω0 and thus ρ(ω) =

1 2N " , π ω2 − ω2 0

(5.33)

which is shown in ﬁg. 5.5. As noted earlier, the vibrational density of states provides an alternative representation of the information content present in the dispersion relation, though there is a loss of information concerning the q vector associated with each frequency. As will be seen in subsequent discussions, a knowledge of the vibrational density of states will allow us to compute key thermodynamic properties such as the entropy associated with thermal vibrations. What has been lost in our treatment of the restricted geometry of the onedimensional chain is the possibility for different wave polarizations to be associated with each wavevector. In particular, for a three-dimensional crystal, we expect to recover modes in which the vibrations are either parallel to the wavevector (longitudinal) or perpendicular to it (transverse). On the other hand, the formalism outlined above already makes the outcome of this analysis abundantly clear. In particular, for a simple three-dimensional problem in which we imagine only one atom per unit cell, we see that there are three distinct solutions that emerge from our matrix diagonalization, each of which corresponds to a different polarization. To make these ideas concrete, we consider the case of a solid characterized by a pair potential and with a total energy of the form E tot =

1 φ(Ri j ). 2 ij

(5.34)

5.2 Mechanics of the Harmonic Solid

225

αβ

Our charter is to ﬁrst compute the matrix K i j introduced earlier and then to evaluate its Fourier transform in preparation for the computation of the spectrum αβ of vibrational frequencies. By deﬁnition, the matrix K i j is obtained as αβ

Ki j =

∂ 2 E tot . ∂ Riα ∂ R jβ

(5.35)

Within the pair potential formalism under consideration presently, this involves a series of exercises in the use of the chain rule since we have to evaluate terms of the form ∂ E tot 1 ∂ Rlm = φ (Rlm ) . (5.36) ∂ Riα 2 lm ∂ Riα Note that there is a slight burden of notational baggage which we will try to dispel by observing that we have deﬁned Rlm = |Rl − Rm |, and at the same time have used Riα to denote the α th Cartesian component of the position vector of atom i. Thus we have adopted a convention in which a pair of Latin indices implies consideration of a pair of atoms, while a mixed pair of a single Latin and a single Greek index refers to a particular component of the position vector of a given atom. Carrying out the differentiations demanded by eqn (5.35), the force constant matrix may be written as αβ

(Riα − Rmα )(Riβ − Rmβ ) δi j 2 Rim m (Riα − R jα )(Riβ − R jβ ) − φ (Ri j ) Ri2j δi j δαβ (Riα − Rmα )(Riβ − Rmβ ) + φ (Rim ) − φ (Rim ) δi j 3 Rim Rim m m

Ki j =

φ (Rim )

+ φ (Ri j )

(Riα − R jα )(Riβ − R jβ ) δαβ − φ (Ri j ) . 3 Ri j Ri j

(5.37)

We show this result primarily to illustrate that what are really required to determine the force constant matrix are the derivatives of the relevant interatomic potential, and then the consideration of a series of lattice sums as embodied in the various m s that appear above. Once the force constant matrix is in hand, the next step in the procedure for obtaining the spectrum of vibrational frequencies is the determination of the dynamical matrix. For the simple case in which there is only one atom per unit cell, this amounts to carrying out the sums illustrated in eqn (5.23). It is worth exploring this question a little further. We note that we require the αβ sum Dαβ (q) = j K 0 j eiq·Rj . Analytic progress can be made by exploiting several

226

5 Thermal and Elastic Properties of Crystals αβ

key symmetries of the force constant matrix K i j . First, we claim that there is a αβ sum rule of the form j K 0 j = 0 which arises from the fact that if every atom is displaced by the same amount, there is no net force on any atom (for further details see the problems at the end of the chapter). This then allows us to note that we can rewrite the self-term in the force constant matrix as αβ αβ K0 j . (5.38) K 00 = − j=0

As a result of the observation implicit in eqn (5.38), we can now write the dynamical matrix as αβ Dαβ (q) = K 0 j (eiq·Rj − 1). (5.39) j=0

This may be further simpliﬁed by noting that for every term R j in the sum we will have a partner term −R j , and also by using the fact that the force constant matrix is the same for these partner terms. As a result, we have 1 αβ iq·Rj Dαβ (q) = K (e + e−iq·Rj − 2), (5.40) 2 j=0 0 j which after simpliﬁcation leaves us with Dαβ (q) = −2

j=0

αβ

K 0 j sin2

q · Rj . 2

(5.41)

The conclusion of this analysis is that we can obtain the dynamical matrix by performing lattice sums involving only those parts of the force constant matrix that αβ do not involve the self-terms (i.e. K 00 ). We note that the analysis we have made until now has been performed in the somewhat sterile setting of a pair potential description of the total energy. On the other hand, the use of more complex energy functionals does not introduce any new conceptual features. As a case study in the calculation of the relation between ω and q (also known as phonon dispersion relations) for three-dimensional crystals, we consider the analysis of normal modes of vibration in fcc Al. As will be evident repeatedly as coming chapters unfold, one of our principal themes will be to examine particular problems from the perspective of several different total energy schemes simultaneously. In the present context, our plan is to consider the dispersion relations in Al as computed using both empirical pair functional calculations as well as ﬁrst-principles calculations. As the analysis given above illustrated for the case of a pair potential, the determination of the dynamical matrix demands the evaluation of lattice sums involving the products of geometric factors and the derivatives of the various

5.2 Mechanics of the Harmonic Solid [q00]

X

[qq0]

227 [qqq]

L

10

Al

T2

(THz)

8

6

4

L L

L

T1

T

T

2

0 0.00 0.25 0.50 0.75 1.00 q

0.75

0.50 q

0.25

0.00

0.25 q

0.50

Fig. 5.6. Phonon dispersion relation for Al as computed using pair functional approach (adapted from Mishin et al. (1999)). The lines correspond to the theoretical results and the points are experimental data obtained from neutron scattering.

energy terms. The basic procedure is unchanged in the case of the pair functional scheme although the presence of the embedding term introduces a whole new set of terms in the force constant matrix and hence in the dynamical matrix as well. A particularly simple description of these additional terms may be found in Finnis and Sinclair (1984). Once the lattice sums required in the computation of the force constant matrix have been carried out, all that remains is the calculation and subsequent diagonalization of the dynamical matrix with results like those shown in ﬁg. 5.6. The results given above can be measured not only against those resulting from experiments, but also against those deduced on the basis of ﬁrst-principles calculations. An example of the outcome of a ﬁrst-principles analysis of phonons in fcc Al is shown in ﬁg. 5.7 (Quong and Klein 1992). These calculations were carried out using pseudopotentials to represent the ion–electron interaction and with a plane wave basis for expanding the wave function. We note in passing that the use of ﬁrst-principles techniques to compute the phonon spectrum involves further subtleties than were hinted at in our discussion above, and we content ourselves only with showing the results of such calculation. We wish to emphasize that our primary ambition in the present setting has not been to debate the vices and virtues of any particular treatment of the lattice vibrations of a particular system. Rather, our aim has been to illustrate what is involved in carrying out such calculations and to reveal the way in which the outcome of these calculations is communicated,

228

5 Thermal and Elastic Properties of Crystals

Fig. 5.7. Phonon dispersion relation for Al as computed using ﬁrst-principles methods (adapted from Quong and Klein (1992)).

namely in terms of the types of phonon dispersion relations shown in ﬁgs. 5.6 and 5.7.

5.2.3 Phonons Until now, our treatment has been built in exactly the same terms that might have been used in work on normal modes of vibration in the latter part of the nineteenth century. However, it is incumbent upon us to revisit these same ideas within the quantum mechanical setting. The starting point of our analysis is the observation embodied in eqn (5.19), namely, that our harmonic Hamiltonian admits of a decomposition into a series of independent one-dimensional harmonic oscillators. We may build upon this observation by treating each and every such oscillator on the basis of the quantum mechanics discussed in chap. 3. In light of this observation, for example, we may write the total energy of the harmonic solid as

1 (5.42) n(q, α) + h¯ ωq,α . E= 2 q,α The interpretation that we adopt in this setting is that the various modes are each characterized by a different occupation number, n(q, α), where q characterizes the wavevector of the mode of interest and α labels the various polarizations. In this context, the occupation of each normal mode is associated with a discrete entity known as a phonon. Each such phonon carries an energy h¯ ω(q, s) and a momentum h¯ q and may be assigned properties traditionally thought of as being tied to particles. For example, phonons may scatter off of one another. However, we also note that in order to develop a full picture of the phonons and their interactions,

5.2 Mechanics of the Harmonic Solid

229

Fig. 5.8. Schematic of the C60 molecule (adapted from Woo et al. (1993)).

it is necessary to extend the harmonic treatment of vibrations entertained above to include the anharmonic effects which give rise to such scattering.

5.2.4 Buckminsterfullerene and Nanotubes: A Case Study in Vibration One of the approaches favored in the present work is the idea of attempting to give a thorough description of robust physical principles followed by more speculative application of those principles to problems of current interest. One class of materials that has garnered particular attention in recent years is the class of fullerenes in which by virtue of either ﬁve- or seven-membered rings, curvature is induced in the normally ﬂat packings of carbon based upon six-membered rings. The most celebrated such example is perhaps the C60 molecule in which a total of 60 carbon atoms form a molecular structure with vertices reminiscent of those on a soccer ball. Beyond the interest that has attached to C60 itself, there has been a surge of interest in carbon nanotubes. The aim of the present subsection is to give a sense of how the physics of phonons introduced above plays out in the context of relatively complex molecules and solids. The C60 molecule is shown in ﬁg. 5.8. The distinctive ﬁve-fold rings are clearly evident in the ﬁgure. In this instance, we have 3N = 180 independent degrees of freedom, although six of them are associated with uninteresting rigid body translations and rotations. Our aim in the present section is to examine the nature of vibrations in several exotic carbon structures, and we begin with the C60 itself. The calculations to be described here were based on ﬁrst-principles techniques in which the electron–ion interaction was handled using pseudopotentials in conjunction with a mixed basis including both plane wave states and localized s- and p-orbitals associated with the carbon atoms (Bohnen et al. 1995). As has already been made clear, to

230

5 Thermal and Elastic Properties of Crystals

Fig. 5.9. Vibrational displacement patterns associated with ﬁve different modes of the C60 molecule (adapted from Heid et al. (1997)). The left and right hand panels correspond to opposite extremes in motion associated with a given mode. Labels associated with each mode characterize the symmetry of the displacement pattern.

obtain the phonon frequencies, it is necessary to construct the dynamical matrix. Diagonalization of this matrix results in a series of vibrational frequencies ωs and associated eigenvectors which give the relative amplitudes of vibration for the different degrees of freedom. The disposition of the vibrational frequencies may be summarized pictorially via the vibrational density of states. Note that in a highly symmetric object like the C60 molecule the occurrence of certain degeneracies in this spectrum is not accidental and can be predicted on the grounds of this symmetry without doing any explicit matrix diagonalizations. In addition to our interest in the spectrum of vibrational frequencies that emerge from the type of analysis being described here, it is also of interest to characterize the nature of the associated eigenvectors. Recall that these eigenvectors yield the nature of the displacement patterns that will be associated with a given mode of vibration. In the case of C60 , some of the different displacement patterns are revealed in ﬁg. 5.9, though the amplitudes of the displacements are exaggerated to more easily reveal the symmetry of the various modes. As noted above, in addition to the interest that has been attached to the C60 molecule and its crystalline incarnations, a torrent of interest has also developed around the existence of carbon nanotubes in which planar graphite-like packings of carbon atoms are folded onto themselves to form cylinders. We note that there is great variety in the structures that can be created since the line along which the original planar sheet is cut prior to wrapping it to form a tube can be chosen in many different ways. In addition, different tube radii can be selected. In ﬁg. 5.10

5.3 Thermodynamics of Solids

231

Fig. 5.10. Dispersion relations for several different carbon nanotube structures (adapted from Yu et al. (1995)).

we show the results of tight-binding calculations of the vibrational spectrum of several different nanotube variants. Part of the value in presenting these results is the reminder that calculations of quantities such as the vibrational spectrum of a material can be carried out in any of a number of different ways. Already in this chapter we have seen such dispersion relations computed using pair functionals (for Al), ﬁrst principles (for fcc Al and C60 ) and tight-binding analysis (the present case). Just as was possible with the analysis revealed of the displacement patterns in C60 , it is possible to examine the nature of the vibrations associated with nanotubes as well. An example of the various eigenvectors associated with a particular nanotube is shown in ﬁg. 5.11.

5.3 Thermodynamics of Solids 5.3.1 Harmonic Approximation As we saw above, what emerges from our detailed analysis of the vibrational spectrum of a solid can be neatly captured in terms of the vibrational density of states, ρ(ω). The point of this exercise will be seen more clearly shortly as we will observe that the thermodynamic functions such as the Helmholtz free energy can be written as integrals over the various allowed frequencies, appropriately weighted by the vibrational density of states. In chap. 3 it was noted that upon consideration of a single oscillator of natural frequency ω, the associated Helmholtz free energy is F=

h¯ ω ) ¯ + kT ln(1 − e−(hω/kT ). 2

(5.43)

232

5 Thermal and Elastic Properties of Crystals

Fig. 5.11. Illustration of a variety of different vibrational modes of one of the broad class of carbon nanotubes (adapted from Yu et al. (1995)).

In light of our observations from above, namely that the vibrational contribution to the energy of the crystal may be written as a sum of independent harmonic oscillators, this result for the Helmholtz free energy may be immediately generalized. In particular, we note that once the vibrational density of states has been determined

5.3 Thermodynamics of Solids

it is immediate that ∞ ∞ h¯ ω ) ¯ ρ(ω)dω + kT ρ(ω) ln(1 − e−(hω/kT )dω. F= 2 0 0

233

(5.44)

Note that all reference to the wavevector has been eliminated as a result of the fact that ρ(ω) is obtained by averaging over all wave vectors within the Brillouin zone, and is hence indifferent to the polarization and propagation vector of a given normal mode. In sections 5.22 and 5.24, we have made schematic evaluations of the nature of the vibrational spectrum (see ﬁg. 5.5). At this point, it is convenient to construct approximate model representations of the vibrational spectrum with the aim of gleaning some insight into how the vibrational free energy affects material properties such as the speciﬁc heat, the thermal expansion coefﬁcient and processes such as structural phase transformations. One useful tool for characterizing a distribution such as the vibrational density of states is through its moments, deﬁned by ∞ µn = ωn ρ(ω)dω. (5.45) 0

The most naive model we can imagine is to insist that whatever model we select for the density of states faithfully reproduces the ﬁrst moment of the exact vibrational density of states. That is, ∞ ∞ ωρexact (ω)dω = ωρmodel (ω)dω. (5.46) 0

0

We can guarantee this by following Einstein and asserting that all of the spectral weight is concentrated in a single vibrational frequency, ω E . That is, we approximate the full density of states with the replacement ρexact (ω) → ρ E (ω) = 3N δ(ω − ω E ). The partition function for the model presented above is given by 3N β hω ¯ E e− 2 Z= . ¯ E 1 − e−β hω

(5.47)

(5.48)

This may be seen by noting that the partition function may be written as a series of sums of the form

∞ ∞ 1 h¯ ωi . ··· exp −β ni + (5.49) Z= 2 n 3N i n =0 1

234

5 Thermal and Elastic Properties of Crystals

However, in the case of the Einstein model ωi = ω E for all ω and hence the sum indicated above may be rewritten as

∞ ∞ 1 1 h¯ ω E · · · h¯ ω E , (5.50) exp −β n 1 + exp −β n 3N + Z= 2 2 n =0 n =0 1

3N

which is equivalent to the product written in eqn (5.48). As noted already in chap. 3, once the partition function is in hand, we are in a position to evaluate properties of thermodynamic interest such as the average energy which is given by eqn (3.98) and in the present context may be written as U = −

3N h¯ ω E 3N h¯ ω E ∂ ln Z = + β hω . ∂β 2 e ¯ E −1

(5.51)

Recalling the deﬁnition of the speciﬁc heat as the temperature derivative of the average energy (see eqn (3.99)), it is found that for the Einstein solid C V = 3N k(β h¯ ω E )2

¯ E eβ hω . β hω (e ¯ E − 1)2

(5.52)

The average energy and the associated speciﬁc heat are plotted in ﬁg. 5.12. These are precisely the same results derived in our treatment of the statistical mechanics of a single oscillator in chap. 3, but now imbued with the extra insights that come from knowing how the vibrational frequencies emerge from microscopic analysis. This model represents one of the ﬁrst (if not the ﬁrst) examples of the use of reasoning based on quantum theory in order to deduce the properties of materials. One of the key features of this result is the fact that at high temperatures it reduces to the known high-temperature limit, C V = 3N k, while vanishing at low temperature (though not with the proper scaling with T as we shall see in our discussion of the Debye model). As yet, we have made a very crude approximation to the exact density of states. In particular, we have replaced the full vibrational density of states by a single delta function according to the prescription ρ(ω) = δ(ω − ωn ) → 3N δ(ω − ω E ). (5.53) n

We now consider a more quantitative model of the vibrational density of states which makes a remarkable linkage between continuum and discrete lattice descriptions. In particular, we undertake the Debye model in which the vibrational density of states is built in terms of an isotropic linear elastic reckoning of the phonon dispersions. Recall from above that in order to effect an accurate calculation of the true phonon dispersion relation, one must consider the dynamical matrix. Our approach here, on the other hand, is to produce a model representation of the phonon dispersions which is valid for long wavelengths and breaks down at

5.3 Thermodynamics of Solids

235

Fig. 5.12. Plots of the dimensionless average energy and speciﬁc heat resulting from the Einstein model. The average energy is scaled by 3N E E , where E E = h¯ ω E , while the speciﬁc heat is reported in units of 3N k. The temperature is also plotted in units of the Einstein temperature given by TE = h¯ ω E /k.

shorter wavelengths. One approach to this analysis is to linearize the dynamical matrix. An alternative route is to compute the linear elastic dispersion relation explicitly. In order to make this calculation it is well to recall the equations of linear elastodynamics, namely, Ci jkl u k,l j = ρ

∂ 2ui . ∂t 2

(5.54)

In the present setting ρ is the mass density while the subscript i identiﬁes a particular Cartesian component of the displacement ﬁeld. In this equation recall that Ci jkl is the elastic modulus tensor which in the case of an isotropic linear elastic solid is given by Ci jkl = λδi j δkl + µ(δik δ jl + δil δ jk ). Following our earlier footsteps from chap. 2 this leads in turn to the Navier equations (see eqn (2.55))

236

5 Thermal and Elastic Properties of Crystals

which it is to be remembered are given by (λ + µ)∇(∇ · u) + µ∇ 2 u = ρ

∂ 2u , ∂t 2

(5.55)

in the dynamical case. These equations admit of wave solutions of the form u i = u i0 ei(q·r−ωt) like those advanced in the treatment of vibrations in terms of the dynamical matrix. Substitution of this trial solution into the Navier equations yields their q-space analog, namely, [(λ + µ)qi q j + µq 2 δi j − ρω2 δi j ]u j0 = 0.

(5.56)

Once again, our problem of determining the wave solutions associated with our medium has been reduced to a problem of matrix diagonalization. The eigenvalues of the acoustic tensor or Christoffel tensor, Ai j = (λ + µ)qi q j + µq 2 δi j , are found to be µ q (5.57) ωT = ρ and

ωL =

λ + 2µ q, ρ

(5.58)

corresponding to transverse (ωT ) and longitudinal (ω L ) waves, in which the displacements are either perpendicular or parallel to the propagation direction, respectively. The solution associated with transverse waves is doubly degenerate in that there are two distinct solutions with this same eigenfrequency. The solution arrived at in our linear elastic model may be contrasted with those determined earlier in the lattice treatment of the same problem. In ﬁg. 5.13 the dispersion relation along an arbitrary direction in q-space is shown for our elastic model of vibrations. Note that as a result of the presumed isotropy of the medium, no q-directions are singled out and the dispersion relation is the same in every direction in q-space. Though our elastic model of the vibrations of solids is of more far reaching signiﬁcance, at present our main interest in it is as the basis for a deeper analysis of the speciﬁc heats of solids. From the standpoint of the contribution of the thermal vibrations to the speciﬁc heat, we now need to determine the density of states associated with this dispersion relation. As was noted earlier in the context of phonons, the density of states in q-space is constant, with one state per unit volume V /(2π )3 of q-space. That is, the set of allowed q-vectors form a lattice in q-space with each and every lattice point corresponding to a different allowed state. Our intention now is to recast this result in frequency space. We know that in a volume d 3 q of q-space there

5.3 Thermodynamics of Solids

237

Fig. 5.13. Dispersion relation obtained if solid is characterized by linear elastic constitutive model.

are V /(2π)3 d 3 q states. We now interest ourselves in the total number of states between two constant ω surfaces at ω and ω + dω. The total number of states in this shell is V dq⊥ d A, N= (5.59) (2π )3 where dq⊥ is the height of the volume element at a given position on the constant frequency surface being integrated over and d A is the area element on the constant frequency surface. The logic behind this equation is that we have asked how many states are in the shell of thickness dq⊥ . Now we note that the increment in frequency over that same height is given by dω = |∇q ω|dq⊥ , suggesting the alternative and more useful expression V dω ρ(ω)dω = , (5.60) d A (2π )3 |∇q ω| for the vibrational density of states. Use of this expression in the context of the dispersion relations obtained above yields 2 V ω2 1 (5.61) + 3 , ρ(ω) = 2π 2 c3L cT where we have introduced the elastic wave speeds, c L = dω L /dq and cT = dωT /dq. We are now in a position to make an evaluation of the speciﬁc heat within this model. Recall from earlier that the average energy of an oscillator of frequency ω

238

5 Thermal and Elastic Properties of Crystals

is given by U =

h¯ ω , ¯ −1 eβ hω

(5.62)

where we have dropped reference to the zero point energy for simplicity. For our collection of oscillators described by the vibrational density of states determined above, we have then ωD h¯ V 1 2 ω3 dω U = , (5.63) + ¯ −1 2π 2 c3L eβ hω cT3 0 where as yet all that remains undetermined is the upper cutoff frequency ω D , known as the Debye frequency. However, we know that the total number of modes of the system is 3N , where N is the number of atoms. As a result, we know that the density of states when integrated up to ω D must yield 3N . That is, ωD ρ(ω)dω = 3N . (5.64) 0

The reasoning invoked here is really no different than that associated with the Fermi level in electronic problems where we insisted that upon integrating the electronic density of states up to this level, the correct number of electrons was obtained (see eqn (4.88), for example). If we deﬁne the mean wave speed via 3 1 2 = 3 + 3, c¯3 cL cT

(5.65)

then the density of states may be rewritten as ρ(ω) = 3V ω2 /2π 2 c¯3 , which when substituted into the equation constraining the number of modes to 3N yields ω D = 1 2 c(6π ¯ N /V ) 3 . If we further deﬁne the Debye temperature θ D via h¯ ω D = kθ D , our expressions for the average energy may be differentiated to yield the speciﬁc heat which may itself be written in the considerably simpliﬁed form 3 θ D 4 u T T u e du . (5.66) Cv = 9k N u − 1)2 θD (e 0 The Debye result for the speciﬁc heat of a solid is of profound signiﬁcance in elucidating the key physical features that attend the thermal properties of solids. One key observation that is immediate is that in the limit when the temperature is low in comparison with the Debye temperature, we have θ D /T → ∞, which implies that the upper limit in the integral given in eqn (5.66) may be taken as inﬁnity. The consequence of this insight is that the low-temperature speciﬁc heat scales with the temperature as T 3 . This result emerges in light of the fact that the integral is a pure number which has no dependence on the temperature. In particular, we note the characteristic T 3 scaling that is compared with experimental

5.3 Thermodynamics of Solids

239

values in ﬁg. 5.1. In the other extreme, namely at very high temperatures, we note that the Debye result may be rearranged to recover the classical result C V = 3N k of Dulong and Petit. Physically, the success of the Debye model may be attributed to the fact that at low temperatures it is only the low-energy (or low-frequency) parts of the phonon spectrum which are excited. This part of the spectrum corresponds in part to the long-wavelength part of the spectrum which is precisely that part of the dispersion relation that is captured correctly by the Debye model. By way of contrast, the high-temperature result recovers the equipartition theorem and is predicated upon a correct assessment of the total number of modes to be shared. The Debye result then smoothly interpolates between these two limits. As a reminder of what we have accomplished and where it ﬁts into our broader program, we summarize the arguments of the chapter up until this point. We begin by noting that in the limit in which it is imagined that the excursions of atoms as they exercise thermal vibrations are sufﬁciently small, the potential energy of all solids reduces to a sophisticated model of coupled springs. This is a fascinating example of the type of effective theory construction that we have harped on repeatedly and note that in this case it is an especially intriguing conclusion since this result is indifferent to the type of bonding in the solid, whether it be metallic, covalent, ionic or something else. Once the energetics of the harmonic solid was in hand, we were then able to demonstrate that there exists a natural set of coordinates (i.e. normal coordinates) for characterizing the vibrations of a solid as a set of independent oscillators. Finally, as a result of our knowledge of the vibrational spectrum of a solid, the tools of statistical mechanics were invoked in order to determine the mean energy and speciﬁc heat, and as will be shown in the next chapter, these same arguments can be exploited to examine the vibrational entropy and to determine its role in the free energy balance separating competing different crystal structures. We now turn to an examination of some of the anharmonic effects in solids such as the thermal expansion and the thermal conductivity.

5.3.2 Beyond the Harmonic Approximation Thus far, our analysis has been entirely predicated upon the harmonic approximation advanced in eqn (5.2). On the other hand, real crystals are characterized by nonlinear force laws and the resulting anharmonic effects are part of the story from the outset. If we conﬁne our interest to the speciﬁc heat, we see that much may be made of the harmonic approximation. However, if we aim to press our modeling efforts further, for example, to consider the thermal expansion or the thermal conductivity, we will see that the harmonic approximation does not sufﬁce. Let us ﬂesh out the logic in the case of the coefﬁcient of thermal expansion. Our ﬁrst ambition will be to demonstrate that the harmonic approximation predicts

240

5 Thermal and Elastic Properties of Crystals

zero thermal expansion. This will be followed by an explicit incorporation of anharmonicity. We have seen that as a consequence of the harmonic Hamiltonian that has been set up thus far, our oscillators decouple and in cases which attempt to capture the transport of energy via heating, there is no mechanism whereby energy may be communicated from one mode to the other. This shortcoming of the model may be amended by including coupling between the modes, which as we will show below, arises naturally if we go beyond the harmonic approximation. The simplest route to visualizing the physics of this problem is to assume that our harmonic model is supplemented by anharmonic terms, such as αβγ i jk u iα u jβ u kγ + · · · . (5.67) H anh = iα

jβ

kγ

This result urges us to consider the nonlinear terms which must supplement the αβγ quadratic model set forth in eqn (5.2). The coefﬁcients i jk are deﬁned in analogy αβ with the K i j deﬁned in eqn (5.3) and are given by αβγ

i jk =

∂ 3 E tot . ∂ Riα ∂ R jβ ∂ Rkγ

(5.68)

There are certain subtleties associated with the order to which the expansion of eqn (5.67) is carried and for a discussion of which we refer the perspicacious reader to chap. 25 of Ashcroft and Mermin (1976). If we maintain the use of normal coordinates, but now including the anharmonic terms which are represented via these coordinates, it is seen that the various modes are no longer independent. For the purposes of the present discussion, we see that these anharmonic terms have the effect of insuring that the equation of motion for the n th mode is altered by coupling to the rest of the mode variables. This result bears formal resemblance to the Navier–Stokes equations which when written in terms of the Fourier variables yield a series of mode coupled equations. We have already noted that the physics of both thermal expansion and thermal conductivity demand the inclusion of these higher-order terms. Recall that the coefﬁcient of thermal expansion is deﬁned as 1 ∂P α= , (5.69) 3B ∂ T V where B is the bulk modulus, itself deﬁned as B = −V (∂ p/∂ V )T . We may evaluate the pressure, needed to compute the thermal expansion coefﬁcient, as p = −(∂ F/∂ V )T . Using the fact that the Helmholtz free energy is obtained as

5.3 Thermodynamics of Solids

a sum over all modes as h¯ ω(q, α) ¯ + kT ln(1 − e−β hω(q,α) ), F= 2 q,α q,α the pressure may be written in turn as h¯ −∂ω(q, α) −∂ω(q, α)

1 + . p= h¯ β hω(q,α) ¯ ∂V ∂V e −1 q,α 2 q,α

241

(5.70)

(5.71)

In both of these sums, we are summing over the wavevector q and the polarization α of the various phonons. What we have found is that all of the putative volume dependence of the free energy is tied to the vibrational frequencies themselves. Once we have determined p, then the thermal expansion coefﬁcient may be computed as

∂ω(q, α) ∂n(ω, T ) 1 , (5.72) −h¯ α= 3B q,α ∂V ∂T where we have deﬁned n(ω, T ) =

1 . )−1 ¯ e(hω/kT

(5.73)

Though we have determined the coefﬁcient of thermal expansion in principle, the entirety of our analysis is focused on how the vibrational frequencies are altered under a uniform dilatational strain. However, in the absence of some form of anharmonicity, this model is as yet plagued with a fatal ﬂaw; the vibrational frequencies within the harmonic approximation have no such volume dependence. At this point, our idea is to revisit the expansion of eqn (5.2) with the ambition of determining how an effective volume dependence to the phonon frequencies can be acquired. In particular, we return to the expansion given in eqn (5.2), but now adjusted to reﬂect the presence of a homogeneous strain. If we imagine that ref the equilibrium positions of the undeformed crystal are given by Ri , then in the presence of a state of deformation characterized by the deformation gradient F, ref these positions are amended to FRi . The thermal vibrations about these positions ref follow by expanding E tot ({FRi + ui }). Terms will now arise that couple the homogeneous strain to the thermal vibrations. In particular, if we keep terms only to second order in the expansion we have, ∂ E tot ref ref u iα E tot ({FRi + ui }) = E tot ({FRi }) + ∂ Ri,α F i,α 2 ∂ E tot 1 + u iα u jβ . (5.74) 2 i,α j,β ∂ Riα ∂ R jβ F

242

5 Thermal and Elastic Properties of Crystals

Note that the stiffness coefﬁcients are now evaluated at the strained reference state (as signiﬁed by the notation (∂ E tot /∂ Riα )F ) rather than for the state of zero strain considered in our earlier treatment of the harmonic approximation. To make further progress, we specialize the discussion to the case of a crystal subject to a homogeneous strain for which the deformation gradient is a multiple of the identity (i.e. strict volume change given by F = λI). We now reconsider the stiffness coefﬁcients, but with the aim of evaluating them about the zero strain reference state. For example, we may rewrite the ﬁrst-order term via Taylor expansion as 2 ∂ E tot ∂ E tot ∂ E tot = + λ. (5.75) ∂ Ri,α F ∂ Ri,α 0 ∂ Ri,α ∂λ 0 Note that when this expansion is reinserted into eqn (5.74), the ﬁrst term will clearly vanish on account of the equilibrium condition, namely, (∂ E tot /∂ Riα )0 = 0. Through use of the chain rule, we rewrite the term that is linear in λ as 2 ∂ 2 E tot ∂ E tot λ= λRkγ . (5.76) ∂ Riα ∂λ 0 ∂ Riα ∂ Rkγ 0 kγ Substituting this result back into the expansion for the total energy, it is noted that for crystals with centrosymmetry, this term will vanish because every term involving λRkγ will have a compensating partner −λRkγ . We now adopt precisely the same strategy, this time with respect to the terms in the total energy that are quadratic in the displacements. In particular, we have 2 2 ∂ E tot ∂ E tot ∂ 3 E tot = + λ. (5.77) ∂ Riα ∂ R jβ F ∂ Riα ∂ R jβ 0 ∂ Riα ∂ R jβ ∂λ 0 αβ

The ﬁrst term on the right hand side is recognized precisely as the matrix K i j introduced earlier. The term that is linear in λ may be evaluated via the chain rule as ∂ 3 E tot ∂ 3 E tot λRkγ . = (5.78) ∂ Riα ∂ R jβ ∂λ ∂ Riα ∂ R jβ ∂ Rkγ kγ As a result of these manipulations, eqn (5.74) may be rewritten as 1 αβ 1 αβγ ref E tot ({FRi + ui }) = K i j u iα u jβ + λRkγ u iα u jβ , 2 i,α j,β 2 iα jβ kγ i jk (5.79) where we have thrown away uninteresting constant terms. This result may be rewritten more provocatively as 1 αβ ref αβ (K + δ K i j )u iα u jβ , (5.80) E tot ({FRi + ui }) = 2 i,α j,β i j

5.3 Thermodynamics of Solids

where we have made the deﬁnition αβ

δ Ki j =

αβγ

i jk λRkγ .

243

(5.81)

kγ

The consequence of this analysis is that the original stiffness matrix has been amended by terms that are linear in the strain λ and that therefore adjust the vibrational frequencies under a volume change. In particular, the ‘renormalized’ frequencies arise as the eigenvalues of the stiffness matrix

K = K + δK.

(5.82)

We are now in a position to reconsider the vibrational frequencies in light of the imposition of a small homogeneous strain. Recall that our strategy was to use the quadratic potential energy to produce equations of motion. Inspection of the potential energy developed above makes it clear that the term that is quadratic in the displacements has acquired additional complexity. In particular, if we derive the equations of motion on the basis of both our earlier quadratic terms and those considered here, then we ﬁnd that they may be written as αβ αβ (K i j + δ K i j )u jβ . (5.83) m u¨ iα = − jβ

Because of the term δK, when we evaluate ∂ω(q, α)/∂ V , as demanded by eqn (5.72) in our deduction of the thermal expansion coefﬁcient, it will no longer vanish as it would if we were only to keep K. The phonon frequencies have acquired a volume dependence by virtue of the quasiharmonic approximation which amounts to a volume-dependent renormalization of the force constant matrix. There are a few lessons learned from this analysis. First, we note that as was claimed above, keeping only the harmonic terms in the expansion of the potential energy results in no volume dependence to the vibrational frequencies, and hence to no thermal expansion. This is seen because the parameter λ, which carries the information about such volume dependence, makes its ﬁrst appearance in αβγ conjunction with the manifestly anharmonic term, i jk . This insight prepares us for the quasiharmonic approximation in which the volume dependence of the vibrational frequencies appears in a way that masquerades as a harmonic term. We are now in a position to revisit the analysis of the thermal expansion presented earlier. In particular, we note that the thermal expansion coefﬁcient may now be evaluated by attributing a particular form to the volume dependence of the phonon frequencies. In order to reveal the application of the developments advanced above, we undertake an analysis of the thermal expansion in the

244

5 Thermal and Elastic Properties of Crystals

relatively sterile setting of a one-dimensional chain of atoms interacting through a near-neighbor pair potential model for the total energy. As usual, the elaborations of the model to either higher dimensions or other total energy methods do not involve any new questions of logic, though they may imply severe notational and computational demands. It is one of my largest regrets to have foregone a discussion of the thermal conductivity. Such a discussion would have been opportune at this point since it involves much of the same logic that we invoked in our discussion of the thermal expansion, though reworked along the lines of examining the way in which mode coupling leads to phonon scattering. The interested reader is referred to several of the books described in the Further Reading section at the end of the present chapter. 5.4 Modeling the Elastic Properties of Materials As was discussed in some detail in chap. 2, the notion of an elastic solid is a powerful idealization in which the action of the entirety of microscopic degrees of freedom are subsumed into but a few material parameters known as the elastic constants. Depending upon the material symmetry, the number of independent elastic constants can vary. For example, as is well known, a cubic crystal has three independent elastic moduli. For crystals with lower symmetry, the number of elastic constants is larger. The aim of the present section is ﬁrst to examine the physical origins of the elastic moduli and how they can be obtained on the basis of microscopic reasoning, and then to consider the nonlinear generalization of the ideas of linear elasticity for the consideration of nonlinear stored energy functions. 5.4.1 Linear Elastic Moduli If a crystal is subjected to small strain elastic deformation it is convenient to imagine the energetics of the strained solid in terms of the linear theory of elasticity. As we noted in chap. 2, the stored strain energy may be captured via the elastic strain energy density which in this context is a strictly local quantity of the form 1 (5.84) W () = Ci jkl i j kl . 2 As usual, we are employing the summation convention which demands that we sum over all repeated indices. This relation is posited to apply pointwise, meaning that even if the state of deformation is spatially varying, the energy stored in the body by virtue of elastic deformation is obtained by adding up the energy of each volume element as though it had suffered homogeneous deformation. Despite our

5.4 Modeling the Elastic Properties of Materials

245

replacement of the entirety of the set of atomistic degrees of freedom with an effective description in terms of elastic strains, we may restore contact with the microscopic degrees of freedom via the elastic moduli in a way that will be made evident below. For our present purposes, we note that the correspondence of interest is given by 1 1 def undef Ci jkl i j kl = [E tot ({Ri }) − E tot ({Ri })]. (5.85) 2 The logic embodied in this expression is built around the recognition that from the continuum perspective the elastic strain energy density is the energy per unit volume above and beyond that of the perfect crystal and is given by the left hand side of eqn (5.85). The microscopic evaluation of this same quantity is def obtained by computing the energy of the deformed state (i.e. E tot ({Ri })) and subtracting off the energy of the perfect crystal which we have referred to as undef E tot ({Ri }), and then appropriately normalizing that energy with a volume factor so as to produce an energy density. To make the connection given in def eqn (5.85) computationally useful, we expand the total energy E tot ({Ri }) about the unstrained reference state, keeping terms only to second order in the strains. In particular, we write def

undef

E tot ({Ri }) ≈ E tot ({Ri

}) +

∂ E tot ∂i j

i j + ref

2 1 ∂ E tot i j kl . 2 ∂i j ∂kl ref

(5.86)

On the recognition that the expansion is about the reference state and hence that the linear term in the expansion vanishes (i.e. (∂ E tot /∂i j )ref = 0), eqn (5.85) reduces to 1 ∂ 2 E tot 1 Ci jkl i j kl = i j kl , 2 2 ∂i j ∂kl

(5.87)

where as usual we sum over all repeated indices, which illustrates that the elastic moduli are obtained as Ci jkl =

1 ∂ 2 E tot . ∂i j ∂kl

(5.88)

It is worth noting that this expression is generic as a means of extracting the elastic moduli from microscopic calculations. We have not, as yet, specialized to any particular choice of microscopic energy functional. The physical interpretation of this result is recalled in ﬁg. 5.2. The basic observations may be summarized as follows. First, we note that the actual energy landscape is nonlinear. One next adopts the view that even in the presence of ﬁnite deformations, there is a

246

5 Thermal and Elastic Properties of Crystals

strain energy density of the form W (F) which is a function of the macroscopic deformation gradient. In the neighborhoods of the minima of this nonconvex energy surface, it is convenient to parameterize the potential as a series of parabolic wells, the curvatures of which may be identiﬁed with the elastic moduli as we have done in eqn (5.88). In light of these gains we are now in a position to explicitly determine the elastic properties. As a ﬁrst step in this direction we exploit a pair potential description of the total energy. As promised in chap. 4, it will emerge shortly that such a description has serious shortcomings as concerns the elastic properties of materials. On the other hand, the pair potential picture has the salutary effect of demonstrating just how the atomic-level interactions manifest themselves in macroscopic observables such as the elastic moduli. Once we have seen just how these ideas emerge, the way will be paved for a more quantitative analysis of elasticity using more sophisticated total energy functionals. Within the pair potential setting where the total energy is given by E tot = 1 mn Veff (r mn ), the elastic moduli are given by 2 Ci jkl =

1 ∂ ∂ Veff (rmn ). 2 ∂i j ∂kl mn

(5.89)

Through judicious use of the chain rule, we end up with the generic expression

1 ∂rmn ∂rmn ∂ 2rmn + V (rmn ) V (rmn ) . (5.90) Ci jkl = 2 mn ∂i j ∂kl ∂i j ∂kl In this case, rmn refers to the distance between the m th and n th atoms in the deformed state in which the crystal is subjected to some homogeneous strain. If we assume that the deformed and reference positions are related by ri = FRi , then ri j may be rewritten as (5.91) ri j = Ri j · Ri j + 2Ri j · E · Ri j , where we have used the fact that the deformation gradient F and the Lagrangian strain tensor E are related by E = 12 (FT F − I) as shown in eqn (2.6), and we have used the deﬁnition Ri j = Ri − R j . In the limit of small displacement gradients we may replace E with in eqn (5.91). As a result of these geometric insights, the geometric derivatives written above may be evaluated with the result that

(Rm ) Rmi Rmj Rmk Rml Veff 1 Veff (Rm ) − . (5.92) Ci jkl = 2at m Rm Rm2 We have added another layer of notation in the form of the quantity at which is the volume per atom associated with the crystal of interest as well as the quantities Rmi , which refer to the i th Cartesian component of the position vector of the m th atom,

5.4 Modeling the Elastic Properties of Materials

247

with the sum over m referring to the various neighbors that the atom at the origin is coupled to via the potential Veff (Rm ). The notation is admittedly unpleasant, but I am too entrenched in the habit of writing Ci jkl rather than the more consistent Cαβγ δ , where Greek indices are associated with Cartesian components. The result obtained in eqn (5.92) is of interest for a number of reasons including what it has to teach us about the energetics associated with pair potentials. For concreteness, we consider the case of an fcc crystal and specialize to the case of a near-neighbor pair potential for which Veff (Rm ) = 0 as a result of the equilibrium condition. We are interested in obtaining the three cubic elastic moduli, C11 , C12 and C44 . Note that all neighbors of a given atom are characterized by position vectors of the form R = (a0 /2)(110). If we are to√assess the sums called for in eqn (5.92), what emerges is that C11 = 2Veff (a0 / 2)/a0 and C12 = C44 = C11 /2, a result which is generally at odds with experimental ﬁndings. In fairness to our pair potential calculations, our results could have been improved by the inclusion of terms in the energy which are explicitly volume-dependent and structure-independent such as the electron gas terms described in chap. 3 (see eqn (3.64)). In addition, our reason for introducing this calculation was not so much to criticize pair potentials as to illustrate the conceptual ideas associated with a real calculation of the elastic moduli. An alternative to the analytic approach adopted above is to take a computational strategy in which the energies of the various deformed states in the neighborhood of the reference state are computed explicitly using whatever total energy method is under consideration. The set of total energies obtained in this way is then ﬁt as a quadratic function of the relevant strain measure, with the elastic modulus of interest (or some linear combination of the moduli) being related to the curvature of this function about the minimum. For example, as shown in ﬁg. 5.14, one can carry out a series of calculations of the energy of a crystal as a function of the volume. As long as the departures from the equilibrium volume are sufﬁciently small, the energy can be written in the form 1 E tot = α(V − V0 )2 , 2

(5.93)

where α is a stiffness parameter related to the bulk modulus and V0 is the equilibrium volume. Similar results are obtained for other types of deformation (for example, shearing deformations) resulting in the possibilty of obtaining a complete set of linear elastic moduli directly on the basis of microscopic calculations. Note also that in describing this strategy we have not made any particular choice about the nature of the underlying microscopic energy functional. Indeed, this strategy is robust and can be carried out with methods ranging all the way from pair potentials to ﬁrst-principles techniques.

248

5 Thermal and Elastic Properties of Crystals

Fig. 5.14. Energy as a function of volumetric strain as computed using atomic-scale analysis in terms of embedded-atom potentials (courtesy of D. Pawaskar). The atomistic result is compared with the quadratic ﬁt like that suggested in eqn (5.93).

5.4.2 Nonlinear Elastic Material Response: Cauchy–Born Elasticity As yet, our reﬂections on the elastic properties of solids have ventured only so far as the small-strain regime. On the other hand, one of the powerful inheritances of our use of microscopic methods for computing the total energy is the ease with which we may compute the energetics of states of arbitrarily large homogeneous deformations. Indeed, this was already hinted at in ﬁg. 4.1. As one of our central missions is to uncover the relation between microscopic and continuum perspectives, it is of interest to further examine the correspondence between kinematic notions such as the deformation gradient and conventional ideas from crystallography. One useful point of contact between these two sets of ideas is provided by the Cauchy–Born rule. The idea here is that the rearrangement of a crystalline material by virtue of some deformation mapping may be interpreted via its effect on the Bravais lattice vectors themselves. In particular, the Cauchy–Born rule asserts that if the Bravais lattice vectors before deformation are denoted by Ei , then the deformed Bravais lattice vectors are determined by ei = FEi . As will become evident below, this rule can be used as the basis for determining the stored energy function W (F) associated with nonlinear deformations F. The Cauchy–Born strategy yields interesting insights in a number of contexts one of which is in the kinematic description of structural transformations. A

5.4 Modeling the Elastic Properties of Materials

249

Fig. 5.15. Schematic of the assumption inherent in the Cauchy–Born rule which assumes that the crystal lattice may be thought of as locally having suffered an afﬁne deformation (courtesy of K. Bhattacharya).

schematic of the fundamental geometric idea associated with the Cauchy–Born rule is shown in ﬁg. 5.15 in which it is seen that even though the overall state of deformation may be spatially varying, it is possible to advance the assumption of a deformation that is locally afﬁne. As seen in the ﬁgure, despite the fact that the overall body has been subjected to an inhomogeneous deformation, locally, the crystal behaves as though it is of inﬁnite extent and has been subjected to homogeneous deformation. From the standpoint of the microscopic total energy methods presented in the previous chapter, the Cauchy–Born rule may be used to compute the stored energy function W (F). Indeed, we have already shown two different examples of this thinking in ﬁgs. 2.14 and 4.1. The key message of both of these ﬁgures is not only the nonlinearity of the energy landscape once the displacements become too large, but even further, its nonconvexity. The idea invoked in carrying out such calculations is that we can evaluate the energy of a given conﬁguration, characterized by Bravais lattice vectors ei = FEi as W ({ei }), via W ({ei }) =

E tot ({ei }) − E tot ({Ei }) .

(5.94)

In a word, the problem is reduced to one of computing the energy of two different homogeneous conﬁgurations, and as usual, the concept is indifferent to choice of underlying microscopic energy functional. A particularly important example of this strategy concerns the energetics of shearing deformations. In particular, as shown in ﬁg. 2.14, the energetics of shearing deformations immediately reveals the presence of lattice invariant shears. Further, the presence of zero-energy wells corresponding to speciﬁc values of the shear is precisely the physics that gives rise to the existence of dislocations. We will later see (see section 10.3) that similar ideas are relevant to the emergence of microstructures in systems having multiple degenerate energy wells. It is also important to note that a strain energy density

250

5 Thermal and Elastic Properties of Crystals

function like that given in eqn (5.94) can be used as the basis of a hyperelastic constitutive model which permits the calculation of stresses via P=

∂ W (F) . ∂F

(5.95)

Further details of this idea can be found in Tadmor et al. (1996).

5.5 Further Reading Introduction to Lattice Dynamics by M. Dove, Cambridge University Press, Cambridge: England, 1993. I really like Dove’s book. Unlike the present work, it has the virtue of being short and to the point. The discussion of anharmonic effects is instructive. ‘Group Theory and Normal Modes’ by A. Nussbaum, Am. J. Phys., 36, 529 (1968) provides an interesting tutorial introduction to the use of symmetry to reduce the computational overhead associated with a given calculation of the normal modes. Theory of Lattice Dynamics in the Harmonic Approximation by A. A. Maradudin, E. W. Montroll, G. H. Weiss and I. P. Ipatova, Academic Press, New York: New York, 1971. A formidable volume with not only a full accounting for the fundamentals of vibrations in solids, but also including issues such as the effects of defects on vibrations in solids. Imaging Phonons: Acoustic Wave Propagation in Solids by James P. Wolfe, Cambridge University Press, Cambridge: England, 1998. Wolfe’s book has a number of different insights into the concepts discussed in the present chapter as well as a wealth of material which goes well beyond the present discussion. Thermodynamics of Crystals by D. C. Wallace, Dover Publications, Inc., Mineola: New York, 1998. Wallace’s chaps. 2–4 give a thorough discussion of the material that has been sketched in the present chapter. Thermal Conduction in Solids by R. Berman, Clarendon Press, Oxford: England, 1976. A useful compendium of insights into the problem of thermal conduction. ‘Thermal Conductivity and Lattice Vibrational Modes’ by P. G. Klemens, in Solid State Physics edited by F. Seitz and D. Turnbull, Academic Press, San Diego: California, Vol. 7, pg. 1, 1958. I ﬁnd the sections on scattering due to defects in this article to be quite useful. ‘Theory of Thermal Conductivity of Solids at Low Temperatures’ by P.Carruthers, Rev. Mod. Phys., 33, 92 (1961). This article is probably severely dated, but I still ﬁnd it to be instructive reading.

5.6 Problems

251

5.6 Problems

1 Normal Modes for Chain with Three Masses Consider a three-mass generalization of the system shown in ﬁg. 5.3. Compute the vibrational frequencies and associated eigenvectors on the assumption that each mass has only one degree of freedom, namely, motions along the line joining the masses. Assume that the masses are all identical as are the spring constants.

2 Properties of the Force Constants and the Dynamical Matrix In this problem, we revisit the formalism associated with the force constants and the dynamical matrix. Recall that the force on the i th atom in the α th direction is given by αβ K i j u jβ , (5.96) Fiα = − jβ

where u jβ denotes the displacement of the j th atom in the β th Cartesian direction. Using this expression for the force, show that if all atoms are displaced by the same constant vector, that this implies the sum rule αβ K i j = 0. (5.97) j

3 Phonons in Morse Potential Cu Obtain an analytic expression for the zone edge phonons in fcc Cu using the Morse potential derived in the previous chapter. To do so, begin by deriving eqn (5.37) and then carry out the appropriate lattice sums explicitly for the Morse potential to obtain the force constant matrix. In addition, obtain a numerical solution for the phonon dispersion relation along the (100) direction. 4 Phonons using the Pair Functional Formalism Generalize the discussion given in this chapter based on pair potentials in order to deduce the force constant matrix for a total energy based on pair functionals. The result of this analysis can be found in Finnis and Sinclair (1984). Having obtained this expression for the force constant matrix, use the Johnson potential presented in the previous chapter and compute the phonon

252

5 Thermal and Elastic Properties of Crystals

dispersion relations in Cu. In addition, compute the phonon density of states for Cu and compare the resulting structure of this function to the parabolic shape expected on the basis of the Debye model. 5 Elaboration of the Debye Model In this problem, deduce the eigenvalues of the Christoffel tensor and also recreate the vibrational density of states for the Debye model given in eqn (5.61). In light of these results, ﬁll in the various steps culminating in eqn (5.66). 6 Elastic Moduli for fcc Cu from Morse Potential Using the Morse pair potential for Cu derived in the problems of the previous chapter, derive C11 , C12 and C44 . Carry out this analysis both analytically and numerically. For the numerical results, you will need to compute the energetics of three independent deformations and then to ﬁt the resulting energy curves to obtain these moduli. 7 Expression for Elastic Moduli of Cubic Crystals from Pair Functionals Using the generic deﬁnition of the total energy as deﬁned within the pair functional formalism, derive an expression for the elastic moduli. Once this result is in hand, use the explicit expressions associated with the Johnson potential to obtain the elastic moduli for Cu. 8 Cauchy–Born Elasticity Using the Cauchy–Born rule in conjunction with the Johnson embedded-atom potential, compute the energy of a shearing deformation on (111) planes in the [110] direction. Show that the energy has the form given in ﬁg. 2.14.

SIX

Structural Energies and Phase Diagrams

6.1 Structures in Solids A central tenet of materials science is the intimate relation between structure and properties, an idea that has been elevated to what one might call the structure–properties paradigm. However, we must proceed with caution, even on this seemingly innocent point, since materials exhibit geometrical structures on many different scales. As a result, when making reference to the connection between structure and properties, we must ask ourselves: structure at what scale? This chapter is the ﬁrst in a long series that will culminate in a discussion of microstructure, in which we will confront the various geometric structures found in solids. The bottom rung in the ladder of structures that make up this hierarchy is that of the atomic-scale geometry of the perfect crystal. It is geometry at this scale that concerns us in the present chapter. In crystalline solids, the atomic-scale geometry is tied to the regular arrangements of atoms and is described in terms of the Bravais lattice. At this scale, the modeling of structure refers to our ability to appropriately decipher the phase diagram of a particular material. What is the equilibrium crystal structure? What happens to the stable phase as a function of an applied stress, changes in temperature or changes in composition? And a more subtle question, what are the favored metastable arrangements that can be reached by the system? At the next level of description, there are a host of issues related still to the atomic-level geometry, but now as concerns the various defects that disturb the perfect crystal. For example, as we raise the temperature, what will be the distribution of vacancies within a crystal, and what governs the dislocation structures that are revealed in electron microscopy images? These defects will occupy much of our attention in coming chapters. At larger scales yet, an investigation of the relation between structure and properties must by necessity also acknowledge structure at the scale of the microstructure itself. Here, it is evident that we are faced again with questions 253

254

6 Structural Energies and Phase Diagrams

related to metastability and that our theory must answer to these demands. Our ﬁrst step towards answering these questions will show how microscopic analysis can yield meaningful insights into the nature of atomic-level geometry.

6.2 Atomic-Level Geometry in Materials As noted above and hinted at in the sections on microscopic approaches to the total energy, the ability to correctly capture the energetics of competing crystal structures and their various defects is a central mission faced in the modeling of materials. Before embarking on an analysis of the structure and energetics of the many defects that populate solids and lend them their fascinating properties, we must ﬁrst ensure our ability to differentiate the various competing crystal structures found in the elements and their compounds that serve as the backbone of materials science. Casual inspection of the periodic table reveals that already at the level of elemental materials, a whole range of atomic-level structures may occur. The room temperature structures of elemental materials are summarized in ﬁg. 6.1. A fascinating resource concerning the structure of the elements is Young’s Phase Diagrams of the Elements (1991), a book that rewards its reader with insights into the startling complexity found in crystalline solids, even without the complicating inﬂuence of the compositional degrees of freedom that are present in compounds. Fig. 6.1 reveals a number of important and intriguing structural trends, all of which serve as a challenge to our analysis. For example, it is seen that a wide assortment of elements adopt the close-packed fcc and hcp structures. In particular, the rare-gas solids (aside from He) all adopt the fcc structure. We also note that the transition metals (i.e. the rows running from Sc to Cu, Y to Ag and La to Au) adopt a nearly regular progression starting with the hcp structure, passing to the bcc structure at the middle of the transition series and ending with the fcc structure at the noble metals (Cu, Ag, Au). These structural trends can be traced in turn to the ﬁlling of the transition metal d-band as the number of d-electrons per atom increases as the transition series is traversed from left to right. The bcc structure also plays a crucial role in the description of elemental materials, with the most regular trend being the occurrence of this structure in the alkali metals such as Li, Na and their partners in the same column of the periodic table. Covalent materials, such as Si and Ge, are also cubic but take on the much more open diamond structure. A more exotic cubic structure is adopted by elemental Mn which is built up of 58 atoms. In this case, it is the complicating effects of magnetism that can be blamed for the structural complexity. In addition to the high-symmetry cubic phases, there are a collection of bad actors which adopt structures of much lower symmetry. For example, the group

6.2 Atomic-Level Geometry in Materials

255

Fig. 6.1. Periodic table with identiﬁcation of the crystal structures adopted by the various elements (adapted from McMahon and Graham (1992)).

V elements (N, P, As, Sb and Bi) adopt several orthorhombic and rhombohedral phases. Additional structural complexity is ushered in as a result of the fact that in certain cases, the basic building blocks are no longer individual atoms, but rather molecules. The most stunning example of this effect is revealed in S which has a room temperature orthorhombic crystal structure built up of 16 S8 molecules in each unit cell. To drive home the complexity revealed at the structural level even in the case of elemental materials, ﬁg. 6.2 shows the temperature–pressure phase diagrams of a few representative elements. There are a few trends to be remarked. First, we note that for several of the close-packed metals that at high temperatures they undergo a transformation to the bcc structure, as seen in the ﬁgure for the representative example of Ti, and as is true in addition for Zr and Hf. A more complex situation featuring a series of cubic structures is that of Mn which undergoes a number of different structural transformations with increasing temperature. Oxygen is also characterized by a phase diagram of remarkable complexity, in this case with the fundamental structural building blocks being O2 molecules. In addition to the role of the temperature as a control parameter which serves to tune the relative stability of competing phases, the application of a hydrostatic stress can also induce structural change. This claim is substantiated in the particular case of Si shown in ﬁg. 6.2 which undergoes a transition from the diamond cubic to the centered

256

6 Structural Energies and Phase Diagrams

Fig. 6.2. Pressure–temperature phase diagrams of a few representative elements (adapted from Young (1991)).

tetragonal β-Sn phase at a pressure of roughly 11.3 GPa, and more generically in ﬁg. 6.3. Indeed, an important open question is how such phase diagrams will generalize when the material is subjected to more general states of stress. In the case of a material like sulfur (see ﬁg. 1.4), we have already seen that the equilibrium structure is a delicate function of the particular region of parameter space under consideration. From the standpoint of equilibrium thermodynamics, despite the unarguable complexity of the phase diagrams described above, we must conclude that these various structures are nothing more than different realizations of the minima in the appropriate free energy. Our present challenge is to see if

6.2 Atomic-Level Geometry in Materials

257

Fig. 6.3. Dependence of the equilibrium structure on the pressure for several representative transition metals (adapted from Young (1991)).

we can learn what competing features give rise to the stability of the different competitors. Beyond the simple elemental structures considered above, we are faced with the more serious task of deducing the structures that arise once we allow for more than a single element and the attendant chemical complexity. Here again, the challenges to the materials modeler are seemingly limitless. To reveal this complexity, we consider a few representative binary systems as shown in ﬁg. 6.4. For intermetallics, the Cu–Au system may be the most celebrated of all examples. In this case, one of the key qualitative features to note is the existence of both low-temperature ordered phases and a high-temperature disordered phase. The low-temperature ordered phases are particularly appealing from a modeling perspective since they can all be thought of as superstructures on the fcc lattice which are built up as different decorations of the fcc lattice on the basis of the various Cu and Au atoms. A second example of an intermetallic phase diagram is that of the TiAl intermetallic system shown in ﬁg. 6.4(b), a material that has been the subject of intense interest in recent years. In addition to the α (hcp) and β (bcc) solid solutions, we note the presence of the ordered Ti3 Al hexagonal phase, the TiAl L10 phase and the ordered fcc TiAl2 phase. Phase diagrams associated with systems other than intermetallics are also of interest. Our third example, shown in ﬁg. 6.4(c), the Si–Ge system, is interesting primarily for what it is not. In particular, we note the marked lack of complexity

258

6 Structural Energies and Phase Diagrams

(Au,Cu)

1800 1700 1600 1500 1400 ( -Ti) 1300 1200 1100 1000 Ti3Al 900 800 ( -Ti) 700 600 500

(a)

20

30

40

50

60 70 80 90100

0

10

2100

(Al) TiAl2

-TiAl3

20

2046.5+ 7.5˚C

30

40 ~60

L1 + L2

2054˚C M.P.

Temperature ˚C

Temperature ˚C

2300

1414˚C

1400

TiAl3

Weight Percent Oxygen

Weight Percent Silicon 10

TiAl

0 10 20 30 40 50 60 70 80 90 100 Al Ti Atomic Percent Aluminum (b)

Atomic Percent Copper 0

L

LPS

Temperature ˚C

Temperature ˚C

Weight Percent Copper

1300

1200

1100

1000

+0.5 59.5_

1900 1700 1500

Al2O3

1300

L1+ Al2O3

1100 900 660.452 C 0, the jump in the displacement ﬁeld be equal to the Burgers vector (i.e. u 3 (x1 , 0+ ) − u 3 (x1 , 0− ) = b). Our notation u 3 (x1 , 0+ ) means that the ﬁeld u 3 is to be evaluated just above the slip plane (i.e. x2 = ). This geometry of this problem inspires a description in terms of cylindrical coordinates, within which a plausible form for the displacements is the assumption that, like a helical ramp in a parking garage, the displacements increase linearly in the winding angle, θ, yielding the solution bθ . (8.10) 2π This displacement ﬁeld may also be represented simply in terms of Cartesian coordinates, resulting in the expression b −1 x 2 , (8.11) tan u 3 (x1 , x2 ) = 2π x1 u 3 (r, θ, z) =

and the associated strains b x2 , 2 4π x1 + x22 x1 b 32 (x1 , x2 ) = . 4π x12 + x22

31 (x1 , x2 ) = −

The stress tensor corresponding to these strains may be written as 0 0 −x2 µb 0 σ = 0 x1 . 2π(x12 + x22 ) −x2 x1 0

(8.12) (8.13)

(8.14)

384

8 Line Defects in Solids

Note that care must be taken with the choice of sign of the Burgers vector to actually use these equations in practice. The signiﬁcance of the results given above may be seen in a number of different contexts. Indeed, the solution for the perfect screw dislocation in an isotropic linear elastic medium provides a window on much of what we will wish to know even in the more generic setting of an arbitrary curved dislocation. Further, this simple result also serves as the basis for our realization that all is not well with the continuum solution. One insight that emerges immediately from our consideration of the screw dislocation is the nature of the energies associated with dislocations. Cursory inspection of the dislocation solution determined above reveals that the strain ﬁelds are singular as the dislocation core region is approached; a feature that highlights the ultimate need for calculations that respect the discrete lattice scale, either through explicit resolution of the atomic degrees of freedom or through use of suitable constitutive and kinematic nonlinearity within a continuum framework. If we are willing to suspend momentarily the question of the behavior in the nearcore region, it is of great interest to determine that part of the total energy of a dislocation that arises by virtue of the elastic energy stored in its deformation ﬁelds. The simplest statement of the energy associated with a dislocation by virtue of its deformation ﬁelds is to integrate the strain energy density over the volume. Recall that for a linear elastic solid, the strain energy density may be written as 1 W () = Ci jkl i j kl . 2

(8.15)

Alternatively, if we assume that there are no body forces, then the divergence theorem in conjunction with the equilibrium equations asserts 1 1 tk u k d A. (8.16) Ci jkl i j kl = 2 ∂ 2 Hence, we ﬁnd that the total elastic energy can be found by performing surface integrations associated with the tractions. It is this device that we will follow here. Though in principle we must evaluate the surface integral not only on the slipped surface, but also on both an outer and an inner circular surface, the only surface that must be considered in ∂ is that of the cut along the slip plane as shown in ﬁg. 8.17. In fact, it can be shown that the contribution on both the outer and inner surfaces vanish. In terms of the coordinate system speciﬁed above, we are left with the necessity of evaluating the traction vector ti = σi2 n 2 , which yields t3 = σ32 . From our assessment of the displacement ﬁelds, we note that the relevant component of the stress tensor is given as σ32 = µu 3,2 =

µb x1 . 2π x12 + x22

(8.17)

8.4 Elastic Models of Single Dislocations

385

Fig. 8.17. Schematic of slip plane as used within a continuum setting.

In light of this result, we are prepared to evaluate the strain energy which is obtained by integrating R µb2 1 L , (8.18) dz dx E =2 2 0 4π x r0 where we have exploited the fact that along the slip plane, x2 = 0. The factor of 2 in front of the integral reﬂects the presence of both symmetry equivalent terms, σ32 and σ23 . The limits of integration for the integral along the line direction make it clear that we are reckoning the energy per unit length of dislocation, while the x-integral reﬂects the existence of a large distance cutoff corresponding to the dimensions of the body and a lower scale cutoff, corresponding loosely with the scale at which elasticity theory breaks down. The result of this analysis is that the energy per unit length along the dislocation line is R µb2 ln E= . (8.19) 4π r0 This result is at once enlightening and troubling. On the one hand, on the basis of relatively little effort we have constructed an evaluation of the elastic energy associated with a screw dislocation, and while our analysis depended upon the simplicity of the screw dislocation solution, we will ﬁnd that the qualitative features of our result are unchanged by the introduction of subtleties such as mixed character to the dislocation’s Burgers vector and elastic anisotropy. On the other hand, to avoid a divergence in the energy we have been forced to introduce a phenomenological parameter r0 known as the core radius, which can only be guessed at within the conﬁnes of our continuum model. Further, we note that our result for the energy is logarithmically divergent not only for the short-range part of the ﬁelds, but for the long-range parts as well. Clearly, there is more to be discovered. An interesting estimate of the signiﬁcance of the core parameter can be constructed by harking back to our discussion of the ideal strength concept. There, we noted that when shear stresses reach a value on the order of µ/2π, the forces

386

8 Line Defects in Solids

Fig. 8.18. Model of stresses in core region of dislocation based upon the ideal shear strength. The elastically diverging stresses are cutoff for r < rc on the assumption that the stresses within the core region have a constant value τideal .

are sufﬁciently high to begin the shearing of adjacent crystal planes. Hence, we take the view here that the core radius may be deﬁned as that region over which the stresses have reached values consonant with the ideal strength. One estimate of the core radius is to take that distance along the x-axis at which the shear stress reaches the ideal strength, which yields r0 = b. As noted above, it is standard to idealize the core as a cylindrical region, although the locus of points of constant shear stress is certainly not circular as such a model would suppose. This simple model of the core radius can be exploited to make an estimate for the energy associated with the core itself. The basic idea is to make the pessimistic assumption that within the region of radius r0 , the stresses are constant at the level of the ideal shear strength. This situation is depicted schematically in ﬁg. 8.18. Our estimate of the core energy amounts to nothing more than computing the strain energy stored in this region on the assumption of a constant state of strain corresponding to that at the ideal strength limit. In particular, we note that the only terms appearing in the assessment of the strain energy density are of the form σ31 31 and σ32 32 . The total strain energy within the core region is given as 1 (8.20) E core = (σ31 31 + σ32 32 )(πr02 )L , 2 where the last two factors are geometric and characterize the cylindrical volume element under consideration. We note that for the special case of the screw dislocation, σ31 31 + σ32 32 = µb2 /8π 2r02 , with the result that E core = µb2 L/8π .

8.4 Elastic Models of Single Dislocations

387

Hence, within this simple model, the energy of the dislocation per unit length may be written as 1 R µb2 E disloc ln + . (8.21) = L 4π r0 2 For concreteness, it is of interest to examine the typical energy scale associated with a straight dislocation line. Consider a hypothetical material for which the ˚ and take as our outer cutoff and shear modulus is 50 GPa, the Burgers vector is 3 A ˚ inner cutoff radii, 1 µm and 3 A respectively. In this case, we see that the energy associated with each segment with a length comparable to the lattice spacing is of order 6 eV. Though our analysis can be reﬁned in a number of ways, there is no escaping the fact that the energy scale here is huge on the scale of that associated with room temperature. As a result, we are momentarily left to wonder whether dislocations can arise purely by virtue of thermal ﬂuctuations. We have still not exhausted the insights that can be gleaned from this simplest of dislocation models. Before taking up the question of the displacement ﬁelds associated with a generic dislocation loop, we ﬁrst examine the question of whether or not it is plausible that entropic effects can compensate for the huge energy associated with the dislocation, thereby raising the possibility of the existence of an equilibrium distribution of such defects. There are a few different entropic mechanisms that can be imagined as a consequence of the presence of dislocations. On the one hand, it is clear that the presence of such dislocations will alter the vibrational spectrum of the material with an attendant change in its vibrational entropy. Another contribution to the entropy is that due to the wandering of the dislocation line itself and corresponds to a conﬁgurational term. A crude estimate of this latter effect is to assume that on passing from one atomic layer to the next, the dislocation can change directions towards any of the neighboring atoms. Hence, the entropy per layer spacing is of the order S = k ln z,

(8.22)

where z represents the number of neighbors along the line direction and we will make the simplifying assumption that ln z ≈ 1. Hence, the contribution of conﬁgurational terms to the free energy of a dislocation is of order T S = kT , which is negligible in comparison with the enormous internal energy cost of the dislocation line itself. Our initial foray into the elastic theory of dislocations has revealed much about both the structure and energetics of dislocations. From the continuum standpoint, the determination of the displacement ﬁelds (in this case u 3 ) is equivalent to solving for the ‘structure’ of the dislocation. We have determined a generic feature of such ﬁelds, namely, the presence of long-range strains that decay as r −1 . Another

388

8 Line Defects in Solids

generic feature of the elastic solution is the fact that in the immediate vicinity of the dislocation core, the elastic theory breaks down. It has also become evident from our analysis that unlike point defects, dislocations have energies well above those for which an equilibrium distribution can be expected.

8.4.2 The Volterra Formula As yet, our treatment of the elastic theory of single dislocations has depended upon the simplicity of the equilibrium equations that emerge for the particular geometry of a straight screw dislocation. While further progress can be made for specialized geometries, it is perhaps more instructive to seek generic insights into the deformation ﬁelds that attend the presence of dislocations of arbitrary geometry. In particular, we will concern ourselves with a closed dislocation loop. One approach for the elastic analysis of dislocations that is especially appealing is built around the use of the elastic Green function. As is customary, we will initially restrict our analysis to isotropic materials, though extension to an anisotropic setting, while not trivial, can be managed, at least formally. The aim of our elastic analysis will be a full characterization of the elastic ﬁelds (i.e. stresses, strains and displacements) associated with the dislocation of interest, as well as a description of its energy. Though the elastic ﬁelds are of interest in their own right, we will see in section 8.5 that it is the coupling of these ﬁelds, either to applied stresses or to internal stresses due to other defects, that makes for the beginnings of a picture of the origins of phenomena such as strain and solution hardening. The reciprocal theorem points the way to an idea that will allow for the calculation of the displacements associated with a dislocation loop of arbitrary shape. As discussed in chap. 2, the reciprocal theorem asserts that two sets of σ (2) , u(2) , f (2) ), associated with the same σ (1) , u(1) , f (1) ) and (σ equilibrium ﬁelds (σ body (i.e. they satisfy the equilibrium equations), are related by the expression t(1) · u(2) d A + f(1) · u(2) d V = t(2) · u(1) d A + f(2) · u(1) d V. (8.23) ∂

∂

Within the context of the elastic Green function, the reciprocal theorem serves as a jumping off point for the construction of fundamental solutions to a number of different problems. For example, we will ﬁrst show how the reciprocal theorem may be used to construct the solution for an arbitrary dislocation loop via consideration of a distribution of point forces. Later, the fundamental dislocation solution will be bootstrapped to construct solutions associated with the problem of a cracked solid. We consider the generic problem of a dislocated solid with a loop such as that shown in ﬁg. 8.10. Here we imagine two different conﬁgurations associated with

8.4 Elastic Models of Single Dislocations

389

the same inﬁnite body that is described appropriately as an isotropic linear elastic solid. In the ﬁrst body, we imagine a dislocation loop as shown with ﬁelds labeled by the superscript (d), while in the second, we consider a point force at position r and the associated ﬁelds which are labeled with a superscript ( p). For the dislocation case there are no body forces and hence f (d) = 0. By the reciprocal theorem we note that (d) ( p) ( p) (d) t ·u dA = t ·u dA + f ( p) · u(d) d V. (8.24) ∂

∂

The basic idea is to exploit the fact that the displacements associated with the point force are already known, and correspond to the elastic Green function. Further, the displacements associated with the dislocation are prescribed on the slip plane. We can rewrite the surface integral that spans the slipped region as t(d) · u( p) d A = t(d) (−) · u( p) (−)d A + t(d) (+) · u( p) (+)d A. (8.25) ∂

∂−

∂+

(d)

In this case t (+) refers to the traction associated with the dislocation just above the slip plane while t(d) (−) refers to the value of the traction just below the slip plane. However, since the displacement ﬁelds (u( p) ) associated with the point force are continuous across the slip plane, u( p) (−) = u( p) (+). Similarly, the tractions across the slip plane must be equal and opposite (i.e. t(d) (+) = −t(d) (−)). As a result, we are left with (d) ( p) (d) ( p) t ·u dA = t (+) · u (+)d A − t(d) (+) · u( p) (+)d A = 0. ∂

∂−

∂+

(8.26) Hence, the only terms remaining from our implementation of the reciprocal theorem yield the rather simpler expression ( p) (d) t · u d A = − f ( p) · u(d) d V (8.27) ∂

Following the same decomposition of the surface integrals suggested above, we may rewrite the term involving the tractions as t( p) · u(d) d A = t( p) (+) · [u(d) (+) − u(d) (−)]d A. (8.28) ∂

∂

If we now recall that the jump in the displacement ﬁeld across the slip plane is nothing more than the Burgers vector and we exploit the fact that the traction vector is related to the stress tensor via t( p) = σ ( p) n, then the left hand side of eqn (8.28) may be rewritten as ( p) t( p) · u(d) d A = − σi j n j bi d A. (8.29) ∂

∂

390

8 Line Defects in Solids

Recalling our linear elastic constitutive assumption, we may further simplify this result to read ( p) (d) p) t ·u dA = − Ci jmn u (m,n n j bi d A. (8.30) ∂

∂

Thus far, we have treated only one side of eqn (8.27). Our next task is to probe the signiﬁcance of the term involving the body force. Through the artiﬁce of choosing the ﬁelds associated with a point force as our complementary ﬁelds, the dislocation solutions can be obtained directly. In particular, we note that if ( p) f j (r ) = f j δ(r − r ), then we have

f ( p) · u(d) d V = u (d) k (r) f k ,

(8.31)

which involves the unknown dislocation displacement ﬁeld. We may tidy up this ( p) result by recalling that u m that appears in eqn (8.30) is the solution for the point ( p) force problem and hence is given by u m = −G mk f k . As a result, our efforts culminate in the expression, u k (r) = − Ci jmn G mk,n (r − r )n j bi d A , (8.32) ∂

a result known as Volterra’s formula. Note that this result is a special case of the formula we wrote earlier in the eigenstrain context as eqn (2.96). The physical content of this result is that we have found a way by integrating only on the slipped surface to determine the displacement ﬁelds (in linear elasticity) throughout space. In practice, this method is unwieldy for consideration of the standard textbook examples concerning straight dislocations of either pure edge or screw character. On the other hand, for determining the ﬁelds resulting from dislocation loops of arbitrary shape, this formula and its variants are considerably more enlightening. Despite the heavy-handedness of the Volterra formula in the context of straight dislocations, it is instructive to see it in action. As an example of this line of thought, we now use the Volterra formula to reconstruct the displacement ﬁelds associated with a screw dislocation. As was shown earlier, the displacement ﬁelds that are carried by a screw dislocation in an isotropic linear elastic medium may be easily arrived at through the insight that the equilibrium equations reduce to Laplace’s equation in the single unknown ﬁeld, u 3 . Here we instead consider these ﬁelds as the result of our Green function analysis. We orient our coordinate system such that the Burgers vector is given by b = (0, 0, b) and the normal to the slip plane is n = (0, 1, 0). Further, we recall eqn (2.54) which gives the elastic modulus tensor in terms of the Lam´e constants. Substitution of these quantities into the

8.4 Elastic Models of Single Dislocations

Volterra formula yields u m (r ) = −µb

391

∂

(G 33,2 + G 23,3 )d A.

(8.33)

The derivatives of the Green function that we are instructed to evaluate can be carried out through reference to eqn (2.91) resulting in 0 ∞ −µby (λ + 3µ) dx dz u 3 (r ) = 3 8πµ(λ + 2µ) −∞ −∞ [(x − x )2 + y 2 + z 2 ] 2 3(λ + µ)z 2 . (8.34) + 5 [(x − x )2 + y 2 + z 2 ] 2 Not surprisingly, the resulting integrals are entirely tractable and lead to the result b −1 y , (8.35) tan u 3 (r ) = − 2π x in exact coincidence with the displacements that emerge in the simpler, more standard treatment as already revealed in eqn (8.11). A similar analysis can be performed in the context of the conventional edge dislocation within the isotropic elasticity context (see Problems).

8.4.3 The Edge Dislocation We have now succeeded in identifying the deformations induced by a screw dislocation, and have also found a generic formula for the ﬁelds due to an arbitrary dislocation. Our present task is to return to the edge dislocation for the purposes of completeness and because this solution will make its way into our future analysis. This is particularly evident in the case of isotropic linear elasticity where we will ﬁnd that even for dislocations of mixed character, their geometries may be thought of as a superposition of pure edge and pure screw dislocations. Recall from our discussion in chap. 2 that the solution of elasticity problems of the two-dimensional variety presented by the edge dislocation is often amenable to a treatment in terms of the Airy stress function. Consultation of Hirth and Lothe (1992), for example, reveals a well-deﬁned prescription for determining the Airy stress function. The outcome of this analysis is the recognition that the stresses in the case of an edge dislocation are given by σx x (x, y) = − σ yy (x, y) =

y(3x 2 + y 2 ) µb , 2π(1 − ν) (x 2 + y 2 )2

y(x 2 − y 2 ) µb , 2π(1 − ν) (x 2 + y 2 )2

(8.36) (8.37)

392

8 Line Defects in Solids

σx y (x, y) =

µb x(x 2 − y 2 ) . 2π(1 − ν) (x 2 + y 2 )2

(8.38)

Earlier we made the promise that the energy stored in the elastic ﬁelds had a generic logarithmic character, regardless of the type of the dislocation. To compute the elastic strain energy associated with the edge dislocation we use eqn (8.16). In the context of the stress ﬁelds given above, R E strain µb b µb2 R dx = = ln . (8.39) L 2 2π(1 − ν) r0 x 4π(1 − ν) r0 The integrand is determined by computing the tractions on the slip plane using the stresses for the edge dislocation described above, and as claimed, the structure of the energy is exactly the same as that found earlier for the screw dislocation. 8.4.4 Mixed Dislocations As noted earlier, generic dislocations have neither pure screw nor pure edge character. If we consider a straight dislocation with line direction ξ = (0, 1, 0), then the dislocation has a Burgers vector of the form b = b(sin θ, cos θ, 0), where θ is the angle between the line direction and the Burgers vector. We see that using this notation, a screw dislocation is characterized by θ = 0 and an edge dislocation similarly by θ = 90◦ . For the special case in which we consider an isotropic linear elastic material, the total stress ﬁeld due to a mixed dislocation is a superposition of the ﬁelds due to its edge and screw components treated separately. What this means in particular is that the stress tensor can be written as e e s σ11 σ12 σ13 e e s σ = σ12 (8.40) σ22 σ23 . s s e σ13 σ23 σ33 The superscripts e and s refer to edge and screw and serve as an instruction to use the isotropic linear elastic stress ﬁelds for the edge and screw dislocation, respectively, but with the Burgers vector adjusted to account for relevant trigonometric weighting factors. Elastic isotropy considerably simpliﬁes the analyses that we are forced to undertake in our goal of characterizing the deformation ﬁelds associated with a dislocation. On the other hand, there are some instances in which it is desirable to make the extra effort to include the effects of elastic anisotropy. On the other hand, because the present work has already grown well beyond original intentions and because the addition of anisotropy is for the most part an elaboration of the physical ideas already set forth above, we refer the reader to the outstanding work of Bacon et al. (1979).

8.5 Interaction Energies and Forces

A

(a)

393

B

(b)

(c)

Fig. 8.19. Schematic illustration of breaking of translational invariance by (a) the presence of a free surfaces, (b) an internal interface between two dissimilar materials, and (c) a precipitate particle.

8.5 Interaction Energies and Forces Though the elastic theory of single dislocations is interesting in its own right, our elucidation of the elastic ﬁelds of such dislocations leaves us in a position to begin to explore what can be learned about the plastic deformation of crystalline solids on the basis of dislocations. At the very heart of the questions of both yield and hardening is the issue of how a given dislocation responds to the presence of a stress ﬁeld. Whether that stress ﬁeld has its origins in some remotely applied external load or from the presence of inhomogeneities such as point defects, surfaces and interfaces, voids or other dislocations themselves, ultimately we require a quantitative theory of how the dislocation will respond to such forces. We follow the lead of Eshelby already introduced in chap. 2 in our discussion of conﬁgurational forces. Recall that a small excursion δξi of the defect of interest will result in a change of the total energy of the system and attendant loading devices of the form δ E tot = −Fi δξi , where the conﬁgurational force Fi is the work-conjugate partner of the excursion δξi . As we noted earlier, the origin of such conﬁgurational forces is the breaking of translational symmetry. In the case of a single dislocation in an inﬁnite body that is treated within the conﬁnes of the theory of linear elasticity there is no such symmetry breaking, and this is manifested in the fact that translation of the dislocation core results in no energy change. This situation is to be contrasted with those shown in ﬁg. 8.19 in which we examine a dislocation in the presence of other defects. In these cases, it is clear that a small translation of the dislocation will result in a change in the total energy, signaling the presence of a nonzero conﬁgurational force on the dislocation. For the moment, we will restrict our attention to the general statements that can be made concerning such forces in the context of the linear theory of elasticity. In this case, the results simplify considerably in that we can think of such energetic

394

8 Line Defects in Solids

Fig. 8.20. Organization of surface integrals for computing the interaction energy between the ﬁelds of the defect of interest and all other ﬁelds.

forces as arising from the interaction terms between the separate stress systems. Let us parcel the stresses and strains into two groups, those of the singularity of interest which we will label σiSj and those from the remaining singularities and external ﬁelds, σiTj . Eshelby’s idea is to note that if we write the total elastic energy as 1 (σ S + σiTj )(iSj + iTj )d V, (8.41) E elastic = 2 ij then only the cross terms will be affected by the small excursions we intend to impose on the singularity S. Hence, we may rewrite the part of the total energy that is not translationally invariant as 1 E interaction = (σ S T + σiTj iSj )d V. (8.42) 2 ij ij Consideration of ﬁg. 8.20 suggests a strategy for rewriting the interaction energy. Note that within region I, the ﬁelds T are jump free while for region II, the same may be said of the ﬁelds S. Hence, we rewrite the interaction energy as σiTj u i,S j d V. (8.43) E interaction = σiSj u i,T j d V + I

II

This expression insures that our integrations are organized such that the integrands are well behaved in the regions of interest. If we use the fact that the stress ﬁelds satisfy the equilibrium equations (i.e. σi j, j = 0) in conjunction with the divergence theorem, this expression may be rewritten as E interaction = (σiSj u iT − σiTj u iS )n j d S, (8.44) ∂in

where the surface integral is evaluated on the dividing surface ∂in separating the

8.5 Interaction Energies and Forces

395

defect of interest from the rest of the crystal. This interaction energy is independent of the choice of ∂in so long as it encloses the singularity S. Though eqn (8.44) is abstract, it forms the basis of our calculation of the conﬁgurational forces on dislocations. In particular, on the basis of this expression we are now in a position to derive the Peach–Koehler formula which relates the force on a dislocation to the local stress ﬁeld and the geometric descriptors of the dislocation itself such as the Burgers vector b and the line direction ξ . 8.5.1 The Peach–Koehler Formula The expression derived above lays the foundation for much of our work on the forces on dislocations. In particular, we shall ﬁnd it convenient to direct our attention to the way in which an externally applied stress couples to the motion of a dislocation. This will culminate in the elucidation of the so-called Peach–Koehler force which explicitly reckons the force on a dislocation. Before invoking the Peach–Koehler formula, it is perhaps useful to ﬁrst examine the force between two screw dislocations from the perspective of the interaction energy. Our interest is in determining the force of interaction between these dislocations using the Eshelby philosophy espoused above. In particular, we must evaluate the interaction energy when the dislocations are separated by a distance d and when they are separated by a distance d + ξ , which reﬂects the existence of the small excursion which serves as the basis of our calculation of the conﬁgurational force. In this case, we note that the total energy is given by 1 1 1 1 (1) (1) (2) (2) (1) (2) (1) σi j i j d V + σi j i j d V + σi j i j d V + σi(2) E elastic = j i j d V. 2 2 2 2 (8.45) The last two terms, which are equal, represent the interaction energies, and are the only terms that will be affected by the excursion of the dislocation. Hence, we may write E int =

(2) σi(1) j i j d V,

(8.46)

which in terms of the particular dislocation ﬁelds for this case is y2 x(x − d) µb1 b2 d V. + E int = 4π 2 (x 2 + y 2 )[(x − d)2 + y 2 ] (x 2 + y 2 )[(x − d)2 + y 2 ] (8.47) The result of this integration may be derived after some calculations demanding algebraic care, with the result that R µb1 b2 E int (d) = , (8.48) ln 2π d

396

8 Line Defects in Solids

Fig. 8.21. Small excursion of dislocation segment.

where R is a large distance cutoff. In order to compute the conﬁgurational force, we require the difference between E int (d + ξ ) and E int (d) which to lowest order in ξ is given by E int = −

µb1 b2 ξ , 2πd

(8.49)

which implies that the interaction force is given by F=

µb1 b2 . 2πd

(8.50)

We see that in the case in which the Burgers vectors are equal, the force of interaction is repulsive, whereas in the case in which they are equal and opposite, the resulting force is attractive. In reality, all of this was vastly more work than was really needed to derive this elementary result. Our reason for pursuing this heavy-handed approach was not so much in the name of the particular result as to illustrate how the broken translational invariance induced by the presence of two dislocations manifests itself in the emergence of an interaction energy. The whole enterprise of computing the conﬁgurational forces can be worked out in explicit and gory detail in this case, although a more intelligent approach to the integrations would have been to compute the work done in bringing the second dislocation up to the ﬁrst one. The result derived above is but a special case of a more general formula which can be derived from eqn (8.44). In order to compute the more general result, we imagine a small excursion of the segment of dislocation as shown in ﬁg. 8.21. In

8.5 Interaction Energies and Forces

light of eqn (8.44), we must evaluate S T σi j (+)u i (+)n j (+)d S − E int (S, T ) = +

+ ∂in

− ∂in

σiSj (−)u iT (−)n j (−)d S

−

+ ∂in

− ∂in

397

σiTj (+)u iS (+)n j (+)d S

σiTj (−)u iS (−)n j (−)d S, (8.51)

where the label S refers to the ﬁelds associated with the dislocation that is bowing out and the label T refers to all other contributions to the stress. The labels + and − refer to the integration surfaces which are just above and just below the slip plane. We now use the fact that for the case in question, the stresses σiSj associated with the dislocation are continuous (i.e. σiSj (+) = σiSj (−)) and that the displacements associated with system T are continuous (i.e. u iT (+) = u iT (−)). Finally, upon noting that n i (+) = −n i (−), we may rewrite the expression above as bi σiTj n j (−)d S. (8.52) E int (S, T ) = ∂in

Recall that the deﬁnition of the Burgers vector is bi = u i (+) − u i (−), which has been used in writing the above expression in this ﬁnal form. For the special case of the inﬁnitesimal bow-out of a dislocation segment under the action of the stress σiTj , we note that δ E int = bi σiTj (dy × dl) j .

(8.53)

This equation is written on the basis of the observation that the inﬁnitesimal element of area swept out by the dislocation is characterized by the vector product dy × dl. Note that dy is the local excursion of the segment, while dl is a vector along the line at the point of interest. If we now recall that the conﬁgurational force is given as δ E int = −Fm δξm , then we may evidently write the conﬁgurational force in the present context as Fm = m jn bi σi j ζn , (8.54) dl where we have used dl = dlζζ . We apologize for temporarily denoting the local tangent vector as ζ , but note that had we not done so, the symbol ξ would be doing double time, serving to denote both the excursion of the dislocation as well as its local tangent vector. In vector form, we may write this as F σ b) × ζ . = (σ (8.55) dl The physical interpretation of this result is that it is the force per unit length of dislocation acting on a segment by virtue of the presence of the stress ﬁeld σ . This expression is the famed Peach–Koehler formula and will be seen to yield a host of interesting insights into the interactions between dislocations.

398

8 Line Defects in Solids

8.5.2 Interactions and Images: Peach–Koehler Applied In the discussion given above, we have resurrected the notion of an energetic force as ﬁrst described in chap. 2. The key point is the existence of a conﬁgurational force associated with energy changes that attend small excursions of the defect of interest. In the dislocation setting, we have shown that such arguments lead naturally to the Peach–Koehler formula. Presently, we use this formula to investigate the interactions between dislocations in different contexts. Part of our interest in this topic arises from our ultimate interest in explicating hardening in crystals as a consequence of dislocation interactions. Though the elastic theory will be found wanting once the dislocations in question are in too close a proximity, for larger distances of separation, the elastic theory offers an enlightening description of the types of dislocation interactions that are important. Interactions of Two Straight Edge Dislocations We begin with an analysis of the simple case of two parallel edge dislocations. Our aim in the present context is to compute the component of the force which will lead to gliding motion if it is sufﬁciently large as to overcome the intrinsic lattice resistance. The line directions of both dislocations are given by ξ 1 = ξ 2 = (0, 0, 1), and their Burgers vectors are b1 = b2 = (b, 0, 0). The Peach–Koehler formula instructs us to compute F = σ b × ξ . Further, we consider a geometry in which dislocation 1 is at the origin while dislocation 2 is to be found at (x, d). The state of stress at dislocation 2 due to the presence of dislocation 1 is given by d(3x 2 + d 2 ) x(x 2 − d 2 ) 0 − (x 2 + d 2 )2 (x 2 + d 2 )2 2 2 2 2 µb d(x − d ) x(x − d ) . σ = (8.56) 0 2π(1 − ν) (x 2 + d 2 )2 (x 2 + d 2 )2 dν 0 0 − 2 x + d2 By exercising the instructions dictated by the Peach–Koehler formula using the state of stress given above, the force on dislocation 2 is given by F1on2 =

µb2 {i[x(x 2 − d 2 )] + j[d(3x 2 + d 2 )]}. 2 2 2 2π(1 − ν)(x + d )

(8.57)

If we work in units in which x is measured as a fraction f of d (i.e. x = f d) then the glide force (i.e. the force in the x-direction) may be rewritten in dimensionless form as f ( f 2 − 1) 2π d(1 − ν)F = . (8.58) µb2 ( f 2 + 1)2

8.5 Interaction Energies and Forces

399

Fig. 8.22. Force of interaction between two dislocations on adjacent slip planes.

The normalized glide force is plotted in ﬁg. 8.22 where it is seen that there are two equilibrium points for the dislocations one of which is stable and the other of which is unstable. In fact, we have plotted the interaction force for the alternative case in which the dislocations have opposite Burgers vectors as well so as to contrast the resulting solutions. In preparation for our discussion of dislocation junctions, we now consider the case of two dislocations that are not parallel. This analysis is important as a ﬁrst step in evaluating the origins of ‘forest hardening’ in which it is presumed that dislocations gliding on one plane are blocked as a result of dislocations that are piercing their slip plane. The suggestive imagery of a forest of trees serves as a mnemonic for this blocking action and is taken up presently. For simplicity, consider the case depicted in ﬁg. 8.23 in which two screw dislocations characterized by ξ 1 = (0, 0, 1), ξ 2 = (0, 1, 0), b1 = (0, 0, b) and b2 = (0, b, 0), interact according to σ (1) b(2)

0 0 0 −y µb 0 0 s b . = 2π(s 2 + y 2 ) 0 −y s 0

(8.59)

Note that we denote the distance of closest approach of the dislocations (i.e. along the x1 -axis) as s. Carrying out the relevant algebra in conjunction with the Peach– Koehler formula leads to the result that F=−

µb2 s i. 2π(s 2 + y 2 )

(8.60)

This result yields the insight that everywhere along the dislocation line the force of interaction is attractive. However, we note that as a function of the perpendicular

400

8 Line Defects in Solids

Fig. 8.23. Interaction force between two perpendicular screw dislocations (adapted from Hartley and Hirth (1965)).

distance from the line of closest interaction, the interaction becomes weaker. The force proﬁle is indicated schematically in ﬁg. 8.23. Image Forces One of the key manifestations of the broken translational invariance resulting from the presence of a free surface is that of an image force. The presence of a free surface (or an internal interface) implies a breaking of the translational symmetry so that a small excursion of a dislocation will have an attendant energy cost and thereby an attendant conﬁgurational force. In the present section, we undertake an analysis of the image forces that emerge in the simplest of cases, namely that of a screw dislocation near a free surface. The geometry of interest is depicted in ﬁg. 8.24 which shows a screw dislocation a distance d below a free surface. From the standpoint of the elastic boundary value problem involving the dislocation and the free surface, the crucial additional requirement beyond the normal jump condition on the dislocations slip plane is the requirement that the free surface be traction free. What this means in particular is that tn = σ n = 0. If we begin our analysis by considering the ﬁelds due to the dislocation beneath the surface, pretending for the moment that the appropriate ﬁelds are those for a dislocation in an inﬁnite body, we have σ31 (x, y) = −

y+d µb , 2π x 2 + (y + d)2

(8.61)

8.5 Interaction Energies and Forces

401

S

d

d

S

Fig. 8.24. Subsurface screw dislocation and its image partner.

σ32 (x, y) =

x µb . 2 2π x + (y + d)2

(8.62)

These ﬁelds imply a surface traction of the form tn = (0, 0, σ32 ). This observation inspires the conclusion that if we could arrange for a compensating stress −σ32 at the free surface, then the boundary conditions would be satisﬁed. In particular, for this simple geometry it is well known that a parallel dislocation of Burgers vector −b at a distance d above the surface (as depicted in ﬁg. 8.24) accomplishes this end. The full ﬁelds for this problem are y+d y−d µb µb + , 2 2 2 2π x + (y + d) 2π x + (y − d)2 x x µb µb − . σ32 (x, y) = 2 2 2 2π x + (y + d) 2π x + (y − d)2

σ31 (x, y) = −

(8.63) (8.64)

A few remarks on the signiﬁcance of our assumptions are in order. First, we note that the linearity of our elasticity problem is central to the ability to write this solution. Because the sum of two solutions is itself a solution, we know that the elastic ﬁelds themselves are a solution to the problem. Furthermore, by construction, the ﬁelds satisfy the free surface boundary conditions, and hence these ﬁelds are the solution. In light of this result, we are now ready to pose the question concerning the conﬁgurational force induced by the presence of the free surface. We ask the question just how does the energy change if the subsurface dislocation makes a small excursion towards the free surface. However, we have already successfully carried out this calculation in an earlier section and the resulting force was given in eqn (8.50), although in the present case the signs of

402

8 Line Defects in Solids

the dislocations in question are opposite and hence there is an attractive force Fimage = −

µb2 . 4πd

(8.65)

Note that in contrast to the result in eqn (8.50), there is a factor of 4 rather than 2 in the denominator. This arises because the separation of the image dislocations themselves is 2d, not d. We have now seen that by virtue of the presence of a free surface, an image force is induced on a subsurface dislocation. In addition, the idea of an image force has further reinforced our use of conﬁgurational forces and their origins in the breaking of translational symmetry.

8.5.3 The Line Tension Approximation In many instances, the evaluation of the complete set of interactions between several dislocations can be prohibitive, at least at the level of the kind of analysis that one might wish to make with a stick in the sand. Indeed, though in the vast majority of this chapter we have been engaged in the development of the elastic theory of dislocations, we now undertake a different framework in which the complex interactions between various inﬁnitesimal segments of a given dislocation are entirely neglected. An alternative to the full machinery of elasticity that is especially useful in attempting to make sense of the complex properties of three-dimensional dislocation conﬁgurations is the so-called line tension approximation. The line tension idea borrows an analogy from what is known about the perturbations of strings and surfaces when they are disturbed from some reference conﬁguration. For example, we know that if a string is stretched, the energetics of this situation can be described via energy change = T δl.

(8.66)

Similarly, if the surface area of a particular interface is altered, the energetics may be handled through a similar idea, namely, energy change = γ A,

(8.67)

where γ is a surface energy. The analogy with the interfacial energy is more appropriate since dislocations, like free surfaces, have an anisotropy which leads to the conclusion that the energy cost for a small excursion from some ﬂat reference state depends upon the orientation of that reference state. However, the analogy between dislocations and interfaces is imperfect since models of this type have an inherent locality assumption which is exceedingly fragile. To explore this further, we note that in

8.5 Interaction Energies and Forces

403

the line tension approximation, the total energy of a dislocation line may be written as E disloc =

E[θ(s)]ds,

(8.68)

where we have written the dislocation line parameterically in terms of the parameter s, reminds us to integrate along the length of the dislocation of interest and θ is the angle between the local tangent vector and the Burgers vector. The subtlety of the assertion embodied in this equation is that of locality. The basic premise is that the contribution of a given segment to the total energy of the dislocation line depends only on one thing, namely, its local orientation, and is indifferent to the disposition of the remaining segments on the dislocation line. In the context of surfaces, this locality assumption may well be appropriate. On the other hand, because of the long-range elastic interactions between different segments, the energy of a given segment is patently not independent of the disposition of the remaining segments on the line. Nevertheless, as an approximate procedure for reckoning the total energy of some complex dislocation conﬁguration, we can make this locality assumption and use what we have learned earlier about the energetics of straight dislocations to build up a local line energy E(θ ) which depends only on the misorientation θ between the line direction and the Burgers vector. The most naive of all line tension models is that in which a single constant energy is assigned to all orientations. Based on what has been learned earlier (see eqns (8.19) and (8.39)), the assertion is made that E(θ) = T = 12 µb2 , independent of the angle θ . In this case, the line tension becomes a strictly geometric approximation and results in comparisons between different geometries predicated on the overall dislocation line length. In particular, in this approximation the energy is given by dx(s) dx(s) · ds. (8.69) E disloc = T ds ds Note that we have exploited a parameteric representation of the dislocation line in which the position of the line is given by x(s). A more sophisticated version of the line tension approximation is based upon the idea of using the energy per unit length that is obtained for a mixed dislocation in which the angle between the Burgers vector and the line direction is denoted by θ. In this case, the isotropic linear elastic results of section 8.4.4 can be used to obtain the energy per unit length of a mixed dislocation which is given by R µb2 sin2 θ E(θ ) . (8.70) = + cos2 θ ln L 4π 1 − ν r0 Once we are in possession of this result, we are then prepared to examine the

404

8 Line Defects in Solids

energetics of a given dislocation conﬁguration by exploiting it in conjunction with eqn (8.68). We will resort to the line tension approximation repeatedly since as was noted above, much may be learned about the key features of a given problem on the basis of such arguments, which are largely geometrical. Again, what is especially appealing about the line tension approach is the prospect for making analytic headway on fully three-dimensional problems.

8.6 Modeling the Dislocation Core: Beyond Linearity Our discussion of dislocations has thus far made little reference to the signiﬁcant role that can be played by the dislocation core. Whether one thinks of the important effects that arise from the presence of stacking faults (and their analogs in the alloy setting) or of the full scale core reconstructions that occur in materials such as covalent semiconductors or the bcc transition metals, the dislocation core can manifest itself in macroscopic plastic response. Our aim in this section is to take stock of how structural insights into the dislocation core can be obtained. Perhaps the simplest of those features of dislocations that may be thought of as core effects are those associated with the splitting of dislocations into partial dislocations which have associated Burgers vectors that do not correspond to lattice invariant shears. These ideas were already introduced in section 8.3.2. Though the slip associated with partial dislocations does not restore the lattice completely it is nevertheless energetically tolerable with an energy that scales with the stacking fault energy. A dislocation may undergo a splitting reaction into two dislocations that bound a stacking fault. In simple terms, we would describe the resulting dislocation as having a complex core structure. Our treatment in this section will cover three primary thrusts in modeling dislocation core phenomena. Our ﬁrst calculations will consider the simplest elastic models of dislocation dissociation. This will be followed by our ﬁrst foray into mixed atomistic/continuum models in the form of the Peierls–Nabarro cohesive zone model. This hybrid model divides the dislocation into two parts, one of which is treated using linear elasticity and the other of which is considered in light of a continuum model of the atomic-level forces acting across the slip plane of the dislocation. Our analysis will ﬁnish with an assessment of the gains made in direct atomistic simulation of dislocation cores.

8.6.1 Dislocation Dissociation In this section, our aim is to compute the core geometry associated with a dissociated dislocation in an fcc material. Our model will be founded upon a

8.6 Modeling the Dislocation Core: Beyond Linearity

405

Fig. 8.25. Geometry of dislocation splitting.

linear elastic analysis of the interactions between the partial dislocations, but supplemented with a constant energy cost γs f per unit area of stacking fault. To make the analysis eminently tractable, we restrict our attention to an isotropic material. The total energy of the system composed of two partials and the stacking fault they bound is E tot (d) = E self + E int (d) + γs f d.

(8.71)

What we have noted here is that the self-energies of the two Shockley partials are independent of their spacing. It is only the interaction energy between the partials and the stacking fault area itself that involves the splitting distance d. The equilibrium spacing is to be determined by minimizing this total energy with respect to d. We note that the interaction energy may be written as (2) σi(1) (8.72) E int = j i j d V,

where the labels 1 and 2 refer to the two partners in the dissociation reaction as shown in ﬁg. 8.25. The dislocation lines are characterized by ξ (1) = ξ (2) = (0, 1, 0), b(1) = (b sin θ, b cos θ, 0) and b(2) = (b sin θ, −b cos θ, 0). For the special case of elastic isotropy we note that the stress tensor decomposes as shown in eqn (8.40) where we have invoked the observation that the partial dislocations themselves are mixed dislocations. The signiﬁcance of this observation is that it implies that the interaction energy may be written as the sum of two interactions, edge screw . Using the interaction energies derived earlier, this result E int = E int + E int

406

8 Line Defects in Solids

may be rewritten as E int

µb2 cos2 θ d d µb2 sin2 θ + . ln ln =− 2π(1 − ν) R 2π R

(8.73)

The minimization of eqn (8.71) is effected by differentiating the total interaction energy with respect to d and leads to

sin2 θ µb2 deq = − cos2 θ . (8.74) 2π γs f (1 − ν) Thus we see that the splitting of dislocations into partials is characterized by a stacking fault width that is set by the magnitude of the stacking fault energy, with low stacking fault energy materials having larger splittings. As said above, the splitting of dislocations into partials can be thought of as the most elementary of core effects.

8.6.2 The Peierls–Nabarro Model Despite the signiﬁcant gains that have been made with atomistic models of the dislocation core (which we will take up in the next section), it remains of interest to produce analytical insights into the role of the core. One compelling strategy in this regard is that known as the Peierls–Nabarro model which is but one example of the general class of cohesive surface strategies that we will take up in more depth in chap. 12. The cohesive surface strategy in this context is an artiﬁcial mixture of conventional continuum thinking in the form of a linear elastic treatment of the vast majority of the body with a planar constitutive model whose aim it is to mimic the atomic-level forces that act across the slip plane of the dislocated body. This example serves as yet another reminder of the way in which information gleaned at one scale (in this case the interplanar potential) can be used to inform models of a different type. The basic idea of such thinking is embodied in ﬁg. 8.26, where the separation of the dislocated body into two elastic half-spaces joined by atomic-level forces across their common interface is shown. The formulation is aimed at determining the energy minimizing slip distribution on the slip plane. From a kinematic perspective the dislocation is characterized by the slip distribution δ(x) = u(x, 0+ ) − u(x, 0− ) which is a measure of the disregistry across the slip plane. In order to provide a proper variational setting within which to pose this problem we must ﬁrst identify the total energy itself as a functional of this unknown slip distribution. The total energy is built up of two distinct contributions that impose competing inﬂuences on the equilibrium slip distribution. One of the terms in the total energy accounts for the atomic-level interactions across the slip plane which reﬂect the fact that there is

8.6 Modeling the Dislocation Core: Beyond Linearity

407

Fig. 8.26. Schematic of key elements in Peierls–Nabarro dislocation model (courtesy of R. Miller). The key idea is the use of a nonlinear constitutive model on the relevant slip plane which is intended to mimic the atomic-level forces resulting from slip.

an energetic penalty for the disregistry across the slip plane. In particular, we may write −∞ φ(δ(x))d x, (8.75) E misﬁt = ∞

where φ is the interplanar potential which accounts for the disregistry mentioned above. This interplanar potential is the essence of the cohesive surface approach in this context. The most distinctive characteristic of the interplanar potential is the fact that it is nonconvex, implying the existence of multiple wells, and thereby, the possibility for the emergence of complex microstructures such as dislocations. The particular signiﬁcance of this feature in the present setting is that the multiple well character of the interplanar potential allows for a disregistry across the slip plane of a Burgers vector without any attendant energy cost. For the present purposes, the interplanar potential should be thought of as the energy cost associated with sliding two half-spaces with respect to one another by some slip vector. We have already encountered this idea in our discussion of the ideal strength, and in fact, will once again invoke the energetics of rigid sliding given in eqn (8.2). Note that the interplanar potential has the same periodicity as the lattice and that whenever atoms across the slip plane have suffered a relative translation equal to a lattice translation, there is no attendant energy penalty.

408

8 Line Defects in Solids

Fig. 8.27. Decomposition of slip distribution into a superposition of inﬁnitesimal dislocations.

The second contribution to the total energy, which also depends upon the as-yet undetermined slip distribution δ(x) is the elastic energy associated with the dislocation. As indicated schematically in ﬁg. 8.27, the Peierls–Nabarro dislocation may be thought of as a continuous distribution of inﬁnitesimal dislocations. These dislocations in turn are imagined to suffer the usual elastic interactions between dislocations that were described above. Because of our use of linear elasticity, the dislocation ﬁelds are obtained through the superposition principle by adding up the contribution from each inﬁnitesimal dislocation separately. Recall that for the case of two edge dislocations at positions x and x within the conﬁnes of isotropic linear elasticity, the interaction energy is given by E int =

1 µb2 . 2π(1 − ν) x − x

(8.76)

This result may be borrowed for the continuous distribution imagined here once we recognize that the Burgers vector of each such inﬁnitesimal dislocation is related to the local gradient in the slip distribution as is seen in ﬁg. 8.27. Hence, the elastic energy due to all such dislocations is given by dδ(x) dδ(x ) µ R d x d x ln . (8.77) E elastic = 2π(1 − ν) x − x dx dx In the equation given above, R is an inconsequential constant introduced as a large distance cutoff for the computation of the logarithmic interaction energy. Given the energy functional which depends upon the unknown slip distribution we are now set up to use standard techniques to ﬁnd the energy minimizing slip distribution. Evaluating the functional derivative of the total energy with respect to the function δ(x) (which amounts to balancing the atomic-level forces with those due to the elastic interactions) results in the Peierls–Nabarro integro-differential

8.6 Modeling the Dislocation Core: Beyond Linearity

409

equation which may be written as µb ∂φ(δ) = − ∂δ 2π(1 − ν)

1 dδ(x ) dx . x − x dx

(8.78)

For the special case in which we make the simplifying assumption that the interplanar potential takes the simple cosine form given in eqn (8.2) and advocated earlier in the context of the ideal strength model, this problem allows for direct analytic solution. In particular, the solution is b b −1 x δ(x) = − tan . (8.79) 2 π a One of the key features that emerges from this solution, and a crucial hint for the type of analyses we will aim for in the future, is the fact that the stresses implied by the Peierls–Nabarro solution do not suffer from the same singularities that plague the linear elastic solution. A detailed examination of this point may be found in Hirth and Lothe (1992) and is illustrated in their eqn (8-13). By introducing an element of constitutive realism in the form of a nonlinear (and in fact nonconvex) interplanar potential, the solution is seen to be well behaved. One of the outcomes we require of our analysis of dislocations is an insight into the value of the stress needed to move a dislocation. The Peierls–Nabarro model offers the possibility of examining this question. The key qualitative feature that will emerge from our calculations will be the idea that a straight dislocation may be thought of as living in an effective potential that is periodic. The periodicity of this potential reﬂects the fact that there are many degenerate wells within which we may place the dislocation, each separated by a fundamental length determined by the crystal symmetry. In order to induce dislocation motion, the applied stress must be sufﬁciently high so as to overcome the lattice resistance provided by the periodic Peierls potential. As usual, we hark back to the role of symmetry breaking terms in inducing conﬁgurational forces, of which the Peierls stress is but one example. One of the dominant objectives posed in the context of the theory of dislocations is how such models may assist us in the understanding of crystal plasticity. As noted earlier, one measure of our success is our ability to shed light on the tandem questions of yield and hardening. As yet, our focus has primarily centered on the behavior of single dislocations, and is hence at best only an initial foray into these type of problems. From the single dislocation perspective, one of the ﬁrst questions we might hope to answer is that of how a single dislocation responds to the presence of an applied stress. Our earlier efforts were based upon the linear elastic theory of dislocations, and revealed that even in the presence of a very small stress, a dislocation will experience a force compelling it to motion. On the other

410

8 Line Defects in Solids

hand, the phenomenology of plasticity teaches us that dislocation motion is one of many examples of a phenomenon that exhibits threshold behavior. Until a certain critical stress is reached, the dislocation remains sessile. Our task is to uncover the microscopic origins of this threshold response. One immediate route that allows for the examination of this question is offered by the Peierls–Nabarro model discussed above. Recall that the total energy of the Peierls dislocation was seen as arising from two distinct sources. On the one hand, there is an elastic contribution that arises from the two half-spaces that are adjacent to the slip plane. Secondly, we argued that there is an energy cost associated with the disregistry across the slip plane (the so-called misﬁt energy). Within the conﬁnes of the continuum description offered above, the energy of the Peierls dislocation is invariant under translations of the dislocation coordinate. This result emerges from the fact that we treat the misﬁt energy as an integral over the slip plane disregistry. To remedy this ﬂaw, it is necessary to make further concessions in the direction of atomistic realism. In particular, we must sample the interplanar potential at those discrete positions that are consonant with the underlying crystal lattice. In particular, to compute the Peierls stress, we make the transcription ∞ ∞ φ(δ(x − xc ))d x → φ(δ(nb − xc ))x, (8.80) E misﬁt (xc ) = −∞

n=−∞

where we have introduced the parameter xc to denote the position of the dislocation as measured by the position on the slip distribution where the slip is b/2, for example (i.e. δ(xc ) = b/2). The signiﬁcance of this replacement is that rather than evaluating the misﬁt energy at a continuum of points along the slip plane, the energy of disregistry is computed at a series of equally spaced points meant to mimic the atomic positions themselves. In this context, it is imagined that the dislocation core is translated with respect to the atomic positions. For the particular choice of interplanar potential suggested by Frenkel, this sum may be written as ∞ 2π b b µb2 −1 x c + nb 1 − cos E misﬁt (xc ) = . (8.81) − tan 4π 2 d n=−∞ b 2 π a All that we have done to arrive at this equation is to use eqn (8.2) to evaluate the energy at various points on the slip plane which have undergone slip characterized by eqn (8.79). After appropriate massaging using obvious trigonometric identities, this sum may be rewritten as E misﬁt (xc ) =

∞ µb2 a 2 1 , 2 2 2π d n=−∞ a + (xc + nb)2

(8.82)

which has the look of a sum that might be handled by the Poisson summation

8.6 Modeling the Dislocation Core: Beyond Linearity

formula. The Poisson summation formula states ∞ ∞ ∞ f (n) = f (x)e2πikx d x, n=−∞

k=−∞

411

(8.83)

−∞

and is predicated on the hope that the transformed sum in the variable k will be more directly amenable than was the sum in n. If we introduce the dimensionless variables γ = a/b and δ = x/b, the sum may be rewritten as ∞ 2πiku ∞ µa 2 d du −2πikδ e , (8.84) E misﬁt = 2 2 2 2π d k=−∞ −∞ γ + u which after performing the relevant integrations leads in turn to 2π xc − 2πa µab b 1 + 2 cos e E misﬁt (xc ) ≈ . 2πd b

(8.85)

In performing this sum, we have kept only the terms corresponding to k = 0 and k = ±1. What has been achieved thus far? Our claim is that the calculation just performed tells us the energy proﬁle for a straight dislocation as that dislocation is moved against the background of the ﬁxed lattice. That is, the straight dislocation is now seen to have a series of wells in which it has a minimum energy and in the act of passing from one well to the next it must cross a barrier known as the Peierls barrier which gives rise to the intrinsic lattice resistance to dislocation motion. Our next task is to use our newly found Peierls potential to estimate the stress to move a straight dislocation. The stress is essentially provided as the derivative of the energy proﬁle with respect to the coordinate x, and is given by µ 2π x −πd/(1−ν)b ∂ E(x) =− sin e , (8.86) ∂x 1−ν b where we have used the recollection that the parameter a is a measure of the core width and is given by a = d/2(1 − ν). By evaluating the derivative of this expression in turn, we ﬁnd that the maximum value of the stress occurs when x = b/4, yielding an estimate of the Peierls stress of µ −π d/(1−ν)b . (8.87) τP = e 1−ν Our analysis calls for a number of observations. First, we note that the formula for the Peierls stress leads to the expectation that the stress to move a dislocation will be lowest for those planes that have the largest interplanar spacing at ﬁxed b. In the case of fcc crystals, we note that the spacing √ between (001) planes is given by a0 /2, while for (110)√planes the spacing is 2a0 /4, and ﬁnally for the (111) planes this value is a0 / 3. A second observation to be made concerns

412

8 Line Defects in Solids

the magnitude of the Peierls stress. What we note is that the stress to move a dislocation is down by an exponential factor in comparison with the shear modulus. Recall that in our discussion of the ideal strength, the expectation was that aside from numerical factors, the ideal strength goes as the shear modulus itself. By way of contrast, we now see that the presence of the dislocation modulates this estimate. A ﬁnal observation that should be made is that even this case is too idealized. Real dislocation motion often takes place by kink mechanisms in which a bulge on the dislocation line brings a segment of the dislocation into adjacent Peierls wells, and the resulting kinks propagate with the end result being a net forward motion of the dislocation.

8.6.3 Structural Details of the Dislocation Core Thus far, our discussion of dislocation core effects has been built around those tools admitting of direct analytic progress such as is offered by the Peierls–Nabarro dislocation core model. This model has many virtues. However, it is also strictly limited, with one of its primary limitations being that without huge machinations, it may only be applied to dislocations with planar cores. To explore the full atomic-level complexity that arises in dislocation cores, we must resort to numerical techniques, and direct atomistic simulation in particular. The remainder of our discussion on dislocation cores will take up the question of how one goes about carrying out such simulations and what may be learned from them. One of the central conclusions derived from the Peierls–Nabarro analysis is the role of nonlinear effects in the dislocation core. From an atomistic perspective, the far ﬁeld atomic displacements could be derived just as well from linear elasticity as the full nonlinear function that results from direct atomistic calculation. By way of contrast, in the core region it is the nonlinear terms that give rise to some of the complex core rearrangements that we take up now. Our discussion will be built around two key examples: cores in fcc metals and the core reconstructions found in covalent semiconductors such as in Si. Before embarking on the speciﬁcs of these cores, we begin with an assessment of the basic ideas needed to effect an atomistic simulation of the dislocation core. We begin with a picture of lattice statics in which the core geometry is determined by energy minimization. To proceed, what is needed is an energy function of the type discussed in chap. 4 which may be written generically as E tot = E({Ri }),

(8.88)

which gives the total energy once the atomic positions have been speciﬁed. For the moment, we are indifferent to the particulars of the choice of total energy scheme. Later we will see that the detailed core geometry can depend critically on this

8.6 Modeling the Dislocation Core: Beyond Linearity

413

choice, and that not all choices are equally satisfying. On the other hand, since our present ambition is the description of how to perform such a simulation we leave these details aside. From the standpoint of energy minimization, we have said all there is to say except for the all important issue of boundary conditions. For the moment, we describe the most naive approach to this problem and will reserve for later chapters (e.g. chap. 12) more sophisticated matching schemes which allow for the nonlinear calculations demanded in the core to be matched to linear calculations in the far ﬁelds. As we have repeatedly belabored, the objective is to allow the core geometry to emerge as a result of the full nonlinearity that accompanies that use of an atomistic approach to the total energy. However, in order to accomplish this aim, some form of boundary condition must be instituted. One of the most common such schemes is to assume that the far ﬁeld atomic positions are dictated entirely by the linear elastic ﬁelds. In particular, that is xi = Xi + u(Xi ),

(8.89)

where xi is the position of the far ﬁeld atom i in the dislocated crystal, Xi is the position of the same atom in the perfect crystal and u(Xi ) is the displacement of that atom in the dislocated crystal as obtained using Volterra ﬁelds for a single straight dislocation like those described in section 8.4. To perform the energy minimization, the atoms in the far ﬁeld are rigidly ﬁxed to their linear elastic values. As an initial guess, it is often elected to assume that the initial positions even for the atoms that are being relaxed is well described by the linear elastic solution. The forces are computed using the total energy scheme and the local minimum is found by any of a number of schemes including conjugate gradient, Monte Carlo, Newton–Raphson, etc. Core structures in fcc materials A key example of the strategy for direct atomistic simulation of dislocation cores advocated above is that of fcc metals. In this case, we consider the atomic-level geometry of a perfect dislocation (which by virtue of the relaxation will split ¯ and Burgers vector (a0 /2)(110). ¯ into partials) with line direction (112) The Volterra ﬁelds associated with this geometry are introduced using the scheme suggested in eqn (8.89). For the case shown here, the atomic-level relaxation has been performed using the conjugate gradient method on an arrangement of Al atoms described by the embedded-atom potentials of Ercolessi and Adams. These potentials are of the traditional pair functional form. As noted above, the key structural rearrangement that occurs for this type of dislocation is the splitting of the perfect dislocation into Shockley partials. This result is shown in ﬁg. 8.28. We note that the resulting atomic-level geometry is a concrete realization of the arguments made earlier in this section concerning dislocation dissociation.

414

8 Line Defects in Solids

Fig. 8.28. Atomic-level geometry of the dislocation core for the conventional edge dislocation in Al (courtesy of Kedar Hardikar): (a) a view along the line direction of the dislocation showing two partials, and (b) a view looking down on the slip plane, revealing the stacking fault region bounded by the two partials.

Core reconstructions in Si A more substantial rearrangement in the dislocation core can be found in the case of a covalent material. Probably the single greatest inﬂuence on the structures adopted by defects in covalent materials is the severe energy penalty that attends dangling bonds. Free surfaces, grain boundaries and dislocation cores all have geometries that reconstruct in a manner that preserves (albeit in a distorted way)

8.7 Three-Dimensional Dislocation Conﬁgurations

415

Fig. 8.29. Atomic-level geometry of the dislocation core for the 30◦ partial dislocation in Si (adapted from Bulatov et al. (1995)). (a) Unreconstructed core structure and (b) reconstructed core structure with dimerization along line direction.

the fourfold coordination of the atoms in question. In the present discussion, we examine a manifestation of this antipathy for dangling bonds in the context of dislocation core structures. For concreteness, we consider the core geometry of the 30◦ partial in Si as computed using Stillinger–Weber potentials. Recall from the discussion of chap. 4 that the Stillinger–Weber potentials incorporate an angular term which penalizes deviations from the ideal tetrahedral angles found in the cubic diamond structure. For the present purposes, the key feature of the atomic-level relaxations is the presence of a dimerization reaction as seen in ﬁg. 8.29. Prior to relaxation, the Volterra ﬁelds leave each atom in the core region missing one of its full complement of four neighbors. The relaxation remedies this loss by pairing up the atoms along the core direction, restoring fourfold coordination and lowering the energy.

8.7 Three-Dimensional Dislocation Conﬁgurations To have any hope of honestly addressing the dislocation-level processes that take place in plastic deformation, we must consider fully three-dimensional geometries. Though we earlier made disparaging remarks about the replacement of understanding by simulation, the evaluation of problems with full three-dimensional complexity almost always demands a recourse to numerics. Just as the use of analytic techniques culminated in a compendium of solutions to a variety of twodimensional problems, numerical analysis now makes possible the development of catalogs of three-dimensional problems. In this section, we consider several very important examples of three-dimensional problems involving dislocations, namely, the operation of dislocation sources and dislocation junctions.

416

8 Line Defects in Solids

Fig. 8.30. Geometry associated with dislocation bow-out between two pinning points.

8.7.1 Dislocation Bow-Out A recurring theme in a number of different contexts is that of dislocation bow-out. In a number of different circumstances, a dislocation segment of ﬁnite extent, pinned at its two ends, is subjected to a resolved shear stress which has the effect of bowing out the segment in its slip plane. The simplest setting within which to view this process is the line tension approximation set forth earlier in this chapter. Dislocation pinning is a ubiquitous phenomenon. Pinning arguments arise in the context of solution and precipitate hardening as well as the discussion of dislocation sources. Our present discussion has as its aim the development of some of the theoretical apparatus needed to discuss the response of dislocations in this context, without giving any attention to the attributes of the pinning centers themselves. We simply imagine a geometry like that shown in ﬁg. 8.30 in which the dislocation is pinned at the two endpoints, leaving a segment of length l that is free to glide. The energetics of the bowed-out segment may be constructed simply on the basis of line tension arguments. We begin by adopting the simplest possible model of line tension, namely, that in which the angular dependence is ignored altogether. In this case, the energy of the bowed segment as a functional of its displacement proﬁle u(x) is given by l l 2 2 2 T 1 + u dx − σ bu(x)d x. (8.90) E[u(x)] = − 2l

− 2l

Our interest is in determining the energy minimizing conﬁguration of the bowedout segment. To do so, we note that this has become a simple problem in variational calculus, with the relevant Euler–Lagrange equation being

T u d = −σ b. (8.91) d x (1 + u 2 ) 12

8.7 Three-Dimensional Dislocation Conﬁgurations

417

Even at the level of the line tension approximation, this equation may be solved to various levels of approximation. In the limit in which the bow-out is small (i.e. |u | 1), the denominator in the expression given above can be neglected with the result that the equilibrium equation takes the form, σb d 2u =− . 2 dx T The solution to this equation can be written down by inspection as

(8.92)

σb 2 x + cx + d, (8.93) 2T where c and d are as-yet undetermined constants. Note that the solution we seek satisﬁes the boundary conditions u(−l/2) = u(l/2) = 0. Application of these boundary conditions results in the solution σ b l2 2 (8.94) −x , u(x) = 2T 4 u(x) = −

which may be recast in dimensionless terms if the stress is measured in units of σ = f (2T /bl), and f is what fraction of 2T /bl the stress has attained, and similarly, we take x = δ(l/2). In light of these notational simpliﬁcations, our expression for the bowed-out proﬁle may be rewritten as fl (8.95) (1 − δ 2 ). 4 The equation for bow-out may also be solved exactly without resorting to the approximation in which |u (x)| 1. In this case, the equation of equilibrium may be written (after performing the ﬁrst integration) 2 σ bx u 2 +c , = − (8.96) 1 + u 2 T u(x) =

where c is a constant of integration to be determined in light of the boundary conditions. This equation is separable and leads immediately to the solution T2 T2 l2 2 u(x) = . (8.97) − x − − σ 2 b2 σ 2 b2 4 Like its approximate partner derived above, this equation can be rewritten in dimensionless variables as 1 1 l 2− − δ − 1 . (8.98) u(δ) = 2 f2 f2 In the treatment above, we have used the line tension approximation to deduce both an exact and an approximate treatment of bow-out. The comparison between

418

8 Line Defects in Solids

Fig. 8.31. Comparison of the bow-out geometry resulting from exact (full line) and approximate (dashed line) treatment of the line tension approximation. f is a dimensionless stress such that f = σ bl/2T .

the resulting solutions is shown in ﬁg. 8.31. As expected, we note that in the small bow-out limit, the exact and approximate treatments are in very good accord, while for larger stresses, their correspondence is completely unsatisfactory. We have deemed it worthwhile to examine this comparison since in many instances, the treatment of curved dislocations is made not only in the constant line tension approximation, but also with the assumption that |u | 1, an assumption we are now in a better position to view skeptically.

8.7.2 Kinks and Jogs Our treatment thus far has centered on idealized geometries in which the dislocation is presumed to adopt highly symmetric conﬁgurations which allow for immediate insights from the linear elastic perspective. From the phenomenological standpoint, it is clear that we must go beyond such idealized geometries and our ﬁrst such example will be the consideration of kinks. The formation of kink–antikink pairs plays a role in the interpretation of phenomena ranging from plastic deformation itself, to the analysis of internal friction. For the purposes of our modeling efforts here, we will treat the formation energy of kinks via a hybrid scheme in which the elastic energy of the dislocation line that has adopted a conﬁguration like that shown in ﬁg. 8.32 is treated in the line tension approximation. The line tension picture supposes that the energy associated with perturbing a dislocation line can be accounted for in much the same way that one describes the potential energy of a stretched string. If we ignore the dependence of the line energy on the angle between the line and the Burgers vector, then the line

8.7 Three-Dimensional Dislocation Conﬁgurations

419

Fig. 8.32. Schematic of the geometry associated with the formation of a kink in the dislocation line (adapted from Sch¨ock (1980)).

tension may be treated as a scalar T and the energy associated with distorting the line is given by E elastic = T 1 + u 2 d x. (8.99) The kink conﬁguration emerges as the result of a competition between the elastic energy as characterized by the line tension which favors a straight dislocation line and a nonlinear term whose origins are crystallographic. By virtue of the translational periodicity of the underlying lattice the dislocation line may be thought of as riding in a periodic potential that we will call W p (u) and which is really nothing more than the result obtained in eqn (8.85). The idea here is that there are a series of wells that the line can occupy and the kink is a mechanism whereby the line can pass from one such well into another. As noted above, the nature of the kink reﬂects a competition between two different factors. Consideration of ﬁg. 8.32 illustrates that in the limit that the energy scale associated with the line tension is much larger than that of the multiple welled Peierls potential, the dislocation line will vary slowly with a resulting wide kink. Alternatively, in the limit that the peaks in the Peierls potential are high, the lowest-energy conﬁguration will correspond to a kink that has as little of its length on that peak as possible. The mathematical setting for examining this competition is the functional minimization of the energy E[u(x)] = T 1 + u 2 d x + W p (u)d x. (8.100) As seen in the ﬁgure, the function u(x) characterizes the displacement of the line from the well at the origin. The boundary condition of interest here is that u(−∞) = 0 and u(∞) = b. Our ambition is to ﬁnd the energy minimizing disposition of the dislocation as described by the function u(x). This function in the present context is a complete

420

8 Line Defects in Solids

characterization of the kink geometry. Evaluation of the variational derivative of the total energy given in eqn (8.100) leads to an Euler–Lagrange equation of the form u d − W p (u) = 0. T√ (8.101) dx 1 + u 2 If we further assume that |u | 1, then the equation simpliﬁes to T u − W p (u) = 0.

(8.102)

Upon multiplication by u , we are immediately led to a ﬁrst integral of the problem, which implies in turn that the proﬁle satisﬁes du 2 = W p (u). (8.103) dx T This equation may be integrated to yield a kink geometry of the form " Wp 2π x 2b −1 e b T . (8.104) tan u(x) = π Furthermore, we may determine the energy of the kinked conﬁguration in light of our solution in conjunction with the ﬁrst integral of the motion found above. The deﬁnition of the kink formation energy is f

E k = E kink − E straight .

(8.105)

This may be rewritten using our knowledge of the line energy and the periodic potential W p (u) as ∞ ∞ ∞ 2π u f 2 Ek = dx − T 1 + u dx + W p 1 − cos T d x. (8.106) b −∞ −∞ −∞ If we now expand the square root and recall from our ﬁrst integral that T u 2 /2 = W p [1 − cos(2π u/b)], the resulting kink energy is given by ∞ 2π u f E k = 2W p d x. (8.107) W p 1 − cos b −∞ If we now substitute the solution for the kink proﬁle (i.e. u(x)) obtained in eqn (8.104), the resulting integral is elementary and results in a kink energy 4b f T Wp . (8.108) Ek = π In addition to the insights that can be gleaned from continuum arguments, atomistic analysis has been used to shed light on some of the structural complexity that attends the motion of kinks. The basis for our case study will be the partial dislocations that are known to exist in covalent materials such as Si. In particular,

8.7 Three-Dimensional Dislocation Conﬁgurations

421

Fig. 8.33. Schematic of the computational cell used to model the structure and energetics of kinks using atomic-level analysis (adapted from Bulatov et al. (1995)).

there have been a variety of atomic-level calculations of the structure and energetics of kinks in Si using both empirical potentials such as the Stillinger–Weber potentials introduced in chap. 4, but also on the basis of tight-binding theory and density functional theory. The key insight that will emerge from our discussion of atomic-level calculations of the structure and energetics of kinks is that the kinks themselves are capable of supporting a number of defects within a defect which can alter the properties of the kinks and which may invalidate some of the ideas on kinks advanced in the continuum setting. As was shown in ﬁg. 8.29, partial dislocations in Si admit of a core reconstruction that includes dimerization along the line direction. It is that reconstructed geometry that will serve as our jumping off point for the calculation of the structure and energetics of kinks in Si. The calculations to be considered here were carried out using a computational cell of the form shown in ﬁg. 8.33 in which a kink–antikink pair are imposed on the dislocation line. The energy minimizing geometry was determined in this case by resorting to a simulated annealing algorithm. Since the kinked conﬁguration, and even the dislocation conﬁguration itself, is metastable, care had to be taken to ﬁnd only local minima and to guard against falling into the deeper well corresponding to a conﬁguration free of any vestiges of the dislocation. Though the issues that were confronted in achieving this are interesting in themselves, we leave them here for our more immediate concern, namely, the kink geometries themselves. As can be seen in ﬁg. 8.34,

422

8 Line Defects in Solids

Fig. 8.34. Series of conﬁgurations associated with motion of kink on the 30◦ partial in Si (adapted from Bulatov et al. (1995)).

in addition to the ability to determine the energy wells corresponding kinks, it is also possible to ﬁnd the transition pathways connecting one kink conﬁguration to another. In addition to the questions that can be raised about kink motion, the type of atomistic analysis being described here has also been used to examine the propensity for nucleation of kinks themselves. Though plausible mechanisms for

8.7 Three-Dimensional Dislocation Conﬁgurations

423

homogeneous nucleation of kink–antikink pairs exist, a more compelling argument can be made for heterogeneous nucleation off of in-core defects known as antiphase defects (APD). These antiphase defects arise from the fact that when the core of the partial dislocation like that under consideration here reconstructs, a given atom can form a partnership (i.e. dimerize) with its partners either to the left or to the right. If a sequence of partnerships is struck to the right and then changes to a partnership to the left, the point at which this transition occurs will bear the imprint of this transition in the form of a dangling bond. An especially interesting conclusion deriving from the atomistic analysis is that these antiphase defects can serve as the hosts for the nucleation of kink–antikink pairs. The mechanism for this nucleation is shown in ﬁg. 8.35. The atomic-level calculations described above were carried out using the Stillinger–Weber potentials. A step toward a higher level of realism in the description of the total energy can be made by accounting for the electronic degrees of freedom. As has already been made evident throughout the book, an intermediate position which strikes a compromise between computational tractability and accuracy is the tight-binding method. A series of tight-binding calculations have been carried out on the same systems described above (Nunes et al. 1998) resulting in the same sort of structural information. An example of these results is shown in ﬁg. 8.36. Our main objective in this section has been to illustrate the way in which continuum and several different atomistic schemes can be brought to bear on the same underlying problem.

8.7.3 Cross Slip Another important class of three-dimensional dislocation conﬁgurations are those associated with the cross slip process in which a screw dislocation passes from one glide plane to another. The most familiar mechanism for such cross slip is probably the Friedel–Escaig mechanism, which is illustrated schematically in ﬁg. 8.37. The basic idea is that an extended dislocation suffers a local constriction at some point along the line. This dislocation segment, which after constriction is a pure screw dislocation, can then glide in a different slip plane than that on which is gliding the parent dislocation. This mechanism, like those considered already, is amenable to treatment from both continuum and atomistic perspectives, and we take them each up in turn. Since it is presumed that the process of cross slip is thermally activated, to the extent that we are trying to explicate the unit processes that make up plasticity it is of great interest to come up with an estimate for the activation energy for cross slip. In broad terms, what this implies is a comparison of the energies between the unconstricted and constricted states. The simplest continuum estimate

424

8 Line Defects in Solids

Fig. 8.35. Nucleation of a kink–antikink pair from an antiphase defect (adapted from Bulatov et al. (1995)).

of this process derives from the line tension approximation. At a higher level of sophistication it is also possible to investigate this process from the point of view of full three-dimensional elasticity. An overview of some of the continuum thinking on these problems can be found in Saada (1991). On the other hand, the continuum treatment of cross slip is attended by a number of uncertainties. An

8.7 Three-Dimensional Dislocation Conﬁgurations

425

Fig. 8.36. Series of conﬁgurations associated with motion of kink on the 30◦ partial in Si as computed using the tight-binding model (adapted from Nunes et al. (1998)).

attractive feature of atomic-level calculations is that they allow for a systematic investigation of some of the complex questions that have earlier been attacked from the line tension or linear elastic perspective. The cross slip process has attracted attention with a resulting series of impressive calculations of the various intermediate conﬁgurations connecting the initial and ﬁnal states of a dislocation that has undergone cross slip as well as the energy barrier that separates them

426

8 Line Defects in Solids

Fig. 8.37. Schematic of the Friedel–Escaig cross slip mechanism (adapted from Bonneville et al. (1988)).

(Rasmussen et al. 1997a). These calculations were undertaken using a pair functional description of the total energy. Though there are a number of technical details associated with the calculations to be presented here, we will concentrate primarily on what these calculations have to say about cross slip itself without entering too much into the ﬁne points of the calculation. Sufﬁce it to say that like in any problem in which one is in search of an activation pathway, it is not always true that this pathway is that which presents itself to intuition, and hence a number of clever schemes have been set forth for ﬁnding the transition state. In the present setting, the series of steps taking a dislocation from one glide plane to another are shown in ﬁg. 8.38. From a visual perspective, what we wish to take away from this calculation is that the mechanism of cross slip in this case is largely similar to that indicated schematically above in ﬁg. 8.37. The energy of the intermediate state is ≈ 2.7 eV higher than that of the starting conﬁguration, which raises serious questions as to whether the homogeneous nucleation of a constriction is really plausible. Future work will have to explore the possible catalytic effect of heterogeneities which can induce cross slip. An interesting continuum model of cross slip induced by the presence of slip plane heterogeneities may be found in Li (1961). As an illustration of the type of observations that can be made on cross slip, we show a set of beautiful experimental pictures of the cross slip process in ﬁg. 8.39.

8.7.4 Dislocation Sources Frank–Read Sources. It is well known that with increasing deformation, the density of dislocations increases. This effect is illustrated in ﬁg. 8.40 in which the number of dislocations as a function of the strain is indicated schematically. The immediate conclusion from this observation is the fact that there are sources

8.7 Three-Dimensional Dislocation Conﬁgurations

427

Fig. 8.38. Series of intermediate conﬁgurations during the cross slip process as computed using atomistics (adapted from Rasmussen et al. (1997b)).

Fig. 8.39. Experimental image of the cross slip process (courtesy of I. Robertson).

of dislocations within solids which serve to increase the number of dislocations present. Though there have been a number of mechanisms postulated for the multiplication of dislocations, the most celebrated mechanism is known as the Frank–Read source and will serve as the cornerstone of the present discussion. The increase in the net dislocation density with increasing deformation illustrates that even with the passage of some fraction of the dislocations out of the crystal at the surface, there must be sources operating within the crystal. From an experimental perspective, the nature of these sources at the statistical level remains largely unexplored. On the other hand, speciﬁc mechanisms have been suggested, one of which we take up in quantitative detail here. An overview on the subject of dislocation sources can be found in Li (1981). The Frank–Read mechanism postulates the existence of some ﬁnite segment that can be bowed out in the same sense as was discussed earlier in this section. With increasing stress, the segment

428

8 Line Defects in Solids

Fig. 8.40. Illustration of the increase in dislocation density with deformation (adapted from Asaro (1983)).

continues to bow out until a critical stress is reached beyond which the dislocation’s line tension is no longer able to resist the bow-out and the segment continues to expand indeﬁnitely. The speciﬁc analytic ideas associated with the bowing-out of a pinned segment were already described earlier in this section. As a result of these arguments, we ﬁnd that the applied stress and the radius of curvature of the bowed-out segment are related by R=

T . τb

(8.109)

An additional insight may be garnered from this discussion which applies to the Frank–Read source. For a segment that is pinned between two points by a spacing d, and that will operate as a Frank–Read source, we now see that with increasing stress the radius of curvature will reduce. For a given pinning geometry, the maximum stress will occur when the radius of curvature is half the spacing between

8.7 Three-Dimensional Dislocation Conﬁgurations

429

obstacles or 2T . bd

τsource =

(8.110)

If we now invoke an approximate expression for the line energy, namely, T = 1 µb2 , then the critical stress may be rewritten as 2 b . L

τsource = µ

(8.111)

Thus we note that we have argued for a dislocation source which operates at a stress that is smaller than the shear modulus by a factor of b/L. Though the argument given above was offered in the spirit of the line tension approximation, the Frank–Read mechanism can be examined from the linear elastic perspective as well. The segment which is to serve as the Frank–Read source has a geometry that is determined by two competing effects. On the one hand, the applied stress has the tendency to induce glide in the various segments that make up the dislocation. On the other hand, the mutual interactions of the various segments (the effect giving rise to the line tension in the ﬁrst place) tend to maintain the dislocation line in its straight conﬁguration. The playing out of this balance can be carried out dynamically by supposing that a given dislocation segment glides with a velocity that is proportional to the force it experiences. That is, the n th segment on the dislocation line is attributed a velocity vn = M Fn ,

(8.112)

where M is a parameter characterizing the mobility of dislocations in the overdamped limit considered here. The main point behind a dynamics like that described here is that we are considering the limit in which dissipative effects are dominant and the dislocation is maintained in a steady state of motion with the work of the applied stress all going into feeding the relevant dissipative mechanisms such as phonon drag which results from the coupling of the dislocations center of mass motion to the vibrations of the atoms around it. The sequence of states reached by a dislocation subjected to a sufﬁciently large applied stress is shown in ﬁg. 8.41. A second view of the dislocation dynamics approach to Frank–Read sources is shown in ﬁg. 8.42. A further elaboration of this so-called ‘dislocation dynamics’ approach will be set forth in chap. 12. One of the more intriguing features of ﬁgure 8.42 is the realization that the full elasticity treatment conﬁrms our intuition about those parts of the bowing-out process which occur at stresses larger than the critical stress.

430

8 Line Defects in Solids

Fig. 8.41. Frank–Read source as obtained using dislocation dynamics (adapted from Zbib et al. (1998)).

Fig. 8.42. Three-dimensional rendering of a Frank–Read source as obtained using dislocation dynamics (adapted from Ghoniem et al. (1999)).

8.7.5 Dislocation Junctions From the standpoint of the phenomenology of plastic deformation, one of the most important classes of three-dimensional conﬁguration is that associated with dislocation intersections and junctions. As will become more evident in our

8.7 Three-Dimensional Dislocation Conﬁgurations

431

Fig. 8.43. Two different competing geometries (courtesy of D. Rodney): (a) Two dislocations with Burgers vectors b1 and b2 and (b) junction case in which the junction segment has Burgers vector b1 + b2 .

discussion of work hardening (see chap. 11), dislocations on one glide plane can pierce the glide plane of another slip system, with the result that the gliding dislocation must pass through a ‘forest’ of obstacles. From our present perspective, we are interested in examining the geometric and energetic characteristics of the intersection of two such dislocations. Our arguments will begin in generic terms with the aim being an overall assessment of the structure and energetics of dislocation junctions with special reference to the stress needed to break them. The simplest picture of junction formation is largely geometric and relies on the line tension approximation introduced earlier. Perhaps the most fundamental insight to emerge from these studies is the conclusion that the stress to break such junctions scales as (arm length)−1 . Important discussions of the line tension approach may be found in Saada (1960) and Hirth (1961). The basic idea concerning the structure of junctions is the assessment of the energetics of two competing states, one in which the two parent dislocations (with Burgers vectors b1 and b2 ) remain unattached and the other in which the two parent segments join along the line of intersection of the relevant slip planes to form a new dislocation segment with Burgers vector b1 + b2 . The competition being played out here in three dimensions is much like its two-dimensional analog in which a perfect dislocation dissociates to form two partial dislocations bounding a stacking fault. The two competing geometries are illustrated in ﬁg. 8.43. For the purposes of examining the energetics of junction formation, we will concentrate on a highly symmetric geometry such that the arm lengths l1 and l2 are equal, and similarly, such that the angles φ1 and φ2 between the two dislocations and the line of intersection of the two relevant glide planes are equal. Within the conﬁnes of this

432

8 Line Defects in Solids

Fig. 8.44. Schematic of the behavior of the arms of a dislocation before and after junction formation.

geometric setup the energy of the state in which the two lines have not formed a junction is given by 1 1 E lines = 2 µb12l0 + 2 µb22l0 . (8.113) 2 2 Similarly, within the line tension approximation, the energy of the state in which a junction of length l j has formed is given by 1 1 1 E junction = 2 µb12l1 + 2 µb22l1 + 2 µ|b1 + b2 |2l j . (8.114) 2 2 2 Because of the choice of the highly symmetric geometry, the junction geometry is characterized by a single parameter. In particular, the parameters l j and l1 may be rewritten purely in terms of the angle φ1 and the initial arm length l0 . These geometric relations are illustrated in ﬁg. 8.44. What we note is that by the law of sines, l j and l1 are given by lj =

sin(φ1 − φ0 ) l0 , sin φ1

(8.115)

sin φ0 l0 . sin φ1

(8.116)

and l1 =

Further, we choose a conﬁguration in which |b1 | = |b2 | = |b1 + b2 |, corresponding to the three edges of one of the faces of the Thompson tetrahedron. The signiﬁcance of this geometric choice is that it guarantees that the line tensions of all three dislocation segments of interest will be equal. To examine the structure and energetics of junction formation from the line tension perspective, we now seek the equilibrium angle φ1 corresponding to a given

8.7 Three-Dimensional Dislocation Conﬁgurations

433

Fig. 8.45. Dimensionless length of junction within the line tension approximation as a function of the initial angle.

choice of initial angle φ0 and arm length l0 . The equilibrium condition is equivalent to ﬁnding the energy minimizer, which for the symmetric geometry considered here results in a one-parameter optimization problem. From above, we note that the energy change relative to the junction-free state is given by E = E junction − E lines = 2µb2

sin φ0 sin(φ1 − φ0 ) l0 + µb2 l0 − 2µb2l0 , (8.117) sin φ1 sin φ1

where l j and l1 have been eliminated in favor of φ1 and we have used the fact that the magnitude of all relevant Burgers vectors are equal. If we now seek equilibrium with respect to the angle φ1 , we are led to the equilibrium condition sin φ0 1 ∂E = (−2 cot φ1 + cosec φ1 ) = 0. 2 µb l0 ∂φ1 sin φ1

(8.118)

Solution of this equation leads to the conclusion that for this particular choice of Burgers vectors (i.e. the Lomer–Cottrell junction) the equilibrium angle is 60◦ . Using this result, and in light of eqn (8.115), we can now plot the junction length as a function of initial angle, namely, π sin − φ0 lj 3 . (8.119) = π l0 sin 3 The result is plotted in ﬁg. 8.45.

434

8 Line Defects in Solids

(a)

(b)

Fig. 8.46. Junction results from atomistics as computed using atomic-level analysis (adapted from Rodney and Phillips (1999)).

Atomistic Models of Dislocation Junctions. As noted above, the line tension approximation is largely geometrical and it is clear that an assessment of the accuracy of these ideas can be addressed from an atomistic perspective. One of the questions that one hopes to address from the atomistic perspective is the extent to which dislocation core effects (including the presence of dislocation splittings) alter the basic picture set forth in the line tension approximation. In keeping with the arguments given above, we continue to consider the geometry of the junction in which |b1 | = |b2 | = |b1 + b2 |. When carrying out an atomistic calculation of a problem of this type, it is obviously necessary to impose some choice of boundary conditions. Often, the imposition of such boundary conditions has unwanted side effects, and that is the case thus far with regard to the structure and energetics of junctions. Fig. 8.46 shows a sequence of snapshots in the deformation history of a junction in fcc Al as computed using pair functionals of the embedded-atom variety. Fig 8.46(a) illustrates the junction geometry in the presence of zero applied stress, while ﬁg. 8.46(b) illustrates the evolution of the junction in the presence of an applied stress. Linear Elastic Models of Junction Formation. Yet another scheme for addressing the structure and energetics of dislocation junctions is using the machinery of full three-dimensional elasticity. Calculations of this type are especially provocative since it is not clear a priori to what extent elastic models of junction formation will be hampered by their inability to handle the details of the shortest range part

8.8 Further Reading

435

Fig. 8.47. Lomer–Cottrell junction as computed using three-dimensional elasticity representation of dislocation dynamics (adapted from Shenoy et al. (2000)).

of the dislocation–dislocation interaction. It is important to emphasize that these calculations include far more physics than do their line tension counterparts since within the elasticity framework the interactions between the various segments are taken into account. The calculations to be considered here, shown in ﬁg. 8.47, are built around a linkage of the type of dislocation dynamics models set forth earlier in the context of Frank–Read sources and the ﬁnite element method which is used to discretize the dislocation lines themselves. In addition, this elastic model explicitly treated the interaction energies (and corresponding forces) that arise from the presence of stacking faults.

8.8 Further Reading The entire series Dislocations in Solids edited by F. R. N. Nabarro, North Holland Publishing Company, Amsterdam: The Netherlands is replete with articles pertinent to all aspects of dislocations (and many other topics as well). Many of those articles are relevant to the discussion advanced here. In particular, with reference to the crystallographic aspects of dislocations and the complex dislocation arrangements that occur in three dimensions I strongly recommend the article by S. Amelinckx in volume 2.

436

8 Line Defects in Solids

Dislocations by J. Friedel, Pergamon Press, Oxford: England, 1964. One of the great classics in the ﬁeld, what makes Friedel’s book particularly appealing is that almost every time a new theoretical construct is introduced, it is done so with reference to a particular experimental question in mind. ‘Dislocations and Walls in Crystals’ by J. Friedel in Physique des D´efauts/Physics of Defects edited by R. Balian et al., North Holland Publishing Company, Amsterdam: The Netherlands, 1980 makes for very interesting reading as Friedel revisits the theory of dislocations after a twenty-year interlude. I recommend this article very highly. Dislocation Based Fracture Mechanics by Johannes Weertman, World Scientiﬁc, Singapore: Singapore, 1996. What I ﬁnd especially engaging about this book is its idiosyncratic treatment of a number of problems. Weertman shows repeatedly how in adopting the notion of dislocation solutions as being fundamental, many interesting concepts may be explained concerning cracks and dislocations. Introduction to Dislocations by D. Hull and D. J. Bacon, Butterworth-Heinemann Ltd, Oxford: England, 1984. Ostensibly, this book is aimed at an audience uninitiated in the subject of dislocations. However, this may be deceptive since there are a variety of interesting discussions that are of interest even to seasoned veterans. Theory of Dislocations by J. P. Hirth and J. Lothe, Krieger Publishing Company, Malabar: Florida, 1992. The classic treatise on the mathematical theory of dislocations. This is always the ﬁrst place I look when I want to ﬁnd out something about dislocations. Mathematical Theory of Dislocations and Fracture by R. W. Lardner, University of Toronto Press, Toronto: Canada, 1974. This book treats a variety of interesting problems in dislocation theory without shying away from mathematically sophisticated treatments using the elastic Green function. A reference that I return to repeatedly. Thermodynamics and Kinetics of Slip by U. F. Kocks, A. S. Argon and M. F. Ashby, Pergamon Press, Oxford: England. This book is volume 19 of the series Progress in Materials Science, edited by B. Chalmers, J. W. Christian and T. B. Massalski. This book reﬂects the considerable knowledge of three leaders in the ﬁeld. One of the key features that makes the book so useful is that rather than concentrating on elastic solutions it considers how dislocations give rise to observed macroscopic behavior. Micromechanics of Defects in Solids by T. Mura, Kluwer Academic Publishers, Dordrecht: The Netherlands, 1993. A highly nonconventional treatment of

8.9 Problems

437

dislocations built around the idea of eigenstrains. This perspective is quite valuable in that it calls special attention to the lattice invariant shears that make such defects possible. ‘Dislocations in Particular Structures’ by S. Amelinckx from the 1979 volume of Dislocations in Solids is an incredible achievement in which Amelinckx considers the peculiarities of dislocations that attend particular crystal structures. A truly incredible article!

8.9 Problems

1 Microscopic description of the ideal shear strength Use the Morse pair potential constructed in chap. 4 to compute the periodic energy proﬁle for sliding one half-space relative to another for the fcc crystal. In particular, consider the sliding of adjacent (111) planes along the [110]-direction. Make a plot of this periodic energy proﬁle and include for comparison the Frenkel sinusoid for the same slip system. You will need to be careful to insure that your program computes the distribution of neighbors of an atom of interest to large enough distances. Also, multiply your potential by some rapidly decaying function at large distances so as to eliminate the artifact of atoms going in and out of the cutoff radius.

2 Displacements associated with an edge dislocation In this chapter we derived the strain ﬁelds associated with an edge dislocation. In this problem your goal is to derive the displacement ﬁelds implied by those strains and to use them to generate a projected atomic view of an fcc lattice with such a dislocation. (a) Using the strains for an edge dislocation, derive an expression for the displacements associated with such a dislocation. Hint: You will want to integrate the strains with respect to speciﬁc variables, but bear in mind that when you integrate with respect to x, for example, you still have an unknown function of y that is unspeciﬁed. (b) Consider the fcc crystal with a conventional perfect edge dislocation with a line direction of the type [112]. Use the displacement ﬁelds to generate a plot of the displaced atoms resulting from the Volterra solution. Explain why the picture results in the addition of two additional planes of atoms.

438

8 Line Defects in Solids

3 Asymptotic ﬁelds for dislocation dipoles In this problem, our aim is to investigate the far ﬁelds produced by a dislocation dipole. For simplicity, begin by considering two screw dislocations, both situated on the x-axis at positions (δ, 0) and (−δ, 0). (a) Using linear superposition of the ﬁelds due to these two screw dislocations, write an analytic expression for the ﬁelds at an arbitrary position (x, y). Comment on how the solution depends upon the relative signs of the Burgers vectors at these two dislocations. (b) Consider both the case in which the dislocations have opposite signs and that in which they have the same signs, and ﬁnd the leading order expansion for the far ﬁelds for both components of the stress tensor (i.e. σx z and σ yz ) in terms of the parameter δ. Note the enhanced decay rate of the stresses with distance in the case in which the dislocations have opposite signs. Further, observe that for the case in which the dislocations have the same sign, the far ﬁeld behavior is equivalent to that of a single dislocation with Burgers vector 2b. (c) Make your observations from the end of the previous part of the problem concrete by making a plot of the far ﬁelds for the case in which the signs of the two dislocations are the same. In particular, plot the exact stress ﬁeld for this dipole conﬁguration (which you know from part (a)) and that of a dislocation with Burgers vector 2b. Make your plot with respect to the dimensionless parameter r/δ and for a line at 45◦ with respect to the x-axis.

4 Edge dislocation ﬁelds using the elastic Green function This problem is a bit nasty, but will illustrate the way in which the Volterra formula can be used to derive dislocation displacement ﬁelds. (a) Imitate the derivation we performed for the screw dislocation, this time to obtain the displacement ﬁelds for an edge dislocation. Use the Volterra formula (as we did for the screw dislocation) to obtain these displacements. Make sure you are careful to explain the logic of your various steps. In particular, make sure at the outset that you make a decent sketch that explains what surface integral you will perform and why. 5 Isotropic Line Tension We advanced the idea that the energy of a dislocation line could be written in a local approximation as E(θ)ds. (8.120) E line =

(a) Explain the meaning of ‘locality’ and reproduce the argument leading to

8.9 Problems

439

E(θ) given as eqn (8.70). (b) By averaging over all θ , derive a result for a θ -independent line energy. Compare this with the conventional use of 12 µb2 .

6 Bow-out in the Line Tension Approximation In this chapter, the bow-out of a dislocation segment of length a was derived on the basis of an isotropic line tension approximation. This derivation culminated in eqn (8.97). Derive this equation and its dimensionless counterpart by ﬁrst writing down the functional E[u(x)] and then deducing the corresponding Euler–Lagrange equation which will then be solved via separation of the resulting differential equation.

7 Energy of Curved Dislocation in Line Tension Approximation We wrote down the energy of a curved dislocation as L T 1 + u 2 (x)d x. E line =

(8.121)

0

The problem with this expression is that it assumes that the line can be parameterized in terms of x. In this problem I want you to write down a fully general version of this result such that the line can wander in any direction and we can still write the energy as an integral over the line. Hint: Consider a parameteric representation of the dislocation and write the arc length in terms of this parameter. Show that your new expression reduces to the expression given above in the case in which your curve is parameterized by x. In addition, sketch a winding line for which more than one part of the line corresponds to a given x (i.e. it has overhangs) and discuss why the form derived in this problem is still applicable while that given in the equation above is not.

8 Elastic Forces for Three-Dimensional Dislocation Conﬁgurations Use isotropic linear elasticity to compute the elastic forces of interaction between two dislocations oriented as: (a) two perpendicular screw dislocations, (b) two perpendicular edge dislocations.

9 Line Tension Model for Dislocation Junctions Reproduce the arguments culminating in eqn (8.119).

440

8 Line Defects in Solids

10 fcc Dislocation Core Structure using Pair Functional Description of Total Energy Using the Johnson potential, determine the structure of the dislocation core in an fcc material. Consider a conventional edge dislocation on the (111) plane ¯ line direction. For a computational cell use a large cylinder in with a [1¯ 12] which the atoms in an annular region at the edge of the cell are frozen in correspondence with the Volterra solution. 11 Displacements due to a Dislocation Loop In eqn (2.96) we obtained the displacements due to a distribution of eigenstrains. In this problem, show that the eigenstrain associated with a dislocation loop with Burgers vector b on a plane with normal n is given by 1 (8.122) i∗j = (bi n j + b j n i )δ(r · n). 2 By integrating eqn (2.96) by parts and substituting this experession for the eigenstrain into the resulting formula, show that the expression given in eqn (8.32) is recovered.

NINE

Wall Defects in Solids

9.1 Interfaces in Materials Much of materials science and engineering is played out at the level of a material’s microstructure. From a more reﬁned perspective, the quest to tune or create new microstructures may also be thought of as a series of exercises in interfacial control. Indeed, interfaces in materials are the seat of an extremely wide variety of processes ranging from the conﬁnement of electrons to the fracture of polycrystals. The character of the interfaces that populate a given material leaves an indelible imprint on that material’s properties. Whether we consider the susceptibility of a given material to chemical attack at its surfaces, the transport properties of complex semiconductor heterostructures, or the fracture of steels, ushered in by the debonding of internal interfaces, ultimately, interfaces will be seen as one of the critical elements yielding a particular material response. In some cases, the presence of such interfaces is desirable, in others, it is not. In either case, much effort attends the ambition of controlling such interfaces and the properties that they control. Until this point in the book we have concerned ourselves with defects of reduced dimensionality. The present chapter aims to expand that coverage by turning to two-dimensional wall defects. The analysis of these defects will serve as our jumping off point for the consideration of microstructures within materials. From the start, the notion of material interface will be broadly construed so as to encompass free surfaces which are the terminal interface separating a material from the rest of the world, stacking faults which are planar defects in the stacking arrangement of a given crystal, grain boundaries which separate regions with different crystalline orientations and the interfaces between chemically or structurally distinct phases. The plan of the chapter is to begin with an introductory commentary on the role of interfaces in materials. This will be followed by three primary sections which treat surfaces, stacking faults and grain boundaries in turn. 441

442

9 Wall Defects in Solids

9.1.1 Interfacial Conﬁnement One organizing paradigm for examining the signiﬁcance of material interfaces is to think of them in terms of their role in producing conﬁnement. For the purposes of the present discussion, conﬁnement refers to the localization of some process or object either to the vicinity of the interface itself, or to a region that is bounded by such interfaces. In this section, we will consider examples of such conﬁnement in the context of elastic waves, which in certain cases are conﬁned to the vicinity of interfaces (i.e. Rayleigh and Stoneley waves), mass transport, in which interfaces serve as short-circuit diffusion paths and sinks for chemical impurities, and as impediments to dislocation motion, thus conﬁning plastic action to certain favorably oriented grains. Finally, we will note the signiﬁcance of internal interfaces in their role in providing a localizing pathway for fracture. Interfacial Conﬁnement of Mass and Charge. One of the key forms of conﬁnement induced by interfaces is associated with mass transport. What we have in mind is the localization of the diffusion process to the immediate vicinity of the interface in question. In particular, the presence of interfaces can lead to wholesale alteration of the rate at which processes involving mass transport transpire with a huge enhancement in the rate of diffusion along interfaces relative to bulk values. The macroscopic evidence for this claim is presented in ﬁg. 9.1 in which the rate of diffusion is shown not only for the bulk processes considered in chap. 7, but also for the short-circuit diffusion pathways presented by dislocation cores, free surfaces and internal interfaces. The origins of such phenomena are the conﬁning properties of interfaces with respect to point defects such as vacancies and substitutional impurities. As will be seen in more detail later, the structure of interfaces (whether surfaces or internal interfaces) reduces the barrier to the activated processes that occur during diffusion. From the standpoint of the analytic machinery set up in chap. 7, these short-circuit diffusion pathways are characterized by an activation energy for diffusion that is smaller than that found in the bulk. In addition to the role of interfaces in serving as a conduit for easy diffusion, the chemical potential proﬁle near such interfaces also makes them an ideal sink for point defects. The existence of such sinks leads in turn to the emergence of precipitate-free zones, local regions near grain boundaries characterized by the conspicuous absence of second-phase particles such as those that riddle the remainder of the material which is more distant from boundaries. An example of this phenomenon is depicted in ﬁg. 9.2. Again, the explanation for this behavior is the argument that because of the strong driving force which encourages foreign atoms in the vicinity of boundaries to diffuse to those boundaries, these foreign atoms are unavailable to participate in the nucleation and growth of second-phase particles.

9.1 Interfaces in Materials

443

Fig. 9.1. Diffusion data revealing the alteration in diffusion rates as a result of short-circuit pathways provided by interfaces and other defects such as dislocations (adapted from Gjostein (1972)).

Fig. 9.2. Illustration of a precipitate-free zone in a Cr-3 at.% Nb alloy (courtesy of Sharvan Kumar). The grain boundary runs from left to right through the middle of the picture, and reveals the existence of Cr2 Nb precipitates along the boundary itself and in the Cr matrix and the absence of such precipitates in a band near the boundary.

444

9 Wall Defects in Solids

In addition to their role in conﬁning mass, in some cases interfaces also have the effect of conﬁning charge to certain regions. As will be discussed in greater detail below, one of the most signiﬁcant types of internal interface is that representing a boundary between chemically distinct phases. Such interfaces play a pivotal role in modern microelectronics, and can be understood in part as a result of their role in serving as potential barriers for electronic properties. In chap. 3, the problem of conﬁnement in this context was evident in our solution of both the particle in the box and the quantum corral. Our interest at this juncture is to call attention to three-dimensional analogs of those systems, with special emphasis on the ways in which the internal interface serves as such a potential barrier which can have the effect of conﬁning electrons. Interfacial Conﬁnement of Waves. A knowledge of the complex interactions between waves and interfaces is at least as old as the ﬁrst explanation of Snell’s law of refraction on the basis of the wave theory of light. Indeed, with the further insight that upon passing from a medium with larger index of refraction to one with a smaller index of refraction, light could suffer total internal reﬂection, we see the roots of the ideas of interest to the current discussion. Not only do interfaces serve as the basis of conﬁnement in the context of electromagnetic waves, but they similarly alter the behavior of elastic waves. As was already discussed in chap. 5, the theory of linear elasticity may be used in order to consider dynamics in solids, illustrating the possibility of elastic waves within a medium. From the perspective of bulk excitations, we have already seen (see section 5.3.1) the formalism involving the acoustic tensor, and the subsequent propagating solutions. This earlier work may be generalized to consider waves at interfaces. Such waves have been dubbed Rayleigh waves in the context of those elastic waves conﬁned to surfaces, and Stoneley waves for the case in which such propagation is conﬁned to internal interfaces. The basic argument is that the equations of elastodynamics already highlighted in eqn (5.55), for example, admit of solutions not only in the bulk context, but also those localized to a region near the interface of interest. To see this, a trial solution to the equations of elastodynamics of the form u i (x, t) = Ae−γ z ei(k·r−ωt) ,

(9.1)

is considered. The key feature of this trial solution is its property that the displacement ﬁelds decay in the direction z perpendicular to the interface substantiating the claim that the wave amplitude is nonzero only in the vicinity of the interface. Interfacial Conﬁnement of Plasticity and Fracture. From the perspective of the mechanical properties of materials, interfaces are key players as a result of their unequivocal role in dictating mechanical response. The role of such interfaces in

9.1 Interfaces in Materials

445

Fig. 9.3. Pile up of dislocations against a grain boundary in Ti (courtesy of Ian Robertson).

mechanical response is perhaps most evident in the context of intergranular fracture in which the crack path follows the grain boundaries. As the crack propagates, it traverses the medium in a manner such that it is internal interfaces themselves that are the victims of bond breaking. Such fracture processes jibe with our contention that by virtue of interfaces, there is a conﬁnement of processes to a spatial region localized about these interfaces. However, internal interfaces can manifest their presence in the mechanical properties of materials in more subtle ways. In particular, in the context of plasticity in polycrystals, grain boundaries serve as obstacles to dislocation motion, leading to either dislocation pile-ups or grain boundary absorption of these dislocations. An example of the piling up of dislocations against a grain boundary in Ti as revealed by transmission electron microscopy is shown in ﬁg. 9.3. The detailed accounting for the elastic ﬁelds associated with such pile-ups as well as their implications for plastic deformation is given in chap. 11, whereas at present we only wish to remark upon the obstacle to dislocation motion offered by the presence of interfaces.

446

9 Wall Defects in Solids

In the discussion given above, we have illustrated the sense in which interfaces can alter material properties. The entirety of all interfaces found within a given material forms one of the key backbones of that material’s microstructure. Indeed, much of the actual business of microstructural control takes place at interfaces, either by eliminating them through processes such as grain growth, or by intentionally creating them such as in processes like the carburization of steel. Having motivated the idea of the importance of material interfaces, we will begin our analysis of interfaces in much the same way we treated point and line defects. Our analysis will begin by examining interfacial phenomena from a geometric perspective with an attempt to consider not only the geometry at the level of atomic positions, but also with regard to the macroscopic geometries associated with interfaces. Particular attention will be directed ﬁrst towards surfaces which are largely the point of communication between a crystal and the external world. Once the geometric and energetic preliminaries have been dispensed with, the discussion will lead in the direction of increasing geometric complexity as we confront ﬁrst, the reconstructions that attend many surfaces, and then the step features and roughening that are present on most real surfaces. Surfaces will be followed by a discussion of stacking faults and twin boundaries. The point of this part of the discussion will be to examine how the structure and energetics of such interfaces may be determined, and once such features are known, how they may be used to provide insights into observed material behavior. Stacking faults and twins may perhaps be thought of as the least severe of internal interfaces in that they represent the smallest departure from the monotony of the perfect crystal. After having examined the fascinating structural polytypes that can occur as a result of repeated ‘mistakes’ in the packing sequence of various crystal planes, we will take up the geometric and energetic features of grain boundaries. Our discussion on grain boundaries will commence with bicrystallography. However, the ultimate aim of these conceptual notions will never be far from the fore: an analysis of grain boundaries should leave us poised to tackle the more difﬁcult problem of the structure and energetics of polycrystals.

9.2 Free Surfaces The crystal surface is the seat of the vast majority of interactions that take place between a material and the rest of the world. Catalysis, crystal growth, and degradation via corrosion are but a few of the key processes that take place at surfaces. In each case, it is the interaction between a crystal on the one hand and the atoms arriving at the surface on the other that leads to the properties of interest. Another way in which the crystal surface has emerged as one of the key players in the study of solids is by virtue of the recent development of a number

9.2 Free Surfaces

447

of experimental probes which allow the direct observation of the behavior in the vicinity of the surface. In addition to their importance to the enterprise of materials science itself, surfaces have been one of the central proving grounds in the quest to construct a viable computational materials science. Because of the experimental capacity for explicit determination of surface structure, many calculations have been aimed at establishing the nature of the atomic-level geometries that occur on a given surface. With the increasing sophistication of experimental and theoretical tools alike, not only have the geometries of an increasing number of metal, semiconductor and ceramic surfaces been determined unambiguously, but also a rich variety of new phases associated with adsorbates, islands and steps have been uncovered. Our starting point for the analysis of this class of problems will be to consider the structure and energetics of ideal crystal surfaces.

9.2.1 Crystallography and Energetics of Ideal Surfaces From a geometrical perspective, if one imagines terminating a crystal on some particular crystal plane, there is a well-deﬁned and unambiguous idealized geometry. By this we mean that by virtue of the simple conceptual act of terminating the repeated packing of crystal planes along a particular direction, we are left with an exposed surface whose structure is determined unequivocally by the particulars of the underlying crystal lattice. We adopt the standard characterization of the crystallographic features of such a surface by exploiting the Miller indices. Stated simply, the Miller indices of a given surface are determined by ﬁrst noting the points of intersection of the surface of interest and the Cartesian axes. These numbers are then inverted and multiplied by an appropriate integer such that all three fractions have been converted into integers. These integers are the Miller indices. For the purposes of the present argument, our intention is to convey a sense of the structure and energetics of ideal surfaces. The single most obvious feature of these geometries is the loss of neighbors to those atoms at the surface. In the case of a covalent material, such as Si, this loss will be most signiﬁcant as a result of the formation of dangling bonds in which the Si atom is left with fewer neighbors than is energetically favorable. Clearly, the creation of such surfaces has energetic consequences. As a starting point for our foray into the energetics and motion of surfaces, we will consider the energetics of such idealized geometries. These calculations will serve as our point of departure for more elaborate analyses involving reconstructions, surface steps and islands. For the sake of physical transparency, our calculations will begin on the basis of an idealized pair potential model. Once these calculations are in hand, a more general

448

9 Wall Defects in Solids

Fig. 9.4. Schematic of the (100) surface of an fcc crystal. Filled circles correspond to atoms on the top layer, open circles are those one layer beneath the surface.

discussion of computing surface energies will be undertaken, ﬁrst with respect to pair functionals, and then through consideration of the general concepts appropriate to all energetic descriptions. Our endeavor to uncover the energetic features of surfaces begins with a pair potential description. For convenience, we leave the speciﬁc details of the pair potential unspeciﬁed, noting only that the total energy of the solid is written as E tot =

1 V (Ri j ). 2 ij

(9.2)

Further, we restrict our attention to the simpliﬁed analysis in which it is assumed that only near-neighbor interactions contribute to the energy. Consider a slab of fcc material with periodic boundary conditions in two of the three Cartesian directions, and exposed (100) surfaces in the third direction with a geometry like that shown in ﬁg. 9.4. For concreteness, we imagine a total of N atoms in the slab with m atoms per layer. Once we have adopted the pair potential mindset, which will be our temporary preferred mode of thought, the determination of the surface energy is reduced to little more than a proper accounting of the number of bonds lost by those atoms in the vicinity of the surface. In this case, it is only those atoms on the surface itself that suffer any reduction in coordination number and hence have an altered energy. In particular, consideration of ﬁg. 9.4 reveals that surface atoms on the fcc (100) surface are deprived of four neighbors. As a result of this argument, the total energy of the slab of atoms is given by E tot = 6(N − 2m)V (Rnn ) + 8mV (Rnn ),

(9.3)

where the ﬁrst term on the right hand side corresponds to bulk atoms that are not

9.2 Free Surfaces

449

disturbed by the presence of the free surface, while the second term corresponds to the 2m atoms participating in the two free surfaces. One of the key linkages between continuum and microscopic descriptions of interfaces is the notion of an interfacial energy. Though the use of such energies is by now entirely routine, nevertheless, this exempliﬁes the type of information passage that is one of the hallmarks of multiscale modeling. Note that from the perspective of the continuum mechanics of materials with interfaces, the total energy is often written in the form W (F)d V + γ (n)d A, (9.4) E tot =

∂

where F is the deformation gradient and W (F) is the strain energy density accounting for the energy of bulk deformation and where we have included the possibility of an anisotropic surface energy through the dependence of the surface energy γ on the surface normal n. The question of current interest is the microscopic origins of such a surface energy. On the basis of the total energy for the slab considered above, we are in a position to evaluate the surface energy. The key point is that the surface energy is computed by evaluating the difference between the N -atom system including the free surfaces and that of N atoms in the perfect crystal, and then dividing by an area factor that reﬂects the amount of exposed surface. For the case of the (100) surface, this amounts to E N (surface) − E N (bulk) , (9.5) 2A where the factor of 2 in the denominator accounts for the fact that there are two exposed faces on the slab under consideration. Our notation calls for the energy of the N -atom system in the presence of free surface (i.e. E N (surface)) and the energy of an N -atom bulk solid (i.e. E N (bulk)). In this case, E N (surface) is given by eqn (9.3), while E N (bulk) = 6N V (Rnn ), our result for the energy of an fcc crystal in a near-neighbor pair potential approximation. Hence, we ﬁnd that the surface energy is given by √ 4V (a0 / 2) γ100 = − . (9.6) a02 γ100 =

Note that in deducing this result we have not allowed for the possibility of structural relaxations that might occur for surface and near-surface atoms. The type of calculation illustrated above can be elaborated by appeal to more sophisticated descriptions of the total energy. Regardless of choice of energy function, the fundamental concept is embodied in eqn (9.5). In preparation for our discussion of surface reconstructions, we will generalize the description given above to the case of pair functionals such as the embedded-atom method. We adopt

450

9 Wall Defects in Solids

the Johnson-type embedded-atom functions already described in chap. 4 which permit analytic progress in the context of questions such as that raised here. Recall that in this case, our task is to supplement the pair potential description of the surface energy (already deduced above) with the contribution due to the embedding energy. Following the discussion from chap. 4, recall that within a pair functional description the energy takes the form, 1 F(ρi ) + φ(Ri j ), (9.7) E tot = 2 ij i where the former term is the embedding energy and is a function of the density at site i (i.e. ρi ). The density at site i may be deduced in turn according to f (Ri j ), (9.8) ρi = j

where the function f (R) yields the contribution to the density at site i from a neighbor at a distance R. We will denote f (Rnn ) = ρnn , with the result that the energy of N atoms in a bulk fcc environment is given by E N (bulk) = N F(12ρnn ) + 6N φ(Rnn ). As with our evaluation of the surface energy in the strictly pair potential setting, the pair functional assessment of the total energy can be obtained essentially on the basis of bond counting. Again, if we assume a near-neighbor model in which not only is the pair potential range restricted to near neighbors, but so too is the function determining the electron density, then only atoms that are at the surface itself have environments that are distinct from the bulk. In particular, the total energy of the N -atom system in which there are two exposed (100) surfaces is given by, E N (surface) = (N − 2m)F(12ρnn ) + 6(N − 2m)φ(Rnn ) + 2m F(8ρnn ) + 8mφ(Rnn ),

(9.9)

where we have used the same geometry as that considered in the pair potential calculation. The ﬁrst two terms on the right hand side arise from the bulk atoms, while the second two terms reﬂect the presence of the free surface atoms. If we imitate the strategy used above in the pair potential context, it is found that the surface energy is given by γ100 =

2[F(8ρnn ) − F(12ρnn )] − 4φ(Rnn ) . a02

(9.10)

To put these expressions in perspective, we now examine the types of numerical values they imply for fcc surfaces. Using the analytic potentials of Johnson introduced in chap. 4, the surface energies of fcc Cu are γ111 = 0.99 J/m2 ,

9.2 Free Surfaces

451

γ100 = 1.19 J/m2 and γ110 = 1.29 J/m2 , which are nearly identical to the experimental values for this system, although we should recall that the potentials are ﬁtted to a number of important properties, though not the surface energies themselves. These results for the energy of free surfaces represent the ﬁrst in a hierarchy of interfacial energies that will be discussed in this chapter. As was already hinted at above, interfaces in solids come in a number of different forms resulting in several different energy scales. At the low end of the energy spectrum are the energies of twin boundaries and stacking faults. These are followed by the energies of grain boundaries which are superseded by the even higher energies associated with free surfaces. In the preceding parts of this section, our emphasis has been on the fundamental ideas associated with the energetics of ideal surfaces. Before embarking on the reﬁnement of our arguments to the consideration of surface reconstructions, we close this section with a few details related to the use of microscopic analysis to analyze in a systematic way the energies of free surfaces. First, we reiterate the importance of eqn (9.5), which is the basis of surface energy calculations whether one uses the lowliest of pair potentials or the most sophisticated ﬁrst-principles techniques. On the other hand, the details of implementation can differ depending upon the situation. One of the critical questions that must be faced when using more computationally expensive techniques is the thickness of the computational slab. On the one hand, one aims for carrying out such calculations using the fewest number of atoms possible. By way of contrast, failure to use a thick enough computational cell will result in interactions between the two surfaces. As with many of the ﬁrst-principles calculations that we have already described, there are a series of generic issues that must be faced in making a systematic analysis of features such as the surface energy. One useful class of calculations examines trends in important material parameters such as the surface energies. A systematic analysis of the surface energies of 60 metals has been carried out by Vitos et al. (1998) using a variant of the LMTO method. As we described in chap. 4, there are a number of different versions of the ﬁrst-principles solution to the Schr¨odinger equation which differ in the details of how they handle the ionic potential, the basis functions used to represent the wave function, and so on. The LMTO method is one of this set of methods. Periodic boundary conditions are employed with the added twist that vacuum layers separate surfaces along the stacking direction of interest. For example, in their analysis of fcc (111) surfaces, they use a slab that is four atomic layers thick with an associated vacuum layer that is two atomic layers thick. An example of the type of results that are obtained for the 4d transition metals is shown in ﬁg. 9.5. Note that as the number of d-electrons per atom (i.e. the band ﬁlling) increases, the surface energies exhibit a characteristic rise until the d-band is half-ﬁlled and then decline as the number

452

9 Wall Defects in Solids

Fig. 9.5. fcc (111) surface energies for 4d transition metals (adapted from Vitos et al. (1998)).

of d-electrons is further increased. This behavior is reminiscent of that associated with the cohesive energies reported in ﬁg. 4.18. Another way of representing the trends in surface energies is to examine the anisotropy in passing from one low-index surface to another. The surface energy anisotropy between the (100) and (111) surfaces is characterized by the ratio γ100 /γ111 . Fig. 9.6 reveals the surface energy anisotropies for the 4d transition metals where it is seen that there are systematic, but rather small, variations in the surface energy anisotropies. The discussion given above has concentrated on the energetics of metal surfaces. Though we could similarly enter into a description of the energetics of ideal semiconductor surfaces, such a discussion is much less revealing since in the case of semiconductor surfaces, the driving force for structural reconstruction is so high. As a result, we ﬁnd it convenient to await a discussion of semiconductor surfaces until we have introduced the next level of structural elaboration, namely, that of surface reconstructions.

9.2.2 Reconstruction at Surfaces The previous section highlighted the geometric aspects of surfaces that arise on carrying out the conceptual exercise of abruptly terminating the packing sequence along a given crystallographic direction. In the vast majority of cases, this ideal geometry is little more than a ﬁction and what is really found is a reconstructed geometry in which the atomic positions in the vicinity of the surface are distinct from those that are implied by merely truncating the crystal on a particular plane. Such reconstructions are the two-dimensional analog of the type of reconstructions

9.2 Free Surfaces

453

Fig. 9.6. Surface energy anisotropies for 4d transition metals (adapted from Vitos et al. (1998)).

described in the previous chapter as concerns dislocations in semiconductors (see section 8.6.3). The intention of this section is ﬁrst to provide plausibility arguments as to the origins of the structural rearrangements that attend the formation of free surfaces, several key examples of which are given in ﬁg. 9.7. The two key structural rearrangements to be considered here are: (i) structural relaxations in which the spacing between adjacent layers in the direction perpendicular to the surface is altered as is shown schematically in ﬁg. 9.7(a), and (ii) surface reconstruction in which there is a complete rearrangement of the surface geometry as shown schematically in ﬁgs. 9.7(b) and (c). In the case of these reconstructions, the symmetry of the surface can be completely altered relative to the bulk termination. Once we have spelled out the conceptual features of both surface relaxation and reconstruction we will give the particular details associated with a few different representative examples on both metal and semiconductor surfaces. We further idealize the discussion through the assumption that the various competing structures are thought of in a vacuum, since a further intriguing but difﬁcult complexity is introduced once foreign species are adsorbed on the surface. Plausibility Argument for Surface Relaxation. As already noted above, crystal surfaces are characterized by a wide range of structural rearrangements relative to the ideal surface. One such rearrangement is surface relaxation, with the entire surface layer moving either towards or away from the subsurface layers as shown

454

9 Wall Defects in Solids

Fig. 9.7. Schematic of some of the key rearrangement mechanisms at surfaces (adapted from L¨uth (1993)): (a) surface relaxation, (b) surface reconstruction and (c) missing-row reconstruction.

Fig. 9.8. Schematic illustrating the strengthening of back bonds at a free surface (adapted from Carlsson (1990)). Double and triple lines associated with surface atoms are meant to indicate the strengthening of bonds associated with those atoms that have lost neighbors due to the free surface.

in ﬁg. 9.7(a). One way to see the origins of this tendency is via the types of simple arguments we used earlier to justify the extra physics incorporated in pair functionals. In particular, we recall the essence of such models is in the fact that the bond strength is dependent upon the coordination number of the atom of interest. The coordination number dependence of the bond strength was illustrated in ﬁg. 4.5. In the context of free surfaces, as a result of the loss of neighbors to those atoms at the surface, there is a subsequent strengthening of back bonds between the surface atoms and their subsurface partners. This effect is indicated schematically in ﬁg. 9.8. Plausibility Argument for Surface Reconstruction. In addition to the types of relaxations discussed above, surfaces may also suffer massive rearrangements referred to as reconstructions. These reconstructions often represent a complete rearrangement of the underlying ideal geometry and may bear no resemblance to the subsurface structure. The crystallography of these symmetry breaking rearrangements is illustrated in ﬁg. 9.9. As is evident from the ﬁgure, there is some new notational baggage that goes along with the description of surface reconstructions. In particular, if we elect to denote the symmetry of the ideal

9.2 Free Surfaces

455

Fig. 9.9. Schematic of the symmetry changes that attend surface reconstruction for case of several surfaces (adapted from L¨uth (1993)).

surface in terms of two lattice vectors a and b, then the bulk termination of the surface is designated as having a (1 × 1) symmetry since the surface unit cell is bounded by the vectors a and b themselves. In the event that the surface undergoes a symmetry breaking reconstruction, the surface unit cell will be built up of larger multiples of the vectors a and b. In particular, if the surface unit cell is bounded by the vectors n 1 a and n 2 b, then the surface reconstruction is designated as the n 1 × n 2 reconstruction. Four distinct examples of this thinking are illustrated in ﬁg. 9.9 where frames (a) and (b) show a 2 × 2 reconstruction on a (100) surface, and frames (c) and (d) show examples from (111) surfaces. As we have already emphasized, the energy computed in the previous section is the ideal surface energy, and does not reﬂect the possible further energy reduction that attends a symmetry breaking surface reconstruction. On the other hand, we seek to understand the driving force towards such reconstruction in energetic terms. Perhaps the most immediate context within which to view the emergence of reconstructions is on semiconductor surfaces where simple arguments concerning

456

9 Wall Defects in Solids

Fig. 9.10. Representation of ideal and 2 × 1 reconstructed geometries for Si (001) (courtesy of Lloyd Whitman).

the necessity to saturate unfulﬁlled bonds give intuitive plausibility to such reconstructions. For example, in the case of the (001) surface in Si as depicted in ﬁg. 9.10, we see that the ideal surface is replete with dangling bonds. As in the case of the semiconductor dislocation cores discussed earlier, there is a driving force towards dimerization which has the effect of eliminating the dangling bonds through reconstruction. In particular, in this case we see that in the ideal 1×1 state, each surface atom has two dangling bonds. By virtue of the pairing up of adjacent surface atoms a 2 × 1 symmetry is induced which has the effect of reducing the number of dangling bonds on each atom. Computing Surface Reconstructions and Their Energies. Thus far, we have succeeded only in giving plausibility arguments for the emergence of reconstructions as structural competitors to the ideal bulk terminations. On the other hand, it is by now evident from preceding chapters that an analysis of the energetics and dynamics of such surfaces may be made through an appeal to the energetic methods of microscopic simulation. One difﬁculty faced in trying to carry out a systematic study of such reconstructions on the basis of energetic analyses is the biasing role played by the supercell dimensions. For example, if the overall lateral supercell size is 5 × 5, this implies that it is not possible to obtain structures with periodicities incommensurate with the underlying substrate, nor those structures with a surface unit cell larger than the 5 × 5 cell made available in the computation. One remedy to this difﬁculty is the construction of effective Hamiltonians from which it is possible to carry out not only much larger simulations, indeed with the

9.2 Free Surfaces

457

possibility for the emergence of long-period structures, but also to use the tools of statistical mechanics which in some cases allows for direct analytic progress to be made on the relevant Hamiltonian. We will give examples of this strategy in the pages that follow in the context of reconstructions on both the Au and W surfaces. Case Studies on Metal Surfaces We have already emphasized the revolution in surface science ushered in on the heels of high-quality vacuum technology and surface scanning probes. One subbranch of surface science that has been the beneﬁciary of these advances is the study of metal surfaces. The intention of this subsection is to consider two distinct case studies, namely, the surfaces of fcc Au and those of bcc W. These choices are inspired by the combination of high-quality experimental data, richness of surface phases, their diversity from the standpoint of the demands they place on atomistic simulation and their relevance to later generalizations to surfaces with steps, islands and even more extreme forms of roughness. Surface Reconstructions in Au. Gold is one of a number of systems that exhibits a wide range of fascinating surface reconstructions, which includes a host of orientational phases in the presence of steps. For our purposes, the Au system serves as a rich example not only for our arguments concerning surfaces and their reconstructions, but also as a basis for contrasting many of the different energetic arguments that have been set forth so far in the book. What we will ﬁnd is that the Au surfaces have been attacked from a wide variety of pair functional approaches, by recourse to ﬁrst-principles techniques and using different effective Hamiltonians. In fact, much of the theoretical effort on the Au(001) surface will be reminiscent of our earlier treatment of the Peierls–Nabarro model and treatments yet to come of cohesive zone models. Finally, the existence of a variety of X-ray, scanning tunneling microscopy and other experimental data makes the Au surfaces very appealing. For concreteness, we consider the (001) surface of Au. The unreconstructed geometry corresponds with the bulk termination along this direction and is nothing more than a square lattice, rotated at 45◦ with respect to the cubic directions. This geometry may be contrasted with a depiction of the reconstructed geometry, shown in ﬁg. 9.11. The key qualitative features of the reconstructed geometry are related, namely, a tendency towards close packing which is manifested as a nearly hexagonal arrangement of the surface atoms. As can be seen in the ﬁgure, the ideal bulk termination corresponds to the square grid, while the actual atomic positions form a pseudohexagonal arrangement. These structural insights have been garnered from a series of X-ray measurements as reported in Gibbs et al. (1990).

458

9 Wall Defects in Solids

Fig. 9.11. Reconstructed geometry for Au(001) surface (adapted from Gibbs et al. (1990)). The ﬁgure shows only the surface layer of atoms.

Fig. 9.12. Sequence of phases associated with Au(001). At high temperatures, distorted hexagonal phases are superseded by disordered phase with 1 × 1 symmetry. RDH refers to rotated–distorted hexagonal phase, DH refers to distorted hexagonal phase and DIS refers to disordered phase. Note that the schematic of the rotated hexagon associated with RDH exaggerates the rotation. In addition, the orientation relationship between the hexagonal structures and the subsurface atoms is not represented.

The experimental data associated with this surface are actually more revealing than we have suggested (Gibbs et al. 1990, Abernathy et al. 1992). On the basis of systematic X-ray reﬂectivity studies, it has been deduced that a sequence of phases are found as a function of temperature: these phases are shown schematically in ﬁg. 9.12. In particular, two related pseudohexagonal phases have been found which differ by a small relative rotation in addition to a high-temperature disordered phase in which the pseudohexagonal symmetry is lost. However, despite the apparent abruptness and reversibility of the transition between the two distorted hexagonal phases, it remains unclear whether or not these structures constitute true equilibrium phases. The mission of any energetic methods that might be brought to bear on the structure of this surface is to explicate the origins of its tendency towards close-packing, even at the cost of abandoning its epitaxial relationship with the subsurface layers. Our strategy is to contrast pair functional and ﬁrst-principles approaches to this reconstruction. In addition, we will examine the way in which ﬁrst-principles calculations may be used to construct an effective Hamiltonian for

9.2 Free Surfaces

459

this system and through which the competing inﬂuences governing the transition become more clear. A repeating theme that has been played out in modeling defects ranging from vacancies and interstitials, to dislocation cores and surface reconstructions is that of successive approximation. Often, the ﬁrst treatment of a new problem is put forth from the perspective of some empirical description of the total energy. The Au(001) surface is no different. The initial efforts to uncover the origins of this reconstruction were built on pair functional descriptions of the total energy (Ercolessi et al. 1986, Dodson 1987, Wang 1991). The argument was made that by virtue of the embedding term, the complex interplay of in-plane densiﬁcation and subsurface pinning could be considered. An example of the type of results that emerge from such simulations is shown in ﬁg. 9.13. The basic idea of the simulations was to construct a slab with some ﬁnite size and associated periodic boundary conditions. Note that the selection of a particular periodicity in the in-plane directions rules out symmetry breaking distortions whose periodicities (if any) are larger than these cells. The geometries are then relaxed, usually via some ﬁnite temperature annealing scheme (Monte Carlo or molecular dynamics) and are slowly cooled until the resulting energy minimizing conﬁguration is determined. The claim has been made that by carrying out molecular dynamics calculations at a sequence of increasing temperatures, pair functional schemes are sufﬁciently accurate to capture the series of transitions that are observed with increasing temperature. This claim is substantiated by appeal to calculations of the structure factor which provides a geometric signature of the surface geometry. Inspection of the results of such pair functional calculations of the Au(001) reconstructed geometry reveal a marked tendency towards the close-packed distorted hexagonal structures implied by experiment, though the precise surface periodicity probably remains out of reach of these methods. More accurate ﬁrst-principles calculations have also been undertaken with respect to the Au(001) reconstruction (Takeuchi et al. 1991). These calculations were conceptually identical in all essentials to those carried out using the pair functional description of the total energy. However, an important added feature was the additional task of considering the isoelectronic Ag system, with the aim of examining why the (001) surface of Au reconstructs while that of Ag does not. Further, by treating the subsurface layers of the Au crystal as a uniform electron gas, the ﬁrst-principles analysis was able to separate the competition between the surface atoms increasing their coordination number and the subsurface atoms locking the surface atoms into crystallographic positions. The desire for both computational tractability and physical transparency suggests the usefulness of effective Hamiltonians. We have emphasized the desirability of ﬁnding degree of freedom reducing strategies in which only those degrees

460

9 Wall Defects in Solids

Fig. 9.13. Several views of the (34 × 5) Au(001) surface reconstruction as obtained using a pair functional description of the total energy (courtesy of Furio Ercolessi). The atoms in the ﬁrst layer are colored in gray scale according to their z-coordinates: the lighter the color the larger z. The second layer atoms are colored black.

of freedom of real importance to the physical question at hand are considered. The Au(001) surface features two competing energetic factors: (i) the in-plane energy gain associated with a local increase in coordination number and favoring

9.2 Free Surfaces

461

a close-packed hexagonal arrangement, (ii) the subsurface pinning potential which favors a locking in of the surface atoms into registry with those beneath the surface. This competition suggests an effective Hamiltonian of the form 2π xi 2π yi V (Ri j ) + A cos , (9.11) E tot ({Ri }) = + cos a a ij i where the set {Ri } characterizes the entirety of atoms on the surface. The ﬁrst term on the right hand side represents the in-plane interactions between neighboring atoms, and for our purposes should be thought of as a pair potential that favors a near-neighbor distance smaller than that determined by the bulk termination of the surface. In particular, this term inclines the surface atoms to a two-dimensional close-packing geometry. The second term is a lock-in term and characterizes the interaction between the surface atom with coordinates (xi , yi ) and the atoms beneath the surface which have been buried in this effective potential. Note that this pinning term carries exactly the same sort of information as the interplanar potential introduced in the context of the Peierls–Nabarro model, and similarly, exploits the same sorts of locality assumptions favored there. In addition to the general theme of degree of freedom reduction, we have noted the objective of information transfer in which calculations at one scale are used to inform those used at a different scale. In the current context, we refer to the use of ﬁrst-principles calculations to inform the effective Hamiltonian of eqn (9.11). Like with the treatment of the interplanar potential associated with the Peierls–Nabarro model, the coefﬁcient A in eqn (9.11) is obtained on the basis of rigid sliding geometries in which the surface layer is slid with respect to the subsurface layer and the resulting energy is computed. In this case, it is the difference in energy between the conﬁguration in which all atoms have their bulk-terminated in-plane positions and that conﬁguration in which all surface atoms have slid by the vector δ = (a/2, a/2). The potential determined in this way is shown in ﬁg. 9.14. As usual, once the effective Hamiltonian is in hand, it is possible to investigate its implications for the equilibrium phases of the system. In this case, the outcome of examining the equilibrium structure associated with this Hamiltonian is shown in ﬁg. 9.15. Surface Reconstructions in W. In earlier sections, we have noted that the pair functional formalism is not always appropriate as the basis for an energetic description of metals. One case where this is evident is in the context of the surface reconstructions seen on certain bcc transition metals. In particular, the (001) surface of both W and Mo exhibits fascinating reconstructions, and as in the case of the Au(001) surface, the symmetry breaking distortions leave few vestiges of their crystallographic ancestry.

462

9 Wall Defects in Solids

Fig. 9.14. Representation of interplanar potential characterizing the locking in of surface atoms to their subsurface partners.

Fig. 9.15. Minimum energy conﬁguration for Au(100) as obtained using the effective Hamiltonian deduced from ﬁrst principles (adapted from Takeuchi et al. (1991)).

The ideal (001) surface of crystals with the bcc structure is illustrated in ﬁg. 9.16(a). We note that the ideal termination of this surface is a square lattice with a lattice parameter equal to that associated with the bulk crystal itself. This geometry may be contrasted with that of the reconstructed geometry in W in ﬁg. 9.16(b). The surface geometry can be continuously altered from the ideal bulk termination to the reconstructed state by imposing a series of surface displacements

9.2 Free Surfaces

463

Fig. 9.16. Schematic of the ideal bulk termination and reconstruction associated with certain bcc (001) surfaces: (a) ideal bulk termination for (001) surface of bcc crystal, (b) (001) reconstruction of W. The amplitude of the reconstruction is exaggerated for ease in viewing. Dark circles correspond to surface layer atoms and gray circles are associated with atoms in ﬁrst subsurface layer.

of the form umn = u0 cos(q · Rmn ),

(9.12)

where mn is a label for√the atom √ at surface position Rmn = mai+naj, u0 is a vector of the form u0 = δ(1/ 2, 1/ 2) and characterizes the amplitude and direction of the surface distortion and q is a wavevector that characterizes the periodicity of the surface reconstruction itself. For the reconstruction of interest here, the wavevector q is of the form q = (π/a)(1, 1, 0). The reconstructed surface is characterized by two distinct phases, one with c(2 × 2) symmetry (below ≈ 210 K) and one with (1 × 1) symmetry above that temperature, with the high-temperature phase thought to be a disordered state rather than the ideal bulk termination. The low-temperature ˚ phase is characterized by lateral displacements δ ≈ 0.25 A. The (001) surface reconstructions of bcc metals have become something of a proving ground for new total energy schemes. Our discussion in chap. 4 of angular potentials considered the role of angular forces in stabilizing certain characteristic geometric features of bcc crystals, and these features are revealed again in the context of the reconstruction. Instability of the surface with respect to a distortion of wavevector q can be considered via a series of static calculations in which the energy is repeatedly computed for increasing δ. An example of calculations of this sort is shown in ﬁg. 9.17. We note that the basic strategy adopted here is one that has done service for us repeatedly in a wide range of contexts. The basic idea is to compute (either analytically or numerically) the energies for the putative unstable state and to determine whether in fact there is an energy reduction associated with

464

9 Wall Defects in Solids

Fig. 9.17. Energy as a function of reconstruction amplitude for W(100) reconstruction as computed using angular potentials (adapted from Carlsson (1991)). The ﬁgure reveals the importance of the angular term in stabilizing the reconstruction. The units of δ are measured in a˚ ngstroms.

such an instability. The dynamic analog of this procedure is to consider the growth of the presumed unstable state in time and if the state does grow, then this is seen as evidence of an instability of the reference state. In the present setting, an angular force scheme similar to that presented in section 4.4 was used to examine the energetics of reconstruction. As shown in ﬁg. 9.17, the energetics of this instability may be decomposed into the part emerging from pair terms (E el(2) + Er ep ) and that due to four-body angular terms (E el(4) ). The energy is plotted as a function of the reconstruction amplitude δr ec and reveals a minimum at a nonzero value signaling the propensity for reconstruction. Further, we note that the driving force leading to this reconstruction can be traced to the angular terms. As we have already seen a number of times, empirical calculations can be supplemented and even supplanted by their ﬁrst-principles counterparts. The reconstructions on (001) surfaces have been explained not only on the basis of angular force schemes, but also using density functional theory. In this case, it is a brute force reckoning of the electronic structure and the associated energies that is used to probe the instability toward surface reconstruction. An analog of ﬁg. 9.17 obtained using electronic structure calculations is shown in ﬁg. 9.18. One of the advantages of calculations of this sort is that they can provide insight into the electronic features giving rise to a given phenomenon. In the present context, an intriguing distinction was made between the isoelectronic partners W and Ta, with the insight that emerged being that the propensity for reconstruction could be ascribed to particular structure in the electronic density of states.

9.2 Free Surfaces

465

Fig. 9.18. Energy as a function of reconstruction amplitude as computed using density functional √ theory (adapted from Singh et al. (1986)). The parameter δ is given by δ = δact / 2a0 , where δact is the actual displacement magnitude and a0 is the lattice parameter.

The type of ﬁrst-principles analysis presented above can serve an additional purpose which is tied to the creation of effective theories. In particular, it has been found possible to construct an effective Hamiltonian which represents the energetics of various surface distortions. The perspective adopted here is that the ﬁrst-principles calculations are used to inform the higher-level effective Hamiltonian. Extra importance attaches to the construction of effective Hamiltonians in cases like this since the use of ﬁrst-principles methods by themselves does not allow for a systematic investigation of the ﬁnite temperature aspects of the structural transformation. In particular, in the case of the W(001) surface of interest here, it is of interest to explore the nature of the structural transition at around 210 K. In the present setting, the functional form advanced for the effective Hamiltonian is

1 1 4 1 1 2 4 2 2 Au + Bu i + V4 u i cos(4θi ) + A z (z i − z 0 ) + Vz u i z i Heff = 2 i 4 2 2 i + [J1 ui · u j + K 1 Si j (u i x u j x − u i y u j y ) + R1 [u i x u j x (u i2x + u 2j x ) i j1

+ u i y u j y (u i2y + u 2j y )] +

J2 ui · u j .

(9.13)

i j2

There is a variety of notation associated with this model which includes the use of ui to represent the in-plane displacement of atom i, z i to represent the out-of-

466

9 Wall Defects in Solids

plane displacement of atom i, u i x as the x component of displacement of the i th atom, i jk to denote summing over k th neighbor pairs and the use of a variety of energetic coefﬁcients such as A, B, V4 , A z , Vz , J1 , J2 , R1 and K 1 . In addition, Si j is 1 if sites i and j are displaced from each other in the x-direction and −1 if they are displaced from each other in the y-direction. On the basis of a series of ﬁrst-principles total energy calculations, the various parameters that appear in this effective Hamiltonian can be deduced. An example of a set of calculations used to inform the effective Hamiltonian given above is shown in ﬁg. 9.19. As indicated in the ﬁgure, the basic idea is to carry out a family of distortions for which the energy can be computed ‘exactly’ on the basis of atomistics and approximately on the basis of the effective Hamiltonian. The parameters are then chosen so as to yield an optimal ﬁt to the ‘exact’ results on the basis of the effective Hamiltonian. Just as we saw in the context of phase diagrams (see section 6.5.5), once an effective Hamiltonian has been adopted, it becomes possible to carry out the associated statistical mechanical analysis which makes possible a systematic exploration of the phase diagram associated with that model. In the present case, Roelofs et al. (1989) carried out a series of Monte Carlo calculations on the W(001) surface using the effective Hamiltonian of eqn (9.13), all the while monitoring the diffraction amplitude associated with the superlattice peaks in the diffraction pattern emerging from the c(2 × 2) symmetry. At high temperatures (in fact at temperatures twice those of the observed transition temperature) the diffraction intensity in these satellite peaks was seen to decay, signaling the onset of the transition. The mismatch between observed and computed transition temperatures provides some idea of the challenges that still remain in the construction of material speciﬁc effective Hamiltonians. Case Studies on Semiconductor Surfaces Our discussion in the previous part of this section showed some of the variety associated with surface reconstructions on the surfaces of metals with both the fcc and bcc structures. Just as such surfaces have served as a proving ground for our understanding of metals, semiconductor surface reconstructions have played a similar role in the study of covalent systems. The starting point for the analysis in this section is a synthesis of a wide variety of experimental data in the form of a phase diagram for the Si surfaces. The objective in the remainder of the section will be to try to rationalize, even predict, such phases on the basis of microscopic analysis. Beyond their academic interest to surface science, the reconstructions in Si also impact the nature of the growth processes that occur when atoms are deposited on exposed surfaces.

9.2 Free Surfaces

467

Fig. 9.19. Calculations used in the construction of an effective Hamiltonian for the W(001) surface (adapted from Roelofs et al. (1989)). Panel (a) shows the surface Brillouin zone while panels (b)–(e) show the energy associated with various displacement patterns, with the solid lines corresponding to the energetics of the effective Hamiltonian while the discrete points are the energies associated with ﬁrst-principles total energy calculations.

468

9 Wall Defects in Solids

Fig. 9.20. Series of surface reconstructions associated with Si (adapted from Baski et al. (1997)). The graph depicts the stable planar reconstructions found between the (001) and (111) orientations and gives scanning tunneling microscopy images of the observed surface structures.

Si surface structures. The surfaces of Si present an entirely different set of challenges than do those of the metal surfaces considered thus far. As a prelude to the discussion to follow, we follow Baski et al. (1997) in pictorially representing the various stable planar surfaces between the (001) and (111) orientations as shown in ﬁg. 9.20. One of the key ideas to be conveyed by this ﬁgure is that each of the bold lines corresponds to a stable planar surface, and associated with each such surface is a corresponding scanning tunneling microscopy image of the associated reconstructions. The regions between the stable planar reconstructions are characterized by more complex structures involving steps or facets. For the purposes of the present discussion, we will consider the (001) and (111) surfaces as our representative case studies in semiconductor surface reconstruction. We note that from the point of view of intrinsic complexity, the Si(111) surface is characterized by a large unit cell and hence an intricate arrangement of atoms. The Si(001) Surface. Our analysis begins with perhaps the most studied of such surfaces, namely, the (001) surface. The ideal and reconstructed geometries were presented in ﬁg. 9.10 and are contrasted in more detail in ﬁg. 9.21 where it is noted that the presence of two dangling bonds per surface atom for the ideal bulk termination should provide a strong driving force for structural change. We have already remarked on the analogy between this tendency on the (001) surface and

9.2 Free Surfaces

469

Fig. 9.21. Schematic of the ideal and reconstructed (001) face of Si (adapted from Ramstad et al. (1995)).

that seen at the core of certain dislocations in Si. The presence of dangling bonds like this often manifests itself in structural rearrangements involving dimerization. However, the statement that the surface suffers such a dimerization reaction does not sufﬁce to fully characterize the reconstructed geometry. Though the original LEED (low-energy electron diffraction) experiments indicated the presence of a (2 × 1) symmetry on the reconstructed surface, more recent experiments indicated a phase with (4 × 2) symmetry as well. The presence of a series of such phases, each differing from the other by rather subtle geometric rearrangements poses serious challenges to efforts at modeling these surfaces. In particular, as shown in the ﬁgure (via open and ﬁlled circles for the surface layer) in addition to the lateral displacements related to dimerization, different atoms can suffer different out-of-plane displacements. Indeed, the ﬁlled and open circles correspond to

470

9 Wall Defects in Solids

Fig. 9.22. Comparison of the atomic-level displacements associated with the Si(001) (2 × 1) surface reconstruction as obtained using alternative total energy schemes (adapted from Balamane et al. (1992)). Arrows illustrate the atomic displacements in a˚ ngstroms in comparison with the (1 × 1) reference state. The numbers in each group correspond to the displacements as obtained using density functional theory and Biswas–Hamann, Stillinger–Weber and Tersoff potentials, respectively.

perpendicular displacements either up or down, resulting in a buckling in addition to the dimerization. One theoretical point of departure for examining the surface reconstructions seen on Si(001) is zero-temperature energy minimization using empirical descriptions of the total energy. Two key articles (Balamane et al. 1992, Wilson et al. 1990) have made systematic attempts at characterizing the extent to which empirical total energy schemes can be used to examine the energetics of semiconductor surfaces (as well as other defects). As shown already in ﬁg. 9.10, the distinctive feature of the Si(001) reconstruction is the dimerization of the surface layer atoms. A quantitative assessment of the propensity for such reconstruction as well as its extent is given in ﬁg. 9.22 which shows the computed atomic-level displacements associated with this reconstruction for both the Stillinger–Weber- and Tersoff-type potentials in addition to yet another empirical scheme (the Biswas–Hamann potentials) and the results of a full ﬁrst-principles analysis. The basic point to be made is that while the empirical potentials are unable to account for the subtleties of bond buckling once dimers have formed, the existence of the dimers themselves is well reproduced by the various alternative angular force schemes set forth to account for covalent bonding in semiconductors. In fact, the energy difference between the ideal (1 × 1) surface and the (2 × 1) reconstruction is also reasonably well reproduced.

9.2 Free Surfaces

471

Fig. 9.23. Energies for Si(001) surface. Energy obtained for both ideal and competing reconstructed geometries and illustrating errors (adapted from Ramstad et al. (1995)).

More reliable calculations of the energetic ranking of the various structural competitors on Si(001) have been performed using traditional ﬁrst-principles methods. In particular, a careful zero-temperature analysis has been performed with attention to the errors involved as a result of choice of both k-point sampling and plane wave cutoffs (Ramstad et al. 1995). This work attempts to discriminate between the energetics of the ideal unreconstructed surface and two different (2×1) competitors and the (4 × 2) reconstruction. In ﬁg. 9.23, we show the energy differences associated with the Si(001) reconstruction as well as the error bars associated with these energy differences. In particular, the four panels in the ﬁgure report the energy differences between various structural competitors and give the associated error bars in the calculations. For example, the upper left ﬁgure reports the difference in energy between the bulk terminated (1 × 1) surface and the symmetric dimerized (2 × 1) reconstruction. The label ‘This’ refers to the results from Ramstad et al. while the others (i.e. YC, DS, etc.) refer to the results of calculations of other groups. From a philosophical perspective, it is worth noting that while such calculations are highly tedious and lack glamor, they are also extremely instructive in that through them it is possible to quantify the level of conﬁdence that should be placed in the results. In this case, we see that the error bars associated with the (2 × 2)/(4 × 2) energy difference are so large as to render the result impotent since it was not possible even to conclude the sign of the energy difference. The structure and energetics of the Si(001) surface

472

9 Wall Defects in Solids

provide a series of interesting insights into the nature of surface reconstructions. Indeed, in addition to the simple question of dimerization considered above, there are fascinating issues that arise in conjunction with the presence of vacancies on these surfaces. The Si(111) Surface. As noted already at the beginning of the present subsection, the (111) surface is characterized by a complex (7 × 7) reconstruction which presents signiﬁcant challenges from both an experimental and theoretical point of view. Our current discussion is aimed at examining the structure of this surface in slightly more detail. A schematic depiction of the reconstructed (111) surface is shown in ﬁg. 9.24. The accepted reconstructed surface geometry is known as the dimer adatom stacking fault (DAS) model and is characterized by three distinctive structural features: in particular, the second-layer atoms undergo a dimerization rearrangement, the presence of twelve adatoms in an adatom layer on the surface (the twelve large ﬁlled circles in ﬁg. 9.24) and the existence of a stacking fault over part of the reconstructed area (seen in the left part of the surface cell in ﬁg. 9.24). Just as was possible with the Si(001) surface, a series of comparisons have been made for the energetics of various structural competitors on Si(111) using different total energy schemes. We appeal once again to the careful analysis of Balamane et al. (1992). In this case, the subtlety of the structural rearrangement leads largely to an inability on the part of various empirical schemes to correctly reproduce the energetics of this surface. In particular, as discussed by Balamane et al. (1992), only one of the Tersoff potentials leads to the conclusion that the 7 × 7 reconstruction is stable with respect to the ideal 1 × 1 surface. As a result, as yet the only reliable means whereby one can successfully explore energetic questions concerning these surfaces is through the use of electronic structure-based total energy methods. Surface Reconstructions Reconsidered In the preceding pages we have tried to convey a ﬂavor of the structure and energetics of surface reconstructions. We note that the great advances in this area have been largely experimentally driven and reﬂect the routine atomic-scale resolution that is now enjoyed in the analysis of surface structures. By dividing our analysis along the lines of material type (i.e. metals vs semiconductors) we have been able to contrast the relative merits of different schemes for computing the energetics of crystal surfaces. As a ﬁnal example of some of the exciting developments in considering surfaces, ﬁg. 9.25 shows a surface in amorphous Si with relaxed atomic positions obtained using density functional theory calculations. Now in keeping with our overall theme of examining the departures from the monotony of

9.2 Free Surfaces

473

Fig. 9.24. The 7 × 7 reconstruction of Si(111) in ultrahigh vacuum. Both empty and ﬁlled state constant-current scanning tunneling microscope images are shown for a 14 nm × 14 nm region (adapted from Whitman (1998)). The diamond shaped (7 × 7) unit cell is indicated in the scanning tunneling microscope images. The ﬁgure also gives a schematic of the reconstructed unit cell for both a top and a side view (through the long diagonal) with the topmost atoms largest and darkest. Some of the atoms are labeled to aid correlating the two views.

474

9 Wall Defects in Solids

Fig. 9.25. Surface geometry associated with amorphous Si as computed using density functional theory (courtesy of Martin Bazant and Tim Kaxiras). The surface layer is at the top of the ﬁgure and the atoms colored black are those having ﬁvefold coordination.

Fig. 9.26. Schematic of vicinal surface with low-index terraces bounded by surface steps (adapted from Poon et al. (1992)).

the perfect crystal, we push our analysis of crystal surfaces yet a step further in the form of an examination of steps on crystal surfaces.

9.2.3 Steps on Surfaces Despite our foray into the structure and energetics of surface reconstructions, the class of departures from the perfection of the bulk terminated surface that we have considered is still incomplete. In addition to the relaxations and symmetry breaking reconstructions that are present on surfaces, we must also consider the role of surface steps. Such steps arise from a variety of different sources: the inability to cut a crystal at exactly the face that is desired, the development of steps and islands during the growth process itself and the presence of thermal roughening. Surfaces with a slight misorientation relative to the conventional low-index surfaces are known as vicinal surfaces and are characterized by a series of terraces of the nearby low-index surface, separated by steps which accommodate the overall misorientation. Indeed, the relation between the step height (h), terrace width (lw ) and misorientation can be written as θ ≈ h/lw . A schematic of such a vicinal surface is given in ﬁg. 9.26.

9.2 Free Surfaces

475

Fig. 9.27. Scanning tunneling microscope image, 100 nm × 100 nm, of a stepped Si(001) surface (courtesy of A. Laracuente and L. J. Whitman).

We begin with a consideration of the experimental situation. The advent of scanning tunneling microscopy has made the examination of surface steps routine. In ﬁg. 9.27, we show a representative example of a stepped semiconductor crystal surface. There are a few key observations to be made about these scanning tunneling microscope results. First, we note that the presence of steps is a common occurrence on surfaces. In addition, we note that the morphology of the steps themselves (i.e. smoothly wandering or jagged) poses interesting challenges as well. Our strategy for examining the physics of such steps is to attend to a microscopic description of the energetics of steps. For the Si(001) surface, recall that the surface structure is characterized by dimer pairs. Depending upon which layer in the AB packing along this direction is exposed, these dimers will be oriented parallel to either the x-direction or the y-direction. This effect is indicated schematically in ﬁg. 9.28, where we see that if the surface is exposed on layer A, then the dimerization will occur with one orientation, while if it occurs on layer B, the dimerization will be rotated by 90◦ . This is precisely a schematic of the experimental situation shown in ﬁg. 9.27. The ﬁgure also reveals the presence of these different variants and shows the distinction between the two different step types that occur. The geometry of vicinal surfaces is extremely complex and gives rise to a richness in the series of resulting surface phases that was already foreshadowed in ﬁg. 9.20. In particular, that ﬁgure revealed that as a function of misorientation relative to stable planar surfaces, the surface geometry can range from terraces to facets.

476

9 Wall Defects in Solids

Fig. 9.28. Stepped Si(001) surface and different dimer orientations that result from different layers being exposed (adapted from Alerhand et al. (1990)).

As we have already noted a number of times, the analysis of defects in solids is served both by atomistic and continuum approaches. Like many of the other defects that we have already examined, surface steps are amenable to a description on the basis of atomistic analysis. Microscopic analysis is especially suitable for exploring the short-range contributions of these defects to the total energy that derive from the disruption of the atomic-level geometry at the surface. Without entering into a detailed description of what is involved in computing the energetics of steps, we note that many of the same ideas presented in this and earlier chapters are used. In particular, once a computational cell is in hand, one resorts to a computation of E tot ({Ri }). For our present purposes, we note that microscopic analysis has been invoked in order to carry out a systematic ﬁrst-principles analysis of step energies on metal surfaces as shown in ﬁg. 9.29. We note in closing that we have certainly not done justice to this important topic and a major omission in our discussion has been a failure to report on the continuum theory of surface steps. For a review, the reader is urged to consult Jeong and Williams (1999).

9.3 Stacking Faults and Twins In the previous section we highlighted some of the key issues that arise in considering free surfaces which are themselves one of the key wall defects found in solids. As noted in the introduction, in addition to free surfaces, there are a number of important internal interfaces that are found in solids. Perhaps the lowest-energy class of such internal interfaces are those associated with mistakes

9.3 Stacking Faults and Twins

477

Fig. 9.29. Step energies for 4d transition metals (adapted from Vitos et al. (1999)). The straight lines reﬂect the outcome of a model near-neighbor calculation for the step energies on these surfaces. The ﬁrst-principles calculations were done using the LMTO method.

in the stacking sequences that lead to a given crystal structure. The role of stacking faults as a key player in dislocation core phenomena has already been introduced in section 8.3.2. However, beyond their presence in dislocations, stacking faults can arise in the course of crystal growth, and in some cases form a part of the structural complexity in certain crystal phases. The goal of the current section is to make a deeper examination of the structure and energetics of stacking faults in crystalline materials. 9.3.1 Structure and Energetics of Stacking Faults Geometries of Planar Faults. In chap. 8 we introduced the geometric characteristics of stacking faults. One perspective for characterizing these faults is that they arise as the outcome of rigidly translating an entire set of (111) crystal planes ¯ That with respect to the rest of the crystal by vectors of the form (a0 /2)(211). is, we consider translating the entire half-space above some certain plane by the vector given above. The result is a stacking fault at this plane. Alternatively, these faults may be seen as disruptions in the regular ABCABC arrangement associated with packing of spheres. This perspective is taken up in ﬁg. 9.30. In keeping

478

9 Wall Defects in Solids

Fig. 9.30. Various stacking mistakes associated with (111) close packings (adapted from Rosengaard and Skriver (1993)).

with our earlier discussion concerning the transcription between microscopic and continuum descriptions of interfacial energies, these disruptions in the regular stacking sequence are characterized by an interfacial energy, γ S F . Once again, we see the emergence of a single material parameter which serves to characterize the behavior of materials and which is amenable to microscopic evaluation. We begin ﬁrst with an investigation of the geometric character of the atomiclevel geometry of stacking faults and then turn to the explicit numerical evaluation of their energies. Fig. 9.30 permits a comparative analysis of some of the key stacking fault geometries in fcc crystals. The ﬁrst two schematics illustrate the way in which the fcc and hcp structures can be generated by regular arrangements of either the ABCABC. . . (fcc) or ABABAB. . . (hcp) stacking sequence. The geometrically simplest of the possible faults in the stacking sequence is that of the twin boundary which results from a reversal in order of the stacking sequence and can be induced by a shearing transformation. In addition to the twinning fault introduced above, mistakes in the fcc stacking sequence can also be induced by either adding a plane in the sequence or by removing one. The former case is known as an extrinsic stacking fault and is characterized by a stacking sequence of the form ABCABCBABC. . . . The latter fault is known as an intrinsic fault and is characterized by a stacking sequence of the form ABCBCABC. . . . A systematic discussion of these geometries may be found in chap. 10 of Hirth and Lothe (1992). The ﬁrst geometric question we might pose concerning the stacking fault is how the bond lengths are redistributed by virtue of the presence of this defect. We note that in a perfect fcc crystals the twelve near neighbors of a given atom are associated with the vertices of a cube-octahedron, while the six second neighbors correspond to the vertices of an octahedron. What emerges in comparing the atomic conﬁgurations in the perfect crystal and in a crystal with a stacking fault is the recognition that at the near- and next near-neighbor level, the perfect and faulted

9.3 Stacking Faults and Twins

479

crystals have the same near-neighbor distributions. The details of this geometric analysis are taken up in the problems at the end of the chapter. This geometric fact has energetic consequences that will be taken up below. Energetics of Planar Faults. As shown in the previous chapter, the particulars of the dislocation reactions that will be found in a given material are determined by the numerical values of the relevant interfacial energies (i.e. stacking fault or antiphase boundary energies). One of the dominant philosophical thrusts of the book has been the idea that when it is possible, our aim should be to exploit insights from one level of modeling to inform models at a different scale. In this case, our aim will be to show how insights based upon atomistic calculations of the various interfacial energies can be used as the basis of the type of elasticity calculations that were carried out in the previous chapter in order to determine the dissociation width of dislocations that have undergone splitting reactions and which culminated in eqn (8.74). Our application of the continuum theory of dislocations required an external parameter, namely γ S F , which we now discuss from the perspective of microscopic analysis. Unlike the gross differences between a crystal with and without a free surface, the stacking fault constitutes a less severe perturbation and thereby, generically, has a lower energy than that of a free surface. Our discussion of the bond lengths in faulted regions given above provided a plausibility argument in favor of the relatively low energy of stacking faults in the hierarchy of interfacial defects. Both empirical and ﬁrst-principles methods have been used to evaluate stacking fault energies in crystals. For the purposes of numerical evaluation of the stacking fault energy, we must ﬁrst insure that the stacking fault itself is embedded in a box that is sufﬁciently large so as to mimic the presence of a stacking fault in an inﬁnite crystal. We will ﬁrst give an overview of how the stacking fault energy may be computed within the conﬁnes of empirical energy functionals, and will close our discussion with a representative example from the use of ﬁrst-principles methods for computing the stacking fault energy. Regardless of the choice of energy functional, the type of computational box that is used to evaluate the stacking fault energy is shown schematically in ﬁg. 9.31. The key elements of the simulation box are, evidently, the presence of the stacking fault itself, and the presence of a sufﬁcient distance between the stacking fault and the distant free surfaces, or periodic boundaries. Once the simulation box has been established, it is a routine matter to compute the stacking fault energy itself. The stacking fault energy may be computed on the basis of a generic total energy scheme according to E N (S F) − E N (bulk) . (9.14) γS F = A

480

9 Wall Defects in Solids

Fig. 9.31. Computational box used to compute the energy of an intrinsic stacking fault in Al (adapted from Wright et al. (1992)).

As with the surface energy as deﬁned in eqn (9.5), the stacking fault energy is obtained by computing the energy of two different N -atom conﬁgurations, one corresponding to the perfect crystal and the other corresponding to the N -atom supercell within which is a stacking fault. In practice, once the computational cell is in hand, the energy difference called for above can be evaluated in exactly the same way that we obtained the vacancy formation and surface energies earlier. From the perspective of a pair potential description of the total energy and in the context of the geometric distributions of neighbor environments shown above, the evaluation of stacking fault energies becomes an exercise in delicate choices about the long-range part of the potential of interest. As has been seen in earlier chapters, the introduction of higher-order terms in the energy functional can improve the pair potential treatment substantially. We note that in the case of stacking faults, even pair functionals are relatively ineffective at reproducing the energetics of stacking faults, suffering from routine underestimates of the stacking fault energy which lead in turn to unreasonably large dissociations for dislocations. On the

9.3 Stacking Faults and Twins

481

other hand, these results can be improved by incorporating angular terms in the energy functional. An example of the type of results that have been obtained in the empirical setting is shown in ﬁg. 9.32. The key idea being presented here is that the stacking fault energy can be thought of as being built up of both pair and four-body contributions. In particular, the total energy is written in the form E tot = E pair + E 4-body , where the four-body term is of the form ( f cc) α(µ(i) ). E 4-body = 4 − µ4

(9.15)

(9.16)

i

The four-body term is an application of exactly the ideas introduced in section 4.5.3 and culminating in eqn (4.95). Fig. 9.32 shows the relative contributions of different atoms in the faulted region to the overall fault energy. In particular, for a series of different metals the overall contribution to the stacking fault energy is decomposed layer by layer and each such contribution is itself decomposed into the relative contributions of the pair and four-body terms. The computation of stacking fault energies from ﬁrst principles is a more delicate matter. There are tedious questions that arise concerning convergence with respect to box size, energetic cutoffs and k-point sampling. Again, since we have repeatedly described the essential conceptual steps involved in carrying out a total energy calculation, we note here that the calculation of stacking fault energies involves the same basic elements such as building an appropriate computational cell, etc. An example of the types of results that emerge from these calculations is shown in ﬁg. 9.33. As was done in ﬁg. 9.32 (a calculation which was itself inspired by the present one) the stacking fault energies are decomposed into the contributions of the different layers in the faulted region. A rough rule of thumb which is substantiated by these calculations can be written in the form ≈ γ Sextrinsic ≈ 2γ Stwin γ Sintrinsic F F F .

(9.17)

Just as was found possible in the context of alloy phase diagrammatics and in the evaluation of surface energies, it is possible to exploit atomic-level calculations as the basis of effective Hamiltonians describing the energetics of stacking faults. Once again, the calculations are made on the basis of an Ising-like model of the stacking fault. Our development follows that of Hammer et al. (1992) in which the energy of a crystal with a stacking fault is written as E = ξ0 −

1

n max N atoms

Natoms

n=1 i=1

Jn σi σi+n .

(9.18)

The parameters Jn are the effective Ising parameters that are determined from

482

9 Wall Defects in Solids

Fig. 9.32. Systematics of stacking fault energy in different metals as computed using multiatom interactions (adapted from Stokbro and Jacobsen (1993)).

atomic-level analysis. The notation is such that σi = 1 if the atom in layer i + 1 maintains the integrity of ABC stacking whereas σi = −1 if the atom in layer i + 1 is part of CBA stacking. For example, if the i th layer is of C-type and the following layer is an A-type, then σi = 1. By way of contrast, if the i th layer is of the type C and the following layer in the stacking sequence is of the B-type, then σi = −1. To make the correspondence more concrete, the sequence ABCABCBABC, corresponding to an extrinsic stacking fault leads to

9.3 Stacking Faults and Twins

483

Fig. 9.33. Systematics of stacking fault energy in different metals as computed using ﬁrst-principles total energy methods (adapted from Crampin et al. (1990)).

the transcription ABCABCBABC = 1 1 1 1 1 −1 −1 1 1 1.

(9.19)

To compute the stacking fault energy, we must evaluate E = E faulted (N layers) − E perfect (N layers). For the extrinsic case given above only four layers (i.e. 1 1 −1 −1 have contributions that are different from the perfect crystal contribu-

484

9 Wall Defects in Solids

Fig. 9.34. Schematic of several polytypes occurring in SiC (adapted from K¨ackell et al. (1994)). Each polytype represents a different stacking of A, B and C layers.

tions, so the energy difference is of the form E = [−J1 + J2 + J1 + J2 − J1 + J2 + J1 + J2 ]−4(−J1 − J2 ) = 4J1 +8J2 . (9.20) The terms in square brackets come in pairs involving J1 and J2 correspond to working from left to right while the term involving 4(−J1 − J2 ) is the energy of four layers worth of perfect lattice on the assumption of one atom per layer. The use of these ideas is ﬂeshed out in problem 5 at the end of the present chapter. Once this effective Hamiltonian is in hand, it is possible to begin considering the distribution of such faults in crystals. One particularly interesting venue within which planar faults arise is in the context of some of the complex structures that arise in alloys. 9.3.2 Planar Faults and Phase Diagrams As noted above, stacking defects are relevant in the context of the phase diagrammatics of complex alloys. In this setting, there are a range of polytypes that a particular material may adopt depending upon the tuning of some control parameter such as the temperature or the chemical composition. For our present purposes, such polytpes represent different structural variants in which the regular packing of planes along a particular direction is disturbed relative to the stacking in some reference state. These mistakes in packing correspond in the fcc case to exactly the sort of stacking faults that have entered our discussion thus far. Example of

9.3 Stacking Faults and Twins

485

Fig. 9.35. Schematic of the different polytypic phases found in SiC (adapted from Trigunayat (1991)).

the types of structural rearrangements that occur in the SiC system are shown in ﬁg. 9.34. In addition, ﬁg. 9.35 gives a schematic indication of the stability ranges of the various structures. In addition to its importance in the type of covalent systems described above, the phenomenon of polytypism is also found in intermetallics. For example, in ﬁg. 9.36, we show a schematic rendering of the various structure types found in a series of Mg-based ternary alloys such as Mg(Znx Ag1−x )2 and Mg(Cux Al1−x )2 . The basic idea is that by varying x, and hence the proportions of the elements in the alloy, the mean electron/atom ratio (denoted as z in the ﬁgure) for the alloy can be altered. This ﬁgure reveals that depending upon the value of z, a whole range of different stacking sequences emerge. The notation presented in the ﬁgure is such that a given layer is labeled with an h if the two adjacent layers are of the same type and a given layer is labeled c otherwise. For example, the hcp structure (ABABABA. . . ) would be labeled as hhhhh. . . since every layer is such that the two adjacent layers are identical (i.e. A is sandwiched between two Bs and vice versa). The fcc structure, on the other hand, characterized by a stacking sequence ABCABC. . . , would be denoted as cccccc. . . in this notation since the two layers adjacent to a given layer are never the same. As shown in the ﬁgure, for the more complex case of interest here, different values of z, the electron per atom ratio (which is another way of saying for different compositions), the resulting stacking sequence will be a different arrangement of h and c layers. For our present purposes, all that we really aim to take away from this ﬁgure is a sense

486

9 Wall Defects in Solids

Fig. 9.36. Series of stable stacking sequences in Mg-based Laves phases as a function of the electron per atom ratio, z (Bruinsma and Zangwill 1985).

of the diversity of structural types that can be thought of from the ‘stacking fault’ perspective and to note the way in which control parameters such as the electron per atom ratio can govern structural stability. The emergence of the types of polytypes described above may be rationalized on the basis of a variety of different ideas. Rather than exploring the phenomenon of polytypism in detail, we give a schematic indication of one approach that has been used and which is nearly identical in spirit to the effective Hamiltonian already introduced in the context of stacking fault energies (see eqn (9.18)). In particular, we make reference to the so-called ANNNI (axial next-nearest-neighbor Ising) model which has a Hamiltonian of the form H = E0 −

1 1 J1 σi σi±1 − J2 σi σi±2 . 2 2 i i

(9.21)

The basic idea is to represent the energy of a given stacking sequence in terms of effective Ising parameters. The relative importance of ﬁrst (J1 ) and second (J2 ) neighbor interactions gives rise to a competition that can stabilize long-period

9.4 Grain Boundaries

487

10

∆E (meV)

5

0

SiC

ZnS

Si

Fig. 9.37. Ranking of structural energies associated with different polytypes using the Ising-like effective Hamiltonian described in the text (adapted from Engel and Needs (1990)).

equilibrium states. In particular, this competition is especially relevant in the case in which the magnitudes of the two terms are nearly equal and their signs are opposite. From the standpoint of the analysis of this model there are two different considerations. First, it is necessary to inform the effective Hamiltonian on the basis of atomic-level analysis. Secondly, the representation of polytypic energies in terms of an Ising parameterization like that described above opens up the possibility for a statistical mechanics analysis of the temperature dependence of phases. A representation of the ranking of polytype energies in three different material systems is shown in ﬁg. 9.37. In each of these cases, the energies shown in the ﬁgure are based upon the effective Hamiltonian, with the parameters in that Hamiltonian ﬁt on the basis of a ﬁrst-principles analysis of the total energy.

9.4 Grain Boundaries One of the dominant themes upon which much of our analysis has been predicated is the idea that a solid is populated by structures at many different scales. At the most fundamental level, a crystal may be thought of as an uninterrupted arrangement of atoms according to the simple decomposition Rm 1 ,m 2 ,m 3 = m 1 e1 + m 2 e2 + m 3 e3 ,

(9.22)

488

9 Wall Defects in Solids

where m i is a member of the integers, ei is a Bravais lattice vector and R(m 1 , m 2 , m 3 ) is the position of the lattice point indexed by the triplet (m 1 , m 2 , m 3 ). Here we are imagining the simplest of crystals in which there is only one atom per unit cell. At the next level of structure, we imagine this perfect regularity to be disturbed both by a distribution of point defects such as vacancies and interstitials as well as by arrangements of dislocations and possibly also by their attendant stacking faults. At even larger scales (i.e. the micron scale), there is yet another level of structure, namely, that of the multiple grains that make up a typical crystalline solid. Different regions within the crystal are tied to different orientations of the same fundamental Bravais lattice. These grains are bounded by interfacial defects known as grain boundaries which serve as an integral part of the geometry of crystalline solids and it is the business of the present section to examine the structure and energetics of such boundaries from the perspective of models of material behavior. As a reminder of the way interfaces, as key microstructural elements, can impact material response, we note one of the celebrated relations between a material’s microstructure and its physical response, namely, the Hall–Petch relation which holds that the yield strength of a material scales as 1

σ y = σ0 + kd − 2 ,

(9.23)

where d is the average ‘grain size’ and k and σ0 are constants. We have already exhibited pictorial evidence for this effect in ﬁgs. 1.3 and 8.2(c). We have elected to surround grain size in quotes as a reminder that despite the ease with which those words are used in everyday conversation in discussing materials, the geometric characterization of microstructure is subtle. Our reason for calling attention to the Hall–Petch relation is to anticipate some of the questions that are tied to the existence of grain boundaries. In the long history of efforts to piece together the connection between a material’s microstructure and its properties, one series of arguments has been built around a reductionist perspective. In these arguments, it is held that by building up an appropriate understanding of a single grain boundary perhaps it will be possible to bootstrap these insights to an analysis of microstructures themselves. As a result, not only has there been considerable effort in trying to ferret out the implications of polycrystalline structure on properties, but a great deal of effort has gone into examining the deformation and fracture of bicrystals. An entire hierarchy of geometric structures involving grain boundaries can be considered as illustrated in ﬁg. 9.38. As is evidenced by ﬁg. 9.38, there are a number of points of entry into a discussion of polycrystalline microstructures. In particular, ﬁg. 9.38 shows that at the simplest level (frame (a)) we can consider bicrystal geometries. In keeping with

9.4 Grain Boundaries

489

Fig. 9.38. Schematic of increasingly complex grain boundary distributions within materials (adapted from Randle (1994)): (a) bicrystal geometry with a single grain boundary, (b) bamboo-like distribution of grain boundaries in a one-dimensional array, (c) polycrystalline ﬁlm, and (d) three-dimensional polycrystal.

that suggestion and as a preliminary to investigating the physics of polycrystals, we begin by examining the geometry of bicrystals with an eye to examining such geometries from both a microscopic and continuum perspective.

9.4.1 Bicrystal Geometry In this section, we begin with consideration of the fundamental geometric degrees of freedom that characterize bicrystals and then turn to the descriptions of the structures themselves. The reference geometry around which the discussion of grain boundaries acquires meaning is the perfect lattice of eqn (9.22). Denote the Bravais lattice vectors of the ﬁrst grain by ei(1) , where 1 is a label denoting this grain, and the subscript ranges from one to three and labels the three linearly independent Bravais lattice vectors characterizing the crystalline state. The basic

490

9 Wall Defects in Solids

Fig. 9.39. Interpenetrating lattices used to consider grain boundary structure (courtesy of D. Pawaskar). Open and ﬁlled circles correspond to the two host lattices and ﬁlled squares correspond to those atoms that are common to both lattices (i.e. the lattice of coincident sites).

idea for describing the grain boundary structure is embodied in two fundamental geometric notions. First, we must characterize the orientation of the second grain with respect to the ﬁrst. Having done this, the boundary itself is not fully determined since we must also say which plane serves as the dividing surface between the two grains. Together, these two geometric descriptors, the relative orientations of the two grains and the identiﬁcation of the boundary plane, serve to completely specify the macroscopic grain boundary geometry. We now set ourselves the task of casting these geometric questions in a proper mathematical light. We begin by imagining ﬁlling space with two interpenetrating lattices, both built around the same Bravais lattice type, but with different orientations, and possibly a different overall origin. In particular, if we are given the two sets of Bravais lattice vectors, their relative orientations are connected via a rotation matrix Q by ei(2) = Qi j e(1) j .

(9.24)

In addition, as was mentioned above, it is possible that there is a shift of origin associated with some translation vector τ . The matrix Q imposes a linear transformation which, since it describes a rotation, may be characterized by three parameters. We now have two interpenetrating lattices as indicated in the simpliﬁed two-dimensional setting in ﬁg. 9.39. As yet, there is no grain boundary. The remainder of our work in identifying the macroscopic degrees of freedom is to select the boundary plane itself. This plane is characterized by a unit vector n

9.4 Grain Boundaries

491

Fig. 9.40. Schematic of degrees of freedom associated with choice of boundary plane (adapted from Wolf et al. (1992)). This ﬁgure illustrates the idea that once the relative orientation of the two grains has been chosen there is still a freedom to choose the grain boundary plane.

which can be identiﬁed by two additional degrees of freedom. The choice of boundary plane is illustrated in ﬁg. 9.40. We now imagine a shaving operation in which only one group of atoms is retained on each side of the boundary. For example, we might elect to keep those atoms associated with the Bravais lattice set ei(1) on one side and those from the other Bravais lattice set on the other side of the boundary. What we have learned is that with the speciﬁcation of ﬁve macroscopic degrees of freedom, the overall character of the boundary may be speciﬁed. For the special case in which the rotation axis is contained within the boundary plane, such a boundary is known as a tilt boundary, while for the other special case in which the rotation axis is perpendicular to the boundary plane, one speaks of a twist boundary. Just as the most generic dislocations are neither pure edge or pure screw, the generic grain boundary is neither pure tilt nor pure twist.

492

9 Wall Defects in Solids

The description of grain boundary geometry as given above is somewhat deceptive. In addition to the overall macroscopic descriptors of that boundary, there are also microscopic features that may be assigned to such boundaries. For example, even though we have selected the relative orientations and the boundary plane, it is possible that the two grains may have also suffered a relative translation. As will be seen in subsequent sections, the search for the particular energy minimizing translation is a tedious but important step in the analysis of grain boundary structure. Bicrystallography has been dominated by the analysis of special boundaries in which symmetry plays a pivotal role. In particular, the geometry of those boundaries with a high degree of symmetry is most easily captured through an appeal to certain important classiﬁcation schemes, such as that of the coincident site lattice (CSL). The qualitative idea behind this classiﬁcation is the insight that for certain choices of rotation matrix Q, there will be a fraction of the sites that are common to both lattices. The fraction of such overlapping sites serves as a measure of the boundary symmetry. This lattice of overlapping sites is known as the coincident site lattice. From a quantitative perspective, this degree of overlap of the two lattices is characterized by the ' number. To compute this number, we ﬁnd what fraction of the sites from a given lattice are coincident with those of the other. The reciprocal of this number is the ' number. For example, if one in every ﬁve sites is coincident, this would be referred to as a '5 boundary, precisely the case shown in ﬁg. 9.41. An example of a set of coincident site lattices is shown in ﬁg. 9.41. Interestingly, even in those cases in which a tilt boundary has relatively little symmetry, the boundary structure may be thought of as a limiting case in which the coincident site lattice has a very high ' number, where we note again that this number is deﬁned such that 1/' of the sites on a given lattice are common.

9.4.2 Grain Boundaries in Polycrystals In light of our characterization of the structures of individual grain boundaries, it is important to now undertake the statistical question of what the distribution of grain boundaries is like in real polycrystals. We have already noted that the important role of bicrystals was born of a reductionistic instinct in which it was argued that proper understanding of the structure and energetics of single boundaries must precede a fundamental understanding of the consequences of an assembly of such boundaries. Our task in the present section is to examine the geometric character of real polycrystals, paying special attention to the distribution of different boundary types within polycrystals. We have already seen that boundaries of high symmetry have been the workhorse of most research in examining the structure and energetics

9.4 Grain Boundaries

493

Fig. 9.41. Schematic of several representative grain boundaries with structures described by coincident site lattice model. This set of boundaries corresponds to a (001) rotation axis, and the atomic-level geometries have not been relaxed (courtesy of D. Pawaskar). The ﬁlled circles correspond to those sites (coincident sites) that are common to both lattices.

of grain boundaries. This raises the question of to what extent such boundaries are representative of those found in real microstructures. As pointed out in Randle (1997), there are two aspects to the statistics of grain boundary distributions. On the one hand, the question of how different grains are misoriented can be posed. This leads in turn to an analysis of the distribution of various coincident site lattice types. By way of contrast, it is also important to obtain quantitative insights into the distribution of grain boundary planes. Indeed, the character of the grain boundary plane is critically related to the nature of the underlying grain boundary structure. As a ﬁrst exercise in the statistics of grain boundaries, ﬁg. 9.42 shows the distribution of ' boundaries for an Fe–Si alloy. In this case, it is the relative frequency of different misorientations that is being reported. An example of this type of statistical distribution with regard to the boundary plane is shown in ﬁg. 9.43. In particular, this ﬁgure reveals the distribution of

494

9 Wall Defects in Solids

Fig. 9.42. Frequency of various coincident boundaries as a function of the ' number (adapted from Watanabe (1989)). The data are for a fully annealed Fe–6.5 wt% Si alloy. The two distributions (different color histograms) correspond to samples with different textures.

grain boundary plane types in annealed high purity Cu and Ni. All of the reported boundaries are for the same underlying crystal misorientation and correspond to '3 boundaries. The numbers on the left hand axis of the ﬁgure give the orientation of the grain boundary plane. Our intent in this section was not to give an exhaustive account of the nature of grain boundaries in real polycrystals. Rather, it was meant as a gentle reminder that despite the importance of bicrystals, they are but a ﬁrst step in understanding the deeper question of the nature of grain boundaries in real microstructures.

9.4.3 Energetic Description of Grain Boundaries We now take up the issue of how one goes about using microscopic calculation to determine grain boundary structure and energetics. The principles of these calculations will be essentially independent of whether or not empirical or ﬁrstprinciples schemes are adopted. However, the goodness of the results will clearly be inﬂuenced by that choice. As a preliminary, we recall the transcription between the microscopic and continuum description of grain boundary energies. As was noted in eqn (9.4), the introduction of interfacial energies in a continuum setting is effected via a scalar parameter (i.e. γsurf , γ S F or γG B ) which has a dependence on crystallographic features such as the interfacial normal and the relative orientations of adjacent grains in the case of grain boundaries. For grain boundaries, as

9.4 Grain Boundaries

495

Fig. 9.43. Distribution of grain boundaries in polycrystals (adapted from Randle (1997)). The numbers on the vertical axis refer to the coordinates of the boundary plane, while ATGB and TWGB refer to the asymmetric tilt boundaries and twist boundaries, respectively.

for surfaces and stacking faults, the transcription between the microscopic and continuum notions is based upon γG B =

E N (G B) − E N (bulk) . A

(9.25)

As with our previous treatments of interfacial energy, the fundamental idea is to make a comparison between an N -atom state in which all of the atoms are in their ideal bulk positions and an N -atom state in which the interface of interest is present. As an example of the type of supercell that can be used in this analysis, ﬁg. 9.44 shows a scheme in which the grain boundary is at the interior of a cell whose outer boundaries perpendicular to the boundary are treated as rigid slabs. In this case, the forces on the atoms in the region being relaxed are computed in exactly the

496

9 Wall Defects in Solids

Fig. 9.44. Schematic of the type of computational cell used in computing the energy of a grain boundary.

manner already emphasized repeatedly in the book, and the atoms are subsequently relaxed. Our thinking for the remainder of this section is to examine a few different case studies in grain boundary structure with the aim of seeing both how such calculations are done, and what can be learned from them. Semiempirical determination of grain boundary structure and energetics. Simple grain boundaries in metals have been exhaustively considered from the standpoint of empirical descriptions of the total energy. The logic of much of this work is founded on the contention that prior to understanding the susceptibility of boundaries to segregation and fracture or their role as short-circuit paths for diffusion, it is necessary to ﬁrst understand the structures themselves. The majority of this work has emphasized bicrystals. A series of studies in Ni have been made for tilt boundaries that elucidate the role of misorientation in boundary structure. The case study of interest to our present discussion (Rittner and Seidman 1996) involved the use of a pair functional description of the total energy to investigate 21 distinct symmetric tilt boundaries with a 110 tilt axis. Representative examples of the relaxed structures are shown in ﬁg. 9.45 and the corresponding grain boundary energies are shown in ﬁg. 9.46. One of the most important points of contact between models like those described above and experiment is the use of transmission electron microscopy to examine grain boundaries. In particular, there is a well-established tradition of effecting direct comparisons between the outcome of a given atomic-level simulation of

9.4 Grain Boundaries

497

Fig. 9.45. Series of grain boundary structures for 110 symmetric tilt boundaries as computed using a pair functional description of the total energy (adapted from Rittner and Seidman (1996)).

grain boundary structure and the corresponding images obtained on the basis of high-resolution transmission electron microscopy (HRTEM). The way such comparisons are effected is by taking the results of the atomic-level calculation and using them as input for image simulation tools which compute the nature of the high-resolution transmission electron microscopy image that would be expected on the basis of that collection of atoms. An example of this strategy is illustrated in ﬁg. 9.47 which shows the atomic-level structure for a tilt boundary in Al.

498

9 Wall Defects in Solids

Fig. 9.46. Grain boundary energy as a function of tilt angle for 110 symmetric tilt boundaries (adapted from Rittner and Seidman (1996)).

Fig. 9.47. Comparison of high-resolution images of a grain boundary with structures obtained from atomistic simulation (adapted from Mills (1993)).

First-principles determinations of grain boundary structure and energetics. We have repeatedly emphasized the complementary (and sometimes antagonistic) role of empirical and ﬁrst-principles calculations of the many structures that inhabit materials. The structure and energy of grain boundaries is clearly yet another defect

9.4 Grain Boundaries

499

Fig. 9.48. Computational cell used for computing energetics of '11 grain boundary in aluminum (adapted from Wright and Atlas (1994)). The numbering of atoms was used in the original work in order to describe electron densities. Atoms in different layers normal to the page (i.e. along the [110] direction) are shown with open and ﬁlled circles.

that is amenable to treatment within the ﬁrst-principles setting. The analysis is predicated on the creation of a computational cell of the sort shown in ﬁg. 9.48. In this case, a high-symmetry grain boundary in Al is of interest. All of the usual machinery is exploited in the usual way (i.e. periodic boundary conditions, computing energies and forces, structural relaxation), with the result that it is possible to obtain insights into the structure and energetics of grain boundaries with ﬁrst-principles accuracy. One of the interesting insights to emerge from the ﬁrst-principles calculations highlighted in ﬁg. 9.48 is that though there is reasonable accord between the structures obtained using ﬁrst-principles techniques and those using pair functionals to examine the same boundary, the grain boundary energies are underestimated in the pair functional calculations by a factor of the order of 2. The intent of the present section was to demonstrate that just as was the case in the context of point defects such as vacancies and interstitials and line defects such as dislocations, it is possible to bring a variety of microscopic methods to bear on the question of grain boundary structure and energetics. At this late stage in the book, the basic ideas behind such structural simulations have been illustrated repeatedly with the result that our discussion has aimed only to highlight via the device of case studies, the results of such calculations.

500

9 Wall Defects in Solids

Fig. 9.49. Schematic of grain boundary triple junction.

9.4.4 Triple Junctions of Grain Boundaries As we will discuss in chap. 10, the consideration of polycrystals demands an analysis not only of the grain boundaries that separate different grains, but also of the points at which several different boundaries intersect. The simplest model of a triple junction is of the type indicated schematically in ﬁg. 9.49. For our present purposes, the basic idea is to determine a condition for the stability of such triple junctions which will at once determine both the structure and energetics of these triple points. For the geometry considered in ﬁg. 9.49, we imagine three separate segments of grain boundary, all pinned at their extremeties as shown. Our aim is to write the total energy as a function of the as-yet undetermined position x. Once this energy has been set forth, we then minimize the energy with respect to the parameter x resulting in a condition for the optimal geometry. Before illustrating the details, we note that the calculation envisaged here constrains the class of possible triplejunction geometries and that a more general treatment requires an analysis of the variation in energy for both x and y displacement of the triple point. The more general calculation is considered in the problem section at the end of this chapter. The energy of the triple junction may be written by adding up the energy γ l which results from each interfacial segment of length l. Note that this calculation is the interfacial analog of the line tension calculations used to characterize the energetics of dislocations in the previous chapter. For the particular geometry of interest here, the energy may be written as (9.26) E(x) = γ x + 2γ h 2 + (d − x)2 ,

9.5 Diffuse Interfaces

501

where the ﬁrst term is the energy associated with the horizontal segment, while the second term is that associated with the two interfacial segments that are oriented at an angle φ = θ1 /2 with respect to the horizontal. Differentiation of this energy with respect to x provides us with the equilibrium condition which is

d−x

1 = . 2 h 2 + (d − x)2

(9.27)

Further, we note that the expression on the left hand side of this equation is nothing more than cos φ, resulting in the conclusion that the equilibrium angle is φ = θ1 /2 = 60◦ . This relatively simple calculation is aimed at illustrating the way in which energy minimization arguments may be used to deduce the structure and energetics of triple points which are yet another ingredient in our overall collection of defects used to build up material microstructures.

9.5 Diffuse Interfaces Our thinking on the treatment of interfaces has been largely inspired by atomiclevel understanding. In particular, we have acceded to the atomistically motivated picture of an interface as a sharp line of demarcation between distinct regions. On the other hand, as will become more evident in the next and subsequent chapters, there are advantages to adopting a continuum view of interfaces as regions over which certain continuum ﬁeld variables suffer rapid spatial variations. This idea will serve as the basis for the general class of phase ﬁeld models that have been used in settings ranging from the analysis of grain growth to the patterns that arise during the process of solidiﬁcation. To be concrete, though not detailed, we consider the case of a two-phase microstructure in which two distinct crystalline phases coexist. One way of characterizing the state of such a system is by recourse to an ‘order parameter’ ﬁeld which we denote η(x). Imagine that within one of the phases, this order parameter takes the value 1, while in the other phase it is assigned a value 0. The phase ﬁeld treatment of interfaces is indicated schematically in a simpliﬁed one-dimensional form in ﬁg. 9.50. What we note is that there are three distinct regions. First, there is a region in which η(x) = 1, second a region over which η(x) = 0 and most importantly for the purposes of the present discussion, there is a region over which the ﬁeld η(x) is making the transition from η(x) = 1 to η(x) = 0. Though we cannot necessarily assign a precise location to the interface, we can say that the interface occupies that region over which dη(x)/d x = 0. The discussion given above illustrates how the question of ‘structure’ at interfaces is handled within the phase ﬁeld setting. In addition to these structural questions, the phase ﬁeld concept allows for a treatment of interfacial energetics.

502

9 Wall Defects in Solids

Fig. 9.50. Schematic representation of the use of continuous ﬁelds to represent grain boundaries. In particular, the interfacial region is characterized by gradients in the order parameter η.

In particular, again in keeping with the simpliﬁed one-dimensional framework suggested above, these can ideas can be endowed with an energetic interpretation by introducing an energetics of the form E[η(x)] =

dη κ dx

2 d x.

(9.28)

This functional introduces an energetic penalty associated with those parts of the distribution of η(x) involving gradients. The parameter κ is a material parameter that characterizes the severity of the penalty associated with a given interface. The energy functional given in eqn (9.28) is a simpliﬁed version of one of the key terms in the overall free energy functional that is used in the derivation of the so-called Cahn–Hilliard equation which will be taken up in chap. 12. We note that the present section has only sketched some of the key ingredients in the phase ﬁeld approach to modeling interfaces and that a detailed description of these ideas will have to await later chapters.

9.6 Modeling Interfaces: A Retrospective This chapter has argued for the critical role of interfacial defects in solids. We have favored an artiﬁcial classiﬁcation into three primary types of interfacial defects, namely, surfaces, stacking faults and twins, and grain boundaries. In each of these cases, it has been argued that a continuum description of the energetics of such

9.7 Further Reading

interfaces may be marshaled through an appeal to equations of the form γ (n)d S, E int =

503

(9.29)

∂

where γ (n) is a generic interfacial energy which depends upon the particular interfacial plane. As evidenced by the various discussions throughout the present chapter, despite the seeming innocence of introducing quantities such as γ (n), the structure and energetics of interfaces is a complex problem when viewed from the atomic scale. In retrospect, it is clear that the energetics of the three different interfacial types considered here can be grouped. In particular, we have found an energetic ranking of the form γsurf > γgb > γ S F .

(9.30)

Ultimately, this ranking of energies could be rationalized on the basis of bond counting arguments in which we examine the extent to which atoms in the interfacial region have lost their partners. 9.7 Further Reading Generalities on Interfaces The Physics of Low-Dimensional Semiconductors by John H. Davies, Cambridge University Press, Cambridge: England, 1998. Chapter 4 of Davies’ book considers the properties of quantum wells and elaborates on some of the arguments concerning conﬁnement given earlier in the present chapter. Surfaces The literature on surface science is vast, and well represented in a number of different books and review articles. Here I give a few that have been most useful or enjoyable to me. Physics at Surfaces by A. Zangwill, Cambridge University Press, Cambridge: England, 1988. Zangwill’s book is thoughtfully constructed and wide in its coverage. He passes freely between questions of geometrical and electronic structure, the adsorption of atoms at free surface and the properties implied by the presence of surfaces. ‘Surface Reconstructions’ by D. King, in Physics World, 2, 45 (1989). This brief article is characterized by plain English and excellent pictures that take the reader right to the crux of the geometries that attend surface reconstruction. ‘Reconstructions and Relaxations on Metal Surfaces’ by J. E. Inglesﬁeld, in Prog. Surf. Sci., 20, 105 (1985). By now this article is somewhat dated, but still

504

9 Wall Defects in Solids

gives an introduction to issues faced in considering the reconstructions on Au, Pt and W surfaces. Inglesﬁeld’s article can be contrasted with ‘Scanning tunneling microscopy studies of metal surfaces’ by F. Besenbacher, in Rep. Prog. Phys., 59, 1737 (1996). This article is full of beautiful pictures substantiating our claim that the scanning tunneling microscope has revolutionized our knowledge of surface structure. Two complementary articles related to semiconductor surfaces are ‘Scanning tunnelling microscopy of semiconductor surfaces’ by H. Neddermeyer, in Rep. Prog. Phys., 59, 701 (1996) and ‘Theory of semiconductor surface reconstruction’ by G. P. Srivastava, in Rep. Prog. Phys., 60, 561 (1997). The article on scanning tunneling microscopy applied to semiconductor surfaces is replete with pictures of some of the huge variety of surfaces that have been considered in semiconductor systems. Physics of Crystal Growth by A. Pimpinelli and J. Villain, Cambridge University Press, Cambridge: England, 1998. This book is included here because it has an interesting discussion both of surface reconstructions and, more importantly, of the elastic theory of interactions between steps. Grain Boundaries Interfaces in Crystalline Materials by A. P. Sutton and R. W. Ballufﬁ, Oxford University Press, Oxford: England, 1995. An enormous compendium with broad coverage on interfacial structure, energetics, deformation, segregation and everything else. This book should be seen as doing for the study of interfaces what Hirth and Lothe (1992) did for the study of dislocations. This is the reference on interfaces. Materials Interfaces edited by D. Wolf and S. Yip, Chapman Hall, London: England, 1992. This book is a compilation consisting of articles by leading practitioners on all aspects of interfaces in solids. ‘The Inﬂuence of Grain Boundaries on Mechanical Properties’ by J. P. Hirth, Met. Trans., 3, 3047 (1972). Hirth offers a variety of insights on the role of grain boundaries in dictating mechanical properties. Miscellaneous Fractography – Observing, Measuring and Interpreting Fracture Surface Topography by Derek Hull, Cambridge University Press, Cambridge: England, 1999. Hull’s book is excellent whatever criterion is used to judge it. I include it here since fracture surfaces are another type of interface that emerges in considering solids.

9.8 Problems

505

9.8 Problems

1 Energetics of fcc Surfaces Using Pair Potentials In eqn (9.6) we revealed the surface energy for an fcc (100) surface in the near-neighbor pair potential approximation. Deduce analogous results for the (110) and (111) fcc surfaces.

2 Energetics of Surfaces Using Pair Functionals Use the Johnson embedded-atom analysis to compute the energies of the (111) and (110) surfaces in fcc materials. Carry out a ranking of the relative magnitudes of the (100), (110) and (111) surfaces using these potentials.

3 Energetics of Surfaces Using Stillinger–Weber Potentials Compute the energy of the unrelaxed and unreconstructed (100) surface in Si. Next, use either static energy minimization or molecular dynamics to relax this surface and examine the resulting reconstruction.

4 Geometry and energetics of stacking faults In this problem, you will investigate the geometry and energetics of stacking faults in fcc crystals. (a) Construct a histogram which shows the number of neighbors that a given atom has as a function of distance to these neighbors. ˚ Identify all neighbor First, make such a plot for fcc Cu (a0 = 3.61 A). ˚ (b) Next, repeat the same exercise for a shells out to a distance of 5.0 A. twinned conﬁguration. In particular, make two graphs, one for the atoms right at the twin plane, and one for the atoms one layer away from the twin plane. Compare the distribution of neighbors with those in the perfect crystal. Without doing any calculation, what will the twin fault energy be for the Morse potential for Cu that was derived in problem 2 of chap. 4? (c) Carry out the same procedure as in part (b), but now for the intrinsic stacking fault. Again, comment on the energy of such a fault as implied by the Morse potential. What do you conclude about the nature of the interactions that are responsible for the stacking fault energy? (d) Use an embedded-atom potential of the Johnson form (see chap. 4) and compute the stacking fault energy.

506

9 Wall Defects in Solids

5 Effective Hamiltonian for Stacking Fault Energy In the discussion culminating in eqn (9.18), we described the use of an Isinglike effective Hamiltonian for the description of fault energies. Show that if we use eqn (9.18) in the case when n max = 2 then the energy of a twin is given by E twin = 2J1 + 4J2 , the energy of an intrinsic stacking fault is given by E intrinsic = 4J1 + 4J2 and the energy of an extrinsic stacking fault is given by E extrinsic = 4J1 + 8J2 . Note that the extrinsic fault energy was worked out in the chapter to illustrate how to make such calculations. 6 Atomic-Level Simulation of Grain Boundary Structure Use the Johnson potential to simulate the structure of a '5 symmetric tilt boundary with a (001) rotation axis. In particular, ﬁnd the relaxed structure associated with the '5 boundary shown in ﬁg. 9.41. 7 Treatment of the Structure and Energetics of Triple Junctions (a) Our discussion of triple junctions in this chapter was intentionally simpliﬁed such that the equilibrium structure was presumed to depend only on a single geometric parameter. In this problem, generalize the treatment given in the chapter such that the triple junction has a position characterized by two parameters, namely, its x and y coordinates. (b) Write down the equilibrium condition in the case in which the interfacial energies differ for the three boundary segments.

TEN

Microstructure and its Evolution

We have made no secret of the pivotal role played by various geometric structures within materials in conspiring to yield observed properties. However, one of the abiding themes of our work thus far has been the observation that this notion of ‘structure’ is complex and scale-dependent. The properties of materials depend upon geometry not only at the microscopic scale, but at larger scales as well. Recall that the hierarchy of geometric structures that populate materials begins with the underlying atomic arrangements. Questions of structure at this level are answered through an appeal to phase diagrams in the way considered in chap. 6. These atomic-level geometries are often disturbed by the various defects that have served as the centerpiece of the previous three chapters, and which introduce a next larger set of length scales in the hierarchy. However, much of the effort in effecting the structure–properties linkage in materials science is carried out at a larger scale yet, namely, that associated with the various microstructures within a material. The current chapter has as its primary aim a discussion of some of the many types of microstructures that populate materials and how such microstructures and their temporal evolution can be captured from a theoretical perspective. This discussion will also serve as the basis of our later efforts to examine the connection between structure and properties in materials. We begin with an attempt at microstructural taxonomy with the aim being to give an idea of the various types of microstructures that arise in materials. Once we have built up an overall impression of the empirical backdrop concerning microstructures in materials, we will attempt to consider how modeling can be brought to bear on a few representative examples. Because of the vast diversity in different microstructures and materials, we will not attempt anything like an exhaustive discussion of microstructural evolution. Rather, through the device of considering a few well-placed examples, our hope is to give an impression of the types of questions that can be posed, and the theoretical machinery that might be used to address them. 507

508

10 Microstructure and its Evolution

10.1 Microstructures in Materials We begin with a brief overview that attempts to make sense of the wide variety of microstructures that are found in materials (primarily metallic). This part of our task should be seen as taxonomical: we aim to observe and classify with the hope that certain classes of microstructures will suggest broad classes of models. The observations of these structures will then be supplemented by an analysis of how by exploiting the twin strategies of heating and beating a material, microstructures can be tailored to a desired form. Microstructural taxonomy has reached a sufﬁcient level of sophistication that it is possible to identify certain broad classes of microstructure. Before beginning, however, it is necessary to reiterate what this chapter is not. Our primary emphasis will be on metals. The majority of experimental data to be highlighted will be drawn from the metallurgical literature with occasional reference to nonmetallic precipitates within such metals. This is not to say that other material systems are without interesting microstructures. On the contrary, the subject is so vast as to have escaped even a modicum of competency on the part of the author. 10.1.1 Microstructural Taxonomy Evidence for the existence of microstructures is often present even at those scales that can be discerned by the naked eye. This claim is substantiated in ﬁg. 10.1 which shows the microstructures of turbine blades associated with different generations of casting technology. The leftmost ﬁgure in the group reveals a series of grains that appear statistically homogeneous. The basic observation is that a generic crystalline solid will be composed of many different grains, each with a particular crystalline orientation and separated by grain boundaries. The entirety of these grains and the associated boundaries make up the polycrystalline microstructure. Polycrystals of this sort are but one example of the types of microstructures that can be found. The second picture in the sequence in ﬁg. 10.1 reveals an anisotropic microstructure in which the grains are elongated along a preferred direction. The ﬁnal picture in this sequence, though remarkable as a single crystal of enormous proportions, is perhaps less interesting as a representative example of a material with microstructure. Microstructure in Single Phase Polycrystals. We begin with a discussion of the simplest microstructure (at least to characterize geometrically) in which the grain size is the dominant microstructural parameter. We are all used to the idea that the technologies that surround us are constrained by various codes which attempt to standardize products and the processes used to realize them. Such codes exist for everything ranging from skyscrapers to microwave ovens. It is

10.1 Microstructures in Materials

509

Fig. 10.1. Microstructures for turbine blades produced using different casting technologies.

less evident, however, that there might exist codes that serve to standardize the discussion of microstructure as well. The ASM has standardized this ﬁeld in a way that is revealed in the Metals Handbook (ASM 1972) and which we show in ﬁg. 10.2. The frames of ﬁg. 10.2 show some representative examples of different grain structures in steel. The distinguishing feature from one frame to the next is the grain size. For the case shown here which is for a class of low-carbon steels, the grains range in size from roughly 10 µm to 250 µm. Recall that these observations are more than idle musings since, as was noted earlier (see ﬁgs. 1.3 and 8.2), the grain size normally has a direct impact on mechanical properties such as the yield strength. Already, there are many questions that might be asked concerning the microstructures shown in ﬁg. 10.2. First, we note that the two-dimensional cross sections shown here can be deceptive. One of the most frustrating features in studying solids and one of the largest challenges that must still be fully owned up to is the difﬁculty of attaining three-dimensional understanding of the various structures that populate materials. As a step in this direction, we interest ourselves in different ways of characterizing a material’s microstructure. As is evident from the ﬁgures discussed above, the microstructure is characterized by an element of randomness. On the other hand, there are also key elements of statistical regularity which may be exploited. Note that in the discussion given above, we have only made reference to the average grain size which is the simplest gross parameter for

510

10 Microstructure and its Evolution

Fig. 10.2. Representative examples of ASTM grain sizes in low-carbon steel: (a) grain size 2 (≈ 180 µm), (b) grain size 5 (≈ 60 µm), (c) grain size 7 (≈ 30 µm), (d) grain size 10 (≈ 10 µm). Mean grain sizes associated with each microstructure are given in parentheses.

characterizing a material’s microstructure, and that which enters into many of the simple empirical scaling models of material response. The microstructure described above may be seen as the most homogeneous limit of those we will consider here. A complementary set of information concerning microstructures of the type featured above can be obtained by mapping the orientations of the various grains making up the polycrystal. The basic idea is that one may determine the preponderance of different crystal orientations. The new technique of orientation imaging microscopy now allows for the determination of such orientational information with high spatial resolution. An example of the type of results that are obtained via this technique is shown in ﬁg. 10.3. Precipitates and Inclusions. The presence of more than a single species in a material makes it possible that a given microstructure will be far richer than that described above. In particular, by virtue of the presence of several species coupled

10.1 Microstructures in Materials

511

Fig. 10.3. Orientation imaging microscopy image of a partially recrystallized low-carbon steel. The leftmost ﬁgure is an image quality map in which the image quality obtained from the diffraction pattern is mapped onto a gray scale. The middle ﬁgure shows the orientation of the various grains with respect to the normal plane of the sample and the correspondence between colors and orientation is effected via the crystallographic triangle shown on the right of the ﬁgure (courtesy of Stuart Wright).

with the operation of diffusion giving the different atom types the possibility of redistributing, it is possible to have microstructures that are mixtures of different phases. The geometric framework that will serve as the basis of our analysis of these microstructures is that of a ‘matrix’ material that is punctuated by the presence of second-phase particles. In this section, our primary aim is to take stock of the qualitative features of such microstructures and to foreshadow some of the physical properties that are inherited because of them. One of the ﬁrst comments we must make in describing such structures from the standpoint of the modeler is the need to distinguish between coherent and incoherent second-phase particles. The key point is that the constraint of coherency (i.e. the two phases join up smoothly across the interface) implies an attendant possibility for signiﬁcant internal stresses. In ﬁgs. 10.4, 10.5 and 10.6, we show a few different examples of the microstructures involving second-phase particles that arise within different contexts. One feature of these examples that begs an explanation is that of the widely different morphologies exhibited in different cases. Second phase particle shapes range from nearly spherical, to faceted, to highly elongated rods and ultimately, plates and needles. A very useful compendium on some of the variety to be found in precipitate microstructures is Russell and Aaronson (1978). As will be seen later, the simplest model of the equilibrium shapes of such precipitates is based on an isotropic interfacial energy and leads to the expectation of spherical particles.

512

10 Microstructure and its Evolution

Fig. 10.4. Rod-shaped precipitates in Cr–Nb alloy (courtesy of Sharvan Kumar). The precipitates are Cr2 Nb and have the C15 Laves phase crystal structure.

Fig. 10.5. Al2 Cu (θ ) precipitates in Al (courtesy of Bob Hyland).

As the ﬁgures indicate, the most naive theoretical intuition is incomplete. Below we will take up the challenge of how to explain the origins and characteristics of these microstructures. In addition, in chap. 11, we will examine the way in which a distribution of second-phase particles can alter the mechanical properties of a material. Lamellar Microstructures. The precipitate microstructures described above have a geometric distribution such that a description in terms of a background matrix that is riddled with second-phase particles is appropriate. A second class of multiphase microstructure is lamellar microstructure like that shown in ﬁg. 10.7. To better

10.1 Microstructures in Materials

513

Fig. 10.6. As cast microstructure of Cu–O alloy with 0.78% oxygen content. The dendritic regions are Cu2 O. Micrograph 2257 from Metals Handbook (ASM 1972).

appreciate the nature of these microstructures, we begin by referring once again to the iron–carbon phase diagram as given in ﬁg. 1.5 in which it is seen that in the low-carbon concentration limit, we should expect the presence of both α-Fe (also known as ferrite) and Fe3 C. The presence of both of these constituents together gives rise to a lamellar microstructure like that considered here. The basic idea is the emergence of structure on a few different scales. At the larger scale are overall colonies (or grains) within which the α-Fe and Fe3 C have the same orientation relationship. The structure within such a grain is characterized by an alternation between α-Fe and Fe3 C regions. This characteristic morphology is revealed in ﬁg. 10.7. From the perspective of constructing models of such microstructures, both for their evolution and their impact on material properties, it is clear that this is a completely different class of problems than those built around second-phase particles. The diversity of the various microstructures we have considered thus far is depicted schematically in ﬁg. 10.8. From a structural perspective, these different structures permit interpretation crystallographically in terms of the various phases that make up the microstructure. A different class of microstructural feature can arise by virtue of the presence of dislocations. Organization and Patterning of Dislocations. As a result of deformation, the dislocations present in a given material form structures. These structures bear no resemblance to the featureless and homogeneous dislocation arrangements that might be thought of at ﬁrst blush. Nor, as remarked above, do these structures

514

10 Microstructure and its Evolution

Fig. 10.7. Lamellar pearlite microstructure of a hot rolled steel bar. Micrograph 354 from Metals Handbook (ASM 1972). This ﬁgure is at a magniﬁcation of 2000×.

Fig. 10.8. Classiﬁcation of various two-phase microstructures (adapted from Hornbogen (1984)).

10.1 Microstructures in Materials

515

Fig. 10.9. Transmission electron microscopy image revealing the organization of dislocations in single-crystal Cu into a labyrinthine pattern as a result of cyclic loading (adapted from Suresh (1998)).

admit of the relatively clear cut interpretation offered for the several microstructural types introduced above. The dislocation structures found in materials exhibit even more remarkable patterning as is evident when the loading to which the material is subjected is cyclic. In this case, the repeated loading allows the formation of yet sharper and more organized structures such as those shown in ﬁg. 10.9.

Microstructure at Surfaces. Our previous discussion has emphasized the microstructures that are present in generic bulk crystals. On the other hand, with the increasing reliance on layered materials in a variety of contexts including microelectronics (also revealed in ﬁg. 10.8) and in particular, on thin ﬁlms, a new generation of microstructures has grown up which are to a large extent two-dimensional. Though there is much that can be said on this point, we but mention them so as to signal the reader to the need for thinking in these areas as well. Because of the conﬂuence of high-quality growth systems and attendant surface probes, one area of especial interest is that of the variety of ‘self-organized’ microstructures that are seen during growth. A particular example in the Si–Ge system is shown in ﬁg. 10.10. Thus far, our discussion has centered on some of the qualitative geometric and chemical features of microstructures found in different classes of materials. Now that we have seen in broad brush strokes the classiﬁcations that are possible, we turn to the question of how such microstructures can be produced by appropriate processing strategies, and what the consequences of such microstructures are to the underlying physical properties of a material.

516

10 Microstructure and its Evolution

Fig. 10.10. Atomic force microscopy image of an island array in Si80 Ge20 alloy grown on Si(001) (courtesy of J. Floro and Eric Chason). The morphology is built up of pyramidal ‘hut’ clusters with (501) facets.

10.1.2 Microstructural Change Until now, our microstructural description has been geometric and qualitative without any real discussion of how such microstructures are prepared. Tuning microstructures is one of the oldest forms of engineering and may be traced to the historic ages when chemical impurities were used to harden metallic materials, though the microstructural understanding that went with these processes was clearly not present. The key insight, and the thrust of the present section, is the recognition that by subjecting a material either to deformation or heating or both, the underlying microstructure may be altered, another reminder that in dealing with microstructures we are treating nonequilibrium phenomena. As has already been mentioned, entire historic ages may be thought of as having emerged from particular types of microstructural control. Microstructural change occurs both intentionally and by accident. No doubt, most readers of this book have been confronted with the rusted remains of some favorite gadget – the terminal state of what was once a metastable arrangement. Despite the apparent permanence of many materials on everyday time scales, when viewed over longer times they are seen to be teeming with activity. Our present discussion aims to describe a few different processing histories, with an eye to explaining the way in which such processing steps alter a given microstructure. The particular modeling strategies for describing these processes will be taken up in turn as the chapter proceeds. Traditional metallurgy is sometimes derogatorily referred to as the science of ‘heat and beat’ where the tandem operations of annealing and working the material via a sequence of carefully selected, albeit often empirically derived,

10.1 Microstructures in Materials

517

processing steps are used to obtain some desired properties. On the other hand, the importance of thermomechanical processing to everyday materials technology cannot be underestimated. In addition, the processes that transpire under these circumstances provide a wide range of problems that any complete theory of nonequilibrium processes must answer to. Working a Material (Beat) Generically, beating a material refers to the act of subjecting a material to plastic deformation via processes such as systematic stretching or through cyclic loading. One of the particular means whereby materials are deformed in the name of reaching some desired ﬁnal shape or microstructure is that of rolling. The principal idea is to take the specimen and to subject it to preferential deformation which tends to elongate and squish it, for example. In ﬁg. 10.11, we show two snapshots in the deformation history of a sample of tungsten which has been subjected to such rolling processes. In this instance, it is seen that one of the primary outcomes of the deformation process is the elongation of the underlying grain structure. In addition, the working of the material is also attended by microstructural change at the dislocation level in that the dislocation density can be increased by orders of magnitude. The increase in dislocation density is attended by changes in the mechanical properties. An indication of the relation between plastic strain and dislocation density was already given in ﬁg. 8.40. What that ﬁgure showed was the way in which by virtue of the working of a material, dislocations are stored in that material. We have also already noted (see ﬁg. 8.2) that these microstructural changes are attended by concomitant changes in the properties of the material. Annealing a Material (Heat) In a worked material, the microstructure is characterized by a series of heavily dislocated grains. As was evidenced in our discussion of dislocations in chap. 8, such microstructures are inherently metastable. If the material is heated, a series of discernible changes will occur. An obvious example of this type of outcome is shown in ﬁg. 10.12 in which it is seen that in the vicinity of a weld, the grain structure is completely different than in those regions far from the heating. Systematic investigation of the properties of materials subject to annealing have resulted in a convenient classiﬁcation of the processes undergone within the solid. In particular, it has been found convenient to separate these changes into three separate processes, namely, recovery, recrystallization and grain growth. The onset of recovery can be discerned in electrical resisitivity measurements in which it is found that the resistivity decreases as a function of time, signaling a decrease in the number of scattering centers. There are a number of different mechanisms that can be associated with the recovery process, one of which corresponds to the removal

518

10 Microstructure and its Evolution

Fig. 10.11. Grain structure of tungsten polycrystals. Upper ﬁgure shows polycrystal with equiaxed grain structure while lower ﬁgure illustrates polycrystal that has suffered deformation via wire drawing (courtesy of Clyde Briant).

of point defects from the material. The recrystallization stage is characterized by a reduction of the net dislocation density, with the development of grains which are relatively dislocation-free. Finally, in the grain growth stage, the mean grain size increases with a corresponding reduction in the total grain boundary area. All of these processes are further elaborated in both Martin et al. (1997) and Humphreys and Hatherly (1995). In addition to processes involving the alteration of the defect structures within a material upon heating, it is also clear that by altering the temperature, phase changes can be induced as well. Indeed, the control of the relative proportions of different phases within a material is one of the primary ways that microstructural

10.1 Microstructures in Materials

519

Fig. 10.12. Illustration of changes in microstructure that attend the welding process in a copper cold rolled bar. Adapted from micrograph 2307 in Metals Handbook (ASM 1972).

control is exercised. As we have already mentioned, one of the scenarios in which phase transformations are sure to occur is that in which there is the potential for precipitation reactions due to an overabundance of some foreign atoms. With increasing temperature, the likelihood of diffusion increases and with it the possibility that atoms can organize into precipitates. With increasing time at elevated temperature, the size of such precipitates can increase due to coarsening effects.

10.1.3 Models of Microstructure and its Evolution We now wish to undertake an examination of various case studies in the analysis of microstructure. Perhaps the simplest example is that of a single second-phase particle in an otherwise homogeneous medium. For many purposes, this problem serves as the starting point for subsequent analyses, and ﬁnds its way into the analysis of problems ranging from two-phase microstructures to the effective properties of polycrystals. Our analysis will begin with one of the key elastic models of material microstructure, namely, the problem of the Eshelby inclusion. One direct route to the properties of this solution is to consider an elastically homogeneous medium (i.e. the same elastic properties throughout) but for which a certain region has undergone a transformation strain. Using the Green function techniques developed in earlier chapters, it is then possible to deduce the elastic ﬁelds associated with such an inclusion. Once we have deduced the elastic consequences of second-phase particles, we will be in a position to examine questions of both the nucleation and subsequent evolution of such particles, with special attention being given to the equilibrium sizes and shapes attained by these particles. The second modeling centerpiece considered in this chapter will be our discussion of martensitic microstructures. This work is offered on the basis of our

520

10 Microstructure and its Evolution

contention that this theory offers much of the analytic insight that one might hope to ﬁnd in models of more generic microstructures. In particular, by virtue of the conjunction of kinematic and energetic arguments, the theory of martensitic microstructure to be offered here is able to make detailed predictions about these microstructures, including the fractions of different martensitic variants that are to be expected. The discussion will be rounded out by our taking stock of microstructural evolution as seen from the more traditional metallurgical viewpoint. In particular, grain growth will be taken up from a theoretical perspective. This discussion should be seen as a continuation of those given in the previous chapter since the attempt to understand these phenomena rests heavily on a synthetic understanding of point, line and interfacial defects in concert. Our contention will be that despite the exertion of Herculean efforts, a number of key difﬁculties remain.

10.2 Inclusions as Microstructure As noted many times already, phase diagrams instruct our intuition concerning the temporal evolution of certain metastable states. In particular, for the case in which one has a supersaturation of foreign atoms, one is led to expect that if the atoms have sufﬁcient mobility, sooner or later they will ﬁnd each other out and colonize new phases, namely, precipitates. Examples of some of the resulting microstructures were shown in ﬁgs. 10.4, 10.5 and 10.6. We also note that by virtue of particular thermomechanical histories (i.e. by suitable processing) the nature and distribution of these precipitates may be tailored to yield desirable physical properties. For the purposes of the present discussion, one of our ambitions is to consider a class of second-phase microstructures in which the two phases are coherent. In these instances, the constraint of coherency carries with it an elastic penalty which results in elastic distortions in both the precipitate particle and the matrix material surrounding it. As a preliminary to the concrete mathematical investigation of such structures, we must ﬁrst learn something of the elastic consequences of a single inclusion.

10.2.1 Eshelby and the Elastic Inclusion The elastic solution upon which many approaches to the consideration of microstructure are built is that of the so-called Eshelby inclusion in which one considers a single ellipsoidal inclusion in an otherwise unperturbed material. From the standpoint of the linear theory of elasticity, this problem is analytically tractable

10.2 Inclusions as Microstructure

521

Fig. 10.13. Schematic of an ellipsoidal inclusion within an elastic medium.

and provides valuable insights concerning the stresses in adjacent grains and the compatibility issues that must be faced at the interfaces between such grains. Our intention in the present section is to examine the elasticity solution to the problem of a single elastic inclusion and to attempt to use the insights afforded by this solution to learn something about that class of microstructures that can be thought of in terms of inclusions. Our starting point is the notion of an eigenstrain as discussed already in chap. 2. We picture an elastically homogeneous medium (i.e. the elastic moduli are the same throughout) with some spatial region that has undergone a strain ∗ as indicated schematically in ﬁg. 10.13. The philosophy espoused in the method of eigenstrains is that the presence of these eigenstrains may be thought of as giving rise to some distribution of body forces. However, as we have already shown repeatedly, once such a distribution is speciﬁed, the elastic Green function may be invoked to write down the displacement ﬁelds as an integral over this distribution. In the present setting, this argument proceeds as follows. The equilibrium equations of elasticity may be written as ∇ · σ e = 0,

(10.1)

where the superscript e refers to the fact that it is only the elastic part of the strain that gives rise to stresses. However, this statement of equilibrium may be rewritten on the basis of the observation that the total strain is given by tot = e + ∗ . In particular, we have tot ∗ Ci jkl kl, j − C i jkl kl, j = 0.

(10.2)

Recall that the distribution of eigenstrains is prescribed and hence the term

522

10 Microstructure and its Evolution

∗ ∗ Ci jkl kl, j is known. If we make the transcription C i jkl kl, j = − f i , where f i is the th i component of a ﬁctitious body force ﬁeld, then our problem has been mapped onto a boundary value problem for the unknown total displacement,

Ci jkl u tot k,l j = − f i .

(10.3)

For the particular case of interest below, we imagine an inﬁnite body and an associated condition that the ﬁelds vanish at inﬁnity. As already remarked, once the body force distribution has been speciﬁed, by invoking the elastic Green function, the displacement ﬁelds are immediately obtained as the integral tot ∗ 3 (10.4) u k (x) = − Cmjpl pl, j G km (x − x )d x .

For our present purposes, we assume that the eigenstrain of interest is uniform throughout the region . Using integration by parts, the differentiation on the eigenstrain itself can be pushed onto the Green function with the result that tot ∗ u k (x) = Cmjpl pl G km, j (x − x )d 3 x . (10.5)

Note that the differentiation of the Green function is with respect to the primed variables. We can now use the relation ∂ ∂ G km (x − x ), (10.6) G km (x − x ) = − ∂ xj ∂ xj to rewrite our expression for the displacements as tot ∗ G km, j (x − x )d 3 x , u k (x) = −Cmjpl pl

(10.7)

where in this instance the differentiation of the Green function is with respect to the unprimed variables. Thus far, our results are primarily formal. As an exercise in exploiting the formalism, we will ﬁrst examine the ﬁelds associated with spherical inclusions, and then make an assessment of the elastic strain energy tied to such inclusions. These results will leave us in a position to consider at a conceptual level the nucleation, subsequent evolution and equilibrium shapes associated with inclusion microstructures. To compute the displacements and strains associated with an inclusion explicitly, we must now carry out the operations implied by eqn (10.7). To make concrete analytic progress, we now specialize the analysis to the case of an elastically isotropic solid. As a preliminary to the determination of the elastic ﬁelds, it is necessary to differentiate the elastic Green function which was featured earlier as

10.2 Inclusions as Microstructure

523

eqn (2.91). In particular, if we evaluate the derivative of G km with respect to x j , we ﬁnd G km, j (x − x ) =

(x j − x j ) 1 −(λ + 3µ)δkm 8π µ(λ + 2µ) |x − x |3 (xk − xk ) (xm − xm ) + (λ + µ)δk j + (λ + µ)δ m j |x − x |3 |x − x |3

(xm − xm )(xk − xk )(x j − x j ) , − 3(λ + µ) |x − x |5

(10.8)

a mess that can be simpliﬁed considerably if we follow Mura (1987) in adopting the notation li = (xi −xi )/|x−x |. In particular, contracting this expression to form ∗ G km, j as is demanded by our expression for the displacements, eqn (10.7), Cmjpl pl we ﬁnd that the displacements can be written as ∗ pl

d 3 x (µδkl l p + µδkp ll − µδ pl lk + 3(λ + µ)lk l p ll ). 4π(λ + 2µ) |x − x |2 (10.9) Our ﬁrst exercise in computing the displacements themselves will be to consider the ﬁelds due to a spherical inclusion with a dilatational eigenstrain of the form i∗j = 0 δi j and with radius a. In this case, the contraction implied by the presence of the δi j simpliﬁes considerably such that u tot k (x)

=

∗ Cmjpl pl G km, j

0 3λ + 2µ (xk − xk ) =− , 4π λ + 2µ |x − x |3

(10.10)

and hence the computation of the displacements reduces to the evaluation of the integral (xk − xk ) 3 0 3λ + 2µ tot d r. (10.11) u k (x) = 3 4π λ + 2µ |x − x | For the sake of checking the correspondence of our present results with those favored by others where the elastic constants µ and ν are used, we note the identity (3λ + 2µ)/(λ + 2µ) = (1 + ν)/(1 − ν). Note that in light of these results, the determination of the elastic displacements has been reduced to the evaluation of a geometric integral over the inclusion itself. For an isotropic solid with a spherical inclusion, the displacements ﬁelds are themselves spherically symmetric. As a consequence, without a loss of generality, we can evaluate the u 3 component of displacement along the z-axis, resorting to spherical coordinates to simplify the integrals. By symmetry, this is equivalent to the radial component of displacement,

524

10 Microstructure and its Evolution

Fig. 10.14. Radial displacements associated with a spherical inclusion for which the eigenstrain is given by i∗j = 0 δi j . Displacements have been cast in dimensionless terms.

u r (r ). In particular, the expression for the displacements reduces to a π 0 3λ + 2µ r − r cos θ tot 2 r dr sin θ dθ . u r (r ) = 3 2 λ + 2µ 0 0 (r 2 + r 2 − 2rr cos θ ) 2 (10.12) For a point outside of the inclusion, evaluation of the requisite integrals results in 0 a 3 3λ + 2µ tot u r (r ) = . (10.13) 3r 2 λ + 2µ Similarly, if we are to evaluate the displacements within the inclusion, it is found that 0r 3λ + 2µ tot , (10.14) u r (r ) = 3 λ + 2µ indicating that within the inclusion the strain is constant, as was hinted at earlier. The displacement as a function of the radial coordinate is shown in ﬁg. 10.14. From the point of view of our efforts to examine the energetics of microstructures, our assessment of the elastic ﬁelds due to inclusions must be supplemented with insights into their energies. In light of our success in deducing the elastic ﬁelds, it is relatively straightforward to compute the strain energy associated with such an inclusion and the most naive approach is to add up the elastic energy throughout the entire medium via 1 E elastic = σi j iej d V, (10.15) 2 where denotes the entire region of matrix and inclusion. (A simpler scheme for carrying out this evaluation of the elastic strain energy is reserved for the problem

10.2 Inclusions as Microstructure

525

section at the end of this chapter.) Note that the integral demands a knowledge of the elastic strain. Since our calculations have yielded the total displacement, there is a bit of work needed to recast our results in a form that is suitable for the determination of the elastic energy. In particular, we ﬁnd it most convenient to work with an alternative form for the strain energy density, namely, ν 1 ∗ tot ∗ 2 tot ∗ 2 . (10.16) σi j (itot [tr( − ) = µ ( − ) + − )] j ij ij ij 2 1 − 2ν Note that we have resorted to the use of µ and ν for our description of the elastic properties for ease of comparison with many of the expressions that appear elsewhere. In order to compute the total elastic energy, we separate the volume integral of eqn (10.15) into two parts, one which is an integral over the inclusion, and the other of which is an integral over the matrix material. The reason for effecting this separation is that, external to the spherical inclusion, the displacements we have computed are the elastic displacements. On the other hand, within the inclusion, it is the total ﬁelds that have been computed and hence we must resort to several manipulations to deduce the elastic strains themselves. For the particular eigenstrain chosen here, note that we have i∗j = 0 δi j . Within the inclusion this led to the displacement given in eqn (10.14) which can be differentiated to yield the strain 0 1 + ν in i j = δi j . (10.17) 3 1−ν As a consequence, we ﬁnd that the elastic strain is given by 20 1 − 2ν elastic ∗ δi j . = i j − i j = − i j 3 1−ν

(10.18)

In light of this result, we are now prepared to evaluate the strain energy within the inclusion, which using eqn (10.16) is in = E strain

16πa 3 02 µ (1 − 2ν)(1 + ν) . 9 (1 − ν)2

(10.19)

We are also interested in the elastic energy external to the inclusion. To compute this, we demand the strains outside of the inclusion, which can be simply evaluated on the basis of eqn (10.13) with the result that 20 a 3 1 + ν (10.20) rr = − 3r 3 1 − ν 0 a 3 1 + ν . (10.21) θθ = φφ = 3r 3 1 − ν The elastic energy stored in the region outside of the inclusion may now be

526

10 Microstructure and its Evolution

evaluated in a fashion similar to that invoked to evaluate the energy stored within the inclusion with the result that out = E strain

8πa 3 02 µ (1 + ν)2 . 9 (1 − ν)2

(10.22)

Hence, the total strain energy of the medium is arrived at by summing the contributions from within and outside of the inclusion, and leads to E strain =

8πa 3 02 µ (1 + ν) . 3 (1 − ν)

(10.23)

What we have learned is that the elastic energy associated with a spherical inclusion characterized by an eigenstrain i∗j = 0 δi j scales in a simple way with the volume of the inclusion itself. Similar analytic progress can be achieved for other simple geometries such as ellipsoidal and cube-shaped inclusions. The main point of the efforts described above is that we are now in a position to evaluate the elastic consequences of coherent precipitates as will be necessary in our consideration of equilibrium shapes in coming sections. What we note now is that by virtue of our knowledge of the features of this highly idealized problem and its corresponding solution, we are prepared to make inroads on a variety of problems including that of the coarsening of two-phase microstructures and the effective properties of multiphase media. Despite the insight provided by analytic solutions like those given above, there are many instances in which the geometries, materials and loads are sufﬁciently complex as to defy useful analytic description. Indeed, note that our solution was predicated on the use of a Green function which was itself derived on the assumption of material homogeneity, an assumption which is manifestly not warranted in many cases of interest. In these cases, one must resort to numerical calculation. We have already noted that there is both a synergy and tension between analytic and numerical results. On the one hand, analytic results are highly instructive in that they provide insights into the qualitative dependence of solutions on material and geometric parameters. On the other hand, such solutions are limiting in that they usually do not allow for a treatment of a wide range of geometries. Though the analytic solution set forth here will be of great use for providing insights into the nature of elastic ﬁelds surrounding inclusions, our ultimate discussion of the temporal evolution of precipitate microstructures and their equilibrium shapes will be largely predicated upon numerical schemes for solving the types of elastic boundary value problems posed above.

10.2 Inclusions as Microstructure

527

10.2.2 The Question of Equilibrium Shapes Having now developed a feel for the elastic consequences of the presence of a second-phase particle in a given material, we are poised to investigate the equilibrium morphologies of second-phase particles as well as their temporal evolution. We begin with the question of the equilibrium shapes of coherent second-phase particles which will be expressed as the playing out of a competition between the types of elastic terms considered above and other energetic inﬂuences such as the energy of the interface between the two particles. This type of reasoning is ubiquitous and ultimately rests on the variational character of thermodynamic equilibrium. Of course, such arguments skirt the question of whether or not the particular situation of interest is really an equilibrium state or not. Stated simply, our initial foray into these questions will be predicated upon the idea that in certain cases, microstructures of interest may be thought of as energy minimizers. For the problem at hand, the competition of interest may be expressed in its simplest incarnation with relative ease. If we are to return to the experimental circumstances of interest, our starting point is a situation in which an alloy has been cooled to the point that there is an overabundance of foreign atoms within the host matrix. As a result of the process of diffusion, these foreign atoms collect and begin to form precipitates. However, because of the difference in structure between the matrix and precipitate (this difference in structure may mean nothing more than a different chemical distribution on the same underlying lattice), there is an energy penalty for both the interface between the matrix and the precipitate as well as for the elastic strains induced by this difference in structure. Both of these energies depend, in turn, upon the particle shape as well as upon the arrangements of the precipitates with respect to each other. If we are to consider the simplest case in which a ﬁxed quantity of mass is assigned to the second-phase particle of interest and demand what shape results in the lowest free energy, it is easily imagined that the free energy depends upon those parameters characterizing the shape through a number of different terms. The conceptual underpinnings of our investigation of equilibrium shapes is represented by the formula 1 γ (n)d A + σi j i j d V. (10.24) E tot (shape) = 2 ∂ The ﬁrst term on the right hand side represents the energy cost associated with the interface between the particle and the matrix, and for generality we have assumed (temporarily) that the interfacial energy is anisotropic, a fact that is revealed by the dependence of this energy on the normal n as γ (n). The second term is the elastic energy of the medium by virtue of the presence of the second-phase particle. Note that both of these terms are functionals of the particle shape and our ambition is to

528

10 Microstructure and its Evolution

minimize the energy with respect to the various possible shapes. We note that in the discussion that follows, the use of the term anisotropy will do double service to characterize both the morphological anisotropy of the particles themselves, as well as the crystallographic anisotropy of the various material parameters such as the interfacial energy and the elastic moduli.

10.2.3 Precipitate Morphologies and Interfacial Energy The simplest picture that can be considered for describing equilibrium shapes is predicated entirely on the presence of the interfacial energy. In particular, the elastic energy given in eqn (10.24) is dropped all together and instead, we are left with minimizing γ (n)d A + λ d V, (10.25) E tot (shape) = ∂

where the second term on the right hand side introduces a Lagrange multiplier λ with the constraint of ﬁxed volume. Note that we have ignored the complicating inﬂuence of ﬁnite temperatures. Before continuing with our discussion of the minimizers of this functional, it is important to recall the extent to which the physics it entails can be informed on the basis of microscopic insights. In particular, in light of the discussion of chap. 9, it is clear that microscopic analysis can be used to construct the interfacial energy γ (n). Indeed, both ﬁgs. 9.46 and 11.9 illustrate the dependence of interfacial energy upon the relative orientation of the different crystallites which the interface separates. In the present case, it is the relatively simple generalization of these results to the case in which the interface separates two different phases that is of interest, and we conclude this comment by noting that the microscopic evaluation of these quantities offers no compelling new twists on what we have done before. Though it would take us too far aﬁeld to provide a detailed discussion, we at least mention the idea of the Wulff construction in which the equilibrium shapes of particles are inherited from the properties of the interfacial energy as a function of orientation. The starting point of an analysis of the equilibrium shapes associated with minimizing the interfacial energy is made by appealing to a Wulff plot (or γ -plot) in which a three-dimensional closed surface is constructed with the property that the distance of a given point on that surface from the origin is equal to the interfacial energy associated with the orientation of that point. That is, the surface is speciﬁed as the collection of points r of the form r = γ (n)n. The set of points corresponding to all of the unit vectors n corresponds to the unit sphere. The idea of the γ -plot is to take each such point and to scale its distance from the origin by the corresponding γ (n). Once we are in possession of the

10.2 Inclusions as Microstructure

529

γ -plot, we are then prepared to determine the equilibrium shape itself by recourse to Wulff’s construction which instructs us to convexify the γ -plot with the result that the equilibrium shape corresponds precisely with the resulting polygon (in two dimensions) or polyhedron (three dimensions). Concretely, what this means is that we are to visit each and every normal vector n and to construct a perpendicular plane which passes through the intersection of that normal with the γ -plot. The equilibrium shape corresponds to the inner envelope of this collection of planes. We also make the important point that the resulting equilibrium shape has no dependence on particle size, a conclusion that is at marked odds with observed microstructures. These ideas are elaborated further in the problem section at the end of the chapter. An excellent discussion of these ideas may be found in section 5.4 of Martin et al. (1997). An alternative discussion with more emphasis on the statistical mechanical underpinnings of this problem may be found in Rottman and Wortis (1984). The construction described above now permits us to hint at the relevance of the interfacial energy to the question of equilibrium shapes. Indeed, an example of the outcome of such reasoning in the context of a Cu–Zn alloy is shown in ﬁg. 10.15. The precipitates being evaluated here arose as a result of isothermal heat treatment of supersaturated β phase which resulted in the formation of faceted polyhedra of the γ phase of composition Cu5 Zn8 . The ﬁgure shows various sections through the precipitate centroids associated with γ phase precipitates in the Cu–Zn system. In particular, note that these sections are made through the (100), (111) and (110) planes. The dotted curves in the ﬁgures reveal the Wulff plots associated with these measured particle morphologies. In fact, the reasoning is really run in reverse relative to the usual Wulff argument since in this case it is the shapes that are observed and the γ -plots that are backed out. Nevertheless, our main point in bringing up these issues was to call attention to the ideas used in addressing the case in which the interfacial energy dominates the equilibrium shape.

10.2.4 Equilibrium Shapes: Elastic and Interfacial Energy A more complete description of the question of equilibrium shapes than that given above must account for both of the terms indicated in eqn (10.25). Our strategy in this section is to consider models which synthesize the effects of both interfacial and elastic energy from ever increasing levels of sophistication. As usual, these formulations will illustrate the tension between analytic tractability and physical realism, with the most realistic models almost entirely defying analytic progress. Two-Dimensional Analysis of Johnson and Cahn. For starters, we consider the equilibrium shape for second-phase particles in a two-dimensional setting.

530

10 Microstructure and its Evolution

Fig. 10.15. Series of equilibrium shapes as observed in γ Cu–Zn (solid lines) and estimated values of the interfacial energy vs orientation (dashed lines) (adapted from Stephens and Purdy (1975)). The precipitate sizes are roughly 60 µm for all but the 500 ◦ C case, in which the precipitates have a size on the order of 500 µm.

In particular, we consider a single such particle with a dilatational misﬁt (i.e. i∗j = 0 δi j ) with the restriction that the particle shape derives from only a family of such shapes that can be parameterized in terms of a few simple geometric quantities. In essence, we adopt the Rayleigh–Ritz variational procedure in which the energy function of interest depends upon a ﬁnite set of parameters and with respect to which the energy function is minimized. We follow Johnson and Cahn (1984) in considering the family of elliptical shapes characterized by their area A = πab and aspect ratio a/b. Though it is a point we have raised repeatedly, it is worth reiterating that the space of energy minimizing solutions has been shrunk to include only those that are elliptical. From the standpoint of the quantitative model used to describe this system, we assume that both the matrix and precipitate are elastically isotropic and characterized by the same elastic moduli and that the misﬁt strain associated with the precipitate is purely dilatational and is given by 0 . Further, it is assumed that the interfacial energy γint (n) is isotropic (i.e. γint (n) = γ0 ). Recall from

10.2 Inclusions as Microstructure

531

our discussion in chap. 9 that interfacial energies can vary signiﬁcantly from one crystal face to the next. What is being assumed here is that this variability can be suppressed without losing the essential features of the competition being played out. Of course, these restrictions can be relaxed, and it is interesting to do so. On the other hand, as a tool for illustrating the fundamental ideas being considered here, the simpliﬁcations that attend these assumptions make them highly attractive. As a prelude to writing the dependence of the energy on the particle shape and size, Johnson and Cahn found it convenient to carry out a change of variables which respected important symmetries that this energy must satisfy. For example, the energy should be indifferent to an interchange of the major and minor axes of the ellipse. That is, the energy associated with an ellipse with its long axis along the (10) direction and its short axis along the (01) direction should be no different from the reverse circumstance. These symmetries imply that a more useful set of coordinates are (a − b) √ , 2 (a + b) v= √ . 2

u=

(10.26) (10.27)

In terms of these new variables, the geometric description of the elliptical particles is given by π (10.28) A = (v 2 − u 2 ), 2 which is the area of the particle and U=

a−b u = , v a+b

(10.29)

which provides a measure of the departure of the ellipse from a circle. In order to determine the lowest-energy shape for a given particle size, it is necessary to express the energy in terms of the variables U and A. In principle, what we have learned from the previous two sections permits the construction of an exact energy as a function of these parameters. On the other hand, an alternative idea is to map the exact energy onto an approximate surrogate which has the form of a Landau free energy, well known from the study of phase transitions, which permits us to exploit what is known about such free energies from other contexts. The strategy is to seek an expansion of the energy in powers of U in which the expansion coefﬁcients depend upon the parameter A. Much can be said about the energy minimizing structure on the basis of general symmetry considerations which we will discuss shortly. However, we ﬁrst examine the detailed character of

532

10 Microstructure and its Evolution

these energies themselves. The interfacial contribution to the total energy in the isotropic approximation contemplated here is given by E int = γ0l,

(10.30)

where l is the circumference of the ellipse. For an ellipse with semimajor axis a and semiminor axis b, the circumference can be evaluated through the integral a a2 − ξ 2 x 2 l(a, b) = 4 d x, (10.31) a2 − x 2 0 where we have deﬁned the dimensionless parameter ξ 2 = 1 − (b/a)2 . This result is a special case of an elliptic integral and may also be written as √ 2 a − b2 π , , (10.32) l = 4a E a 2 where E is an elliptic function. By resorting to Taylor expansion, the interfacial energy term may be rewritten as √ 3 33 (10.33) E int (A, U ) = 2 π Aγ0 1 + U 2 + U 4 + · · · . 4 64 In addition to the interfacial energy, the competition at play here depends also on the elastic energy associated with the second-phase particle. Using ideas quite similar to those introduced already in the context of the Eshelby inclusion the elastic energy may be written as 1 + κδ − (1 − δ)U 2 , (1 + κδ)(1 + δ − 2ν ∗ ) + (1 − δ)(κδ − 1 + 2ν ∗ )U 2 (10.34) where the precipitate is characterized by elastic constants µ∗ and ν ∗ , while the matrix has elastic constants µ and ν. The dimensionless ratio δ = µ∗ /µ characterizes the difference in shear moduli between the two media and κ = 3−4ν. Like the interfacial energy, this term may be expanded in powers of U yielding 2A02 µ∗ δ(1 − δ)(1 + κ) 1− U2 E elastic (A, U ) = ∗ 1 + δ − 2ν (1 + κδ)(1 + δ − 2ν ∗ )

δ(1 − δ)2 (1 + κ) 4 + U ··· . (10.35) (1 + κδ)2 (1 + δ − 2ν ∗ )2 E elastic (A, U ) = 202 µ∗ A

Given our knowledge of both the elastic and interfacial energies, the total energy as a function of the particle size and shape parameters now has the character of a Landau expansion like that seen in the theory of phase transitions. In particular, we

10.2 Inclusions as Microstructure

533

have 1 1 E tot (A, U ) = E int (A, U )+ E elastic (A, U ) = F0 (A)+ F2 (A)U 2 + F4 (A)U 4 · · · , 2 4! (10.36) the minima of which will tell us the optimal U for a given A. If we truncate the expansion at fourth order, the minima are realized by those U satisfying

∂ E tot 1 (10.37) = 0 = U F2 (A) + F4 (A)U 2 . ∂U 6 On physical grounds, F4 (A) will be seen to be positive, leading to the conclusion that the energy minimizing U is given by 0 if F2 > 0 √ . (10.38) U= ± −6F2 /F4 if F2 < 0 Hence, within this approximate model, the entire question of equilibrium shape has been reduced to the dependence of F2 on A which is gotten by adding the quadratic contributions to the energy from both the interfacial and elastic terms and is given by 2A02 µ∗ δ(1 − δ)(1 + κ) 3 √ F2 (A) = γ0 π A − . (10.39) 2 (1 + κδ)(1 + δ − 2ν ∗ )2 By setting F2 (A) to zero we can obtain the critical particle size, Ac , which also √ permits the deﬁnition of a size parameter λ = A/Ac . Recall that in the present model, the parameter A has the role of characterizing the particle size, and hence suggests that with increasing particle size there could be a transition from the U = 0 regime (i.e. circular particles) to the broken symmetry regime in which the particles exhibit elliptical shapes. This transition is most simply described in considering the ratio F2 /F4 as a function of the parameter λ. Note that the transition can only occur in the case in which δ < 1 which is the limit in which the particles are softer than the matrix. The results of our analysis of the question of equilibrium shapes may be depicted graphically as shown in ﬁg. 10.16. This graph is shown for the speciﬁc case in which ν = ν ∗ = 1/3 and δ = 1/2. The key point is that with increasing particle size (measured by the dimensionless parameter λ), there is a transition from circular to elliptical shapes as the energy minimizing geometry. Note that the onset of this transition in the graph is observed by monitoring the value of U , the parameter which measures the deviation about the limit of circular particles, as a function of the particle size as measured by λ. An additional remark is to note the physical competition that is being played out. For small particle sizes, the surface to volume ratio is such that the particle shapes will be dominated by the interfacial energy while in the large-particle-size limit, the elastic terms will

534

10 Microstructure and its Evolution

Fig. 10.16. Representation of energy minimizing U as a function of a dimensionless representation of the particle size (adapted from Johnson and Cahn (1984)).

have an increasing importance. Because the interfacial energy is isotropic, it favors circular geometries while the elastic energy prefers the elongated geometries found at larger particle sizes. Numerical Calculation of Two-Dimensional Equilibrium Shapes. To go beyond the relative simplicity of the set of shapes considered in the analysis presented above it is necessary to resort to numerical procedures. As a preliminary to the numerical results that will be considered below and which are required when facing the full complexity of both arbitrary shape variations and full elastic anisotropy, we note a series of ﬁnite-element calculations that have been done (Jog et al. 2000) for a wider class of geometries than those considered by Johnson and Cahn. The analysis presented above was predicated on the ability to extract analytic descriptions of both the interfacial and elastic energies for a restricted class of geometries. More general geometries resist analytic description, and thus the elastic part of the problem (at the very least) must be solved by recourse to numerical methods. Jog et al. use a two-dimensional numerical implementation of an iterative scheme in which the geometry of the interface is parameterized by a set of nodes which serve as the conﬁgurational degrees of freedom associated with the question of the equilibrium shape. Their scheme is predicated on computing the elastic ﬁelds at ﬁxed geometry and then these ﬁelds are used ﬁrst to compute the energy and then to compute the conﬁgurational forces on those same nodes (i.e. the derivatives of the energy with respect to the interfacial coordinates) providing a search direction

10.2 Inclusions as Microstructure

535

Fig. 10.17. Comparison of analytic and numerical results for the critical size at which the circle– ellipse bifurcation takes place as a function of particle size (adapted from Jog et al. (2000)).

for the next increment in the quest for the equilibrium structure. The signiﬁcance of this implementation is that it imposes no requirements on the particle shape. As a result, the search for the energy minimizers is over a much larger space of possible shapes. One way of testing such numerical implementations is to recover known results. In the present setting, this means recovering the results of Johnson and Cahn for the transition from circular to elliptical shapes. In ﬁg. 10.17 we show the results for the critical size (the inverse of this size is actually plotted) at which the bifurcation from circular to elliptical shapes takes place as a function of the inhomogeneity factor δ = µ∗ /µ, where µ∗ and µ are the shear moduli for the precipitate and the matrix, respectively. Of course, we should note that in the case of the analysis by Jog et al., the shape transition is from circular to nearly elliptical shapes, since their geometries are no longer constrained to the single degree of freedom geometry (at ﬁxed particle size) considered by Johnson and Cahn. The numerical results beautifully complement those resulting from the Johnson and Cahn analysis since they allow for an examination of the way in which elastic anisotropy and different forms of misﬁt other than dilatational can alter the equilibrium shapes. Equilibrium Shapes in Three Dimensions. The analyses described above have illustrated the fundamental competition between interfacial energies and elastic energies in governing the outcome of the question of equilibrium shapes. These calculations were introduced in the setting of reduced dimensionality with the

536

10 Microstructure and its Evolution

Fig. 10.18. Series of equilibrium shapes for three-dimensional particles (adapted from Mueller and Gross (1998)). The parameter L is a measure of the particle size and governs the competition between the surface energy terms (dominant at small L) and the elastic terms (dominant at large L).

result that analytic progress could be made. On the other hand, the importance of the answer to the question of equilibrium shapes is much greater in the context of three dimensions and it is for that reason that we also sketch the application of ideas like those described above in their full three-dimensional generality. As before, the fundamental competition being played out in selecting equilibrium shapes in three dimensions is between interfacial and elastic energies. In the analysis of Mueller and Gross (1998), energy minimizing geometries are searched for by recourse to a boundary element treatment of the elastic energies of a given three-dimensional shape. Their treatment is fully anisotropic and relies conceptually on exactly the same eigenstrain ideas introduced earlier (see section 2.5.3) in conjunction with the elastic Green function, but now tailored to problems involving elastic anisotropy. Because their methods are numerical, the elastic ﬁelds for a given conﬁguration can be computed directly, and the driving forces on the conﬁgurational coordinates describing the interfacial position are computed in exactly the same spirit as those introduced in our discussion of conﬁgurational forces in chap. 2. The three-dimensional equilibrium shapes found in their analysis are shown in ﬁg. 10.18. The elastic parameters chosen in these calculations were meant to mimic those of Ni, with the result that in the elastically dominated large-particle limit, there is a tendency for the particles to be cube-like. The arguments given above were concerned more with the terminal privileged state that would be arrived at by a particular second-phase particle than with the dynamical trajectory by which these equilibrium states are attained. In addition, we ignored the possible interactions between different particles, which in addition to interacting elastically can exchange matter via mass transport. All of these complaints can be remedied by recourse to a more computationally intensive approach in which the dynamical evolution of a given particle is considered as

10.2 Inclusions as Microstructure

537

a function of time and the equilibrium shape is a ﬁxed point of this dynamical system. This approach will be taken up later in this chapter. However, we should note that it is also possible to go beyond the types of continuum analyses introduced here and rather to use the type of effective Hamiltonian introduced in chap. 6 in conjunction with Monte Carlo simulation to revisit the question of equilibrium shapes. Using these methods, there are no restrictions concerning particle shapes, elastic homogeneity, isotropy of interfacial energies, nor is there even any restriction to linear elasticity. These ideas will be described in chap. 12 (see section 12.4.4 in particular). 10.2.5 A Case Study in Inclusions: Precipitate Nucleation As noted above, the question of equilibrium shapes is essentially a static one and can be answered without recourse to an analysis of the temporal processes that occur in conjunction with microstructural evolution. On the other hand, we are interested in examining the theoretical apparatus that has grown up around problems in which time is considered explicitly. One of the ﬁrst questions we can address in light of our elastic solution for the energetics of an inclusion and the ﬁrst step in our attempt to understand the temporal evolution of such particles is that of nucleation of second-phase particles. As with many questions concerning an instability toward the development of some new phase, the discussion centers on a competition between two different effects, each of which tends to favor a different terminal state. In the present setting, it is the competition between a term which scales as the volume of the second-phase particle and tends to favor the formation of the second-phase particle, and an interface term which carries an energy penalty associated with the interface between the inclusion and the matrix and thus favors removal of the second-phase particle. So as to permit analytic progress, we consider the restricted class of spherical geometries. The volume term is of the form 4 (10.40) E V = πr 3 E b , 3 where E b is an energy density such that E b < 0, and r is the particle radius. On the basis of arguments made in this and earlier chapters, we are in a position to seek an interpretation of the term E b . First, we note that there is a contribution to E b that arises from the fact that the second-phase particle has a different structure and hence a different structural energy than the matrix. Our use of the term ‘structure’ here is meant to include even the difference between ordered and disordered states on the same underlying lattice. The microscopic route to computing the energy lowering represented by a second-phase particle was described in chap. 6. However, we note that this energy will be renormalized by the energy penalty

538

10 Microstructure and its Evolution

Fig. 10.19. Schematic of the bulk and interfacial energies as a function of particle size.

arising from the elastic strains as was computed in section 10.2.1. As a result, in the present model, E b can be thought of as arising from two terms, one negative and essentially a structural energy difference, the other positive and representing the elastic strain energy associated with the inclusion. The volume term described above is balanced against an interfacial energy of the form E surf = 4πr 2 γint ,

(10.41)

where for the present purposes we have assumed an isotropic interfacial energy. The generalization to the anisotropic case introduces no new physical ideas. Again, because of the types of arguments made in previous chapters, it is now clear how to appeal to microscopic calculations in order to compute γint . The energy balance to be considered here is familiar and is depicted graphically in ﬁg. 10.19. The key observation is that with increasing particle size, a certain critical particle radius r ∗ is reached such that a further increase in particle size leads to an energy reduction. From the standpoint of our discussion of conﬁgurational forces (see section 2.3.3), we see that the sign of the driving force (i.e. ∂G(r )/∂r ) depends upon the size of the particle. For small particles, the driving force is in the direction of particle shrinkage, while for particles greater than the critical size, the driving force results in growth of the particle. To cast these ideas in mathematical form, we note that the total free energy in the present model may be written as 4 (10.42) G(r ) = 4πr 2 γint + πr 3 E b . 3 To determine the critical radius r ∗ , we need to satisfy the condition ∂G(r )/∂r = 0. The consequence of performing the relevant differentiation and solving for the

10.2 Inclusions as Microstructure

539

critical radius is r∗ = −

2γint . Eb

(10.43)

Though the results of nucleation theory are well worn, it is worth emphasizing the way in which a number of disparate threads have been woven into the discussion. First, armed with the results of the previous chapter, we are now well placed to understand the microscopic origins of γint . Similarly, because of our earlier discussion of structural energies, the structural contribution to E b is also clear. Finally, the elastic solution to the problem of a spherical inclusion given earlier in this chapter has instructed us concerning the strain energy penalty that arises on forming the inclusion which has been modeled as carrying a transformation strain. The model developed above serves as a convenient starting point for carrying out a dynamical analysis of the nucleation problem from the perspective of the variational principle of section 2.3.3. A nice discussion of this analysis can be found in Suo (1997). As with the two-dimensional model considered in section 2.3.3, we idealize our analysis to the case of a single particle characterized by one degree of freedom. In the present setting, we restrict our attention to spherical particles of radius r . We recall that the function which presides over our variational statement of this problem can be written generically as ˙ r ; r ), (˙r ; r ) = (˙r ; r ) + G(˙

(10.44)

and speciﬁcally in the present context as r˙ 2 + G˙ int (˙r ; r ) + G˙ bulk (˙r ; r ). (10.45) 2M We recall that M is the mobility of the interface between the two phases as the particle changes size. To compute the rate of change in the interfacial contribution to the free energy, we evaluate G int (r + r˙ t) − G int (r ), recognizing that G int (r ) = 4πr 2 γint . This amounts to computing the difference in the interfacial energy at an initial instant when the radius of the particle is r and at a time t later when the radius of the particle is r + r˙ t. As a result of these arguments, we ﬁnd (r, r˙ ) = 4πr 2

G int (r + r˙ t) − G int (r ) = 8πr r˙ γint . G˙ int = lim t→0 t

(10.46)

A similar argument is made in the case of the rate of change of the bulk contribution to the free energy. In this case, we interest ourselves in the free energy when the particle has radius r (i.e. G bulk (r ) = 43 πr 3 E b ) and when the particle has radius r + r˙ t. In this case, the result is G bulk (r + r˙ t) − G bulk (r ) = 4πr 2r˙ E b . G˙ bulk = lim t→0 t

(10.47)

540

10 Microstructure and its Evolution

Fig. 10.20. Flows for the differential equation describing evolution of a spherical particle with growth (or dissolution) dictated by the balance of interfacial and bulk energy. The particle size (f) and time (τ ) are plotted in the same dimensionless form used in the text.

If we now invoke the variational principle (i.e. ∂/∂ r˙ = 0), then it is found that 2Mγint . (10.48) r As seen earlier, there is a natural length scale in this problem, namely, rc = 2γint /|E b |, and it is similarly convenient to introduce the dimensionless time t0 = 2γint /M E b2 . In light of these deﬁnitions, the radius may be written in dimensionless form as f = r/rc , with a similar dimensionless time given by τ = t/t0 . Using these deﬁnitions, eqn (10.48) may be rewritten as r˙ = M|E b | −

df f −1 = . dτ f

(10.49)

This equation is separable and has the solution, f − f 0 + ln |

1− f | = −τ. 1 − f0

(10.50)

The temporal evolution of particles starting with different fractions of the critical size is shown in ﬁg. 10.20. Note that as expected, if a particle happens to start with an initial size equal to the critical radius, it will remain invariant in time. On the other hand, particles smaller than the critical size will shrink while those larger than the critical size will grow indeﬁnitely.

10.2.6 Temporal Evolution of Two-Phase Microstructures Though the calculation given above was both fun and interesting, it suffered from a number of defects. First, the class of intermediate shapes was entirely restrictive

10.2 Inclusions as Microstructure

541

since we assumed that the only possible shape was spherical. This assumption ignores all possibile instabilities of spherical particles to other shapes. In addition, our treatment of the mechanism of interfacial migration was implicit and was referenced only through the parameter M without any appeal to an underlying mechanism. To remedy these deﬁciencies, we now resort to schemes that can be spelled out in analytic terms, but for which one must have recourse to numerics to make any real progress in explicitly examining the particle shapes. Diffusional Dynamics. In the present analysis, we consider the explicit treatment of diffusion as the mechanism of interfacial migration, with the rate of such diffusion inﬂuenced in turn by the elastic ﬁelds implied by a particular particle shape. As a result, the problem of the temporal evolution of particles is posed as a coupled problem in elasticity and mass transport. The particles are given full scope to develop in any way they want. Our treatment of the temporal evolution of inclusion microstructures will be predicated on the following physical ideas. First, we note that the mechanism of microstructural change that is envisioned is that of mass transport. A given particle, by virtue of its shape and attendant elastic ﬁelds induces a local chemical potential. This chemical potential serves as a boundary condition in our solution of the diffusion equation for the entire medium. The update of the particle shape is based, in turn, upon the concentration gradients resulting from the solution of the diffusion equation with the local velocity increment scaling as vn ∝ ∇c · n. The logic behind this form for the velocity is the claim that the ﬂux of mass to or from the interface is of the form j ∝ ∇c and hence that the normal motion of the interface as a result of this mass ﬂux should scale as ∇c · n. The strategy is essentially iterative since once the particle shape has been altered, the elastic ﬁelds are also changed which demands another solution of the elasticity problem so that the chemical potential can be redetermined and from it, the next shape increment computed. The conceptual philosophy of these calculations is one of instantaneous equilibrium in which it is assumed that at every instant in the temporal history, the equations of mechanical equilibrium are instantaneously satisﬁed. The physical reasoning that is attached to this assumption has the same spirit as the Born–Oppenheimer approximation introduced in section 4.2.2. In particular, there is the expectation of a separation of time scales with the rearrangements (i.e. displacements) that maintain mechanical equilibrium taking place essentially inﬁnitely fast in comparison with the diffusion time. In addition to statements about mechanical equilibrium, it is also assumed that there is an instantaneous chemical equilibrium across the interface. Our discussion follows in a conceptual way (with different notation) that of Voorhees et al. (1992). These statements of equilibrium are imposed as follows.

542

10 Microstructure and its Evolution

Mechanical equilibrium is imposed by demanding that the elastic ﬁelds satisfy ∇ · σ = 0.

(10.51)

We note that just as with our analytic solution for the Eshelby inclusion, the equilibrium equations within the inclusion will have a ‘source’ term (i.e. an effective body force ﬁeld) associated with the eigenstrain describing that inclusion. In addition, we require continuity of both displacements, uin = uout , and tractions, tin = tout , at the interface between the inclusion and the surrounding matrix. The point of contact between the elastic problem and the diffusion problem is the observation that the interfacial concentration depends upon the instantaneous elastic ﬁelds. These interfacial concentrations, in turn, serve as boundary conditions for our treatment of the concentration ﬁelds which permits the update of our particle geometries in a way that will be shown below. The concentration at the interface between the inclusion and the matrix may be written as

1 σ : ]] − σ [[ ]] + γint κ . C = C0 + B [[σ (10.52) 2 Note that C0 is the equilibrium concentration associated with a ﬂat interface, B is a constant term, the two jump terms correspond to the jump in the Eshelby tensor across the interface and the ﬁnal term corresponds to the Gibbs–Thomson term and depends upon the interfacial curvature κ. Having solved the elastic boundary value problem and from it obtained the relevant interfacial concentrations, we are then prepared to obtain the concentration ﬁelds throughout the solid from which we compute the ﬂux to or away from the various particles. Since we are assuming the situation to be quasistatic, the instantaneous concentration ﬁelds must satisfy an equilibrium condition, namely, ∇ 2 c = 0.

(10.53)

This equation follows from our discussion of chap. 7 in which it was shown that in the simplest model of diffusion the concentration ﬁelds must satisfy the diffusion equation, which in the time-independent setting of interest here, reduces to Laplace’s equation. Once the concentration ﬁelds have been obtained we are ﬁnally positioned to update the conﬁguration of the system by recourse to vn = (∇c) · n,

(10.54)

where vn is the velocity of the interface. When the particle shapes have been updated, the procedure is repeated anew. To elaborate on the signiﬁcance of the interfacial concentrations as implied by eqn (10.52), we examine the playing out of these ideas in the context of a spherical particle. The question we pose is how to determine the chemical potential at

10.2 Inclusions as Microstructure

543

the interface between the spherical precipitate and the matrix and from it, the corresponding interfacial concentration. The essential idea is that this chemical potential can be written as µ=

∂G ∂a ∂G = . ∂N ∂a ∂ N

(10.55)

That is, we must compute the free energy change associated with a small excursion of the radius a. The relevant energy is built up of both interfacial and elastic terms as well as a chemical energy that we will ignore. In particular, we can write the free energy as 8πa 3 02 µ 1 + ν 2 , (10.56) G(a) = 4πa γint + 3 1−ν where the ﬁrst term is the interfacial energy associated with a spherical inclusion of radius a and the second term is the elastic energy associated with such an inclusion, as already computed in eqn (10.23). As a result of this insight, the chemical potential is immediate by effecting the derivative ∂G/∂a and exploiting it in the context of eqn (10.55), resulting in

2γint 1+ν , (10.57) + 202 µ µ = at a 1−ν where we have used the fact that for a small excursion of the radius a, the change in the number of particles is d N = ρ4πa 2 da and we introduce the deﬁnition of the atomic volume, ρ = 1/at . Note that the ﬁrst term on the right hand side is the conventional Gibbs–Thomson term relating the chemical potential to interfacial curvature, while the second term represents a purely mechanical effect due to the strain ﬁelds that are present in the system. If we now use the relation between chemical potential and concentration that corresponds to an ideal solution, namely, µ = kT ln(c/c0 ), and expand the resulting exponential, we are left with

c0 at 2γint 1+ν 2 + 20 µ , (10.58) c = c0 + kT a 1−ν a relation precisely of the form of that given in eqn (10.52). We note again that the key point here is that by virtue of solving a problem concerning the instantaneous mechanical equilibrium, we can compute interfacial concentrations which then permit the solution of the diffusion and the calculation of the resulting ﬂuxes which lead to the shape changes of interest. Equilibrium Shapes Revisited. In section 10.2.4, we described the examination of equilibrium shapes. Though the question of equilibrium shapes is one of terminal privileged states, nevertheless, the ideas introduced here which can in

544

10 Microstructure and its Evolution

Fig. 10.21. Series of equilibrium shapes for particles (adapted from Thompson et al. (1994)). The parameter L is a measure of the particle’s size, while a2R is one of the Fourier coefﬁcients that deﬁnes the shape of the particle and is a measure of the deviation away from the circular shape.

principle tell us about temporal evolution, can be used just as well to ﬁnd those terminal states. An example of the type of results that have been achieved with this type of method in two dimensions is shown in ﬁg. 10.21 (Thompson et al. 1994). This result should be contrasted with that of ﬁg. 10.16 which showed the analytic results of Johnson and Cahn in the restricted search over elliptical particle shapes. For the set of calculations shown in ﬁg. 10.21, the elastic anisotropy ratio is chosen to correspond to that of Ni, resulting in elastically soft 100 directions. The eigenstrain associated with the inclusion is assumed to be purely dilatational (i.e. i∗j = δi j ). In the limit of vanishingly small particles, the equilibrium shapes are circular reﬂecting the dominance of the interfacial energy term. With increasing particle size, the solution acquires a fourfold symmetry signaling the increasing relevance of the elastic energy. For yet larger particles, a critical size is reached at which the symmetry is broken resulting in particles with twofold symmetry. Coarsening of Two-Phase Microstructures. As yet, we have made reference to the formulation involving mass transport only in the context of the problem of equilibrium shapes. The method has deeper signiﬁcance in the context of problems involving real temporal evolution such as that of coarsening. Coarsening refers to the increase in size of certain particles at the expense of others. This additional elaboration on the problem of the temporal evolution of a single particle is intriguing since it introduces yet another interesting physical effect, namely, the elastic interactions between different particles which can affect their morphology as well. An example of this process from the experimental perspective is revealed in ﬁg. 10.22 in which Ni3 Si precipitates in a Ni–Si alloy are shown at various times, revealing the marked tendency of certain particles to increase in size while

10.2 Inclusions as Microstructure

545

Fig. 10.22. Series of snapshots of the coarsening of Ni3 Si precipitates in a Ni–Si alloy (adapted from Cho and Ardell (1997)).

others disappear. In addition to changes in particle size, the temporal evolution of this system is also attended by changes in shape as well. In particular, at short times the particles are nearly spherical while at later times they acquire a deﬁnite cuboidal shape. A more quantitative spin on results of the kind noted above can be given such as that shown in ﬁg. 10.23 in which the average particle radius as a function of time is revealed. These data suggest that the particle radius grows via a scaling law of the form r ∝ t 1/3 . In addition to well-developed theoretical ideas such as the theory of Lifshitz–Slyozov–Wagner, understanding of this phenomenon can be developed on the basis of numerical simulations involving a formalism like that described above in which mass transport is treated explicitly, and elastic effects are given full scope to drive the relevant rearrangements of matter. In principle, the coarsening phenomenon was included implicitly in the treatment of temporal evolution given above, though when posed in the numerical terms given above, it is perhaps difﬁcult to attain the sort of understanding that might be wished for blackboard level discussion. Using methods that solve for the same basic physics as has been described earlier in this section, Jou et al. (1997) have carried out a series of two-dimensional studies on the temporal evolution of a distribution of precipitates. Mediated by mass transport that is driven in turn

546

10 Microstructure and its Evolution

Fig. 10.23. Average particle radius as a function of time for coarsening of γ precipitates in Ni–13.23 at.% Al alloy aged at 750 ◦ C (adapted from Ardell (1997)).

by the elastic ﬁelds, their analysis allowed for a numerical examination of the coarsening process with results like those shown in ﬁg. 10.24. Qualitatively, the coarsening process as revealed by the diffusional dynamics introduced above has all the features expected of the coarsening phenomenon, namely, large particles grow at the expense of the small particles which eventually disappear. We close by noting that this section on the microstructure in two-phase solids has illustrated a number of key ideas that can be brought to bear on the question of the spatial and temporal evolution of these structures. The foundational statement for our analysis was given in eqn (10.24) which asserts that the instantaneous conﬁgurational forces derive from both interfacial and elastic energies. We should note that our treatment of the elastic effects in these systems has ignored stresses that are induced by composition variations, though such terms can be included. Similarly, we have also ignored the way in which externally applied stresses can tip the energy balance in favor of particular orientations, breaking the degeneracies between different crystallographically equivalent versions of a given second-phase particle. Finally, we note that some ideas that invoke the diffuse interface concepts introduced in section 9.5 have not been introduced with regard to two-phase microstructures and we alert the reader that concepts like these, with precisely this application in mind, will be featured in our discussion of bridging scales in section 12.4.4. 10.3 Microstructure in Martensites In the previous section, we showed one quantitative scheme for treating microstructure and its evolution. Earlier in the chapter we discussed the geometrical

10.3 Microstructure in Martensites

547

Fig. 10.24. Coarsening of particles in two-dimensional simulation (adapted from Jou et al. (1997)).

characterization of grain structures, and noted the want of a quantitative theory of such microstructure that at the same time admits of analytic progress. One area in which considerable progress has been made is in the study of microstructure in systems which undergo reversible martensitic transformations. What is found in this setting is that on the basis of kinematical constraints and fairly simple nonconvex models of the energetics of the competing phases, a quantitative theory of martensitic microstructure may be laid down which makes veriﬁable predictions. We give special attention to this theory in that it provides an inspirational example of the type of theoretical description that is desirable within the setting of more general microstructures.

10.3.1 The Experimental Situation The class of transformations known as martensitic are those cases in which upon cooling, the system undergoes a spontaneous change of lattice from a high-symmetry parent phase to some lower-symmetry ‘martensite’. These transfor-

548

10 Microstructure and its Evolution

Fig. 10.25. Change in Bravais lattice and well structure associated with the cubic–tetragonal transformation (adapted from Bhattacharya (1991)). U1 , U2 and U3 are the matrices that map the original cubic Bravais lattice into the three tetragonal variants.

mations are distinctive since they occur in a diffusionless manner (sometimes also called ‘displacive’) in which the atoms undergo only local rearrangements while preserving the same distribution of near neighbors. Perhaps the most well-known example of such transformations is that offered by the case of steel. Similar transformations occur in other intermetallic systems such as the cubic–tetragonal transformation in the Ni–Al system and the cubic–orthorhombic transformation in the Al–Cu–Ni system, to name but two. In addition to the geometric signature of these transformations at the lattice scale, even more fascinating (and beautiful) geometric changes are evinced at the microstructural scale. Martensitic microstructures are those in which a partnership has been struck between different variants of a given structure, and possibly the parent phase as well. For the sake of concreteness, consider ﬁg. 10.25 which depicts a transformation between a parent (austenite) phase that is cubic and a tetragonal (martensite) product phase. One of the ﬁrst observations that emerges from the schematic is the presence of multiple degenerate realizations of the martensitic phase. This degeneracy arises from the fact that any of the choices of the original cubic axes serves, by symmetry, as an appropriate axis along which to carry out the tetragonal distortion. As seen in the ﬁgure, the transformation matrices which map the original Bravais lattice vectors onto the transformed Bravais lattice vector are denoted by U1 , U2 and U3 . If our only interest were in the equilibrium crystal structures, our work would already be done. However, if we further interest ourselves in the actual geometric arrangements that are realized in a crystal that has undergone such a transformation, it is evident that the possibility of peaceful coexistence of the different variants results in a richness of structures at the microstructural level.

10.3 Microstructure in Martensites

549

Fig. 10.26. Fine structure at martensite interface (courtesy of Richard James).

An example of the type of martensitic microstructure that can arise when there is more than one degenerate well is given in ﬁg. 10.26. For the moment, we interest ourselves in a particular aspect of these microstructures, namely, the ﬁne structure at twinned interfaces. In particular, this ﬁgure demonstrates the geometry adopted in the Cu–Al–Ni system as the various twins arrive at a second internal interface. The alternating light and dark regions in the ﬁgure correspond to different variants separated by twin boundaries. For the moment, our interest is more in what takes place between these interfaces. To illustrate the types of quantitative questions that can be addressed by the theory of ﬁne-phase microstructures, we ﬁrst elaborate further on the character of these microstructures. As seen above, the martensitic microstructure is characterized by the presence of different variants. However, in the presence of an applied stress, the relative proportion of the different variants can be changed. The experiments are carried out in a biaxial loading apparatus like that shown schematically in ﬁg. 10.27. If we align our Cartesian axes with the two loading directions, then the state of stress to which the sample is subjected can be characterized by the scalars σ1 and σ2 which are a measure of the magnitudes of the load in these two loading directions. A compelling series of snapshots in the type of loading program that can be attained in this biaxial machine are shown in ﬁg. 10.28. What is noted is that, indeed, the stress has the effect of biasing one variant over another. In the ﬁrst frame, the volume fraction of the dark variant is much higher than the lighter one. However, we see that with the decrease in the load σ2 , the light variant begins to grow at the expense of its darker partner. Consequently, one class of questions that

550

10 Microstructure and its Evolution

Fig. 10.27. Schematic of biaxial loading apparatus used to examine stress-induced transformations and resulting microstructures in martensites (courtesy of R. James).

Fig. 10.28. Sequence of snapshots of martensitic microstructure corresponding to different load levels (courtesy of R. James and C. Chu) as obtained using polarized light. Different shades correspond to different variants of the Cu–Al–Ni martensite. Biaxial stress state applied using ¯ directions: (a) σ1 = machine shown in ﬁg. 10.27, with stresses applied along (011) and (011) 7.4 MPa, σ2 = 11.1 MPa, (b) σ1 = 7.4 MPa, σ2 = 9.1 MPa, (c) σ1 = 7.4 MPa, σ2 = 8.3 MPa, (d) σ1 = 7.4 MPa, σ2 = 7.4 MPa, (e) σ1 = 7.4 MPa, σ2 = 6.9 MPa, (f) σ1 = 7.4 MPa, σ2 = 6.2 MPa. Field of view in pictures is roughly 2.5 mm.

10.3 Microstructure in Martensites

551

Fig. 10.29. Illustration of deformation satisfying the rank-one connection condition.

can be posed about these microstructures is how do the volume fractions of the different variants depend upon the state of stress?

10.3.2 Geometrical and Energetic Preliminaries Much of the action associated with the emergence of martensitic microstructures can be traced to kinematic constraints. In particular, on purely geometric grounds, we can identify what types of interfaces are permitted between the austenite and martensite phases, and between the different variants of the martensite itself. It is the aim of the present section to describe these geometric preliminaries in preparation for the theory of ﬁne-phase microstructures which will be given below. Our treatment closely parallels that of Bhattacharya (1998) who in addition to discovering much of what we will say here has codiﬁed a wealth of insights on martensitic microstructure in review article form. We begin by considering the compatibility we will demand across a particular interface. The fundamental physical statement is our insistence on a certain invariant plane such that whether we approach the plane from below or above, when we reach the plane, our prescription for displacing the atoms on that plane will be the same. The reasoning here is illustrated graphically in ﬁg. 10.29. We imagine transformations speciﬁed by the deformation gradients F1 and F2 and ask what constraints must be placed on them in order that the crystals maintain their continuity across the interface between the two transformed regions. As said above, the physical requirement is the existence of a certain invariant plane such that whether or not we use F1 or F2 to compute the transformation on the plane itself we will ﬁnd the same result. The solution to this demand is that the two

552

10 Microstructure and its Evolution

deformation gradients be related by F1 − F2 = a ⊗ n,

(10.59)

the so-called rank-one connection of the pertinent deformation tensors. The vector n is the normal to the putative invariant plane in the reference conﬁguration and a is a vector to be determined. Indeed, another way to see what we have wrought with this equation is to rewrite eqn (10.59) as F1 = F2 + a ⊗ n,

(10.60)

and to note that the action of F1 is the same as F2 except that it picks off the components of vectors normal to the invariant plane. That is, if we take our origin of coordinates somewhere on the invariant plane and ask how F1 acts on the vector r = r# e# +r⊥ n, we see that it is only if r has a nonzero component perpendicular to the invariant plane that the deformation gradients F1 and F2 have a different action on that vector. This guarantees that whether we approach the interface from above or below, the deformation gradients F1 and F2 will agree as to the displacements of atoms (or more generally, of points) on the invariant plane. These ideas are further elaborated in the problem section at the end of the chapter. Part of the beauty of the theory of martensite is the far-reaching implications of the simple geometric constraint represented by eqn (10.59). One of the key results that emerges from this constraint is the nature of the allowed twinning planes that can coexist between different variants of the same underlying martensite. To see this, we must ﬁrst examine in a bit more detail the symmetries present in the energy landscape. For the time being, we interest ourselves in the properties of afﬁne deformations characterized by the deformation gradient F. On the basis of the known transformation strains and the invariances implied by crystal symmetry and overall rotational symmetry, much can already be said about the nature of the energy landscape, φ(F, T ), connecting the austenite and martensite phases. In schematic terms, we know that the energy as a function of the deformation gradient F has the basic character depicted in ﬁg. 10.30. Note that this energy is something that can in principle be evaluated directly on the basis of microscopic calculation. Indeed, we have already shown an example of such a calculation in ﬁg. 4.1. The basic point of a free energy like that mentioned above is that at high temperatures, the energy landscape is characterized by a global minimum for F = I (i.e. the austenite is the most stable structure). On the other hand, below the critical temperature, there are a number of degenerate wells corresponding to the different variants of martensite, F = Ui . Of course, in the ﬁgure, the set of possible deformations has only been indicated schematically since we have represented the deformation gradient as a scalar, and in reality, such deformations are characterized by the nine parameters needed to specify the full deformation gradient. From the

10.3 Microstructure in Martensites

553

Fig. 10.30. Schematic representation of the relative positions of competing minima in the energy landscape as a function of temperature (courtesy of K. Bhattacharya). φ(F, T ) is the free energy function, which depends upon both the deformation gradient F and the temperature T , U1 and U2 are the deformation gradients associated with the two martensite variants considered in this ﬁgure and the identity I is associated with the austenite well.

present standpoint, the key feature of the energy function φ that gives rise to the existence of microstructures is the presence on its energy landscape of multiple wells. As was said before, it is the degeneracy of different martensitic variants that makes it possible for one region of the microstructure to have selected one variant and some other region to have selected another. An alternative way to characterize the various wells is through the device of the James diagram in which each well is characterized by a circle like those shown in ﬁg. 10.31. The point of such diagrams is to represent a crucial feature of the symmetry of the stored energy function φ(F, T ). Material frame indifference requires that φ(F, T ) = φ(RF, T ), the meaning of which is that if we ﬁrst apply the deformation gradient and then rotate the resulting crystal, the energy is the same as if we had only applied the deformation gradient itself. The signiﬁcance of this insight is that the additional freedom associated with the ability to apply rotations broadens our scope to ﬁnd compatible interfaces between the different variants. As shown in the ﬁgure, each well is identiﬁed by a different circle, with the circle meant to indicate the entire group of allowable rotations R, namely, S O(3). Though F1 and F2 themselves may not satisfy the rank-one connection, material frame indifference illustrates that it is possible to ﬁnd a rotation R such that RF1 and F2 do satisfy the rank-one condition, and it is this additional freedom that is conveyed by the James diagram.

554

10 Microstructure and its Evolution

Fig. 10.31. Schematic illustration of deformation gradients in different wells for the cubic to tetragonal transformation that satisfy the rank-one connection condition (adapted from Ball and James (1992)).

As was shown in ﬁg.10.25, for the case of the cubic–tetragonal transformation there are three distinct wells to be considered, each corresponding to the tetragonal distortion occurring along a different Cartesian direction. Recall that our discussion of compatibility culminated in eqn (10.59). Part of the virtue of the James diagrams is that they provide a geometrical representation of part of the information content of eqn (10.59). What we note is that compatible deformations on different wells can be signiﬁed by connecting them with a line as shown in ﬁg. 10.31. In particular, what ﬁg. 10.31 tells us is that while there is no rank-one connection between U1 and U2 , for example, there is a rank-one connection of the form U2 − Rα U1 = a ⊗ n, where we have introduced the notation Rα to signify the particular choice of R on the U1 well that results in a rank-one connection to well U2 . The dotted lines in the ﬁgure connect two rank-one connected deformation gradients on different wells. To see all of these ideas in action, we now turn to a consideration of some of the many different types of compatible interfaces that can be found in martensitic systems.

10.3.3 Twinning and Compatibility The questions we will pose in this section concern the ability of different energetically favorable structures to coexist geometrically. We have already seen that the conﬂuence of two key ideas gives rise to the possibility for diverse microstructures. In particular, the identiﬁcation of a series of degenerate energy wells makes it possible that, for example, a cubic crystal will transform into several different (but

10.3 Microstructure in Martensites

555

Fig. 10.32. Schematic of interface between structures characterized by deformation gradients F1 = R1 U1 and F2 = U2 .

energetically equivalent) variants. On the other hand, we have also seen that it is not evident a priori that a compatible interface can be formed between both the different variants and the host austenite. To explore this question further, we require compatibility equations which specify under what conditions a compatible interface may be formed between two structures, each characterized by its own well. In ﬁg. 10.32, we indicate the type of interface we have in mind. On one side of the interface, the structure is characterized by a deformation gradient R1 U1 while on the opposite side of the interface the deformation is characterized by a deformation gradient U2 . Note that without loss of generality, we have rewritten the compatibility condition in terms of the stretch tensors U1 and U2 and a single rotation R1 . For a given set of structures characterized by the matrices U1 and U2 our question may be posed as: can we ﬁnd a rotation R1 as well as vectors a and n such that the condition R1 U1 − U2 = a ⊗ n,

(10.61)

is satisﬁed? Recall that in formal terms this is precisely the compatibility condition developed earlier and identiﬁed as the rank-one connection. We answer this question in the form of a theorem which asserts that if the eigenvalues of the matrix −1 T U−T 2 U1 U1 U2 may be ordered as λ1 ≥ 1, λ2 = 1 and λ3 ≤ 1, then there exists a rank-one connection. For details, see Proposition 4 of Ball and James (1987). From a physical perspective, we note that the signiﬁcance of this result is that the compatibility condition introduced above can only be satisﬁed for certain special choices of lattice parameters, a theme that will recur repeatedly in our discussion of martensitic microstructures.

556

10 Microstructure and its Evolution

−1 T If the eigenvalues of the matrix C = U−T 2 U1 U1 U2 satisfy the conditions described above, then we may go further and compute the vectors a and n as well as the rotation matrix. In particular, we assert that the vector a is given by

λ3 (1 − λ1 ) λ1 (1 − λ3 ) (10.62) e1 ± e3 , a=c λ3 − λ1 λ3 − λ1

while the vector n is given by √ √ λ3 − λ1 (− 1 − λ1 U2T e1 ± λ3 − 1U2T e3 ). n= √ c λ3 − λ1

(10.63)

Note that there are two solutions corresponding to the ± sign in our equations. In addition, the requirement that n be normalized is satisﬁed by exploiting the as-yet undetermined constant c. To determine the rotation matrix, we substitute the values for a and n back into eqn (10.61) and solve for R1 . Our intention in the remainder of this section is to build up a picture of some of the various interfaces that are present in martensitic systems. Our approach will be to consider microstructural elements of increasing complexity, beginning ﬁrst with the case of the simple austenite–martensite interface and culminating in the investigation of martensitic wedges within the host austenite. In all of these cases, the primary theoretical engine in our analysis will be the compatibility conditions and their outcome as typiﬁed by eqns (10.62) and (10.63). Austenite–Martensite Interfaces. As a ﬁrst exercise in the machinery set forth above, we pose the question of whether or not a simple interface can exist between a cubic crystal and its tetragonal offspring. Without loss of generality, this situation can be represented via the condition RU − I = a ⊗ n, where the matrix U is of the form

α 0 0 U = 0 β 0 . 0 0 β

(10.64)

(10.65)

For the special choice of stretch matrix U made here, all we are saying is that to produce the tetragonal crystal, all one need do is stretch by a factor α along the x-direction and by a factor β along the y- and z-directions. That is, the crystal axes of the cubic and tetragonal variants are parallel. Note that in light of the theorem set forth above, all that remains is to ask how the eigenvalues of the matrix C = U2 are ordered. However, since the matrix is already diagonal, we know that its eigenvalues are λ1 = α 2 , λ2 = λ3 = β 2 .

10.3 Microstructure in Martensites

557

For concreteness, we assume that α > 1 > β as is the case in systems such as In–Tl (α = 1.0221 and β = 0.9889) and Ni–Al (α = 1.1302 and β = 0.9392). As a result, we note that there is not an ordering of the eigenvalues of the form λ1 ≥ λ2 = 1 ≥ λ3 , which immediately lends itself to the conclusion that in the case of a cubic–tetragonal transformation, there is no simple interface between the host austenite and a single variant of the tetragonal martensite except in the unlikely event that the parameter β takes the value 1.0. Martensite–Martensite Interfaces. At the next level of complexity, we consider the nature of the interfaces that characterize the coexistence of different martensitic variants. In this case, the compatibility condition takes the more general form given earlier in eqn (10.61) where for explicitness we choose α 0 0 U1 = 0 β 0 (10.66) 0 0 β and

β 0 0 U2 = 0 α 0 . 0 0 β

(10.67)

Once again, our exercise is reduced to that of determining the eigenvalues of the matrix C. In the case in which the different variants in question are described by U1 and U2 as given above, the matrix C is of the form 2 2 0 0 α /β (10.68) C= 0 β 2 /α 2 0 . 0 0 1 In this case, we ﬁnd that the eigenvalues are precisely arranged so as to allow for the existence of a martensitic interface between the two variants in question. The question of the martensitic interface can be further explored by recourse to the equations that determine the vectors a and n themselves. In particular, by exploiting the results spelled out in eqns (10.62) and (10.63), we see that in the cubic–tetragonal case under consideration here, the vectors a and n are given by a=

√ β 2 − α2 2 2 (β, ±α, 0) β + α2

(10.69)

and 1 n = √ (−1, ±1, 0). 2

(10.70)

What we have learned from this analysis is that the invariant plane allowing for

558

10 Microstructure and its Evolution

Fig. 10.33. Schematic of interface between twinned martensite and the parent austenite (adapted from James and Hane (2000) and Chu (1993)).

the development of an interface between two different variants of the tetragonal martensite is of the (1, 1, 0)cubic -type. Austenite in Contact with Twinned Martensite. An even more interesting example is that of an interface between austenite and a twinned version of the martensite. In this case, the strategy is to satisfy the conditions of compatibility across the austenite–martensite interface in an average sense. The geometry of interest is indicated schematically in ﬁg. 10.33. Recall that in the case of the cubic–tetragonal system, we could ﬁnd no interface between the host austenite and a single variant of martensite. In the present context, the idea is to seek an average deformation gradient F = λF1 + (1 − λ)F2 that satisﬁes the compatibility condition. Note that here λ is not an eigenvalue of the matrix C, but is rather the volume fraction of F1 . For simplicity, we take the deformation gradient in the austenite to be the identity I, while the two variants of martensite are characterized by RU1 and U2 . The compatibility condition within the twinned martensite region is nothing more than was written earlier and takes the speciﬁc form RU1 − U2 = a ⊗ n.

(10.71)

In addition to this constraint, we must also satisfy compatibility across the austenite–martensite interface which in light of the deformation gradients speciﬁed

10.3 Microstructure in Martensites

559

above may be written R (λRU2 + (1 − λ)U1 ) − I = b ⊗ m.

(10.72)

The latter of these equations is sometimes referred to as the habit-plane or austenite–martensite equation. This equation imposes the rank-one connection across the austenite–martensite interface, with the rotation R governing the overall orientation of the twinned martensite with respect to the austenite across the austenite–twinned-martensite interface. We also note that this equation embodies the classic results of the crystallographic theory of martensite as expounded in Wayman (1964), though now interpreted energetically in terms of the various energy wells available to the system. As it stands, we must determine the matrices R and R , as well as the vectors a, b, n and m and the mixing parameter λ, given our knowledge of the tensors U1 and U2 . To do so, we resort to a divide and conquer strategy in which ﬁrst we solve eqn (10.71) using exactly the same technique described earlier and culminating in the solutions of eqns (10.62) and (10.63). Once these solutions are in hand, we then turn to a solution of eqn (10.72). The key point concerning this solution for our present purposes is that it depends critically on particular choices of the relevant lattice parameters. In particular, as shown in Ball and James (1987) and explained in James and Hane (2000), necessary and sufﬁcient conditions for the existence of a solution are δ ≡ a · U2 (U22 − I)−1 n ≤ −2

(10.73)

and |a|2 ≥ 0. 2δ The resulting volume fraction λ of variant 1 is given by 2 1 1− 1+ . λ= 2 δ η ≡ tr(U22 ) − det(U22 ) − 2 +

(10.74)

(10.75)

The dependence of the volume fraction λ on the parameter δ shows that it too is material speciﬁc and depends upon the particular values of the various lattice parameters. Wedge Structures. As our ﬁnal exercise in examining the conjunction of energetic and compatibility arguments, we consider the case of wedge-like structures in which a series of twins are arranged in such a way that a wedge of martensite can be embedded within austensite. The situation we have in mind is depicted schematically in ﬁg. 10.34. We also note again that our discussion leans heavily on that of Bhattacharya (1991) who considered the issue of wedges in martensite in detail.

560

10 Microstructure and its Evolution

Fig. 10.34. Schematic of a martensite wedge embedded within an austenite structure (adapted from Bhattacharya (1991)).

From the standpoint of the kinematic arguments introduced earlier, the additional complexity that attends situations such as the wedge microstructure considered here is the fact that we no longer have only a single interface on which to satisfy the conditions of compatibility. Our calculations on the austenite–twinnedmartensite interface served as a warm up exercise for the present case. Each and every interface of the type in ﬁg. 10.35 must itself satisfy conditions such as that of eqn (10.59). As a result, the imposition of compatibility across all of the interfaces takes the form of the collection of equations A − B = a1 ⊗ n1 ,

(10.76)

C − D = a 2 ⊗ n2 ,

(10.77)

λ1 A + (1 − λ1 )B − λ2 C − (1 − λ2 )D = a3 ⊗ m,

(10.78)

λ1 A + (1 − λ1 )B − I = a4 ⊗ m1 ,

(10.79)

λ2 C + (1 − λ2 )D − I = a5 ⊗ m2 .

(10.80)

Like in the simpler case of the interface between an austenite region and twinned martensite, this set of equations can be solved by recourse to a divide and conquer policy. Our main interest in showing these equations is to show the reader what is involved in setting up such a problem and to inspire him or her to read Bhattacharya’s beautiful 1991 paper.

10.3.4 Fine-Phase Microstructures and Attainment We have now structured the problem of martensitic microstructre in accordance with key geometric and energetic notions. What we have seen is that once the

10.3 Microstructure in Martensites

561

Fig. 10.35. Detailed schematic of the variants within a martensite wedge which is itself embedded within an austenite structure (adapted from Bhattacharya (1991)).

energy wells have been identiﬁed, largely on the basis of geometric arguments it is possible to classify the various types of interfaces that can be realized within a given microstructure. We now pose the deeper question of the character of the overall microstructure itself. For example, what are the volume fractions of the different variants, and what features of the problem determine the typical length scale associated with these variants? The answer to such questions demands a discussion of the subtlety that can attend the notion of minimization of the type of nonconvex energies introduced above. For the present purpose, our ﬁrst observation is that under certain circumstances, it is possible that the minimizer will be represented as the limit of a sequence of increasingly ﬁne microstructures. Alternatively, this can be stated by noting that in some cases there are no smooth deformations that minimize the energy. Instead, we extend the space of possible minimizers by including those deformations which are piecewise continuous and are allowed to have a vanishingly small thickness. A two-dimensional model problem described in depth by Bhattacharya (1998) which illustrates this idea is built around the idea of trying to ﬁnd a scalar ﬁeld y(x1 , x2 ) that minimizes the free energy functional φ(∇ y(x1 , x2 ))d x1 d x2 , (10.81) E[y(x1 , x2 )] =

subject to the boundary condition that y = 0 on the boundary ∂ of the body . To make the problem interesting, the free energy itself is chosen to have two wells,

562

10 Microstructure and its Evolution

and is of the form

φ(∇ y(x1 , x2 )) =

∂y ∂ x1

2

2 −1

+

∂y ∂ x2

2 .

(10.82)

The free energy density given above has two wells, corresponding to ∂ y/∂ x1 = ±1 and ∂ y/∂ x 2 = 0. In addition to the speciﬁcation of the free energy itself, our problem is supplemented with the boundary condition that the deformation vanish on the boundary of the region. We see that this free energy functional and the associated boundary conditions pose contradictory demands on the deformation mapping y(x1 , x2 ), resulting in a lack of ‘attainment’, a word that signiﬁes that the class of continuous deformations is unable to provide a minimizer, even though the free energy is bounded from below. To see this, we note that on the boundaries we would like to choose y = 0. On the other hand, within the ‘volume’ , the choice y = 0 is energetically unfavorable since it corresponds to a choice of ∇ y that deﬁnitely does not occupy either of the wells. Hence, we are unable to attain the minimum with any continuous deformation. On the other hand, using the construction to be described below, we can get as close as we like to the state of zero energy by considering ever ﬁner mixtures of the two variants. It is evident at the outset that there is no continuous deformation that minimizes this energy function. On the other hand, we can also note that by adopting the approach of setting up a series of piecewise continuous deformations with a corresponding energetic boundary layer near the boundaries, we can construct structures that approach the lowest energy to within arbitrary accuracy. This construction is revealed pictorially in ﬁg. 10.36, and illustrates the enlargement of our space of solutions to include so-called minimizing sequences. The idea is to build up the overall microstructure by considering strips with ∇ y = (1, 0) and ∇ y = (0, 1). In each of these strips, the contribution to the overall energy is zero. On the other hand, these strips fail to satisfy the boundary condition (y = 0) at x2 = 0 and x2 = L, where L is the dimension of the region of interest. As seen in ﬁg. 10.36, the remedy to this problem is to cut the strips off at the ends so they vanish at x2 = 0 and x2 = L. Of course, in so doing, we must pay an energy penalty for this boundary layer since in these regions ∇ y is not associated with either of the energy wells. In fact, as shown in Bhattacharya (1998), the energy associated with this boundary layer is of the form E layer = L 2 /2n, where n is an integer that characterizes how many strips are present in our microstructure. This demonstrates that the boundary layer contribution to the energy goes to zero in the limit that the ﬁneness of our microstructure is increased without bound. As a result of the arguments set forth in this part of the chapter, we are now prepared for the job of evaluating the structure and energetics of martensitic microstructures. The fundamental idea is to construct arrangements of the different

10.3 Microstructure in Martensites

563

Fig. 10.36. Illustration of two members of the minimizing sequence for two-dimensional problem posed in the text (adapted from Bhattacharya (1998)).

variants that simultaneously satisfy the geometric constraints associated with the rank-one connection and the energetic constraints introduced by presence of the pertinent free energy function. The discussion given above centered on the use of analytic reasoning to deduce the general characteristics of martensitic microstructures. Such analytic investigations have been complemented successfully using numerical solutions in which minimizers of the relevant free energy functional are sought after by recourse to a ﬁnite element description of the deformation ﬁelds (see Luskin (1996) for example). An example of the type of results that emerge upon implementing the ideas of the previous few sections in a numerical sense is

564

10 Microstructure and its Evolution

Fig. 10.37. Outcome of numerical calculation of the energy minimizers associated with martensite (adapted from Luskin (1996)): (a) an example of a ﬁnite element mesh used to model the martensitic microstructure, (b)–(d) the results of microstructure computations using different levels of mesh reﬁnement.

shown in ﬁg. 10.37. These calculations were made for a two-dimensional model free energy which is intended to mimic the energetics of the three-dimensional orthorhombic to monoclinic transformation. The calculations are made for a square geometry in which the boundary deformation gradient is prescribed and corresponds to neither of the competing wells. Like in the model problem resulting in ﬁg. 10.36, this choice of boundary condition guarantees the type of nonattainment described above. Though we will not elaborate on this point in any great detail, it is important to note that on physical grounds there is a lower cutoff to the type of runaway reﬁnement of the microstructure described above. Recall that our assessment of the free energy has until now been predicated entirely upon searching for a means to minimize the elastic contributions to this energy subject to particular boundary conditions. On the other hand, it is clear that the increased level of reﬁnement

10.3 Microstructure in Martensites

565

is accompanied by energy penalties associated with the various interfaces, terms which we have so far ignored. As said above, the physical consequence of these terms is to regularize the problem and to impose a length scale resulting from the balance of the surface energy and the elastic energy associated with the boundary layers in which the deformations are not associated with either the austenite or martensite wells.

10.3.5 The Austenite–Martensite Free Energy Reconsidered In ﬁg. 10.30, we gave a schematic description of the free energy as a function of deformation gradient for various temperatures above, below and at the transformation temperature. This discussion was built upon an intuition of what the basic character of the free energy must be in order to give rise to the phenomenology of these systems. We now reconsider the question of the alloy free energy from the perspective of chap. 6, with the aim of trying to explicate such free energies on the basis of microscopic calculation rather than on the phenomenological grounds introduced earlier in this chapter. For the present purposes, we write the free energy φ(F, T ) as a sum of two terms: φ(F, T ) = Fel (F, T ) + Fvib (F, T ),

(10.83)

where the ﬁrst term is the electronic contribution to the free energy of structures characterized by the deformation gradient F, while the second term is the vibrational contribution to the free energy, and it too depends upon the state of deformation. This equation is essentially an imitation of that given already as eqn (6.2). For an assessment of the ﬁrst term, we turn to a discussion of the so-called Cauchy–Born rule introduced in section 5.4.2, while for the second, we will revisit experiments on the free energy of structural transformations. For the purposes of computing Fel (F, T ), we can exploit the Cauchy–Born rule, as was done in the calculations leading to ﬁg. 4.1. Such calculations are conceptually simple in comparison with some of the more complex defect calculations introduced elsewhere throughout the book. All that one need do is take the original Bravais lattice (i.e. the reference state), deform the relevant basis vectors according to the prescription given above and compute the resulting energy using one’s favorite total energy scheme. We will not belabor the point other than by noting that the basic character of the results will resemble those of ﬁg. 4.1 in the sense that there can be more than one local minimum.

566

10 Microstructure and its Evolution

To compute the vibrational contribution to the free energy, we remind the reader of the results of chap. 6 in which we argued that entropy contributions can arise from vibrations (both harmonic and anharmonic) as well as electronic excitations. For the moment, we will advance the hypothesis, supported in some cases by experiment (see ﬁg. 10.38), that in the context of martensitic transformation the contribution of harmonic lattice vibrations to the entropy will tell most of the story. Further, our interest is in sketching ideas, in suggesting possible origins for effects rather than being exhaustive, and hence perhaps an overly facile representation of a rather complex problem can be forgiven. In the context of the Cu–Zn–Al system, a series of measurements were undertaken (Ma˜nosa et al. 1993) with the aim of sorting out the relative importance of the various contributions mentioned above to the overall entropy of transformation. In a word, their method was to use calorimetric techniques to obtain the total entropy. Using magnetic susceptibility measurements it is possible to independently pick off the electronic contribution to the total entropy which is known already from the calorimetric measurements. Finally, by taking the difference between this electronic contribution and the total entropy it is possible to compute the vibrational contribution to the entropy. Fig. 10.38 shows both the electronic (Se ) and vibrational (Sv ) contributions to the entropy in a series of different Cu–Zn–Al alloys. As is seen in ﬁg. 10.38, the magnitude of the vibrational entropy (and this is itself almost all harmonic) is quite large in comparison with that due to electronic degrees of freedom as is evidenced by comparing the scales of the two contributions. The conclusion to be drawn from these experiments is that in this case we can go a long way towards deducing the type of free energy function shown in ﬁg. 10.30 by combining what we know about the zero-temperature part of Fel (F, T ) (i.e. the zero-temperature structural energies) and the free energy of harmonic vibrations.

10.4 Microstructural Evolution in Polycrystals Our third and ﬁnal microstructural example centers on the question of polycrystals and their temporal evolution. Here we imagine the perfect crystal disturbed not by the presence of other phases, but rather by a series of grain boundaries separating crystalline regions each having a different orientation. We have already hinted at the implications of such a polycrystalline microstructure for the mechanical properties of a material. The aim of the present section is to examine how such microstructures evolve in time. We will begin with an examination of the observations that have been made on such microstructures, with an emphasis on the quantitative features of their temporal evolution. This will be followed by a reexamination of the driving forces that induce grain boundary motion as well as the mechanisms whereby such motion is realized.

10.4 Microstructural Evolution in Polycrystals

567

Fig. 10.38. Entropy difference between austenite and martensite in Cu–Zn–Al alloys (adapted from Ma˜nosa et al. (1993)). Different values of the electron per atom ratio correspond to different concentrations of the three alloy constituents.

10.4.1 Phenomenology of Grain Growth One of the palpable effects of annealing a polycrystal is a systematic change in the mean grain size, a phenomenon known as grain growth. A quantitative view of this process is evoked by plotting the mean grain size as a function of time as shown in ﬁgs. 10.39 and 10.40. Though we will not enter into the debate (for further details see Atkinson (1988)), the question of how to characterize three-dimensional microstructures on the basis of two-dimensional cuts is a subtle one. A more satisfying kinematic framework for characterizing polycrystalline microstructures, and grain growth in particular, is offered by considering the entire grain size distribution rather than just the mean grain size itself. In particular, consider the function F(R, t) which is the probability density for ﬁnding grains of size R within the microstructure. In particular, F(R, t) gives the number of grains per unit volume with size between R and R + d R at time t. Just as the mean grain size is amenable to experimental evaluation, so too is the grain size distribution function as shown in ﬁg. 10.41. One of the claims associated with these distribution functions is that they can nearly be thought of as lognormal

568

10 Microstructure and its Evolution

Fig. 10.39. Evolution of grain size as a function of time during the annealing process (adapted from Rhines and Craig (1974)). The vertical axis reveals the average grain volume as obtained by taking the reciprocal of the number of grains per cubic centimeter.

distributions. Perhaps more important yet is the assertion of a scaling property of the grain size distribution function. In particular, if the grain size is plotted, not in terms of the absolute size of the various grains, but rather in terms of the normalized grain size R/R (where R is the mean grain size, labeled by R¯ in the ﬁgure), then the distribution is statistically invariant. Exactly this point is made in ﬁg. 10.41 which shows the grain size distribution using scaled variables for various times in the temporal history of the microstructure. The process of grain growth bears some resemblance to the coarsening process discussed earlier in the context of precipitate microstructures. From the point of view of the driving force for such structural change, as we have repeatedly emphasized, such microstructures are metastable. A state of lower free energy may be reached by eliminating grain boundary area. By virtue of the presence of a variety of grain boundaries, it is plausible to imagine a state of lower free energy in which there are fewer such boundaries, and hence a lower overall boundary energy. One of the challenges posed by such microstructures is the way in which such metastable systems evolve in time.

10.4.2 Modeling Grain Growth As noted above, ostensibly, part of the empirical background concerning grain growth that demands explanation is the power law growth in time of the grain size. One of the justly famous contributions in that regard is the work of Burke

10.4 Microstructural Evolution in Polycrystals 99.9999% Cd

569

240 C

1.4 1.2

D (mm)

1.0 0.8 0.6 0.4 0.2

(a)

25

75

175

225

240 C

D2-D2 (mm2) 30

99.9999% Cd

125

(b)

Fig. 10.40. Evolution of grain size as a function of time during the annealing process (adapted from Simpson et al. (1971)). The parameter D is a measure of the grain size. In the lower frame the grain growth data are plotted with respect to t − t0 , where t0 is the time from which the subsequent grain growth is measured.

and Turnbull (1952) in which a parabolic growth law in which the mean grain 1 size scales as R ∝ t 2 was deduced on the grounds of arguments much like those leading to our eqn (10.48). The basic hypotheses behind the Burke–Turnbull argument are that the properties of the distribution itself can be understood by concentrating on the properties of one grain only, and that this one grain evolves under the action of curvature-induced forces. Recalling the variational statement of ˙ the variational eqn (10.45), but now treating only the interfacial contribution to G,

570

10 Microstructure and its Evolution

Fig. 10.41. Scaled grain size distribution function for various times in annealing history of sample of Fe (adapted from Pande and Marsh (1992)). In addition to the experimental results, the ﬁgure also shows the lognormal and Rayleigh distributions thought to be relevant to describing the distribution F(R, t).

principle can be written as ˙2 ˙ R). ˙ R) = 4π R 2 R + G˙ int ( R; ( R; 2M

(10.84)

On the assumption of an isotropic interfacial energy γint , G˙ may be written ˙ int . Following the usual procedure (i.e. (see eqn (10.46)) as G˙ int (R) = 8π R Rγ ∂/∂ R˙ = 0) results in an equation for the evolution of R of the form 2Mγint dR =− , dt R which when integrated yields the grain size scaling relation

(10.85)

1 2 1 2 R − R0 = −2Mγint t. (10.86) 2 2 Highly idealized arguments like that given above have been complemented by more realistic numerical simulations in which the various interfaces move in conjunction. Since our aim is the illustration of ideas rather than to exhaustively detail the ultimate solution to particular problems, we will take up three distinct schemes for considering the problem of microstructural evolution in the grain growth setting. The three paradigmatic examples to be considered here are shown in ﬁg. 10.42. Our intention is to consider in turn the Potts model approach to grain growth, phase ﬁeld models for grain growth and their sharp interface

10.4 Microstructural Evolution in Polycrystals

571

Fig. 10.42. Schematic of various paradigms for considering the evolution of polycrystal (adapted from Frost and Thompson (1996)). The upper panel shows the representation of the polycrystal from the perspective of each of the different models and the lower panel illustrates the way in which the interfaces between different grains migrate.

counterpart. As will be seen in the coming sections, each of these schemes has a different underlying philosophy, though they all attempt to capture the energy penalty associated with the presence of interfacial areas. Potts Models of Microstructural Evolution. Perhaps the simplest representation of the energetics of grain growth is provided by the so-called kinetic Monte Carlo models of grain growth. Here a model Hamiltonian is set forth that provides an energy penalty for all interfaces within the microstructure. The basic idea is to exploit the Potts model which is highly reminiscent of the Ising model. In concrete terms, the model is set up as follows. An order parameter σi is introduced which labels the orientation of the i th grain. Each possible orientation within the model is assigned a different integer. This kinematic scheme allows for each different orientation within the polycrystal to be represented by a different integer, though clearly the continuous set of misorientations has been replaced with a discrete (and ﬁnite) approximation. Note that the lattice considered here is not a crystalline lattice but rather a modeler’s lattice and represents a spatial discretization of the microstructure that is presumed ﬁne enough to capture the essential features of grain growth while at the same time being coarse on the scale of the lattice parameter. One scheme for deciding upon a length to associate with the lattice in the model is through reference to the typical curvatures that must be accounted

572

10 Microstructure and its Evolution

Fig. 10.43. A Potts microstructure in which different grains are identiﬁed by different values of the occupation number σ (adapted from Anderson et al. (1984)).

for in the lattice model of the microstructure. A Potts microstructure using the kinematic description of the microstructure described above is shown in ﬁg. 10.43. One means to generate such a microstructure is to select a series of grain centers, each of which will have a different orientation, set up the corresponding Voronoi tiling and then specify each grain according to its occupation label. As yet, the model is purely descriptive and says nothing about the possible subsequent evolution of the microstructure. To endow this geometric model with an underlying ‘dynamics’, we ﬁrst require a statement of the energetics. One conventional choice is a Hamiltonian of the form Ji j (1 − δσi ,σj ), (10.87) H= ij

where the sum is over lattice sites in the model and Ji j is an energy parameter that essentially mimics the grain boundary energy. A given grain is made up of many lattice sites, and the energy penalty implied by eqn (10.87) is associated with changes in the local spin variables from one lattice site to the next corresponding to the presence of a grain boundary. What the Hamiltonian tells us is that if two neighboring lattice sites i and j are identical (i.e. δσi ,σj = 1) then there is no associated energy penalty. On the other hand, if the neighboring sites have different values of σ , then there will be an energy cost parameterized by Ji j . In the general form with which the Hamiltonian was written above, each type of interface characterized by a different pair i j potentially has a different energy Ji j . However, a simpler realization of the model is to consider a single value J of the Potts coupling parameter which is equivalent to attributing an isotropic interface energy to the grain boundaries.

10.4 Microstructural Evolution in Polycrystals

573

The temporal evolution of a microstructure (i.e. grain growth) is examined by recourse to Monte Carlo methods. A trial change in occupation number is selected. If the move results in a net reduction of the energy, it is accepted. If not, it is accepted with a probability given by a Boltzmann weight. As a result of this ‘dynamics’, the trend is towards states of lower overall energy which in the context of the present model of energetics means less overall grain boundary area. A series of snapshots in a Potts microstructure as computed in this manner is shown in ﬁg. 10.44. One of the ways in which these results can be examined is from the perspective of the types of experiments on grain growth described earlier in this section. In particular, it is possible to monitor the grain size as a function of time.

Phase Field Models for Grain Growth. One of the complaints that can be registered about the type of analysis given above is the fact that the underlying dynamics is not really tied to the physics of interfacial motion. A partial remedy for this problem is provided by a second class of models that we will feature several times, namely, phase ﬁeld models. Note that these models are the logical extension of the ideas introduced in section 9.5. In this setting, the set of orientations corresponding to the polycrystalline microstructure is associated with a collection of ﬁeld variables (i.e. order parameters) ηi (r, t), with each ηi corresponding to a different orientation. The total energy of the system is written in such a way that its minimizers (i.e. there is only a single orientation present) are of the form that either ηi = 1 or ηi = −1 and all the other η j s are zero. Further, there is an energy penalty associated with spatial variations in the ﬁelds ηi which can be construed as an interfacial energy. Note that in this setting the interface is endowed with a ﬁnite width of the type described in the previous chapter and shown in ﬁg. 9.50. It is also worth noting that there are signiﬁcant similarities between the continuum model set forth here and the Potts model described above. To be concrete, one scheme that has been used to model grain growth in the phase ﬁeld setting is to identify a set of N ﬁeld variables (η1 (r, t), η2 (r, t), . . . , η N (r, t)) corresponding to 2N distinct orientations (since each ηi can assume the values ±1). The kinematic idea of such models is illustrated in ﬁg. 10.45 which shows the ‘interface’ between two different grains. As said above, the generalization to the situation involving more orientations is built around having a larger number of ﬁelds. Once these kinematic preliminaries have been settled, the total free energy functional is then written as the integral f [{ηi (r, t)}] =

[ f 0 ({ηi (r, t)}) +

κi i

2

(∇ηi (r, t))2 ]d 3 r.

(10.88)

574

10 Microstructure and its Evolution

Fig. 10.44. Series of snapshots in the life history of a Potts microstructure (courtesy of E. Holm): (a)–(d) represent various stages of the time evolution of this system.

The term f 0 is written explicitly as f 0 ({ηi (r, t)}) = −

α 2 β 4 ηi + ηi + γ ηi2 η2j , 2 i 4 i i j>i

(10.89)

which has energy wells corresponding to a given ηi being ±1 while all of its competitors are zero. The interpretation of the gradient term is relatively straightforward and imposes an energetic penalty for variations in the ﬁelds {ηi (r, t)} with a length scale set by the parameters {κi }. To summarize, the energetics set forth

10.4 Microstructural Evolution in Polycrystals

575

Fig. 10.45. Representation of the ‘interface’ region between different grains, one characterized by η1 (x) and the other by η2 (x).

above has two key features. First, there is a preference for one of the ηi s to be ±1 with all others zero. The demonstration of this point is taken up in the problem section at the end of the chapter. Secondly, the gradient term assigns an energy penalty to the ‘interfaces’ between regions in which the order parameter ﬁeld is different. That is, in passing from one grain (say ηi = 1) to another (say η j = 1), the order parameter ﬁeld will vary smoothly between 1 and 0 with a corresponding energy penalty for this interface. The basic idea of the phase ﬁeld approach is to play out this competition in a continuum setting. In addition to the deﬁnition of the energy functional, it is necessary to institute a dynamics associated with a model of this sort. In the present setting, the dynamics is obtained by asserting that the temporal evolution of a given ﬁeld variable is linear in the driving force, namely, δf ∂ηi (r, t) = −L i + ζi (r, t), ∂t δηi (r, t)

(10.90)

where the parameter L i is a kinetic coefﬁcient that modulates the driving force. ζi is a noise term which is intended to mimic the effects of thermal ﬂuctuations. We will return to the subject of gradient ﬂow dynamics like that introduced here in more detail in chap. 12. Notice that one of the challenges of a model of this type is that there are as many equations as there are components to the order parameter. As a result, for the simulation of a polycrystal with many different grains, there will be as many ﬁeld variables as there are grains resulting in both conceptual and computational

576

10 Microstructure and its Evolution

Fig. 10.46. Phase ﬁeld model for two-dimensional grain growth (adapted from Chen and Wang (1996)). Figure shows grain distribution at various times in the evolution of the grain structure with: (a) t = 1000, (b) t = 3000, (c) t = 5000 and (d) t = 8000. Time is measured in units of how many integration steps have taken place.

complexity. An example of the type of grain growth that occurs in a model like that sketched above is shown in ﬁg. 10.46 (Chen and Wang 1996). One of the outcomes of these calculations is the ability to characterize the kinetics of grain growth. In particular, it is possible to address the question of the mean grain size R as a function of time as well as the distribution of grain sizes. The temporal evolution of the average grain area is shown in ﬁg. 10.47 An outcome of this analysis is that it is found that the mean grain size scales with time with an exponent of 1/2. It should be noted that we have only outlined one of the many different diffuse interface approaches to the problem of grain growth. For the present purposes, our main point has been to call attention to the possibility of a strictly continuum model of grain growth in which the interfaces are endowed with a ﬁnite width and the kinematics of the polycrystal is encoded in a series of continuum ﬁelds. We

10.4 Microstructural Evolution in Polycrystals

577

7.5

7.0

6.5

(

ln A − Ao

) 6.0

5.5

5.0

4.5 6.0

6.5

7.0

7.5

8.0

8.5

9.0

9.5

ln(t)

Fig. 10.47. Temporal evolution of mean grain size in phase ﬁeld model of grain growth (adapted from Chen and Yang (1994)). Plots are of logarithm of average grain area as a function of time, with the two curves corresponding to four (crosses) and thirty-six (circles) different order parameter ﬁelds.

will see later that this class of models (i.e. phase ﬁeld models) has a much wider application than that of its particular incarnation in the context of grain growth. Sharp Interface Models of Grain Growth. An alternative paradigm for considering grain growth is offered by the class of sharp interface models. From a kinematic perspective, the polycrystal may be thought of as a series of lines (in two dimensions) or a series of interfaces (in three dimensions), the positions of which may be parameterized continuously or discretely. This class of models is especially appealing since the full kinematic complexity of the polycrystal has been collapsed onto nothing more than a discrete set of nodal coordinates which identify the interfacial position. The kinetics of the system is built around the idea of considering the various interfaces that make up the polycrystal of interest as being subjected to an array of driving forces of different physical origins. For example, driving forces can be present because of curvature of the boundary plane or because of differences between the stored strain energy in adjacent grains, or because of chemical inhomogeneities, or yet further mechanisms. These ideas may be put on a more formal basis by resorting to the variational arguments set forth in section 2.3.3 in which the power associated with the various driving forces is balanced with the various dissipative mechanisms that are present.

578

10 Microstructure and its Evolution

The application of this theoretical framework to the problem of grain growth is instructive, both as a case study in the use of the variational approach, and for the insights it provides into the grain growth process itself. Recall that the variational formulation is indifferent to the number of different dissipative mechanisms that are incorporated in the analysis. On the other hand, for the purposes of the present discussion we will only consider grain boundary motion induced by curvature without reference to the variety of other possible mechanisms. The driving force for microstructural change is the energy reduction that attends the elimination of grain boundary area and is given by γgb κvn d, (10.91) G˙ = G Bs

with κ the curvature of the boundary at the point of interest, γgb the grain boundary energy and vn the interfacial normal velocity. The overall variational function can be written as Nb Nb Nt 3 vn2 j ds + γb κvn ds + γb vk · sk . (10.92) [vn (s); r (s)] = 2D L L i i i=1 i=1 k=1 j=1 The ﬁrst two terms have already been discussed in several other contexts (see eqns (2.46) and (10.45)) with the new twist that now we have a summation over all of the different interfaces. The third term, on the other hand, is a new feature and reﬂects the extra attention that must be given to triple points within the polycrystalline microstructure when attacked from the sharp interface perspective. In order to turn the variational scheme given above into a calculational scheme, the various interfaces are discretized, thus turning the functional given in eqn (10.48) into a corresponding function which depends only upon the nodal coordinates that deﬁne the boundaries. The variational statement is then invoked in order to determine a set of nodal velocities which are used to update the microstructure. The results of this type of sharp interface treatment of grain growth is shown in ﬁg. 10.48. As noted above, the temporal evolution of the microstructure in this case is the result of a driving force that emerges from the reduction in grain boundary energy by reducing the overall length of such boundaries. Our treatment of grain growth was intentionally diverse, with the aim being to show some of the different paradigms that have been put forth for the consideration of grain growth. In broad terms, the key ideas can be divided between those having to do with computing the driving force on a given interface, and those whose aim it is to attribute a kinetics with these driving forces. The Potts model offered a very simple energetic description of grain boundaries in which the thermodynamic driving force was seen to be associated with the reduction in energy that attends the overall grain boundary area. Phase ﬁeld models

10.4 Microstructural Evolution in Polycrystals

Time = 0.00

Number of cells = 1024

Time = 8.54

Number of cells = 269

Time = 1.95

Number of cells = 707

Time = 30.0

Number of cells = 85

Time = 4.21

Number of cells = 464

Time = 336

Number of cells = 10

579

Fig. 10.48. Series of snapshots from simulation of temporal evolution of two-dimensional polycrystal (courtesy of S. Gill).

could be interpreted as the continuous partners of Potts-type models in that they assign an energy penalty to the presence of interfaces which translates into a driving force for grain boundary migration. Our treatment of the sharp interface

580

10 Microstructure and its Evolution

approach to grain growth illustrated the effects of curvature driven boundary motion.

10.5 Microstructure and Materials The root level argument set forth in this chapter has been that in light of the critical role played by structures at the microstructural scale in determining material properties, a crucial prerequisite to a fuller understanding of materials demands an analysis of the factors governing microstructural evolution. The treatment given in this chapter has in no sense been exhaustive. Our discussion has been heavily biased in favor of metallic materials and has made no reference to the rich microstructures found in polymeric materials, for example. On the other hand, our aim has been to illustrate some of the key methodologies (primarily geometric and energetic) which have been brought to bear on the question of microstructure and its evolution. One of the important unanswered questions at the foundation of the approaches provided here concerns the general principles giving rise to the kinetics of microstructural evolution, and whether or not it is appropriate to express microstructures (as in the martensite case) as energy minimizers. A further query that must be posed is that of how best to synthetically couple approaches to the evolution of microstructures and the effect of these microstructures on properties. Part of the quest of the remaining chapters will be to spell out in several case studies how microstructural features manifest themselves in macroscopic properties.

10.6 Further Reading The Structure of Materials by S. M. Allen and E. L. Thomas, John Wiley and Sons, New York: New York, 1999. This text is part of an excellent MIT series on materials science. This particular volume considers structure in materials from the hierarchical perspective considered here as well. Chap. 6 on microstructure provides a number of interesting discussions and ﬁgures to illuminate the nature of microstructure in wide classes of materials. The Theory of Transformations in Metals and Alloys by J. W. Christian, Pergamon Press, Oxford: England, 1965. This classic text provides a deﬁnitive account of many of the key ideas that attend the study of microstructure. Unfortunately, the book has not been reissued in an updated form, but still makes for excellent reading. Theory of Structural Transformations in Solids by A. G. Khachaturyan, John Wiley & Sons, New York: New York, 1983. I haven’t spent as much time with Khachaturyan’s book as I would have liked, but I can say that it is full of insights into a variety of topics covered in the present chapter.

10.6 Further Reading

581

Microstructure and Properties of Materials edited by J. C. M. Li, World Scientiﬁc, Singapore: Singapore, 1996. This work has a number of interesting articles on the implications of microstructure for material behavior. Stability of Microstructure in Metallic Systems by J. W. Martin, R. D. Doherty and B. Cantor, Cambridge University Press, Cambridge: England, 1997. This book gives a deep coverage to many of the ideas raised in the present chapter. Recrystallization and Related Annealing Phenomena by F. J. Humphreys and H. Hatherly, Pergamon Press, Oxford: England, 1996. A useful discussion of the connection between observed macroscopic changes in microstructure and the underlying defect mechanisms that engender it. Introduction to Engineering Materials: The Bicycle and the Walkman by C. J. McMahon, Jr and C. D. Graham, Jr, published by C. J. McMahon, Jr, 1994 (available from author: http://www.seas.upenn.edu/mse/fac/mcmahon.html). This is one of my favorite books. Despite the claimed low level of the book, the discussion of recovery, recrystallization and grain growth is highly instructive as are many other topics covered by the authors. ‘Modeling of Phase Separation in Alloys with Coherent Elastic Misﬁt’ by P. Fratzl, O. Penrose and J. L. Lebowitz, J. Stat. Phys., 95, 1429 (1999) is one of a series of outstanding papers collected in a volume honoring John Cahn on his 70th birthday. This paper provides an outstanding treatment of many of the ideas that have been put forth from both the sharp and the diffuse interface perspective for thinking about two-phase microstructures. ‘Modeling Microstructure Evolution in Engineering Materials’ by A. C. F. Cocks, S. P. A. Gill and J. Pan, Advances in Applied Mechanics, Vol. 36, edited by E. van der Giessen and T. Y. Wu, Academic Press, San Diego: California, 1999. This article gives a unifying perspective on the role of the variational principle associated with conﬁgurational forces as the basis for numerical investigations of microstructural change. ‘Theory of Martensitic Microstructure and the Shape-Memory Effect’ by Kaushik Bhattacharya, unpublished (1998) (a huge pity!) – available from author: [email protected] Bhattacharya’s article gives a complete and thorough discussion of the many ideas that have been brought to bear on the problem of microstructure in martensites. ‘On the computation of crystalline microstructure’ by Mitchell Luskin, Acta Numerica, pg. 191, Cambridge University Press, Cambridge: England, 1996. Luskin’s article covers many similar issues to those found in the article of

582

10 Microstructure and its Evolution

Bhattacharya and provides an alternative view on some of the issues related to energy minimization. ‘The Analytical Modeling of Normal Grain Growth’ by C. S. Pande and S. P. Marsh, JOM, Sept., 25 (1992). Though brief, this article provides an interesting overview of many of the issues involved in modeling grain growth. ‘Theories of Normal Grain Growth in Pure Single Phase Systems’ by H. V. Atkinson, Acta Metall., 36, 469 (1988). A thorough review that mixes insights on both the experimental situation and the models that have been put forth to confront these experiments. ‘Some Fundamentals of Grain Growth’ by D. Weaire and S. McMurry, in Solid State Physics edited by H. Ehrenreich and F. Spaepen, Vol. 50, Academic Press, San Diego: California, 1997. This article is full of interesting ideas on the geometrical aspects of grain growth and includes a discussion of key theoretical ideas as well.

10.7 Problems

1 Details in the Eshelby Inclusion One of the fundamental solutions from which much is made in the evaluation of microstructure is that of the elastic ﬁelds due to ellipsoidal inclusions. (a) In this part of the problem, revisit the problem of the elastic ﬁelds due to inclusions by deriving the expression given in eqn (10.12). Further, perform the integrations required to determine the displacements, and show that the displacements external to the inclusion are given by a 3 3λ + 2µ (10.93) u r (r ) = 2 3r λ + 2µ while those internal to the inclusion are given by r 3λ + 2µ . (10.94) u r (r ) = 3 λ + 2µ Hint: Recall that (r − r )2 = sgn(r − r ). (b) Imitate our analysis of the ﬁelds due to a spherical inclusion, but now deducing the ﬁelds for a cuboidal inclusion.

10.7 Problems

583

2 Elasticity and Diffusion for a Circular Inclusion In this problem we try to imitate in analytic terms the various arguments that have been set forth coupling mechanics and diffusion in the context of microstructural evolution. Consider a single circular precipitate of initial radius R0 . (a) Solve for the elastic ﬁelds of such a circular inclusion on the assumption that it has the same elastic properties as the matrix, but is characterized by an eigenstrain i∗j = 0 δi j . (b) Using the results of part (a) in conjunction with the expression for the concentration given in eqn (10.52) to obtain the instantaneous concentration at the interface between the particle and the matrix. (c) Use this concentration to solve the diffusion equation for a circular region of outer radius Rout with the far ﬁeld boundary condition, c = C0 . (d) Compute ∇c · n at the interface between the particle and the matrix and update the radius of the particle accordingly. (e) What is the ﬁnal size of the particle? 3 Compatibility at Martensite Interfaces Earlier we introduced the compatibility condition F1 = F2 + a ⊗ n,

(10.95)

and noted that the action of F1 is the same as F2 for points within the invariant plane. Prove this assertion in detail by examining the effect of F1 and F2 on points characterized by the vector r = r# e# + r⊥ n. Show that only if r has a nonzero component perpendicular to the invariant plane will the deformation gradients F1 and F2 have a different action on that vector. 4 Rank-One Connection for Model Deformations Examine the deformation mapping given by x1 = X 1 ± γ X 2 ,

(10.96)

x2 = X 2 ,

(10.97)

x3 = X 3 ,

(10.98)

with the ± sign signifying that we are to take + if the region of interest is above the invariant plane, and − if below. First, sketch the outcome of applying this mapping to points lined up along vertical lines, and then compute the deformation gradients in the two regions. Finally, show that the deformation gradients in question satisfy the rank-one condition, and ﬁnd the vectors a and n.

584

10 Microstructure and its Evolution

5 Different Paradigms for Motion of a Curved Interface Implement the Potts, phase ﬁeld and sharp interface descriptions for the motion of a curved interface. In particular, in ﬁg. 10.42, we showed schematically how these three classes of models are used to describe the evolution of the same microstructure. In this problem, use these three schemes to obtain the ﬂattening of an initially curved interface. Assume an initial parabolic proﬁle and examine the time evolution predicted by these three schemes as the interface becomes ﬂat.

Part four Facing the Multiscale Challenge of Real Material Behavior

ELEVEN

Points, Lines and Walls: Defect Interactions and Material Response

11.1 Defect Interactions and the Complexity of Real Material Behavior In previous chapters, we have begun the attack on the problem of the observed thermomechanical properties of materials from a number of different perspectives. One of our key realizations has been the conspiratorial role of defects in governing the response of materials. Thus far, we have largely concentrated on the structure and energetics of individual defects with less attention given to the implications of these defects for material response. Our efforts have been primarily divided along dimensional lines, with point defects, line defects and interfacial defects each being treated as an end unto itself. The concern of the present chapter is to make evident the claim that such divisions are a theorist’s artiﬁce and that, in general terms, it is the synthetic response of all of these different types of defects in concert that gives rise to the observed complexity of materials. We begin our discussion with the consideration of diffusion. In earlier chapters, we noted that diffusion is mediated by the presence of point defects. However, until now, we have not given any quantitative analysis of the lubricating effect of other defects in the context of diffusion. We have already seen in ﬁg. 9.1 that bulk diffusion can be negligible in comparison with the diffusion that takes place along surfaces, grain boundaries and dislocations. As a particular realization of this class of problem, we consider the case of surface diffusion with special reference to some of the counterintuitive diffusion mechanisms that take place at surfaces. A second fundamental theme that will be taken up in this chapter in which there is an interplay between the various types of defects introduced earlier is that of mass transport assisted deformation. Our discussion will build on the analysis of diffusion at extended defects. We will begin with an examination of the phenomenology of creep. A third example in which there is a mutual interplay between the different types of defects that we have discussed in previous chapters is that provided by the 587

588

11 Points, Lines and Walls: Defect Interactions and Material Response

dislocation–grain boundary interaction. In the context of polycrystal plasticity, it is clearly of interest to determine the conditions under which plasticity in one grain can be communicated to adjacent grains. Experiments indicate that under certain conditions, dislocations may pass from one grain into neighboring grains. Clearly, the presence of grain boundaries can have the effect of impeding dislocation motion, and we will take up this topic in section 11.4. The next example that will be set forth as an example of a problem in which multiple defect types can be present simultaneously is that of fracture. Our discussion will begin with an examination of the way in which cracks can be built up as superpositions of dislocations. This leads naturally to questions of the interaction of dislocations and cracks and culminates in the analysis of the intriguing problem of crack tip nucleation of dislocations. An age old observation around which entire revolutions took place is that if a pure metal is mixed with small amounts of some other metal, the resulting strength of the material will be altered. Witness the Bronze Age. These observations will be codiﬁed in quantitative terms in section 11.6 where we show how the yield stress varies as a result of obstacles to dislocation motion. These observations, once again, drive home the potency of the synthetic effect of different types of defects in tandem. We will sketch some of the key qualitative ideas that have been elucidated with respect to both solution and precipitate hardening which are the technical names for the area of study that has arisen in response to the simple observations that made the Bronze Age possible. The development in this part of the chapter will culminate in certain scaling arguments which reveal how the yield stress scales with various microstructural parameters. In keeping with the theme of the present chapter, our basic argument will be that although dislocations are the key players in plastic deformation, it is their interactions with each other and other obstacles that gives rise to much of the observed richness of plastic deformation. The basic aim of this chapter is to illustrate the way in which the various defects we have introduced in previous chapters can form partnerships that enrich the properties of materials and the processes that transpire within them. The logic of the chapter is to provide evidence for this viewpoint through the medium of case studies. As usual, we have not been exhaustive. 11.2 Diffusion at Extended Defects 11.2.1 Background on Short-Circuit Diffusion In chap. 7, we discussed the fundamental role of point defects in diffusion. We also hinted at the serious amendment to diffusion rates that is mediated by the presence of extended defects such as dislocations and grain boundaries (see ﬁg. 9.1). As was noted above, diffusion rates along defects can often be so much larger than those in

11.2 Diffusion at Extended Defects

589

the bulk that the bulk mechanisms can be rendered almost irrelevant. As a result of this insight, it is evident that we must reconsider diffusion more carefully in light of the presence of line and interfacial defects. Our present task is to build on the foundations laid in chap. 7, but now with special reference to the diffusive processes that take place at extended defects. The basic argument will be that by virtue of the more open atomic-level environments near extended defects, the activation energy both for point defect formation and migration will often be reduced relative to bulk values. We will build our case around a fundamental case study through the consideration of diffusion at surfaces. The surface diffusion example will illustrate not only how diffusive processes are amended at extended defects, but will also illustrate the shortcomings of the transition state formalism when the detailed atomic-level mechanisms are not known a priori.

11.2.2 Diffusion at Surfaces Because of the widespread interest in growth of material systems by deposition, the subject of surface diffusion is one of enormous current interest. The example of surface diffusion being taken up here is of interest to our overall mission for several different reasons. First, as noted above, surfaces are one of the most important sites of communication between a given material and the rest of the world. Whether we interest ourselves in oxidation and corrosion, catalysis, the crystal surface is the seat of tremendous activity, most of which is mediated by diffusion. A second reason that we have deemed it important to consider the role of surface diffusion is that our analysis will reveal the dangers that attend the use of transition state theory. In particular, we will appeal to the existence of ‘exchange mechanisms’ for diffusion that reveal that the diffusion pathways adopted on some crystal surfaces are quite different than those that might be suggested by intuition. Exchange Mechanisms for Surface Diffusion. Our discussion of transition state theory in chap. 7 showed that in those cases when we are lucky enough to know the details of the transition pathway associated with a given diffusion mechanism, atomic-level analysis can shed important light on the process of diffusion. On the other hand, as we have already emphasized, the successful application of the ideas of transition state theory ultimately requires a knowledge of the transition pathway. Field-ion microscopy in conjunction with ﬁrst-principles analysis of the energetics of metal surfaces has led to a convincing picture of surface diffusion in some instances that is entirely contrary to the ideas built around intuition. The simplest picture of diffusion on the (001) surface of an fcc metal such as Al or Pt would hold that atomic jumps take place from one binding site to the next via

590

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.1. Competing surface diffusion mechanisms on an fcc (001) surface (adapted from Feibelman (1990)): (a) intuitive mechanism in which adatom moves from one fourfold site to another by passing across bridge site, and (b) exchange mechanism in which diffusion occurs by concerted motion both of adatom and its subsurface partner.

the pathway illustrated in ﬁg. 11.1(a). The contention in this case would be that diffusion takes place by the simple motion of the atom from one fourfold binding site to the next through the intermediate twofold bridge site. On the other hand, observations on Pt and Ir (001) determined that diffusion takes place by hopping exclusively along 100 and 010 directions as opposed to the 110 direction that would correspond to crossing the bridge site. Reconciliation of the simplest intuitive notions concerning diffusion with these observations would require that the adatom pass through an intermediate state in which it is onefold coordinated and sits directly above one of the surface atoms. This mechanism is associated with an unphysically high activation energy. Because of the failure of the mechanism suggested above to account for observed diffusion, alternative mechanisms must be sought. To quote Feibelman (1990), ‘The key to developing a correct model of surface diffusion is to think of it as a chemical phenomenon rather than in terms of a hard sphere moving on a bumpy plane.’ In terms of what we have learned about the energetics of atomic-level bonding in previous chapters, Feibelman’s exhortation is a reminder that there may be alternative mechanisms in which the adatom does not suffer the signiﬁcant loss of coordination implied by the intuitive diffusion mechanism involving bridge sites suggested above. In particular, an alternative ‘exchange mechanism’ in which the adatom burrows into the surface at the same time that the atom previously at one of the surface sites vacates its position has led to a plausible explanation for all of the observations. This mechanism is illustrated in ﬁg. 11.1(b). In the case of Al, Feibelman (1990) found that this mechanism was associated with an activation energy of only 0.20 eV, in contrast with the 0.65 eV associated with the naive but intuitive mechanism discussed earlier. As a result, the exchange mechanism explains both the orientational preferences observed in ﬁeld-ion microscopy experiments as well as the corresponding activation energies. One of the key reasons we have considered the exchange mechanism for surface diffusion is as a reminder of the inherent difﬁculties in using transition state theory.

11.2 Diffusion at Extended Defects

591

While it is true that once there is conﬁdence that the correct mechanism has been identiﬁed that transition state theory will usually yield a reasonable description of the energetics, it is also true that ignorance of the correct pathway can lead to results that are completely misleading. As a result, work has concentrated on important new developments in the area of determining the relevant reaction pathways in complex systems. In particular, sophisticated techniques have been set forth that are aimed at uncovering the optimal reaction pathway in cases where intuition does not sufﬁce as a guide. Surface Steps and Diffusion. Recall from our discussion of surfaces in chap. 9, there are a series of structures at increasing levels of complexity that may be found on crystal surfaces. Beyond the reconstructions that attend ﬂat surfaces, we also noted the important role of surface steps as key structural components of generic surfaces. These steps are interesting not only from the perspective of their geometry, but also from the point of view of their role in altering the nature of the diffusive processes that take place on surfaces. In this section, our intention is to examine a particular feature of such diffusion, namely, the existence of a barrier resulting from surface steps. The evidence for reﬂecting barriers at the edge of surface terraces derives from a number of different sources, one important example of which is ﬁeld-ion microscopy. For example, it has been found that there is an enhancement in the likelihood of ﬁnding an adatom just adjacent to the top edge of a surface step. From the standpoint of the simple random walk analysis put forth earlier, one way to interpret the results of the types of experiments sketched above is via the random walker with reﬂecting walls. The basic idea in this case is the presumption that the random walker can exercise excursions within the conﬁnes of some ﬁnite region, but whenever the walker reaches the boundary of the region it is reﬂected from the walls. These phenomenological ideas have been lent quantum mechanical credibility through consideration of the energetics of adatoms near steps. In particular, examination of the energetics of adatoms near a surface step has led to the elucidation of the concept of the Schwoebel barrier. The total energies of adatoms in the vicinity of a surface step have been computed using both empirical and ﬁrst-principles techniques though for the present purposes we will consider but one example of a calculation of this barrier from the empirical perspective. The rough physical expectation is that as an adatom approaches a surface step from above, in the immediate vicinity of that step it will suffer an even greater loss of coordination than that it already experiences on a free surface, with a concomitant energy penalty. A series of energetic snapshots for the (111) surface of Pt are shown in ﬁg. 11.2 and reveal the energetics of different conﬁgurations of the adatom near

592

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.2. Illustration of energetics of an adatom near a surface step on the (111) surface of Pt (adapted from Jacobsen et al. (1995)).

a step. As claimed above, the key remarkable qualitative feature of the near-step energetics is the existence of both a barrier to adatom motion across the step from above, and an enhanced bonding for those adatoms arriving at the step edge from below. From the overall perspective of the present chapter, our ambition in brieﬂy describing the energetics of surface diffusion has been to illustrate the additional complexity that is ushered in as a result of the simultaneous action of more than one type of defect. In particular, we have shown that via a counterintuitive exchange mechanism, the activation energy for surface diffusion can be lowered by 0.4 eV relative to the intuitive motion associated with an imagined random walker on a surface. In addition, we have also shown that the presence of surface steps can have signiﬁcant implications for the nature of diffusion on surfaces.

11.3 Mass Transport Assisted Deformation In chap. 7 we laid the foundations for the analysis of mass transport in solids. In the current section, our aim is to examine the ways in which mass transport can assist the deformation that occurs in a given material. As a preliminary, we remind the reader of one of the key features of the deformation mechanism map introduced in ﬁg. 7.7. We refer to the fact that in many instances for stresses well below the putative yield stress, permanent deformation is still observed. Such deformation usually occurs at temperatures which are larger than, say, 0.3TM ,

11.3 Mass Transport Assisted Deformation

593

Fig. 11.3. Schematic of strain as a function of time in a constant-stress creep test (adapted from Courtney (1990)).

where TM is the melting temperature. These high-temperature mechanisms are referred to generically as creep and will be our present concern.

11.3.1 Phenomenology of Creep The phenomenology of creep is best illustrated through the vehicle of the so-called creep test in which a specimen is subject to either a constant load or a constant stress, and the deformation is monitored as a function of time. The generic outcome of such a test is illustrated in ﬁg. 11.3 and suggests that the creep behavior may be divided into three distinct regimes, denoted primary, secondary and tertiary creep. The primary regime is characterized by an initially high strain rate which decreases with increasing time until a so-called ‘steady-state’ regime is entered in which the strain rate is roughly constant. The tertiary regime is characterized by an increase in the strain rate and terminates with the failure of the material. In considering creep, there are several different control parameters that are known to inﬂuence the resulting deformation. Clearly, with increasing stress, the strain rate ˙ will be increased. Similarly, an increase in temperature also serves to increase ˙ . We continue our discussion by examining these two different parameters in turn. Before embarking upon that discussion, we note that our analysis will highlight the signiﬁcant empirical insights that have been gained into the creep process, with less emphasis on the models that have been advanced to rationalize these empirical gains.

594

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.4. Schematic of strain rate ˙s as a function of normalized stress (adapted from Nabarro and de Villiers (1995)). D refers to the bulk diffusion constant and b is a measure of the lattice parameter.

One of the elemental empirical insights into the creep process concerns the stress dependence of the creep rate. A broad range of experimental data can be captured on the assumption of a power law relation between the strain rate ˙ and the stress σ . In particular, the strain rate can be written in the form n σ , (11.1) ˙ ∝ µ where the exponent n varies depending upon the situation. This behavior is illustrated qualitatively in ﬁg. 11.4. Another critical question is how the creep rate depends upon temperature. As hinted at in the title of this section, creep is in many instances mediated by the presence of mass transport. Part of the basis of this insight is the observed temperature dependence of the creep rate. In particular, it has been found that creep is thermally activated. Indeed, one can go further than this by noting the relation between the activation energy for diffusion and that of the creep process itself. A plot of this relation is shown in ﬁg. 11.5. As a result, we see that the temperature dependence of the creep rate may be written in the form ˙ = const.e−E/kT .

(11.2)

Our insights on both the stress and temperature dependence of the strain rate may thus be uniﬁed in a single phenomenological equation of the form n σ ˙ = A e−E/kT . (11.3) µ

11.3 Mass Transport Assisted Deformation

595

Fig. 11.5. Plot of activation energies for creep and bulk diffusion (adapted from Courtney (1990)).

From a theoretical perspective, what we are left with is the ambition of explaining the stress and temperature dependence of the strain rate evoked in eqn (11.3) from a mechanistic perspective. As we will see, the problem is not so much a shortage of ideas in this regard, but rather an embarrassment of choices, without any clear scheme which will permit the falsiﬁcation of these models. In the remainder of our discussion on mass transport assisted deformation, the plan is to sketch the ideas associated with Nabarro–Herring and Coble creep. I should note that this discussion is little more than a report on the party line as regards the modeling of creep phenomena and further that we have not done justice to both what is known and what remains unknown in this important ﬁeld. In particular, we omit all reference to an important alternative mechanism related to the mass transport assisted climb of dislocations, thus allowing them to breach obstacles to their further glide.

11.3.2 Nabarro–Herring and Coble Creep The class of creep mechanisms of interest here are those that are mediated by stress-biased diffusion. If we are to consider the vacancy ﬂux in a given grain within a material that is subjected to an applied stress, it is argued that the vacancy formation energy differs in different parts of the grain, and hence that there should be a gradient in the vacancy concentration leading to an associated ﬂux. This

596

11 Points, Lines and Walls: Defect Interactions and Material Response

ﬂux of vacancies (or atoms) can, with the accumulated weight of time, lead to a macroscopic change in the shape of the material. This mechanism results in a strain rate that is linear in the applied stress and with an activation energy that is identical to that for self-diffusion. The distinction between the Nabarro–Herring and Coble mechanisms is one of variety rather than form. In particular, the Nabarro–Herring mechanism is associated with lattice diffusion within the grains, while the Coble mechanism is built around diffusion along the grain boundaries. In both cases, however, the key point is the presence of a gradient in the vacancy concentration induced by the applied stress. Our ambition in the paragraphs to follow is to illustrate an approximate heuristic model which shows how the presence of an applied shear stress can result in mass transport mediated deformation. We begin with the notion that the crystal of interest is subjected to a shear stress. From a two-dimensional perspective, for example, we then make use of the fact that the shear stress 0 σ σ = , (11.4) σ 0 may be rewritten in principal coordinates as σ 0 . σ = 0 −σ

(11.5)

In principle, we are thus faced with solving a boundary value problem for a region like that shown in ﬁg. 11.6 with the aim being to evaluate the mass transport that arises by virtue of the spatially varying chemical potential, and hence, mass currents, that arise in response to the nonuniform stress. In practice, since we are only interested in an estimate of the effect, we resort to an approximate analysis in which the relevant chemical potentials and mass ﬂux, and attendant strain rate are all evaluated heuristically. The argument begins with reference to ﬁg. 11.6 with the claim that the vacancy formation energy for the faces subjected to tensile stresses differs from that on the faces subjected to compressive stresses. Again, a rigorous analysis of this effect would require a detailed calculation either of the elastic state of the crystal or an appeal to atomistic considerations. We circumvent such an analysis by asserting that the vacancy concentrations are given by f

c(T ) = e−(vac −σ )/kT ,

(11.6)

and f

c(C) = e−(vac +σ )/kT ,

(11.7)

where the superscripts T and C refer to tensile and compressive, respectively. To

11.3 Mass Transport Assisted Deformation

597

MACROSCOPIC STRESS

Fig. 11.6. Schematic of how stress assisted mass transport results in a net strain rate (adapted from Herring (1950)).

really understand this result, we need to reﬂect further on the deﬁnition of the vacancy formation energy given in section 7.3.3. In particular, we need to see how those arguments should be amended to account for the presence of a stress. A simple plausibility argument can be constructed as follows. From an atomistic perspective, the vacancy formation energy associated with plucking a near-surface f atom out and placing it on the surface can be represented approximately as vac ≈ f¯b, where f¯ is the mean force exerted by neighboring atoms as the atom is plucked to the surface. In the presence of the tractions imagined above, there is either a suppression (tensile case) or enhancement (compressive case) in this energy cost, which can now be written as f f vac (stress) = vac ± σ Aatom b,

(11.8)

f f vac (stress) = vac ± σ ,

(11.9)

or

where we have deﬁned Aatom as the area over which the traction is working during the plucking process. The next step in the argument is to estimate the amount of mass transported from one face to the other by virtue of the concentration gradient embodied in eqns (11.6) and (11.7). In particular, the ﬂux is given by j = −D(∂c/∂ x), where the gradient term is estimated as ∂c c(T ) − c(C) ≈ , ∂x l

(11.10)

598

11 Points, Lines and Walls: Defect Interactions and Material Response

where the parameter l is a measure of the size of the region in question. We note that our objective is to compute the strain rate which is deﬁned as ˙ =

1 dl , l dt

(11.11)

and may be written in terms of the amount of volume arriving on the face of interest per unit time as a result of the relation 1 dV dl = 2 . dt l dt

(11.12)

The rate d V /dt can be evaluated by recourse to the relation dV = l 2 j, dt

(11.13)

with the result that when all the pieces of our analysis are assembled, we have ˙ =

f 2D0 σ −(vac m )/kT +vac . e 2 l kT

(11.14)

At this point, several comments are in order. First, we note that we have recovered an expression for the strain rate which jibes with the empirical result presented in eqn (11.3). In this case, the stress exponent is unity. Our discussion of creep given above implicitly assumed that the mass transport resulting in an overall shape change took place through the crystalline region itself. An alternative diffusion mechanism, founded upon the same principles as the discussion of Nabarro–Herring creep given above is based on reconsidering those arguments when the mass transport is mediated by grain boundary diffusion rather than bulk diffusion. The result of this analysis is a change in the way that eqn (11.14) scales with grain size. In particular, in the context of the Coble mechanism, the strain rate is written ˙ =

2Dgb σ δ . l 3 kT

(11.15)

The new features of this result in comparison with that of eqn (11.14) are the presence of the grain boundary diffusion constant, Dgb , and the introduction of a parameter δ which is a measure of the thickness of the region over which diffusion is enhanced in the vicinity of the grain boundary. Note that in the context of both the Nabarro–Herring analysis and that of Coble, the strain rate is found to vary linearly with the applied stress. In particular, this result is consistent with dubbing this process ‘diffusional viscosity’ as did Herring (1950) in his original work. Indeed, the identiﬁcation of a material parameter such as the ‘viscosity’ and its associated scaling properties with grain size and temperature represents another example of the type of micro–macro connection

11.4 Dislocations and Interfaces

599

Fig. 11.7. Examination of the success of the hypothesis of linear stress dependence of the creep strain rate in the high-temperature regime (adapted from Nabarro and de Villiers (1995)).

which is at the heart of the viewpoint taken in the present work. The question of how such models jibe with experience is partially addressed in ﬁg. 11.7 which reveals that the linear stress dependence is well obeyed for a range of materials. It bears repeating that our discussion has been little more than a caricature of this important ﬁeld.

11.4 Dislocations and Interfaces In the previous chapter we took preliminary steps to examine grain boundary motion. However, in the absence of considerations of dislocations in the vicinity of such grain boundaries, this description is incomplete. In the present section, we begin by examining the way in which dislocations and grain boundaries merge. In particular, for the special geometric case of low-angle grain boundaries, the boundary may be thought of as nothing more than a superposition of dislocations, with tilt boundaries being built up of edge dislocations and pure twist boundaries being built up by screw dislocations. However, our analysis can go further than this. In addition, we pose the question of how dislocations that impinge on a grain

600

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.8. Representation of grain boundary as an array of dislocations (adapted from Amelinckx (1979)).

boundary are greeted by the boundary which serves as an obstacle. Such processes can lead to both dislocation pile-ups and slip transmission in which crystal slip in one grain passes to adjacent grains.

11.4.1 Dislocation Models of Grain Boundaries We begin our geometric discussion with the case of pure tilt boundaries on the grounds that the connection between dislocations and the boundary is most evident visually in this case. As was discussed in some detail in chap. 9, a tilt grain boundary is characterized by a simple misorientation between the two grains as was discussed in chap. 9. The intent of this section is to illustrate that a simple superposition of the elastic displacements implied by the Volterra solution for straight dislocations discussed in chap. 8 can lead to exactly the same type of misorientation. First, we consider the most elementary geometrical arguments that can be set forth in this regard. The question we pose at this moment is what is the relation between the dislocation spacing and the misorientation. For concreteness, consider a series of uniformly spaced edge dislocations with Burgers vector of length b such as is shown in ﬁg. 11.8. What we note immediately is that this geometry may be thought of as the introduction of an extra half-plane each time we traverse the distance D along the boundary plane. As a result, the dislocation spacing and the

11.4 Dislocations and Interfaces

601

misorientation angle are related by D=

b . 2 sin(θ/2)

(11.16)

Although a length scale tied to the underlying discrete lattice is present in this equation, there is no clear selection mechanism that distinguishes between those geometries that have a special relation to the underlying crystalline lattice and those that do not. What we are noting is that not all dislocation spacings are equal and that for certain special choices of this spacing the lattice and the dislocations are locked into a commensurate relationship. One of the immediate questions that arises in the context of such a model of grain boundaries is what it might have to say about the stress ﬁelds and energies of that boundary. An immediate reaction to the claim that grain boundaries may be thought of as arrays of dislocations is that this must mean that boundaries have long-range stress ﬁelds. However, as will be shown in short order, the long-range dislocation stress ﬁelds when superposed in the special way demanded by a grain boundary lead to cancellations that leave exponentially decaying ﬁelds. For simplicity, consider the isotropic linear elastic description of the problem. The total stress is obtained by summing up the contributions of the constituent dislocations. If we consider the shear stress components for concreteness, then the total stress for the boundary with dislocation spacing D is ∞ µb 1 x3 σx y (x, y) = 2 2 2 2π(1 − ν) n=−∞ [x + (y − n D) ] ∞ (y − n D)2 . −x 2 2 2 n=−∞ [x + (y − n D) ]

(11.17)

All this formula instructs us to do is to take the contribution to the total stress of each dislocation using the results of eqn (8.38) and to add them up, dislocation by dislocation. We follow Landau and Lifshitz (1959) in exploiting the Poisson summation formula to evaluate the sums. Note that while it would be simple enough to merely quote the result, it is fun to see how such sums work out explicitly. If we use dimensionless variables α = x/D and β = y/D, then the sum may be rewritten as σx y (x, y) =

∞ µbx α 2 − (β − n)2 . 2π D 2 (1 − ν) n=−∞ [α 2 + (β − n)2 ]2

(11.18)

The next step in the thrust to beat the sum into submission is to recognize that if

602

11 Points, Lines and Walls: Defect Interactions and Material Response

one deﬁnes J (α, β) =

∞ n=−∞

α2

1 , + (β − n)2

then the expression for the stresses is given in turn as

∂ J (α, β) µbx J (α, β) + α . σx y = − 2π D 2 (1 − ν) ∂α

(11.19)

(11.20)

With these clever algebraic machinations behind us, the original problem has been reduced to that of evaluating the sum J (α, β). Recall that the Poisson summation formula tells us ∞ ∞ ∞ f (n) = f (x)e2πikx d x. (11.21) n=−∞

k=−∞

−∞

For the problem at hand, the Poisson summation formula allows us to rewrite our sum as ∞ −2πiku ∞ e 2πikβ e du. (11.22) J (α, β) = 2 2 −∞ α + u k=−∞ Evaluation of the relevant integrals is immediate and results in J (α, β) =

∞ π 2π + e−2πkα cos 2πkβ. α α k=1

(11.23)

Consultation of Gradshteyn and Ryzhik (1980) or some other reference permits −kt cos kx = sinh t/(cosh t − cos x), the exact evaluation of the sum 1 + 2 ∞ k=1 e which for our case leads to the stress 2π x 2π y cosh −1 cos µbπ x D D σx y (x, y) = 2 (11.24) . D (1 − ν) 2π x 2 2π y − cosh cos D D However, we could have made more immediate progress with eqn (11.23) by recalling the signiﬁcance of the parameter α. In dimensionless terms this parameter is a measure of the distance from the boundary and for large distances we could safely keep only the term associated with k = 1. In this case, we ﬁnd σx y (x, y) =

2π µbx − 2π x 2π y e D cos . D 2 (1 − ν) D

(11.25)

Having attained our end, namely, the determination of the grain boundary stresses (note that the computation of σx x and σ yy proceeds similarly), what may be learned about boundaries themselves? We begin with a simple, but profound

11.4 Dislocations and Interfaces

603

observation concerning the solution. Because of the exponential dependence of the stresses on the distance from the boundary, we see that the elastic perturbation due to a boundary is short-ranged. Though dislocations have their characteristic long-range elastic signature, grain boundaries lead only to a localized inﬂuence. As we have already remarked in earlier discussions on interfaces in materials, there is a hierarchy of energies associated with such interfaces commencing with surfaces, which have the highest energies, passing through grain boundaries, which are intermediate in energy, and ﬁnishing with stacking faults, which are usually at the bottom of the energy scale. One issue of interest that our dislocation model of grain boundary permits us to revisit is that of the energies of grain boundaries. The simple argument that is made in exploiting the dislocation model for an estimate of the grain boundary energy is that the boundary may be thought of energetically as the sum of the energies of the isolated dislocations, where the long-range cutoff is taken to be determined by the dislocation spacing itself. To make this argument more plausible, consider the stress at the boundary in the immediate vicinity of a particular dislocation. Note that the total stress is given by eqn (11.24), and we are interested in a point (x, y) in the immediate vicinity of a particular dislocation. Expansion of the relevant cos and cosh factors to quadratic order in their arguments results in σx y (x, y) =

x 2 − y2 µbx , 2π(1 − ν) (x 2 + y 2 )2

(11.26)

which is seen to be exactly the shear stress component for a single dislocation at the origin. This result suggests the plausibility of treating the boundary as a series of single dislocations, each with an energy E disl =

D µb2 ln . 4π(1 − ν) 2r0

(11.27)

To obtain this result, all we have done is to use the results from chap. 8 for the energy of a single dislocation within isotropic linear elasticity. We may make an approximate evaluation of the grain boundary energy on the grounds that each dislocation speciﬁes the energy of its local neighborhood on the boundary. Hence, the energy per unit depth of boundary is given by E gb =

D µb2 ln , 4π D(1 − ν) 2r0

(11.28)

which if we recall that θ = b/D may be rewritten as E gb = θ(A − B ln θ),

(11.29)

with A = [µb/4π(1 − ν)] ln(b/2r0 ) and B = [µb/4π(1 − ν)]. This is the

604

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.9. Energy of tilt grain boundary as a function of misorientation angle (adapted from Sutton and Ballufﬁ (1995)).

noted result of Read and Shockley for the energy of a grain boundary, and is plotted in comparison with experimental values in ﬁg. 11.9. As was remarked earlier, one of the serious shortcomings of the present model, and a fact which is revealed in considering the experimental numbers, is that there is no provision for the possible commensurability of the lattice parameter and the dislocation spacing D. In particular, for certain choices of the misorientation angle, very special geometries arise as was noted in our earlier discussion on coincidence site lattices. By way of contrast, the dislocation model holds that the parameter D may be varied continuously without prejudice.

11.4.2 Dislocation Pile-Ups and Slip Transmission Dislocations and grain boundaries form partnerships other than the one described above. Another intriguing mechanism involving dislocations and grain boundaries arises when dislocations, during the process of their gliding motions, impinge on a grain boundary in their pathway which serves as an obstacle. Our thinking in the current section will be founded upon two alternative approaches to the question of dislocation pile-ups. We will begin with a discrete analysis of such problems. However, it will be seen to be mathematically more convenient to assume that the set of dislocations piled up against a boundary are continuously distributed, unleashing the powerful machinery of integral equations to make analytic headway. We begin with a consideration of the relevant phenomenology. Fig. 11.10 shows a number of different possible outcomes of the interaction between an array of

11.4 Dislocations and Interfaces

605

Fig. 11.10. Schematic of interactions between dislocations and grain boundaries (courtesy of Ian Robertson).

piled-up dislocations and a grain boundary. Several of the mechanisms feature the development of plastic deformation (i.e. dislocation motion) in the adjacent grain. On the other hand, the pile up of dislocations against a boundary can result in processes within the grain boundary plane itself. As shown in the ﬁgure, two possible outcomes are the development of dislocation motion within the grain boundary plane or wholesale fracture along the grain boundary. The advent of transmission electron microscopy opened the doors to the direct observation of processes such as the pile-up of dislocations at a grain boundary and the subsequent commencement of dislocation motion in adjacent grains. The process of slip transmission described above may be seen from the perspective

606

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.11. Slip transmission process (taken from Lee et al. (1990)).

of transmission electron microscopy in ﬁg. 11.11. What we note in inspecting this ﬁgure is that the geometric positions of the dislocations adopt a pleasing disposition which suggests a regular mathematical relation governing the spacings of the piled up dislocations. Two central questions that arise in the context of this geometry are: (i) what governs the distribution of pile-up dislocations, and (ii) what are the implications of such a pile-up, especially in terms of the stresses it produces in adjacent grains? Our fundamental assertion concerning the geometry of pile-ups is that they reﬂect the equilibrium spacing of the various dislocations which are participants in such a pile-up. From a discrete viewpoint, what one imagines is an equilibrium between whatever applied stress is present and the mutual interactions of the dislocations. In simple terms, using the geometry depicted schematically in ﬁg. 11.12, we argue that each dislocation satisﬁes an equilibrium equation of the form 1 = 0. (11.30) τapp (x) + A x − xi i= j j

11.4 Dislocations and Interfaces

607

Fig. 11.12. Schematic representation of pile-up geometry (adapted from Smith (1979)).

This equation considers the equilibrium of the j th dislocation. In particular, it is nothing more than a dislocation-by-dislocation statement of Newton’s ﬁrst law of = 0, which says that the total force on the j th dislocation motion, namely, F(tot) j is zero. The factor A is determined by the elastic moduli and differs depending upon whether we are considering dislocations of edge (A = µb/2π(1 − ν)), screw(A = µb/2π ) or mixed character. The problem of determining the equilibrium distribution of the dislocations in the pile-up has thus been reduced to one of solving nonlinear equations, with the number of such equations corresponding to the number of free dislocations in the pile-up. For further details see problem 3 at the end of the chapter. A more elegant (and mathematically tractable) description of the problem of dislocation pile-ups is to exploit the representation of a group of dislocations as a continuous distribution. This type of thinking, which we have already seen in the context of the Peierls–Nabarro model (see section 8.6.2), will see action in our consideration of cracks as well. The critical idea is that the discrete set of dislocations is replaced by a dislocation density ρb (x) such that dn(x) = ρb (x)d x.

(11.31)

What this equation tells us is the number of dislocations between x and x + d x. The key constraint on the function ρb (x) is that it be properly normalized so that xmax n tot = ρb (x)d x, (11.32) xmin

where n tot is the number of dislocations in the pile up. Once we have taken this step, the equilibrium condition for the dislocations is represented by an integral equation ∞ ρb (x )d x µb + τext (x) = 0. (11.33) P 2π −∞ x − x This equation should be seen as the continuous analog of eqn (11.30). It expresses the equilibrium of the inﬁnitesimal dislocation at position x with the applied stress, τext (x) and the remaining inﬁnitesimal dislocations in the distribution ρb (x ). The P refers to the principal value integral and eliminates the self-interaction of the dislocation at x with itself.

608

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.13. Representation of dislocation pile-up as a continuous distribution of dislocations.

As a concrete example of such a problem, we follow Lardner (1974) in considering n screw dislocations, each with Burgers vector of magnitude b in the region x > 0, driven to the left by a constant shear stress −τ and bounded by a barrier at x = 0 (in mentioning the barrier, we have a grain boundary in mind, for example). Furthermore, if we assume that the pile-up has a width a, then the solution to this problem which we quote without derivation (for details see Lardner (1974)) is 2τ a − x . (11.34) ρb (x) = µb x To determine the width a, recall eqn (11.32) which in this instance yields a πτa n= , (11.35) ρb (x)d x = µb 0 with the implication that a = µnb/π τ . The dislocation density associated with this proﬁle is shown in ﬁg. 11.13, and demonstrates the same qualitative features as noted in the observed pile-ups. The next question we pose is how such a dislocation distribution affects the stress state in its neighborhood. The pertinence of this question to broader issues in the mechanics of materials is that a quantitative understanding of dislocation pile-ups has been invoked to explain the dependence of the yield stress on the grain size as canonized in the Hall–Petch relation and depicted in ﬁg. 8.2. One hypothesis put forth with the aim of explaining the Hall–Petch behavior is that the presence of such pile-ups reduces the stress needed to inspire slip in adjacent grains. As we will show below, the grain size enters as the characteristic dimension by which the pileup size is measured, and larger pile-ups lead to larger stresses in adjacent grains and thus smaller stresses are needed to induce slip within them. The geometry we have

11.5 Cracks and Dislocations

609

Fig. 11.14. Schematic of the pile-up of dislocations at a grain boundary. Enhancement in the stress ﬁeld in an adjacent grain as a result of the presence of the pile-up is also indicated schematically.

in mind is depicted in ﬁg. 11.14 In attempting to explain the Hall–Petch behavior, the argument has been advanced that once slip has commenced in the grain that is favorably oriented for slip, dislocations will pile-up against the boundary that is the terminus of the slip plane. The presence of this pile-up has the effect of increasing the stress in the adjacent grain which is itself less favorably oriented for slip. The pile-up is thought to catalyze slip in the adjacent grain by virtue of the increased stress there. The total stress ahead of the pile-up is given by µb a ρb (x )d x . (11.36) τ (x) = −τ + 2π 0 x − x This equation reﬂects the addition of the externally applied shear stress, −τ , as well as the contribution of the pile-up itself as embodied in the integral. Substitution of the dislocation density determined above yields x −a τ (x) = −τ . (11.37) x What this result demonstrates is the presence of an enhanced stress in front of the pile up (x < 0). We forego a discussion of the implications of such stress enhancements for dislocation nucleation until section 11.5.3.

11.5 Cracks and Dislocations In chap. 2, we noted that linear elastic fracture mechanics offers powerful insights into the continuum description of fracture processes. On the other hand, we also noted that the occurrence of fracture ultimately depends upon mechanisms that take place in the vicinity of the crack tip, some of which depend upon atomic-level

610

11 Points, Lines and Walls: Defect Interactions and Material Response

details. It is the aim of the present section to recount some of the issues that arise in trying to bring atomic-level insights to bear on the problem of fracture especially in the context of crack tip dislocation nucleation. Our reason for including this discussion in the present chapter is the fact that our understanding of cracks and the fracture process can be signiﬁcantly extended once we adopt a broader view in which cracks and dislocations are considered simultaneously. In coming sections we undertake a discussion of the conspiracy that arises once dislocations and cracks are taken into consideration jointly. In particular, the goal is to examine two key issues related to dislocation–crack interactions. First, we wish to consider the notion of crack tip shielding in which, by virtue of the presence of a dislocation in the neighborhood of a crack tip, the crack tip ﬁelds are amended locally. In particular, we will interest ourselves in the renormalization of the crack tip stress intensity factor by virtue of the presence of dislocations. Once we have built up the tools for handling dislocations and cracks simultaneously, we aim to consider the competition between cleavage and nucleation of dislocations at a crack tip. Our fundamental argument will be that the elastic energy release rate can be balanced either against the creation of new free surface or in the installation of crystalline slip in the form of dislocations.

11.5.1 Variation on a Theme of Irwin In chap. 2 the central role of cracks in fracture mechanics was discussed. One of the universal features of such cracks from the standpoint of the theory of linear √ elasticity is the characteristic 1/ r signature of their stress ﬁelds. In the present section we wish to revisit these ﬁelds with an eye to examining how such ﬁelds may be deduced using arguments from dislocation theory. The approach adopted here will be to use the same superpositions of dislocations already discussed in the context of dislocation pile-ups. The fundamental argument is that by using the dislocation ﬁeld of a single dislocation as a fundamental solution (i.e. a Green function), the ﬁelds due to cracks may be constructed by superposition. Cracks as a Superposition of Dislocations. A scheme that will suit our aim of building a synthetic description of cracks and any allied dislocations is to think of a crack as an array of dislocations. Indeed, the majority of our work has already been done earlier in the context of our consideration of dislocation pile-ups in section 11.4.2. In fact, our present analysis will do little more than demonstrate that the solutions written down there are relevant in the crack context as well. The more fundamental signiﬁcance of the perspective to be offered here is that we will soon want to build up solutions in which cracks and dislocations are equal partners,

11.5 Cracks and Dislocations

611

and it will be seen that the dislocation ideas developed here provide a useful basis for doing so. One of the key points to be made in the present discussion is the substantiation of the claim that a continuous distribution of inﬁnitesimal dislocations can be assembled in a way that respects the traction-free boundary conditions associated with crack faces. In particular, we consider a crack which runs from −a to a, with a remotely applied stress of the form σx y = τ0 . In this mode II setting (see ﬁg. 11.16), we insist that on the crack faces σ yy = σx y = 0. Our claim is that such a crack can be represented by a distribution of inﬁnitesimal dislocations with a density of the form ρb (x) =

x 2(1 − ν)τ0 . √ 2 µb a − x2

(11.38)

This distribution is determined by insisting that the traction-free condition, a µ ρb (x )d x , (11.39) τ0 = − 2π(1 − ν) −a x − x be imposed along the crack, |x| < a. As pointed out by Weertman (1996), the solution to this problem is reached via recourse to a table of Hilbert transforms and is of the form reported in eqn (11.38). In light of this distribution, we may then write the stresses at an arbitrary point (x, y) as the superposition a tot ρb (x )σi(disl) (x − x , y)d x . (11.40) σi j (x, y) = j −a

We denote the stress ﬁeld due to a single Volterra dislocation at position (x , y ) by σi(disl) (x − x , y − y ). We also note that the original interpretation of the elastic j energy release rate offered in section 2.4.4 can be reinterpreted in terms of the driving forces on the various dislocations making up the crack. Now that we have seen how the crack itself may be written in terms of dislocations, we turn to the question of how to think about such a crack when there are other dislocations in its vicinity. 11.5.2 Dislocation Screening at a Crack Tip From the standpoint of the linear theory of elasticity, the problem of crack tip shielding may be seen as a question of solving the boundary value problem of a crack in the presence of a dislocation in its vicinity. As indicated schematically in ﬁg. 11.15, the perspective we will adopt here is that of the geometrically sterilized two-dimensional problem in which both the crack front and the dislocation line are inﬁnite in extent and perfectly straight. As we will see, even this case places mathematical demands of some sophistication. The basic question we

612

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.15. Conformal transformation from wedge + dislocation to the problem of a half-space containing dislocation (adapted from Ohr et al. (1985)).

pose concerns the nature of the stress ﬁelds in the neighborhood of the crack tip, in particular, as a result of the presence of the dislocation. From a physical perspective, what is found is that the presence of the dislocation inspires the introduction of a local stress intensity factor which may be thought of as an effective stress intensity and may be reduced relative to the bare stress intensity that would be present in the absence of the dislocation. In order to perform the mathematical manipulations that allow for the solution of this problem, we turn to the powerful tools of complex analysis. Of course, the moment we take such a step, it is clear that our methods will be impotent once we pose questions concerning more interesting three-dimensional geometries. We begin with a problem of antiplane shear in which the crack of interest has a mode III geometry, as indicated schematically in ﬁg. 11.16, and the associated dislocation is a screw dislocation. In this instance, the problem is that of ﬁnding a harmonic function u 3 (x, y) such that the relevant boundary conditions are satisﬁed. One particularly elegant scheme for solving this problem is the use of conformal mapping. Geometrically, the problem of wedge + dislocation shown in ﬁg. 11.15 is mapped onto a half-space with a subsurface dislocation, a problem we have already encountered in section 8.5.2, and which culminated in the introduction of an image dislocation. Through the device of determining a potential function that satisﬁes the free surface boundary conditions and subsequent inversion of the mapping so that we recover the original problem of a crack in the presence of a dislocation, the solution is rather immediate. To be concrete, we note that we seek a potential function η(z) such that u(z) = (2/µ) Im[η(z)]. Note that the factor of 2 here is consonant with the convention

11.5 Cracks and Dislocations

613

Fig. 11.16. Three independent modes of crack tip loading and associated dislocations (adapted from Ohr (1985)).

used in Ohr et al. (1985). Once this potential function is in hand, the corresponding stresses may be found using the isotropic linear elastic constitutive relation which in the case of antiplane shear reduces to σi j = 2µi j . In terms of the potential η(z), this may be rewritten as σ (z) = σ yz + iσx z = 2η (z).

(11.41)

In general, for complex geometries, direct determination of the function η(z) cannot be carried out simply. The trick with conformal mapping is to map the originally complex problem onto a simpler geometry for which the corresponding solution is known. In particular, if the mapping that effects this transformation is of the form w = g(z) and the potential for the transformed problem is χ (w), then the stresses for the original problem are obtained as dw . (11.42) dz Note that in this case, the function χ(w) is presumed to be known (usually by virtue of the symmetric geometry of the transformed problem), and dw/dz is a geometric derivative determined strictly by the transformation between the two geometries. For the case of interest here, namely, the ﬁelds that arise for a crack in the presence of a dislocation, the procedure described above is disarmingly simple. Through a suitable choice of transformation, the problem of a crack and dislocation can be mapped onto the problem of a single subsurface dislocation beneath a traction-free surface already solved by the method of images in section 8.5.2. σ (z) = 2χ (w)

614

11 Points, Lines and Walls: Defect Interactions and Material Response

Before writing down the solution we must ﬁrst broach the subject of the geometric transformation relating the wedge crack problem to the allied problem of a free surface. If we consider a wedge crack with opening angle α, all points on the line α π z = r ei(π− 2 ) must be mapped onto the line z = r ei 2 . The transformation that effects this mapping is w = z q , with q = π/(2π − α). Given the transformation, all that remains is to determine the potential χ(w) which characterizes the ﬁelds due to the subsurface dislocation and its image. This solution, which we state without derivation, is given by µb w−δ χ(w) = . (11.43) ln 4π w + δ¯ √ The dislocation of interest is at position δ in the w plane (i.e. δ = ξ , where ξ ¯ For is the dislocation position in the z plane) while its image is at position −δ. √ the special case of a sharp crack of interest here, w = z. If we now apply the prescription of eqn (11.42), we ﬁnd that the stresses are given by 1 1 µb . (11.44) σ (z) = √ √ √ −√ 4π z z− ξ z + ξ¯ The signiﬁcance of the result of eqn (11.44) is that it tells us how to account for the stresses in the context of problems in which a crack and a dislocation coexist. A particularly interesting feature of solutions like that given above is their interpretation as providing a source of screening for the crack tip. The use of the word screening in this context refers to the fact that the local stress intensity factor is modiﬁed by the presence of the dislocation and can result in a net reduction in the local stresses in the vicinity of the crack tip. In particular, the total stress intensity factor is a sum of the form K tot = K I I I + K disl ,

(11.45)

where K I I I is the stress intensity factor for the mode III crack in the presence of remote loading. If we imagine the special case in which the screw dislocation is on the prolongation of the crack plane at a distance d, then the contribution due to the dislocation to the stress intensity factor is given by µb . K disl = − √ 2πd

(11.46)

The key qualitative observation to be made is that the sign of K disl can be negative resulting in the local screening effect alluded to earlier. We note that while the analysis presented here centered on the mathematically simplest case of antiplane shear, there are analogous situations to be found for other modes of crack tip loading as seen in ﬁg. 11.16.

11.5 Cracks and Dislocations

615

Fig. 11.17. Competition at a crack tip between the emission of a dislocation and cleavage (adapted from Beltz et al. (1999)).

11.5.3 Dislocation Nucleation at a Crack Tip The solution constructed above provides the necessary tools from elasticity theory in order to consider nucleation of a dislocation at a crack tip. The philosophical perspective adopted here is that due to Rice (1992) in which a comparison is made between the work needed to create new free surface and that needed to create a slip distribution corresponding ultimately to a dislocation. We present this model not so much with the hope that it will deliver quantitative insights but on the grounds that it is highly instructive concerning the atomic-level processes near a crack tip. In particular, the model is appealing because the treatment of dissipative processes such as dislocation nucleation is endowed with atomic-level realism, while still maintaining an overall continuum description. For an atomically sharp crack subjected to remote mode I loading we may imagine a variety of irreversible mechanisms that might transpire once the load is sufﬁciently large. Two of these processes are the creation of new free surface (cleavage) and the nucleation of dislocations. We have already discovered that the energy release rate tied to the opening displacement discontinuities is that accounted for in the Grifﬁth model of the fracture toughness. Our present task is to ﬁnd the analogous description for dislocation nucleation and to do so, we follow the development of Rice. The basic idea is to express these two processes as a competition and to determine which one will commence at a lower stress level. This competition can be couched in terms of the energy release rates of the two competing processes as shown in ﬁg. 11.17. As noted in the ﬁgure, if the creation of new free surface can occur with a smaller energy release rate than the process of dislocation nucleation, it will be the winner in the competition. Alternatively, if the energy release rate to create a dislocation is the smaller of the two, it will be

616

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.18. Mode II crack with an incipient dislocation along prolongation of the crack plane (adapted from Rice and Beltz (1994)).

the process that transpires. As a result, the question becomes one of obtaining a measure of how much energy is fed to each of these processes during incremental crack extension, with G cleave and G disl being the relevant energy release rates for these two processes. Our preliminary analysis centers around the geometry shown in ﬁg. 11.18 in which an atomically sharp crack is subjected to mode II loading and the slip distribution is assumed to occur along the prolongation of the crack plane. Borrowing from the Peierls–Nabarro analysis described in section 8.6.2, it is assumed that the atomic-level forces across the slip plane may be characterized in terms of an interplanar potential φ(δ). This description asserts that the tractions which arise on account of the sliding discontinuity are given by τ = −∂φ/∂δ. The implementation of the Peierls–Nabarro analysis in the crack tip context is really quite similar to that advanced already in the analysis of dislocations (see section 8.6.2), with the added complication that the energy functional must now account not only for the energy on the slip plane and the interactions between dislocations, but also for the terms resulting from the presence of a crack tip. We begin by writing down an energy functional which features the as-yet undetermined slip distribution. The total energy of the system of crack with its attendant incipient dislocation is a sum of terms representing the energy cost for the slip, the energy associated with the elastic ﬁelds of the crack, and a part reﬂecting the energy associated with the crack interacting with the dislocations. In particular, we have ∞ ∞ KI I δ(r )dr φ[δ(r )]dr − E[δ(r )] = √ 2πr 0 0 ∞ ∞ ρ 1 dδ(ρ) µ δ(r )dr dρ. (11.47) + 4π(1 − ν) 0 r r − ρ dρ 0 Functional differentiation of this equation with respect to the slip distribution

11.5 Cracks and Dislocations

results in the equilibrium equation ∞ dφ µ ρ 1 dδ(ρ) KI I dρ = . − √ 2π(1 − ν) 0 r r − ρ dρ dδ 2πr

617

(11.48)

From a numerical perspective, the critical load for dislocation nucleation can be obtained by repeatedly solving this equation for increasing loads (as reﬂected in the value of K I I ) and seeking that load at which solutions fail to exist. An alternative appealing numerical approach is to map the continuous variational problem described above onto a corresponding discrete problem by parameterizing the solution in terms of a ﬁnite set of variational parameters (i.e. the Rayleigh–Ritz method) and solving the resulting coupled equations. This approach is described in Sch¨ock (1996). On the other hand, Rice has shown through an ingenious application of the J -integral how this problem may be solved analytically. The fundamental philosophy adopted in computing the energy spent in building up the incipient slip distribution is to use the J -integral, the path independence of which allows for a remote and near ﬁeld determination of the energy release rate. The far ﬁeld reckoning of this quantity is given in terms of Irwin’s stress intensity factor introduced in section 2.4.4. By way of contrast, the near ﬁeld evaluation of J reduces to an integral along the slip plane. In particular, we have ∞ − ∂(u + x − ux ) d x, (11.49) τ J =− ∂x 0 This integral may be rewritten as

δti p

J=

τ dδ,

(11.50)

0

which, because the shear stress is known in terms of the interplanar potential may = be directly evaluated yielding J = φ(δti p ). Thus, we have found that K Icrit I 2µφ(δti p )/(1 − ν). What we have learned is that dislocation nucleation will occur once φ(δti p ) reaches its maximum allowable value. This idea is depicted graphically in ﬁg. 11.19 where it is seen that instability to dislocation nucleation occurs when φ(δti p ) = γus , where γus is a material parameter that Rice has christened the unstable stacking energy. This idea is intriguing since it posits that the competition between cleavage and dislocation nucleation has been reduced to consideration of the relative values of two simple material parameters, both of which admit of ﬁrst-principles determination, and relevant geometrical factors. One of the problems with the analysis we have made thus far is its geometric simplicity. For the mode I case of primary interest here, the assumption that dislocations will be nucleated on the prolongation of the slip plane is overly

618

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.19. Potential energy for sliding adjacent crystal planes across one another (adapted from Rice (1992)).

severe. The type of geometry that is more appropriate in this setting is such that dislocations will be nucleated on slip planes that are at an angle θ with respect to the crack plane. In fact, to treat this problem with full generality, it is necessary to consider the role of oblique planes as possible contenders and will be considered further in section 12.6.3. As was hinted at in the previous section, the ease with which dislocations may be produced at a crack tip can clearly alter the mechanical response of a solid containing such a crack. In particular, for the special case of the clean geometry and samples that can be found in a material such as Si, the consideration of the cleavage–dislocation emission dichotomy may encompass all of the relevant mechanisms to attempt model building. As we have done so often before, we look to Ashby for a revealing systemization of the data around which the micromechanical study of fracture is built. In ﬁg. 11.20 a summary of the various fracture mechanisms is presented. One idea that emerges is that often at low temperatures, the sample undergoes virtually no plastic deformation before fracture, while at high temperatures, the material is seen to deform enormously. In addition, examination of the fracture surfaces reveals that different mechanisms are at play in the different results.

11.5 Cracks and Dislocations

619

Fig. 11.20. Schematic of a variety of different fracture mechanisms (adapted from Ashby et al. (1979)).

Despite the overwhelming complexity of real fractures processes, it is possible to discern dominant failure mechanisms under different conditions. However, we should bear in mind that in most instances many different processes transpire simultaneously. In ﬁg. 11.20, the different mechanisms are elucidated schematically. For high loads and low temperatures, we see that our intuition about failure by cleavage is correct, although the crack path can travel either along or through grains depending upon speciﬁc details of a given material. On the other hand, at higher temperatures, other mechanisms such as void nucleation and coalescence can assume a dominant role. The energy expended in such processes deﬁes description in simple Grifﬁth terms in which it is held that all of the elastic energy loss goes to the creation of new free surface. Those mechanisms involving appreciable plastic deformation require the expenditure of greater quantities of energy. This energy increase is revealed in the increased toughness of the material, with typical toughnesses far exceeding their Grifﬁth values. Fracture toughness data are shown in ﬁg. 11.21. The challenge grappled with in the current section

620

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.21. Schematic representation of data on fracture toughness of different materials (adapted from Ashby and Jones (1996)).

is that of explaining the dramatic increase in fracture toughness that can occur, sometimes after a temperature change of only a few degrees. The beginnings of an answer to that question can in some cases be tied to the type of analysis undertaken here, namely, to the energetics of dislocation nucleation at a crack tip.

11.6 Dislocations and Obstacles: Strengthening The fact that we refer to entire historic periods in terms of the names of certain metals is a powerful indirect testimony to the role played by chemical disorder in altering the mechanical properties of materials. Indeed, the appellation Bronze Age refers to precisely that moment in a civilization’s development when it was learned that the addition of tin to copper not only lowers the melting temperature of the resulting alloy relative to pure copper, but increases its strength as well. The goal of the present section is to set the stage for understanding why the addition of tin to copper can change its mechanical properties, and more generally, to recount the role of various strengthening mechanisms in the understanding of the mechanics of materials, and to seek the microscopic origins of hardening

11.6 Dislocations and Obstacles: Strengthening

621

phenomena in their roots in dislocation theory. After describing certain generic features of strengthening mechanisms related to the interactions of dislocations with obstacles, we will take up solution, precipitate and work hardening in turn. A visit to a steel mill results in the immediate recognition that there is more to a given steel than just iron and carbon. This is not accidental. Various chemical elements are introduced in a material with a wide variety of aims including the hardening effects to be considered here. Similarly, entire classes of Al alloys are described on the basis of the impurities that populate them. Beyond the capacity to raise the ﬂow stress by populating the material with either foreign atoms or particles, the stress to induce permanent deformation can be raised by working a material. The key point to be made is the recognition that what all of these hardening mechanisms reﬂect is the fact that some form of microstructural control has been exercised on the material. In that sense, the present section is a follow up on our earlier discussion of microstructure itself (see chap. 10) since we now attempt to explicate the ‘properties’ part of the structure–properties paradigm by tracing the inﬂuence of microstructure on dislocations. As an explicit reminder of the signiﬁcance of microstructural control in the context of strengthening, we recall ﬁg. 8.2 in which the variation in ﬂow stress with various microstructural parameters is shown. For example, ﬁg. 8.2(a) shows the way in which the ﬂow stress increases with the increasing concentration of foreign atoms. From a mechanistic perspective, what transpires in the context of all of these strengthening mechanisms when viewed from the microstructural level is the creation of obstacles to dislocation motion. These obstacles provide an additional resisting force above and beyond the intrinsic lattice friction (i.e. Peierls stress) and are revealed macroscopically through a larger ﬂow stress than would be observed in the absence of such mechanisms. Our aim in this section is to examine how such disorder offers obstacles to the motion of dislocations, to review the phenomenology of particular mechanisms, and then to uncover the ways in which they can be understood on the basis of dislocation theory. This program to understand hardening involves two distinct parts. First, we examine the interaction between a single dislocation and a localized elastic perturbation such as is offered either by an impurity atom or a foreign particle. This analysis demonstrates the force on a dislocation induced by such particles and hints at the possibility that a group of such impurities acting in concert could harden the material. Inspired by the insights gained by considering the role of a single obstacle to dislocation motion, the second part of our argument will be built around the statistical question of how to compute the average effects of a distribution of such obstacles. We begin with a conceptual overview of the hardening process as viewed from the dislocation perspective, followed by a systematic quantitative analysis of both the one-body interaction between a given dislocation and an associated

622

11 Points, Lines and Walls: Defect Interactions and Material Response

obstacle as well as the statistical question of how many such obstacles act in unison. We round out the discussion with an application of these ideas to three of the prominent hardening mechanisms, namely, solution, precipitate and work hardening.

11.6.1 Conceptual Overview of the Motion of Dislocations Through a Field of Obstacles As noted above, our working hypothesis concerning the various hardening mechanisms is that chemical impurities, second-phase particles and even other dislocations serve as obstacles to the motion of a given dislocation. As a result of the presence of these obstacles, the intrinsic lattice resistance τ p is supplemented by additional terms related to the various strengthening mechanisms. We further assume that the ﬂow stress can be written as τc = τ p + τ,

(11.51)

where τc signiﬁes the overall critical ﬂow stress, τ p is the intrinsic lattice friction (i.e. the Peierls stress) and τ is the change in the critical stress resulting from the presence of the obstacles. For simplicity, we will carry out our analysis in the limit in which τ p is negligible and hence use τc and τ interchangeably. As our ﬁrst step in the attempt to model the various strengthening mechanisms within crystals, we consider a problem in the abstract: what is the stress needed to induce glide of a dislocation through an array of obstacles? For the moment, we leave unspeciﬁed the particulars concerning the origins of such obstacles, since our present thinking will aid us in considering a variety of different speciﬁc mechanisms. A pictorial representation of the situation of interest is given in ﬁg. 11.22 in which the dislocation moves through an array of obstacles. As was already noted in chap. 8, much of the business of the metallurgical use of dislocation theory takes place at the level of the line tension approximation. To make our arguments deﬁnite, we consider the case in which the dislocation line tension is assumed to be orientation-independent. We next suppose that the dislocation, which is pinned at two points separated by the distance L, has bowed out under the action of an applied stress τ resulting in an equilibrium at the pinning point between the line tension and the pinning force F of the obstacle itself. As shown in the free-body diagram for the pinning point in ﬁg. 11.23, the equilibrium of the pinning point may be written as F = 2T cos

φ . 2

(11.52)

Recall from the discussion on line tension and dislocation bow-out given in

11.6 Dislocations and Obstacles: Strengthening

623

Fig. 11.22. Dislocation in a random array of obstacles (adapted from Foreman and Makin (1967)).

section 8.7.1, the radius of curvature is related to the applied stress and the line tension via T τb = . (11.53) R We recall the signiﬁcance of this result by noting that it tells us that in the isotropic line tension approximation, the segment bows out into a circular arc with the radius determined by a competition between the line tension and the applied stress. The next step in the general argument being set forth here is to unite eqns (11.52) and (11.53) in such a way that R and φ are replaced by the more metallurgically accessible parameter L which characterizes the mean spacing between obstacles. To do so, we note on the basis of ﬁg. 11.23 that R = L/[2 sin(θ/2)]. Hence, if we rewrite eqn (11.53) using the fact that T = F/[2 cos(φ/2)] and on the grounds that the angles θ and φ are related by sin(θ/2) = cos(φ/2), we ﬁnd the simple and central relation, F (11.54) τc b = . L This equation serves as the foundation of all that we will have to say about hardening. We begin by noting that the numerator is a reﬂection of the interaction between a single obstacle and a single dislocation. As a result, it is something that we can expect to understand on the basis of local calculations that concern themselves only with the properties of a single such interaction. By way of contrast, the denominator reﬂects the statistical properties related to the distribution of obstacles. As we will see below, there are a number of different ways of

624

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.23. Free-body diagram for the interaction of a dislocation and an obstacle characterized by a pinning force F.

constructing approximate models of the mean dislocation spacing, a fact which we signify by adopting the notation L eff which reminds us that the obstacles are distributed throughout the solid, and that to use an equation like eqn (11.54) to describe the yield properties of the solid as a whole (as opposed to describing the properties of a single segment of length L between two pinning points) we will have to determine L eff using some sort of statistical arguments. There are two scenarios which can develop in the context of the type of bow-out considered here. Either, the line tension forces become so large that they exceed the maximum resistance of the pinning point, or the pinning force is so strong that two adjacent bowed-out segments rejoin through a process known as Orowan looping. In the context of the former process, breakaway of the dislocation can be seen to occur when the applied stress reaches the critical value corresponding to the maximum resistance that can be offered by the obstacle, Fmax . Hence, eqn (11.54) may be rewritten in the form Fmax . (11.55) τc = bL eff By way of contrast, the resisting force offered by the obstacle at the moment of breakaway corresponding to the Orowan process is dictated by the equilibrium equation written above as eqn (11.52). In particular, since φ = 0 in this case, we have Fmax = 2T , and therefore the critical stress is τc =

2T . bL eff

(11.56)

11.6 Dislocations and Obstacles: Strengthening

625

The beauty of this result is that it requires no particular insight into the details of the pinning force, only requiring a bound on its net strength. We will see in our discussion of precipitate hardening that both bow-out scenarios are possible and result in different conclusions as to the way in which τ scales with the particle size and distribution. There are a number of different complaints that can be registered concerning our arguments. First, our results are cast in the abstract language of the modeler, without any reference to the more important microstructural parameters that are experimentally accessible. For example, we would clearly prefer a statement of the critical stress in terms of parameters such as the volume fraction of obstacles and their mean size. In addition, there is a distinctly approximate ﬂavor to our treatment of the distribution of obstacles which appears only through the parameter L eff . In coming sections, we will see just how far we might go in remedying these shortcomings. As yet, we have made no reference to the physical origins of the obstacle force Fmax . In the next section, we examine the way in which insights may be borrowed from the linear theory of elasticity in order to develop plausible models of these forces.

11.6.2 The Force Between Dislocations and Glide Obstacles Our current ambition is to elucidate one of the microscopic mechanisms that has been charged with giving rise to solution and precipitate hardening. The argument is that by virtue of the elastic ﬁelds induced by an obstacle there will be a force on a dislocation which the dislocation must overcome in its motion through the crystal. As a ﬁrst step towards modeling this phenomenon, we imagine the obstacle to be a spherical disturbance within the material. As was already demonstrated in chap. 7, such an obstacle produces spherically symmetric displacement ﬁelds of the form u r = Ar + b/r 2 . Once again invoking arguments about conﬁgurational forces, our expectation is that the force of interest is given by the derivative in the interaction energy as a function of some small excursion of the dislocation line. In generic terms, to ﬁnd the interaction energy we must evaluate the integrals 1 disl obs obs disl σ dV + σi j i j d V , (11.57) E int = 2 ij ij where the superscripts refer to the ﬁelds of the dislocation (disl) and obstacle (obs). This equation derives from the recognition that the total elastic energy is given by an integral 1 E tot = σ tot tot d V, (11.58) 2 ij ij

626

11 Points, Lines and Walls: Defect Interactions and Material Response

and the observation that by linearity, the total ﬁelds can be written as a superposition of the separate obstacle and dislocation ﬁelds. Furthermore, if we note that both the dislocation and obstacle stress ﬁelds are obtained using the same elastic modulus tensor, then eqn (11.57) collapses to disl σiobs (11.59) E int = j i j d V,

which will serve as the starting point for the remainder of our analysis. In principle, eqn (11.59) is all that we need to go about computing the interaction force between an obstacle and a dislocation. However, we will ﬁnd it convenient to rewrite this equation in a more transparent form for the present discussion. Using the principle of virtual work, we may rewrite the interaction energy as f obs · udisl d V. (11.60) E int =

Recall that the obstacle elastic ﬁelds may be arrived at by solving a boundary value problem in which three force dipoles are superposed as we did in chap. 7. In particular, we had

3 a a obs F δ x − x − ei − δ x − x + ei ei . (11.61) f (x) = 2 2 i=1 Substituting this expression into eqn (11.60), we are led to

3 a a F u idisl x + ei − u idisl x − ei . E int = 2 2 i=1

(11.62)

If we now go about expanding the displacement ﬁelds about the point x , then we are left with E int ≈ Fa∇ · udisl .

(11.63)

Recall from our review of continuum mechanics that the divergence of the displacement ﬁeld is a measure of the volume change associated with a given deformation. In this case, it is the volume change associated with the dislocation ﬁelds at the obstacle that gives rise to the interaction energy. At this level of description, only an edge dislocation will have any interaction with our spherical obstacle since tr( ) = 0 for a screw dislocation. On the other hand, for an edge dislocation we have ∇ · u = tr( ) = −

b 1 − 2ν sin θ . 2π 1 − ν r

(11.64)

With this result in hand, the interaction force between the dislocation and the

11.6 Dislocations and Obstacles: Strengthening

627

Fig. 11.24. Schematic of the geometry of interaction between a spherically symmetric obstacle and an edge dislocation.

obstacle may be computed by differentiating the interaction energy with respect to the coordinates of the dislocation. In particular, if we consider the case depicted schematically in ﬁg. 11.24, and interest ourselves only in the component of the force acting along the glide direction of the dislocation, we have Fx = −

x ∂ E int = −C 2 , ∂x (x + d 2 )2

(11.65)

where we have absorbed all of the material and geometric constants describing the dislocation and√obstacle themselves into the constant C. The maximum force occurs for x = d/ 3. To complete this model, we must return to an explicit reckoning of the quantity Fa which appears in the discussion above. In particular, recall that this product is the dipole moment associated with the obstacle and we wish to reconcile this quantity with the geometric features of the spherical inclusion such as its radius and the displacement at its surface. To do so, we recall from our earlier discussion that the displacement induced by such a collection of force dipoles is given by u(x) =

r Fa . 4π(λ + 2µ) r 3

(11.66)

Hence, if we insist that the displacement at the surface of this hole (i.e. for r = a0 /2) is δ, then we ﬁnd Fa = 4π δa02 (λ + 2µ).

(11.67)

If we rewrite λ + 2µ in terms of µ and ν and substitute the resulting expression

628

11 Points, Lines and Walls: Defect Interactions and Material Response

into our equation for the interaction force, we are left with E int = −4µδa02 bd

d , x2 + d2

(11.68)

and Fx = −8µδa02 bd

(x 2

x . + d 2 )2

(11.69)

As yet, our analysis has concerned itself with the total interaction force between the dislocation and the obstacle to its motion. However, a deeper understanding of the pinning process itself can be reached if we compute the force on the dislocation segment by segment. The geometry of interest is indicated in ﬁg. 11.24. We are now interested in obtaining the force on a segment at the point shown in the ﬁgure with coordinates (x, y, 0). The calculation amounts to nothing more than computing the Peach–Koehler force df = (σ b) × dl. The glide component of that bdl, where the stress ﬁeld is that due to the obstacle. force is given by −σxobstacle z Recall from our earlier discussion that the displacements for the obstacle (assumed spherically symmetric for the moment) are u r = δ(a0 /r )2 . Such displacements imply a strain x z = −

3δa02 xh 5

(x 2 + y 2 + h 2 ) 2

,

(11.70)

where the parameter h is the distance of the obstacle beneath the slip plane. As a result of this analysis, we ﬁnd that the localized force on the dislocation segment due to the obstacle is 6µbδa02 dh Fglide = . (11.71) 5 dl (d 2 + h 2 + y 2 ) 2 Although there are a number of interesting features of this analysis, it also leaves us with serious concerns about the formulation of an elastic theory of the obstacle forces that impede dislocation motion. In particular, this analysis suggests that for an obstacle on the slip plane itself, there is no interaction with the dislocation. Despite this elastic perspective, it seems certain that core effects will amend this conclusion.

11.6.3 The Question of Statistical Superposition In the previous subsection, we considered the emergence of the parameter F in eqn (11.54) on the basis of an elastic treatment of the interaction between a single dislocation and a single obstacle. In order to complete the analysis associated with eqn (11.54) we must now determine the parameter L eff which characterizes the distribution of obstacles. To do so, we will invoke statistical arguments of varying

11.6 Dislocations and Obstacles: Strengthening

629

Fig. 11.25. Schematic of the random forces exerted on a dislocation by virtue of the presence of point disorder such as is induced by foreign particles (adapted from Mott and Nabarro (1948)).

levels of sophistication. Our key approach will be that of localized point obstacles which Nabarro (1972) points out ‘provides an anchor in the sea of uncertainty.’ In light of our understanding of the interaction between a single localized obstacle and a dislocation, we next take up the question of how many such interactions conspire to yield observed hardening behavior. Again, we begin with a qualitative discussion aimed at examining some of the generic issues that must be addressed in tackling the question of statistical superposition of interest here. To that end, ﬁg. 11.25 shows a schematic from one of the famed early papers of hardening (Mott and Nabarro, 1948) in which an attempt was made to show the sort of random assemblage of forces that would act on a dislocation in the presence of a statistical distribution of obstacles. For our present purposes, what we wish to note is that unlike the ideal situation considered in our discussion of the Peierls stress which culminated in eqn (8.87), the intrinsic lattice friction must be supplemented by the statistical superposition of the random forces considered here. A more sophisticated consideration of the forces that are exerted upon a dislocation as it glides through a medium populated by a distribution of obstacles is depicted in ﬁg. 11.26. In this case, the fundamental idea that is being conveyed is to divide the character of various obstacles along the lines of whether or not they are localized or diffuse and whether or not they are ‘strong’ or ‘weak’. These different scenarios result in different scaling laws for the critical stress to induce dislocation motion.

630

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.26. Four distinct regimes suggested for the interactions between a dislocation and the disorder distributed throughout the body (adapted from Nabarro (1972)). The four regimes of interest are: (a) weak, localized obstacles, (b) strong, localized obstacles, (c) weak, diffuse obstacles and (d) strong, diffuse obstacles.

Periodic Array of Point Obstacles. The simplest picture that can be developed, and one for which our analysis leading up to eqn (11.54) is essentially exact, is one in which it is imagined that the obstacles are arranged periodically in the slip plane. One argument that we might set up to compute the areal density in terms of the known volume concentration c of obstacles, is to note that if we assign a slip plane of area A a volume Ab, then the number of obstacles found in that plane will be c Ab. We have used the discrete packing of atomic planes to obtain a volume per plane c Ab. As a result of this argument, we see that the areal density may be written either as c Ab/A or in terms of L eff as 1/L 2eff . What we have said is that the c Ab obstacles which ﬁnd themselves in the slip plane of interest are arranged on a square lattice with lattice parameter L eff . By equating our two expressions for the areal density, we are left with the relation 1 L eff = √ . bc

(11.72)

If we take the result given above and exploit it in the context of eqn (11.54) we obtain one of the crucial scaling relations for obstacle limited motion of dislocations, namely, √ (11.73) τc ∝ c.

11.6 Dislocations and Obstacles: Strengthening

631

Fig. 11.27. Schematic of two consecutive conﬁgurations in the unpinning history of a given dislocation.

This result is one which Kocks (1977) goes so far as to note already contains ‘the most important result of dislocation theory: namely, that the ﬂow stress is proportional to the square root of concentration’. Indeed, to the extent that we are interested in understanding the observed macroscopic plastic properties of materials, scaling relations involving the concentration of obstacles are pivotal. Random Array of Point Obstacles. At the next level of sophistication we imagine the opposite extreme in which the distribution of point obstacles is taken to be completely random. As was mentioned above, there are a variety of circumstances √ in which the τc ∝ c scaling is obtained, and we will see that in the present setting this same scaling is found. Our strategy is to compute the so-called Friedel length, which is a stress-dependent measure of the effective spacing between obstacles. In this case, the argument is altogether more subtle. The basic idea is to consider two consecutive pinned conﬁgurations such as are shown in ﬁg. 11.27. Physically, the idea is that as the stress increases, the number of pinning points that the dislocation joins up with will vary. As a result, even though the areal density of such pinning points is unchanged, the mean spacing between such pinning points along the dislocation (i.e. L eff ) will change. Our aim is to estimate L eff and in particular, its stress dependence. The key physical assumption made in the Friedel argument√is that once the dislocation becomes unpinned it will sweep an area l 2 = 1/ bc before encountering another pinning point. Comparison of the two conﬁgurations shown in ﬁg. 11.27 √ shows that in passing from the initial to the ﬁnal 2 conﬁguration, an area l = 1/ bc is swept out. To make these arguments concrete, we note that we are insisting that the area A swept out be given by the relation 2L eff L eff 1 A = = u 2 (x)d x − 2 u 1 (x)d x. (11.74) bc 0 0 We have introduced the function u 1 (x) to characterize the dislocation position

632

11 Points, Lines and Walls: Defect Interactions and Material Response

of the initial conﬁguration and u 2 (x) to characterize the dislocation of the ﬁnal conﬁguration. Note that the as-yet undetermined (and desired) parameter L eff appears in the limits of integration and will be determined in the end as a function of the concentration and the applied stress. In fact, to obtain the functions u 1 (x) and u 2 (x) we use what we already learned about dislocation bow-out in section 8.7.1. In particular, in the limit of weak driving force (which corresponds to the presumed weakness of the obstacles) generically, the dislocation proﬁle is of the form u(x) = −

τb 2 x + cx, T

(11.75)

where the constant c is determined by appealing to the boundary conditions. In the present case, we have u 1 (0) = u 1 (L eff ) = 0 and u 2 (0) = u 2 (2L eff ) = 0. Application of these boundary conditions results in the solutions τb (L eff x − x 2 ) 2T

(11.76)

τb x2 L eff x − . T 2

(11.77)

u 1 (x) = and u 2 (x) =

With these results in hand we may evaluate the integrals demanded in eqn (11.74) with the result that τ bL 3eff . (11.78) A = 2T Note that as a result of these arguments we may now determine L eff as L eff =

2T τ b2 c

13

.

(11.79)

This result is now in a form that may be fed back into eqn (11.55) with the result that 1 Fmax τc b2 c 3 , (11.80) τc = b 2T which may be solved for τc with the result that τc =

3 Fmax 2T b

12

1

c2.

(11.81)

We note that even in the context of this more roundabout description of the superposition of the effect of different obstacles, we once again recover the τc ∝ c1/2 scaling discussed earlier.

11.6 Dislocations and Obstacles: Strengthening

633

Continuously Distributed Disorder. Our treatment until this point has treated the disordering effect of the obstacles on the basis of a picture in which the homogeneous medium is punctuated by localized forces. An alternative viewpoint is one in which the disordering effect is imagined to be distributed continuously throughout the medium resulting in a local contribution to the resistance at every point on the dislocation. As a result of this picture, rather than attempting to assert equilibrium conditions only at pinning points, equilibrium is represented in integral form along the entire length of the dislocation. For the present purposes, the crucial conclusion of this analysis which we quote without derivation is the assertion that the critical stress to induce dislocation glide scales as τc ∝ c2/3 . Our reason for bringing this result up at all is mainly to serve as a point of comparison when we consider the actual data on solution hardening to be taken up in the next section.

11.6.4 Solution Hardening The use of impurities to alter the behavior of materials is a technique of great signiﬁcance, and solution hardening is but one of many ways in which this is carried out. Our intention in this section is to present a few experimental highlights which reveal the level of the quantitative understanding of solution hardening which will serve to catalyze the modeling discussion to follow. Having introduced the experimental backdrop, the remainder of our discussion will be ﬁxed on how well the ideas introduced in the previous few subsections rise to the challenge of the data. An example of the type of data associated with solution hardening it is the mission of our models to explain was shown in ﬁg. 8.2(a). For our present purposes, there are questions to be posed of both a qualitative and quantitative character. On the qualitative side, we would like to know how the presence of foreign atoms dissolved in the matrix can have the effect of strengthening a material. In particular, how can we reconcile what we know about point defects in solids with the elastic model of dislocation–obstacle interaction presented in section 11.6.2. From a more quantitative perspective, we are particularly interested in the question of to what extent the experimental data permit a scaling description of the hardening effect (i.e. τ ∝ cn ) and in addition, to what extent statistical superposition of the presumed elastic interactions between dislocations and impurities provides for such scaling laws. The metallurgical approach to coming to terms with data like that considered above is by virtue of an appeal to various parameters that signal the presence of foreign atoms and which can be used as the basis of contact with the elastic theory of interaction forces. Indeed, although results like that revealed in eqn (11.81) are extremely provocative, our work will only be done once plausible strategies are

634

11 Points, Lines and Walls: Defect Interactions and Material Response

found for linking quantities such as Fmax to underlying parameters of metallurgical signiﬁcance. In particular, two of the most immediate parameters that measure the extent to which a given set of foreign atoms will make their presence known to the dislocation elastically are the size misﬁt parameter deﬁned by δ=

1 da , a dc

(11.82)

η=

1 dµ . µ dc

(11.83)

and the modulus misﬁt parameter

The symbols introduced here include the lattice parameter a, the concentration c and the shear modulus µ. The purpose of these parameters is to provide a measure of the extent to which the presence of foreign atoms within the matrix will result in elastic interactions between these impurities and dislocations present in the material. My own take on these ideas is that they are largely inspired by the desire to make contact with the ideas on elastic ﬁelds of inclusions developed by Eshelby. We remind the reader that in that setting (see section 7.3.2), a foreign particle can make its presence known by virtue both of a difference in size and of a difference in moduli between the matrix and the particle. Of course, when speaking of a single foreign atom, these continuum notions become highly suspect. Nevertheless, what our elastic models have shown us is that if we are to install an inclusion within a continuum, the distinction between that particle and the surrounding matrix material can be introduced either by attributing a different size to that particle or by asserting that it is characterized by different moduli than that of the matrix material. The parameters δ and η introduced in eqns (11.82) and (11.83) measure the strength of these two effects. In addition to the two mechanisms introduced above, there are a variety of other mechanisms that have been invoked to explain the origins of solution hardening, including contributions due to the presence of stacking faults, the difference in valence of the matrix and solute and ordering effects. The key point to be taken away from this part of the discussion is the recognition that there are a wide variety of different ways in which we can construct elastic models of the interaction between foreign atoms and dislocations. We have seen that if we model a given foreign atom as a source of dilatation, a dislocation–obstacle interaction arises that depends upon the parameter δ. Similarly, if a given foreign atom is modeled as a source of elastic inhomogeneity (i.e. a region of different elastic constants than the matrix) then a dislocation–obstacle interaction arises that depends upon parameters like η introduced above. In addition to these models, it is also possible to imagine more sophisticated effects related to elastically induced redistribution

11.6 Dislocations and Obstacles: Strengthening

635

2 √ Fig. 11.28. Illustration of ﬁt to c and c 3 scaling to observations on solid solution hardening in Au–Al (adapted from Haasen (1979)).

of the foreign atoms around the dislocations. All of these models share the feature that they inhibit the motion of dislocations. Though the qualitative ideas introduced above are instructive, to really make contact with experiment we must calculate something. In particular, we need to ﬁnd a way to average over the types of disorder described schematically in ﬁg. 11.26 so as to obtain a concrete result for the scaling of the ﬂow stress with the concentration of foreign atoms, for example. Indeed, this is precisely what was done in various approximations in section 11.6.3. For the present purposes what we wish to really note about the outcome of the arguments given there is the emergence of two different scaling laws for how the critical stress scales with the concentration √ of impurities, namely, τc ∝ c and τc ∝ c2/3 . A provocative representation of experimental data on solution hardening is shown in ﬁg. 11.28. What we see on the basis of these data is that although clearly increasing the concentration increases the critical stress, identifying the particular scaling relation is a more challenging proposition. In addition to the attempt to link observed solution hardening with ideas on the scaling with concentration, efforts have been put forth on examining how the strengthening effect scales with the parameters δ and η. A particular example which reveals the magnitude of the hardening effect as a function of the size of the foreign atoms is shown in ﬁg. 11.29. The reader is encouraged to examine these issues in the article of Haasen (1979). A second facet to this discussion that we have omitted but which is immensely important is the temperature dependence of the ﬂow stress. As it stands, our discussion really only attempts to answer to the challenge of the zero-temperature contribution to the ﬂow stress.

636

11 Points, Lines and Walls: Defect Interactions and Material Response 20

c, MN m-2/at -%

16

Cu

Mn

12 Mg 8

4

Ag

Ge

Li Zn 0

10

20

30 40 50 * [( s- A)/ A] x 100

60

70

Fig. 11.29. Magnitude of solution hardening effect in Al alloys as a function of the size mismatch of the foreign atoms (adapted from Embury et al. (1989)).

11.6.5 Precipitate Hardening In the previous section, we saw that we can arrange that a particular material be endowed with a supersaturation of impurities by quenching some concentration of foreign atoms in the material beyond the solubility limit. On the other hand, the resulting microstructure is metastable. The equilibrium phase that is preferred in this part of the phase diagram is two-phase coexistence between the pure phase and a second phase, which is often an ordered alloy built up from the two components. For example, in the context of the Fe–C phase diagram, this coexistence is struck between α-Fe (bcc) and an orthorhombic phase of Fe3 C. From a modeling perspective for considering the mechanics of such two-phase microstructures, the simplest picture we might imagine is that the nuclei of these precipitates are spherical and that their radii increase with time. The presence of such second-phase particles makes itself known through a substantive change in the mechanical properties of the material, a speciﬁc example of which is shown in ﬁg. 8.2(b) Observations on precipitation hardening make it evident that in certain cases the key microstructural features in this context are the mean particle radius and the

11.6 Dislocations and Obstacles: Strengthening

637

Fig. 11.30. Illustration of the variation in ﬂow stress as a function of precipitate radius (adapted from Reppich (1993)).

volume fraction of such precipitates. In particular, the type of generic results that emerge are indicated schematically in ﬁg. 11.30 in which the variation in the ﬂow stress is shown as a function of particle size. Our present ambition is to explain this behavior on the basis of the type of simple models developed above. In simplest terms, the key feature of the ﬂow stress increment as a function of particle size is the fact that there is an ‘optimal’ particle size. What we will ﬁnd is that this maximum reﬂects a change in mechanism from particle cutting, which is dominant at small radii, to the Orowan process, which is easier at large particle radii. Our discussion in section 11.6.1 culminated in two possible outcomes to the encounter of a dislocation with an array of pinning points. On the one hand, we found that if the obstacles are sufﬁciently weak (characterized by a maximum force Fmax ), they will be breached at a critical stress of τc = Fmax /bL eff as shown in eqn (11.55). On the other hand, if the obstacles are strong enough, they will be traversed by an alternative mechanism in which the dislocations loop around the obstacle and rejoin on the opposite side, a mechanism known as Orowan looping and characterized by a strength τc = 2T /bL eff as shown in the derivation leading up to eqn (11.56). These two different eventualities are illustrated schematically in ﬁg. 11.31. We now undertake a systematic analysis of these two mechanisms, with special emphasis being placed on how to rewrite eqns (11.55) and (11.56) in terms of the metallurgical parameters relevant to two-phase microstructures.

638

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.31. Schematic of the Orowan looping and particle cutting mechanisms that arise from interaction of dislocations with foreign particles (adapted from Gerrold (1979)).

Particle Cutting For small radii, the mechanism of dislocation interaction with the foreign particles is that of particle cutting in which after a certain maximum force is reached, the dislocation shears the foreign particles themselves. As a result, in this context the relevant equation for the critical stress is eqn (11.55) and our charter is to reﬂect once again on Fmax and L eff from the perspective of the microstructure itself. Without entering into details, we note that L eff can be obtained using exactly the same arguments given in section 11.6.3 with the proviso that we replace bc with the areal density ρArea . If we carry out this substitution, eqn (11.55) may be rewritten as 3

2 Fmax √ ρArea . τc = √ b 2T

(11.84)

At this point our task is to relate the areal density ρArea to the volume fraction of second-phase particles, denoted by f , and to the particle radius R. To convert the result given above into these more usable terms, we make a highly simpliﬁed argument based on the following assumptions. (1) The particles are all of the same size and are characterized by a radius R. (2) The estimate of the mean particle spacing is determined by assuming full correlation between the particles positions. For simplicity, we imagine them arranged on a three-dimensional cubic

11.6 Dislocations and Obstacles: Strengthening

639

Fig. 11.32. Schematic of the geometry of the precipitate particles.

lattice. Note that despite the seeming artiﬁcial nature of these assumptions, in some cases the distribution of precipitates can indeed be highly regular. To determine the mean spacing between obstacles, we begin with the modeling assumption that any particle whose center lies within a distance R of the slip plane of interest is considered to provide a glide obstacle on that slip plane. Further, we assert that the volume fraction of such particles is given by the parameter f . The geometrical ideas are depicted in ﬁg. 11.32. The volume occupied by the precipitate particles in this slab of thickness 2R and area A is 2A f R. Hence the number of particles in this slab volume can be estimated by dividing the volume occupied by particles within the slab by the volume per particle, resulting in # particles in slab = 3A f /2π R 2 . This result may be used to compute the area per obstacle (Aobstacle ). Note that the area per obstacle is related to the areal density by ρArea = 1/Aobstacle . The area per obstacle is found by dividing the total area of the slip plane by the number of such particles and yields the estimate 3f . (11.85) 2π R 2 In light of these arguments, the critical stress for particle cutting is of the form 3/2 Fmax 3 f 1 τc = √ . (11.86) b 2T 2π R ρArea =

In order to complete the discussion, we must say something about how Fmax depends upon the mean particle radius. It is crucial to note that a wide variety of different Fmax s associated with particle cutting have been determined. For a broad discussion of this topic see section 2.3 of the article by Gerrold (1979) and

640

11 Points, Lines and Walls: Defect Interactions and Material Response

Fig. 11.33. Schematic cross section of a precipitate particle as it is being cut by a gliding dislocation.

the discussion in section IV of the article by Embury et al. (1989). Rather than entering into the particulars of these different mechanisms, we note that much can be learned by examining the scaling of τc with f and R for different choices of Fmax . In particular, we note that if we make the assumption that Fmax s